An overview of the optical effects in solids, addressing the physics of various materials and their response to electrom

*938*
*145*
*23MB*

*English*
*Pages 414*
*Year 2019*

*Table of contents : Cover......Page 1Front Matter......Page 3Optical Effects in Solids......Page 5Copyright......Page 6Dedication......Page 7Contents......Page 9Preface......Page 131 Introduction......Page 152 Maxwell’s Equations and PlaneWaves in Matter......Page 203 The Complex Dielectric Function andRefractive Index......Page 314 Classical Theories for the Dielectric Function......Page 445 Phonons......Page 766 A Look at Real Solids......Page 957 Transmission and Reflection......Page 1108 Free-ElectronMetals......Page 1299 Optical Excitations: Quantum Mechanics......Page 15110 Kramers–Kronig Relations and SumRules......Page 16611 Superconductors......Page 18912 Semiconductors and Insulators......Page 22113 Strongly Interacting Solids......Page 25514 Nonlocal Effects......Page 27715 Anisotropic Crystals......Page 29016 Magneto-Optics......Page 31817 Inhomogeneous Materials......Page 347Appendix A. Notes about Units......Page 361Appendix B. Maxwell’s Equations in SI......Page 364Appendix C. Partial Derivatives and VectorOperators Acting on PlaneWaves......Page 366Appendix D. TheWave Equation......Page 367Appendix E. Reflection and Transmission atOblique Incidence......Page 368Appendix F. A Field Guide to Optical “Constants”......Page 379Appendix G. Software......Page 386References......Page 387Index......Page 411*

Optical Effects in Solids

An overview of the optical effects in solids, this book addresses the physics of materials and their response to electromagnetic radiation. The discussion includes metals, superconductors, semiconductors and insulators. The book begins by introducing the dielectric function into Maxwell’s macroscopic equations and ﬁnding their plane-wave solution. The physics governing the dielectric function of various materials is then covered, both classically and using basic quantum mechanics. Advanced topics covered include interacting electrons, the anomalous skin effect, anisotropy, magneto-optics, and inhomogeneous materials. Each subject begins with a connection to the basic physics of the particular solid, after which the measurable optical quantities are derived. It allows the reader to connect measurements (reﬂectance, optical conductivity, and dielectric function) with the underlying physics of solids. Methods of analyzing experimental data are addressed, making this an ideal resource for students and researchers interested in solid-state physics, optics, and materials science. David B. Tanner is a distinguished professor of physics at the University of Florida. His research focuses on condensed matter physics and on astrophysics. He has previously served as department chair and chair of the Division of Condensed Matter Physics for the American Physical Society (APS). In 2016 he received the APS Frank Isakson Prize for Optical Effects in Solids and, in the same year, shared a Special Breakthrough Prize in Fundamental Physics for the discovery of gravitational waves.

Optical Effects in Solids DAVID B. TANNER University of Florida

University Printing House, Cambridge CB2 8BS, United Kingdom One Liberty Plaza, 20th Floor, New York, NY 10006, USA 477 Williamstown Road, Port Melbourne, VIC 3207, Australia 314–321, 3rd Floor, Plot 3, Splendor Forum, Jasola District Centre, New Delhi – 110025, India 79 Anson Road, #06–04/06, Singapore 079906 Cambridge University Press is part of the University of Cambridge. It furthers the University’s mission by disseminating knowledge in the pursuit of education, learning, and research at the highest international levels of excellence. www.cambridge.org Information on this title: www.cambridge.org/9781107160149 DOI: 10.1017/9781316672778 © David B. Tanner 2019 This publication is in copyright. Subject to statutory exception and to the provisions of relevant collective licensing agreements, no reproduction of any part may take place without the written permission of Cambridge University Press. First published 2019 Printed in the United Kingdom by TJ International Ltd, Padstow Cornwall A catalogue record for this publication is available from the British Library. Library of Congress Cataloging-in-Publication Data Names: Tanner, David B., 1945– author. Title: Optical effects in solids / David B. Tanner (University of Florida). Description: Cambridge ; New York, NY : Cambridge University Press, [2019] | Includes bibliographical references and index. Identiﬁers: LCCN 2018046542 | ISBN 9781107160149 (hardback) Subjects: LCSH: Solids–Optical properties. | Light. | Materials–Optical properties. | Light–Scattering. | Reﬂection (Optics) | Electromagnetic waves. Classiﬁcation: LCC QC176.8.O6 T36 2019 | DDC 530.4/12–dc23 LC record available at https://lccn.loc.gov/2018046542 ISBN 978-1-107-16014-9 Hardback Cambridge University Press has no responsibility for the persistence or accuracy of URLs for external or third-party internet websites referred to in this publication and does not guarantee that any content on such websites is, or will remain, accurate or appropriate.

for Marcia

Contents

Preface

page xi

1

Introduction

2

Maxwell’s Equations and Plane Waves in Matter 2.1 2.2 2.3 2.4 2.5 2.6 2.7 2.8 2.9 2.10

3

Optical Constants Maxwell’s Equations Total, Free, and Bound Charges and Currents Maxwell’s Equations for Solids Plane-Wave Solutions Converting Differential Equations to Algebraic Ones Vector Directions Electromagnetic Waves in Vacuum Five Easy Simpliﬁcations Maxwell’s Equations for These Easy Cases

The Complex Dielectric Function and Refractive Index 3.1 3.2 3.3 3.4 3.5 3.6 3.7 3.8

Conductivity and Dielectric Constant The Complex Dielectric Function The Optical Conductivity The Complex Refractive Index Energy Density, Poynting Vector, and Intensity Normal-Incidence Reﬂectance What If My Solid Is Magnetic? Negative Index Materials

4 Classical Theories for the Dielectric Function 4.1 4.2 4.3 4.4 4.5 4.6

vii

A Polarizable Medium Drude Absorption by Free Carriers The Plasma Frequency Lorentz Model: Absorption by Bound Electrons Comments on Wave Propagation The Absorption Coefﬁcient and a Not Uncommon Mistake

1 6 6 6 8 9 10 11 11 11 12 15 17 17 18 18 19 21 24 27 28 30 30 31 42 44 55 61

viii

Contents

5

Phonons 5.1 5.2 5.3 5.4 5.5 5.6 5.7 5.8

Harmonic Oscillator Lattice Dynamics Interaction with Electromagnetic Waves Transverse and Longitudinal Modes The Lyddane–Sachs–Teller Relation Other Notations Multiple Modes Polaritons

6 A Look at Real Solids 6.1 6.2 6.3 6.4 6.5 6.6

7

Silver Other Noble Metals Aluminum Silicon Sodium Chloride Other Alkali Halides

Transmission and Reflection 7.1 7.2 7.3 7.4

Incoherent Light Coherent Light The Matrix Method Inverting R and T to Find

8 Free-Electron Metals 8.1 8.2 8.3 8.4 8.5 8.6 8.7 8.8 8.9

Schr¨odinger Equation for Free Electrons Wave Function Exclusion Principle and Boundary Conditions The Fermi Energy The Effect of Temperature The Density of States Electrical Conductivity Discussion of the Drude Model The Boltzmann Transport Equation

9 Optical Excitations: Quantum Mechanics 9.1 9.2 9.3 9.4 9.5 9.6 9.7

The Solid with an Electromagnetic Field Perturbation Expansion The Matrix Element of the Perturbation Fermi’s “Golden Rule” Electric Dipole Transitions The Oscillator Strength Oscillator Strength Sum Rule

62 62 64 72 73 75 76 76 78 81 81 85 86 87 90 93 96 96 99 107 109 115 115 116 117 119 121 122 122 125 130 137 138 139 141 143 145 146 148

ix

Contents

10 Kramers–Kronig Relations and Sum Rules 10.1 10.2 10.3 10.4 10.5 10.6

Absorption and Dispersion Must Be Related Kramers–Kronig Integrals Kramers–Kronig Analysis of Reﬂectance Another Look at the Conductivity Sum Rules Partial Sum Rules

11 Superconductors 11.1 11.2 11.3 11.4 11.5 11.6 11.7 11.8

Superconducting Phenomena Theoretical Background The London Model Length Scales for Superconductors Excitations in a Superconductor The Optical Conductivity of a Superconductor Thin Film Superconductors Unconventional Superconductors

12 Semiconductors and Insulators 12.1 12.2 12.3 12.4 12.5 12.6 12.7 12.8 12.9 12.10 12.11

Band Structure Nearly Free Electrons Bloch’s Theorem The Brillouin Zone Band Gaps of Semiconductors Effective Mass Direct Interband Transitions The Joint Density of States and Critical Points Indirect Band Gap Absorption Excitons Impurity-Induced Absorption

13 Strongly Interacting Solids 13.1 13.2 13.3

Notation: The Generalized Drude Model Electron–Electron Interactions Electron–Phonon Interactions

14 Nonlocal Effects 14.1 14.2 14.3 14.4 14.5

The Normal Skin Effect The Anomalous Skin Effect The Extreme Anomalous Limit ω–τ Plot The Surface Impedance

152 152 157 164 169 170 173 175 175 180 181 188 189 195 201 203 207 207 209 212 213 215 216 218 224 225 233 236 241 242 247 257 263 263 266 267 268 270

x

Contents

15 Anisotropic Crystals 15.1 15.2 15.3 15.4 15.5 15.6 15.7 15.8 15.9 15.10

Optics of Crystals Polarized Light Crystal Symmetry The Dielectric Tensor Plane-Wave Propagation in Anisotropic Materials The Uniaxial Crystal The Biaxial Crystal Anisotropic Material with Boundaries: R and T Polarizers and Waveplates Things Not in This Chapter

16 Magneto-Optics 16.1 16.2 16.3 16.4 16.5

Charged Particle in a Magnetic Field Magneto-Conductivity Tensor of a Metal Electromagnetic Wave Propagation Other Magneto-Optical Effects Faraday Rotation in an Insulator

17 Inhomogeneous Materials 17.1 17.2 17.3 17.4

The Effective Medium Response of a Single Grain Effective Medium Theories Other Approaches

Appendix A Appendix B Appendix C Appendix D Appendix E Appendix F Appendix G References Index

Notes about Units Maxwell’s Equations in SI Partial Derivatives and Vector Operators Acting on Plane Waves The Wave Equation Reﬂection and Transmission at Oblique Incidence A Field Guide to Optical “Constants” Software

276 276 276 279 282 285 288 295 297 300 303 304 304 309 315 324 325 333 335 336 337 344 347 350 352 353 354 365 372 373 397

Preface

This book is a discussion of optical effects in solids, addressing the physics of many types of solids (metals, superconductors, semiconductors, insulators, and others) and their response to electromagnetic radiation. I try to make a connection between what an experimenter can measure or extract from measurements (reﬂectance, transmittance, optical conductivity, and dielectric function) and the microscopic physics of the solid. Methods of analyzing experimental data are addressed: the optics of thin ﬁlms and the Kramers–Kronig relations. I begin with introducing the dielectric function into Maxwell’s macroscopic equations and ﬁnding their plane-wave solution. Then I discuss (ﬁrst classically and then using basic quantum mechanics) the dielectric function of various materials. Other topics include interacting electrons, the anomalous skin effect, anisotropy, magneto-optics, and inhomogeneous materials. I’ve attempted to write as a relatively complete coverage of the subject, starting with Maxwell’s equations for the electromagnetism and with the Schr¨odinger equation and Newton’s laws for the solid-state physics. The level of the presentation is aimed at the ﬁrst- or second-year experimental graduate student. The electromagnetism assumed is undergraduate (Grifﬁths or Marion); the level of quantum mechanics is about the same (Grifﬁths or Peebles). Finally, it is helpful to have gone through solid-state physics (Kittel or Burns). When I was a postdoc, the book by Frederick Wooten, Optical Properties of Solids (1972), appeared in the University Bookstore. I bought a copy and went through it during the next few weeks. It was just what I needed to read at the time: It was clear, it covered topics of interest to me, and it was at a level I could follow. I refer to it still and recommend it to others; I have also used it several times as a text in a course on optical properties for ﬁrst-year graduate students in physics, materials science, electrical engineering, and chemistry. Unfortunately, the book is long out of print. I’ve attempted to write at the same level as Wooten and cover many of the topics of his book. (The exception is photoemission, which is a huge subject of its own by now.) I have included a number of things that Wooten did not address, such as phonons, superconductivity, anisotropy, magneto-optics, and inhomogeneous materials. This book started life as the 2013 lecture notes for a graduate class in the optical properties of solids. This class has been offered to University of Florida graduate students at two- to six-year intervals over more than 25 years. That these started as lectures may be responsible for a certain informality in presentation. I’ve written in the ﬁrst person, trying to avoid the royal or inclusive “we” that in much exposition attempts to co-opt the reader or the listener. I think that whenever a person hears “and now we see” or “ in the future xi

xii

Preface

we must,” a quite proper response is “What do you mean by we Kemo Sabe.” First person avoids this response. I have also tried to avoid second-person instructions: “If you look at the ﬁgure, you can see . . . ” Well, a person looking at the ﬁgure may see what I want her or him to see, but may not. If not, it is my fault for not designing the right ﬁgure, not explaining it correctly, or not providing adequate background. In any event, it is better if I say what I see when I look at the ﬁgure and not presume more. All solids may be divided into three classes based on conductivity: metals, semiconductors, and insulators. I use silver, silicon, and sodium chloride as examples of these classes. These materials are useful to persons other than solid-state physicists. The cover of the book shows one example. It shows the bowl of a toddy ladle made in England around 1760. Set into the bowl of the ladle is a silver sixpence that was minted in 1758. The coin was designed during the reign of George II by John Sigismund Tanner, Chief Engraver of the Royal Mint. The sixpence coin was called a “tanner” by the British right up until decimalization. (Six pennies may not seem a lot but the hourly wage at the time was 2–8 pence.) I’ve had discussion with many persons over many years about the subject of optical effects in solids. I am grateful for all these discussions. A number of these discussions had direct inﬂuence on what I wrote here. For such discussions I thank Larry Carr, Jim Garland, Alan Heeger, Claus Jacobsen, Kati Kamar´as, Ricardo Lobo, Frank Marsiglio, Dmitri Maslov, Jan Musfeldt, Michael Rice, Danilo Romero, Al Sievers, David Stroud, Lila Tache, Tom Timusk, Axel Zibold, the students who took PHY7097 and made comments and found typos, and the editors at Cambridge University Press for patience and accommodation.

1

Introduction

The way in which light interacts with material objects is determined by the optical properties of the materials. Why might you want to think about these optical properties? There are at least two reasons. First, you can make use of known optical materials to design and build devices to manipulate light: mirrors, lenses, ﬁlters, polarizers, and a host of other gadgets. Second, you can measure the optical properties of some new material and obtain a wealth of information about the low energy excitations that govern the material’s physics. Figure 1.1 is a chart that identiﬁes some of these excitations and indicates the part of the spectrum where they might be expected to appear. In common parlance, “optical” can be a synonym of “visual,” and hence related to human eyesight. This interpretation would restrict discussion to the visible part of the electromagnetic spectrum, light with wavelengths of 390–780 nm, indicated by the little rainbow in Fig. 1.1. (I will need to introduce the variety of measures used for the wavelength or the frequency or the photon energy of electromagnetic waves. Four are shown in Fig. 1.1: λ in μm, f in THz, E in meV, and another frequency unit, wavenumbers or cm−1 . The latter may be unfamiliar to persons who have not worked in the ﬁeld of optical effects in solids; it is the inverse of the wavelength in cm. The visible spectrum spans 385–770 THz, 1.59–3.18 eV, and 12,800–25,600 cm−1 . Units used in papers about the optical properties of solids are discussed in Appendix A.) Of course I will not in this book make the interpretation that optical means visible; instead, materials properties will be considered over a wide range of frequencies or wavelengths.∗ Plausible ranges are discussed toward the end of this chapter. Even if you were constrained to the use of your own eyes, you would see that solids have a wide range of optical properties. Silver is a lustrous metal used for centuries in coins and ﬁne tableware, with a high reﬂectance over the whole visible range. Silicon is a crystalline semiconductor and the foundation of modern electronics. With its surface oxide freshly etched off, silicon is also rather reﬂective, although not as good a mirror as silver.† Salt (sodium chloride) is a transparent ionic insulator, is necessary for life, and makes up about 3.5% (by weight) of seawater. A crystal of salt is transparent over the entire visible spectrum; because the refractive index is about 1.5, the reﬂectance is everywhere about 4%. If you had ultraviolet eyes, you would see these materials differently. Silver would be a poor reﬂector, with at most 20% reﬂectance and trailing off to zero at the shortest wavelengths. In contrast, the reﬂectance of silicon would be better than in the visible, ∗ I like the notion of “DC to daylight,” used widely in the amateur radio community and also as the name of a

symposium honoring Professor A.J. Sievers, at Cornell University, June 14, 2003.

† Silver reﬂects about 98% of red light and about 80% of violet light; silicon reﬂects about 33% of red and 50%

of violet.

1

2

Introduction

Fig. 1.1

Chart showing optical processes in solids, with an indication of the wavelengths or frequencies where these processes typically may be studied. The uppermost scale shows the vacuum wavelength in μm, 10−6 m. Frequencies (or energies) are given on three scales. Top to bottom they are: THz, 1012 cycles/s; photon energies, meV; and wavenumbers, ν˜ (in cm−1 ), defined by ν˜ = 1/λ with λ the wavelength measured in cm. reaching up to 75%. Sodium chloride would be opaque over much of the spectrum, with a reﬂectance a bit higher than in the visible. Those with infrared eyes would also see things differently from visible or UV-sensitive individuals. Silver would have a reﬂectance above 99%. Silicon would appear opaque at the shortest infrared wavelengths but would then become transparent, so that you could see through even meter-thick crystals.∗ Sodium chloride remains transparent over much of the infrared, but an opaque and highly reﬂecting “reststrahlen” (German for residual ray) region occurs at long wavelengths. In the reststrahlen band, NaCl has a reﬂectivity not much below that of a metal. If you put on your solid-state-physics hat, you can understand the optical properties of these materials, at least qualitatively. Silver is a nearly free-electron metal, with one electron per atom in the metallic Fermi surface. These mobile electrons give the high electrical conductivity; they form a plasma that makes silver opaque and highly reﬂective ∗ Here ultra-high-purity is assumed. Moreover, in the middle infrared region there is a band caused by lattice

vibrational effects – multiphonons in this case – where silicon is opaque unless rather thin.

3

Introduction below the plasma frequency.∗ Silicon is a semiconductor with a gap between the ﬁlled valence band and the empty conduction band. Photons with energies below the gap can propagate without loss in silicon. Photons with energies above the gap are absorbed, generating electron–hole pairs. This absorption renders silicon opaque and, as mentioned, increases the reﬂectance. Sodium chloride is an insulating crystal, with a band gap in the ultraviolet. Similar to silicon, photons with energy larger than the gap are absorbed. Sodium chloride has two atoms per unit cell; these occur as ions, Na+ and Cl− ; an electric ﬁeld displaces these ions, producing induced dipoles in the solid. With a two-atom basis, the lattice vibrations have an optical branch, and the reststrahlen band is a result of the light exciting this optical branch. Now let me return to the question of the range of wavelengths (or the range of light frequencies or of photon energies) over which I can discuss the optical properties of solids. The electromagnetic spectrum extends over a huge range; a representative cartoon illustrating the “electromagnetic spectrum” is shown in Fig. 1.2. This chart shows wavelengths from km to pm along with corresponding frequencies and photon energies. So the question is: What part of this spectrum might be used to study the optics of solids? To start, I’ll want to use continuum electrodynamics, so the short wavelength limit is set by a requirement that the wavelength be larger than the spacing between atoms. When the wavelength is less than the interatomic distances, diffraction effects dominate. X-ray diffraction is essential for determining crystal structure but beyond my scope. At somewhat longer wavelengths, continuum electrodynamics is ﬁne, but the materials properties are essentially a superposition of atomic transitions. Solid-state effects contribute of course but minimally for wavelengths shorter than something on the order of 50 nm.† As wavelengths get longer and longer, there is of course no problem with continuum electrodynamics. However, practically speaking, the physics that govern the electromagnetic response at dc and audio frequencies is the same as the physics at ultra-high radio frequencies and even microwaves. So the lowest frequencies that I will consider are around a few GHz. There is a second reason for setting a long-wavelength limit. One GHz (4 μeV photon energy) corresponds to 30 cm wavelength, and this large scale raises an experimental issue: to shine light on a solid, one sends a beam that one would like to consider to be composed of plane electromagnetic waves. Cartoons of typical experimental setups are shown in Fig. 1.3. The left panel shows a reﬂectance (R) experiment and the right a transmittance (T ) experiment. Light comes from a source (of known properties) that can emit a range of wavelengths, encounters the sample, and goes to a detector where it is converted to ∗ The connection between high absorption, high conductivity, and high reﬂectance is not intuitive. For the

moment, I’ll just assert that all three go together. So at wavelengths where a material is opaque, it also has increased reﬂectance. The more intense is the absorption, the higher the conductivity and also the higher the reﬂectance. A hand-waving argument says that high conductivity means large currents in response to applied electric ﬁelds; the power loss or absorption goes as j · E = σ E 2 . See Section 4.5 for further discussion. † Using λf = c, ν˜ = 1/λ, and E = hf with λ the wavelength, f the frequency in Hz, ν˜ the frequency in cm−1 , or wavenumber, E the photon energy, c the speed of light, and h Planck’s constant, 50 nm corresponds to a frequency of 6 PHz (petaHertz), a wavenumber of 200,000 cm−1 , and photon energies of 25 eV.

4

Introduction

Fig. 1.2

The electromagnetic spectrum over a broad range of wavelengths. Things of various sizes are placed where their dimension equals the wavelength. Spectral ranges are identified and example sources are shown. (“IR”is short for infrared.)

Fig. 1.3

Cartoon of an experiment where one measures reflectance (left) or transmittance (right). an electrical signal, is ampliﬁed, and recorded, yielding a spectrum of R or T vs. the wavelength or the frequency. These ideas are only a good approximation to experiment when the wavelength is small compared to the size of the sample or of the experimental apparatus. When this condition is no longer the case, diffraction effects (by the sample not by the atomic lattice) as well as waveguide effects in the surrounding apparatus become important.∗ ∗ One may of course measure materials properties all the way to zero frequency (inﬁnite wavelength) by

electrical means: apply contacts and measure resistance, capacitance, etc. I will discuss the connection of optical measurements to dc electrical properties a number of times.

5

Introduction

It makes little sense to be very precise in specifying the wavelength or frequency limits over which optical concepts are important for the physics of solids. So I’ll say that I will consider the wavelength range to be several cm to several tens of nm, the frequency range to be a few GHz to a few PHz, and the photon energy range to be tens of μeV to tens of eV. This range covers the bands labeled microwaves, far infrared, midinfrared, near infrared, visible, and ultraviolet in Fig. 1.2. There is a factor of a million between one end and the other; that should be enough for everybody.∗ In the following chapters, I’ll remind you a little bit about electromagnetism, including Maxwell’s equations and their plane-wave solutions. I’ll then restrict myself for some time to local, nonmagnetic, isotropic, homogeneous, and linear solids.† The motivations for these restrictions are that the materials should be local, so that the current at point r is a function only of the ﬁelds at r; nonmagnetic, because most solids are nonmagnetic and because even magnetic materials only show themselves to be magnetic at rather low frequencies; isotropic, so that the properties do not depend on the direction or polarization of the light; homogeneous, so that the response functions do not depend on spatial position; and linear, so that I may make a Fourier decomposition of the ﬁelds and treat each component independently. With these approximations, I’ll introduce the idea of a complex dielectric function, discuss classical theories of free carrier response in metals, interband absorption in semiconductors and insulators, and lattice vibrations (phonons). Next, I will show data from the literature to illustrate some of the concepts of these theories. I return to electromagnetism to calculate the reﬂection and transmission by a thin ﬁlm or slab as a way to link experimental measurements to the optical properties of the material making up the ﬁlm. The next step is to introduce simple quantum mechanics, leading to a discussion of free-electron metals, followed by a presentation of the quantum-mechanical perturbation-theory of optical absorption, culminating in an important sum rule for the conductivity. The sum rule result motivates an interlude about causality where I obtain the Kramers–Kronig relations between the absorptive and dispersive parts of the response function, discuss the analysis of reﬂectivity by Kramers–Kronig methods, and derive other sum rules. My focus shifts back to materials, with a simple treatment of the optics of superconductivity, a distinctly quantum-mechanical phenomenon. Next comes the band structure of simple solids and the interband absorption edge in semiconductors, followed by materials with strong correlations and interactions. After this, it will be time to relax the initial conditions and discuss (one at a time!) nonlocal properties, mostly the anomalous skin effect in a pure metal, wave propagation in anisotropic materials, magneto-optics, and randomly inhomogeneous materials.‡ Several appendices discuss units, some mathematics, and other things “optical.”

∗ In fact there are few materials that have been studied over the entire range. A much more typical range is in wavelength from, say, 0.3 mm to 300 nm, far infrared to ultraviolet, a range of 103 . † Much of this discussion can apply to liquids as well, and even to a dilute gas, but the physics discussion will

rely on solid-state physics ideas: Fermi surfaces, band structure, etc.

‡ I’ll leave the huge subjects of quantum optics and nonlinear optics to others; I think it is better to say nothing

than to make short and probably superﬁcial treatments.

2

Maxwell’s Equations and Plane Waves in Matter

2.1 Optical Constants The response of materials to light is described by a number of quantities, often called “optical constants.” Among these are: • • • • • • •

, the dielectric constant. σ , the electrical conductivity. χ , the susceptibility.∗ n, the refractive index. κ, the extinction coefﬁcient. δ, the electromagnetic skin depth. Z, the surface impedance.

and many others. See Appendix F for a longer but still incomplete list. These quantities are neither constant nor independent. They are functions of the frequency, temperature, pressure, external magnetic ﬁeld, and many other things. By knowing two of these, one that describes the absorption in the solid (such as the electrical conductivity or the extinction coefﬁcient) and one that describes dispersion (such as the dielectric constant or the refractive index), all of the others can be calculated.

2.2 Maxwell’s Equations In my initial Electricity and Magnetism course, the professor said that the subject is governed by equations written in the nineteenth century by Maxwell [1] and that some day a teacher would come in, write these equations on the blackboard on the ﬁrst day of the class and then proceed to develop a theory based on these equations. Of course in a junior-level class, he did not do this, but I can do it here. There are two versions: Maxwell’s microscopic equations and Maxwell’s macroscopic equations. The ﬁrst are more fundamental, because they describe the microscopic ﬁelds arising from every charge in the Universe and from the motion of these charges as well.

∗ Electric and magnetic.

6

7

2.2 Maxwell’s Equations The second are more fun, because they average over the charges in macroscopic media∗ and allow great simpliﬁcation of the subject. After restricting myself to macroscopic charges and currents, I have ρext , the external charge density, and j free , the free current density as sources in Maxwell’s equations. The external charge density is essentially the charge imbalance in the medium; it is zero for electrically neutral objects.† The free current density is the result of the motion of free charges in the metal. The standard example of these mobile charges is the free electrons in a metal, but could also be doped or thermally excited free carriers in a semiconductor or the diffusion of ions in an electrolyte. Note that the free carriers are compensated by bound ions in the electrically neutral material so these charges do not generate any external charge density. So let me begin by writing Maxwell’s equations for macroscopic media [2–8]. I’ll use cgs-Gaussian units; the translation to SI units appears in Appendix B. ∇ · D = 4πρext

(2.1a)

∇ ·B=0

(2.1b)

1 ∂B (2.1c) c ∂t 1 ∂D 4π ∇ ×H= j free + , (2.1d) c c ∂t I must add a connection to classical mechanics to these equations. The force F on a particle with electric charge q satisﬁes the Lorentz force law, v (2.2) F=q E+ ×B , c where v is the particle’s velocity vector. The deﬁnitions of the auxiliary ﬁelds are ∇ ×E=−

D = E + 4π P H = B − 4π M.

(2.3)

The quantities in Eqs. 2.1, 2.2, and 2.3 are all functions of space and time. The vector E is called the “electric ﬁeld” and the vector D is called the “electric displacement ﬁeld.” In vacuum, D and E are proportional to each other, with the multiplicative constant 0 depending on the physical units.‡ Inside a material they are different on account of the polarization of the material. The vector P is the “polarization ﬁeld,” also known as the “electric polarization,” “electric polarization density,” or “electric dipole moment/unit volume.” The vector B is called the “magnetic ﬁeld,” and it and E are deﬁned as the vector ∗ In the absence of external ﬁelds, the positive charges (the nuclei) in a uniform medium are perfectly screened

by the negative charges (the electrons) so that both may be omitted completely from the charges and currents in Maxwell’s equations. External ﬁelds may polarize these charges (pushing + in one direction and − in the opposite direction); the effects of such currents and dipole moments are the subject of our optical properties studies. † And it does not include any charge imbalance caused by external ﬁelds. This polarization gets included in the dipole moment/unit volume P. ‡ Unity in cgs-Gaussian units.

8

Maxwell’s Equations and Plane Waves in Matter

ﬁelds necessary to make the Lorentz law correctly describe the forces on a moving charged particle. B is also called the “magnetic ﬂux density,” or the “magnetic induction.” The vector H is also sometimes called the “magnetic ﬁeld.” Other names include the “magnetic ﬁeld intensity,” the “magnetic ﬁeld strength,” and the “magnetizing ﬁeld.” In vacuum, B and H are proportional to each other, with the multiplicative constant μ0 depending on the physical units.∗ Inside a material they are different on account of the magnetization of the material. The scalar ρext is the “free volume charge density” and the vector j free is the “free electric current density.” The vector M is the “magnetization ﬁeld” or the “magnetic dipole moment/unit volume.” Three of the four Maxwell equations have names: Equation 2.1a is Gauss’ Law; Eq. 2.1c is Faraday’s law of induction; and Eq. 2.1d is Amp`ere’s law with Maxwell’s correction. I’ll just call it Amp`ere’s law. Eq. 2.1b is sometimes called Gauss’ law for magnetism but is sometimes called the no-magnetic-monopole law. Others say that it has no name. I like “the no-monopole law.”

2.3 Total, Free, and Bound Charges and Currents If I view charges as being small point-like particles moving here and there in space, then a classical-physics-style deﬁnition of the microscopic charge density in a solid might be qi δ(r − ri (t)), ρmicro (r,t) = i

whereas the current would be written j micro (r,t) =

qi vi (t)δ(r − ri (t)).

i

Here, the sum i runs over all charged particles, qi is the charge of the ith particle, located at (time-dependent) coordinate ri and moving with (time-dependent) velocity vi . There are quantum mechanical versions of the charge density and current density also. To use them requires a solution of Schr¨odinger’s equation in the solid. With the solution in hand, I could then ﬁnd the contribution of the electrons† (with charge −e) to the total charge density to be ρe = −e e∗ e where e is some total wave function of the electrons, [ e∗ ∇ e − (∇ e∗ ) e ]. and, similarly je = −(he/2mi) ¯ Accounting for all the particles in a material with 1022 particles per cubic centimeter is of course too hard, so I’ll average over some volume V . The scale of V is taken to be large with respect to the interatomic spacing a and small with respect to the electromagnetic wavelength λ, or a 3 V λ3 . ∗ Unity in cgs-Gaussian units. † Because of a choice made by Franklin, the electron is negative. I’ll take e to be a positive number and put the

sign in explicitly as needed.

9

2.4 Maxwell’s Equations for Solids The inequalities are easy to satisfy because a ∼ 0.1 nm and, according to the discussion in Chapter 1, λ is bigger than 10 nm, so there is a factor of 106 between their cubes. The charge and current then are written as averaged quantities, ρ(r,t) = qn(r,t) and j(r,t) = ρ(r,t)vd (r,t), where q is the average charge of the particles, n is their number density, and vd the average velocity in the volume V , known as the “drift velocity.” The electrons and nuclei do not know that I would like to average them out, so they still respond to applied ﬁelds, producing dipole moments in the material, P and M. These bound or polarization charges, electric polarization currents, and magnetization currents are determined by the physics of the solid. Then, the macroscopic polarization charge density ρpol , the polarization current density j pol , and the magnetization current density j mag are deﬁned in terms of polarization P and magnetization M as ρpol = −∇ · P, j pol = ∂P/∂t, and j mag = c∇ × M. Maxwell’s macroscopic equations reduce to the microscopic equations if one recognizes that the microscopic, free, and bound charge and current density are related by ρmicro = ρext + ρpol, and j micro = j free + j pol + j mag, and then uses Eq. 2.3 to eliminate D and H.

2.4 Maxwell’s Equations for Solids I am almost to a point where I can begin to address optical effects in solids. But there are two things still to do. First, the world is in general electrically neutral,∗ so I will take ρext = 0. For notational convenience, I will drop the “free” subscript on the current, with the understanding that it is the free current that is meant.† Thus, j free → j. Henceforth, I’ll use the form of Maxwell’s macroscopic equations written just below. I’ll claim that these cover the most general cases that occur in the studies of optical effects in solids. I’ll make further simpliﬁcations in the next several pages, but can always return to these as a starting point. ∇ ·D=0

(2.4a)

∇ ·B=0

(2.4b) 1 ∂B (2.4c) ∇ ×E=− c ∂t 4π 1 ∂D ∇ ×H= j+ (2.4d) c c ∂t The four parts of Eq. 2.4 have a certain pleasing symmetry. After I’ve deﬁned and used the complex dielectric function, this symmetry will become more perfect.

∗ Anyone who has been shocked by a static discharge after crossing a rug on a dry day or who has seen a lightning

strike from a thunderstorm knows (1) that this statement is not always true but (2) that the charge imbalance does not last. † And see the discussion in Section 3.1 where the distinction between free and bound currents will be blurred as well.

10

Maxwell’s Equations and Plane Waves in Matter

2.5 Plane-Wave Solutions I write the electric ﬁeld as a complex exponential E(r,t) = E0 ei (q·r−ωt )

(2.5)

H(r,t) = H0 ei (q·r−ωt ),

(2.6)

and also the magnetic ﬁeld

where E0 and H0 are constant vectors giving the amplitudes of the ﬁelds (complex quantities in the most general case) and their directions,∗ q is the wave vector of the ﬁeld (measured in cm−1 in cgs), and ω is the angular frequency (in radians/s or s−1 ). I choose to use H rather than B, as does Jackson [2]. √ The quantity i = −1 does not appear in Eqs. 2.1–2.4. Hence the only mechanism to have equations that contain real and imaginary quantities is through writing the ﬁelds as complex quantities, as in Eqs. 2.5 and 2.6. It would be perfectly valid to write E = E0 cos(q · r − ωt + φe ) and H = H0 cos(q · r − ωt + φm ), where the phases φe and φm allow for differing phases in electric and magnetic ﬁelds.† In this case, all quantities in electromagnetism would be purely real quantities. I could do this; at a minimum it would give ﬁne training in the use of trigonometric identities, because as soon as I take a derivative, there will be both sines and cosines in the math. It is conventional to say that one writes the ﬁelds as complex quantities but when one wants to evaluate the observable ﬁelds, the real part should be taken. This statement is basically true, though one has to be careful in cases where two complex ﬁelds are multiplied together. I know from freshman physics that the crests and valleys of the wave repeat in space (at ﬁxed time) by a translation of the wavelength λ. From this assertion I get |q|λ = 2π or |q| = 2π/λ. At a point in space, the wave repeats every time the time advances by the period T ; hence ω = 2π/T = 2πf with f the frequency. Moreover, λf = v and ω = qv with v the wave speed (= c in vacuum). See Appendix A for a discussion of units used for length, time, frequency, energy, ﬁelds, and many other quantities used in optical studies. The use of plane-wave ﬁelds may seem arbitrary or restrictive, but Fourier tells us that 3 E(r,t) = d q dω E0 (q,ω)ei (q·r−ωt ), with

E0 (q,ω) =

3

d r

dt E(r,t)e−i (q·r−ωt ) .

I can write an arbitrary ﬁeld in terms of the Fourier integral, do the usual trick of exchanging order of integration and differentiation, and ﬁnd (for linear, local materials) that Maxwell’s equations apply to each Fourier component. ∗ Hence, to be explicit I could write E = eˆ E eiφ0 , where eˆ is a unit vector pointing in the ﬁeld direction, E is 0 0 0

the ﬁeld magnitude, and φ0 is a constant phase which, when combined with (q · r − ωt), speciﬁes where the zeros, crests, and valleys of the wave occur. † Alternatively, write E = E cos(q · r − ωt) + E sin(q · r − ωt) and a similar equation for H. c s

11

2.8 Electromagnetic Waves in Vacuum

2.6 Converting Differential Equations to Algebraic Ones Now, I insert plane-wave ﬁelds into Eq. 2.4. See Appendix C for the rules of how vector and partial differential operators act on plane wave functions. For example, Eq. 2.4a becomes ∇ · D = iq · D = 0 After doing this type of thing for all four of Maxwell’s equations, cleaning up the signs, and canceling as many of the appearances of i as I can, I get q·D=0

(2.7a)

q·B=0 ω q×E= B c ω 4π i q×H=− D− j c c

(2.7b) (2.7c) (2.7d)

with D = E + 4π P

H = B − 4π M

(2.8)

(I exchanged the order on the right-hand side of Eq. 2.7d for convenience in the steps coming up.)

2.7 Vector Directions Vectors whose inner product is zero are orthogonal. Hence, q is perpendicular to both D and B. The cross product produces a vector normal to the plane containing the other two vectors. Hence, Eq. 2.7c tells me that B is perpendicular to E (and to q, which I already knew). Equation 2.7d says that H is perpendicular to a particular linear combination of D and j and, moreover, that j is perpendicular to q because D is.

2.8 Electromagnetic Waves in Vacuum If there is no medium, there are neither electric nor magnetic dipoles nor free currents. Hence Eq. 2.8 gives D = E and H = B and Eq. 2.7 becomes q·E=0 q·H=0 ω q×E= H c ω q × H = − E. c

(2.9a) (2.9b) (2.9c) (2.9d)

12

Fig. 2.1

Maxwell’s Equations and Plane Waves in Matter

Electromagnetic wave in vacuum. Here, q, E, and H form a right handed orthogonal set, which I may orient respectively along the x, y, and z Cartesian axes. Then∗ qˆ × eˆ = hˆ and qˆ × hˆ = −ˆe, making the magnitudes of Eqs. 2.9c and 2.9d be qE = ωH /c and qH = ωE/c. Solving the second of these for H and substituting in the ﬁrst, I ﬁnd q = ω/c; either of these then give H = E. So in vacuum, electromagnetic waves travel at the speed of light and have equal (cgsGaussian) amplitudes for the electric and magnetic components. The energy density [2] u = (E · D + B · H)/8π becomes in vacuum uvac = (E 2 + H 2 )/8π . Half the energy is carried by the electric component and half by the magnetic component. Figure 2.1 shows a cartoon of the wave in vacuum.† The wave is traveling to the right, with the E ﬁeld (red) in the vertical plane and the H ﬁeld (blue) in the horizontal plane. These waves are plane waves, so the ﬁelds have spatial variation in the propagation direction while being constant in amplitude for perpendicular directions. Figure 2.2 is an attempt to illustrate this condition. It shows the E ﬁeld at its crests (red arrow and red plane) and troughs (blue arrow and blue plane). The propagation vector (black) is normal to the planes of constant phase.

2.9 Five Easy Simplifications Now, I return to Eqs. 2.7 and 2.8 and discuss how they change as simplifying assumptions about the material’s properties are made.

2.9.1 Local Response If I write Ohm’s law as j = σ E, I am making an assumption that the response is local, that the current j at point r depends only on the electric ﬁeld E at that point and the ∗ I’ll deﬁne unit vectors parallel to any vector A as aˆ and the magnitude (length) of the vector as A. † If you look on the web for such cartoons you may note that about half of them show the ﬁelds incorrectly,

ˆ failing to satisfy qˆ × eˆ = h.

13

Fig. 2.2

2.9 Five Easy Simplifications

Plane waves. conductivity σ . This statement is never completely true; the current possesses a certain momentum and, once set in motion, takes a certain time (e.g., the relaxation time τ ) or distance (e.g., the mean free path ) to relax back to zero.∗ Even so, local electrodynamics is the usual case, because the mean free path is typically short compared to the lengths over which the ﬁeld itself varies and so the current is indeed related to the ﬁeld by a local relation. However, in pure metals at low temperatures, the mean free path can become longer than the electromagnetic penetration depth (i.e., the skin depth). In that case, currents generated within the skin depth can travel deep into the metal, where the electric ﬁeld is essentially zero. Nonlocal effects appear also in superconductors. I’ll discuss nonlocal electrodynamics in Chapter 14. Meantime, local behavior will be assumed.

2.9.2 Nonmagnetic Materials If the material is nonmagnetic, M = 0 everywhere and B = H. Then Eq. 2.7 shows that q, D, and H (which is parallel to B) form a right-handed set. E is perpendicular to H, lying in the plane containing D and q. E need not be perpendicular to q, although it cannot be ˆ z. exactly parallel to it either. Analogous to the vacuum case, I’ll set qˆ ˆx, ˆjˆy, and hˆ

2.9.3 Linear Materials For many materials, the electric dipole moment/unit volume obeys ↔

P = χe · E

(2.10)

↔

where χ e is a 3 × 3 tensor, the electric susceptibility. Then ↔

↔

↔

D = E + 4π χ e · E = (1 + 4π χ e ) · E ≡ · E ↔

(2.11)

↔

where = 1 + 4π χ e is the dielectric tensor. ∗ Actually, in time τ it relaxes back to 1/e of what it was at t = 0 and it requires a number of relaxation times to

become unnoticeable.

14

Maxwell’s Equations and Plane Waves in Matter

Similarly ↔

j = σ · E.

(2.12)

↔

with σ the conductivity tensor. And (if the material becomes magnetic again) ↔

M = χm · H

(2.13)

↔

where χ m is a 3×3 tensor, the magnetic susceptibility. Then ↔

H = B − 4π χ m · H and (after a bit of algebra) ↔

B= μ·H ↔

(2.14)

↔

where μ = 1 + 4π χ m is the permeability tensor. Equations 2.10–2.14 indicate linear relations between applied ﬁelds and materials response. The relation is linear because if the E ﬁeld is doubled, the polarization P and current j are doubled. Linearity is not a big restriction. Everything is linear if the ﬁelds are small enough. Everything is nonlinear if the ﬁelds are big enough. Most optical ﬁelds are actually rather weak; the exception being high power and short pulsed lasers. Substituting Eqs. 2.11 and 2.12 into Eq. 2.7d, I get 4π i ↔ ω↔ ·E− σ ·E c c ω ↔ 4π i ↔ + σ ·E =− c ω

q×H=−

(2.15)

I will spend quite a bit of time on the consequences of this equation in Chapter 15, which is about anisotropic media (crystals). For now let me just note that q × H produces a vector that is perpendicular to q and H but that E is not parallel to that vector, because the multiplication of a tensor with a vector produces a new vector that is in general oriented different from the initial vector.∗

2.9.4 Isotropic Materials Amorphous solids, polycrystalline solids, and liquids are isotropic: their properties are uniform for all directions of ﬁelds and propagation. In the case of crystals, there is no requirement for isotropy. Indeed, the optical properties must reﬂect the symmetry of the underlying crystal structure. On the one hand, the majority of all possible crystals are anisotropic; of the seven crystal families only the cubic is by symmetry required to have isotropic optical properties. On the other hand, a large fraction of commonly encountered materials (silver, silicon, and sodium chloride, for example) are cubic and isotropic. On ∗ Only if the tensor is in diagonal form and the ﬁeld is oriented along one of the principal axes of the tensor is the

result of the multiplication not rotated.

15

2.10 Maxwell’s Equations for These Easy Cases

the remaining hand, many of the most interesting solid state systems, such as the hightemperature superconductors, graphene, organic solids, etc., are highly anisotropic. Many persons think their remarkable properties are a consequence of this anisotropy. The optics of anisotropic crystals are worked out in Chapter 15. For the time being, I will assume isotropy. In this case, the tensors of Eqs. 2.10–2.13 become scalars. Formally, one writes ↔

↔

σ =σ1 ↔

with 1 the identity tensor (diagonal, with all diagonal elements equal to 1). In isotropic media, D, E, and P are parallel, as are H, B, and M.

2.9.5 Homogeneous Media There are many materials whose properties vary with position. One class of such materials is exempliﬁed by paint or ink, a collection of particles, small with respect to the wavelength, suspended in a host material. The optical properties of each type of grain and of the host are different but, because of the small grain size, the material has an apparent (or effective) uniform response. I’ll go over some aspects of inhomogeneous materials in Chapter 17. A second class consists of a plane surface where the optical properties change from, say that of a metal to vacuum or a thin ﬁlm of one or more layers. Simple layered materials are covered in Chapter 7. At present, I will consider the material to be spatially homogeneous, so that the response functions, such as the dielectric function, satisfy = (r), so that ∇ · (E) = ∇ · E.

2.10 Maxwell’s Equations for These Easy Cases With the assumptions of the previous section, I can write for local, nonmagnetic, linear, isotropic, and homogeneous materials: j = σ1 E

(2.16)

D = 1 E.

(2.17)

and

The meaning of the subscripts will become clear in a moment.

16

Maxwell’s Equations and Plane Waves in Matter Equation 2.17 replaces D = E + 4π P, Eq. 2.3. With it and Eq. 2.16, I can rewrite Eq. 2.7: q·E=0 q·H=0 ω q×E= H c 4π i ω q×H=− 1 + σ1 E c ω

(2.18a) (2.18b) (2.18c) (2.18d)

Only the fourth one has changed. I am almost to the starting point where I can discuss the optical properties of simple∗ materials. But ﬁrst I have to say what the subscripts on 1 and σ 1 mean, given that I am using electric ﬁelds like E = E0 ei (q·r−ωt ) so that the ﬁeld amplitudes – and the materials related coefﬁcient 1 + 4π iσ1 /ω – contain real and imaginary parts. I will use the ﬁrst part of the next chapter to explain these subscripts.

∗ Simple = local, nonmagnetic, linear, isotropic, and homogeneous solids.

3

The Complex Dielectric Function and Refractive Index 3.1 Conductivity and Dielectric Constant In this this chapter, I’ll deﬁne the complex dielectric function as I’ll use it for the remainder of the book. The ﬁrst topic is the relation between conductivity (σ ) and dielectric function (). For a moment, let me return to Eq. 2.4d, substituting into it Eqs. 2.16 and 2.17: ∇ ×H=

1 ∂E 4π σ1 E + . c c ∂t

(3.1)

As discussed in Section 2.5, the Maxwell equations are only complex if complex ﬁelds are used with them. But how am I to think about σ 1 and 1 ? Are they real numbers or complex numbers? Well, if I use sines and cosines for the ﬁelds, both must be real numbers. If I use complex ﬁelds (as I plan to do), I can take one of two philosophical positions. The ﬁrst position omits the subscripts and identiﬁes σ E as the free current density. Similarly ∂E/∂t contains the bound current density and Maxwell’s displacement current. One can defend this distinction. For example, the conduction electrons in a metal are free carriers and their motion in response to an electric ﬁeld is the free current. Because the carriers have inertia, their response will lag the ﬁeld as frequency increases. This phase delay can be represented by having σ be complex, with the imaginary part being an inductive response that results from this inertia. Similarly, the remaining electrons in the solid are bound to their atoms, and their response is the polarization current. Inertial and dissipative effects will ensure that also is complex. I have four independent quantities (the real and the imaginary parts of these functions) but can identify them with the free and with the bound carriers. The second position asserts that the conductivity and dielectric function in Eq. 3.1 are both real quantities, just as they would be if real-valued ﬁelds were used. It goes on to note that the distinction between free carrier and bound carrier response is clear in the case of well understood and well characterized systems such as simple metals. However, for some new material, perhaps with no good theoretical understanding, it would not be possible to make such a clear distinction. It is better to reduce the number of materials “constants” to two. I’ll take the second position. There are two independent quantities, the real conductivity σ1 and the real dielectric function 1 . The ﬁrst leads to a current that is in phase with E (and hence is dissipative) and the second to a current that is 90◦ out of phase (and hence dispersive). I will combine them into a single complex dielectric function. 17

18

The Complex Dielectric Function and Refractive Index

3.2 The Complex Dielectric Function Using this approach, I can substitute our plane-wave ﬁelds into Eq. 3.1; indeed, I did that to derive Eq. 2.18d (the plane-wave-generated algebraic equation) which I copy here: 4π i ω 1 + q×H=− σ1 E. c ω and then I deﬁne a complex dielectric function as 4π i σ1 . (3.2) ω With this deﬁnition, I arrive at the form of Maxwell’s equations which is appropriate for local, nonmagnetic, linear, isotropic, and homogeneous media. I’ll put them in a box to make them stand out. ≡ 1 +

q·E=0 q·H=0 ω q×E= H c ω q × H = − E c

(3.3a) (3.3b) (3.3c) (3.3d)

These equations have a very agreeable symmetry. The materials properties enter only through the presence of the complex dielectric function in Eq. 3.3d. Equations 3.3a and 3.3b tell me that q is perpendicular to E and H, just as it was in vacuum. Equation 3.3c tells me that H is perpendicular to q and E; the three vectors form ˆ Then, with qˆ × eˆ = h, ˆ the vector part of a right-handed set, with unit vectors {ˆq, eˆ, h}. ˆ Eq. 3.3d gives qˆ × h = −ˆe as it should, telling nothing new about vector directions. I’ll generally write complex quantities in the form Z = Z1 + iZ2 , with Z1 the real part and Z2 the imaginary part.∗ The dielectric function is one such complex quantity, = 1 + i2 . From the deﬁnition, Eq. 3.2, I see that the imaginary part of the dielectric function is related to the real part of the conductivity, 2 =

4π σ1 . ω

(3.4)

3.3 The Optical Conductivity There are times when it is convenient to work with a complex conductivity σ = σ1 + iσ2 rather than a complex dielectric function. There is no difference in the physics when I use ∗ Some authors use primes instead, Z = Z + iZ

.

19

3.4 The Complex Refractive Index

σ rather that , just a change of perspective. When using the conductivity, I have to get the case where σ = 0 correct, keeping the vacuum displacement current of Eq. 2.9d. This I do by starting with Eq. 2.7d, writing D = E + 4π P, using j pol = ∂P/∂t = −iωP. Then, as before, I write Ohm’s law, j = σ1 E and then deﬁne j pol = σ2 E. With all this, I get 4π i ω 4π i ω 1+ q×H=− E− σE = − σ E, (3.5) c c c ω where σ ≡ σ1 + iσ2 is complex. Equation 3.5 preserves Maxwell’s displacement current in the vacuum.∗ By equating the right sides of Eqs. 3.3d and 3.5, I see that the relation between and σ is 4π i σ, (3.6) ≡1+ ω and then the complex conductivity is iω (1 − ). (3.7) 4π Finally, I put = 1 + i2 and σ = σ1 + iσ2 into Eqs. 3.6 and 3.7 and equate real and imaginary parts to obtain Eq. 3.4 and ω (3.8) σ2 = (1 − 1 ). 4π Note that σ2 is positive when 1 is negative, or at least less than than +1. I will show in Chapter 4 that metals and insulators both may have 1 negative over certain frequency ranges and positive over others. A negative 1 or σ2 should not worry you. Recall that the reactance of inductors (iωL, positive imaginary) and capacitors (1/ iωC, negative imaginary) have opposite signs, allowing resonant circuits to be constructed.† When considering a speciﬁc type of material (metal, insulator, ionic solid, superconductor) it is sometimes better to work out the conductivity and other times better to derive the dielectric function. Equations 3.6 and 3.7 allow one to translate back and forth between them. σ =

3.4 The Complex Refractive Index With the directions removed, Eqs. 3.3c and 3.3d become qE = ωc H and qH = ωc E with both E and H varying as ei (q·r−ωt ) . I’ll solve the ﬁrst for H and substitute into the second to ﬁnd ω√ q= , (3.9) c thus motivating the deﬁnition of the complex refractive index, √ N = n + iκ ≡ , (3.10) ∗ The vacuum has σ = 0! In fact, the vacuum has = 1 + i0 and σ = 0 + i0. † A negative σ should worry you. 1

20

The Complex Dielectric Function and Refractive Index so that q = N ω/c. The real part of N , n, is the refractive index and the imaginary part, κ, is the extinction coefﬁcient.∗ The electric ﬁeld for plane waves becomes ˆ ) . E = E0 ei (q·r−ωt ) = E0 ei (N c q·r−ωt ω

(3.11)

ˆ so qˆ · r = x, and For deﬁniteness, let qˆ = x, ω

ω

E = E0 ei (n c x−ωt ) e−κ c x .

(3.12)

Recall that in vacuum, q = ω/c, so the wave vector (wavelength) in the material is larger (smaller) by a factor n. The wave decays with a decay length δ = c/ωκ. (In terms of the vacuum† wavelength λ0 = 2π c/ω = c/f , the wavelength inside is λ = λ0 /n and the decay length is δ = λ0 /2π κ.) The wave crests move at c in vacuum and at v = c/n in the medium. Equation 3.12 can then be rewritten as x

x

E = E0 e2π i ( λ −f t ) e− δ .

(3.13)

Figure 3.1 the shows observable (real part) of the electric ﬁeld,‡ E = E0 cos[2π (x/λ − f t)]e−x/δ . Three cases are shown. The curve marked “strong absorber” has the inside wavelength (λ) and the damping length (δ) equal to each other and equal to about 90% of the vacuum wavelength. The amplitude dies away in about 5–7 vacuum wavelengths. The curve marked “weak absorber” has the inside wavelength (λ) also equal to about 90% of the vacuum wavelength while damping length (δ) is 10 times the vacuum wavelength. The amplitude decays slowly, requiring 140 vacuum wavelengths to be reduced to 1 ppm of the initial amplitude. The curve marked “metal” has a wavelength inside that is 100 times longer than the vacuum wavelength and a damping length around 10% of λ0 . The ﬁeld amplitude decays exponentially to zero with no oscillations at all.§ With directions removed, Eq. 3.3c is H = (cq/ω)E, and, then, with q = ωN/c, I get √ (3.14) H = N E = E. N and are both generally complex, so the phase of H is different from the phase of E. Squaring Eq. 3.10 gives N 2 = n2 − κ 2 + 2inκ = = 1 + i2 so that it is easy to see that 1 = n2 − κ 2

(3.15)

∗ The refractive index is a counterexample to the Z = Z + iZ convention. Note also that some (older) texts 1 2

write N = n(1 + iκ). Furthermore, it is more common to use k than κ as the symbol for the extinction coefﬁcient. I choose the latter because I want to use k as a wave vector. † The word “wavelength” sometimes means the vacuum wavelength, c/f , and sometimes means the wavelength inside the medium, c/nf . If not speciﬁed or obvious from context, take it to mean the vacuum wavelength. ‡ Here, I take E to be real. 0 § To get the long wavelength inside, I use n = 0.01. A refractive index less than unity may seem impossible, but I shall show in Chapter 4 that both free carriers and weakly damped bound carriers may have such values of refractive index. It happens when 1 < 0 and 2 1.

21

3.5 Energy Density, Poynting Vector, and Intensity

Strong absorber Weak absorber “Metal”

1

Amplitude

0.5

0 1

2

3

4

5

Distance (units of l0) –0.5

–1

Fig. 3.1

Three damped cosinusoidal waves. and 2 = 2nκ.

(3.16)

It takes a bit more labor to calculate things the other way, but after this labor I get || + 1 (3.17a) n= 2 || − 1 κ= (3.17b) 2 where || = 12 + 22 .

3.5 Energy Density, Poynting Vector, and Intensity Electromagnetic waves carry energy and can deposit that energy as heat in absorbing materials.∗ So here I will work out energy aspects of electromagnetic waves in local, linear, isotropic, and homogeneous materials. I’ll start with a quick derivation of Poynting’s theorem. I note that this theorem will be derived from Maxwell’s equations, so that it adds no real new physics, only some additional insight. I start by taking the dot (or inner or scalar) product of H with Eq. 2.4c and E with Eq. 2.4d. After doing so, I subtract the results, obtaining ∂B 4π 1 ∂D 1 − E·j− E· . H·∇ ×E−E·∇ ×H=− H· c ∂t c c ∂t

(3.18)

∗ I know this because if I stand in the sun or near a ﬁre, I become warm through radiative heat transfer. Indeed,

humans have known of radiative heat transfer at least as early as the discovery of ﬁre, and physicists investigated this process for centuries, culminating in the blackbody theory of Planck and the birth of the quantum theory.

22

The Complex Dielectric Function and Refractive Index Now, I use the vector identity ∇ · (E × H) = H · ∇ × E − E · ∇ × H. Moreover, B = μH and∗ D = 1 E so that quantities on the right-hand side can be manipulated to give H·

∂H μ ∂H 2 ∂B = μH · = ∂t ∂t 2 ∂t

and ∂E 1 ∂E 2 ∂D = 1 E · = . ∂t ∂t 2 ∂t Therefore, with a modest rearrangement of the right-hand side, I get

∂H 2 4π ∂E 2 1 1 +μ − j · E. ∇ · (E × H) = − 2c ∂t ∂t c E·

Almost done! I deﬁne the Poynting vector c S≡ E × H, 4π and the electromagnetic energy density u≡

1 1 (1 E 2 + μH 2 ) = (D · E + B · H), 8π 8π

(3.19)

(3.20)

and then ∇ ·S=−

∂u −j·E ∂t

(3.21)

is Poynting’s theorem. The meaning of Poynting’s theorem is most easily seen by integrating Eq. 3.21 in some volume V and using the divergence theorem to convert the volume integral on the left-hand side to an integral of S · nˆ over the surface of V . Then S · nˆ represents the energy ﬂowing into or out of V , ∂u/∂t is the change of energy density within V , and j · E is the Joule heating (I 2 R heating) due to currents in the lossy medium within V . Energy is conserved, which I ﬁnd reassuring. My next worry is how to handle the complex ﬁelds that I have been using within Maxwell’s equations. Whenever I am thinking about energy, I better make sure when I insert ei (qx−ωt ) that I end up with pure real quantities when done. I of course will get pure real quantities if I write my ﬁelds as sines and cosines but there are good reasons – already invoked – to eschew sines and cosines and instead to use complex exponentials. Moreover, it is generally the case that I am interested in time-averaged energy ﬂows and not the instantaneous energy ﬂow. This consideration is true even when I have the ability to measure the time-instantaneous energy ﬂux.† ∗ When I backed up to Eqs. 2.4c and 2.4d, I reverted to the state before I deﬁned the complex dielectric function,

so I must use D = 1 E and j = σ1 E. Moreover, I’ll take μ as real. Were it not, I’d need a term like the j · E term to account for the dissipation done by the magnetic ﬁeld. † Many authors argue at this point in the Poynting discussion that the reason to be interested in the time-averaged ﬂux rather than the instantaneous ﬂux is that it is impossible to follow the instantaneous ﬂux. This statement is of course a canard. If I have a laser oscillating at 300 THz, I can mix it on a photodiode with a local-oscillator laser oscillating at 300 THz + 10 MHz and look at the 10 MHz beat note to determine the amplitude and phase of the primary laser. I can shine light at GHz frequencies on a fast photodiode and see the oscillaing output on an

23

3.5 Energy Density, Poynting Vector, and Intensity Let me write the manifestly real ﬁelds (E+E∗ )/2 and (H+H∗ )/2, with E and H complex functions of space and time, speciﬁcally the electric and magnetic ﬁelds of Eqs. 2.5 and 2.6. Moreover, as in the footnote on that page, I’ll write the constant describing the direction, amplitude, and phase (at r = 0 and t = 0) of the electric ﬁeld as E0 = eˆ E0 eiφ0 . The electric and magnetic ﬁelds (and their complex conjugates) are solutions to Maxwell’s equations. ˆ Thus, I look back at my solutions to see that E and H are orthogonal and that eˆ × hˆ = q. ˆ Moreover H = N E where N is the complex refractive index. I S is in the direction of q. use these ﬁelds in Eq. 3.19 and

H + H∗ c E + E∗ , S = qˆ 4π 2 2

c EH ∗ + E ∗ H + EH + E ∗ H ∗ , = qˆ 16π c = qˆ (N ∗ + N )EE ∗ + N E 2 + N ∗ (E ∗ )2 . 16π As always N = n + iκ, so that N + N ∗ = 2n. The complex electric ﬁeld has an amplitude |E| and a phase φ, so that E = |E|eiφ . If the wave is traveling along the x axis, the time and space dependent phase φ is of the form φ = nωx/c − ωt + φ0, while the amplitude is |E| = |E0 |e−ωκx/c . This amplitude is a function of x in absorbing media but is not a function of time. With these, I get c [n + n cos 2φ − κ sin 2φ] |E|2 . (3.22) S = qˆ 8π S has a time-independent and a time-dependent component. The time-dependence is embedded in φ; S oscillates at twice the frequency of the electric ﬁeld. Being mostly interested in the time-independent part, I calculate the average 1 T S = S dt T 0 where T is either the period of the wave or a time large compared to many periods. The oscillating terms average to zero, leaving only the constant-in-time part, c S = qˆ ˆ n|E|2 = qI, (3.23) 8π where I is the wave intensity, the energy ﬂux/unit area. Equation 3.23 gives the energy ﬂow in local isotropic, homogeneous, and linear media. One upshot of this discussion is that the usual deﬁnition of the time-averaged Poynting vector for harmonically varying ﬁelds [2], c S = E × H∗ (3.24) 8π is only correct for nonabsorbing media. It does give the direction and take care of the factor ei (qx−ωt ) in both E and H because the effect of the complex conjugation is to eliminate this oscilloscope. It is interesting to set up a photodiode looking up at 50 Hz or 60 Hz ﬂuorescent lights illuminating an ofﬁce or lab and observe that the intensity follows I ∼ cos2 (2πf t) = (1 + cos 4πf t)/2. Of course my eyes cannot quite follow this 100 or 120 Hz ﬂicker but electronics can.

24

The Complex Dielectric Function and Refractive Index term. But H = N E and N is a complex function. If however I decide that the real part is the observable, Eq. 3.24 agrees with Eq. 3.23. Returning to Eq. 3.12 for the ﬁeld, I have at last the simple result for the Poynting vector as a function of distance traveled in the solid: ω c n|E(0)|2 e−2 c κx , S(x) = qˆ 8π where E(0) is the value of the electric ﬁeld at x = 0. The only part of the ﬁeld that I need to care about is its amplitude. I’ll simplify by writing the intensity as ω

I = I0 e−2 c κx ≡ I0 e−αx , where I0 is the intensity in the y–z plane at x = 0 and I deﬁne ω α = 2 κ, c

(3.25)

(3.26)

the absorption coefﬁcient (with units cm−1 ) of the material. It is understood that I follow the ray traced by the light wave from x = 0 in calculating the intensity. Equation 3.25 is known as Lambert’s law, Beer’s law, or the Beer–Lambert law.∗ Note that because 2 = 2nκ, one can also write 4π σ1 ω 2 = . (3.27) α= c n nc √ Eq. 3.27 is exact but is often most useful when 2 1 so that n ≈ 1 . Another useful result is that α = 2/δ with δ the penetration depth of the ﬁeld (the “skin depth”). √ If 2 = 0 and 1 > 0 , then n = 1 and κ = 0. Because κ governs the damping of the wave, a material with positive 1 and 2 = 0 is nonabsorbing; the electromagnetic wave √ propagates to inﬁnity without loss of amplitude. If 1 < 0 and 2 = 0, then κ = −1 ω and n = 0. The electric ﬁeld is damped as e−κ c x with no oscillatory part at all. (The wavelength is inﬁnite.)†

3.6 Normal-Incidence Reflectance I’ll discuss reﬂection and transmission of a sample (with a front and a back surface) in Chapter 7. For the moment I want to consider the simpler case of Fig. 3.2. Light is incident normally on an interface between two semi-inﬁnite media, one with complex dielectric function a (refractive index Na ), occupied by the incoming and reﬂected ﬁelds, and a second with complex dielectric function b (refractive index Nb ), occupied by the transmitted ﬁeld. ∗ Beer’s law is conventionally written in terms of the concentration c of a molecule in solution, and breaks

the absorption coefﬁcient into two parts: α = cε where ε is a molecular constant called the molar extinction coefﬁcient. † It is not immediately obvious whether this damping in the negative plus = 0 case is accompanied by 1 2 energy absorption. I need to consider energy ﬂow across an interface to determine that, in fact, there is no ◦ absorption. I can argue here that the current j is 90 out of phase with the electric ﬁeld E, so the time average dissipation, j · E, is zero.

25

Fig. 3.2

3.6 Normal-Incidence Reflectance

Field vectors for incoming, reflected, and transmitted waves at an interface between two media. Let me orient the qˆ vector of the incoming ﬁeld along the xˆ axis and its E ﬁeld along the yˆ axis, so that the H ﬁeld is along zˆ . The interface is in the y–z plane at x = 0. The incident ﬁelds are ˆ i (qx−ωt ) Ei = E0 ye and Hi = Na E0 zˆ ei (qx−ωt ), where I’ve used Eq. 3.14 to write the magnetic ﬁeld amplitude. ˆ Its The reﬂected ﬁeld is traveling along the −x axis, so q · r = −qx or qˆ = −x. amplitude is proportional to E0 and to the amplitude reﬂection coefﬁcient r. ˆ i (−qx−ωt ) Er = rE0 ye and Hr = −Na rE0 zˆ ei (−qx−ωt ) . ˆ Both Reversing qˆ means that one of eˆ and hˆ (but not both!) must reverse also. I chose h. ﬁelds have q = ωNa /c. The transmitted ﬁeld is in the second medium (b). Hence, it has q = ωNb /c. It also is linear in E0 and in the amplitude transmission coefﬁcient t. ˆ i (qx−ωt ) Et = tE0 ye and Ht = tNb E0 zˆ ei (qx−ωt ) .

26

The Complex Dielectric Function and Refractive Index

All ﬁelds are parallel to the interface, so the boundary conditions are that the tangential components of the total ﬁelds are continuous across the interface.∗ So, let’s dot with the appropriate unit vector, cancel E0 , which appears in every ﬁeld, and evaluate the boundary conditions at the interface, x = 0. I can evaluate the boundary conditions at any convenient time, zero being the most convenient. The boundary conditions produce two equations: E is continuous (Ei + Er = Et ): 1 + r = t.

(3.28)

Na (1 − r) = Nb t.

(3.29)

H is continuous (Hi + Hr = Ht ):

Substitute t from Eq. 3.28 into Eq. 3.29 and solve for r to ﬁnd: r=

Na − Nb . Na + Nb

(3.30)

This clearly gives the intuitive answer when Na = Nb . Now that I know r, it is easy to ﬁnd t using Eq. 3.28: t=

2Na . Na + Nb

(3.31)

Now, I’ll specialize to the case where the incident and reﬂected waves are traveling in vacuum, so Na = 1. I can let Nb ≡ N and write Eq. 3.30 as r=

1−N . 1+N

(3.32)

It seems that for N > 1 and mostly real (a common case) the amplitude reﬂection coefﬁcient is negative. This fact is usually expressed by saying the reﬂection from less-dense to moredense media has a 180◦ phase shift. In most experiments, one measures the intensity of incident and reﬂected light.† The normal-incidence reﬂectance is proportional to |Er |2 , i.e., R = rr ∗ . With N = n + iκ, the reﬂectance is 1 − N 2 R = 1+N =

(n − 1)2 + κ 2 . (n + 1)2 + κ 2

(3.33)

The range of R is 0 ↔ 1. To see how R depends on the refractive index, let me ﬁrst look at the case where the material is weakly absorbing, so that κ can be neglected and R ≈ (n − 1)2 /(n + 1)2 . Then, if n is not large (say in the range of 1.1–1.9, common values for glass and other materials

∗ The condition on H is actually that the ﬁelds are discontinuous by the surface current density 4π K/c but right

now let me assume no surface charges or currents.

† Detectors typically can respond to amplitudes at low frequencies (up to GHz) but not at optical frequencies

(THz to PHz and more). Instead they respond to the intensity or power in the optical beam.

27

3.7 What If My Solid Is Magnetic? in the visible), R is in the range 0.002–0.1. It requires n = 6 to raise R to 0.5 or so. R = 1 only when n is very, very large If κ is large, n can be close to unity and the reﬂectance still will be large. In the case∗ when n 1, R approaches 1 independent of κ.

3.7 What If My Solid Is Magnetic? If I keep the requirements of linear, isotropic, and homogeneous materials, but allow there to be an induced magnetization M, I will have a nonzero magnetic susceptibility χ m . The magnetization in a linear material is proportional to the magnetizing ﬁeld H: M = χ m H. Then, using B = H + 4π M, I see that B = μH (rather than B = H). In a microscopic picture, the magnetic dipoles within the material are rearranged by the external ﬁeld. Materials with μ > 1 are “paramagnetic” (aluminum, platinum, MnO2 ); those with with μ < 1 are “diamagnetic” (bismuth, silver, water, benzene).† Typical deviations from unity are small. I have to modify Eq. 3.3 when M = 0. Using B = μH, Eq. 3.3c becomes ω (3.34) q × E = μH. c Having the permeability in Eq. 3.3c increases the symmetry; now two equations have materials properties in them. Note that μ is complex, with μ = μ1 + iμ2 . Continuing with the algebra which gave Eqs. 3.9 and 3.10 I ﬁnd ω√ μ (3.35) q= c and √ N = μ. (3.36) The algebra which gave Eq. 3.14 leads to H =

E. μ

Finally, the normal incidence amplitude reﬂectivity (Eq. 3.30) becomes a − b μa μb r= a + b μa μb

(3.37)

and the reﬂectance (intensity) is R = rr∗. ∗ That case occurs in metals. In the extreme limit of materials with n = 0 and κ ﬁnite, R = 1. Any value for κ

sufﬁces here. This result is the proof for the assertion in the footnote at the end of Section 3.5 that there is no absorption when 2 = 0. † The conduction electrons of a metal exhibit Pauli paramagnetism, a deﬁnite quantum mechanical effect. The core electrons or ﬁlled shells exhibit core diamagnetism, another quantum effect. The sum of these terms determines whether the material is overall paramagnetic or diamagnetic.

28

The Complex Dielectric Function and Refractive Index

3.8 Negative Index Materials The refractive index, Eq. 3.36, is the square root of the product of the dielectric function and the permeability. It is interesting to ask if there is ever a case where I should use the negative square root? The answer to the question is yes [9–13]. To simplify the discussion of negative refractive indices, let me restrict myself to materials where and μ are pure real numbers and allow them to be either positive or negative. In this case, the material is nonabsorbing. Start by writing N 2 = μ. In the usual case of transparent materials, > 0 and μ > 0. Then I have a pure real and positive √ refractive index, N = n = μ. If one or the other of and μ is negative and the other one positive,∗ then I have a pure imaginary refractive index, N = iκ. Now let me consider the case where both and μ are negative. Their product is positive so their square root is real. I’ll start my discussion with Eqs. 2.7a–2.7d. I’ll rewrite them using constitutive relations D = E and B = μH. I take j = 0 because j = σ1 E = (2 /4π ω)E and 2 is zero for real . Then, q · E = 0

(3.38a)

μq · H = 0

(3.38b) ω (3.38c) q×E=μ H c ω (3.38d) q × H = − E c The ﬁrst two show as always that q is orthogonal to E and H. The third shows that E and H are orthogonal. (The fourth is redundant as to direction; it also shows H and E are orthogonal.) To be speciﬁc, I can without loss of generality orient once again E along yˆ and H along zˆ . ˆ Indeed, eˆ × hˆ = sˆ, so that S, Then, according to Eq. 3.23, the Poynting vector S is along x. E, and H form a right-handed set. Energy ﬂows along the positive x axis. Now, both μ and are negative, so that the directional parts of Eqs. 3.38c and 3.38d read ˆ These equations both show that q is oriented along −x. ˆ qˆ × eˆ = −hˆ and qˆ × hˆ = +e. Thus q, E, and H form a left-handed set. For this reason the term “left-handed materials” is sometimes used. Wave motion is along the negative x axis. I can achieve this by writing Eq. 3.12 (with κ = 0) ω

E = E0 ei (n c x−ωt ) √ and deﬁning n = − μ to be a negative number. Thus I’ve shown that I must choose the negative square root when both and μ are negative. Finding a material with both and μ negative at the same frequency is not easy. Moreover, many applications want the magnitudes not to be too large. Therefore, studies in this area have relied on synthetic materials, usually called “metamaterials.” A common ∗ I have not yet shown evidence that negative dielectric functions or permeability exist. In Chapter 4 I will discuss

classical models of the Drude metal and the Lorentz oscillator. In both, there are ranges of frequencies where the dielectric function is negative. Oscillator models for the permeability also give frequencies where it is negative.

29

3.8 Negative Index Materials

example is a periodic array of circuit boards with unit cells made up of conducting straight wires for the negative elements and metallic split-ring resonators (looking like a c inside a reversed C) for the negative μ elements [14]. The materials are, however, far from nonabsorbing, requiring both and μ—to be complex. The theory can handle this, but at some cost in complexity [9, 10, 12]. The normal incidence amplitude reﬂection is still given by Eq. 3.37. More interesting things happen for oblique incidence. Snell’s law (Appendix E) for refraction across an interface separating an ordinary material with refractive index no > 0 and a negative index material with refractive index nn < 0 reads no sin θo = nn sin θn , appearing identical to the ordinary Snell’s law. However, the negative nn then requires a negative θn , and the refracted ray is on the same side of the interface normal as is the incident ray, rather than crossing over it as happens in the usual case.

4

Classical Theories for the Dielectric Function

4.1 A Polarizable Medium In my junior E&M class the lecturer worked out the case of a capacitor with a dielectric inside and found that the capacitance is increased by a factor of 1 , the dielectric constant. (Dissipation was not considered at this initial stage.) The enhancement was attributed to the polarization of the atoms or molecules in the dielectric medium, typically viewed as little spheres or ellipsoids, each with a net dipole moment p. This dielectric constant was not taken to be a function of frequency.∗ I can quantify this a bit more by considering a single atom between the capacitor plates, with the plates charged up to produce a ﬁeld E at the site of the atom. The atom thereby acquires a dipole moment, whose magnitude is determined by the atomic polarizability αe : p = αe E.

(4.1)

As long as the atom has at least one excited state (of the right symmetry) the polarizability can be calculated using second-order perturbation theory [15]. In cgs-Gaussian units, the polarizability has dimensions of volume, cm3 . Hence, the polarizability is often considered as a measure of the size of the charge-distribution. (Recall [2] that for a conducting sphere, αe = r 3 .) Now consider placing N atoms, all the same, in the volume V between the capacitor plates. At low densities of atoms, the dipole moment per unit volume so produced is P=

N 1 αei E = nαe E, V

(4.2)

i=1

where n = N/V is here the number density of atoms. Equation 4.2 ignores the effects that the polarization of one atom has on its neighbors. I’ll work this out in some detail in Section 4.4.2 of this chapter. For now, because P = χ e E, I will write the dielectric susceptibility as χ e = nαe and c = 1 + 4π nαe .

(4.3)

The subscript (c) appearing in Eq. 4.3 stands for “core” and is meant to represent the contribution of tightly-bound core electrons to the optical properties. As long as hω ¯ E0 − E1 where E0 is the ground-state binding energy of these core electrons and ∗ Although it is. But if I neglect the frequency dependence, I get to call it the dielectric “constant.”

30

31

4.2 Drude Absorption by Free Carriers E1 is their ﬁrst available excited state∗ c can be taken as a real constant. It is often called ∞ , the limiting high frequency value of the dielectric function because, as I shall show, other contributions to are observable at speciﬁc frequencies; these contributions are not important as ω → ∞. As I work out simple models for the dielectric function of solids, I’ll include c where appropriate.

4.2 Drude Absorption by Free Carriers The ﬁrst serious model for optical properties that I will introduce is the one due to Drude [16, 17]. Drude’s model of metallic conduction predates the quantum theory of solids and so omitted several important considerations. The most notable of these are (1) the fact that electrons in a metal obey Fermi–Dirac statistics and are at a temperature low compared to the Fermi temperature and (2) Bloch’s theorem, which says that electrons can effectively propagate without dissipation in a perfect periodic potential. I’ll introduce the theory keeping these concepts in mind, but at the beginning–before worrying about values of things like the mean free path or the effective mass–they make little difference.

4.2.1 Components of the Drude Model The Drude model is based on the following ideas: • The metal has a density n mobile carriers, where n is a number/cm3 (number density, not mass density). • These carriers are typically electrons,† with charge q = −e. • The carriers are free. This statement means that the internal restoring force is zero or the potential is constant. • The carriers do not interact; the electron–electron potential is neglected. • If set in motion, the carriers relax to equilibrium due to damping from collisions. This damping is taken as a frictional or viscous force, proportional to the drift velocity of the carriers.‡ • Newton’s second law for an electron whose coordinate is at r is F = ma = m¨r. • The forces are the external electric ﬁeld −eE and the damping −v = −˙r. • Linear response is assumed, so coordinates, velocities, accelerations have the same time dependence as the ﬁeld E.

∗ The ﬁrst excited state is at the Fermi energy (the chemical potential) or higher. † But not always. Holes are easy to accommodate: change the sign of the charge carrier to positive. The equation

for the conductivity will be the same whether one has holes or electrons.

‡ This is where the Fermi–Dirac statistics ﬁrst rears its head. The electrons at the Fermi energy have very high

speeds; the drift velocity is the deviation from equilibrium. Of course Drude took the equilibrium speed as zero or as a thermal speed for classical particles.

32

Classical Theories for the Dielectric Function

• The electric ﬁeld is the applied ﬁeld Eext and not some local ﬁeld. It is the applied ﬁeld because the electrons sample all parts of the crystal and average over the dipole ﬁelds of the atoms. See Section 4.4.2 of this chapter for more on this point.

4.2.2 Equation of Motion and Its Solution With the above, the equation of motion of one electron is m¨r = −eEext − ˙r.

(4.4)

The electric ﬁeld is the plane wave ﬁeld of Eqs. 2.5 or 3.11. Note that there are two sets of coordinates here. The electron has a location (r) which varies in time as it moves. The electric ﬁeld has a value everywhere in space according to Eq. 2.5. It is the value of E at the location of the particle that matters. (I am considering local response.) For simplicity ˆ making E be only a function of the x coordinate. It is I’ll orient coordinates so that qˆ = x, constant in value for all y and z: Eext = E0 ei (qx−ωt ) . ˆ so the force on the electron is To maintain a nice right-handed set of ﬁelds, I’ll take eˆ = y, ∗ in the yˆ direction. Because the equation of motion contains only the velocity and acceleration of the electron, it makes sense to calculate the current, which, as was discussed in Section 2.3, is j = −nev,

(4.5)

where n is the number density of electrons. So let me write v = v0 ei (qx−ωt ) = r˙,

(4.6)

with v0 a complex constant vector. Taking a time derivative of v gives the acceleration as r¨ = −iωv0 ei (qx−ωt ) . Note that all three terms in Eq. 4.4 have the same complex exponential factor ei (qx−ωt ) , allowing that factor to be hidden. The equation of motion is now an algebraic one, −iωmv = −eEext − v. It is convenient (and conventional) to make the replacement = m/τ , where τ is the relaxation time of the charge carriers.† With this deﬁnition I can solve for the velocity. At the same time I drop the subscript “ext”; that the electric ﬁeld is the external applied ﬁeld is understood when I use Ohm’s law. −e E. (4.7) v= m(1/τ − iω) The velocity is in phase with the applied ﬁeld at low frequencies (ω 1/τ ); it also is independent of frequency. When ω 1/τ it is 90◦ out of phase with the electric ﬁeld and the amplitude of the motion decreases as 1/ω. ∗ −yˆ actually, since the electron has a negative charge. † Suppose that when v = v the electric ﬁeld is turned off. Equation 4.4 with replaced becomes m˙v = −mv/τ . 0 Its solution is v = v0 e−t/τ . τ is the time required to relax the velocity to 1/e of the initial value.

33

4.2 Drude Absorption by Free Carriers

4.2.3 Ohm’s Law and the Drude Conductivity Now, substitute this velocity into Eq. 4.5 to ﬁnd j=

ne2 E. m(1/τ − iω)

This equation is in the form of Ohm’s law, j = σ E. The Drude conductivity is ne2 τ/m . 1 − iωτ

(4.8)

σdc = ne2 τ/m.

(4.9)

σ = At dc (ω = 0) the conductivity is

σdc is proportional to the carrier density n, the relaxation time τ and inversely proportional to the mass m of the carriers.

4.2.4 Some Numbers Silver or copper have a dc conductivity of σdc = 6.2 × 105 −1 cm−1 (i.e., a resistivity of 1.6 μ-cm). After reading Appendix A, I know to multiply σdc by 30c to get the conductivity into esu units; it is 5.6 × 1017 s−1 . This is a fairly high (angular) frequency; it corresponds to about 370 eV photon energy. The approximation σdc ω is certainly valid at low frequencies (ωτ < 1). I can estimate the mean free time from the dc conductivity. Solving Eq. 4.9 for τ , I obtain τ = mσdc /ne2 (with σdc in s−1 !). Using n = 5.9 × 1022 cm−3 (silver or gold), e = 4.8 × 10−10 esu, and m = 9.1 × 10−28 g, I get τ = 3.8 × 10−14 s. If I convert this to a frequency (by inversion) 1/τ = 2.6 × 1013 s−1 . I need to be clear about the units here, because there has been occasional confusion about what this time and rate mean [18]. τ is the mean free time between collisions and 1/τ is the rate at which collisions occur; it also represents the angular frequency at which ωτ = 1. If the static ﬁeld driving the current were suddenly to be extinguished, the currents would decay to zero as j ∝ e−t/τ . Hence, I divide by 2π to convert to ordinary frequency and then by c to convert to cm−1 . I multiply by h¯ to convert to an energy equivalent. Hence, to two digit precision,∗ I have 1/τ = 2.6×1013 s−1 == 4.2 THz == 140 cm−1 == 17 meV/h. ¯

4.2.5 The Real and Imaginary Parts of σ The complex conductivity (σ = σ1 + iσ2 ) may be split into its real (σ1 ) and imaginary (σ2 ) parts by multiplying by unity, written as (1 + iωτ )/(1 + iωτ ): ne2 τ/m σdc = 2 2 1+ω τ 1 + ω2 τ 2 2 ne τ/m ωτ σdc σ 2 = ωτ = . 2 2 1+ω τ 1 + ω2 τ 2 σ1 =

∗ Probably more precision than the calculation deserves.

(4.10a) (4.10b)

34

Classical Theories for the Dielectric Function

Fig. 4.1

Real and imaginary parts of the conductivity of a Drude metal like silver.

Fig. 4.2

Real and imaginary parts of the conductivity of a Drude metal like silver. The curves are plotted on a log-log scale. Figures 4.1 and 4.2 show the real and imaginary parts of the conductivity of a Drude metal. The ﬁrst show these functions on linear scales and the second on logarithmic scales. The parameters are σdc = 6.2 × 105 −1 cm−1 and 1/τ = 140 cm−1 (19 meV). These are meant to mimic the optical conductivity of silver. The real part, σ 1 , is constant at low frequencies but, as frequency increases, it rolls off, falling as 1/ω2 at frequencies above 1/τ . The imaginary part starts off linear in ω and has a maximum at ω = 1/τ (where σ1 = σ2 ) and falls as 1/ω at high frequencies. The shape of the Drude conductivity curve is always the same: a peak in σ1 (ω) at zero frequency and a hump-like feature in σ 2 (ω). Two quantities control the details. One is the

35

4.2 Drude Absorption by Free Carriers area under the σ1 (ω) curve, which (as I shall show) is proportional to ne2 /m and hence is often called the “spectral weight.” The second is 1/τ , the full width at half maximum.

4.2.6 Complex Dielectric Function, (ω) I’ve already written Eq. 3.6 relating the complex dielectric function to the complex conductivity: = 1 + 4π iσ/ω. But the Drude conductivity, Eq. 4.8, considers only the conduction electrons in the metal. As discussed in Section 4.1, there is also the polarization of the ion cores.∗ So, I’ll include c , modifying Eq. 3.6 to read = c + 4π iσ/ω. And then, substituting Eq. 4.8 and doing a little algebra, I get (ω) = c −

4π ne2 /m . ω2 + iω/τ

(4.11)

The Drude contribution comes in with a minus sign in the real part (but a positive imaginary part). Look at the numerator in the second term: 4π ne2 /m. This quantity has dimension of [esu2 /cm3 -g]. But Coulomb’s law in cgs-Gaussian units, F = q1 q2 /r 2 , tells me that [esu2 = dyne-cm2 ]. And, the cgs unit of force is [dyne = g-cm/s2 ], making the units of 4π ne2 /m [1/s2 ], a frequency squared.† So I’ll deﬁne the frequency, which I will call the “plasma frequency,” ωp , to be 4π ne2 , (4.12) ωp ≡ m and write (ω) = c −

ωp2 ω2 + iω/τ

.

(4.13)

Moreover, Eq. 4.9 becomes σdc = ωp2 τ/4π .

4.2.7 The Real and Imaginary Parts of The real and imaginary parts of are obtained by multiplying the top and bottom of the second term by ω − i/τ and doing a small amount of algebra: 1 = c − 2 =

ωp2 ω2 + 1/τ 2 ωp2

ωτ (ω2 + 1/τ 2 )

(4.14a) .

(4.14b)

∗ There is, of course, a lot more than core polarizability. There can be a number of interband transitions, motion of

ion cores (lattice dynamics) and other interesting solid-state physics. These processes, which must be included in a complete dielectric function, are the subject of many later chapters. † I knew this, of course, because is just a number and the denominator of Eq. 4.11 has units of frequency squared.

36

Fig. 4.3

Classical Theories for the Dielectric Function

Real and imaginary parts of the dielectric function of a Drude metal. The dashed line shows 1 multiplied by 1,000, allowing the zero crossing at 32,000 cm−1 (4 eV) to be seen. These functions are plotted in Fig. 4.3. The parameters used, ωp = 73,000 cm−1 (9.0 eV), 1/τ = 140 cm−1 (17 meV), and c = 5.1, are meant to mimic the dielectric function of silver. The real part is negative and large in magnitude at low frequencies. Indeed, the low frequency limit of Eq. 4.14a is 1 ≈ −ωp2 τ 2 (neglecting c , which is almost always appropriate in good metals). As the frequency becomes large with respect to 1/τ , the dielectric function becomes that of pure free carriers, 1 ≈ c − ωp2 /ω2 . √ The zero of 1 occurs near ωp / c . I’ll call this frequency the “screened plasma frequency.” The imaginary part goes as 1/ω at low frequencies, diverging as ω → 0.∗ At high frequencies, 2 ∼ 1/ω3 .

4.2.8 Some More Numbers Plasma frequencies are typically in the visible to ultraviolet for metals but can be in the infrared or far infrared for low-density metals and for doped semiconductors. Using the same parameters as in Section 4.2.4 of this chapter (n = 5.9 × 1022 cm−3 , e = 4.8 × 10−10 esu, and m = 9.1 × 10−28 g), I calculate ωp = 1.4 × 1016 s−1 . If I convert angular frequency (s−1 ) to regular frequency (Hz), wavenumber, and electron volts, I get ωp = 2.2×1015 Hz == 72,000 cm−1 == 9.0 eV/h. ¯ Using the value for the mean free time estimated in Section 4.2.4 of this chapter, τ = 2 × 10−14 , the low frequency value for 1 is −ωp2 τ 2 = −250,000.

∗ This behavior makes not a very useful function for conducting materials. 2

37

4.2 Drude Absorption by Free Carriers If the mass is the free-electron mass, m = me , and the number density n is measured in cm−3 , then the plasma frequency is √ √ √ (4.15) ωp = 8980 n Hz == 2.993×10−7 n cm−1 == 3.711×10−11 n eV/h. ¯ √ √ If m = me , then one replaces n with nme /m.

4.2.9 Factors that Affect the Optical Conductivity Three materials-dependent quantities come into the conductivity of a metal: the carrier density n, the dynamical or effective mass m, and the mean free time τ . The ﬁrst two combine to give the plasma frequency; the result is that only n/m can be extracted from optics alone.∗ The mean free time in the Drude model represents the time between electron collisions (or more correctly [19], the time the electron has before it suffers its next collision). The electron moves under the inﬂuence of the ﬁeld between the collisions and contributes to current ﬂow. I’ll say a lot more about this in Chapter 8. For now, I’ll assert that the mean free time is affected by the purity and crystal quality of the metal and by the temperature. The mean free time is longer when purity is high and temperature is low. Empirically, these scattering rates are independent and add, following Matthiessen’s rule: 1 1 1 = + τ τ (T ) τi where τ (T ) is the temperature-dependent scattering from thermal excitations in the metal and τi is the temperature-independent scattering from impurities or other defects. τ (T ) has a complex temperature dependence, but at high temperatures many metals have 1/τ (T ) ∼ T ; at low temperatures the power law is stronger: T 2 , T 3 , or T 5 . At the lowest temperatures, the scattering rate (and the resistivity) saturates at the impurity-limited value. The ratio between the room-temperature resistivity and the low-temperature resistivity is called the residual resistivity ratio (RRR) and is a measure of purity. It is also a measure of relative scattering times, because the carrier density and mass in simple metals do not change much with temperature.† As an example, Fig. 4.4 shows a simulation at three temperatures of the real parts of the conductivity (left panel) and dielectric function (right panel) for a metal of modest purity, RRR = 10. (I choose this value rather than 100 or 1,000, values which are possible in highpurity metals, to avoid entering the anomalous skin effect regime. See Chapter 14.) Relative to room temperature, the mean free time is assumed 3× longer for the 100 K calculation and 10× longer for the 10 K calculation. The dc conductivity goes up and the width of the peak becomes narrower with decreasing temperature; the areas under the three conductivity curves stay the same. The dielectric function follows −ωp2 /ω2 at high frequencies; with ∗ If I measure the Hall effect or other magneto-optical parameters such as cyclotron frequency, I can determine n

or m individually and then the optical parameters will provide the other.

† There are other systems with other behaviors. Semiconducting materials have a much stronger temperature

dependence to the carrier density than to the mean free time. Heavy-Fermion metals have a huge increase in carrier effective mass at low temperatures.

38

Fig. 4.4

Classical Theories for the Dielectric Function

Left: Optical conductivity of a hypothetical metal with modest purity. Curves are shown for room temperature, 100 K, and low temperatures. Right: Dielectric function of the same metal. decreasing temperature the 1/ω2 behavior continues to lower frequencies. (The curve marked 300 K occupies only a bit of the panel here; it is identical to the 1 shown in Fig. 4.3.) The limiting low frequency value of −ωp2 τ 2 increases 100× as the mean free time becomes 10 times longer.

4.2.10 Fields and Currents This is a good time to take a look at the ﬁelds and currents in the metal. Recall that the physically observable ﬁeld is the real part of the complex ﬁeld. Hence, if I could put probes in and measure the ﬁeld, I would see ˆ −iωt ] = E0 yˆ cos(ωt) E = Re[E0 ye and if I could put a current meter in, I would see ˆ −iωt ] = σ 1 E0 yˆ cos(ωt) + σ 2 E0 yˆ sin(ωt) j = Re[σ yEe so if σ 1 σ 2 (low frequencies), the current is in-phase with the ﬁeld and their time average j · E equals half of the product of peak values. This is the Ohmic loss in the metal. If, however, σ 1 σ 2 (high frequencies), the ﬁeld follows the cosine and the current mostly follows the sine; the time average of their product is nearly zero. The electrical analogy is a nearly ideal inductor.

4.2.11 The Refractive Index √ It is the complex refractive index (N ≡ ) which most directly governs wave propagation in the medium. Figures 4.5 and 4.6 show the real and imaginary parts of the refractive index

39

4.2 Drude Absorption by Free Carriers

Fig. 4.5

Real and imaginary parts of the refractive index of a Drude metal. Data are shown on a log-log scale. The real and √ imaginary curves cross when ω ≈ ωp / c .

Fig. 4.6

Real and imaginary parts of the refractive index of a Drude metal. Data are shown on linear scales. of a Drude metal. These are calculated using the same parameters as for the dielectric function. There are several regimes to discuss. At low frequencies, the refractive index n and the extinction coefﬁcient κ are both large and relatively close in magnitude. (See Fig. 4.5 for the low-frequency region.) At very low frequencies, where 1 2 (i.e., where ω 1/τ ), √ Eq. 3.17 gives n ≈ κ ≈ 2 /2. See Figures 4.3–4.6 for the behavior of and N . For the Drude metal, then,

40

Classical Theories for the Dielectric Function n≈κ≈

ωp2 τ 2ω

=

2π σdc ω

when ω

1 . τ

(4.16)

Both n and κ fall with increasing frequency, with n falling faster than κ. At intermediate frequencies, the refractive index of a metal can be less than one, sometimes much less than one. This behavior is seen in the calculation shown in Figures 4.5 and 4.6 once ω 1/τ up until the screened plasma frequency. In this regime, the phase velocity, v = c/n is bigger than c. I leave it to the reader to show that the group velocity is smaller than c. The waves in the material are of course strongly damped; with the electric ﬁeld penetration length, δ = λ0 /2π κ, smaller than the vacuum wavelength. At a certain frequency (32,000 cm−1 in this case) κ falls rapidly and n jumps up to a value bigger than 1. This jump occurs exactly where crosses zero, the screened plasma √ frequency. Above this frequency, n ≈ c and κ is small. The behavior of N is easy to understand in the extreme case when I can neglect the scattering rate 1/τ . (Even if 1/τ is ﬁnite, this is a good ﬁrst approximation when ω 1/τ .) Then = c −

ωp2 ω2

and ⎧ ⎪ ⎪ ωp2 ⎪ ⎪ 0 + i − c , ⎪ ⎨ ω2 N= ⎪ ⎪ ⎪ ωp2 ⎪ ⎪ − + i0, ⎩ c ω2

√ for ω < ωp / c √ for ω > ωp / c .

Below the screened plasma frequency, this approximation gives a pure imaginary value iκ for N. The real part of the complex refractive index is zero. Above the screened plasma √ frequency, N = n is purely real and has the high-frequency limit of n = c . Metals √ should be transparent above ωp / c , and some are.

4.2.12 Reflectance Once I have N , I can calculate the reﬂectance R from Eq. 3.33. At low frequencies, both parts of N are very large, so the difference between n and 1 is large. In this case, it is sometimes convenient to write Eq. 3.33 as R=1−

4n . (n + 1)2 + κ 2

(4.17)

Note that although Eq. 4.17 might look like an expansion, it is exact. The calculated reﬂectance, using parameters identical to those for Figures 4.1–4.3, 4.5, and 4.6, is shown in Fig. 4.7 as the red curve, marked “300 K.”

41

Fig. 4.7

4.2 Drude Absorption by Free Carriers

Normal incidence reflectance of a Drude metal. A good approximation in the far infrared, where n ≈ κ 1, is to write n + 1 ≈ n and then, using Eqs. 4.16 and 4.17, obtain the so-called Hagen–Rubens [20] equation 2ω R≈1− . (4.18) π σdc The reﬂectance is 100% at ω = 0 and falls in accord with Eq. 4.18 with increasing frequency. Once ω is bigger than 1/τ the reﬂectance ﬂattens out. This behavior is shown in the inset of Fig. 4.7, where one can see the Hagen–Rubens regime at the left and the ﬂattening out at higher frequencies. The reﬂectance is above 99.5% in each case. At high frequencies, the reﬂectance falls rapidly from a value close to unity to a value close to zero. This drop occurs around 30,000 cm−1 (3.5 eV) for the parameters used for Fig. 4.7. This “plasma edge” occurs at the same frequencies where the rapid fall of κ and rise of n occur in Fig. 4.6. There is a minimum value of the reﬂectance, corresponding to the conditions∗ n ≈ 1. (The approximation becomes an equality when κ 1.) The simulations for 100 K and 10 K (actually τ increased by 3× and 10×) are shown also in Fig. 4.7. As the mean free time becomes longer, the turnover between the ﬂat and high reﬂectance and the steep plasma edge becomes sharper and sharper.

∗ The exact location of this “plasma minimum” is a balance of the frequency where n − 1 ∼ 0 and the value of

κ near this frequency. To have a deep minimum, κ must have a relatively small value. It is not the same as the frequency where 1 = 0 although these two frequencies are close to each other. In the case where ωp 1/τ , 2 /ω2 . With a real constant, the zero of (ω) is at ω /√ and the reﬂectance then I can write (ω) = c − ωp c p c √ √ minimum is when n = = 1 = 12 = , making the minimum occur at ωp / c − 1. If c = 1, the minimum is at inﬁnity. If c has dispersion (and an imaginary part), the minimum is still near where Re(c (ω)) = 1 but the exact location can be pushed up or down depending on the functional form of Im(c ).

42

Classical Theories for the Dielectric Function

Fig. 4.8

A slab of free electrons and fixed positive ions. I pretend that the electrons are yellow and the ions blue. The region where both exist is therefore green. Each electron has been displaced upwards by a small amount z0 , creating a yellow region of negative charge on the top of the slab and a blue region of positive charge on the bottom. The central region remains neutral.

4.3 The Plasma Frequency In Eq. 4.12 I deﬁned the plasma frequency as ωp = 4π ne2 /m. What is the meaning of this frequency? There are no peaks in σ 1 (or 2 ) at ωp . The dielectric function 1 changes √ sign near ω = ωp / c but does so smoothly. To see why the name is what it is, consider a slab of metal of thickness L. The metal contains positive ions bound to their lattice positions by the interatomic forces in the metal. Permeating the entire slab is the gas of conduction electrons. The metal is electrically neutral, with a number density of electrons of ne = Nelectrons /V and a number density of ions of ni = Nions /V , where V is the volume of the slab. For conceptual simplicity, let me assume that the ions are singly charged,∗ so that the number of charges is Nelectrons = Nions ≡ N and the number density is ne = ni ≡ n Now, displace the electrons an amount z0 in the upward (ˆz) direction. Take z0 L. Fig. 4.8 shows the slab with the displaced electrons. Because every electron is displaced by the same amount, there is a net dipole moment in the slab. The dipoles all point downward, from the negative electrons to the positive ions. The dipoles are p = −QLˆz where Q is the magnitude of the charge on each surface. This quantity is the product of the number density of charges n, their individual charge e and the volume of uncompensated charge Az0 with A the area of the slab surface: Q = neAz0 . Hence the dipole moment/unit volume, P = p/AL, is neAz0 L zˆ = −nez0 zˆ . AL At the same time, the uncompensated surfaces generate an electric ﬁeld E, just as in the case of a charged capacitor. E points upwards, from the positive charge on the bottom to the negative charge on top. Gauss’ law tells me that E = 4π Q/Aˆz = 4π nezˆz = −4π P. P=−

∗ This assumption is by no means essential; a solid of trivalent ions plus electrons would have

Nelectrons = 3Nions .

43

4.3 The Plasma Frequency

Table 4.1 Experimental plasma frequencies. Material

ωp s−1

νp cm−1

Ep eV

K Na Al “Si”

6×1015 8×1015 2.4×1016 2.6×1016

31,000 48,000 140,000 160,000

3.9 6.0 18.0 20.0

The ﬁeld exerts a force on the electrons, F = −eE = m¨z. The equation of motion of the electrons is thus m¨z = −4π ne2 z. The solution to this equation is that of a harmonic oscillator, z = z0 e−iω0 t with ω0 the resonant frequency of the oscillator. Substitution gives −mω02 z0 = −4π ne2 z0 . So, I get the frequency of the free oscillations to be 4π ne2 ω0 = ≡ ωp . m This equation is identical to Eq. 4.12, the plasma frequency I deﬁned when calculating the Drude dielectric function of the metal. This plasma oscillation is a normal mode of the electrons in the metal slab. The frequency of oscillation is the plasma frequency. If the atomic core polarizability is included in the problem, it becomes analogous to a capacitor with a dielectric material between the plates. The Gauss’ law problem ﬁnds D; the electric ﬁeld E, dipole moment/unit volume P, and the restoring force on the electrons are all reduced by a factor of c , and the resonant frequency becomes ωp ω0 = √ . c A measurement of reﬂectance over the appropriate frequency range can provide me with the plasma frequency. There are four methods in common use. I can ﬁt the reﬂectance to a model dielectric function that includes a Drude term; ωp is a parameter from the ﬁt. I can carry out Kramers–Kronig analysis (Chapter 10) and analyze the 1/ω2 term in 1 . Alternatively, a sum-rule analysis of σ 1 (ω) (also Chapter 10) provides an estimate of ωp . Finally, I can measure the reﬂection and transmission of a thin ﬁlm (Chapter 7) and extract the optical constants and plasma frequency from those data. Each method then gives the ratio of carrier density to effective mass, n/m. Metal plasma frequencies are typically rather high, in the ultraviolet for ordinary metals. Table 4.1 lists a few experimental values while Table 4.2 gives a calculated plasma frequency for a number of elemental metals. The assumptions are: (1) the carrier density is the atomic density times the valence, and (2) the carriers have the free-electron mass.∗ ∗ The charge is e, in esu!

44

Classical Theories for the Dielectric Function

Table 4.2 Calculated plasma frequencies for a variety of metals. Valence

Metal

n 1022 cm−3

ωp 1015 s −1

νp cm−1

Ep eV

1

Li Na K Rb Cs Cu Ag Au Be Mg Ca Sr Ba Zn Cd Al Ga In Pb Sn(w)

4.7 2.65 1.4 1.15 0.91 8.45 5.85 5.9 24.2 8.6 4.6 3.56 3.2 13.1 9.28 18.06 15.3 11.49 13.2 14.48

12.23 9.18 6.67 6.05 5.38 16.40 13.64 13.70 27.75 16.54 12.10 10.64 10.09 20.42 17.19 23.97 22.07 19.12 20.50 21.47

64,800 48,700 35,400 32,000 28,500 86,900 72,300 72,600 147,200 87,700 64,100 56,400 53,500 108,300 91,100 127,100 117,000 101,400 108,700 113,800

8.03 6.04 4.39 3.97 3.53 10.77 8.96 9.00 18.25 10.87 7.95 6.99 6.63 13.43 11.29 15.76 14.51 12.57 13.48 14.11

24.5 32.7 44.9 49.6 55.7 18.3 22.0 21.9 10.8 18.1 24.8 28.2 29.7 14.7 17.5 12.5 13.6 15.7 14.6 14.0

0.1 1

1.78 5.64

9,460 29,900

1.17 3.71

168 53.2

2

3

4

1 × 1021 1 × 1022

c/ωp nm

These assumptions are excellent for the monovalent alkali and noble metals and poor for multivalent metals. The last two rows show the numbers for two carrier densities a factor of 10 apart, taking the mass as the free electron mass. The frequency for any other density can be calculated by multiplying by the square root of the carrier density ratio.

4.4 Lorentz Model: Absorption by Bound Electrons The Lorentz model is designed for insulators or at least for electrons which are bound by some force to an atom or ion in the solid. I’ll also use it for the contribution to the dielectric function from optically active vibrational modes (phonons). This latter role for the model plays out in Chapter 5. I will view the potential for these bound electrons as harmonic, i.e., the electrons are attached to their equilibrium positions by a spring. The spring constant will be the same for all the electrons in a particular orbital. On the one hand, the harmonic potential (a spring)

45

4.4 Lorentz Model: Absorption by Bound Electrons

is quite different from the Coulomb potential that–as is well known–governs the electronic properties of an atom, molecule, or solid. On the other hand, whatever the potential is, I know that it will look harmonic for small displacements from equilibrium. My assumption of linear response suggests that the displacements are indeed small.

4.4.1 Dilute Limit To begin, I’ll consider the dilute limit, just as I did in Section 4.1. The reason I want to start with the dilute limit is that an electric ﬁeld applied∗ to the molecule polarizes the molecule. Near the location of each polarized molecule, there is also a dipolar ﬁeld [2] ˆ rˆ − p 3(p · r) (4.19) r3 where r is a vector from the origin to the ﬁeld point, rˆ = r/r, p = αe Eloc and Eloc is the local ﬁeld at the position of the molecule. I want the strength of these dipolar ﬁelds to be negligible at the other nearby molecules so as to make the local ﬁeld (the ﬁeld responsible for the polarization) equal to the ﬁeld at the molecule from the external electromagnetic wave. The dipolar ﬁeld varies in space, looping from the + end of the dipole around to the − end. Its magnitude is of order Ed ≈ (αe /r 3 )Eapplied . I’ll take for the polarizability α of the molecule the polarizability of a conducting sphere, αe ∼ a03 with a0 the sphere’s radius. To keep the ﬁeld from the polarized molecule smaller than, say, 0.1% of the external ﬁeld, the nearby molecules have to be separated by ∼10× the molecular size, whereas in close packing the separation is of order the molecular size. The density is 1,000 times smaller than the close-packed density; hence, the system is a gas. The molecule has zero dipole moment without an external ﬁeld. The electron is considered to be bound to the position where p = 0 by a harmonic force. Ed (r) =

Fh = −Kx = −mω02 x where K is the spring constant, m is the electronic mass,† and mω02 is a complicated way to write the spring constant.‡ A second force acting on the electron is a damping force proportional to the velocity, just as in the case of the Drude model, Fv = −v ≡ −mγ x˙ , where γ = 1/τ is the damping rate. This damping is formally identical with the Drude model for a metal but the ∗ I think it is easy to be confused about the meaning of the “applied ﬁeld.” In continuum electrodynamics it of

course means the electric ﬁeld applied to the medium from external sources (lamps, lasers, generators). From the point of view of a microscopic picture of the medium as a body consisting of polarizable entities, it is of course the ﬁeld seen by the polarizable entities. These ﬁelds are not necessarily the same. The second one is the superposition of the external ﬁeld and the ﬁelds emitted by all the other polarizable entities. So I need to be careful with the use of “applied ﬁeld;” perhaps “external ﬁeld” and “local ﬁeld” are better terms. I also need to be aware that when I send light into the material from an external source, some of it will be reﬂected at the surfaces of the material and some will be absorbed on its way to the point where I want to evaluate the ﬁeld. I can measure the total ﬁeld at any point by inserting a (small) test charge at that point and seeing what force the test charge feels. Dilute media are those in which the external ﬁeld is the applied ﬁeld. † It is the reduced mass in fact, but the ion mass is big enough that it can be ignored. I’ll take m to be the effective mass – which can be quite different from the free-electron mass – in the solid. ‡ I write −mω2 rather than K because I know how it will work out, anticipating that the resonant frequency 0 √ ω0 = K/m. I have solved the harmonic oscillator problem in the past.

46

Classical Theories for the Dielectric Function

underlying physics is a bit different. In a metal the damping is associated with collisions of the Fermi surface electrons with impurities, phonons, etc. In semiconductors and insulators there is no Fermi surface; the chemical potential lies in a forbidden band gap between valence and conduction band. The damping may be considered as due to collisions of photoexcited carriers with impurities, phonons, or other electrons, leading to relaxation to the ground state. Damping also can come from the emission of excitations like phonons, with a corresponding scattering of the electron. The remaining force is the force due to the external electric ﬁeld, which I’ll take as Fe = −eE = −eE0 e−iωt . Newton’s law is then written as m¨x = −mω02 x − mγ x˙ − eE0 e−iωt .

(4.20)

In linear response, the location of the electron is x = x0 e−iωt . Taking the ﬁrst derivative (bringing down −iω) and the second derivative (bringing down −ω2 ), Eq. 4.20 for the position of the electron becomes mω02 x − iωmγ x − mω2 x = −eE or

−e/m E. (4.21) − ω2 − iωγ Clearly, x is resonant at ω0 ; it diverges at this frequency if γ = 0. With this displacement, the dipole moment is p = −ex, and the polarizability is x=

ω02

e2 /m . (4.22) − ω2 − iωγ The dipole moment/unit volume P = np, where n is the number of molecules per unit volume. Thus αe =

P=

ω02

ne2 /m E = χ e E, ω02 − ω2 − iωγ

with χ e the dielectric susceptibility of the semiconductor or insulator. I then write = 1+4π χ c +4π χ e where χ c is the core polarizability from Section 4.1 (c ≡ 1+4π χ c ) and ﬁnd (ω) = c +

4π ne2 /m . ω02 − ω2 − iωγ

(4.23)

Eq. 4.23 contains a “plasma frequency” which I’ll call ωpe ≡ 4π ne2 /m. The e subscript stands for “electron, bound.” With this deﬁnition I get the ﬁnal form of the Lorentz dielectric function for dilute gases. (ω) = c +

2 ωpe

ω02 − ω2 − iωγ

.

As ω → 0, the dielectric function becomes the static dielectric constant, (0) = c +

2 ωpe

ω02

.

Unlike a metal, the static dielectric constant of this nonconducting gas is positive.

(4.24)

47

4.4 Lorentz Model: Absorption by Bound Electrons

Table 4.3 “Optical”dielectric constant for some gases Molecule

1

He O2 HCl CS2

1.000068 1.00054 1.0009 1.003

Values of this dielectric constant for common gases at STP, and for visible wavelengths (which are below the ﬁrst electronic transitions in the molecule and above any molecular vibration or rotational modes) are given in Table 4.3. The values are not much different from unity.

4.4.2 The Depolarizing Field As the density increases, the difference between the local ﬁeld and the external ﬁeld grows rapidly. I’ll write p = αe Eloc, where αe is the polarizability and Eloc is the value of the ﬁeld at the molecule, including the external ﬁeld and the ﬁeld from the neighboring dipoles, in principle at distances all the way to inﬁnity. This problem was studied in the nineteenth century [21]. The solution is known as the Lorentz–Lorenz model or the Clausius–Mossotti model. I’ll start by writing the electric ﬁeld at some point as a sum of three terms Eloc = Eapp + Eneighbor + Emedium . In this equation, Eapp ≡ E is the external (light) ﬁeld. Eneighbor is the sum of the ﬁelds from the nearby polarized molecules, and Emedium is the contribution from the uniformly polarized medium far from the molecule. To calculate the ﬁeld from the polarization of the medium, one carves out a hollow spherical cavity (shown in Fig. 4.9) in the polarized medium centered on the polarizable molecule being considered and computes the ﬁeld inside the cavity. The uniform polarization P outside the cavity leads to a surface charge density = P · n. ˆ This charge density varies as cos(θ ), and leads to a uniform ﬁeld in the cavity. This ﬁeld, found in electricity and magnetism textbooks [2], is Emedium =

4π P. 3

(4.25)

For a crystalline material, the ﬁelds of the individual dipoles in the cavity, given by Eq. 4.19, all contribute to the ﬁeld at the center. The individual ﬁelds point in a set of

48

Fig. 4.9

Classical Theories for the Dielectric Function

A sphere is carved out from a uniformly polarized material. There is a surface charge density on the surface of the spherical cavity that is the source of a uniform depolarizing field in the cavity. speciﬁc directions which depend on the coordinates of the dipoles. Their sum depends on the crystal symmetry. For a cubic system, the ﬁelds from the neighbors add to zero. Essentially the ﬁelds from the two dipoles behind and in front of the origin are canceled by the oppositely directed and half-strength ﬁelds from the four on either side, above, and below. This cancellation continues as one moves out from the center.∗ Consequently, the local ﬁeld is Eloc = Eapp + where P=

4π P, 3

(4.26)

1 1 pi = αei Eloc = nαe Eloc, V V i

and (now writing Eapp as just E),

i

4π P , P = nαe E + 3

or P=

nαe

E. 1 − 43π nαe

(4.27)

As an aside, there is a possibility of a catastrophe here. Consider the denominator in the equation above. It contains n, the number of atoms per unit volume. Clearly n = 1/ 0 , with 0 the volume of one molecule. Now the polarizability of a metal sphere is αe = r 3 , with r the radius of the metal sphere. Then 4π 3 4π αe ∼ r = 0, 3 3

∗ Clausius and Mossotti actually used a “tight” cavity that closely jacketed the molecule. The crystal structure

was brought in by making the cavity an ellipsoid representing the anisotropy of the crystal.

49

4.4 Lorentz Model: Absorption by Bound Electrons

and P=

nαe E 1−1

is ﬁnite when E → 0. Variations on such a model have been used in the theory of ferroelectrics, solids which have a spontaneous polarization.∗ So now, making sure to keep α e below r 3 , I can write the complex dielectric function with local ﬁeld corrections, and with a core polarizability, = c + 4π χ e as = c +

4π nαe . 1 − 43π nαe

(4.28)

This equation can be turned around. I write c = 1 for simplicity, and then solve for αe in terms of . 4π −1 nαe = (4.29) 3 +2 in which form it is known as the Clausius–Mossotti equation.† It is approximately obeyed by simple molecular solids.

4.4.3 The Lorentz Dielectric Function in the Dense Limit My model for the polarizability, Eq. 4.22, is unchanged, so I can substitute that expression into Eq. 4.28: = c +

4π ne2 /m ω02 −ω2 −iωγ ne2 /3m 1 − ω42π−ω 2 −iωγ

.

0

Using the deﬁnition of the “plasma frequency” ωpe and doing a little algebra, I get = c +

2 ωpe 2 ω02 − ω2 − iωγ − 13 ωpe

.

(4.30)

Let me combine the two constants in the denominator into a single frequency, ωe . Local ﬁeld corrections make this frequency smaller than the bare resonant frequency. 1 2 . ωe ≡ ω02 − ωpe 3 With this deﬁnition I ﬁnally arrive at the Lorentzian dielectric function for solids: = c +

2 ωpe

ωe2 − ω2 − iωγ

.

(4.31)

∗ It is not enough to have a polarizability catastrophe; the crystal symmetry must allow the polarization to exist. † If = 1 then this becomes (4π/3)nα = ( − )/( + 3 − ). c e c c

50

Classical Theories for the Dielectric Function

4.4.4 The Real and Imaginary Parts of The real and imaginary parts of are obtained by multiplying the top and bottom of the second term by ωe2 − ω2 + iωγ and doing a small amount of algebra: 1 = c + 2 =

2 (ω2 − ω2 ) ωpe e

(ωe2 − ω2 )2 + ω2 γ 2 2 ωγ ωpe

(ωe2 − ω2 )2 + ω2 γ 2

.

(4.32a) (4.32b)

These functions are plotted in Fig. 4.10. The parameters are ωpe = 50,000 cm−1 (6.2 eV), ωe = 5,000 cm−1 (0.62 eV), γ = 1,000 cm−1 (0.12 eV) and c = 3.0. These are meant to mimic∗ the optical properties of Ge or perhaps AlGaAs. The real part is positive at low frequencies. The imaginary part is very small at low frequencies. As the frequency approaches ωe , the real part of the dielectric function has a derivative-like shape while the imaginary part shows a resonance. The full width at half maximum is ω = γ . Just above the resonance, 1 < 0. It crosses zero above the resonance. (See the green dashed line, which shows 1 scaled by 100.) I’ll now calculate the actual “screened” plasma frequency ω˜ p where 1 (ω) equals zero. Setting the left side of Eq. 4.32a to zero and doing some considerable algebra, I get 2 ωpe 1 ωe2 γ 2 1 2 2 + − 2 ω˜ p = −γ (4.33) + ωe2 . c 2 4 (ωpe /c − γ 2 )2 This equation is not very illuminating, so let me evaluate it in the case ωpe ωe > ∼ γ. This is the usual case and in this usual case

Fig. 4.10

Real and imaginary parts of the dielectric function of a Lorentzian oscillator. ∗ The mimicry is not very good. The linewidth is too narrow and the static dielectric constant too high.

51

4.4 Lorentz Model: Absorption by Bound Electrons

ω˜ p2 =

2 ωpe

c

+ ωe2 .

As a general statement, one can say that the zero is pushed up by ωe and pulled down by γ .

4.4.5 Limiting Behavior Low frequencies: The low frequency limit of Eq. 4.32a is 1 ≈ c + ωp2 /ωe2 . The imaginary part goes as ω at low frequencies; the conductivity σ 1 as ω2 . 2 /ωγ Mid frequencies: At ω = ωe , 1 = c . The imaginary part is a maximum with 2 = ωpe 2 and σ1 = ωpe /4π γ . I have identiﬁed γ = 1/τ so that this combination of parameters is 2 τ/4π , the dc conductivity of a metal with plasma frequency ω and mean also: σ1 = ωpe pe free time 1/τ .

High frequencies: Above the resonance, 1 is negative, rising as the frequency increases, 2 /ω2 . It crosses through zero at the frequency given by Eq. 4.33. following 1 ≈ c − ωpe At these frequencies, 2 ∼ 1/ω3 .

4.4.6 The Linewidth The three parameters, ωpe , ωe and γ , control respectively the area, the frequency location, and the full width at half maximum of the resonance. The effect of changing γ is shown in Fig. 4.11. 2 is plotted in the main plot and 1 in the inset for three values of γ , 300, 1,000, and 3,000 cm−1 . The other parameters are as before: ωpe = 50,000 cm−1 , ωe = 5,000 cm−1 , and c = 3.0. The resonance becomes broader and the maximum becomes lower as γ increases. The total area is nearly preserved.∗ A small movement of the peak value to lower frequencies can be discerned when γ is large. The behavior for the real part is analogous. The maxima and minima, which are separated by ∼ γ , become smaller and move further apart. It cannot be seen on the plot, but the zero of 1 moves to slightly lower frequencies as γ increases.

4.4.7 Conductivity It is easy to write σ1 (ω); it is related to 2 by σ1 (ω) = ω2 /4π . Then σ1 (ω) =

2 ω2 γ /4π ωpe

(ωe2 − ω2 )2 + ω2 γ 2

.

(4.34)

The real and imaginary parts of σ are plotted in Fig. 4.12. The shape of the Lorentzian is always the same: a peak in σ1 (ω) and a derivative-like 2 (as I shall structure† in σ 2 (ω). Three parameters control the details: ωe the location, ωpe show) the area under the σ1 (ω) curve, and γ the full width at half maximum. The value of 2 /4π γ . the conductivity at the maximum is σ1 (ωe ) = ωpe ∗ Were I to plot the conductivity, the preservation would be perfect. † The negative of the derivative actually.

52

Classical Theories for the Dielectric Function

Fig. 4.11

The main plot shows the imaginary parts of the dielectric function of a Lorentzian oscillator for three values of the damping constant γ . The inset shows the real part.

Fig. 4.12

Real and imaginary parts of the optical conductivity of a Lorentz oscillator.

4.4.8 The Refractive Index Figure 4.13 shows the real and imaginary parts of the refractive index of the Lorentz model. At low frequencies, n is much bigger than κ. κ increases with frequency. At the resonance, n ≈ κ and both are relatively large. Above the resonance, n falls well below unity but κ stays large (because 1 < 0). Then, at a certain frequency 1 changes sign and κ falls

53

Fig. 4.13

4.4 Lorentz Model: Absorption by Bound Electrons

Real and imaginary parts of the refractive index in the Lorentz model. Note the log-log scale. rapidly while n jumps upward to a value bigger than 1. Note that both the lowest-frequency and the highest-frequency values of the refractive index n are just n ≈ 1 (ω) at that frequency.

4.4.9 Reflectance Once I have N , I can calculate the reﬂectance from Eq. 3.33. The reﬂectance of the Lorentz model is shown in Fig. 4.14. At low frequencies, the real part of N dominates. As the frequency approaches ωe , the reﬂectance increases, and above the resonance approaches that of a metal. Then, the reﬂectance falls rapidly from a value close to unity to a value close to zero. This drop occurs around 30,000 cm−1 (3.5 eV) for the parameters used for Fig. 4.14. This “plasma edge” occurs at the same frequencies where the rapid fall of κ and rise of n occur in Fig. 4.13. There is a minimum value of the reﬂectance, corresponding to the conditions∗ n ≈ 1 and κ 1.

4.4.10 Multiple Polarizable Electron Levels Let’s suppose that there are a number of different electrons† with different binding energies in the solid. I’ll indicate the different levels with an index j , where j runs from the least ∗ The exact location of this “plasma minimum” is a balance of the frequency where n − 1 ∼ 0 and, at the same

time, κ has fallen to a relatively small value. It is not the same as the frequency where 1 = 0 although these two frequencies are close to each other. † Electrons are of course indistinguishable particles. However, in the multielectron atom and in solids made from such atoms, the electrons occupy different energy levels or energy bands, with the binding energy (or spring constant in the Lorentz model) different for each band.

54

Fig. 4.14

Classical Theories for the Dielectric Function

Normal incidence reflectance in the Lorentz model. tightly bound electron to the most tightly bound electron I want to consider. (Even more tightly bound electrons remain of course polarizable and will contribute to c .) Because I am ignoring electron–electron interactions, the equation of motion for the j th carrier remains unchanged from Eq. 4.20, except that it needs subscripts: mj x¨j = −mj ω02j xj − mj γj x˙j − eE0 e−iωt , where I’ve allowed for each level to have its own∗ spring constant (mj ω02j ) or resonant frequency ω0j , dynamical mass mj , and damping factor γj . The solution is unchanged from Eq. 4.21 except (still) for subscripts. The j th electron will have dipole moment pj = −exj and the total dipole moment per unit volume becomes nj pj P= j

where nj is the number density of type-j electrons. Local ﬁeld corrections are identical to those in Section 4.4.2. The dielectric function becomes a sum of Lorentzian oscillators of the form in Eq. 4.31. = c +

2 ωpj

j

ωj2 − ω2 − iωγj

,

(4.35)

where ωpj = 4π nj e2 /mj is the plasma frequency associated with the j th kind of electrons and ωj is the (local-ﬁeld corrected) resonant frequency for that kind. By assumption, each kind of electron has its own resonant frequency. If these frequencies are separated by amounts large compared to the linewidth, then 2 and σ1 will have a peak ∗ But not its own charge!

55

4.5 Comments on Wave Propagation

Table 4.4 Parameters for five Lorentz oscillators. Oscillator number j

ωpj

ωj

γj

1 2 3 4 5

5,000 10,000 50,000 55,000 200,000

500 1,000 5,000 5,500 20,000

30 60 300 330 1,200

c = 3.0

Fig. 4.15

Dielectric function for five Lorentz oscillators. at each resonance. 1 will have a derivative-like structure and will step down to a lower value as the frequency is increased past the resonance. If the separation is small compared to the linewidth, there will be a single combined peak in σ1 , with corresponding feature in 1 . Figure 4.15 shows one such calculation. The parameters are given in Table 4.4. I chose the parameters so that ωj /γj was the same for all and also so that ωpj /ωj was the same for all. This choice makes the “quality factor” Q of all resonances the same as well as their contributions to the static dielectric constant, 1 (0).

4.5 Comments on Wave Propagation I’ll end this relatively long chapter with comments on how electromagnetic waves propagate in a material, using the Lorentz and the Drude models as a basis for my comments.

56

Classical Theories for the Dielectric Function

Electromagnetic wave propagation (and reﬂection/transmission at interfaces) is governed by the dielectric function, which in turn sets the refractive index. A wave traveling along x is written ω

ω

ω

E = E0 ei (N c x−ωt ) = E0 ei (n c x−ωt ) e−κ c x with refractive index N=

√

and optical absorption coefﬁcient α=

2ω κ, c

(4.36)

which I already wrote as Eq. 3.26.∗

4.5.1 Insulators: Lorentz Model I will discuss wave propagation in the Lorentz model ﬁrst. In the discussion I’ll take the hierarchy of frequencies as ωp ωe γ = 1/τ . Even if the ratio of these quantities is only 3 or 5, I’ll consider the inequality satisﬁed. The dielectric function and refractive index are plotted again in Figs. 4.16. These functions are the same as those in Figs. 4.10 and 4.13. I have added vertical bars to separate the diagram into 4 parts, labeled A–D. Each of these has its own ﬂavor of wave propagation.

4.5.1.1 Mostly Transparent with Small Absorption Coefficient In Region A, 1 is positive and in fact larger than unity. Moreover, 1 2 and n κ. The solid is a transparent insulator with an absorption length (the inverse of α) that is longer than the wavelength, often much longer. The reﬂectance is governed largely by n; R ≈ [(n − 1)/(n + 1)]2 . Because n increases with frequency,† so does the reﬂectance. This behavior is termed “ordinary dispersion.”

4.5.1.2 Strongly Absorbing, Near the Resonance At the center of Region B, 2 1 , so that n≈κ=

2 1. 2

Waves are strongly damped, but currents and ﬁelds are more or less in phase. The damping length (δ or 1/α) and the wavelength differ by about 2π .

∗ Recall that the absorption coefﬁcient describes the attenuation of the intensity, I ∼ EE ∗ ∼ e−αx , in the solid

(x is the distance the wave has traveled); the factor of 2 comes from the fact that the ﬁelds are squared to give the intensity. † Believe me, it does. I know it is not obvious in the semilog plots of Fig. 4.16. I could make a better plot, or just 2 /(ω2 − ω2 ) as ω → ω from below. consider the approximation n2 ≈ 1 ≈ c + ωpe e e

57

Fig. 4.16

4.5 Comments on Wave Propagation

(Top) dielectric function and (bottom) refractive index for the Lorentz oscillator. The four regions A–D are separated by vertical lines. The boundaries are fuzzy, and the exact location of the lines is not to be taken seriously. Note that (as asserted in Chapter 1) “strongly absorbing” and “highly reﬂecting” go hand-in-hand here. To estimate the reﬂectance, I’ll start with Eq. 4.17: R=1−

4n , (n + 1)2 + κ 2

which becomes, near the resonance, R=1−

2 . κ

58

Classical Theories for the Dielectric Function 2 /ωγ so that the reﬂectance becomes Exactly on resonance, 2 = ωpe 8ωγ R=1− . 2 ωpe

This behavior is the equivalent of Hagen Rubens, Eq. 4.18, derived originally for metals in the far infrared. A Drude metal may be considered a Lorentz oscillator with a zero frequency resonance.∗ Around the middle of region B, the refractive index begins to decrease with increasing frequency. This behavior is termed “anomalous dispersion.”

4.5.1.3 Mostly Damped, ωe ω the Zero of 1 In Region C, 1 < 0 (negative) and |1 | 2 , so that n is a fraction of unity. and can be √ taken as close to zero. Then, κ ≈ |1 |. So long as the frequency is not too close to either 2 /ω2 and κ ≈ ω /ω. The wave the resonance or the zero crossing, I may take 1 ≈ −ωpe pe is strongly damped with 2ωpe 2ω κ= c c and a wavelength much larger than the vacuum wavelength. To estimate the reﬂectance, I need to estimate n. I will start with 2nκ = 2 and use 2 γ /ω3 and κ ≈ ω /ω (see above), so that n = ω γ /2ω2 . Then taking R from 2 ≈ ωpe pe pe Eq. 4.17 in the case where κ n, I arrive at α=

2γ 4n . R=1− 2 =1− ωpe κ The reﬂectance is independent of frequency. It is also high. Here the response is inductive, so the dissipation is not high; instead, most of the incident energy is reﬂected.

4.5.1.4 High Frequencies, Above the Zero of 1

2 /ω2 . The Here 1 is positive and bigger than 2 ; κ becomes small and n ≈ c − ωpe † material is transparent again. The reﬂectance has a minimum very close to the frequency where n = 1. Ordinary dispersion is recovered. The limiting high-frequency value of the reﬂectance is √ ( c − 1)2 . (4.37) R= √ ( c + 1)2

4.5.1.5 Really High Frequencies Equation 4.37 suggests that the reﬂectance is constant and remains that way as ω → ∞. But this suggestion is wrong. The high frequency “limiting” value of c is a crude ∗ A resonance at zero implies of course zero restoring force. † It would be exact except for the frequency dependence of κ.

59

Fig. 4.17

4.5 Comments on Wave Propagation

Refractive index for the Drude metal. Three regions B–D are shown by the vertical lines. The boundaries are fuzzy, and exact location is not to be taken seriously.

approximation for the polarizability of the ion cores of the atoms making up the solid. Atomic physics [22] tells me that there are a series of resonances with the dielectric function decreasing a bit above each one. At the very highest frequencies, ≈ 1 − ωP2 /ω2 where ωP = 4π nP e2 /me is a plasma frequency for every electron in the solid (whose density √ is nP ). As ω gets large, is just below unity and the refractive index is n = ≈ 1 − ωP2 /2ω2 . I then get R ≈ ωP4 /4ω4 .

4.5.2 Metals: Drude Model A plot analogous to Fig. 4.16 is shown in Fig. 4.17. Everything I said in sections B–D above applies here too. (There is no region analogous to section A in metals.) I can rewrite the relevant equations, replacing ωpe with ωp , γ with 1/τ , and setting ωe = 0.

4.5.2.1 Strongly Absorbing, ω 1/τ In metals, region B starts at zero frequency. At these low frequencies, 2 1 or σ 1 σ 2 . In this limit, n ≈ κ. I can write 1 ≈ −ωp2 τ 2 and 2 ≈

ωp2 τ ω

60

Classical Theories for the Dielectric Function

and

n=κ≈

ωp2 τ 2ω

=

2π σdc ω

where the last equality comes from σdc = ωp2 τ/4π . The dispersion is “anomalous” everywhere from ω = 0 to just below the screened plasma frequency. The ﬁeld decays as e−x/δ with c c2 2c2 ≈ δ= . (4.38) = ωκ 2π ωσdc ωp2 ωτ Eq. 4.38 is the classical skin depth of the metal. It correctly gives the penetration length in the low frequency limit, where σ1 (ω) ≈ σdc . I’ll return to the skin effect in Chapter 14. I’ll start with Eq. 4.17 but let n = κ 1 and write R = 1 − 2/κ. Then the reﬂectance becomes 8ω 2ω =1− . R=1− π σdc ωp2 τ This is what Hagen and Rubens found and what I wrote already in Eq. 4.18.

√ 4.5.2.2 Mostly Damped, 1/τ < ω < ωp / c In Region C, 1 ≈ −ωp2 /ω2 and κ ≈ ωp /ω. The wave has a wavelength much larger than the vacuum wavelength and is strongly damped with skin depth c c ≈ (4.39) δ= ωκ ωp and α=

2ωp 2ω κ≈ . c c

Anomalous dispersion for n continues. To estimate the reﬂectivity, I need to estimate n. I will start with 2nκ = 2 and use 2 ≈ ωp2 /ω3 τ and κ = ωp /ω, so that n = ωp /2ω2 τ . Then, taking R from Eq. 4.17 in the case where κ n, I arrive at 4n 2 , R=1− 2 =1− ωp τ κ

(4.40)

a frequency-independent reﬂectance.

4.5.2.3 High Frequencies, Above the Zero of 1 Here 1 is positive and quickly becomes bigger than 2 , i.e., 1 ≈ c − ωp2 /ω2 whereas 2 ≈ ωp2 /ω3 τ . The reﬂectance has a minimum very close∗ to the frequency where n = 1. ∗ It would be exact except for the frequency dependence of κ. Note that if and n = 1 then ≈ 1 also. 1 2 1

61

4.6 The Absorption Coefficient and a Not Uncommon Mistake

See Fig. 4.7. The limiting high-frequency value of the reﬂectance is

√ c − 1 2 . R= √ c + 1

(4.41)

The light that is not reﬂected is transmitted, as long as the sample is not too thick.∗

4.5.2.4 Really High Frequencies Equation 4.41 suggests that the reﬂectance is constant and remains that way as ω → ∞. But, see the discussion in Section 4.5.1; the high frequency reﬂectance is R ∼ 1/ω4 .

4.6 The Absorption Coefficient and a Not Uncommon Mistake Light traveling in an absorbing medium is attenuated; the amount of attenuation is governed by the extinction coefﬁcient κ, by the penetration depth δ, or, almost equivalently, by the absorption coefﬁcient α. Starting with Eqs. 3.26 and 4.36, these are related by α = 2/δ = 2ωκ/c. κ has no dimensions, α is in cm−1 in cgs units. After traveling a distance d, the intensity is reduced by a factor of e−αd . So it is tempting to say that the transmittance of a sample of thickness d is T ≈ e−αd .

(4.42)

If the reﬂectance is not large, this equation is a reasonable approximation; see the discussion in Chapter 7, Section 7.1.1, for the complete equation. But what I want to mention here is another case: strongly absorbing materials where κ n. This case corresponds to the upper half of region B and all of region C in Figs. 4.16 and 4.17. The decay length (the penetration depth or skin depth) is much less than the wavelength inside the solid, so that the picture in Fig. 3.1 does not represent the situation. The ﬁeld decays over lengths so short that the oscillating part of the ﬁeld is almost constant; oscillations are not observed. Were I to use Eq. 4.42 and calculate the absorption coefﬁcient from − ln(T )/d, I would be wrong. The reﬂection from the two surfaces is much more likely to govern the transmission than the absorption in the interior. Moreover, the sample is probably thinner than the wavelength, so that coherence of the multiple internal reﬂections needs to be incorporated into the solution. See the discussion in Section 7.2.

∗ How thick is too thick? Well, the intensity decays as e−αx so too thick is a few times larger than

1/α = c/2ωκ = nc/4π σ1 (ω) = δ/2.

5

Phonons

The atoms in a solid may be set to vibrating either by temperature or by external forces. One such force is the electric ﬁeld of light. For the ﬁeld to do anything, there must be a charge on the atom, where the charge is the sum of the positive nuclear and negative electronic charges. There is no need for there to be a charge, but most compounds, materials made up from two or more types of atoms, do have a certain amount of charge transfer from one type to another.∗ In the extreme case of ionic solids, like NaCl, valence electrons are transferred from one atom to the other. In NaCl, the sodium atoms have lost an electron and are present as Na+ while the chlorine atoms have gained an electron and are present as Cl− . NaCl is face-centered cubic, with each atom having six nearest neighbors of the opposite kind. These nearest neighbors are arranged at the corners of an octahedron surrounding the central atom. The bonding arises from the Coulomb attraction of the ions for their opposite-sign partners. Even though there are charged ions throughout the solid, there is no net polarization (P = 0) because of the symmetrical arrangement of nearest neighbors.† However, if an electric ﬁeld is applied, the positive ions will be pushed in the direction of the ﬁeld, and the negative ions will be pulled in the opposite direction, creating a net polarization. There is a natural vibrational frequency, the transverse optical phonon, at which these ions will oscillate and couple most strongly to an external electromagnetic ﬁeld. Here I will calculate the dielectric function contribution of these phonons. I’ll start with a completely oversimpliﬁed model and then work up to something a little better.

5.1 Harmonic Oscillator I’ll start with a simple harmonic oscillator model of a diatomic molecule. This system is shown in Fig. 5.1. The electrical force on the ions is F± = ±Z ∗eEloc , where ±Z ∗e is the effective charge of the ions and Eloc is the local ﬁeld at the ions. The ﬁeld, varying as e−iωt , affects the ion separation x.

∗ Even if the bonding is mostly covalent, there is usually a small charge difference across the bonds of dissimilar

atoms. It is this charge difference that leads to the infrared spectra of organic materials, an extremely important tool in analytical chemistry. † I know a counterexample: ferroelectrics. These solids lack inversion symmetry and have a spontaneous electric polarization below their Curie temperature.

62

63

5.1 Harmonic Oscillator

Fig. 5.1

The ionic force between a positive and a negative ion is represented by a spring. When light shines on the crystal, the spring is stretched and shrunk at the oscillation frequency of the light. The upper (lower) arrows show the force on the ions when the field is pointing right (left).

5.1.1 Equation of Motion Newton’s law is μ¨x = −μω02 x − μγ x˙ + Z ∗eEloc,

(5.1)

where μ is the reduced mass of the ions,∗ μω02 = K, the spring constant, and γ determines the strength of the damping force, which is proportional to the velocity. I’ll take Eloc = E + 4π P as before. Equation 5.1 is analogous to Eq. 4.20 for the Lorentz model, with a change of notation. The solution is then the analog to Eq. 4.21. I’ll write the induced dipole as p = Z ∗ex and deﬁne an ionic plasma frequency as 4π ni (Z ∗e)2 , p = μ where ni is the number density of ion pairs. The next step is to make the local ﬁeld correction, ﬁnding eventually the dielectric function for the optical phonons, the analog of Eq. 4.31: = e +

2p ωT2 − ω2 − iωγ

(5.2)

where e is the electronic contribution, including both the core electrons and the valence transverse optical phonon frequency, related to the dilute-limit electrons,† and ωT is the 2 resonance by ωT = ω0 − 2p /3. The dielectric function and other optical function for the Lorentz oscillator are plotted in Figs. 4.10–4.14. The functions for the vibrational absorption are the same Lorentzian, except that the frequency scale is different. The TO mode frequencies are typically at 40–600 cm−1 (6–100 meV or 1.6–25 THz).‡

∗ Relative motion! † Here I assume – as typically is the case for insulators where phonon features are seen in the optical spectra –

that the excitation energies for the electrons are much higher than the phonon energies, hω ¯ T. ‡ The modes for very light atoms, such as C−H or O−H can be as high as 3,300 cm−1 . The frequencies for vibrations in organic solids, such as the C−C, C=C, and C=O bonds, are in 800–1,600 cm−1 range.

64

Phonons

5.2 Lattice Dynamics Like any mechanical object, a solid has a set of normal modes or vibrations of the lattice. If I want to describe these modes in terms of the motions of the individual atoms, there are an enormous number of them. Fortunately there are lots of simpliﬁcations I can make and the problem is quite tractable and much closer to real physics than the two-masses-on-a-spring problem I solved in the previous section. The most important is that the solid is crystalline, i.e., it has translation symmetry in the placement of the atoms as well as (sometimes) other symmetries. I’ll discuss lattices and their symmetry in Chapter 15; for now I refer to solidstate physics texts [19, 23, 24]. I will still think in terms of springs and masses, but now the spring constant is not an actual spring but arises from the second derivative in a Taylor series expansion of the interatomic potential for the lattice. (The constant term can be suppressed by choosing the zero of energy and the linear term is zero because otherwise there would be an unbalanced force on the atoms and they would move to new equilibrium position where it was zero.) When quantized, the lattice vibrations are called “phonons” by analogy to photons. In fact I’ll seek plane wave solutions to the equations of motions. There are many physical effects due to the phonons, including a T 3 low-temperature speciﬁc heat, thermal conductivity in insulators, thermal expansion (due to anhamonicity), electron scattering in metals and semiconductors affecting the resistivity (and optical conductivity), and direct infrared absorption by certain vibrational modes. That the phonons are quantized is most easily proven by looking at neutron scattering and light scattering from them, processes that require them to have energy hω ¯ and momentum hk. ¯

5.2.1 Equations of Motion I’ll now consider the problem of phonons in a diatomic crystal. The geometry is sketched in Fig. 5.2. The ﬁgure shows a single line or chain of atoms arranged with equal separation and connected by springs with force constant K. The charges and masses alternate along the chain, negative atoms with mass M− and positive atoms with mass M+ . The springs are relaxed and each atom is at its equilibrium position, r = na xˆ for the negative ions and r = (na + a/2)xˆ for the positive ions. The lattice constant a is the length of the unit cell in the xˆ direction and there are two atoms per unit cell. Clearly, I have restricted the problem to nearest-neighbor forces only, as there are no springs going to more distant atoms.

Fig. 5.2

A line or chain of atoms in a crystal. Positive and negative atoms alternate along the chain, linked by springs. Each atom can move from its equilibrium position by an amount u. The springs are stretched or compressed by the vector difference in the motions.

65

5.2 Lattice Dynamics

Note that this appears to be a one-dimensional problem but I show vestigial springs leading to neighboring atoms above and below the atoms shown. Other springs can connect atoms above and below the plane of the ﬁgure. As Kittel [24] has argued, if entire planes of atoms move together along xˆ (parallel to the chain shown), or along yˆ or zˆ (perpendicular to the chain shown), one spring per atom is expanded and one compressed, just as in the one-dimensional case. (See the ﬁgures in his chapter on phonons.) Thus, especially for those diatomic crystals where each atom has six nearest neighbors (such as most of the alkali halides), the one dimensional model is a good representation of the three dimensional crystal. So now, let me set the atoms in motion. Each atom has a displacement from equilibrium, which I’ll denote as un,− for the negative ion in the nth unit cell and un,+ for the positive ion in the nth unit cell. These are both vectors, but if I consider displacements only along x, y, or z (or if I do a one-dimensional problem) I only need to keep track of the signs. Now, I could write equations of motion for the atoms from inspection∗ but instead I’ll use energy considerations. The reason is that writing the potential energy V and kinetic energy T and using Hamilton’s equations is much more easily extended to longer-ranged forces and more complex structures [19]. The potential energy is stored in the springs and the kinetic energy in the motion of the atoms. All I need is to specify these energies in one unit cell and then I can sum over cells for the total. The potential energy held by the nth cell is 1 1 K(un,− − un,+ )2 + K(un,+ − un+1,− )2 . (5.3) 2 2 The motion un,− also extends and compresses the spring between it and the positive atom to its left but that energy is allocated to unit cell n − 1. Note also that the energy (and the forces) depend on the difference in displacement of the neighbors. That suggests that long wavelength sinusoidal motion (where all neighbors undertake to move together) will have low frequencies and that motion where they move in opposite directions will have high frequencies. The kinetic energy of the nth cell is just Vn =

Tn =

2 2 pn,− pn,+ + , 2M− 2M+

(5.4)

where pn,j = Mj u˙ n,j is just the momentum of atom n,j with j counting atoms within the unit cell. (Here, j = ±.) The Hamiltonian is the sum of total kinetic plus potential energies: (Tn + Vn ). (5.5) H= n ∗ I would start with

Fn,− = −K(un,− − un−1,+ ) − K(un,− − un,+ ), and Fn,+ = −K(un,+ − un,− ) − K(un,+ − un+1,− ), for the nearest-neighbor forces as in Fig. 5.2. And then use Newton’s law.

66

Phonons

One of Hamilton’s equation (the one I need) applied to Eq. 5.5 is −p˙ n,− =

∂H ∂H and − p˙ n,+ = . ∂un,− ∂un,+

I have to be aware that there is a term containing un,− in Vn−1 and take that derivative too. I take the derivatives, collect terms, write p˙ n,j = Mj u¨ n,j , and get the equation of motion of the negative atom to be M− u¨ n,− = K(un,+ + un−1,+ − 2un,− ),

(5.6)

while the motion of the positive atom satisﬁes M+ u¨ n,+ = K(un,− + un+1,− − 2un,+ ).

(5.7)

5.2.2 Plane-Wave Solutions, Range of k, and Boundary Conditions I will seek plane-wave solutions to these equations. The reason for this choice∗ is that Eqs. 5.6 and 5.7 are those of a set of harmonic oscillators and I know that sines, cosines, and complex exponential functions solve the simple harmonic oscillator. I start with trial functions that are plane waves and which specify the displacement of the atoms from their equilibrium locations: un,j = u0 j ei (kna−ωt )

(5.8)

where u0 is the amplitude of the wave, j (with j = − or +) is the relative amplitude of atom j , and na = x, the distance of the start of unit cell n from the origin. The wave is traveling along the xˆ direction, but the motion j could in principal be along any of the Cartesian axes. I have started with a plane wave whose general form is u ∼ ei (kx−ωt ) . As I will show, this plane wave does the job and generates the relation between ω and k as well as the relative amplitudes and phases of the motion of the atoms. Initially, there is no obvious limit to the values that k could take on. But there is a well-justiﬁed upper limit to k that I should respect and it has to do with the ﬁnite spacing between the atoms. The motion of the atoms is all I can know about the vibrations in the crystal. In fact, it is the motion of the atomic nuclei that I can in principal measure and calculate. It makes little sense to talk about vibrations at places where no mass exists. That is why I restricted the values of x to x = na right at the beginning. If now I want to represent a sine wave by specifying the amplitude of the wave at a discrete set of points separated by distance a, I must satisfy the Nyquist criterion that at least two points per cycle of the wave are needed, so that λ ≥ 2a. The wavelength can be longer than this but not shorter. Another way of saying this is that if there is a sine wave that passes through a set of points, then there are many higher frequency sine waves that also pass through the points but oscillate also in the space between the points. If the longest wavelength going through the points is λ ≥ 2a, then the wave vector has magnitude |k| = 2π/λ ≤ π/a. The other waves that pass through the points have wave vector k ± n · 2π/a ∗ Other than that it has been shown to work and is in all the textbooks.

67

Fig. 5.3

5.2 Lattice Dynamics

A linear chain of N atoms is bent into a circle and the first and N th atoms are connected by a bond. The system is periodic with period N a. with n any integer. In the language of crystallography, the range −π/a < k ≤ π/a is the ﬁrst Brillouin zone of the reciprocal lattice of the crystal [19, 23, 24]. The values k = ±π/a are the zone boundaries of the linear chain. The range of k extends∗ over ∼ ±108 cm−1 . In contrast, the vacuum q vector for an infrared electromagnetic wave of ω = 160 cm−1 is q = 2π/λ = 103 cm−1 . Any lattice vibration with the same wavelength as the light wave is essentially at k = 0. Now I specify the boundary conditions. If the linear chain has ﬁxed ends, the solutions will be sines and cosines, i.e., standing waves. It is preferable to use “periodic boundary conditions.” I’ll write these mathematically (in one dimension) as un,j (x + L) = un,j (x),

(5.9)

chain.†

To be concrete, think about a one-dimensional chain where L is the length of the of N atoms. Such a chain is illustrated on the left side of Fig. 5.3. Then one connects the ﬁrst and N th atoms with a bond, bending the chain into a circle in order to make all bond lengths the same. Clearly, this loop satisﬁes Eq. 5.9 because the atomic displacements must be single valued and have the same value every time one goes once around the chain. This requirement means that k is quantized in steps of 2π/L.

5.2.3 The Dispersion Relation I put the function of Eq. 5.8 into the equations of motion (Eq. 5.6 and 5.7). The second derivative with respect to time brings down −ω2 . There are common factors of u0 and ei (kna−ωt ) that can be canceled. After doing these steps and collecting the coefﬁcients of j in a convenient way, I get (2K − M− ω2 )− − K(1 + e−ika )+ = 0,

(5.10)

−K(1 + e+ika )− + (2K − M+ ω2 )+ = 0.

(5.11)

and

∗ For NaCl, the repeat distance along the directions (the cube edges) is a = 5.64 A, ˚ so π/a = 5.57 × 107 cm−1 . † In three dimensions, I would make the displacements periodic along all three directions (x, ˆ y, ˆ or zˆ ).

68

Phonons

I have two equations and two unknowns. For there to be a solution, the determinant of the coefﬁcients has to be zero. Calculating the determinant gives: (2K − M− ω2 )(2K − M+ ω2 ) − K 2 (1 + e−ika )(1 + e+ika ) = 0 Working on the algebra of this equation, I ﬁrst use (1 + e−ika )(1 + e+ika ) = 2 + 2 cos ka. A bit more algebra and the trigonometric identity 1 − cos ka = 2 sin2 (ka/2) leaves ω4 − 2K

M− + M + 2 4K 2 ω + sin2 (ka/2). M− M+ M− M+

The reduced mass μ is μ = M− M+ /(M− + M+ ). (1/μ = 1/M− + 1/M+ .) The total mass (in the unit cell) is M = M− + M+ so that Mμ = M− M+ . These deﬁnitions simplify the equation above to ω4 −

2K 2 4K 2 ω + sin2 (ka/2) = 0, μ Mμ

which is quadratic in ω2 . The solution, after a bit of factoring, is K 4μ 2 2 sin (ka/2) . ω = 1± 1− μ M

(5.12)

The equation for ω(k), called the “dispersion relation” is found by taking the square root of both sides. Next, I can return to Eqs. 5.10 or 5.11 to ﬁnd the ratio of + to − . I choose Eq. 5.11: + 1 + eika = . 2 − 2 − M+ K ω

(5.13)

Note that the ratio is complex, indicating a phase difference between the motion of positive and negative atoms. In principal, I can substitute Eq. 5.12 to ﬁnd the ratio as a function only of k or invert Eq. 5.12 to ﬁnd k(ω) and substitute that to get the ratio as a function only of ω. I’ll do this where it helps but only in limiting cases. Moreover, because I have a free parameter u0 , I should have deﬁned a normalization for + and − that makes, say, the sum of their squares equal to one. Because the system is perfectly linear, it does not matter very much unless I need to constrain the total energy of the oscillations to some value. In several pages, I’ll write an equation relating the displacement to the electric ﬁeld of the light and this will set the values of the displacements.

5.2.4 Acoustic and Optical Branches For any value of k there are two values (called “branches”) of ω, one where I chose the minus sign in Eq. 5.12 and one where I choose the plus sign. Figure 5.4 shows the dispersion relation, ω vs. k. I’ve chosen parameters to give a frequency scale appropriate for sodium chloride. Cl is heavier than Na by a little more than a factor of 1.5 so that the ratio μ/M = 0.24. The two branches are quite different. The lower branch has zero frequency at k = 0, rises linearly, and then bends over to have zero slope at the zone boundary ±π/a.

69

5.2 Lattice Dynamics

Fig. 5.4

Dispersion relation for the phonons in a diatomic crystal. The acoustic branch is shown in blue and the optic branch in red. The k = 0 optical phonon frequency was chosen to match NaCl. The range of k shown is within the first Brillouin zone, which also is one full cycle of sin2 (ka/2). The upper branch has a high frequency (the highest in the ﬁgure) when k = 0. It decreases as k increases. The slope is zero both at k = 0 and at the zone boundary. There is a gap between the lower branch and the upper branch. No normal modes of the chain exist for frequencies in this gap.

5.2.5 Limiting Behavior Let me look at limiting behavior of each branch individually. I’ll start with the minus sign. The dispersion relation becomes ωa =

1/2 K 4μ 2 sin (ka/2) . 1− 1− μ M

(5.14)

The subscript a stands for “acoustic” and this branch carries sound waves. As k → 0 the sine can be replaced by its argument; the second term in the inner square root is small and I can expand it to give 1/2 2μ k 2 a 2 K 1− 1− , ωa = μ M 4 2K ka . (5.15) = M 2

70

Phonons

There is a linear relation between the normal mode frequency and the wave vector, making the product of the frequency and the wavelength (f λ) of the vibrations a constant. The √ constant is the speed vs of a sound wave in the crystal: vs = 2K/Ma/2, equivalent to the Debye model for the solid.∗ In the same limit, the displacement ratio becomes + 1+1 = 1, = − 2−0

(5.16)

showing that both atoms move together, in phase. When k = π/a, the sine is unity; this zone boundary frequency is the maximum possible for this branch. Equation 5.14 becomes 1/2 K 4μ . ωa = 1− 1− μ M If I substitute for μ and M and do a little simpliﬁcation, the term in square brackets becomes [] = [1 − M/M] where M is the mass difference between the two atoms. I now must specify which is heavier because M must be positive. (I made the choice that the square root itself is a positive quantity when I solved the quadratic equation.) Because NaCl is the prototype for phonons in an ionic crystal, I’ll take M− > M+ . With this choice, the zone boundary acoustic branch frequency is 2K . (5.17) ωa = M− Now I look at the case when I choose the plus sign. The dispersion relation becomes 1/2 K 4μ sin2 (ka/2) . (5.18) ωo = 1+ 1− μ M The subscript o stands for “optic.” This branch interacts with electromagnetic waves. As k → 0 the sine can be replaced by its argument; the second term in the inner square root is small and I can expand it to give 1/2 2μ k 2 a 2 K 1+ 1− , ωo = μ M 4 μ 2 2 2K 1− k a . (5.19) = μ 8M The optic mode has a very high frequency (the highest of all the normal modes) when k = 0, which I’ll call the transverse optic (TO) frequency 2K ωT = . (5.20) μ ∗ The various factors of 2 are unfamiliar if I only know the solution for the monatomic chain. But of course

M = M− + M+ and a = 2d where d is the distance between neighboring atoms. If the masses are identical, the monatomic chain result is returned.

71

5.2 Lattice Dynamics

The reason for this frequency being highest can be seen by looking at the displacement ratio. At k = 0, Eq. 5.13 is 1+1 + = . 2 − 2 − M+ K ωo I substitute ωo =

√ 2K/μ and after some algebra obtain + M− =− . − M+

(5.21)

The atoms vibrate in opposite directions with the lighter atom having the larger amplitude. This opposing motion gives maximal compression and expansion amplitude to the springs and therefore has the highest possible frequency. It also moves positive charge in one direction and at the same time negative charge in the opposite direction. A time-dependent dipole moment is generated in the chain, analogous to what is sketched in Fig. 5.1. I’ll therefore expect this k = 0 resonance to give rise to the Lorentzian dielectric function of Eq. 5.2. When k = π/a, the sine is equal to unity and ωo =

1/2 K 4μ . 1+ 1− μ M

Here the square bracket is [] = [1+ M/M]. Then (with, as before, taking negative heavier) I ﬁnd that the frequency at k = π/a, 2K . (5.22) ωo = M+ The optic-mode frequency is higher than the acoustic-mode frequency at any wave vector.

5.2.6 Phonon Notes Here I’ll just make a few random remarks about lattice dynamics and phonons. First, suppose the mass difference gets larger and larger, so M+ M− . When the masses are quite different the gap between the acoustic and optic branches becomes quite large. In addition, the reduced mass μ ∼ M+ , so the dispersion (the variation of ω with k) is small; the optical branch in a plot like Fig. 5.4 appears almost ﬂat. There are cases where the masses are all the same but the spring constants take two values. I could have a linear chain of carbon atoms with alternating single and double bonds. This example occurs as the polyacetylene chain, the ﬁrst highly conducting polymer. It can be schematically represented as −C = C−C = C−C = C− . (Each carbon has a hydrogen attached to it as well; from the side the chain takes a zig-zag form.) The double bonds are stronger than the single bonds and the lattice dynamics have an acoustic and an optic branch.

72

Phonons

Many solids have more than one phonon branch. As the chemical formula becomes more complex, the numbers of degrees of freedom increase. For the phonons, the key quantity is the number N of distinct atoms in the unit cell.∗ There is one for Ag, two for NaCl, and perhaps ﬁve for Al2 O3 . With N atoms in the unit cell, there are 3N degrees of freedom for the normal modes. Three of these are always the acoustic phonons, in which the entire unit cell moves as single unit, leaving 3N − 3 optical modes. The optical modes involve relative motion of the atoms within the unit cell. Although not all of these modes are infrared active, many are. For crystals with high symmetry, there are degeneracies. For example, the two transverse modes for a given k direction are degenerate in a cubic crystal but not degenerate in orthorhombic crystals. The effective charge on the ions, Z ∗e in Eq. 5.1 and to appear again in the next section, might naively be taken to be the charge of the closed shell ion. Then Na would have Z ∗e = +1, Ca would have +2, O −2, and Cl −1. This guess would not be too far off but it would not be very accurate. Instead, modern theories of electronic structure/lattice dynamics theories [25–27] can calculate the “Born effective charge tensor,” Zij∗ =

∂Pi e ∂dj

where is the primitive cell volume, Pi is the ith component of the dipole moment/unit volume, and dj is the j th component of the ion’s displacement vector. Many lattice dynamical computational programs will calculate the Born tensor.† The phonons are actually quantum mechanical objects. Phonons have no spin, so they obey Bose–Einstein statistics. It is straightforward to take the Hamiltonian of Eq. 5.5, view p and u as operators, Fourier transform them, and then replace with phonon creation and + annihilation operators a + and a to arrive at H = kν hω ¯ skν (askν askν + 1/2) where ν is the polarization (two transverse and one longitudinal) and s is the branch (acoustic, optic). The analogy to photons is good: there is a thermal spectrum, transport of energy, Compton scattering, Bremsstrahlung, and photoelectric-effect-like interactions.

5.3 Interaction with Electromagnetic Waves So now, I will add electromagnetic ﬁelds to the equation of motion for the lattice. I’ll take the electric ﬁeld to be the friendly plane wave with wave vector q and frequency ω: ˆ I add this to Eqs. 5.7 E = E0 ei (qz−ωt ) with z the direction of travel. Let E be parallel to x. and 5.6 M+ u¨ n,+ = K(un,− + un+1,− − 2un,+ ) + Z ∗eE, ∗ By “distinct” I mean atoms that occupy distinct crystallographic positions. Atoms can be distinct even if they

are the same element. For example, silicon, a monatomic solid, has two atoms per unit cell. Si has even got optical phonon branches, though not infrared active ones. † Google “Born charge.”

73

5.4 Transverse and Longitudinal Modes

and ¨ = K(un,+ + un−1,+ − 2un,− ) − Z ∗eE, M− un,− where Z ∗e is the Born charge of the ion. If I need to solve these equations for all values of phonon wave vector k, then the index n is critical. But if (as is the case here) the wavelength of the electromagnetic ﬁeld is much larger than that of the lattice, I can ignore the eika variation from site to site and therefore drop the index n. So these equations become u¨ + =

2K Z ∗e (u− − u+ ) + E, M+ M+

and −u¨ − =

2K Z ∗e (u− − u+ ) + E, M− M−

where I’ve divided through by the mass and changed signs in the second of these. Now add these, deﬁne 1/μ = 1/M+ + 1/M− and the equation for x ≡ u+ − u− is x¨ = −

Z ∗e 2K x+ E. μ μ

(5.23)

Using Eq. 5.20 makes it evident that Eq. 5.23 is identical to Eq. 5.1 (for the γ = 0 case). I want some damping and do not need to go through the solution again. The dielectric function is just the one given by Eq. 5.2, a Lorentz oscillator with damping. The reﬂectance of the Lorentz oscillator may be seen in Figs. 4.10–4.14. Some data for a few ionic solids will be shown in Chapter 6, Sections 6.5 and 6.6.

5.4 Transverse and Longitudinal Modes The phonon modes of a three-dimensional crystal may be separated into transverse and longitudinal modes [24]. Some modes are optically active but not all. Some are Raman active and some are “silent.” The selection rules can be determined by group theoretical analysis [28–30]. The infrared active modes are those that transform like the momentum (px , py , or pz ) or position (x, y, or z). In general, these are modes that are odd under inversion. (In the lingo of group theory, the infrared active modes are ungerade or uneven and carry the subscript u. Other modes are gerade or even with subscript g; these will be Raman active or inactive.) The infrared-active transverse optical (TO) modes are the resonant frequencies of the harmonic oscillator; for each of these there is a corresponding longitudinal optical (LO) mode. In the language of transfer functions in control theory [31], the transverse modes are the poles and the longitudinal modes are the zeros of the dielectric function.∗

∗ Just as the screened plasma frequency, ω /√ , is the zero of the Drude dielectric function. p c

74

Phonons

I discussed the plasma response of a metal in Section 4.3. The electrodynamics of the longitudinal mode of an insulator are similar. If the mode is longitudinal, then q is parallel to E. Thus, ∇ · E = 0. In the insulating solid, there is no free charge, so ∇ · D = 0. For linear materials, D = E, so ∇ · D = ∇ · E = 0. Because ∇ · E = 0, = 0. A further implication is: D = E = 0. But D = E + 4π P so that P = −E/4π . The frequency of the longitudinal mode is higher than that of the corresponding transverse mode. The reason for this difference is the long range Coulomb force that results from this polarization. I return to Eq. 4.26 (writing Eapp as just E) and put in the value of P from above to ﬁnd Eloc = −

8π P. 3

So if the positive atoms move to the right and the negative to the left along the x axis, P ˆ opposing the motion. In fact, because P is linear in the is along +xˆ and Eloc is along −x, displacement, this local ﬁeld is just like a spring. The result is an additional restoring force and a stiffening of the mode. One way to think about it is to realize that on the surfaces of a slab of ionic crystal, a polarization charge density σp = P · nˆ will appear. These surface charges are the sources of the electric ﬁeld that raise the LO frequency. I note that there is also a local ﬁeld correction of the TO frequency. This correction acts to reduce the TO frequency, as I discussed beginning in the context of the depolarizing ﬁeld, Section 4.4.2.

5.4.1 The Longitudinal Frequency The frequency of the zero of the dielectric function is easy to estimate. First, I’ll write Eq. 5.2 on a common denominator: = e

2p /e + ωT2 − ω2 − iωγ ωT2 − ω2 − iωγ

,

and next I deﬁne ω2L = 2p /e + ωT2 ,

(5.24)

ω2 − ω2 − iωγL = e 2L , ωT − ω2 − iωγT

(5.25)

so that

where I’ve put subscripts on the damping factors (relaxation rates) to suggest that different damping factors may affect the transverse and longitudinal modes. The real part of the dielectric function in Eq. 5.25 is zero at a frequency near ωL . The frequency is exactly ωL when the damping is negligible.

75

5.5 The Lyddane–Sachs–Teller Relation

5.5 The Lyddane–Sachs–Teller Relation In the limit as ω → 0, Eq. 5.25 becomes purely real:

ωL 2 1 (0) = e . ωT

(5.26)

Table 5.1 Transverse and longitudinal frequencies in solids, and the static and high-frequency dielectric constants. Transverse mode

Longitudinal mode

Mat’l

cm−1

THz

meV

cm−1

THz

meV

1 (0)

e

LiH LiF LiCl LiBr NaF NaCl NaBr KF KCl KI RbF RbI CsCl CsI TlCl TlBr AgCl AgBr MgO GaP GaAs GaSb InP InAs InSb SiC C Si Ge CaF2 SrF2 BaF2

584 308 191 159 239 164 133 191 143 101 154 74 101 64 64 43 101 80 398 366 271 228 302 218 186 790 1332 525 302 257 217 184

17.5 9.2 5.7 4.8 7.2 4.9 4.0 5.7 4.3 3.0 4.6 2.2 3.0 1.9 1.9 1.3 3.0 2.4 11.9 11.0 8.1 6.8 9.1 6.5 5.6 23.7 39.9 15.8 9.1 7.7 6.5 5.5

72.3 38.1 23.7 19.7 29.6 20.4 16.4 23.7 17.8 12.5 19.1 9.2 12.5 7.9 7.9 5.3 12.5 9.9 49.3 45.4 33.5 28.3 37.5 27.0 23.0 98.0 165.1 65.1 37.5 31.9 26.9 22.8

1114 637 398 324 414 265 207 324 212 138 286 101 164 85 159 101 180 133 743 403 292 244 345 239 196 950 1332 525 302 460 375 328

33.4 19.1 11.9 9.7 12.4 8.0 6.2 9.7 6.4 4.1 8.6 3.0 4.9 2.5 4.8 3.0 5.4 4.0 22.3 12.1 8.8 7.3 10.3 7.2 5.9 28.5 39.9 15.8 9.1 13.8 11.3 9.8

138.1 78.9 49.3 40.1 51.3 32.9 25.7 40.1 26.3 17.1 35.5 12.5 20.4 10.5 19.7 12.5 22.4 16.4 92.1 50.0 36.2 30.3 42.8 29.6 24.3 117.7 165.1 65.1 37.5 57.0 46.5 40.7

12.9 8.9 12.0 13.2 3.1 5.9 6.4 5.5 4.85 5.1 6.5 5.5 7.2 5.65 31.9 29.8 12.3 13.1 9.8 10.7 13.13 15.69 12.37 14.55 17.88 9.6 5.5 11.7 15.8 6.63 6.20 6.94

3.6 1.9 2.7 3.2 1.7 2.25 2.6 1.5 2.1 2.7 1.9 2.6 2.6 3.0 5.1 5.4 4.0 4.6 2.95 8.5 10.9 14.4 9.6 12.3 15.6 6.7 5.5 11.7 15.8 2.04 2.07 2.15

76

Phonons

This is the Lyddane–Sachs–Teller relation [32–35]. The static dielectric constant is larger than the high-frequency (electronic) dielectric constant by the square of the ratio of longitudinal to transverse frequencies. Data for a large number of insulating (and mostly ionic) solids are in Table 5.1, adapted from Kittel [24].

5.6 Other Notations The zero-frequency limit of Eq. 5.2 is 1 (0) = e +

2P ωT2

.

This expression for the static dielectric constant is of course equivalent to Eq. 5.26 given the deﬁnition of ωL in Eq. 5.24. Sometimes it is of interest to highlight the fact that 2P /ωT2 is the (additive) contribution to the static dielectric constant. Then one deﬁnes either = 1 (0) − e or the so-called oscillator strength S as

≡ S ≡

2P ωT2

.

(5.27)

The dielectric function Eq. 5.2 in terms of S is then = e +

SωT2 ωT2 − ω2 − iωγ

.

(5.28)

5.7 Multiple Modes In solids with more than 2 atoms per unit cell, each infrared-active mode will contribute to the dielectric function. I’ll model it as a sum of Lorentz oscillators just as in the case of multiple electronic orbitals. (See Chapter 4; Section 4.4.10.) Equation 5.2 becomes = e +

2pj

j

2 − ω2 − iωγ ωTj j

2 Sj ωTj

j

2 − ω2 − iωγ ωTj j

,

(5.29)

.

(5.30)

while the equivalent Eq. 5.28 is = e +

In Eqs. 5.29 and 5.30, I’ve written the resonant frequency as ωTj rather than ωj . Sometimes one sees one such notation and sometimes the other.

77

5.7 Multiple Modes

By analogy, Eq. 5.25 is written 2 − ω2 − iωγ ωLj Lj

= e j

2 − ω2 − iωγ ωTj Tj

,

and the Lyddane–Sachs–Teller relation, Eq. 5.26, generalizes to

ωLj 2 . (0) = e ωTj

(5.31)

(5.32)

j

Each oscillator contributes to the static dielectric constant, with the ones at the lowest frequencies dominant. If a mode goes “soft” (i.e., its frequency goes to zero as temperature or some other parameter is varied), the dielectric constant will diverge; such soft modes may be found in ferroelectric and almost-ferroelectric crystals. There are interesting interactions among the poles and zeros of the dielectric function when there are two or more modes. The effect is illustrated in Fig. 5.5. The four panels show the real dielectric function, real conductivity, the loss function, and the reﬂectance calculated starting with the dielectric function give by Eq. 5.29. The solid has two modes, a strong optical phonon with ωT 1 = 300 cm−1 , p1 = 1,800 cm−1 (S1 = 36), and γ1 = 4 cm−1 . There is a weak mode that I have given one of two TO frequencies. For the left column of plots it is at ωT 2 = 150 cm−1 and for the right column at ωT 2 = 600 cm−1 . The other parameters are p2 = 200 cm−1 (so S2 = 1.8 when the mode is at 150 cm−1 and 0.11 when it is at 600 cm−1 ), γ2 = 2 cm−1 , and e = 1.5. The real part of the dielectric function shows two of the usual derivative-like excursions. In the left panel, the weak mode has a small range of frequencies where it is negative, from 150 to 152 cm−1 , while the strong mode has a wide range, from 300 to 1,509 cm−1 . (The LO frequencies are 152 and 1,509 cm−1 .) The two modes have poles at the TO resonance frequencies, seen as peaks in σ1 , and zeros at the LO frequencies, seen as peaks in − Im(1/). Finally the reﬂectance is high for frequencies where 1 (ω) < 0 with dips toward zero near the LO frequencies.∗ It is natural to associate the ﬁrst pole and ﬁrst zero with the phonon having the lower TO frequency and the second pole and second zero with the phonon with the higher TO frequency. For the case on the left in Fig. 5.5 this natural interpretation is correct. But for the case on the right, the ﬁrst zero is really associated with the weaker mode, and occurs at a lower frequency than the pole. The behavior of 1 (ω) near the TO2 frequency is shown in the little cartoon at the right of Fig. 5.5. The dielectric function 1 is negative and disperses upward as the TO2 frequency is approached. It crosses through zero just below the TO2 frequency and then, at the resonance, steps down to a minimum and then eventually returns to approach the curve that would be found if the mode did not occur. So it is correct to say that the zero of the weaker mode is below the pole and to continue to assign the zero at 1509 cm−1 to the stronger mode. The consequence of the narrow region where 1 (ω) > 0 is a sharp dip in the reﬂectance. ∗ The dips are at frequencies a bit higher than the zeros of (ω) because they occur where n = 1 rather than 1

where 1 = 0. If there is no damping, the dips reach zero but if there is some damping, the reﬂectance is always above zero.

78

Phonons

Fig. 5.5

Optical functions for a phonon system with both a strong and a weak vibrational mode. Top to bottom, the panels show 1 (ω), σ1 (ω), − Im(1/), and R. 1 (ω) is also shown magnified by 20 as the dashed lines. The left panels are for the case where the TO frequency of the weak mode is below the TO frequency of the strong mode and the right panels are for the case where the weaker mode is above the strong mode. The fragment on the right shows 1 (ω) around ω = 600 cm−1 for the case where the weak mode is above the strong mode (blue solid line) and where it is below it (red dashed line). The horizontal line is the level where 1 = 0. This behavior, where there are narrow dips in the highly reﬂecting reststrahlen region, is seen in many perovskite materials [36–38], some cuprates [39], and other highly polar materials. The same effect occurs in doped polar semiconductors when the plasma frequency of the free carriers is a bit above the LO frequency of an optical phonon [40].

5.8 Polaritons An electromagnetic wave traveling in a material with 1 = 1 induces a polarization P in the material. In the case where the polarization is due to the optical phonons, there is physical motion of the atoms. The wave is a coupled combination of electromagnetic waves

79

5.8 Polaritons

and lattice vibrations, or the coupled motion of photons and phonons. This coupled mode is called a “polariton.” Polaritons actually occur for any wave traveling in a polarizable medium, but the relatively narrow linewidth of the phonon resonances (a few cm−1 ) makes them a good vehicle for discussing these effects. It is fair to ask about the condition required to make these effects important. There are a number of criteria I could construct. The simplest one is to think for a moment about the electric displacement vector D. In general, D = E + 4π P and for linear, homogeneous, and isotropic materials, with P = χ E and χ = ( − 1)/4π (the dielectric susceptibility). So then D = E + ( − 1)E and the polarization is the larger component of D once > 2. The analysis is clearer (and the math easier) if I neglect the damping. So I’ll use Eq. 5.25, setting the damping terms to zero: ω2 − ω2 . = e L ωT2 − ω2 This function is purely real.∗ In turn, the refractive index N = ω2 − ω2 . N = n + iκ = e L ωT2 − ω2

(5.33) √

is (5.34)

When > 0, N is real and waves propagate without attenuation at a phase velocity given by v = c/n. When < 0, N is purely imaginary, and the ﬁelds in the crystal are exponentially damped with attenuation length δ = c/ωκ. What I want is the dispersion relation, the dependence of the frequency ω upon the wave vector q for light propagating in the polar material. I already know the dispersion relation for the phonons; it is given by Eq. 5.12 and plotted in Fig. 5.4 The last couple of sentences in the previous paragraphs signal what the physics is: the wave propagation is governed by n and n grows without bound as ω → ωT from below. Wave speed will become slower and slower. The region of highly damped waves is between ωT and ωL . Above ωL , there are again propagating waves; these are anomalous in that the phase velocity is greater than c until the frequency is high enough that n ≥ 1. To ﬁnd the dispersion relation, I’ll return to Eq. 3.3, Maxwell’s equations for local, nonmagnetic, linear, isotropic, and homogeneous media, and consider plane wave functions √ for the ﬁelds. The answer is in Eqs. 3.9 and 3.10: q = (ω/c) = (ω/c)N . I square both sides and use Eq. 5.33 to obtain q2 =

2 − ω2 ω2 e ωL , 2 2 c ωT − ω2

(5.35)

as an equation relating q to ω. But what I want is ω(q). Equation 5.35 is quadratic in ω2 and the solution is

2 2 2 2 ωL c2 q 2 c2 q 2 1 2 2 + c q ωL + ± − 4ωT2 . ω = 2 2e 2 e e ∗ What happens at ω = ω is implicit in discussions in Chapter 10. For the moment, I’ll just avoid that single T frequency. (The answer is that there is a delta function in the imaginary part 2 (ω) at ω = ωT .)

80

Phonons

Fig. 5.6

Dispersion relation for light traveling in an ionic crystal with a single transverse optic mode. The TO and LO optical phonon frequencies, as well as the high-frequency dielectric constant were chosen to match NaCl. The range of q and k shown is very small compared to the width of the first Brillouin zone. The dispersion relations for light in a medium √ √ with n = 1 (0) and with n = c and the dispersion relations for LO and TO phonons are also shown. For each value of q, there are two frequencies of propagating waves. One (the lower; choose −) is between zero and ωT and the other (the upper; choose +) is between ωL and ∞. A plot of the dispersion relations for photons (electromagnetic waves) and for phonons (lattice waves) is shown in Fig. 5.6. Note that the wave vector range shown is much smaller than the range in Fig. 5.4. If I wanted to plot the dispersion over the entire Brillouin zone but with the same detail as in Fig. 5.6, the diagram would be almost 10,000 times wider. The lower branch starts just as would the case where there was no coupling of photons and phonons, with a slope governed by the refractive index as ω → 0, n = 1 (0). The dispersion in this uncoupled case is shown as a dashed line. But as the frequency approaches the transverse optical phonon frequency, ωT , the polariton dispersion curve bends over and becomes eventually tangent to the TO phonon curve shown. There are no propagating modes between ωT and ωL . Above the LO frequency, the polariton dispersion starts again. The dielectric function is only a little bit positive so that n 1. The dispersion is tangent to the LO phonon curve for a while and then bends upward, eventually rising linearly with the same slope as the case when there was no coupling of photons and phonons. The high frequency propagation is governed by the high √ frequency refractive index, n = c .

6

A Look at Real Solids

Chapters 4 and 5 have given me a framework to discuss optical spectra. I show in this chapter spectra for some metals, a semiconductor, and some ionic insulators, discussing them within this framework. Some of the concepts in Chapters 8–12 will be foreshadowed in this chapter. I think it is helpful to see examples of actual metals, semiconductors, and insulators before diving into the quantum-based theories and that’s why this chapter is here and not later in the text.

6.1 Silver Silver is an elemental metal. The atomic conﬁguration of the 47 electrons in the silver atom is 1s 2 2s 2 2sp6 3s 2 3p6 3d 10 4s 2 4p6 4d 10 5s 1 . The 5s electron is the “free” electron of the metal, so I expect one mobile electron per atom. The 4d levels are 4 eV below the 5s level in the atom [41, 42]. Silver has high reﬂectance in the visible. Indeed, it is the standard for a shiny metal; other things with high reﬂexivity are called “silvery.” An example of “typical” silver reﬂectance data is shown in Fig. 6.1. The data are those collected by Palik [43–53]. The low frequencies are supplemented by a Drude reﬂectance, based on resistivity ρ = 1.63 μ-cm at 300 K. The main panel shows the reﬂectance from 20 to 80,000 cm−1 (2.5 meV–10 eV). One can see the high metallic reﬂectance from far-infrared to near ultraviolet, a sharp and deep plasma edge around 32,000 cm−1 (4 eV), and the transitions from the d-bands to the conduction band above the plasma edge [45, 54]. The reﬂectance at higher photon energies, extending to 1,000 eV, is shown in the inset of Fig. 6.1. Here, one can see additional interband transitions followed by sharp core-level atomic transitions. Note that the reﬂectance above 100 eV (∼ 800,000 cm−1 ) is pretty close to the expected ω−4 power law. I’ll use the Drude model to describe the optical properties of the free-electron metal silver (and many other metals). The high “metallic” reﬂectance and plasma edge are similar to the Drude model reﬂectance in Fig. 4.7. A ﬁt to the silver data gives a plasma frequency of ωp = 71,600 cm−1 (8.88 eV) and a scattering rate of 1/τ = 138 cm−1 (τ = 38 fs).∗ The real and imaginary parts of the optical conductivity,† σ1 (ω) and σ2 (ω), are shown in Fig. 6.2. The real part, σ1 , equals the DC conductivity (610,000 −1 cm−1 ) at zero ∗ I must remember to multiply frequencies in cm−1 by 2π c to get radians/s before inverting. † The conductivities and other optical functions have been calculated using Kramers–Kronig analysis of the

reﬂectance to obtain the reﬂection phase. See Chapter 10.

81

82

A Look at Real Solids

Fig. 6.1

Reflectance of silver [43–53]. The main panel shows the reflectance from far infrared to near ultraviolet on a logarithmic frequency scale. The inset shows the vacuum-ultraviolet and soft x-ray reflectance. The straight green line follows ω−4 .

Fig. 6.2

Real and imaginary parts of the optical conductivity of silver. Inset: real part of the conductivity continued up to frequencies where the interband transitions occur. frequency. It rolls off as frequency increases and becomes quite small above about 1,000 cm−1 . Looking at the inset, where the scale is expanded, I can see that it falls to values of a few hundred −1 cm−1 (probably the limit of accuracy of the measurement). A set of absorption bands begins at 32,000 cm−1 (4 eV) and extend to above 80,000 cm−1 (10 eV).

83

6.1 Silver

The imaginary part, σ 2 , is initially smaller than the real part. It rises (while the real part is falling) and the two functions are equal near ω = 140 cm−1 , the frequency where σ 1 has fallen to half its DC value and where σ 2 has its maximum. Above this frequency, σ 2 falls, but is larger than σ 1 . The peak of σ 2 and the half power point of σ 1 booth occur at ω = 1/τ in the Drude model. I can see by comparison with Fig. 4.1 that the Drude model describes silver metal well. Indeed, the data and ﬁts to the data give 1/τ = 138–140 cm−1 , essentially the same value I calculated in Chapter 4, Section 4.2.4 from the DC conductivity and carrier density. All solids have electronic bands and interband transitions from ﬁlled to empty states are part of the optical spectrum. These interband transitions in silver are responsible for the features that begin at 4 eV (32,000 cm−1 ) and are seen in Fig. 6.1 (inset) up to perhaps 300 eV. I’d use one or more Lorentz oscillators (Eq. 4.31) to represent these interband transitions. In silver the lowest energy interband transitions involve transitions of d electrons to the conduction band. The inset of Fig. 6.2 illustrates one issue with using Lorentz oscillators for the interband transitions. The conductivity spectrum shows an almost step-like onset at 4 eV. In contrast, as can be seen from Eq. 4.34 and Fig. 4.12, the Lorentz dielectric function starts at zero when ω = 0 and increases as ω2 well below the resonance. The sudden onset of interband transitions is easy to understand. There is a minimum energy spacing of the band, equal to the distance between the top of the occupied band and the bottom of the empty band.∗ Consequently the contribution of the interband transitions to the conductivity spectrum is zero until the photon energy exceeds this spacing. The Lorentz oscillator does not represent this onset well at all. I can use many narrow oscillators if I want to ﬁt data; it is not easy to see what the parameters of the ﬁt tell me about the solid. If a Drude model is correct for silver below the interband transitions, I expect large and negative values for the real part of the dielectric function. Silver does not disappoint in this regard; 1 , shown in Fig. 6.3, is indeed large and negative. The limiting low-frequency value is −ωp2 τ 2 = −275,000. As it should, it begins to roll up as ω approaches 1/τ . At higher frequencies, it follows 1 = c − ωp2 /ω2 , as appropriate for free carriers. It crosses zero around 31,000 cm−1 (just under 4 eV). (A 20,000× magniﬁed view of the zero crossing is in Fig. 6.3.) There is considerable structure above the zero crossing qualitatively in accord with multiple Lorentz oscillators from the interband transitions. The real and imaginary parts of the refractive index are plotted in Fig. 6.4. The refractive index of silver resembles closely the Drude model calculation show in Figs. 4.5 and 4.6. At low frequencies, n and κ are almost the same, in accord with Eq. 4.16. With increasing frequency, both become smaller and n becomes quite a bit smaller than κ. n < 1 between 3,000 and 30,000 cm−1 , where 1 changes sign. Unlike the model of Figs. 4.5 and 4.6, κ does not fall above the zero crossing. There is additional absorption due to the interband transitions. Now, I look at the area under the curve of σ1 (ω). I can guess from the inset to Fig. 6.2 that there will be two contributions to this area: the Drude peak that starts at zero frequency

∗ Or the highest occupied level in the partially-occupied band, as is the case in silver.

84

A Look at Real Solids

Fig. 6.3

Real part of the dielectric function of silver.

Fig. 6.4

Real (n) and imaginary (κ) parts of silver’s refractive index. and falls off to a small value by 5,000 cm−1 (0.6 eV) and the interband transitions that begin at 32,000 cm−1 (4 eV) and extend above 100,000 cm−1 . This integral, known as the sum rule, will be discussed in Chapter 10. For the moment, let me integrate Eq. 4.10a: 0

∞

σ1 (ω ) dω =

∞

0

ne2 τ/m π ne2

. dω = 2m 1 + ω 2 τ 2

85

Fig. 6.5

6.2 Other Noble Metals

(m/m∗ )Neff (ω) of silver. I can turn this into an equation for the number Neff of electrons per copper atom with effective mass ratio m/m∗ participating in optical transitions at frequencies below ω by writing 2mVc ω m N (ω) = σ1 (ω ) dω , (6.1) eff m∗ π e2 0 where to allow for the effective mass being different from the electronic mass, I have included the factor m∗ /m, the ratio of the effective mass of the charge carriers to the free electron mass. The quantity Vc is the unit cell volume (or formula volume); the carrier density is n = Neff /Vc . Finally, I put the upper limit to ω rather than ∞, allowing me to plot the integral versus the upper limit ω. If the conductivity spectrum consists of a number of isolated bands, I will be able to see a series of steps in (m/m∗ )Neff (ω) as the upper limit passes through the bands, with ﬂat segments between. Figure 6.5 shows the result of evaluating Eq. 6.1 over 0–80,000 cm−1 (5 mev–10 eV) for the conductivity data in Fig. 6.2. For a simple metal like silver, the free carrier spectral weight is exhausted quickly, in the midinfrared, and the function saturates at the number of conduction electrons/atom (1 in the case of Ag) until the interband transitions set in [45, 54]. Note that the integral saturates at (m/m∗ )Neff (ω) = 1.04, a quite satisfactory result [45].

6.2 Other Noble Metals The reﬂectance of copper [43, 50, 55, 56] and gold [43, 57, 58] are compared to silver in Fig. 6.6. The three metals share a column in the periodic table. Copper and gold have electronic conﬁgurations similar to silver, except that the d levels are not so deep.∗ These metals also have high infrared reﬂectance and similar free-carrier optical conductivity and dielectric function spectra. The absorption from the d levels has onset in the red (copper) or ∗ And, of course, the outermost electron is in a 4s orbital for copper and in a 6s orbital for gold.

86

Fig. 6.6

A Look at Real Solids

Reflectance of copper [43, 50, 55, 56], gold [43, 57, 58], and silver [43–53]. yellow (gold) regions of the visible, and the reﬂectance falls from the high metallic value seen in the infrared to a lower value at this onset. This drop is responsible for the characteristic colors of these metals. Moreover, the “plasma minimum” is not so deep in copper and gold as in silver. A Drude–Lorentz model can describe their optical properties, with several oscillators ﬁtting the interband transitions and a Drude model for the free carriers.

6.3 Aluminum Aluminum is a trivalent atom (1s 2 2s 2 2p6 3s 2 3p1 ) and, as a metal, all of the electrons in the n = 3 level are free carriers, making the carrier density (and the plasma frequency) high. Now, I know that each Brillouin zone of a crystal can hold two electrons per atom, so the free carriers occupy two zones. This fact complicates the electronic properties somewhat, but a Drude model with three electrons per atom is a good starting point for describing the optical properties. The far-infrared–ultraviolet reﬂectance spectrum [43, 50, 59–61] of Al is shown in Fig. 6.7. The main panel shows data from 70 to 50,000 cm−1 (0.01–6.2 eV) whereas the inset shows the vacuum ultraviolet and X-ray reﬂectance up to 6 × 106 cm−1 (800 eV). A trivalent metal, Al has its plasma edge deep in the vacuum ultraviolet, around 140,000 cm−1 /17 eV. In addition, aluminum has a weak interband transition in the infrared [61, 62]. The optical conductivity in the infrared is Drude-like. The far-infrared value of the conductivity is σ1 (ω) = 340,000 −1 cm−1 . It rolls off as frequency increases. A ﬁt gives ωp = 139,000 cm−1 (17.3 eV) and 1/τ = 930 cm−1 (τ = 5.7 ps). Figure 6.8 shows the conductivity of Al, plotted only up to σ1 = 30,000 cm−1 (about 9% of the low frequency conductivity). Using this scale emphasizes the 1/ω2 fall off when ωτ > 1 and shows the interband transition at 13,600 cm−1 (1.7 eV). This band is reasonably well ﬁt by a Lorentz oscillator.

87

6.4 Silicon

Fig. 6.7

Reflectance of aluminum [43, 50, 59–61]. The main panel shows the reflectance from far infrared to near ultraviolet whereas the inset shows the vacuum-ultraviolet and soft x-ray reflectance.

Fig. 6.8

Optical conductivity of aluminum.

6.4 Silicon Silicon is an elemental semiconductor. The atomic conﬁguration of the 14 electrons in the Si atom is 1s 2 2s 2 2p6 3s 2 3p2 but in the crystal the outermost four electrons are hybridized to form equivalent covalent bonds to four neighboring Si atoms; this tetrahedral

88

A Look at Real Solids

coordination gives crystalline Si the same face-centered cubic (fcc) structure as diamond, with two Si atoms per unit cell. A semiconductor, such as silicon, germanium, GaAs, and many other materials, is to my mind just an insulator with a smallish energy “gap” between the highest occupied and the lowest unoccupied electronic orbitals in the crystal. In Si, this gap at 300 K (“room temperature”)∗ is Eg = 1.11 eV = 8950 cm−1 . A consequence of the smallish gap is that the Boltzmann factor e−Eg /kT governing the probability of a thermal excitation to the unoccupied energy levels is small but not zero. The consequence is that very pure† semiconducting silicon has a ﬁnite resistivity, better than ρ = 2,000 -cm at room temperature. This value is a billion times less conductive than good metals like silver but a trillion times better than really good insulators like Teﬂon. From the refractive index at long wavelengths [63, 64], I see that the static dielectric constant is positive: 1 (0) = 11.66 at 300 K. Silicon’s value as the basis of electronic materials comes from the ability to control its electrical properties by the incorporation of atoms such as phosphorous, arsenic, or boron in the crystal. Each of these “dopant” atoms adds to the mobile charge density; at maximum dopant atom concentration of about 2 × 1020 cm−3 (about 0.4%) one ﬁnds about 500 μ−1 cm−1 for the resistivity [65]. This heavily doped material has electrical and optical properties of a metal.‡ I’ll discuss here the optical properties of pure silicon. Even if the impurity concentration is well above that of the most pure materials, it is not high enough to affect the far-infrared– ultraviolet reﬂectance. Figure 6.9 shows the 300 K reﬂectance of silicon [43, 66–71]. The main panel shows the reﬂectance from far infrared to near ultraviolet. The long wavelength reﬂectance is R = 0.3 and is almost constant with frequency, rising slightly as frequency increases. This is the reﬂectance expected for a Lorentz model well below the resonance. See Fig. 4.14. The reﬂectance is completely determined by the real part of the dielectric function, consistent with Eq. 4.32a and Fig. 4.10. See also Fig. 4.13. As frequency increases, the reﬂectance also increases, rising to a series of maxima in the ultraviolet, at 27,500, 37,000, and (broad) 60,000 cm−1 (3.4, 4.6, and 7.4 eV). At still higher frequencies the reﬂectance falls, eventually following the ω−4 behavior of free electrons. (See the inset.) The optical conductivity is shown in Fig. 6.10 and the real part of the dielectric function in Fig. 6.11. The conductivity is zero (or very small) at low frequencies but rises to give a series of peaks in the ultraviolet as in the reﬂectance. The maximum value of the conductivity (27,000 −1 cm−1 ) is below the DC conductivity of silver or other good metals (600,000 −1 cm−1 ) but considerably above the maximum in the interband region of silver (3,000 −1 cm−1 ) or aluminum (9,000 −1 cm−1 ). The details of the conductivity spectrum are determined by the electronic band structure of silicon [72–76]. See Chapter 12 for some more discussion and also see the chapters on semiconductors in solid-state ∗ The gap is slightly temperature dependent, increasing to 1.17 eV at T = 0. † Nothing is perfectly pure, but Si crystals can be had with impurity concentrations of 1 × 1012 cm−3 or 20

impurity atoms for every trillion silicon atoms.

‡ More common doping levels are in the range 1013 –1018 cm−3 . At the higher values metallic properties already

are observed.

89

6.4 Silicon

Fig. 6.9

Reflectance of silicon [43, 66–71]. The main panel shows the reflectance from far infrared to near ultraviolet whereas the inset shows the vacuum-ultraviolet and soft x-ray reflectance. The straight line in the inset follows ω−4 .

Fig. 6.10

Optical conductivity of silicon. textbooks [19, 23, 24]. The peaks correspond to high-spectral weight transitions from the ground state (the valence band) to the excited state (the conduction band). The conductivity spectrum resembles in some ways that of a Lorentz oscillator (Fig. 4.12) – or perhaps as a sum of several overlapping oscillator dielectric functions. It is small at low frequencies, is large in the visible and ultraviolet, and then falls off at higher frequencies. There are differences as well. Most notably, the low frequency edge of

90

Fig. 6.11

A Look at Real Solids

Real part of the dielectric function of silicon. the spectrum is very steep whereas the high frequency falloff is rather gentle. The Lorentzmodel conductivity rises as ω2 while the conductivity of Si rises much more rapidly. This edge is seen more clearly in the inset, where the conductivity is plotted using a logarithmic frequency scale. The conductivity is offscale low in the midinfrared region and rises very steeply at 9,000 cm−1 (1.1 eV). This energy corresponds to the energy band gap of Si. A weak low-frequency peak in the conductivity can be seen in the inset. This absorption occurs between 400 and 1,200 cm−1 (50–150 meV) with considerable structure and is attributed to vibrational overtones, i.e., multiphonon processes. At still lower frequencies a free carrier (Drude) conductivity contribution appears, with the conductivity in the m−1 cm−1 range. That the transitions have high spectral weight is conﬁrmed by the real part of the dielectric function (Fig. 6.11). At low frequencies, ≈ (0) = 11.66. The dielectric function increases monotonically to a maximum near 27,000 cm−1 (3.3 eV), falls with some structure, and becomes negative at 34,000 cm−1 (4.2 eV). There is a minimum a bit above this frequency, and (ω) remains negative over a wide range of frequencies, ﬁnally crossing zero at 132,000 cm−1 (16.4 eV). The negative region of 1 is similar to that of a metal below its plasma frequency. The extinction coefﬁcient κ is large and there is a region where n < 1. But there is high absorption in the region where is positive when frequencies are above the energy band gap, on account of the large value of σ1 (ω).

6.5 Sodium Chloride Sodium chloride (NaCl) is an insulating ionic compound composed of ions of Na+ and Cl− . NaCl is representative of about 20 alkali halides, ranging from LiF to CsI. The alkaline

91

6.5 Sodium Chloride

earth halides, like BaF2 , have quite similar optical properties. The cohesive energy of these crystals is due to the Coulomb attraction of the oppositely charged ions. Both ions are closed shell and the lowest electronic interband transitions are in the ultraviolet region of the spectrum. Most (including NaCl) crystallize in the fcc structure; a few (such as CsI) are body-centered cubic (bcc). The reﬂectance of NaCl [43] is shown over a wide frequency range in Fig. 6.12. The spectrum has electronic transitions across the band gap in the ultraviolet as well as a vibrational peak (transverse-optical or TO phonon) in the infrared. The maximum reﬂectance in the infrared reststrahlen region exceeds 90%, a value that is in the realm of metallic reﬂectance. The minimum near the longitudinal optical (LO) phonon frequency is very close to zero. A Lorentz model ﬁts this feature well, although the structure in the region where the reﬂectance is falling quickly with increasing frequency indicates some deviations from the simple harmonic oscillator. The reﬂectance spectrum in the ultraviolet is more intricate. There are both sharp peaks and broader features. The energy scale is quite high, 50,000–160,000 cm−1 (6–20 eV). These feature are seen better in the optical conductivity spectrum, shown in Fig. 6.13, and in the dielectric function, Fig. 6.14. The lowest-energy feature in the electronic absorption conductivity shows a very strong and narrow peak at 62,500 cm−1 (7.75 eV), with additional broad and sharp features at higher energies. The sharp peak leads to the usual derivative-like signature in the dielectric function. This peak is attributed to an exciton. Excitons are described in Chapter 12, Section 12.10. The exciton is a localized bound state of an electron–hole pair. Because there is a ﬁnite binding energy, it requires less energy to produce the exciton than to promote an electron to the conduction band. I can think of the electron in the conduction band and the hole left

Fig. 6.12

Reflectance of NaCl [43]. The reflectance is shown from far infrared to the ultraviolet.

92

A Look at Real Solids

Fig. 6.13

Optical conductivity of NaCl. The inset shows the infrared region on an expanded scale.

Fig. 6.14

Real part of the dielectric function of NaCl. behind in the valence band as free carriers. These interband transitions appear at just higher energies than the exciton energy in Fig. 6.13. The optical phonon feature that was so prominent in the reﬂectance is a modest feature in the optical conductivity.∗ The phonon spectrum is shown expanded in the inset to ∗ Had I plotted , then the phonon feature would reach ≈ 95 and would have dwarfed the ultraviolet 2 2 electronic peaks. 2 = 4π σ1 /ω and the factor of almost 500 between the frequencies of the phonon and of

the electronic transitions has a big effect.

93

6.6 Other Alkali Halides Fig. 6.13; the peak at the transverse optical phonon frequency, 164 cm−1 , is quite narrow, with a full width at half maximum of about 5 cm−1 and a peak height of about 260 −1 cm−1 . The phonon is quite evident in the dielectric function, with a strong derivative-shape and a rapid change from a large positive value to a large negative value through the resonance (the TO frequency) and a zero crossing back to positive at a higher frequency (the LO frequency). The additional dipole moment available by polarizing the lattice is evident from the larger value of 1 below the resonance than the value above the resonance. The same thing happens across the electronic transitions. It is fair to ask why a material with a conductivity of 260 −1 cm−1 has a reﬂectance not much smaller than that of a metal, for which σ1 ≈ 105 −1 cm−1 . The answer is that it is not the value of the conductivity that matters. Instead, it is the fact that 1 is negative, combined with a small value of 2 over much of the range where R is large. A negative 1 (and small 2 ) means that the refractive index n is small but the extinction coefﬁcient κ is large, making the reﬂectance close to unity. See Eq. 3.33 or, maybe better, Eq. 4.17.

6.6 Other Alkali Halides The optical properties of other alkali halides are very similar to those of NaCl, although of course there are different quantitative values for the parameters. Figure 6.15 shows the optical conductivity spectra of CsI, KBr, NaCl, and LiF and Fig. 6.16 shows their dielectric functions. The frequency of the TO phonon is lowest for CsI and highest for LiF. This behavior is √ completely understandable, because the solution to Eq. 5.1 has a resonance at ω0 = K/μ

Fig. 6.15

Optical conductivity of CsI, KBr, NaCl, and LiF.

94

Fig. 6.16

A Look at Real Solids

Real part of the dielectric function of CsI, KBr, NaCl, and LiF.

Table 6.1 Transverse and longitudinal frequencies in four alkali halides, and the static and high-frequency dielectric constants. Material

ωT cm−1

ωL cm−1

γ cm−1

e

1 (0)

LST 1 (0)

CsI KBr NaCl LiF

62.5 115 164 307

90 159 267 665

3 5 5 17

3.04 2.36 2.25 1.92

5.65 4.58 5.90 9.04

6.30 4.55 5.96 9.01

with K the spring constant and μ the reduced mass. The higher the reduced mass, the lower the frequency. Of course, the force constant K also plays a role, and CsI is softer than LiF, with a lower sound velocity. The behavior of 1 is not monotonic with the mass. The high frequency value is in the order LiF:NaCl:KBr:CsI, consistent with the band gaps of these compounds. (I’m thinking that for ω well below the resonance ωe , the dielectric function of the Lorentzian is 1 (ω) 2 /ω2 . I’m ignoring any variation of plasma frequencies—which there is no doubt.) = 1+ωpe e But the low frequency (as ω → 0) 1 is in the order KBr:CsI:NaCl:LiF. I look at Eq. 5.26 and know that it must be a very large value for ωL that makes the LiF have such a large 1 (0). It is straightforward to read off the relevant parameters from the data in Figs. 6.15 and 6.16. The peak in σ1 occurs at ωT . The zero above the resonance∗ of 1 is at ωL . The

∗ There is another zero right at the resonance as changes sign from positive to negative. 1

95

6.6 Other Alkali Halides

value of 1 at the lowest measured frequency gives 1 (0). The value of 1 well above the resonance∗ gives e . I did what I just described for the data in Figs. 6.15 and 6.16. The results are shown in Table 6.1. The last column shows the static dielectric constant calculated from the Lyddane–Sachs–Teller relation, Eq. 5.26. The agreement is poor for CsI but for the other three compounds, the LST static dielectric constant is within 1% of the measured value. ∗ This value is not as easy to pick as the other parameters. The dielectric function is monotonically increasing

between resonances. See Fig. 4.15; note that it changes from concave down to concave up between the resonances. This inﬂection point is a good place to deﬁne the high frequency limiting value.

7

Transmission and Reflection

Now that I’ve gone through semiclassical models of metals and insulators and have looked at data for some common materials, I’ll discuss an experiment to learn about their optical properties. I want to know how light of different frequencies propagates in the material. I’ve discussed the propagation of light in a solid, starting with Section 3.4 in Chapter 3. The propagation is governed by the complex refractive index or, equivalently, the complex dielectric function. A cartoon of typical experimental setups was shown in Fig. 1.3. To learn about my sample, I need to send light at wavelength λ (or frequency ω) from some optical device (laser, spectrometer, interferometer) to the sample, where some if it will be reﬂected (see Section 3.6) and some will cross the surface and begin to travel in the solid. If the sample is very thick, so that the light has little chance to make it to the back surface,∗ the reﬂectance (Eq. 3.33) is all one can measure. See Chapter 10 for discussion of Kramers–Kronig analysis of this “single-bounce” reﬂectance. Here, I want to consider the right-hand side of Fig. 1.3. A signiﬁcant fraction of the light makes it all the way through the sample, where its intensity may be measured to ﬁnd the transmittance T (ω). Of course some light also is reﬂected (from both surfaces), so I can move the detector to the other side and measure also the reﬂectance R(ω) of the sample.†

7.1 Incoherent Light I’ll begin by considering the case of a slab that is thick compared to the wavelength. Moreover, it has some slight variation in thickness across the beam. The thickness variation is a few wavelengths, so that I can combine intensities and not consider coherence (interference) until later. Figure 7.1 shows a diagram of the paths taken by light as it passes

∗ I know the scale for “very thick”: the electric ﬁeld of light is attenuated as E∼e−ωκx/c at a distance x into the sample; the intensity goes as I = I0 e−αx . So if the thickness d is large compared to c/ωκ or 1/α, the ﬁeld or intensity is e−large when the light reaches the back surface. In this case, the reﬂected light comes entirely

from the ﬁrst surface. In the other limit, where d < 1/α, the light that reaches the back surface will be in part reﬂected. Some of that light will pass through the front surface and become a component of the reﬂected ﬁeld. † The reﬂectance of the partially transmissive sample contains contributions from both front and back surfaces. In contrast the opaque sample returns only the single-bounce reﬂectance. The distinction is important for analysis if reﬂectance using the Kramers–Kronig relations: one must analyze the sample and correct for the extra light coming from the back surface before beginning the Kramers–Kronig analysis.

96

97

7.1 Incoherent Light

Fig. 7.1

Multiple internal reflections in a slab with refractive index Nb and thickness d set between semi-infinite media with refractive indices Na and Nc . The intensity in each successive pass is smaller than the one before it, indicated in cartoon form by the fainter lines of the last few rays. through a slab of thickness d. The light is incident from the left.∗ At the ﬁrst surface, some if the incident light is reﬂected, and some transmitted. This transmitted light passes through and some exits from the rear side. The rest is reﬂected, and then bounces back and forth between front and back, with a fraction leaking out of each surface on each pass.

7.1.1 The Transmittance To set up the problem, I’ll follow the paths of the individual rays shown in Fig. 7.1. I will take the refractive index of the semi-inﬁnite media on both sides to be the same, Na = Nc . Let the incident ray have unit intensity. The reﬂected intensity at the front surface (sometimes called the prompt reﬂectance) is Rab , where the subscripts mean “from a onto b.” The amplitude reﬂectivity rab is given by Eq. 3.30 and the reﬂectance is |rab |2 2 2 Na − Nb 2 = (na − nb ) + (κa − κb ) . Rab = (7.1) Na + Nb (na + nb )2 + (κa + κb )2 The intensity just inside the slab at the front surface is 1 − Rab because there is no absorption at the interface. There is, however, absorption as the light travels through the slab, following Eq. 3.25, I = I0 e−αx . When the light reaches the rear surface, some is reﬂected. The fraction reﬂected is Rbc = Rab . Some, = 1 − Rab , is transmitted. Thus, the intensity of the ﬁrst ray exiting from the slab is T 1 = (1 − Rab )e−αx (1 − Rab ), consisting of reﬂection losses at both surfaces and bulk absorption. I will now follow the other rays that lead to transmission. The second ray travels three times through the sample and has intensity T 2 = (1 − Rab )e−αx Rab e−αx Rab e−αx (1 − Rab ). ∗ The diagram shows the rays inside the slab at an angle to the slab normal; I’ll work out the case for normal

incidence. I drew the oblique incidence to allow me to follow the various partial waves as they travel back and forth in the sample.

98

Transmission and Reflection

It is transmitted at the front, passes through the slab, is reﬂected, passes through, is reﬂected, passes through, and is transmitted. The third ray is T 3 = (1 − Rab )e−αx Rab e−αx Rab e−αx Rab e−αx Rab e−αx (1 − Rab ). It is transmitted at the front, passes through the slab, is reﬂected, passes through, is reﬂected, passes through, is reﬂected, passes through, is reﬂected, passes through, and is transmitted. Now note that T 2 and T 3 both contain all the factors in T 1 multiplied by R2ab e−2αx and R4ab e−4αx respectively. The next term has of course the 6th power of Rab e−αx , and the total transmittance is an inﬁnite sum of the partial rays. The transmittance is then T = (1 − Rab )2 e−αx [1 + R2ab e−2αx + R4ab e−4αx + · · · ]. Now, I remember the expansion of 1/(1 − ε) = 1 + ε + ε2 + · · · , which converges as long as ε < 1. Clearly Rab < 1 as is e−2αx , so the series is convergent. I sum it to get T =

(1 − Rab )2 e−αx 1 − R2ab e−2αx

.

(7.2)

7.1.2 The Reflectance I can use the same approach for the reﬂected rays: R1 = Rab, and R2 = (1 − Rab )e−αx Rab e−αx (1 − Rab ), and R3 = (1 − Rab )e−αx Rab e−αx Rab e−αx Rab e−αx (1 − Rab ). Now I keep R1 separate and add all the partial rays for R2 , R3 . . . R∞ together, factor out common terms, and ﬁnd an inﬁnite series almost the same as in T . The reﬂectance is: R = Rab + Rab

(1 − Rab )2 e−2αx 1 − R2ab e−2αx

.

(7.3)

The second term is positive, so that the slab reﬂectance is larger than the single-bounce reﬂectance Rab .

7.1.3 Some Approximations A common case is the one where κ 1. Why should I say that? Well, the absorption coefﬁcient is α = 2ωκ/c = 4π κ/λ. Suppose the slab thickness is d = 10λ. This is about as thin as it can be and still be considered “thick.” In this case, αd ≈ 120κ, where I’ve used

99

7.2 Coherent Light the old fashioned approximation π ≈ 3. The transmittance is (neglecting reﬂection at the surfaces) T ≈ e−120κ . Now I want to get light through the slab, at least at the 1% level. So I take T = 0.01 and ﬁnd −120κ = ln(0.01). Thus κ = 0.037, and is indeed rather small. The advantage of having small κ is that I can neglect it∗ in Eq. 7.1. Assuming vacuum before and behind the slab, I take Na = Nc = 1 and write Nb = n, making Rab = (n − 1)2 /(n + 1)2 . Substituting this expression into Eq. 7.2 and doing a little algebra, I ﬁnd T =

16n2 . (n + 1)4 eαd − (n − 1)4 e−αd

(7.4)

Eq. 7.4 simpliﬁes further if instead of having small κ, I have zero κ. Then α = 0 and the transmittance simpliﬁes to 2n . T = 2 n +1

(7.5)

Eq. 7.5 has the correct limit when n = 1. Note that it is different from the transmission across the ﬁrst surface, T 1 = 1 − R1 = 4n/(n + 1)2 , which represents the intensity just inside the layer if the back surface is not there. More importantly, Eq. 7.5 is larger than T 1 T 2 = T 21 = 16n2 /(n + 1)4 , the intensity of the ray transmitted without reﬂections through the slab. The multiple internal reﬂections augment the transmitted intensity by about 7% if n = 3 and by 80% if n = 10. They should not be neglected.

7.2 Coherent Light If the material is thin, or if it is thick but the two surfaces are parallel to within a fraction of a wavelength, then the multiple internal reﬂections will add coherently; the consequences are that there are interference patterns (or standing wave effects) in the transmitted and reﬂected light [8, 77]. Layers with thicknesses corresponding to the wavelength will usually show these effects; they are responsible for the iridescent colors in an oil ﬁlm on water [78], for the light scattered off of the wings of certain insects [79], and for many other examples in nature. But it is not necessary for the layer to be comparable to the wavelength. The arm cavities of LIGO [80] are 4 km in length whereas the laser wavelength is 1 μm; nevertheless, the mirrors are held so parallel by a complex and effective control system that there is constructive interference of the light bouncing back and forth between the mirrors even though they are separated by 4 × 109 wavelengths. In the coherent case I must add the amplitudes of the ﬁelds† and, after ﬁnding the ﬁeld resulting from superposing the components, I calculate the intensity or the Poynting vector

∗ Actually, I will be neglecting κ 2 , which is about 0.0014 in this example. † One typically adds the electric ﬁeld and lets the magnetic ﬁeld come along for the ride.

100

Transmission and Reflection in order to ﬁnd out about the energy.∗ One must keep track of the phase of the ﬁelds as the light propagates; the phase advances as eiq for travel along the path . There are also phase changes on reﬂection or transmission across an interface.

7.2.1 The Geometry I’ll start by deﬁning the geometry, illustrated in Fig. 7.2. This diagram is not much different from Fig. 7.1; I show the amplitude (not the intensity) of reﬂected and transmitted partial waves. The layer has thickness d and refractive index Nb . It is sandwiched between media with indices Na and Nc . I’ll take the origin of the x-axis (along which the wave travels) at the front surface; the back is at x = d. A plane wave of unit amplitude is incident at normal ˆ iqa x with qa = Na ω/c. As long as the media incidence from the right medium: Einc = ee are isotropic, I can ignore the ﬁeld direction. I’ll evaluate the ﬁelds at x = 0 and x = d, either inside or outside the layer. The ﬁrst surface has reﬂection coefﬁcient rab , as derived in Chapter 3, Eq. 3.30, rab =

Na − Nb , Na + Nb

and transmission coefﬁcient tab , Eq. 3.31, tab =

2Na . Na + Nb

There are equivalent equations for rbc , rba , tbc , and tba . In each of these, subscripts like ab mean “incident from a into b.”

Fig. 7.2

Amplitude transmission and reflection of a layer with thickness d and refractive index Nb between media with indices Na and Nc .

∗ Actually, one should always combine the ﬁelds coherently. The incoherent case arises because the light is in

a beam wide compared to the wavelength. If the sample thickness varies over this beam dimension, then the phase differences among the combined waves will vary in the same way, with some parts adding constructively and some destructively. An average over these phases gives the resultant transmittance and reﬂectance.

101

7.2 Coherent Light

7.2.2 Transmission Coefficient Now, I will follow the various partial rays to ﬁnd their sum, the transmitted ﬁeld. I start in medium a, at the surface (x = 0). For ray t1 the light is transmitted across the ab interface, travels a distance d, and is transmitted across the bc interface. The ﬁeld is then t1 = tab eiqb d tbc . Some of the light is reﬂected at the back surface and travels to the front surface where some of it is reﬂected and travels to the back surface where some if it is transmitted. Starting with the incident ﬁeld, I ﬁnd that t2 is t2 = tab eiqb d rbc eiqb d rba eiqb d tbc = tab rbc rba tbc e3iqb d = t1 rbc rba e2iqb d . The third partial ray is t3 = t1 (rbc rba e2iqb d )2, because the ray has made ﬁve passes across medium b, internally reﬂecting twice at each surface. Thus, just as in the discussion leading to Eq. 7.2, the multiple internal reﬂections lead to an inﬁnite series, which I can sum to get t, the amplitude transmission coefﬁcient of the layer. t=

tab tbc eiqb d . 1 − rbc rba e2iqb d

(7.6)

7.2.3 Reflection Coefficient An identical analysis (see Eq. 7.3) gives the amplitude reﬂection coefﬁcient of the layer, r r = rab +

tab rbc tba eiqb d . 1 − rbc rba e2iqb d

(7.7)

7.2.4 Intensities The transmitted and reﬂected intensities (transmittance and reﬂectance) are just the absolute value squared of these amplitude coefﬁcients: T = tt ∗

and

R = rr ∗ .

(7.8)

The phase term in the numerator of the transmitted amplitude disappears when multiplied by its complex conjugate,∗ but the denominator contains terms like cos(2n ωc d). The transmittance therefore has oscillations as a function of the frequency or the thickness, with period 2nωd/c = 2π (2d/λin ). Here 2d is the round-trip path length and λin is the wavelength of the light in the slab. ∗ The exponential function containing κ does not disappear of course, and the quantity e−αd appears in the

numerator of T .

102

Fig. 7.3

Transmission and Reflection

Transmittance and reflectance of a slab of “LiF”using a linear frequency scale.

7.2.5 An Example: An Ionic Insulator As an illustration Figs. 7.3 and 7.4 show the calculated transmittance of a material with a strong harmonic oscillator, such as an optical phonon, in its dielectric function. The media on either side of the material are both taken to have Na = Nc = 1. The parameters for layer b are chosen to resemble those of LiF. The dielectric function is the product dielectric function of Eq. 5.25, ω2 − ω2 − iωγL = e 2L ωT − ω2 − iωγT with ωL = 662 cm−1 , ωT = 307 cm−1 , γL = γT = 2 cm−1 , c = 1.5 and d = 0.01 cm. The oscillations in T and R are obvious. They occur below ωT and above ωL . Because the refractive index is larger below ωT than above ωL ∗ the period is smaller and the amplitude larger at low frequencies than at high. In the transparent regions the maxima in reﬂectance correspond to minima in transmittance.† It is not obvious in the ﬁgure, but the period of the oscillations becomes shorter as the frequency is increased from zero to ωT because the refractive index is increasing as the resonance is approached. The transmittance is zero and reﬂectance high in the reststrahlen region where 1 (ω) < 0. The dielectric function becomes positive at ωL = 662 cm−1 , but the reﬂectance has its minimum at about 1,000 cm−1 , the frequency where n = 1. Because the damping in the model is low, one can see interference oscillations in the transmittance and reﬂectance at frequencies below the reﬂectance minimum. ∗ n ≈ 2.6 at low frequencies and ≈ 1.2 at high frequencies. † Energy is conserved; some is absorbed at frequencies near ω . T

103

Fig. 7.4

7.2 Coherent Light

Transmittance and reflectance of a slab of “LiF”using a logarithmic frequency scale.

7.2.6 A Second Example: A Metal Film As a second example, I’ll calculate the transmittance of a thin metal ﬁlm. The ﬁlm will have to be very thin for any light to get through. It is likely that the ﬁlm is thin enough that electron scattering from the surface becomes important, decreasing the conductivity. In the calculations here, I will ignore this likelihood; the optical properties will be those shown in Figs. 4.1 (conductivity) and 4.3 (dielectric function). The parameters for the Drude model are given in Chapter 4, Section 4.2.7; they are meant to mimic silver metal at room temperature. ˚ The results of the calculation are shown in Fig. 7.5 for thicknesses of 10, 30, and 100 A. The transmittance is very low at low frequencies and decreases as the square of the ﬁlm thickness. The ﬂat spectrum continues until ω ≈ 1/τ . Above this frequency the transmittance increases, following approximately T ∼ ω2 . At high frequencies the transmittance approaches 100%. The thinner ﬁlms reach high transmittance at lower frequencies than the thicker ﬁlms do.

7.2.7 Layer Transmittance and Reflectance It is certainly possible to ﬁnd analytic equations for the transmittance and reﬂectance – what one measures – from Eqs. 7.6, 7.7, and 7.8 but it may not be proﬁtable to slog through the algebra involved. Instead, let me make a number of simpliﬁcations. First, I’ll take Na = Nc = 1, i.e., put vacuum on both sides of the layer.∗ I can then write Nb = N , without subscript. Moreover, by symmetry rba = rbc and tba = tbc . Note that these ∗ This simpliﬁcation is not really justiﬁed: many samples consist of a thin ﬁlm on a thick substrate. That case is

additionally complicated in practice by the fact that the ﬁlm is thin and hence coherent whereas the substrate is thick, and incoherent.

104

Fig. 7.5

Transmission and Reflection

Transmittance of a metal meant to represent silver. The calculated transmittance curves for three thicknesses are shown versus frequency. Both axes use a logarithmic scale. coefﬁcients represent what happens when the light is incident on the vacuum from within the material. Then I have from Eqs. 3.30 and 3.31 N −1 = −rab N +1 2N = 1 + rba = N +1 2 = 1 − rba = N +1

rba = tba tab

and Eq. 7.6 becomes (after substituting and multiplying top and bottom by (N + 1)2 e−iqd ), t=

4N (N + 1)2 e−iqd − (N − 1)2 eiqd

(7.9)

whereas Eq. 7.7 becomes (after substituting, multiplying top and bottom by (N +1)2 , combining both terms on a common denominator, doing some algebra, and then multiplying top and bottom by e−iqd , r=

2i(1 − N 2 ) sin(qd) . (N + 1)2 e−iqd − (N − 1)2 eiqd

(7.10)

7.2.8 Nonabsorbing Layer If now the layer is nonabsorbing (κ = 0), the transmittance, tt ∗ , becomes (starting with Eq. 7.9, manipulating the denominator, and making use of the double-angle formula) T =

4n2 . 4n2 + (n2 − 1)2 sin2 (nωd/c)

105

7.2 Coherent Light This Airy function has minimum transmittance when sin2 (nωd/c) = 1

2 2n T min = n2 + 1 and maximum transmittance when sin2 (nωd/c) = 0 T max = 1. The reﬂectance is R=

(n2 − 1)2 sin2 (nωd/c) 4n2 + (n2 − 1)2 sin2 (nωd/c)

with maximum Rmax

2

2 n −1 = n2 + 1

and minimum Rmin = 0. The medium is nonabsorbing; consequently energy conservation tells me that T + R = 1. The period of the oscillations in T and R is the distance between the zeros of sin2 (nωd/c), which occur when nωd/c = J π where J is an integer. Thus πc . (7.11)

ω = nd Here the frequency is in radians/s, ω = 2πf , with f the frequency in Hz. Eq. 7.11 then becomes f = c/(2nd). Finally, if the frequency is in cm−1 , ν = f/c = 1/λ, and 1 , (7.12) 2nd with d in cm. Each period corresponds to adding one more cycle to the standing wave inside the layer. Observation of these multiple-internal-reﬂection in a measurement allows for a simple, if coarse, determination of the refractive index. One picks out the transmittance maxima and calculates 1 , (7.13) n(ν) = 2 νd where ν is the spacing between two adjacent maxima and ν is the average of their frequencies. The resolution can be improved by a factor of two by carrying out the same procedure for the minima. Figure 7.6 shows a calculation of the transmittance of a nonabsorbing layer with variation of the refractive index (top to bottom) from 1.4, 2, 4, 8, 16, to 32. The thicknesses were adjusted to keep nd constant: 70.7, 50, 25, 12.5, 6.25, and 3.125 μm.∗

ν =

∗ I note that a refractive index of 32 (dielectric constant of 1024) is uncommon. But the same effect – a high

reﬂectance at the interfaces – can be achieved by applying multilayer dielectric coatings to the surfaces of a low index spacer.

106

Transmission and Reflection

Fig. 7.6

Transmittance of a layer having a refractive index (top to bottom) of 1.4, 2, 4, 8, 16, and 32 and thickness of 70.7, 50, 25, 12.5, 6.25, and 3.125 μm respectively. Note that the maximum transmittance is independent of the refractive index or reﬂection coefﬁcient of the vacuum-material interface; it is always unity∗ when the partial waves for the multiply-internally-reﬂected light all add constructively (see Fig. 7.2.). As the reﬂection coefﬁcient of the surfaces increase, the minima between the 100% transmittance peaks become deeper and deeper, and the shape of the transmittance spectra, which is close to sinusoidal for low reﬂection surfaces, becomes more and more a set of narrow peaks between low transmittance regions. This spectrum is the Airy function transmittance of a Fabry–Perot interferometer. I’ll not plot the reﬂectance, but I can imagine it by looking at Fig. 7.6 because I know (energy conservation!) that R = 1 − T . So for n = 1.4, the reﬂectance would oscillate between zero and about 10%; the reﬂectance maxima correspond to transmittance minima. For n = 32, the reﬂectance exceeds 99% over much of the spectrum, punctuated by narrow dips to zero when the partial waves inside interfere constructively. The material with n = 32 has a single-surface reﬂectance (n − 1)2 /(n + 1)2 = 0.88. So it is reasonable to ask: how can a slab with two such highly reﬂecting surfaces in series have transmittance equal to 1 and zero reﬂectance? The answer of course is “For most frequencies it does not.” But in the special case where all the partial waves interfere constructively, the energy stored in the slab grows enormously. Some of this energy leaks out of the front surface with a phase that is 180◦ out of phase with the light promptly reﬂected; the two sum to the zero reﬂectance. Some light also leaks out of the back and energy conservation tells me that this leakage is equal to the incident intensity, making T = 1. ∗ Assuming no absorption!

107

7.3 The Matrix Method

7.3 The Matrix Method The use of “ABCD” matrices to calculate wave propagation appears in a variety of guises, such as to follow Gaussian laser beams through lenses, mirrors, and other optical components [81, 82]. Here, I’ll discuss how it is done for multilayer thin ﬁlms [8, 77, 83]. I will do this for normal incidence; the extension to oblique incidence is relatively straightforward. The method resembles the way one solves the barrier penetration problem in quantum mechanics. Instead of following each partial ray as I did in Fig. 7.2 and in the analysis leading to Eqs. 7.6 and 7.7, one considers a forward-going wave and a backwards-going wave in the barrier and in the medium from which the waves come. Matching boundary conditions then gives the solution. So I will (conceptually at least) combine all the forwardgoing waves in Fig. 7.2 into one and will do the same thing with all the backwards-going waves. The geometry is shown in Fig. 7.7. There are L layers in the ﬁlm, each with refractive index N and thickness d . The total number of media is then L + 2 because the light enters the ﬁlm from a semi-inﬁnite space on the left and leaves into a semi-inﬁnite space on the right. The total number of interfaces is L + 1, and these are numbered 0 . . . L according to the medium on the left of the interface. Thus, interface 2 (between medium 2 and 3) is at x = d1 + d2 when the origin is in interface 0 and the light is propagating along the x axis. The ﬁelds are given by Eqs. 3.11 and 3.12, which I rewrite below: ! ω ω ω E0 ein c x e−κ c x ≡ Ef (forward), ˆ iN c q·r = (7.14) E = E0 e −in ωc x +κ ωc x E0 e e ≡ Eb (backward), where qˆ = xˆ for forward and qˆ = −xˆ for backward. I have incorporated the e−iωt time dependence into E0 (or evaluated everything at t = 0).

Fig. 7.7

A multilayer optical system. There are L layers in the film, each with complex refractive index N . The triplets of arrows indicate the q, E, and H vectors of forward-going light (to the right) and backward going light (to the left). Labels are on only some of the electric field vectors. All electric field vectors are along +yˆ although in reality there will be phase reversals at some (but probably not all) reflections.

108

Transmission and Reflection

Some of the light is reﬂected and some transmitted at each interface. The coefﬁcients are given in Eqs. 3.30 and 3.31. I rewrite these here, substituting the interface number for the letters used previously: r,+1 =

N − N+1 = −r+1,, N + N+1

and t,+1 =

2N N + N+1

t+1, =

2N+1 , N + N+1

where a subscript like , + 1 means “incident from into + 1.” Now, let me focus on one interface, say interface 1, which separates medium 1 from 2. Light approaches the interface as forward-going in medium 1, which I will write as Ef (1), and as backward-going in medium 2, Eb (2). Some of each incoming beam is transmitted and some reﬂected, so there are four outgoing waves, which superimpose into two ﬁelds for light leaving the interface: Ef (2) = t1, 2 Ef (1) + r2, 1 Eb (2), Eb (1) = r1, 2 Ef (1) + t2, 1 Eb (2). As the light travels from one side of a single layer to the other it picks up a phase (and a change of amplitude) according to Eq. 7.14, which I will write as ω

Ef (x = d) = Ef (x = 0)eiN c d ≡ Ef (x = 0)eiφ , and ω

Eb (x = 0) = Ef (x = d)e−iN c d ≡ Ef (x = d)e−iφ , where for each layer, φ = N (ω/c)d . So now I’ll combine both of these factors into equations for the th interface: Ef ( + 1) = t,+1 Ef ()eiφ + r+1, Eb ( + 1), Eb ()e−iφ = r,+1 Ef ()eiφ + t+1, Eb ( + 1).

(7.15)

The left sides of these equations give the amplitudes of the waves leaving interface in terms of the waves approaching it, including the phase. If I use r,+1 = −r+1, and 2 t,+1 t+1, = 1 − r,+ 1 which I can prove from Eq. 3.30 and 3.31, I can write Eq. 7.15 in matrix form,

Ef ( + 1) Ef () = M , (7.16) Eb () Eb ( + 1) where the transfer matrix M is a 2×2 matrix that takes me from one layer to another. In turn, M is conveniently written as a product of a propagation matrix P and an interface matrix I , M = P I,

(7.17)

7.4 Inverting R and T to Find

109

where

e−iφl P = 0 and I =

1 t,+1

0 eiφl

1

r,+1

,

r,+1 . 1

(7.18)

(7.19)

The hard part is done. To calculate the transfer matrix for the entire structure, I just multiply the matrices for each interface and layer, starting with interface 0 and ending with interface L, M0–L = I0 P1 I1 P2 I2 . . . PL IL .

(7.20)

The forward and backward waves in medium 0 are respectively the incident and reﬂected ﬁelds. (The incident ﬁeld has unit amplitude.) The forward-going wave in medium L + 1 is the transmitted light; there is no backward-going wave. Thus the entire multilayer structure satisﬁes an equation of the form of Eq. 7.16

t 1 . (7.21) = M0–L 0 r Multiplying out the matrix equation allows me to ﬁnd r and t for the multilayer structure. After computing M0–L , I will ﬁnd it to be of the form

A B M0–L = . (7.22) C D Then 1 = At and r = Ct so that t=

1 A

r=

C . A

(7.23)

Once I have the amplitudes, the transmittance and reﬂectance are T = tt ∗ and R = rr ∗ . (Medium 0 and medium L + 1 both have n = 1.) Computation is quick and relatively easy to program. The curves in Figs. 7.3, 7.4, and 7.6 were calculated using the matrix method.

7.4 Inverting R and T to Find If my goal is to use experimental measurements of R and T to ﬁnd out about the optical constants (n, κ, , . . . ), I’ll need to ﬁgure out how to invert the transcendental equations for the measured quantities to extract the things in which I am interested. The inversion is not trivial, and often involves some approximations or computation. The computational approach is to do some sort of least-square minimization of the difference between measurements and calculation. The trick is to get on the right cycle of the fringe pattern; when that is done, the method can work well.

110

Transmission and Reflection

Fig. 7.8

Geometry of a thin film on a thick substrate. The film (red) has complex optical conductivity σ while the substrate has refractive index n. Light is incident from the left at normal incidence with amplitude Ei . Some is reflected with amplitude Er and some is transmitted with amplitude Et . The wave vectors and electric and magnetic field vectors are shown but only the electric fields are labeled.

7.4.1 The Glover-Tinkham Formula I can derive a useful approximation to the exact formulae, useful for the case where the ﬁlm is very thin. This case is not very restrictive; it is only for very thin layers that any light at all is transmitted through a highly conducting (or superconducting) layer. The formula was derived by Glover and Tinkham [84, 85] many years ago, and probably has origins even earlier. This approximation is easy to invert in order to extract the optical conductivity from the measured transmittance and reﬂectance. The basic physics of the situation is that we know that the electric and magnetic ﬁeld amplitude inside the ﬁlm goes as e−x/δ where x is the distance the wave has propagated into the ﬁlm and δ is the optical penetration depth.∗ If the thickness d of the ﬁlm satisﬁes d δ (and also is small compared to the wavelength inside the ﬁlm), then the ﬁeld does not change measurably within the ﬁlm: E(d) = E(0). I am then permitted to treat the ﬁlm as a sheet of surface current with surface current density K. The geometry is shown in Fig. 7.8 and the boundary conditions [2] are E1 − E2 = 0

(7.24)

4π H1 − H2 = K, (7.25) c where the subscript speciﬁes the tangential or parallel components of the ﬁeld, 1 refers to the side of the ﬁlm where the incident and reﬂected ﬁelds are, and 2 to the side where the transmitted ﬁeld is. The geometry is as follows. The ﬁlm deﬁnes the y–z plane. The incident and transmitted ˆ The electric ﬁelds are all taken as along y. ˆ q are along xˆ while the reﬂected q is along −x. Eq. 3.3c then tells me that the incident and transmitted magnetic ﬁelds are along zˆ and the ∗ To be explicit, I can always write at time t = 0

E(x) = E0 einωx/c e−κωx/c with n and κ the real and imaginary parts of the refractive index N . Then the penetration depth is δ = c/ωκ and the wavelength inside the ﬁlm is λin = 2π c/ωn = λ0 /n with λ0 the vacuum wavelength.

7.4 Inverting R and T to Find

111

reﬂected one along −ˆz. The coefﬁcients I need are the amplitude reﬂection and transmission coefﬁcients r and t, deﬁned via Er = rEi and Et = tEi . Moreover, H = nE in the substrate and H = E in the n = 1 vacuum on the left side of the ﬁlm. I might as well take Ei = 1 and write Eqs. 7.24 and 7.25 as 1+r −t =0 (7.26) 4π K. (7.27) 1 − r − nt = c Compare to Eqs. 3.28 and 3.29, where there was no surface current, but where I did allow both sides of the interface to have a complex refractive index. What should I use for K? Well, it is the surface current density, which for a thin layer with nonzero thickness d is K = j d = σ Ed, where I used Ohm’s law to write it in terms of the complex conductivity σ . This answer only raises another question: What should I use for E? Well, the ﬁeld is the same on both sides of the ﬁlm and continuous across the interface (Eq. 7.24) so I can use either t or 1 + r. (Recall that I took the incident ﬁeld to have unit amplitude.) The former is easier, so I have from the magnetic-ﬁeld boundary condition:

4π σ d t. 1−r = n+ c The electric-ﬁeld boundary condition allows me to eliminate r = t − 1 so that t=

2 n + 1 + Z0 σ d

(7.28)

where I replaced 4π/c with Z0 , the impedance of free space, 377 . (See Appendix A.) The units are correct. Recall the DC resistance of a rectangular slab, R = ρL/W d where ρ is the resistivity, L the length, W the width, and d the thickness. If the slab is a square (L = W ), then the square resistance or sheet resistance is R = ρ/d = 1/σ d. I can consider that at ﬁnite frequencies σ (ω)d = 1/Z and write t = 2/(n + 1 + Z0 /Z ). Either works, and both indicate that the transmission of light by a conducting thin ﬁlm is controlled by the ﬁlm’s impedance. The amplitude reﬂection coefﬁcient is easy to calculate once I have t: r=

1 − n − Z0 σ d , 1 + n + Z0 σ d

(7.29)

The amplitude reﬂection coefﬁcient is negative; the reﬂected electric ﬁeld points opposite to the incident ﬁeld (and opposite to how it is drawn in Fig. 7.8). The transmittance into the substrate is the ratio of intensity behind the ﬁlm to incident intensity. The ratio of the Poynting vector amplitudes, using Eq. 3.23, gives T f = ntt ∗ and 4n Tf = . (7.30) (n + 1 + Z0 σ1 d)2 + (Z0 σ2 d)2 The reﬂectance is rr ∗ Rf =

(n − 1 + Z0 σ1 d)2 + (Z0 σ2 d)2 . (n + 1 + Z0 σ1 d)2 + (Z0 σ2 d)2

(7.31)

112

Transmission and Reflection

The subscript f for “ﬁlm” is there to remind me that this is the transmittance across the ﬁlm and into the substrate. When the light makes it to the back surface, some will be reﬂected, return to the ﬁlm, be reﬂected again, and continue to produce within the substrate either coherent or incoherent multiple internal reﬂections. See the discussion above that leads to Eq. 7.8 and to Eqs. 7.2 and 7.3. The derivations need to be modiﬁed to include the fact that the two surfaces of the thin-ﬁlm-on-substrate sample are not the same. The ﬁlm surface is governed by T f and Rf and the back surface by the usual single-surface coefﬁcients, Rbc = (n − 1)2 /(n + 1)2 and T bc = 1 − Rbc = 4n/(n + 1)2 . Eq. 7.2 becomes T =

T f (1 − Rbc )e−αx , 1 − R f Rbc e−2αx

(7.32)

where I’ve allowed for some absorption in the substrate, with absorption coefﬁcient α. Note carefully the prime on R f . It indicates that the multiple-internal-reﬂection terms have the light incident on the ﬁlm from within the substrate rather than from refractive index unity vacuum. To write R f , I exchange n and 1 in Eq. 7.31. Similarly, the full reﬂectance of the ﬁlm-on-substrate, Eq. 7.3, becomes R = Rf + Rbc

T 2f e−2αx 1 − R f Rbc e−2αx

,

(7.33)

where again I note the presence of R f . It is of course possible to have coherent multiple internal reﬂections in the substrate. Standing waves will occur, like those shown in Figs. 7.3 and 7.4. The ﬁlm typically increases the reﬂectance of the surface on which is is deposited, increasing the amplitude of the standing waves over the uncoated case. Figure 7.9 shows the ﬁlm thickness dependence of the transmittance, reﬂectance, and absorptance (A ≡ 1−R−T , the fraction of the incident energy that is absorbed) of a metal

Fig. 7.9

Thickness dependence of the transmittance, reflectance, and absorptance of a metal film on a transparent substrate. The sheet impedance of the metal is shown on the top axis.

7.4 Inverting R and T to Find

113

ﬁlm on a transparent substrate. The sheet impedance, 1/σ d of the ﬁlm is shown across the top. The metal was taken to have a conductivity σ = 20,000 −1 cm−1 , independent of ﬁlm thickness. Its resistivity is then ρ = 50 μ-cm. This value is typical of a dirty metal such as Nichrome, a nickel–chromium alloy used for resistive heaters. The optical conductivity of such metals is nearly constant from DC to the midinfrared. The substrate index of refraction was taken as n = 1.9, appropriate for crystal quartz and other substrates in the far-infrared region. ˚ a not really realistic thickness, because the ionic radii of Ni and For very thin ﬁlms (∼1A, ˚ the transmittance and reﬂectance are close to those of the substrate. As Cr are about 2 A) thickness increases, the transmittance falls and the reﬂectance and absorptance rise, with ˚ At this thickness and for the the three becoming nearly equal, 1/3 each, for d ≈ 24 A. conductivity chosen, R = 250 . With increasing thickness, the transmittance continues ˚ where to fall, the reﬂectance to rise. The absorptance shows a broad maximum around 33 A, R = 150 , and decreases as thickness continues to increase. What must I keep in mind and what did I learn by making this calculation? (1) The ˚ for this conductivity. Therefore, the approximation I made, 100 cm−1 skin depth is 2,000 A ˚ thickness but not so good for thicker ﬁlms. If d δ, is adequate below about 200 A frequency is lowered, the approximation is better. (2) It is the sheet impedance R that matters and transmittance becomes quite small when R falls below 10–20 . (3) R cannot be too large either; the transmittance is pretty insensitive to conductivity changes when R is above 1,000–2,000 . (4) I cannot make a broadband absorber out of a thin metal ﬁlm. The maximum absorptance is not more than 35%, far below the 99% that might be the requirement for a good absorber.∗

7.4.2 Inverting the Glover-Tinkham Formula If I measure the reﬂectance and the transmittance of the ﬁlm on the substrate and if I know also the refractive index and absorption of the substrate, I can use these measurements to determine the real and imaginary parts of the conductivity. The substrate adds complexity without adding clarity, so let me do this inversion for the free-standing ﬁlm, with refractive index n = 1 on both sides. Eqs. 7.30 and 7.31 become T =

4 (2 + Z0 σ1 d)2 + (Z0 σ1 d)2

(7.34)

R=

(Z0 σ1 d)2 + (Z0 σ1 d)2 . (2 + Z0 σ1 d)2 + (Z0 σ1 d)2

(7.35)

and

This pair may be combined to ﬁnd σ1 =

1 A 1 1−R−T = Z0 d T Z0 d T

∗ In some applications the ∼33% that is transmitted could be considered as lost too. In others, where for example

I want to turn electromagnetic energy into heat, transmitted light does not contribute to generating this heat.

114

Transmission and Reflection where A = 1 − R − T is the absorptance. Then, because I now know σ 1 , I can calculate 4 1 − (2 + Z0 σ1 d)2 . σ2 = Z0 d T Inversion of transmittance and reﬂectance spectra has been done a number of times. In most cases, the experiments were aimed at superconductors [85–88]. I will show a few examples in Chapter 11.

8

Free-Electron Metals

The free-electron theory of metals was developed in the late 1920s and early 1930s by Sommerfeld [89] and others [90, 91]. The basic idea is that one or more electrons of each atom in the solid are detached from their atomic location and free to move throughout the crystal as a free gas. The electrons are fermions, subject to the Pauli principle, and therefore follow the Fermi–Dirac distribution function. Each state is occupied by at most one electron. The electron density is high enough that the Fermi temperature is much higher than the physical temperature, so the Fermi–Dirac function is relatively sharp. The electrons are said to form a “Fermi gas” with a Fermi surface that is the constant-energy surface of the most energetic electrons. The Fermi–Dirac statistics overwhelm other forces. Thus, the free-electron model treats the potential energy in which the electron moves (the ion potential) as a constant. (Including the potential can be done of course; this is the realm of electronic band structure. Bandstructure calculations have been done for many materials systems – not just elements.) For many metals, the effect is mostly to modify slightly the effective mass of the charge carriers, to adjust the numerical value of the density of states at the Fermi surface, and to ﬁnd bands above and below the one where the free carriers live. I discussed in the look at real solids just completed that the band structure – in particular the presence of the ﬁlled d-electron levels below the Fermi level – is the reason why gold, silver and copper appear different. The basic low-energy physics is however very close to what the free-electron model predicts.∗ ) The electron–electron interaction is also left out of the free-electron model, so that one individual electron state is independent of the other electron states. Here, I can take refuge in Landau’s Fermi-liquid theory. This theory of interacting fermions describes the properties of metals in cases where the interaction between the particles of the manybody system is not small. There is a one-to-one correspondence between the elementary excitations of a Fermi gas system and a Fermi liquid system. These excitations are called “quasiparticles;” the quasiparticle states have the same quantum numbers (momentum spin, charge) as the electrons of the Fermi gas.

8.1 Schrödinger Equation for Free Electrons The simple free-electron model is surprisingly successful in explaining many experimental phenomena, including electrical conductivity, heat conductivity, the Wiedemann–Franz law ∗ In contrast, band structure is essential for understanding semiconductors and insulators.

115

116

Free-Electron Metals

(a relation of the ratio of electrical conductivity to thermal conductivity), the electronic contribution to the heat capacity, Hall effect, and optical properties. I’ll start with this Hamiltonian, a sum of kinetic and potential energies: p2 + V, 2m where p is the momentum, m the mass, and V the potential. In general I would have V = V(r) where r is the location of the electron and the potential would be periodic in the lattice structure and account for the interaction of the electron with atoms and ions in the crystal. But in the free electron model I take V = constant and I might as well take it to be zero.∗ My quantum mechanics class told me that the momentum operator is p = −i h∇, ¯ so that the free electron Hamiltonian is H=

h¯ 2 ∇ 2 2m and the time independent Schr¨odinger equation is H=−

(8.1)

Hψ = Eψ,

(8.2)

where E is the energy eigenvalue and ψ is the wave function of the single electron I am considering.

8.2 Wave Function Consider a plane-wave wave function: ψ = ψ0 eik·r,

(8.3)

with ψ0 a complex amplitude and k a wave vector to be determined by solving the Schr¨odinger equation. Of course (Appendix C) ∇ 2 ψ = −k 2 ψ. I need to normalize the wave function: ∗ dV ψ (r)ψ(r) = dV |ψ0 |2 = |ψ0 |2 V 1 = ψ|ψ = V

V

where V is the entire volume of the crystal. Then, eiφ ψ0 = √ V with φ an arbitrary phase. (The time-dependent Schr¨odinger equation leads to a phasor e−iωt where the frequency ω is related to the energy E by Planck’s constant: E = hω.) ¯ Substituting Eq. 8.3 into Eq. 8.2 with the Hamiltonian of Eq. 8.1 yields +

h¯ 2 k 2 ψ = Eψ. 2m

∗ I need a wall at the surface to keep the electrons in the crystal, but the choice of V’s constant value has no effect.

I take the wall height to be inﬁnite. (And then I eliminate the walls by using periodic boundary conditions.)

117

8.3 Exclusion Principle and Boundary Conditions Multiply from the left by ψ ∗ and integrate to ﬁnd h¯ 2 k 2 . (8.4) 2m Eq. 8.4 is just the kinetic energy of a free particle. The momentum operator is p = −i h∇ ¯ and so ψ|p|ψ = h¯ k and so I can identify hk ¯ as the momentum. The plane-wave wave functions are eigenfunctions of both the Hamiltonian and of momentum. The energy is quadratic in k, with zero energy∗ at k = 0. The probability density to ﬁnd the electron at any position in the crystal is constant, P (r) = ψ ∗ ψ = 1/V . For conceptual clarity, let me assume a cube of edge length L = J a where a is the lattice constant of the crystal and J is a (large) integer. There is one free electron per atom. The volume is V = L3 ≈ J 3 a 3 . If L ˚ then the solid contains about 1022 electrons and J ≈ 2.2 × 107 . is 1 cm, and a ≈ 4.6 A, E=

8.3 Exclusion Principle and Boundary Conditions The electrons are fermions; only one electron can have a particular set of quantum numbers. The quantum numbers here are the three components of the wave vector k and the spin: {kx ,ky ,kz,σ } where σ =↑ or ↓. The allowed values of the wave vector components are set by the boundary conditions. If I consider particle-in-a-box conditions, then the wave function will be zero outside the solid, and the solutions are sines and/or cosines depending on the choice of coordinate-system origin. As in Chapter 5, Section 5.2.2, for phonons, it is much better† to use periodic boundary conditions. I’ll write these mathematically as ψ(r + L) = ψ(r),

(8.5)

ˆ y, ˆ or zˆ directions. To begin, look at Fig. where L is oriented along one or another of the x, 5.3 where one takes a linear chain and bends it into a circle, connecting the ﬁrst and N th sites with a bond. Clearly, this loop satisﬁes Eq. 8.5 because the wave function must be single valued and give the same value every time one goes once around the chain. One may also think in a slightly different way, illustrated in Fig. 8.1. I take the block at the center and make many copies of it and lay them all next to each other, ﬁlling space with replicas of the center block. The system boundary is moved off to inﬁnity, but the fact that the copies are exact means that Eq. 8.5 is obeyed. For example the electron colored gray that is about to leave the block on its right-hand side will reappear from the neighbor on the left. I will apply periodic boundary conditions to the free-electron wave function of Eq. 8.3 ˆ for L = J a x: ψ(r) = ψ0 eik·r = ψ(r + L) = ψ0 eik·(r+J a xˆ )

∗ Recall: the potential energy is zero. † The sine/cosine solutions yield standing waves in the block of material, just as the case of waves on a string with

ﬁxed ends. These waves carry no momentum and do not contribute to the current until one forms the proper linear combinations.

118

Free-Electron Metals

Fig. 8.1

A square system, with edge L, containing N electrons is repeated many times and the copies laid as tiles to cover the plane. The system is periodic in both directions with period L. with a the lattice constant. Now, k · xˆ = kx . The periodic boundary conditions for this speciﬁc value of L then yield eikx J a = 1.

(8.6)

This equation has a large number of solutions; the phase of the complex exponential kx J a must be an integer (positive or negative) times 2π radians. Hence 2π jx where jx = 0, ± 1, ± 2, . . . kx = Ja Applying periodic boundary conditions in the yˆ and zˆ directions give equivalent quantization of ky and kz . Because the components of the wave vector are set by the integer values of {jx ,jy ,jz } and are no longer continuous variables, the energy, Eq. 8.4, is also quantized:

h¯ 2 2π 2 2 h¯ 2 k 2 = (jx + jy2 + jz2 ) E(k) = 2m 2m J a I note that there are many degeneracies in the energy spectrum of the free electrons. The two values of spin (up and down) are degenerate as well as many permutations of integers (positive and negative). These permutations are distinguishable because the momentum is distinguishable: k = (2π/J a)(jx xˆ + jy yˆ + jz zˆ ).

(8.7)

The Pauli principle says that no two electrons can have the same quantum numbers. I can call the set {jx ,jy ,jz,σ } the quantum numbers. I now pour electrons into the metal, stopping when I reach electrical neutrality.∗ The ﬁrst few energies are E0 = 0

{0,0,0, ↑} {0,0,0, ↓}

E1 = δ

{1,0,0, ↑} {0,1,0, ↑}

...

{0,0,1, ↓}

E2 = 2δ

{1,1,0, ↑} {1,0,1, ↑}

...

{0,1,1, ↓}

where δ = (2π h) ¯ 2 /2mJ 2 a 2 is a typical spacing between levels. ∗ One to a few electrons per atom in simple metals; one to a few per formula unit in metallic compounds.

119

Fig. 8.2

8.4 The Fermi Energy

The Fermi sphere of the free-electron metal. The surface of this sphere is the Fermi surface.

8.4 The Fermi Energy The values of k allowed by the boundary conditions form a grid of points when plotted in three-dimensional space∗ with axes kx , ky , kz . Because the energy E is quadratic in the wave vector k, the surfaces of constant energy are spheres of radius k. Indeed,

h¯ 2 2π 2 2 j E(k) = 2m J a where j 2 = jx2 + jy2 + jz2 is an integer. The highest energy of any of these electrons (at T = 0) is called the Fermi energy:

h¯ 2 2 h¯ 2 2π 2 2 k = jF EF = 2m F 2m J a where kF is the radius of the sphere corresponding to the highest energy electrons and jF is the radius of an equivalent sphere in coordinates of the integers jx , jy , jz . A diagram of this Fermi sphere is shown in Fig. 8.2. Now let me calculate the radius kF of the Fermi surface. There are N electrons in the metal. Because of the spin degeneracy, two of these electrons occupy each point on the grid of points indexed by jx , jy , and jz . The total number of points inside the sphere is just the volume of the sphere in “j -space.” Hence, 4π 3 N = j (8.8) 2 3 F or

3N 1/3 jF = . 8π The Fermi wave vector is 2π 1 2 1/3 jF = 3π N kF = . Ja Ja ∗ This space is called “momentum space,” “k-space,” or “reciprocal space.” Its axes have units of inverse length.

120

Free-Electron Metals

Table 8.1 Free-electron Fermi surface parameters for simple metals. Valence

Metal

n 1022 cm−3

kF 108 cm−1

vF 108 cm/s

EF eV

TF 104 K

1

Li Na K Rb Cs Cu Ag Au Be Mg Ca Sr Ba Zn Cd Al Ga In Pb Sn(w)

4.70 2.65 1.40 1.15 0.91 8.45 5.85 5.90 24.2 8.60 4.60 3.56 3.20 13.10 9.28 18.06 15.30 11.49 13.20 14.48

1.11 0.92 0.75 0.70 0.64 1.36 1.20 1.20 1.93 1.37 1.11 1.02 0.98 1.57 1.40 1.75 1.65 1.50 1.57 1.62

1.29 1.07 0.86 0.81 0.75 1.57 1.39 1.39 2.23 1.58 1.28 1.18 1.13 1.82 1.62 2.02 1.91 1.74 1.82 1.88

4.72 3.23 2.12 1.85 1.58 7.00 5.48 5.51 14.14 7.13 4.68 3.95 3.65 9.39 7.46 11.63 10.35 8.60 9.37 10.03

5.48 3.75 2.46 2.15 1.83 8.12 6.36 6.39 16.41 8.27 5.43 4.58 4.24 10.90 8.66 13.49 12.01 9.98 10.87 11.64

2

3

4

But (J a)3 = V or J a = V 1/3 . Hence∗

2 1/3

1/3 3π N kF = = 3π 2 n V where n = N/V is the number density of electrons. The Fermi energy is the energy of an electron with wave vector kF .

(8.9)

h¯ 2 2 2/3 3π n . (8.10) 2m Related to the Fermi energy is the Fermi temperature TF , deﬁned as EF /kB , where kB is Boltzmann’s constant. I also deﬁne the Fermi momentum pF and Fermi velocity vF . pF = hk ¯ F = 2mEF EF =

and pF . m These quantities correspond respectively to the momentum and group velocity of an electron at the Fermi surface. Fermi surface parameters for many metals are shown in Table 8.1, after Ref. 24. vF =

∗ I can now forget j and J . It was helpful for me to introduce them; it was not necessary. In fact, the periodic i

boundary conditions may also be left behind at this point.

121

8.5 The Effect of Temperature

Fermi energies are in the range of 1.5–15 eV; Fermi temperatures are thus 18,000–180,000 K. These temperatures are much above 300 K, the temperature of the room. I did not make a bad mistake by considering (as I have done since this chapter began) T = 0. The Fermi velocities are surprisingly large; they are in the range 0.8–2×108 cm/s. The average is about c/200. Our quintessential metal, silver has EF = 5.5 eV, TF = 64,000 K and vF = 1.4 × 108 cm/s. I’ll use these numbers when numbers are needed.

8.5 The Effect of Temperature At zero temperature the Fermi–Dirac distribution is perfectly sharp because every electron is in the lowest energy state that it can access. At ﬁnite temperatures, the probability of occupancy is given by the Fermi–Dirac distribution function f (E), f (E) =

1 1+e

E−μ kB T

(8.11)

where μ is the chemical potential or Fermi level. At zero temperature μ = EF ; it has a weak temperature dependence until T becomes a signiﬁcant fraction of TF . A plot of the Fermi– Dirac distribution function at four temperatures is shown in Fig. 8.3. The calculation was done for silver, with EF = 5.5 eV. The effect of temperature is to broaden the distribution. Some states below the Fermi level are empty; some above it are occupied. The “width” of the distribution, the energy range where it drops from 90% to 10% of the T = 0 value, is

E ≈ 4.4kB T , 38 meV at 100 K.

Fig. 8.3

The Fermi–Dirac distribution function f (E) at four temperatures, 10, 100, 1,000, and 10,000 K. The inset shows the detail around EF at 10 and 100 K.

122

Free-Electron Metals

8.6 The Density of States I may need the density of states, so let me work it out now. I can write an equation for NE , the number of electrons with energy between the zero of energy and energy E, by noting that Eq. 8.10 is such an equation, so

2/3 h¯ 2 3π 2 NE E= 2m V so that

NE =

2mE 3/2 V . 3π 2 h¯ 2

I now raise E by just a little bit dE and ﬁnd that the number goes up by dN.

2m(E + dE) 3/2 V NE + dN = . 3π 2 h¯ 2 Because dE is inﬁnitesimal, I can expand (E + dE)3/2 = E 3/2 (1 + 3dE/2E + · · · ) to ﬁnd

3dE 2mE 3/2 V 1 + . NE + dN = 2E 3π 2 h¯ 2 The ﬁrst term on the right is just NE and the second is dN. The density of states (the number of states between E and E + dE) is

2m 3/2 V √ dN = D(E) = E. dE 2π 2 h¯ 2 The density of states∗ grows as the energy increases, as the square root of the energy.†

8.7 Electrical Conductivity In the absence of an external ﬁeld, the metal does not carry current. The electrons are moving in all directions and the average or net motion is zero. Consider now the effect of an electric ﬁeld on these electrons. To be deﬁnite, I will specify the ﬁeld as our plane wave traveling along xˆ with electric ﬁeld oriented in the yˆ direction. ˆ 0 ei (qx−ωt ) . E = yE

(8.12)

The ﬁeld exerts a force on each and every charged electron: ˆ 0 eiqx e−iωt . Fext = −eE = −eyE ∗ Sometimes the symbol N (E) is used for the density of states. √ † The E behavior is correct for three-dimensional metals, where the energy depends on three—x, y, and √

z—components of k. In two dimensions D(E) is constant and in one dimension D(E) ∼ 1/ E.

123

8.7 Electrical Conductivity

I can put the space variation into E0 and ignore the fact that the ﬁeld varies in space with a length scale λ = 2π/q. The reason is that the wavelength λ is long compared to the effective range of the electron (the mean free path ) and also large compared to the lattice constant. I also have not made a local-ﬁeld correction. The electron is completely delocalized.∗ Hence the local ﬁeld is the average ﬁeld, which is the applied ﬁeld. Newton’s second law, F = ma, is best written dk dp = h¯ . (8.13) F= dt dt So the external force and any internal forces will change the k-state of the electron. The resultant response is not hindered by the Pauli exclusion principle: as the electron in state k evolves to k , the one at k has gotten out of the way by shifting to k

. What other forces act on the electrons? Well, the electrons are not bound; indeed, the potential energy has been set to zero. But the electrons can suffer collisions with impurities, other defects, lattice vibrations (phonons), and the surface. These collisions have a mean free time τ and relax the system back towards equilibrium. In the spirit of Drude’s model, I will consider that the relaxation generates an impulse Fcoll τ which changes the momentum hk ¯ back to the equilibrium value† hk ¯ 0 . Thus, k − k0 δk = −h¯ . (8.14) τ τ The collisions enter the picture as abrupt changes in momentum that occur every τ seconds. Note that hδk = mδv = mvdrift where vdrift is the average velocity acquired by the ¯ collection of electrons, known as the drift velocity.‡ Let me think for a moment about how the applied electric ﬁeld, with its e−iωt time dependence, affects the motion of an electron. The electron has wave vector k0 or velocity v0 = hk ¯ 0 /m; this velocity will be changed (in magnitude, direction, or both) by the ﬁeld. I will write the k of my electron in the presence of the ﬁeld as Fcoll = −h¯

k = k0 + δk e−iωt ,

(8.15)

ˆ δk represents the linear response of the electron to with δk in the direction of the ﬁeld, y. the external ﬁeld. k0 is the wave vector in the absence of the ﬁeld; it does not depend on the time. δk contains the amplitude and phase of the driven motion of the electron. Newton’s second law becomes k − k0 dk = −h¯ − eE. (8.16) h¯ dt τ On substituting for k and E, taking derivatives, and canceling e−iωt , I get −i hωδk = ¯

−hδk ¯ − eE0 τ

(8.17)

∗ ψ has amplitude everywhere in the crystal. † Drude considered the equilibrium value to be zero, but I know that it is close to the Fermi momentum. ‡ Without the electric ﬁeld of the light, the average velocity is zero. The average speed is some fraction of the

Fermi velocity, but speed and velocity are different things.

124

Fig. 8.4

Free-Electron Metals

The momentum-space location of the Fermi sphere in equilibrium is within the dashed line that indicates the Fermi ˆ the electrons are accelerated downward. (They are negatively surface. When an electric field is applied along y, charged.) The displaced sphere is shown in blue. There is a current, because more electrons are going down than are going up. The acceleration continues until it is balanced by the scattering of electrons; one such event is shown. A little algebra then yields this relation between the shift of k and the electric ﬁeld: δk = −

eτ/h¯ E0, 1 − iωτ

(8.18)

where all vectors are in the yˆ direction. Equation 8.18 looks a lot like the Drude velocity, Eq. 4.7, except that h¯ appears. The appearance will be ﬂeeting, however, and the theory is at best semiclassical. The picture of what happen in the metal due to the external electric ﬁeld is not intuitive. Every electron has changed its k-vector under the inﬂuence of the electric ﬁeld. This displacement occurs alike and by the same amount to the deeply buried electrons with small k values and low speeds and to the Fermi-surface electrons which are whizzing along at c/200. The Fermi surface, which is centered at k = 0 in equilibrium, is moved as a whole by δk, as illustrated in Fig. 8.4. Were there no scattering, the displacement of the Fermi sphere would continue to grow; the electric ﬁeld exerts a force on the electrons, causing acceleration. At zero frequency, both δk and the velocity of each electron would change linearly with the time, increasing for left-moving electrons and decreasing for right-moving electrons. With scattering, the relaxation eventually balances the acceleration and there is a ﬁxed, steady-state∗ displacement. Because scattering events are uncorrelated and affect at random one or the other of the independent and noninteracting electrons, the relaxation process, shown schematically in Fig. 8.4, must respect the Pauli principal, taking the electron from a ﬁlled state to an empty state. If the scattering is elastic, then the energy of the initial and ﬁnal states should be the same. So the relaxation process takes an electron from the leading edge of the displaced Fermi surface, where electrons occupy states that are empty in equilibrium, and deposits it just outside the trailing edge, where states that once were occupied have been emptied. ∗ But not equilibrium.

125

8.8 Discussion of the Drude Model

The electrons that are relaxed are therefore very close to the Fermi energy and move at the Fermi velocity.∗ Thus the relation between the mean free time τ and mean free path is = vF τ .

(8.19)

The electrical current is j = −nevd where n is the electron density and vd is an average or drift velocity. This velocity is not the Fermi velocity, but the average of all electrons’ responses to the ﬁeld. The averaging process goes like: vd = vk = v0 + δv = δv = δv where the last equality comes from the fact that every electron feels the same force. In and the above, the velocity of an electron with wave vector k is vk = pk /m = hk/m ¯ making vd = hδk/m, ¯ j=−

neh¯ δk. m

(8.20)

I then substitute δk from Eq. 8.18 to obtain

−eτ/h¯ neh¯ ˆ 0. yE j=− m 1 − iωτ Using Ohm’s law, j = σ E, I ﬁnd ﬁnally σ =

ne2 τ/m , 1 − iωτ

(8.21)

an equation identical to Eq. 4.8. Equation 8.21 gives a complex conductivity. The dielectric function and other optical constants follow immediately as I have shown many times before. I write = c + 4π iσ /ω to allow for core polarizability and have = c − with ωp the plasma frequency,

ωp2 ω2 + iω/τ

(8.22)

ωp =

4π ne2 , m

(8.23)

as before.

8.8 Discussion of the Drude Model 8.8.1 Low Frequencies and the Steady-State To think a bit more about the conduction process in metals, let me ﬁrst address zero frequency (or any frequency low with respect to 1/τ ). In this case, I can take dv/dt ≈ 0, ∗ The realization that electron relaxation involves the fast-moving Fermi-surface electrons is where quantum

mechanics (and quantum statistical mechanics) leads to new concepts in the Drude theory.

126

Fig. 8.5

Free-Electron Metals

Energy plotted vs ky in equilibrium (left) and with a steady current flow (right). An elastic scattering event is also shown. which is the same as saying that dk/dt (k − k0 )/τ in Eq. 8.16. I have a steady state (not equilibrium!) solution; the acceleration is zero. (I ignore the initial transient when the ﬁeld is turned on). The conductivity is σ =

ne2 τ , m

and Eq. 8.18 becomes δk = −

eτ E0 . h¯

The Fermi surface is displaced by an amount δk in the negative ﬁeld direction as shown in Fig. 8.4. Now, the energy dispersion is still E = h¯ 2 k 2 /2m so that the average energy of the electrons has increased. (The ﬁeld did work on them.) Figure 8.5 shows the energy dispersion and Fermi energy as a function of ky (for, say kx = kz = 0) in equilibrium (left) and with an electric ﬁeld applied and corresponding steady-state current ﬂow. Remember that mv = hk; ¯ for electrons moving in the direction of electron ﬂow, the most energetic ones have a bit higher energy than in equilibrium. In contrast, for electrons moving against the direction of electron ﬂow, the most energetic ones have an energy that is a bit smaller than in equilibrium. Scattering can take electrons from the ﬁrst to the second direction. Scattering from impurities, other defects, and the surface generally is elastic. The direction of the electron momentum is changed but not the energy. Scattering by absorption of phonons is inelastic, but phonon energies are tens of meV whereas the Fermi energy is 1,000 times higher. So on the scale of Fig. 8.5 the distinction is not visible.∗

8.8.2 More Numbers Figures 8.4 and 8.5 suggest that δk is large. It is not. Let me estimate it from Eq. 8.20. I’ll take the current density as 107 A/cm2 . (This is a huge current; the electrical code typically restricts current densities in copper house wiring [93] to 115 A/cm2 .) Given that e is 1.6 × 10−19 C, the current is carried by a ﬂow of 0.6 × 1026 electrons/s cm2 . I invert Eq. 8.20: δk = −mj/neh¯ = 104 cm−1 . Compare this to the Fermi wave vector (Table 8.1) ∗ There are phenomena where the distinction is important. Elastic vs. inelastic scattering plays a large role

in localization phenomena where the phase of the wave function is critical. In the far-infrared response at low temperatures there is the Holstein effect [92], where phonon emission affects the optical conductivity at frequencies equal to or larger than the phonon frequencies. See Section 13.3.1.

127

8.8 Discussion of the Drude Model of order 108 cm−1 . Very high current densities displace the Fermi surface by only 0.01% of its radius.∗ The energy change is also small. The energy of the Fermi-surface electrons moving in the −y direction is increased to h¯ 2 (kF + δk)2 /2m. Expanding, we see that the energy goes to EF + δE =

h¯ 2 kF2 h¯ 2 kF δk + 2m m

or δE 2δk = ≈ 10−4 . EF kF This value corresponds to the energy spread of the Fermi surface at temperatures of 1 K or so. So at most temperatures (and most currents) the thermal spread of the Fermi distribution is much larger than the displacement due to the current.

8.8.3 The Perfect Conductor Now suppose there are no collisions; the metal is a perfect conductor.† The equation of motion (Eq. 8.16) is simpliﬁed. h¯

dk = −eE dt

(8.24)

and the solution is (at ﬁnite frequencies)‡ δk = −

ie E0 . hω ¯

The oscillations of k are 90◦ out of phase with the ﬁeld. Equation 8.20 is unchanged and so, after a bit of algebra I ﬁnd for the conductivity. ne2 . (8.25) mω This expression is the high frequency limit of Eq. 8.21. That makes sense because no scattering means that the mean free time for collisions is inﬁnite and any ﬁnite frequency makes ωτ big compared to 1. We have (ω > 0) σ =i

σ1 = 0 σ2 =

ne2 . mω

∗ I would be more correct if I said that very high current densities increase the speed of the fastest electrons–those

at the Fermi surface–by only 0.01% of their zero-current speed.

† But not a superconductor. The perfect conductor does not exhibit the Meissner effect, Josephson effect, or the

energy gap in the optical conductivity. See Chapter 11.

‡ At DC, the solution is a δk that grows linearly with time: a constant acceleration.

128

Free-Electron Metals The dielectric function of the perfect metal is purely real.∗ ωp2 4π ne2 /m = − . c ω2 ω2 So both conductivity and dielectric function tell us that the perfect metal does not dissipate electromagnetic energy. √ But wait! 1 is negative for frequencies below ωp / c , which I’ll call the screened plasma frequency. The ﬁelds inside are damped, and does not that damping mean attenuation and energy loss? The answer is no. The refractive index below the screened plasma frequency is indeed imaginary ωp2 N = c − 2 , ω = c −

making n = 0 and κ ≈ ωp /ω (where I have neglected c ). But in this case the reﬂectance (Eq. 3.33) is R=

1 + κ2 ≡ 1, 1 + κ2

or 100%. All the incident energy is reﬂected. Electromagnetic energy is conserved! Moreover, if I remember that the reﬂected electric ﬁeld direction is 180◦ from the incident ﬁeld direction, then Einc + Ereﬂ = 0 = Etransm , making the ﬁeld in the perfect conductor zero, as it should be.

8.8.4 Intraband Transitions Now, let me look qualitatively at the absorption process (σ 1 ﬁnite and frequency low). If I think of photons, the process is the absorption of a photon of energy h¯ ω and the promotion of the electron to a higher state. Because E ∼ k 2 and p = hk, ¯ this process involves a change of momentum of the electron. The initial and ﬁnal electron states are both on the same E vs. k curve, so this is an intraband – within the same band – transition. I look at the energy and momentum conservation in the process here. The Pauli principle requires that initial state be full (below the Fermi level at T = 0) and the ﬁnal state be empty (above the Fermi level at T = 0).† I write the initial energy as‡ Ei = EF =

h¯ 2 kF2 2m

and the ﬁnal state energy as Ef = EF + hω ¯ =

h¯ 2 (kF2 + 2kF k) 2m

∗ Except at ω = 0 where the imaginary part, or conductivity, is inﬁnite. I’ll calculate the DC conductivity of the

perfect conductor in Chapter 10, Section 10.1.2.

† This statement is a zero temperature picture, but it is unchanged if T is ﬁnite. The electron still goes from

occupied state to empty state.

‡ Instead of taking the initial state at E , I could take at any energy between E − hω and E , but nevermind. ¯ F F F

129

8.8 Discussion of the Drude Model

where k is the amount the ﬁnal state wave vector is beyond kF to account for the ﬁnal state energy. I have neglected ( k)2 . Taking the difference leads to h¯ ω =

h¯ 2 kF k m

or ω mω = . hk v ¯ F F = hq ¯ where q = ω/c and ends with zero. (It is

k = The photon starts with momentum pγ absorbed.) But q k

because

ω ω . c vF

It is not possible to conserve momentum in this energy-conserving process. So how does the metal absorb energy? The collisions change the momentum of the electron and transfer momentum to the crystal as a whole. The process is efﬁcient at low frequencies, when ω 1/τ , and inefﬁcient at high frequencies.

8.8.5 Uncertainty Principle Uncertainty principle arguments are always worth exploring. An electron with quantum numbers k travels freely between collisions for a time τ . Whether the collision is elastic or inelastic, the length of time the electron occupies state ψ(k) is τ . The consequence is that the energy is not known better than E = h/τ ¯ . I use Eq. 8.4, E = h¯ 2 k 2 /2m, to ﬁnd (by differentiation) that the energy blurring of E means a momentum spread of k.

E = h¯ 2 k k/m or (because the relevant energy is the Fermi energy) m 1

EkF h¯ kF = = = hk 2EF 2EF τ vF τ ¯ Fτ But! vF τ is the mean free path ! So the position uncertainty is the mean free path and the momentum uncertainty is h k = h¯ /. This calculation should encourage you to stop ¯ thinking about the electron as a point-like particle skating around like a billiard ball on a table ﬁlled with obstacles and think of it as a quantum-mechanical wave packet that is delocalized over a range given by the mean free path.∗

k =

8.8.6 Yet More Numbers I ﬁrst speciﬁed paramaters for a standard metal in Chapter 4, Section 4.2.4: σ ≈ 6 × 105 −1 cm−1 or ρ = 1/σ = 1.6 μ-cm. The mean free time is τ = 2 × 10−14 s. From this number and vF = 2 × 108 cm/s I get = 4 × 10−6 cm = 40 nm. ˚ A mean free path of 40 nm–400 A–is a characteristic value for the noble metals at room temperature. ∗ If the idea of the physical extent of the wave function being the mean free path bothers you, do not forget that the wave function of the plane-wave state eik·r has ﬁnite amplitude everywhere in the solid.

130

Fig. 8.6

Free-Electron Metals

Resistivity ρdc = 1/σdc of bulk and thin-film silver at temperatures between 4 and 300 K. See Ref. 95. The resistance of pure metals is strongly temperature dependent, decreasing by large factors as the temperature is reduced. The physical reason for this decrease is that the scattering is due to interactions of the electrons with lattice vibrations (phonons) and, as T decreases both the number and the mean energy of the phonons decreases [24, 94]. Figure 8.6 shows an example, the temperature dependence of the resistivity ρdc = 1/σdc of silver ﬁlms of various thicknesses and also that of a bulk (mm-sized) crystal [95]. The resistivity is linear at high temperatures, and then, below the Debye temperature of 220 K, falls rapidly as a power law, ρ ∼ T n , with n in the range 2–5, before settling down to the low temperature residual value. The bulk crystal has a residual resistivity ratio (RRR) of 250. The mean free path at low temperatures is very long, = 10 μm. This is a macroscopic length, about the diameter of a cotton ﬁber. It is by no means a record: crystals of Ga have been produced with mean free paths of millimeters [96], so that electrons traveled the full thickness of the crystal before a collision; was in fact limited by the crystal size, and the collision was with its surface.

8.9 The Boltzmann Transport Equation The Boltzmann equation was devised initially to work out the nonequilibrium behavior of a classical ideal gas [97]. It addresses the changes in the distribution function (the probability of ﬁnding a particle in a unit volume of phase space) arising from external forces, diffusion of particles, and collisions of the particles. The Boltzmann equation can be written also for quantum mechanical particles. It is extremely powerful, allowing the inﬂuence of electric ﬁelds, temperature gradients, magnetic ﬁelds, and chemical potential gradients (alone or in combination) to be included [19, 98–100]. I’ll use it to calculate the optical conductivity

131

8.9 The Boltzmann Transport Equation

and I’ll ﬁnd that it gives me a way to derive (once again) the Drude equation for the conductivity.

8.9.1 The Distribution Function I know that the equilibrium distribution function of electrons in the solid follows the Fermi– Dirac distribution, Eq. 8.11: fk0 =

1 Ek −μ

1 + e kB T where I’ve added a subscript k to indicate that the energies are a function of the wave vector and the superscript 0 to indicate that this is the equilibrium function. In equilibrium there are no electrical currents or ﬂow of energy in the solid. (The cases where there are DC currents are called the steady state.) In the above equation, T is the temperature and μ is the chemical potential. μ is temperature dependent but at practical temperatures in simple metals, μ may be taken to be the Fermi energy. The chemical potential is set by 0 fk = N = dEfk0 (E)D(E) k,σ

where the electrons have quantum numbers k and σ where σ is the spin. They can have a band index n also but I’ll omit the band index; were I to include it, I’d need to sum over bands [19]. Finally, D(E) is the density of states. The nonequilibrium distribution function differs from the equilibrium one in two ways. First, I allow for temperature variations within the sample so that fk (r) =

1 Ek −μ(r) kB T (r)

,

1+e where the varying temperature causes (small) variations in the chemical potential. Second, I’ll impose an external force Fext . Newton’s law gives h¯ k˙ = Fext because k = mv/h. ¯ The velocity can be calculated from 1 (8.26) ∇k E k . h¯ The external force will cause the occupancy of some values of k to increase and of others to decrease. The nonequilibrium distribution fk (r,t) gives the probability that there is an electron at r at time t with wave vector k. Because of spin, I’ll have to say that it is the probability for a speciﬁc spin orientation and there is an equal probability for the other orientation. I’ll take care of the spin degeneracy by multiplying by two at the appropriate points. Moreover, I have to avoid violation of the uncertainty principle by thinking that r points to a volume large enough to accommodate the position uncertainty of the charge carriers.∗ So a correct approach is to say that the number of electrons in a small volume drdk of phase space is vk =

dN =

2 fk (r,t)drdk (2π )3

∗ I made an uncertainly principle argument in Section 8.8.5.

132

Fig. 8.7

Free-Electron Metals

Equilibrium Fermi function, fk0 , a current-carrying nonequilibrium distribution, fk , and the difference, fk − fk0 . where the 2 in the numerator is for spin. I want the number of particles dN to be large enough to be able to consider the statistics of the particles in dr. Figure 8.7 shows the equilibrium Fermi function, fk0 , a current-carrying nonequilibrium distribution, fk , and the√difference, fk − fk0 . All three are plotted against k, which for free electrons is k = ± 2mE/h. ¯ The calculation was done at 100 K, for a metal (silver!) with EF = 5.5 eV and kF = 1.2 × 108 cm−1 . This plot is a cut along the ky axis of the equilibrium and non-equilibrium Fermi spheres shown in Fig. 8.4. The current is upward, so because the electron is negative, fk is shifted downward. In order to make the shift barely visible, I had to shift by 1 × 106 cm−1 , about 100× the amount of the estimate of δk I made earlier in this chapter (Section 8.8.2), which did itself correspond to a huge current. The difference displays a pair of spikes at kF . The current can truly be said to be carried by Fermi-surface electrons. Sums or integrals over the distribution function give physical quantities. The one I need is the current, fk vk j(r,t) = −e k

= −e

2 (2π )3

d 3 kfk (r,t)vk .

(8.27)

The next step in the development is to let time advance by dt. The electron moves according to the equation of motion to a new place in phase space, at r = r + dr at time t + dt with wave vector k = k + dk. Now, conservation of charge tells me that the product of the probability of occupation and the volume of phase space, fk (r,t)drdk, is preserved over time. Liouville’s theorem∗ tells me that the volume of phase space is preserved. Hence, if there are no collisions to take electrons out of the phase space volume or to bring them into it, fk (r ,t + dt) = fk (r,t). (If dt is small enough, collisions will be unlikely.) ∗ See Appendix H of Ref. 19.

133

8.9 The Boltzmann Transport Equation

8.9.2 Boltzmann’s Equations When there are collisions, the change in the distribution function in time dt is due to collisions, because otherwise there is no change. So

∂fk dt (8.28) f (k + dk,r + dr,t + dt) − f (k,r,t) = ∂t coll where I have changed notation, moving the subscript k into the argument of f . (I’ll change back in a minute.) I note that dk =

dk Fext dt dt = h¯ dt

where Fext is the external force, typically Fext = −eE + (v × B)/c (or Fext = −eE if there is no external magnetic ﬁeld) and dr =

dr dt = vk dt, dt

where vk is the velocity of the electron with wave vector k. For linear response, I will do a Taylor expansion of the ﬁrst term in Eq. 8.28: f(k+ dk,r + dr,t + dt) = f (k,r,t)

∂f (k,r,t) Fext · ∇k f (k,r,t) + vk · ∇r f (k,r,t) + + dt h¯ ∂t

(8.29)

I substitute Eq. 8.29 into Eq. 8.28, cancel the two identical f terms, divide by dt and obtain the Boltzmann equation:

Fext ∂fk ∂fk = . (8.30) · ∇k fk + vk · ∇r fk + ∂t ∂t coll h¯ Note that I have returned to writing k as a subscript. There are many approaches to the collision term, including detailed calculations of scattering processes. For examples of some of these approaches, see the Boltzmann equation discussion in Ref. 19. The simplest approach however is to say that the nonequilibrium distribution relaxes to equilibrium with a time scale τk . This relaxation-time approximation then sets

fk − fk0 ∂fk =− . (8.31) ∂t coll τk If I deﬁne δfk = fk − fk0 and note that the partial of fk0 with respect to time is zero (the deﬁnition of equilibrium), then the solution of Eq. 8.31 is δfk (t) = δfk (0)e−t/τk . If the external conditions that lead to the nonequilibrium state are removed, it relaxes to the equilibrium state with time constant τk . That the partial of fk0 with respect to time is zero does not mean that scattering does not occur at equilibrium. What does happen is that the events that remove electrons from the

134

Free-Electron Metals

element of phase space that I am tracking are exactly balanced by events which put other electrons back in. In the nonequilibrium state, the balance is removed. Even in the relaxation-time approximation, the Boltzmann equation needs further simpliﬁcation. I’ll assume that δfk fk0 and write ∂fk0 ∂f 0 ∇k E = k hv ¯ k ∂E ∂E where I used the chain rule to get fourth term and Eq. 8.26 for the last. Also ∇k fk = ∇k (fk0 + δfk ) ≈ ∇k fk0 =

∇r fk = ∇r (fk0 + δfk ) ≈ ∇r fk0 =

∂fk0 ∂f 0 ∇r T + k ∇r μ ∂T ∂μ

(8.32)

(8.33)

where I used again the chain rule to get last term. So now I collect everything, rearrange a few terms, and obtain the linearized Boltzmann equation in the relaxation-time approximation ∂fk0 ∂fk0 ∂fk0 δfk ∂δfk + vk · ∇r T + ∇r μ =− Fext · vk . (8.34) + ∂E ∂T ∂μ ∂t τk I note that each of the three derivatives is peaked at the Fermi level and will be quite narrow, essentially delta functions if kT EF . I show the energy derivative at two temperatures in Fig. 8.8. (The derivative at 10 K is a spike 10 times higher than the 100 K curve and at 10,000 K is quite wide and 10 times smaller than the 1,000 K curve; neither display well on this plot.) Note that the horizontal scale is expanded compared to the one in Fig. 8.3. Even on the expanded scale, the derivatives are sharp at EF . The peaky behavior of the derivatives tells me that all the transport quantities which the Boltzmann equation allows me to investigate are determined by the Fermi-surface properties of the solid. There are many of these quantities if I impose at the same time electric ﬁelds, magnetic ﬁelds, and temperature gradients and measure electrical currents (or voltages) and heat transfer. For some of the details, take a look at Ref. 101.

Fig. 8.8

The energy derivative of the Fermi–Dirac distribution function at two temperatures.

135

8.9 The Boltzmann Transport Equation

8.9.3 The Optical Conductivity For optics I want the temperature the same everywhere in the sample, so that the gradients of temperature and electrochemical potential are both zero. Moreover, the external force is due to the electric ﬁeld E of the light, the magnetic ﬁeld being as inconsequential as ever. The ﬁeld will be the plane-wave ﬁeld I always use, Eqs. 2.5 or 8.12, but in the local approximation I can ignore the space part and write Fext = −eE(r,t) = −eE0 e−iωt . This ﬁeld oscillates and the current and the distribution function will also oscillate, although possibly with different phase. So I write δfk (t) = δk (0)e−iωt . The partial derivative with respect to time in Eq. 8.34 then can be replaced with −iωδfk , leading to −eE · vk

∂fk0 δfk . − iωδfk = − ∂E τk

Now it is just a little algebra to ﬁnd the deviation of the distribution function from equilibrium in response to the electric ﬁeld:

∂f 0 eτk E · vk − (8.35) δfk = − 1 − iωτk ∂E where I ﬁddled the minus signs to have one in front of the partial of the distribution function because that derivative, shown in Fig. 8.8, is by itself negative. Now use Eq. 8.27 to ﬁnd the current as a function of the ﬁeld

∂f 0 eτk E · vk 2 3 0 − vk . k f − d j = −e 1 − iωτk ∂E (2π )3 The integral of the ﬁrst term in the square brace is clearly zero. (There is no current if fk = fk0 !) I simplify the rest and get

∂f 0 e2 3 vk τk (vk · E) − . (8.36) k d j= 1 − iωτk ∂E 4π 3 To proceed towards Ohm’s law, I need to make some assumptions about the system I am studying. If I were interested in very high temperatures, I probably should not treat the energy derivative as a delta function, but evaluate the integral over the entire occupied volume in k space. But for now, I will restrict myself to the low temperature condition, by using

∂f 0 = δ(E − EF ). − ∂E I will also convert the integral over d 3 k to an energy integral times an integral over a constant energy surface. d 3k =

dEdSE dEdSE = |∇k E| h|v ¯ k|

The surface SE becomes the Fermi surface when I apply the delta function and vk → v(k = kF ), with kF the Fermi wave vector. This quantity clearly can vary with direction. I note also that Eq. 8.36 gives a tensor value for the conductivity: j is in general not parallel to E.

136

Free-Electron Metals

A ﬁnal note is that I’ve allowed for k-dependent scattering by writing the scattering time as τk . I’ll simplify things a lot in a minute, but ﬁrst, I write Ohm’s law in components, ji = σij Ej . Clearly i and j can each be x, y, or z. (I will discuss anisotropy and the tensor dielectric function/conductivity in Chapter 15.) With all of this, Eq. 8.36 then allows me to write one of the elements of the conductivity tensor (after doing the trivial energy integration) as τk vki vkj e2 , (8.37) dSE σ ij = 3 |vk |(1 − iωτk ) 4π h¯ SF where the constant energy surface is the Fermi surface and all the wave vectors k become kF . To ﬁnish this section, I’ll use the free electron model with a constant (energy- and wavevector-independent) scattering time. In this case, the velocity vectors whose components √ add to the Fermi velocity, vx2 +vy2 +vz2 = vF2 , are all equal. Hence vx = vy = vz = vF / 3. Thus in Eq. 8.37 the ratio vki vkj /|vk | = vF /3. Thus, the conductivity, now a scalar, can be written.

e2 vF τ σ = dSE , (8.38) 12π 3 h¯ 1 − iωτ SF " It remains to do the surface integral, which is dSE = 4π kF2 , and to remember that vF = hk ¯ F /m to ﬁnd σ = (e2 kF3 /3π m)(τ/1 − iωτ ). The last step is to look back at Eq. 8.9 which gives the Fermi wave vector in terms of the electron density, kF = (3π 2 n)1/3 . The conductivity becomes at last σ =

ne2 τ/m , 1 − iωτ

(8.39)

identical to Eqs. 4.8 and 8.21. So after about ﬁve pages of labor, I get the same conductivity that I found either classically in Chapter 4 or in the simple free-electron model earlier in this chapter. Let me list the assumptions (or simpliﬁcations) I made in order to get here: • Collisions are represented by a scattering time τk . • The scattering time is the same for all electrons, independent of their energy or wave vector. • The deviations from equilibrium are small. • The temperature is uniform in the sample. • The temperature is small.

9

Optical Excitations: Quantum Mechanics

Once I begin to consider the atomic and electronic structure of a solid, I have to move from the comfortable conﬁnes of the free-electron model and allow for there to be a potential energy. For many important solids (silicon!), the electronic structure and optical properties are given by band theory; for others (those called highly correlated or strongly interacting materials), one must go beyond band structure and consider the strong Coulomb forces and other interactions among the electrons. I’ll discuss interband transitions and strongly interacting materials in subsequent chapters. Here, I want to look at the interaction of electromagnetic ﬁelds with a quantummechanical solid. I will introduce the issue by considering that the solid has at least two “bands,” each containing a ﬁxed number of k states. Allowing for spin, I’ll take this number as being equal to two states per atom (or per chemical formula – such as GaAs – in compound materials) in the solid. Moreover, I’ll posit that there are enough electrons to ﬁll completely the lowerenergy band, called the valence band. The higher energy band – the conduction band – consists of empty states.∗ How is the optical response affected by this electronic structure? Well, the Pauli principle remains dominant, so there are no intraband transitions in a full band; all states are occupied.† Thus, the lowest-energy optically allowed excitations are from the highest (occupied) state in the valence band to the lowest (unoccupied) state in the conduction band. More important, all transitions are from valence to conduction band. These optical transitions (lowest or not) must satisfy energy conservation, Ec = Ev + hω ¯

(9.1)

where Ec is the unoccupied state in the conduction band, Ev is the occupied state in the valence band, and hω ¯ is the photon energy. The transition must also satisfy momentum conservation, kc = kv + qγ

(9.2)

where k represents the crystal momentum of the electrons and qγ that of the photon. The scales are quite different. The range of k in each band is ±π/a ∼ ± 5 × 108 cm−1 . But, if Ec − Ev is of order 1 eV, then the photon wave vector is q = 2π/λ ∼ 5 × 104 cm−1 . The ratio of photon momentum to electron momentum is 1×10−4 . Hence, kc = kv ; optical transitions are vertical, because on a plot of energies versus Ev and Ec , the energy of the ﬁnal state is directly above the energy of the initial state. ∗ These names are historical, and a little misleading. In typical semiconductors, conduction can be accomplished

by either electrons in the conduction band or holes in the valence band.

† And none in an empty band either.

137

138

Optical Excitations: Quantum Mechanics

There is one loophole. If the valence band to conduction band transition can take advantage of some other excitation, then energy conservation becomes Ec = Ev + h¯ ω ± h ¯

(9.3)

where h ¯ is the energy of the excitation∗ (e.g., a phonon). Momentum conservation must also be satisﬁed: kc = kv + qγ ± k

(9.4)

where k , the crystal momentum of the excitation, is typically in the range ±π/a (like that of the electrons) so the initial and ﬁnal state can be widely separated on the dispersion relation. The selection rules given by Eqs. 9.1 and 9.2 are for direct optical transitions. Those in Eqs. 9.3 and 9.4 are for indirect optical transitions.

9.1 The Solid with an Electromagnetic Field I start with a crystalline solid and the electromagnetic wave. The Hamiltonian is a sum of kinetic and potential energies: H = T +V. Here, T is the kinetic energy, T =

1 e 2 p+ A , 2m c

with p = −i h∇ ¯ the momentum and A the vector potential.† The potential energy is periodic in T the translation vector of the lattice; V (r) = V (r + T). ∗ The ± is there because the excitation may either be created or (if excited by thermal processes) destroyed. † There is a certain mysterious character to the vector potential. It is a function from which the magnetic ﬁeld and

the electric ﬁeld both can be calculated: In nonmagnetic materials, B=H=∇ ×A

and

E=−

1 ∂A , c ∂t

(9.5)

when the scalar potential is equal to zero. (As it should be for transverse ﬁelds: if is of plane-wave form then the gradient, E, is parallel to k.) Let me construct a vector potential consistent with our plane-wave ﬁelds: ˆ 0 ei (q·r−ωt ) E = eE from which Maxwell’s equations lead to q = N ω/c and H=

c ˆ 0 ei (q·r−ωt ) . q × E = N (qˆ × e)E ω

I write an A that gives E via Eq. 9.5 ˆ 0 A = −i eE

c i (q·r−ωt ) e . ω (Continued on next page.)

139

9.2 Perturbation Expansion

The kinetic energy is proportional to the square of a vector, the scalar product of the vector with itself. I must preserve the order of the terms. Thus

e e2 2 1 e 2 p + p · A + A ·p + 2A . T = 2m c c c Now, look at the commutators [x,px ] = xpx − px x = i h¯ and∗ [f (r),px ] = f (r)px − px f (r) = i h¯

∂ f (r) ∂x

so ∂ Ax ∂x and the same for [Ay ,py ] and [Az,pz ]. I then can reform the vectors, with the derivative turning into a divergence [Ax ,px ] = Ax px − px Ax = i h¯

p · A = A · p − i h∇ ¯ · A. Thus T =

ieh¯ 1 2e p2 + A · p − ∇ ·A+ 2m c c

e2 2 . A c2

(9.6)

Now, the external ﬁeld is weak, so I will keep only the ﬁrst-order terms,† dropping the one in A2 .‡ I use the Coulomb gauge, ∇ · A = 0, eliminating the third term. I also use p = −i h∇ ¯ to ﬁnd H = H0 + H1 = −

h¯ 2 2 ieh¯ ∇ − A · ∇ + V (r). 2m mc

9.2 Perturbation Expansion Perturbation theory is widely used in quantum mechanics and many other areas of physics. The basic idea is to break a problem that cannot be solved exactly into two parts. There is a part with a known solution, described by a zero-order or unperturbed Hamiltonian, and (Check it. The time derivative brings down −iω.) Then c i (q·r−ωt ) ˆ 0 ∇ × A = iq × −i eE e ω ˆ 0 ei (q·r−ωt ) = N (qˆ × e)E =H with H = N E.

∗ The ﬁrst equation is obvious from p = −i h ∂ and xp C = 0 and p xC = −i hC. ¯ ∂x ¯ x x x † In a minute I will start a perturbation theory calculation. ‡ Were it to be kept, there would be nonlinear behavior, as (e−iωt )2 becomes e−2iωt , a doubled frequency.

140

Optical Excitations: Quantum Mechanics

a second part, assumed weak, that is the perturbation Hamiltonian. The wave functions and energy levels of the zero-order system are corrected, usually in a power series in the strength of the perturbation. It is not uncommon to truncate the series after the ﬁrst nonzero term. I’ll take the zero-order Hamiltonian to be the Hamiltonian for the electrons in the solid h¯ 2 2 ∇ + V, 2m which I will not solve. Instead, it is solved by others, who provide me and the world with the energy-band structure of the solid. I therefore suppose that I know the eigenfunctions of H0 , H0 = −

H0 |n = En |n ⇒ n|H0 |n = En, |n are a complete where the En are a set of energies in the various bands and the vectors orthonormal set, satisfying nn = δnn . This zero-order Hamiltonian H0 is independent of the time. Hence I know that the time-dependent wave function associated with |n is ψn (t) = |n e−i En t/h¯ . The perturbation comes from the electromagnetic ﬁeld eh¯ A · ∇. mc This perturbation contains the vector potential A(t) and so is time dependent. I use timedependent perturbation theory, writing the perturbed wave function as a linear combination of the eigenfunctions of H0 , an (t) n e−i En t/h¯ . ψ= H1 = −i

n

(If the energy is in the continuum, the sum becomes an integral.) Now, I calculate using the time-dependent Schr¨odinger equation Hψ = (H0 + H1 )ψ = i h¯ Let me do this in pieces. First H0 H0 ψ =

n

=

∂ψ . ∂t

an (t)H0 n e−i En t/h¯ , an (t)En n e−i En t/h¯ ,

n

then the perturbation H1 ψ =

an (t)e−i En t/h¯ H1 n ,

n

and then the time derivative

∂an (t) ∂ψ E n

−i En t/h¯ = i h¯ n e i h¯ e−i En t/h¯ . + i h¯ an (t) n −i ∂t ∂t h¯

n

n

141

9.3 The Matrix Element of the Perturbation

I put this all together to get an (t)e−i En t/h¯ En n + an (t)e−i En t/h¯ H1 n n

n

= i h¯

∂an (t) n e−i En t/h¯ ∂t

+

an (t) n En e−i En t/h¯ .

n

n

The ﬁrst and last terms are identical and cancel. I am left with an (t)e−i En t/h¯ H1 n = i h¯ a˙ n (t) n e−i En t/h¯ n

n

where the dot over an (t) on the right-hand side signiﬁes a time derivative. Multiply from the left by n| an (t)e−i En t/h¯ nH1 n = i h¯ a˙ n (t) nn e−i En t/h¯ . n

n

Because nn = δnn , only one term on the right, n = n, survives, so i h¯ a˙ n (t)e−i En t/h¯ = an (t)e−i En t/h¯ nH1 n . n

Now I multiply by ei En t/h¯ , deﬁne the matrix element as H1nn = nH1 n , and the frequency difference as ωnn = (En − En )/h, ¯ and I get i h¯ a˙ n (t) = an (t)H1nn eiωnn t . (9.7) n

Other than the omission of the A2 term I have yet to make an approximation. Now is the time to do so. First-order perturbation theory consists of considering the ﬁeld to have been turned on at time t = 0 and using an (0) in Eq. 9.7 rather than an (t). Moreover, I will assume that the system at t = 0 is in its ground state (n = 0) so that a0 (0) = 1 and all the others are zero. Only one term on the right of Eq. 9.7 remains: i h¯ a˙ n (t) = H1n0 eiωn0 t .

(9.8)

9.3 The Matrix Element of the Perturbation Let me take a look again at H1 : H1 = −i

eh¯ A·∇ mc

with c A = −i E. ω

(9.9)

142

Optical Excitations: Quantum Mechanics

I’ll take the electric ﬁeld to be a real (observable) ﬁeld: E = E0 cos(q · r − ωt) =

E0 i (q·r−ωt ) e + e−i (q·r−ωt ) . 2

Hence H1 = −

eh¯ cos(q · r − ωt)E0 · ∇ mω

and the matrix element I need is H1n0 = −

eh¯ n cos(q · r − ωt)E0 · ∇ 0 . mω

I can make a number of simpliﬁcations. First, the matrix element contains cos(q·r−ωt), but I have argued that q = 0. Essentially, the light ﬁeld varies slowly on the scale of the unit cell or the size of an electron wave packet so that I may take it as constant in space on that scale.∗ This long-wavelength approximation allows me to take the time-dependent parts as well as the ﬁeld amplitude vector out of the matrix element. I get eh¯ −iωt e + eiωt n|∇|0 · E0 . (9.10) H1n0 = − 2mω I will return to momentum by using −i h∇ ¯ = p so that n|∇|0 = (i/h) ¯ n|p|0. Note that it is the component of the momentum (i.e., velocity) in the direction of the ﬁeld that is important. Now, I’ll manipulate the momentum matrix element, n|p|0 = m

d n|r|0 . dt

To take the derivative, I need to insert the time dependence of n| and |0. These are eiωn t and e−iω0 t respectively.† The derivative with respect to time then works on d iωn t n|r|0 e−iω0 t = im(ωn − ω0 )eiωn t n|r|0 e−iω0 t . n|p|0 = m e dt Now ωn = En /h¯ for each n, so h(ω ¯ n − ω0 ) is the energy difference between the initial and ﬁnal states, which in turn equals (by energy conservation, Eq. 9.1) the photon energy h¯ ω. So the momentum matrix element is equal to n|p|0 = imω n|r|0 . I put everything together and obtain e −iωt e H1n0 = + eiωt n|r|0 · E0 . (9.11) 2 The quantity −er is the classical value of the electric dipole moment associated with the electron’s optical transition. At this point it is convenient to let the electric ﬁeld be polarized in a speciﬁc direction, which I will take to be the xˆ direction, making n|r|0 · E0 = n|x|0 E0 . Later I may need to do an angular average. ∗ The plane wave states eik·r of course have equal amplitude everywhere in the crystal. But the appropriate length

scale is not the crystal size, but instead is some length between the lattice constant and the mean free path.

† Remember that n| is the complex conjugate of |n.

143

9.4 Fermi’s “Golden Rule”

9.4 Fermi’s “Golden Rule” I put the matrix element of Eq. 9.11 into Eq. 9.8:

e i h¯ a˙ n = ei (ωn0 −ω)t + ei (ωn0 +ω)t n|x|0 · E0 . 2

(9.12)

The next step is to integrate Eq. 9.12. I turn on the perturbation at time t = 0 and integrate to time t. The left side integrates to t dt a˙ n = i ha i h¯ ¯ n (t) 0

because an (0) is by hypothesis zero for all times t ≤ 0. The right side contains terms like t e i ( )t − 1

. dt ei ()t = i 0 Then e an (t) = 2h¯

1 − ei (ωn0 −ω)t 1 − ei (ωn0 +ω)t + ωn0 − ω ωn0 + ω

n|x|0 E0 .

(9.13)

The ﬁrst term inside the parenthesis is resonant when ω ≈ ωn0 and corresponds to a photon absorption process. The energy balance is hω ¯ = hω ¯ n0 = En − E0 : the electron is promoted from state |0 to state |n and a photon disappears. The second term corresponds to a photon emission process. It is resonant when ω = −ωn0 : the electron drops from state |n to state |0 and a photon appears. The second term is negligible for absorption and I’ll discard it at this time.∗ I notice that if a common term of ei (ωno −ω)t/2 is factored from the absorption term, then it can be cast as (ω −ω) (ωn0 −ω) ie sin n02 t n|x|0 E0 ei 2 t . (9.14) an (t) = − h¯ ωn0 − ω What I want to know is not the amplitude to be in state |n but the rate at which transitions to that state occur. So ﬁrst I’ll write the probability Pn to be in that state: (ω −ω) e2 sin2 n02 t ∗ Pn (t) = an an = 2 (9.15) | n|x|0 |2 |E0 |2 . (ωn0 − ω)2 h¯ The transition rate Wn is the derivative of the probability with respect to time. The timedependent factor is the quantity sin2 (ωn0 − ω)t/2 and (using a trigonometric identity in the last step)

∗ The numerators are at most two. The denominator of the absorption term approaches zero at the resonance,

making that term arbitrarily large. The denominator of the emission term is always big and so that term can be neglected.

144

Optical Excitations: Quantum Mechanics

d (ωn0 − ω) (ωn0 − ω) ωn0 − ω 2 (ωn0 − ω) sin t = 2 sin t cos t dt 2 2 2 2

ωn0 − ω sin(ωn0 − ω)t = 2 and so Wn =

e2 2h¯ 2

| n|x|0 |2 |E0 |2

sin(ωn0 − ω)t ωn0 − ω

(9.16)

is the rate at which transitions from the ground state to the excited state occur. The rate is proportional to the square of the electric ﬁeld, or to the intensity, I ∼ |E0 |2 . That the transition rate is proportional to the intensity should not be a surprise. I’ve calculated the response of the semiconductor to photons, and the intensity I is I = γ h¯ ω, where γ is the photon ﬂux (photons/unit area·unit time) and hω ¯ is the photon energy. The quantity at the end of Eq. 9.16, F (ω) ≡ sin(ωn0 − ω)t/(ωn0 − ω), oscillates with time with period T = 2π/|ωn0 − ω|. The period is small and oscillations are fast when |ωn0 − ω| is large. In the other limit, when ω ≈ ωn0 , the period is long; if t T then I can expand the sine function and ﬁnd that F (ω) ≈ t. Figure 9.1 shows the function F (ω) at two times t. The function has a maximum centered at wn0 that grows with t and a width that shrinks with t. As the time becomes larger, the function becomes increasingly narrow. In fact, this function is one representation of the delta function. By integrating it, I ﬁnd that (independent of the time) ∞ sin(ωn0 − ω)t = π. dω (ωn0 − ω) −∞ I can therefore write sin(ωn0 − ω)t/(ωn0 − ω) = π δ(ωn0 − ω). I do that now and get Wn =

Fig. 9.1

π e2 2h¯ 2

| n|x|0 |2 |E0 |2 δ(ωn0 − ω).

Frequency dependence of F (ω) = sin(ωn0 − ω)t/(ωn0 − ω) at two times t.

(9.17)

145

9.5 Electric Dipole Transitions

This equation is a version of Fermi’s “golden rule” of quantum mechanics. It says that the transition rate is proportional to the square of a matrix element between ground and excited state with an energy-conserving delta function.∗ If I integrate it over a density of states ρ(ω) for the excited states, then the delta function picks out ρ(ωn0 ), giving another version of the golden rule. Wn =

π e2 2h¯ 2

ρ(ωn0 )| n|x|0 |2 |E0 |2 .

(9.18)

One generally takes n|x|0 as independent of frequency and removes it from integrals. It is then the frequency dependence of the density of states that governs the transition rate. The physics is contained in Wn , but it would be good to convert to the conductivity or dielectric function. I’ll do so by considering the relation between the absorption of light and the transition rate. If light is absorbed in a small thickness dx in the solid then Eq. 3.25 tells me that the change of intensity is dI (x) = −αI (x)dx; the energy lost per unit area per second is αI (x)dx. Equation 9.16 gives the energy lost per unit area per second as hωW ¯ n dx. Equating these, I get hωW ¯ n . I If now I use Eq. 3.23 to write the intensity in terms of the ﬁeld amplitude and Eq. 3.27 for the relation between α and σ 1 , I can write α=

σ1 =

2hωW ¯ n . |E0 |2

(9.19)

9.5 Electric Dipole Transitions Another approach to the dielectric function goes by way of the dipole moment. The dipole moment† is p = ψf −erψi + ψi −erψf where ψi = |0 e−iω0 t is the initial (ground) state wave function (hω ¯ 0 = E0 ) and an |n e−iωn t (hω ψf = ¯ n = En ) is the excited state wave function. Note that I am letting the excited state be a linear combination of all the unoccupied states |n. Energy conservation will determine which value of n is important when the frequency is ω. The induced dipole moment will be parallel to the electric ﬁeld, the xˆ direction, leading to $ # px = −e an∗ eiωn0 t n|x|0 + an e−iωn0 t 0|x|n with the energy difference ωn0 = ωn − ω0 .

∗ I can show the energy conservation explicitly by writing δ(ω − ω) = hδ(E − E − hω). ¯ ¯ n n0 0 † I’ll use, for the moment, p for the dipole moment because p is used for momentum.

146

Optical Excitations: Quantum Mechanics Now substitute for an (t) from Eq. 9.13 and calculate and substitute for an∗ (t) also. Note that px has one factor of n|x|0 as does an , so there will be terms like | n|x|0 |2 in the dipole moment. After some algebra, I get 2e2 ωn0 px = | n|x|0 |2 E0 cos ωt = αe E h¯ n ωn20 − ω2 where αe is the polarizability and E = E0 cos ωt is the electric ﬁeld. I can add a (simulated) damping by letting ωn0 → ωn0 − iγn /2, with γn a small imaginary part. If I wanted to think about it, I would say that γn is related to the inverse of the excited state lifetime, and so to the width of the transition. I could go further and say that lifetime effects stop the narrowing of F (ω) in Fig. 9.1 when the time reaches this lifetime. With this included, the polarizability is ωn0 2e2 | n|x|0 |2 . (9.20) αe = h¯ n ω˜ n20 − ω2 − iωγn The tilde on ω˜ n0 is meant to indicate that the damping pulls down the resonant frequency. (Expanding a square root, I get ω˜ n0 ≈ ωn0 − γn2 /8ωn0 .) But local ﬁeld corrections, introduced in Chapter 4, Sections 4.4.2 and 4.4.3, will lead to larger shifts. Also, I have cheated a bit and written ωn0 γn = ωγn ; I am comfortable doing this because the delta function in Eq. 9.17 enforces ωn0 = ω. Equation 9.20 gives the polarizability of the site where the excitation lives. All that I have used here is that there is a ground state |0 and a set of excited states |n at some location in the crystal. The details of the location are not speciﬁed, nor is the path taken by the electron going from |0 to |n. I may reasonably assert that the transitions occur within an atom or pair of atoms, or perhaps a molecule in the solid. They involve one electron leaving the ground state (where its absence is called a hole) and entering one or another of the excited states. There is a total of n such electrons in each unit volume of the solid.∗ Now, in the ground state of the solid there are many electrons, and these electrons occupy many energy levels. The ground state, |0, represents the initial energy of any of these electrons. So in one case it might be an electron near the top of the valence band and in another case a core electron in the band made from the 1s orbitals of the atoms in the crystal. With these considerations, I’ll just add up all possible states, make local-ﬁeld corrections (by dropping the tilde!), and obtain the dielectric function: ωn0 8π ne2 | n|x|0 |2 . (9.21) =1+ 2 2 h¯ n ωn0 − ω − iωγn

9.6 The Oscillator Strength Equation 9.21 is of Lorentzian form, just like Eq. 4.31. I can make it look a bit more familiar by deﬁning ∗ I used n as the index of the states in the unperturbed Hamiltonian because I wanted to suggest these were the

principal quantum numbers of the atomic energy levels. So I will use this Gothic n for the number density.

147

9.6 The Oscillator Strength

fn0 ≡

2mωn0 2 | n|x|0 |2 = | n|px |0 |2 h¯ hω ¯ n0 m

(9.22)

where m is the mass of the electron.∗ The quantity fn0 is known as the “oscillator strength” of the transition. Using it, I can write as (ω) = 1 +

fn0 4π ne2 2 2 m n ωn0 − ω − iωγn

(9.23)

and it is clear that n is the total number density of electrons in the solid, n = ZNatoms /V , with Z the atomic number (or the average atomic number in a compound). The imaginary part, 2 , has a series of peaks at the resonant frequencies {ωn0 }. The widths of these peaks are set by the values of {γn }; as γn → 0 the width of that peak becomes narrower and narrower until, eventually, it becomes a delta function,† 2 ∼δ(ω − ωn0 ).

9.6.1 Limiting values of I learn something by thinking about Eq. 9.23 in both low- and high-frequency limits. First, when ω → 0, 1 (0) = 1 +

4π ne2 fn0 . 2 m n ωn0

(9.24)

Note that 2 (0) = 0; this approach does not consider free carriers. Note further that if fn0 is large, ωn0 is small, or both, that value of n contributes a lot to the static dielectric constant. Next, I evaluate at high frequencies. 1 (∞) = 1 −

4π ne2 fn0 . mω2 n

(9.25)

Eq. 9.25 resembles the response of perfectly free carriers.‡

9.6.2 Another Definition of Oscillator Strength Note that in many papers, especially papers about lattice dynamics (phonons), the dielectric function is written as I did in Eq. 5.28, with a factor Sn ωn2 in the numerator: (ω) = 1 +

n

Sn ωn2 . ωn2 − ω2 − iωγn

Clearly Sn ωn2 =

4π ne2 fn0 . m

∗ The actual mass, 9.10938291×10−28 grams, and not some effective mass. † I can prove this from Kramers–Kronig; see Chapter 10. ‡ As it should if the frequency is high enough. Note that f n n0 is just a number. I’ll compute it in a couple of

pages.

148

Optical Excitations: Quantum Mechanics

9.7 Oscillator Strength Sum Rule I turn to the sum that appears in Eq. 9.25, a sum over all the states n of fn0 . 2m fn0 = ωn0 | n|x|0 |2 h ¯ n n Now | n|x|0 |2 = (n|x|0)∗ (n|x|0) = 0|x|n n|x|0 and ωn0 = (En − E0 )/h. ¯ Finally, I’ll use up the factor of 2 by writing the same thing twice: & m % 0|x|n (En − E0 ) n|x|0 + 0|x|n (En − E0 ) n|x|0 . fn0 = 2 (9.26) h¯ n n Of course I did not know that I wanted to write Eq. 9.26 as I just wrote it until I had worked the following little problems: First I look at the matrix element of the commutator of H0 , the unperturbed Hamiltonian with x: n[H0,x]0 = n|H0 x − xH0 |0 = n|En x − xE0 |0 = (En − E0 ) n|x|0 where I used the fact that H0 |n = En |n and went leftward in the ﬁrst term of the commutator and rightward in the second. An identical process yields 0[H0,x]n = −(En − E0 ) 0|x|n . I inspect Eq. 9.26 and see that I can include both commutators neatly into it: & m % 0|x|n n[H0,x]0 − 0[H0,x]n n|x|0 . fn0 = 2 h¯ n n

(9.27)

Next, I recall the trick from quantum mechanics [15] where the teacher “inserts a complete set of states”∗ 0|A|n n|B|0 = 0|A { n |n n|}| B 0 = 0|AB|0 n

where A and B are arbitrary operators and n |n n| = 1. This trick simpliﬁes Eq. 9.27 a lot, m fn0 = 2 ( 0x [H0,x]0 − 0[H0,x] x 0 ) h¯ n m = 2 0(x [H0,x] − [H0,x] x)0 h¯ m = − 2 0[ [H0,x] ,x]0 h¯

∗ Or, rather, the way I have derived it, de-inserts them.

(9.28)

149

9.7 Oscillator Strength Sum Rule

where I chose to write a minus sign in front with the double commutator in the last line because I liked its looks more than the other possibility ([ x, [H0,x]],]). Equation 9.28 is a remarkable result: The sum over all the fn0 would seem to require knowledge of all the excited states {|n} but instead it requires only the ground state wave function |0. However, the analysis can continue a bit further. I recall that H0 = T + V with T the kinetic energy and V the potential energy. The latter is a complicated function of location in the crystal, V = V (r). But! Any function of r commutes with x. Thus [V ,x] = 0 and n

m fn0 = − 2 0[ [T ,x] ,x]0 . h¯

So, in addition to the ground-state wave function being the only one that matters, only the kinetic energy in the ground state, along with the dipole moment (x), appears in the sum. Of course the ground state wave function depends on the potential; the calculation must at some time ﬁnd the eigenfunctions and eigenstates of (T + V ) |n = En |n.

9.7.1 Kinetic Energy In the Schr¨odinger picture, the kinetic energy is just p2 /2m or T =−

h¯ 2 2 ∇ 2m

but this is not the only possibility. In the tight-binding approach to band structure, one often includes a second-quantized term in the Hamiltonian that allows electrons to hop between two atomic orbitals: H = −t

†

(ci,σ cj,σ + h.c.),

i,j ,σ †

where t is a hopping integral, ciσ and cj σ are creation and annihilation operators, i,j are site indices for the two orbitals, and σ is a spin index. The Schr¨odinger picture is particularly useful in the evaluation of n fn0 . I write out the commutator: [ [T ,x] ,x] = [(T x − xT ),x] = T x 2 − 2xT x + x 2 T =−

h¯ 2 2 2 (∇ x − 2x∇ 2 x + x 2 ∇ 2 ). 2m

150

Optical Excitations: Quantum Mechanics Now, as I did earlier,∗ I write [ [T ,x] ,x] C = − Thus,

h¯ 2 2 2 h¯ 2 (∇ x − 2x∇ 2 x + x 2 ∇ 2 )C = − C. 2m m

n

h¯ 2 |0 , fn0 = − 2 0| − m h¯ m

= 0|0 = 1. This extremely simple result is called the Thomas-Reiche-Kuhn sum rule. It sets a limit on the values of all the oscillator strengths in the dielectric function. Moreover, the sum is independent of lots of details about what is happening in the solid.

9.7.2 Sum Rule for the Conductivity I apply this sum rule to the expression I wrote for the conductivity. σ 1 (ω) =

ne2 m

n

fn0 ω2 γn . (ωn20 − ω2 )2 + ω2 γn2

I integrate both sides of this ∞ ∞ ne2 ω 2 γn dω σ 1 (ω) = fn0 dω 2 . m n (ωn0 − ω2 )2 + ω2 γn2 0 0 I can do some changes of variables to simplify the integral on the right, and then look it up. Or I can just look it up. This deﬁnite integral equals π/2. Therefore, ∞ π ne2 π ne2 (9.29) dω σ 1 (ω) = fn0 = 2 m n 2 m 0 because the sum on f is unity. The integral is independent of the value of the resonant frequency or of the damping. ∗ If you do not like this, then I will try it on an arbitrary function f (x). (f (x) = C is one such function.) I do it 2 in one dimension, so ∇ 2 = ∂ 2 and f means derivative with respect to x. ∂x h¯ 2 2 2 [ [T ,x] ,x] f (x) = − (∇ x − 2x∇ 2 x + x 2 ∇ 2 )f (x)

2m ∂ ∂ h¯ 2 [2xf (x) + x 2 f (x)] − 2x [f (x) + xf (x)] + x 2 f

(x) =− 2m ∂x ∂x =−

=−

h¯ 2 {2f (x) + 2xf (x) + x 2 f

(x) + 2xf (x) − 2xf (x) 2m − 2xf f (x) − 2x 2 f

(x) + x 2 f

(x)} h¯ 2 f (x) m

Most of the terms cancel, leaving only the result of taking two derivatives of x 2 multiplied by f (x). Just as in the case where f (x) = C.

151

9.7 Oscillator Strength Sum Rule

I will check this by considering the Drude conductivity. The only charge carriers in this model are those in the Fermi sphere, and σ 1 (ω) =

ωp2 τ/4π 1 + ω2 τ 2

with ωp2 = 4π ne2 /m. Do the integral:

∞

0

dω σ 1 (ω) = =

∞

dω 0 ωp2

4π 0

ωp2 τ/4π 1 + ω2 τ 2

∞

dz

1 1 + z2

where z = ωτ . The integral is π/2 so that ∞ 1 π ne2 . dω σ 1 (ω) = ωp2 = 8 2 m 0

(9.30)

The integral is independent of the mean free time τ . It says that if, for example, the metal is cooled to low temperatures, and the conductivity increases by the residual resistivity ratio, then the increase in the area under σ 1 (ω) at very low frequencies is offset by a decrease at higher frequencies. The Drude function becomes taller and narrower and the sum rule explains how this happens.

10

Kramers–Kronig Relations and Sum Rules

The Kramers–Kronig relation [102, 103] is a consequence of our experience that observable effects are causal, i.e., that the cause precedes the effect.∗ This notion seems sensible and it is a component of most parts of physics. This chapter will start with a couple of examples where I show that there must be some relationship between the real and imaginary parts of the complex dielectric function or of the complex conductivity. Then, I’ll derive the relation for a number of our favorite response functions and follow with the use of Kramers–Kronig analysis for the reﬂectance, a common method for estimating response functions from experiment. The chapter ends with the derivation of some sum rules from the Kramers–Kronig relations.

10.1 Absorption and Dispersion Must Be Related 10.1.1 A Notch Filter To illustrate what causality implies for the optical constants that I have deﬁned and used, let me do a gedankenexperiment. I imagine the following situation: I need an optical ﬁlter that is opaque for one wavelength and transparent for a wide band of wavelengths around the stop-wavelength. The transmission of such a ﬁlter should be 100% except at the speciﬁc wavelength of opacity, where it is zero. This ﬁlter, and others like it, differencing only in the speciﬁc wavelength of operation, could be part of some wavelength multiplexing scheme where the data streams of many receivers are put onto an optical transmission line; the ﬁlter is used to select out the wavelength of a single receiver and to pass the others onward.† The design transmission of the ﬁlter is shown in Fig. 10.1, plotted versus frequency rather than versus wavelength. Now let me imagine that my signal is a pulse such as the one in the upper panel of Fig. 10.2. The pulse has several oscillations over a period of about 1 ps; outside this time window, there is very small pulse amplitude. The power spectrum of the pulse is shown in the inset; the bandwidth is about 4 THz wide, centered at 5 THz. Clearly the pulse is not a sine or cosine with a single frequency. Indeed, Fourier teaches that I can write the function f (t) as an integral: ∞ 1 dω F (ω) eiωt , f (t) = 2π −∞ ∗ Noncausal effects are part of what is called magic. † I know; there are many holes in this concept. It is, after all, only a gedankenexperiment.

152

153

10.1 Absorption and Dispersion Must Be Related

Fig. 10.1

A hypothetical filter that transmits 0–600 cm−1 (0–18 THz) except for a band 0.001 cm−1 (30 MHz) wide at ω0 = 194 cm−1 (5.8 THz).

Fig. 10.2

Upper panel: A pulse with frequency components between 3 and 7 THz. The zero of time is chosen to be at the peak of the pulse. The actual time when the signal arrives at the detector is determined by when it was transmitted and how long it took to get there. The inset shows the power spectrum of the pulse. Lower panel: The pulse after the amplitude at 5.8 THz was set to zero.

154

Kramers–Kronig Relations and Sum Rules where F (ω) is the spectrum needed∗ to give f (t). To give a good representation of the pulse, many frequencies will enter F (ω). Now, I will let the pulse be incident on my ﬁlter. The ﬁlter removes one frequency, ω0 = 5.8 THz, from the spectrum. Suppose the amplitude of the this component is A; the frequency spectrum behind the ﬁlter will be something like† G(ω) = F (ω) − Aeiφ δ(ω − ω0 ) where φ is the phase of the ω0 component. I have subtracted this contribution from the spectrum to represent the effect of the ﬁlter. The pulse will be changed of course, now its spectrum is ∞ 1 dω G(ω) eiωt , g(t) = 2π −∞ ∞ 1 dω [F (ω) − Aeiφ δ(ω − ω0 )] eiωt , = 2π −∞ = f (t) − A cos(ω0 t + φ). This result looks quite reasonable at ﬁrst. My ﬁlter has done what I asked it to do: remove the ω0 part of the pulse and transmit the rest. But then I realize that cos(ω0 t + φ) is ﬁnite at all times,‡ including large negative times! The bottom panel of Fig. 10.2 shows the amplitude after one frequency component was removed. The effect of the ﬁlter is to produce a signal at the detector long before the pulse arrived at the ﬁlter. This early appearance is a violation of causality and of course cannot happen. The ﬁx is exactly the mechanism used to generate the pulse in the ﬁrst place: the phases of nearby Fourier components are adjusted so as to interfere destructively – indeed, perfectly so – and to cancel everything outside the times where the signal is nonzero. The ﬁlter can (and will) produce amplitudes at later times than the end of the original pulse; such ringing is an unavoidable consequence of having a narrow-band ﬁlter response. (Think of a struck bell.) But no signal will appear before the leading edge of the pulse arrives. The ﬁlter must have a dispersive behavior, with a refractive index different from unity, especially near the absorption frequency. The refractive index of the Lorentzian oscillator, shown in Fig. 4.13, displays this behavior. The frequency-dependent refractive index will give frequency dependence to the velocity of the waves in the medium, accomplishing the required phase shifting. The amount of phase shift depends on the absorption properties of the ﬁlter, meaning that there must be a relation between the refractive index and extinction coefﬁcient or between the real and imaginary parts of the conductivity.

10.1.2 The Perfect Conductor The notch ﬁlter example is striking, but gives no easy route to ﬁnding the relation between real and imaginary parts of the response function. Here is a second example, said to be due ∗ I calculate F (ω) by taking the inverse transform of f (t). † I think of the pulse as being measured as a voltage or ﬁeld; I will have to worry about specifying the real and

imaginary parts correctly so that the measured signal will be real. But this is my gedankenexperiment and I won’t think too much about this detail. ‡ Except for its zeros, of course.

155

10.1 Absorption and Dispersion Must Be Related

to Tinkham [104]. If there are no collisions, the conductivity of the Drude metal, Eqs. 4.8 or 8.21, is ne2 (10.1) mω i.e., zero real part and an imaginary part that diverges as 1/ω. This form for σ is easy to derive. The equation of motion, Eq. 4.4, with no damping ( = 0) is σ =i

m¨r = −eEext . I take e−iωt time dependences for Eext and v = r˙ to ﬁnd that e E v = −i mω and then write j = −nev = σ E to obtain Eq. 10.1. This derivation is ﬁne for monochromatic electric ﬁelds, and there can be no causality issues for them because the ﬁeld amplitude is constant∗ for −∞ < t < ∞. But here, I will do the opposite. Let the applied ﬁeld be an impulse, a delta function in time† and of unit amplitude ˆ E(t) = eδ(t). This impulsive ﬁeld has a frequency spectrum that is inﬁnitely wide. I know this because I know that a representation of the delta function is ∞ 1 dω eiωt , δ(t) = 2π −∞ with frequency spectrum

D(ω) ≡

∞ −∞

dt δ(t)e−iωt = 1,

ˆ making the spectrum E(ω) have unit amplitude at all frequencies: E(ω) = e. The time dependence of the current is also the Fourier transform of its frequency spectrum. Using j(ω) = σ (ω)E(ω), I get ∞ 1 dω σ (ω)E(ω)eiωt . j(t) = 2π −∞ Now, I substitute E(ω) = eˆ and Eq. 10.1 for the conductivity: ∞ ne2 eiωt j(t) = i eˆ dω . 2π m −∞ ω

∗ When I took classical mechanics and the instructor covered the forced harmonic oscillator, there was discussion

of the turn-on transient. The oscillator responded at its resonant frequency when the force was initially applied, but then the internal damping reduced the amplitude of oscillations at this frequency to a negligible value after a few relaxation times had passed. If I turn on the ﬁeld at t = −∞, there is not a problem with the transient. † Which might as well be centered at t = 0.

156

Kramers–Kronig Relations and Sum Rules

I look up the integral and ﬁnd

⎧ 2 ⎪ ⎨+ ne eˆ if t > 0 2m . (10.2) j(t) = ⎪ ⎩− ne2 eˆ if t < 0 2m Here is another noncausal result. The current ﬂows in the direction of the electric ﬁeld polarization after the pulse arrives (as I would expect) but ﬂows in the opposite direction beforehand. What is missing? Well, I can get Eq. 10.1 by taking the Drude conductivity, Eq. 4.8, and letting τ → ∞: σ = (ne2 τ/m)/(1 − iωτ ) → (ne2 τ/m)/(−iωτ ) = ine2 /mω. Taking this limit is reasonable as long as I do not think about the ω = 0 case; if I do, I would start with σ = (ne2 τ/m) → ∞. The Drude DC conductivity is real; σ1 (ω) has a maximum at zero frequency and a width of 1/τ (see Fig. 4.1). As τ increases, the peak becomes higher and higher and the width narrower and narrower. In the limit, the real part becomes a delta function in frequency, located at the origin. Let me add this delta function to σ : ne2 , (10.3) mω where A is the weight (unknown at the moment) of the delta function.∗ The delta function term in σ is responsible for a current responding to the impulsive electric ﬁeld as ∞ A 1 ˆ ˆ iωt = e. dω Aδ(ω)ee j(t) = 2π −∞ 2π σ = Aδ(ω) + i

Note that this current is constant in time and also violates causality! However, if I take A=

ne2 π . m

ˆ 2 /2m. The delta-function contribution exactly I can make this contribution be j = ene 2 cancels the current from the −ne /mω term for negative times and doubles it for positive times. The total current is now ! 0 if t < 0 , (10.4) j(t) = ne2 eˆ if t > 0 m a step function. The impulse starts a current which, in the absence of damping, continues indeﬁnitely.† Equation 10.4 makes me much happier than Eq. 10.2. ∗ Although I might guess that it is related to the area under σ (ω) in Eq. 4.10a. I calculated this area already; see 1

Eq. 9.30.

† The result in Eq. 10.4 is easy to obtain from the equation of motion: I write j = −nev and ma = −eE(t) to ﬁnd

dv ne2 ne2 dj ˆ = −ne = E(t) = δ(t)e, dt dt m m where eˆ is a unit vector in the E direction. I can integrate this equation (from −∞ to t) to get ! 0 if t < 0 j(t) = . ne2 eˆ if t > 0 m The current is zero for t < 0 and then jumps to a ﬁnal value when the impulse arrives.

157

10.2 Kramers–Kronig Integrals

10.2 Kramers–Kronig Integrals The Kramers–Kronig integrals are derived in a number of textbooks [2, 3, 54, 105] and have been discussed by many authors [60, 106–114]. The subject is mostly approached by considering integrals on the complex frequency plane, although the original derivations by Kramers and Kronig relied on model dielectric functions [114].

10.2.1 Time Domain Response and Causality To begin, I discuss the way in which the dipole moment per unit volume P depends on the electric ﬁeld E. These vectors are related by χ , a susceptibility,∗ P = χE where χ is the electric susceptibility and χ = ( − 1)/4π . More generally, I can write the dipole moment per unit volume at location r and time t as an integral of the electric ﬁeld over nearby locations and recent times, P(r,t) = d 3 r dt χ (r,r ,t,t )E(r ,t ). Now, I want local response, so that I will be able to use local relations like j = σ E and D = E; to obtain this, I write the space part of χ as a delta function. Moreover, the time part should depend only on the difference between t and t : χ (r,r ,t,t ) = δ(r − r )χ (t − t ). Then

P(r,t) =

∞

−∞

dt χ (t − t )E(r,t ),

(10.5)

where the polarization at r depends only on the ﬁeld at r. Of course, I do not make the response local in time. I know that a response can be retarded in time, with a phase difference between the sinusoidal ﬁeld and the sinusoidal polarization or a ringing after an impulsive ﬁeld. Causality sets a requirement on the form of χ (t − t ): there can be no response before the stimulus. Suppose E = Aδ(t − t0 ), an impulse of amplitude A at time t0 . Then P(t) = χ (t − t0 )A. Causality requires that χ (t − t0 ) = 0 for t < t0 so that P(t) is likewise zero for t < t0 . Equation 10.5 becomes t dt χ (t − t )E(r,t ). (10.6) P(r,t) = −∞

∗ I am going to use χ to represent the relation between dipole moment per unit volume and electric ﬁeld for

linear (and isotropic and homogeneous) media. The ﬁelds are functions of space and time and χ will depend on the time difference between when the ﬁeld had a speciﬁc value and when the dipole moment per unit volume response exists. But later, χ = χ (ω), the relation between ﬁeld at ω and dipole moment per unit volume at ω. I will therefore state the arguments of χ explicitly here. Elsewhere, it will almost always be χ (ω).

158

Kramers–Kronig Relations and Sum Rules

Eq. 10.6 is a statement that the dipole moment at time t can be affected by the electric ﬁeld values at all times before t but none after. Equation 10.6 may be rewritten if I deﬁne τ = t − t . Then dt = −dτ and ∞ P(r,t) = dτ χ (τ )E(r,t − τ ), (10.7) 0

where the lower limit is at zero to force the response to be causal.

10.2.2 Fourier Transformation into the Frequency Domain The Kramers–Kronig integral takes place in the frequency domain. I know that the time response and frequency response are Fourier transform pairs. ∞ ∞ 1 dt E(t)e−iωt , E(t) = dω E(ω)eiωt . (10.8) E(ω) = 2π −∞ −∞ Similarly,

P (ω) =

and (using the shift theorem)

χ (ω) =

∞

−∞

∞

dt P (t)eiωt ,

(10.9)

−∞ ∞

dt χ (t − t )eiω(t−t ),

=

dτ χ (τ )eiωτ ,

(10.10)

0

where the second line uses the same substitution I used in going from Eqs. 10.5 and 10.6 to Eq. 10.7. This version is important because it shows two things. First, I can take P and E to be real in Eq. 10.7. Hence χ (τ ) is also real. Of course χ (ω) is complex on account of the complex exponential in Eq. 10.10. But the reality of χ (τ ) along with Eq. 10.10 means that χ (−ω) = χ ∗ (ω) (ω real) or that χ 1 (−ω) = χ 1 (ω) and χ 2 (−ω) = −χ 2 (ω). Second, in the next few pages I am going to allow ω to be a complex quantity, ω1 + iω2 , so that I can consider the properties of χ (ω) as a complex function of a complex variable. Equation 10.10 then shows that, as long as χ (τ ) is ﬁnite for all τ , as it should be because I am restricting myself to linear materials, χ (ω) has no poles in the upper half plane,∗ even as Im(ω) → +∞. Now, I substitute Eq. 10.5 into Eq. 10.9, noting that the directions of P and E are the same, to get ∞ ∞ dt dt χ (t − t )E(t )eiωt , P (ω) = −∞

−∞

I use the usual trick, exchanging the order of integration. I will also insert e−iωt eiωt = 1 ∞ ∞

iωt −iωt χ eiωt . dt E(t ) dt (t − t )e e P (ω) = −∞

−∞

∗ There are of course divergences in the lower half plane, where e−ω2 t rapidly diverges as −ω or t become 2

large.

159

10.2 Kramers–Kronig Integrals

The term in square braces is χ (ω). After moving it out of the integral, what remains is E(ω). Thus, I get a linear relation between polarization and electric ﬁeld: P (ω) = χ (ω)E(ω)

(10.11)

Note that the convolution theorem of Fourier analysis would allow me to go from Eq. 10.5 to Eq. 10.11 directly; the former is a convolution in the time domain whereas the latter is a product in the frequency domain.

10.2.3 The Complex ω Plane I now consider χ (ω) to be a complex function of a complex frequency, ω = ω1 + iω2 . The range of both real and imaginary parts is −∞ ↔ ∞. The function has these properties: 1. χ (ω) is analytic in the upper half plane. (This arises—as discussed above—because χ (τ ) is zero for τ < 0.) 2. χ (ω) → 0 as |ω| → ∞ at least as fast as 1/ω. 3. χ (ω) is Hermitian: χ (−ω) = χ ∗ (ω). Are these reasonable? Well, the Lorentz oscillator satisﬁes these conditions. It is: χ (ω) =

ne2 /m . ω02 − ω2 − iωγ

This function has poles when the denominator is zero. The poles are at frequencies ω = ± ω02 − γ 2 /4 − iγ /2 and lie in the lower half plane. As the frequencies become very large χ (ω) = −ne2 /mω2 and so is zero as |ω| → ∞. Finally, I write it as χ (ω) =

' 2 ( ne2 /m (ω0 − ω2 ) + iωγ . 2 2 2 2 2 (ω0 − ω ) + ω γ

By inspection, I can see that χ (−ω) = χ ∗ (ω); the only term that is affected either by complex conjugation or by negation—and in the same way—is iωγ . Free carriers have the same high-frequency limiting behavior. Indeed, all particles are free at high enough frequencies, so the χ (ω)∼1/ω2 behavior is quite general. See also Eq. 9.25. Electromagnetism is unchanged as ω → −ω or, equivalently, whether I take an e−iωt or an eiωt form for the electric ﬁeld. Let me start with the former, E = E0 e−iωt Eq. 10.11 can be written P (ω) = [χ 1 (ω) + i χ 2 (ω)][E0 cos(ωt) − iE0 sin(ωt)] but the observable is the real part of this equation, Re(P ) = χ 1 (ω)E0 cos(ωt) + χ 2 (ω)E0 sin(ωt).

160

Fig. 10.3

Kramers–Kronig Relations and Sum Rules

Contour used for deriving the Kramers–Kronig relation in the complex plane, where ω = ω1 + iω2 . The four segments that make up the closed contour are shown. I want this equation to be unchanged when ω is replaced by −ω. This condition does hold, because χ 1 (ω) = χ 1 (−ω) and χ 2 (ω) = −χ 2 (−ω). χ 1 (ω) is said to be an even function while χ 2 (ω) is an odd function of ω. This statement is equivalent to saying that χ is Hermitian, so that χ (−ω) = χ ∗ (ω).

10.2.4 Use of Cauchy’s Theorem I will use Cauchy’s integral theorem [115] to derive the Kramers–Kronig relation [102, 103]. This theorem states that the line integral along a closed path of an analytic function is zero. My susceptibility χ (ω ) is such a function if I restrict myself to the upper half plane in the complex ω space.∗ In addition, the function χ (ω )/(ω − ω), with ω exactly on the real axis, is also analytic in the upper half plane. Cauchy’s theorem then states that ) χ (ω ) =0 (10.12) dω ω −ω for any closed contour in the upper half plane. I will use the contour shown in Fig. 10.3. It starts (1) at (−∞,0), runs along the real axis until it is close to the point (ω,0). It then (2) makes a semicircle around (ω,0) in the upper half plane, and (3) continues along the real axis to (∞,0). The path is closed by making a large† semicircle (4) of radius inﬁnity in the upper half plane, joining the start of segment (1). ∗ I write the frequency with a prime because I want to use ω as the dummy variable of integration. † Very large!

161

10.2 Kramers–Kronig Integrals

Now, I break the integral up into its four segments χ (ω ) χ (ω ) χ (ω ) χ (ω ) + + + , 0= dω dω dω dω ω −ω ω −ω ω −ω ω −ω (1 ) (2) (3 ) (4) and look at each one of these. On segment (4), the length of the semicircle increases proportional to |ω|, but the integrand vanishes. The integral is zero so long as χ (ω) falls at least as fast as 1/|ω|. And it does, according to our assumptions above. The line of segment (2) may be parameterized by writing ω = ω + ueiφ where φ is the angle the radius vector makes to the Re ω axis. As the path moves around the semicircle, the angle goes from π to 0. The quantity u is the (constant) radius of the semicircle. If u is small enough, the value of χ (ω ) is the same for all points on the little semicircle.∗ I can replace χ (ω ) with χ (ω). Finally, dω = ueiφ i dφ. Then 0 χ (ω ) '0 1

χ = iu (ω) dω dφ eiφ iφ = i χ (ω)φ π = −iπ χ (ω). ω −ω ue (2 ) π Segments (1) and (3) combine to make a principal-value integral, ∞ χ χ (ω ) χ (ω ) (ω ) + =P dω . dω dω

ω −ω ω −ω (1) (3) −∞ ω − ω I combine all four segments to obtain ∞ ) χ (ω ) χ (ω )

=P − iπ χ (ω) = 0. dω dω ω −ω ω −ω −∞ This equation can be rearranged to give the Kramers–Kronig relation, ∞ χ (ω ) 1 χ (ω) = P . (10.13) dω iπ ω −ω −∞ There is an i in the denominator, so that the real part of χ is given by an integral of the imaginary part of χ and vice versa. I substitute χ (ω) = χ 1 (ω) + i χ 2 (ω) on both sides; Equation 10.13 must hold for both its real and its imaginary parts, giving ∞ χ 2 (ω ) χ 1 (ω) = 1 P dω π ω −ω −∞ and 1 χ 2 (ω) = − P π

∞ −∞

dω

χ 1 (ω ) ω − ω

,

(10.14)

(10.15)

where P denotes the Cauchy principal value. The real and imaginary parts of χ are not independent: the complex function can be constructed given just one of its parts. If I had chosen segment (2) to be a semi-circle below instead of above the point (ω,0), " I would have had† (2) = +iπ χ (ω) but the pole at ω would be inside the closed contour, so the contour integral will pick up the residue of the pole, 2iπ χ (ω), making the result (of course) be the same. ∗ How small is small enough? In the case of the Lorentz oscillator, I must have u γ . † Because then ω = ω − ueiφ .

162

Kramers–Kronig Relations and Sum Rules

10.2.5 Eliminating Negative Frequencies Equations 10.14 and 10.15 are not as useful as they could be, because the integrals cover −∞ → ∞, implying that I must know the susceptibility at negative frequencies.∗ However, as discussed earlier in this chapter, near the end of Section 10.2.3, χ 1 (ω) is an even function of frequency and χ 2 (ω) is an odd function of frequency. I can use these properties to reduce the integration range to 0 → ∞. I start with Eq. 10.14, which gives the real part, χ 1 (ω), and transform the integral into two of speciﬁc parities by multiplying both the numerator and the denominator of the integrand by ω + ω. Separating into two integrals yields ∞ ∞

χ

χ 2 (ω ) ω

ω 2 (ω )

χ 1 (ω) = 1 P P dω + dω π π ω 2 − ω2 ω 2 − ω2 −∞ −∞ Now, χ 2 (ω) is odd so that the second integral vanishes; the part from −∞ → 0 exactly cancels the part from 0 → ∞. Further, ωχ 2 (ω) is even, so the part of the ﬁrst integral from

−∞ → 0 exactly equals the part from 0 → ∞. So I only need to do the integral from 0 → ∞ and multiply by two, obtaining† ∞ ω χ 2 (ω ) 2 χ 1 (ω) = P dω 2 . (10.16) π ω − ω2 0 I carry out the same derivation for the imaginary part and get ∞ χ 1 (ω ) χ 2 (ω) = − 2ω P dω 2 . π ω − ω2 0

(10.17)

Eqs. 10.16 and 10.17 show the Kramers–Kronig relations in the form usually used for analysis of optical functions.

10.2.6 Case When the DC Conductivity Is Finite I have made a mistake (or, perhaps, have omitted something) in the previous section. Suppose the solid has a ﬁnite DC conductivity. Many solids do, including metals, superconductors, doped semiconductors, and so forth. Then at low frequencies, χ (ω) = iσdc /ω, which diverges at ω = 0. There is a pole at the origin and the contour of Fig. 10.3 runs right through it. To handle this, I will write the susceptibility for the conductor as an analytic part χ a plus the divergent term: χ = χ a + iσdc /ω. I can then assert that χ a ≡ χ − iσdc /ω is analytic in the upper half plane and so satisﬁes the Kramers–Kronig relation. The integral of Eq. 10.17 becomes

∗ My signal generator or spectrometer only has positive frequencies on its dial. † If you want to work through this in detail, break the single integral over −∞ → ∞ (Eq. 10.14) into two, one from −∞ → 0 and a second from 0 → ∞. In the ﬁrst, deﬁne ω

= −ω and substitute for ω everywhere, including dω and the limits. You will arrive a the results given here.

163

10.2 Kramers–Kronig Integrals

χ 2 (ω) =

∞ χ 1 (ω ) σdc 2ω dω 2 . − P ω π ω − ω2 0

(10.18)

(Eq. 10.16 is unchanged.)

10.2.7 Kramers–Kronig Analysis of Other Optical Functions There are many complex optical functions in addition to the susceptibility: dielectric function, conductivity, refractive index, etc. and there are Kramers–Kronig relations among all of them. Many can be obtained by substitution. For example, = 1 + 4π χ and σ 1 = ωχ 2 = ω2 /4π so that ∞ ω 2 (ω ) 2 1 (ω) = 1 + P dω 2 , (10.19) π ω − ω2 0 or 1 (ω) = 1 + 8P

∞

0

dω

σ 1 (ω ) ω 2 − ω2

.

(10.20)

Also, ∞ 2ω [1 (ω ) − 1] 4π σdc − P dω , 2 (ω) = ω π ω 2 − ω2 0

(10.21)

∞ σ2 (ω ) 2ω2 P dω . π ω (ω 2 − ω2 ) 0

(10.22)

or, equivalently, σ 1 (ω) = σdc −

Kramers–Kronig relations are commonly used for estimating many optical functions from experiments that give one member of a complex pair. Among these are σ1 → σ2 , Im(1/) → Re(1/), n → κ, κ or α = 2ωκ/c → n, and R → φ. Of these, the calculation of the phase shift on reﬂectance from the reﬂectance itself is by far the most commonly used and will be discussed in detail in the following subsection. Table 10.1 shows a number of functions used in Kramers–Kronig integrals. But note also that moments of these functions also are consistent with the Kramers–Kronig relations as long as the moments satisfy the convergence condition speciﬁed at the beginning of Section 10.2.3. I write the general integral as ∞ f (x) 2 dx 2 (10.23) I(ω) = P π x − ω2 0 and then show in the left column the form f (x) must take to be put in to Eq. 10.23. The right column shows the function that would be obtained and its dependence on I(ω). The complex quantities here are the dielectric function, = 1 + i2 , the conductivity, σ = σ 1 + iσ 2 , the susceptibility, χ = χ 1 + i χ 2 , the refractive index, N = n + iκ, the loss function, (1/) = 1 /(12 +22 )−i 2 /(12 +22 ), and the surface impedance, Zs = Rs +iXs .

164

Kramers–Kronig Relations and Sum Rules

Table 10.1 A function f (x) is integrated to give I (ω). The possibilities for f (x) and the result in terms of I (ω) are given here. f (x)

→

x2 (x) 1 (x) − 1 σ 1 (x) σ 2 (x)/x x χ 2 (x) χ 1 (x) xκ(x) n−1 x[− Im(1/(x)] Re[1/(x)] − 1 xXs (x) Rs − Z0

→ → → → → → → → → → → →

KK transform 1 (ω) 2 (ω) σ 2 (ω) σ 1 (ω) χ 1 (ω) χ 2 (ω) n(ω) κ(ω) Re[1/(ω)] − Im(1/(ω)] Rs Xs

= = = = = = = = = = = =

1+I (4π σdc /ω) − ωI −ωI σdc + ω2 I I (σdc /ω) − ωI 1+I −ωI 1−I ωI Z0 + I −ωI

Z0 = 377 = 4π/c is the impedance of free space.

10.3 Kramers–Kronig Analysis of Reflectance Kramers–Kronig analysis, of – for the most part – reﬂectance data, is commonly used to estimate the optical conductivity, dielectric function, sum rules, and other optical functions for new materials. Many reports of Kramers–Kronig analysis of reﬂectance have appeared, spanning more than a 50 years [116], with studies of metals [44, 45, 49–52, 59, 60], pure and doped elemental solids [117–119], organic conductors [120–122], charge-density-wave materials [123–125], conducting polymers [126–128], cuprate superconductors [129–139], manganites [140–142], pnictides [143–149], heavy-Fermions [150], multiferroics [151– 154], topological insulators [155–157], and many others. In addition, a number of methods papers have appeared [109, 111, 158–163]. When I measure the reﬂectance,∗ I am taking the ratio of the reﬂected intensity or power to the incident intensity or power. Phase information is not available.† The amplitude reﬂectivity, Eq. 3.32, does have a phase; indeed I can write it as r = ρeiφ =

1−N , 1+N

√ where ρ = R is the magnitude of the reﬂectivity, R is the single-bounce reﬂectance, φ is the phase shift on reﬂection, and N = n + iκ is the complex refractive index. ∗ Reﬂectance here means the single-bounce reﬂectance, R, as discussed in Chapter 3 (Section 3.2) and given in

Eq. 3.33.

† Measuring the phase shift on reﬂection is difﬁcult. The phase of the electromagnetic ﬁeld changes by 2π for

every wavelength of travel of the light, so that a phase-sensitive measurement requires control of lengths to a small fraction of the wavelength.

165

10.3 Kramers–Kronig Analysis of Reflectance

It would be nice to know φ, because I could invert Eq. 3.32 to get √ 1 − Reiφ , N= √ 1 + Reiφ

(10.24)

using the known φ and the measured reﬂectance.∗ Kramers–Kronig analysis is one way of estimating this phase [54, 158, 164, 165]. Consider ln r = ln ρ + iφ. Here, ln ρ is the real part and φ is the imaginary part. The reﬂectance must be causal, and hence so must be the log of the reﬂectance. Equations 10.14 and 10.15 become ∞ φ(ω ) 1 , (10.25) dω ln ρ(ω) = P π ω −ω −∞ and 1 φ(ω) = − P π

∞

−∞

dω

ln ρ(ω ) . ω − ω

(10.26)

The hermiticity of r, r(−ω) = [r(ω)]∗ , proves that ρ is even and φ is odd. I use these properties as I did earlier for χ to obtain ∞ ln ρ(ω ) 2ω dω 2 . (10.27) φ(ω) = − P π ω − ω2 0 Equation 10.27 is perfectly usable for numerical analysis, but there is one improvement that can be made [54]. I write ∞ 1 dω 2 = 0. (10.28) P

ω − ω2 0 The integral is zero because the negative area for ω < ω cancels the positive area for ω > ω. Thus, I can add ∞ 2ω 1 ln ρ(ω)P + dω 2

π ω − ω2 0

∗ Every time I encounter the formula in Eq. 10.24 I think that it contains an algebra error and that the minus and

plus signs are transposed. But then I recall that the phase shift for nonabsorbing materials with n > 1 is −π so that r is negative. The range of φ is −π ≤ φ ≤ 0. If I want to have a positive phase, I could deﬁne θ = φ + π so that eiθ = −eiφ . In this case, √ 1 + Reiθ N= √ 1 − Reiθ and, of course, ρeiθ =

N −1 . N +1

The range of θ is 0 ≤ θ ≤ π . The real part of ρeiθ becomes negative when n < 1 and κ is small, requiring θ > π/2.

166

Kramers–Kronig Relations and Sum Rules

to the right the phase. Collecting terms, replacing √ hand side of Eq. 10.27 without affecting ∗ ρ with R, and using the properties of the log, I get ∞ ln[R(ω )/R(ω)] ω dω . (10.29) φ(ω) = − P π ω 2 − ω2 0 This modiﬁcation has two advantages. First, if there are errors in the calibration of the reﬂectance measurements, so that the data for R are in error by a constant factor, the results for φ are unaffected. Second, both numerator and denominator of the integrand are zero when ω = ω. L’Hˆopital’s rule shows that the ratio does not diverge; hence the pole has been removed. The second consequence is more important than the ﬁrst. Removing the pole is important for simple evaluation of the integral. Although the scale error does not affect the phase, it does affect R, and Eq. 10.24 shows that N depends on both phase and reﬂectance. As a ﬁnal note, Eq. 10.28 shows that the factor [(ω ) − 1] may be replaced by (ω ) in Eqs. 10.21 and 10.22. However, if I want to do a numerical integral, I will prefer to keep it as it is, so that [(ω ) − 1] → 0 as ω → ∞.

10.3.1 Extrapolations The alert reader will have noticed that the range of the integrals in Eqs. 10.16–10.22 and 10.29 is 0 to ∞ and may wonder how one acquires data over that entire range. The answer of course is that data are always limited to a ﬁnite range of frequencies. The experimenter typically has data from far infrared through near ultraviolet, covering, say, 5 meV–5 eV (40–40,000 cm−1 ). This is a reasonably wide bandwidth, but extrapolations must always be made outside the measured range. The high frequency extrapolation is especially problematic and can cause signiﬁcant distortions to the conductivity over the entire measured range, with consequences for sum rules as well. I will discuss these extrapolations in the context of Kramers–Kronig analysis of reﬂectance, but the same approaches can be used for other functions. One must estimate the reﬂectance between zero and the lowest measured frequency. The best approach is to employ a model that reasonably describes the low-frequency data. Such models include Drude for metals, Lorentz for insulators, often a sum of several Lorentzians, sometimes a Drude plus Lorentzians. Many other functions exist. When a good ﬁt of the model to the data is obtained, a set of reﬂectance points may be calculated between zero and the lowest measured frequency, using a spacing between points similar to that of the lowest-frequency data, and combined with the measured data. Other approaches to the low-frequency extrapolations include an assumption that the reﬂectance is constant to DC or the use of the Hagen Rubens formula for a conductor, R = 1 − Aω1/2 . (Other funcitons, such as R = 1 − Aωs , with s in the range 1–4, are used as well.) The constant A is adjusted so the extrapolation goes through the ﬁrst few points and then, using a spacing between points similar to that of the lowest-frequency data, a ∗ ln

√ R = (1 /2 ) ln R and ln A − ln B = ln(A/B).

167

10.3 Kramers–Kronig Analysis of Reflectance

set of extrapolated reﬂectance points is calculated between zero and the lowest measured frequency and combined with the measured data. I have already mentioned that the high-frequency extrapolation can be a source of major error [166]. It is good to use data from other experiments on identical or similar samples if these exist. Or, one can measure far into the ultraviolet with synchrotron radiation if one has access to such a facility. Moving to the highest frequencies, one knows that in the limit as ω → ∞, the dielectric function is mostly real and slightly smaller than unity, following = 1 − ωp2 /ω2 , where ωp is the plasma frequency of all the electrons in the solid and ω ωp . Then n = 1 − ωp2 /2ω2 and R = ωp4 /8ω4 ≡ C/ω4 . It has been usual to ﬁll the region between the highest-frequency data point and the transition to ω−4 with a weaker power law, R ∼ B/ωs with 0 < s < 4. (s does not have to be an integer.) This midrange power law is adjusted to match the slope of the data and to give pleasing curves, but the choice of power (typically between 1 and 3) is arbitrary. The value of B is chosen so that the power law joins smoothly to the data at the high frequency limit; the value of C is also chosen for a smooth transition between mid- and high-frequency extrapolations. The free parameters are the exponent s and the frequency for the crossover from ω−s and ω−4 . The integrals in the extrapolation range may be done analytically [54] and their contributions added to the phase obtained by numerical integration of Eq. 10.29 over the low-frequency extrapolation and the measured data. Although simple, this midrange power-law extrapolation is arbitrary and affects in very noticeable ways the conductivity spectrum, sum rules, etc. There is a better way. It is fairly simple to extrapolate using X-ray atomic scattering functions developed by Henke and coworkers [22, 167]. These extrapolations basically treat the solid as a linear combination of its atomic constituents and, knowing the chemical formula and the density, allow the computation of dielectric function, reﬂectivity, and other optical functions. The “Henke reﬂectivity” can be used over photon energies of 10 eV–34 keV, after which a 1/ω4 continuation is perfectly ﬁne. Photoabsorption in the x-ray region has been considered by a number of authors [168– 175]. It is described by an atomic scattering function, a complex quantity: f = f1 + if2 . The approach used by these authors is to combine experiment and theory and determine the imaginary part of the scattering factor, f2 , for each atomic species. This quantity has peaks or discontinuities at the absorption thresholds for each electronic level and falls to zero as ω → ∞. The real part f1 is obtained by Kramers–Kronig integration of f2 , It increases with frequency via a series of plateaus, each approximately equal to the number of “free” electrons at that photon energy. Electrons are free if their binding energies are much less than the photon energy. The limiting high frequency value is – except for relativistic corrections – then the atomic number Z. The starting point is a set of tables of the scattering factors for each element devised by Henke, Gullikson, and Davis [22] in 1993. A related web site also exists [167] with the ability to calculate optical properties, including reﬂectance. I ﬁnd however that better results are found if two adjustments are made, one to the scattering functions f and one to the procedure of using these function to calculate reﬂectance. The ﬁrst is that the functions of Ref. 22 provide f2 from 10 to 30,000 eV but only have f1 from 30 to 30,000 eV. I have

168

Kramers–Kronig Relations and Sum Rules redone the Kramers–Kronig integrals of f2 to provide f1 also from 10 eV (80,000 cm−1 ), extrapolating f2 ∼ ω2 at low frequencies and f2 ∼ ω−1 at high frequencies. To estimate the high-frequency properties of a material, one makes the assumption that the solid consists of a linear combination of its component atomic constituents, with the dielectric function determined by the scattering factors and the number density of the constituents. The dielectric function is then 4π nj e2 j j (f1 − if2 ), (10.30) =1− mω2 j

where the sum runs over atoms j at number density nj and with complex scattering factor j f j . Note that this has the right limiting high-frequency behavior, because f1 → Z j (with j j Z here the atomic number) and f2 → 0, so that → 1 − j 4π nj Z e2 /mω2 . The complex refractive index∗ is √ (10.31) N= and the reﬂectance Ris

1 − N 2 . R= N + 1

(10.32)

The procedure is implemented in the following way. The user supplies the chemical formula, such as Ag or La1.85 Sr0.15 CuO4 and either the appropriate† volume Vc or the density ρ. With this information, the reﬂectance R can be calculated at 340 logarithmically spaced points over 80,000–2.4×108 cm−1 (10–30,000 eV) using Eqs. 10.30–10.32. A bridge needs to be placed over the gap between the highest experimental point (say, 40,000 cm−1 or 5 eV) and the beginning of the extrapolated reﬂectance at 80,000 cm−1 . The user has the option of a power series in ω, in 1/ω ∝ λ or a cubic spline.‡ As it turns out, the bridge has a modest effect in some cases, minimal in others. Then, the Kramers–Kronig integral, Eq. 10.29, is computed to obtain the phase. ∗ Note that Ref. 22 and the website Ref. 167 write an equation for the refractive index of a monatomic solid:

N =1−

nr0 λ2 (f1 − if2 ), 2π

with r0 = e2 /mc2 the classical radius of the electron and λ = 2π c/ω the wavelength. This is clearly the ﬁrst √ term in an expansion of N = . It is preferable to compute the dielectric function from f using Eq. 10.30, and then take the complex square root to obtain N . † There is occasional confusion – both here and in the application of partial sum rules – about the value to use for the volume Vc . This volume is described variously as the “volume of the unit cell” or the “volume of one formula unit.” Of course any carefully described volume will work, but generally one wants the number of charge carriers per atom or per primitive unit cell. And of course the conventional cell often contains several times more atoms than one would guess from the chemical formula. So the user must decide what she or he wants to determine. It may be the number of carriers per Ag atom in silver metal, the number per buckyball in C60 , the number per dopant in P-doped Si, or the number per copper atom in Bi2 Sr2 CaCu2 O8 . Once the decision is made, compute the volume in the crystal allocated to the desired quantity. One (almost) failsafe approach is to obtain the density ρ of the crystal and the mass M of the entity one is interested in, such as one Ag atom, 60 C atoms, one silicon atom divided by the dopant concentration, or 1/2 the mass of 2Bi + 2Sr + Ca + 2Cu + 8O. Then Vc = M/ρ. ‡ A cubic spline bridge occasionally causes excitement by taking the reﬂectance in the bridge region over unity or below zero.

169

10.4 Another Look at the Conductivity

Persons who wish to test the approach will ﬁnd a Windows version of the code (and the Kramers–Kronig routine that uses the extrapolation and generates the bridge function) in the program suite associated with this book. See Appendix G. Use xro.exe to generate the ﬁle for extrapolation, kk.exe to do the Kramers–Kronig integral, and op.exe to calculate optical functions. The use of reﬂectance calculated from a dielectric function made up of a sum of atomic scattering functions for a material provides a reliable and reproducible method of extrapolating measured data. It removes a certain amount of arbitrariness in the use of Kramers–Kronig analysis of reﬂectance.

10.3.2 Kramers–Kronig Analysis of Transmittance The (coherent) transmittance T of a thin∗ parallel-plate slab is related to the amplitude transmission coefﬁcient by T = |teiφt |2 where t is the amplitude and φ the phase change on passing through the sample, including the coherent addition of multiple internal reﬂections. As in reﬂectance, ln t + iφt are causal functions that satisfy causality [176–179], ∞ ln[T (ω )/T (ω)] ω ω (10.33) φt (ω) = − P dω + d, π c ω 2 − ω2 0 where d is the thickness and the last term is a correction for the phase gained on going through an identical thickness of vacuum. The equation for the transmission of a slab in terms of the refractive index or dielectric function is discussed in Chapter 7. Given T and φt , these may be inverted numerically for n and κ. Like reﬂectance, Kramers–Kronig analysis of transmittance requires extrapolations. At low frequencies, I use one of these: • Transmission is assumed constant to DC • Metallic conductivity assumed: T = B + Cω2 • Superconducting: T = Aω2 Above the experimental regime, it is good to use data from other experiments on identical or similar samples if these exist. At the highest frequencies, in the x-ray range, the data can be extrapolated as T ∼ 1 − Cω−4 as appropriate for completely free electrons. Between the highest data point and the x-ray range atomic scattering factors or a slower power law can be used.

10.4 Another Look at the Conductivity The conductivity σ , which appears in Ohm’s law, j = σ E, is a well behaved function with no poles in the upper half plane. At very high frequencies, the conductivity is that of free ∗ The thickness scale is λ/n, the wavelength divided by the refractive index. If the slab is several wavelengths

thick, the requirements on the variations in thickness and in the parallelism of the light passing through it become severe.

170

Kramers–Kronig Relations and Sum Rules

carriers, Eq. 10.1. Thus it falls like 1/ω and therefore (barely) satisﬁes the requirements speciﬁed earlier in this chapter (Section 10.2.3). Moreover σ 1 is an even function and σ 2 is odd, so that the derivation from Eq. 10.12 to 10.17 goes through exactly, and I arrive at [105] ∞ ω σ 2 (ω ) 2 dω 2 , (10.34) σ 1 (ω) = P π ω − ω2 0 and ∞ σ 1 (ω ) 2ω σ 2 (ω) = − P dω 2 . (10.35) π ω − ω2 0 Eq. 10.35 is identical to Eq. 10.20 but Eq. 10.34 differs from Eq. 10.22. The two integrals employ different moments of σ 1 .

10.5 Sum Rules A sum rule is a statement that the integral of an optical function has a ﬁxed value, is zero, or is related to a speciﬁc value of another optical function. I introduced the oscillator strength sum rule (or f sum rule) in Chapter 9, Section 9.7. Here I will brieﬂy discuss what the Kramers–Kronig relation says about sum rules [60, 107, 180–186].

10.5.1 The f Sum Rule I start by writing the high-frequency limiting value of the real part of the dielectric function. (I have written this several times before.) 1 (ω) = 1 −

ωp2

, ω2 where ωp is a plasma frequency for every electron in the solid. In the notation of Eqs. 9.21 and 9.29, 4π ne2 , ωp = m where n counts every electron in the solid. I use this funny symbol to reduce confusion with the conduction or valence electron density n. I equate this equation to the Kramers–Kronig integral of Eq. 10.20, keeping in mind that ω must be very large, ∞ ωp2 σ 1 (ω ) dω 2 . 1 − 2 = 1 + 8P ω ω − ω2 0 I now split the integral into two integrals, with the boundary frequency, ωf , less than ω but high enough that σ 1 (ωf ) is essentially zero: ωf ∞ ωp2 σ 1 (ω ) σ 1 (ω ) dω 2 +P dω 2 . − 2 =P 8ω ω − ω2 ω − ω2 0 ωf

171

10.5 Sum Rules

Because σ 1 (ωf ) is arbitrarily small, the second integral can be neglected. Because ω ωf , the term ω 2 in the ﬁrst integral can be neglected. Hence ωf ωp2 σ 1 (ω ) − 2 =P dω . 8ω −ω2 0 I can now change sign, cancel the factors of ω−2 , drop the principal value symbol (there are no divergences of the integrand), and extend the upper limit to ∞ (because by ωf I have already gotten all the area under σ 1 ) to get an equation identical to Eqs. 9.29 and 9.30: ∞ ωp2 π ne2 = . (10.36) dω σ 1 (ω ) = 8 2 m 0 See Chapter 9 for an evaluation of Eq. 10.36 for the Drude conductivity. Equation 10.36 is also a sum rule on ω2 because ω2 = 4π σ 1 ; the right hand side is 4π larger of course. A similar development of the energy loss function, Im(1/) gives:

∞ π ωp2 2π 2 ne2 1

= = . (10.37) dω ω Im − (ω ) 2 m 0 For a simple free-electron (Drude) metal, σ 1 has a maximum at zero frequency and rolls off with characteristic width 1/τ . The area under σ 1 mostly occurs at low frequencies. The loss function has a peak at ωp , with width (in a simple model where τ is not a function of frequency) 1/τ . But the integrals of both functions are proportional to the plasma frequency squared.

10.5.2 The Static Dielectric Function Sum Rule Equation 10.20 shows that the real part (the dispersive or reactive part) of the dielectric function is related to the real part of the optical conductivity. Evaluating this equation for ω = 0 yields the static dielectric function dc ≡ 1 (ω = 0) as the ω−2 moment of σ 1 , ∞ σ 1 (ω ) dc = 1 + 8P dω . (10.38) ω 2 0 This equation is not useful for conductors, because there is a divergence of the integrand at ω = 0 unless σ 1 is zero there. For insulators, one can see that conductivity peaks at low frequencies are the largest factors in determining the static dielectric constant. Peaks with high values of the optical conductivity and located at low frequencies are required for high values of the dielectric constant.∗ Moreover, there is a trend for materials with high dielectric constants or refractive indices in their transparent regions to have small band gaps; large-band-gap materials have low values of and n.

∗ The high-temperature paraelectric phase of many ferroelectric insulators has a “soft mode,” a lattice vibration

where the transverse-optic frequency goes to zero as the temperature is reduced towards the Curie temperature. The dielectric constant thus diverges at the transition.

172

Kramers–Kronig Relations and Sum Rules

10.5.3 DC Conductivity Sum Rules A third sum rule uses Eq. 10.34, evaluated at ω = 0: ∞ σ 2 (ω ) π dω = σdc,

ω 2 0 or, substituting for σ 2 ,

∞

0

dω [1 − 1 (ω )] = 2π 2 σdc .

(10.39)

Eq. 10.39 makes it evident that it is OK to convert the principal value integral into a regular integral. This equation says that the parts of 1 that are bigger than unity are balanced by parts below unity except for the free carrier pole. Note that all solids have real parts of their dielectric functions that are slightly smaller than unity at very high energies, becoming unity asymptotically as the frequency goes to inﬁnity.

10.5.4 Sum Rules for the Refractive Index The real and imaginary parts of the refractive index satisfy Kramers–Kronig relations. These are given in Table 10.1 (and Eq. 10.23). I see that 2 ∞ ω κ(ω ) n=1+ dω 2 . π 0 ω − ω2 As in the derivation for the integral of σ 1 , I argue that κ → 0 as ω → ∞ fast enough that I can stop the integral as some frequency ωf ω. I write for these large values of ω, ωp2 √ ≈1− 2ω2 where the factor of 2 comes from expanding the square root. Then ωp2 2 ∞ ω κ(ω ) − 2 = dω π 0 2ω −ω2 or ∞ π dω ω κ(ω ) = ωp2 . 4 0 n=

(10.40)

Equation 10.40 is the f sum rule for the extinction coefﬁcient. It could be written also in terms of the absorption coefﬁcient α, because α = 2ωκ/c. Now, I can write Eq. 10.36 in terms of the imaginary part of the dielectric function, where it reads ∞ π dω ω 2 (ω ) = ωp2 , 2 0 so that the result of the integrations is just twice that of Eq. 10.40. Therefore ∞ ∞

dω ω 2 (ω ) = 2 dω ω κ(ω ). 0

0

173

10.6 Partial Sum Rules But 2 = 2nκ! Hence, after minimal algebra, this equation becomes ∞ dω ω κ(ω )[n(ω ) − 1] = 0.

(10.41)

0

Finally, I can start with the Kramers–Kronig integral for κ in terms of n from Table 10.1 and do the usual high frequency evaluation (where κ = 0) to obtain a sum rule for the refractive index alone, ∞ dω [n(ω ) − 1] = 0, (10.42) 0

known as the inertia sum rule. I think that it is remarkable that the integral of n, whether weighted by ωκ or not, comes out to be the same as the refractive index of the vacuum. At some frequencies n is larger than one and at others smaller than one. But (in two senses) the average value is unity.

10.6 Partial Sum Rules The sum rule integrals extend from zero to inﬁnity. It is often informative to compute a partial sum rule. I can carry out the integral from zero to some frequency ω, and then plot the result as a function of the upper limit of the integration. I’ll formulate the problem as follows. The right-hand side of Eq. 10.36 can be written m π e2 π ne2 Neff ∗ = 2m 2mVc m where m∗ is the effective mass, m is the free electron mass, Vc is the unit cell volume (or formula volume), and Neff is the number of effective electrons within the volume Vc participating in optical transitions. Then I can write m 2mVc ω Neff (ω) = dω σ1 (ω ) (10.43) m∗ π e2 0 for the number of electrons with effective mass ratio m/m∗ participating in optical transitions at frequencies below ω. Figure 10.4 shows Neff (m/m∗ ) for a model of a metal similar to Ag. The model uses a Drude free carrier component, with 1/τ ≈ 130 cm−1 and three Lorentz oscillators, at 40,000 cm−1 (5 eV), 54,000 cm−1 (5.7 eV), and 70,000 cm−1 (8.7 eV). The conductivity is shown in the inset. The main plot shows the partial sum rule. The integral of the Drude conductivity saturates at 1 electron/Ag atom. Neff (m/m∗ ) is ﬂat over a wide frequency range and then steps up when the interband transitions begin. See section 6.1 and Fig. 6.5 for the partial sum rule analysis of Ag. Similar partial sum rules may also be written for the loss function, for the extinction coefﬁcient, and for the absorption coefﬁcient. I may also write a partial sum rule based on Eq. 10.38, ω σ 1 (ω ) dω , (10.44)

dc (ω) = 1 + 8P ω 2 0

174

Fig. 10.4

Kramers–Kronig Relations and Sum Rules

Neff (m/m∗ ) for a model of a metal similar to Ag. The inset shows the conductivity whose integral is shown in the main plot. Vc is the volume allocated to one metal atom. where I write dc (ω) to indicate that the function shows the contributions to the static dielectric constant from successively occurring peaks in the conductivity. Note that Eq. 10.44 is equivalent in some ways to writing the static dielectric function as a sum of Lorentz oscillators, as in Eqs. 4.35 and 5.30, as a functon of the number of oscillators included in the sum:

dc (N ) = 1 +

N ω2 pj j =1

ωj2

,

where I’ve set c = 1. If the oscillators are narrow compared to their separation, the integral in Eq. 10.44 will step up as the upper limit ω includes more and more resonances ωj . A third partial sum rule that I have seen used is based on Eq. 10.42. (One based in Eq. 10.41 is also possible.) I write ω dω [n(ω ) − 1].

n(ω) = 0

This function will start positive and increase as ω increases. Indeed, because the refractive index often looks like the derivative of the extinction coefﬁcient, it will resemble the latter function. But when n becomes smaller than unity at high frequencies, n(ω) will begin to decrease with increasing ω and (if all has gone well) ramp down to zero.

11

Superconductors

11.1 Superconducting Phenomena All discussions of superconductivity are supposed to start in 1911, in Leiden, when and where Kamerlingh Onnes [187] and his assistants discovered that the resistance of solid mercury abruptly falls to zero at a temperature of 4.2 K. Shown in Fig. 11.1, the resistance is falling with temperature, similar to other pure metals. (See Fig. 8.6, for example.) But then, the resistance takes a sudden drop to zero at 4.2 K. Onnes reported that the resistance was smaller than 10−5 compared to 0.11 just above Tc ; it is now believed to be identically zero. Evidence for zero resistance includes experiments, done on rings of superconducting material, in which continuous and steady currents are sustained for years with no applied voltage. In the slightly more than a century since its discovery, superconductivity has been found to be widely distributed, occurring in elements [187], alloys [188], intermetallic compounds [189], oxides [190], ionic compounds [191], organic charge-transfer compounds [192], polymers [193], and many other systems [194–207]. It seems that the only two prerequisites are (1) that the material be conductive, so that there are carriers to condense into the charged superﬂuid, and (2) that it not be a magnet; strong magnetic ﬁelds destroy superconductivity. But I should note that the conductivity does not need to be that of free-electron metals and that there are counterexamples to prerequisite 2. Figure 11.2 shows the “records” for superconductivity over a 107 year period, 1911– 2018. Several classes of materials are shown. The blue circles are metals, alloys and intermetallic compounds that are superconducting due to electron phonon interactions. The record as of 2018 is held by H3 S under enormous (155 GPa) pressure; it is thought to be an electron–phonon superconductor. The high-Tc cuprates are shown as red squares; organic conductors as magenta pincushions; fullerenes as purple triangles; heavy-Fermion metals as gold diamonds; ﬁnally, the Fe-based superconductors are in green oh-plus symbols. The diagram is probably neither complete nor accurate. It does however indicate the enormous range of material types where superconductivity is observed. The second key property of superconductors was discovered in 1929, when Meissner [208, 209] observed that a superconductor expels magnetic ﬂux, making the condition for the ﬁeld inside the superconductor be that B = 0, where B is the magnetic ﬁeld. The ﬂux expulsion is sketched in Fig. 11.3. Start with the constitutive equations, Eqs. 2.3 and 2.14 0 = B = H + 4π M = (1 + 4π χ )H . 175

176

Superconductors

Fig. 11.1

Resistance vs. temperature for Hg. (After Onnes [187].)

Fig. 11.2

Record transition temperatures in many classes of superconductors over a little more than a century. Note that there is a change of scale in the time axis at 1980; the first third covers 80 years and the second two-thirds covers 40 years. The materials with an asterisk attached require pressure to become superconducting (or to reach the Tc shown). The material with a dagger (FeSe) is a monolayer film.

177

11.1 Superconducting Phenomena

Fig. 11.3

Two spheres in a uniform external magnetic field B. The sphere on the left is a normal metal; the field penetrates uniformly. The sphere on the right is a superconductor (below Tc ). The field is expelled, making B = 0 inside. At the same time, the sphere acquires a uniform magnetization.

Fig. 11.4

Magnetization versus applied field for type I and type II superconductors. Parameters are chosen to represent Pb. Clean Pb is a type I superconductor with Hc = 800 G (0.08 T). Adding impurities to Pb renders it a type II superconductor. B is zero but H is not zero. Hence, χ =− 1 . (11.1) 4π In the Meissner state, the superconductor is a perfect diamagnet. The magnetic moment of the sphere is generated by currents which circulate on the surface of the sphere parallel to the equator.∗ The diamagnetic response continues in all or in part as the ﬁeld increases, until an upper critical ﬁeld is reached and superconductivity is destroyed. Superconductors come in two ﬂavors, illustrated in Fig. 11.4. Type I superconductors function as described above, with perfect diamagnetic response, following Eq. 11.1, up to the critical ﬁeld Hc when superconductivity ceases to exist. Type II superconductors are perfect diamagnets up to a (typically relatively low) lower critical ﬁeld called Hc1 . Above this ﬁeld, an inhomogeneous state occurs, with a magnetic ﬂux lattice existing in the superconductor. The density of ﬂux in the material grows with increasing ﬁeld. At a (typically relatively high) upper critical ﬁeld, Hc2 , the ﬂux penetration is complete. Superconductivity (zero resistance) persists up to Hc2 . The materials that remain superconducting at high ∗ Actually the currents are not on the surface but decay exponentially into the superconductor with a characteristic

penetration depth. I will calculate this depth shortly.

178

Superconductors

magnetic ﬁelds are all type II and some of these (NbTi, Nb3 Sn, YBa2 Cu3 O7 , etc.) are used in superconducting magnets. A list of superconductors is given in Table 11.1. The table lists the material, transition temperature, ﬁeld required to destroy superconductivity, and the type (I or II). Transition temperatures can be seen to vary from 15 mK (α-W) to to 200–210 K. The current record∗ is held by H3 S at very high pressure [204–207]. Although you cannot see anything with your eyes, superconductivity affects optical properties in two important ways. First, the inﬁnite DC conductivity (a delta function at ω = 0) gives a large inductive response to the imaginary part of the conductivity, just as

Table 11.1 A list of superconducting materials. The materials are organized into elements, compounds, alloys, organics, cuprates, and pnictides. Hci is the maximum field at which zero resistance is observed. The classification of I or II identifies the way magnetic flux is expelled. Formula α-Hg Al In Sn Ta Pb Nb α-W α-U Zn V C6 K C60 K3 C60 Rbx In2 O3 V3 Si Nb3 Sn Nb3 Ge MgB2 H3 S NbO TiN ZrN NbTi NbN

Tc (K) Metals 4.15 1.20 3.4 3.72 4.48 7.19 9.26 0.015 0.68 0.855 5.03 Compounds 1.5 19.8 28 3.3 17.1 18.3 23.2 39 203 (at 1,500 kbar) Binary alloys 1.38 5.6 10 10 16

∗ There are T ’s below 15 mK but none – so far – at 300 K. c

Hci (T)

Type

0.04 0.01 0.03 0.03 0.09 0.08 0.82 0.00012

I I I I I I II I I I II

0.005 1

0.013

23 24.5 37 74

II II II II II II II II

II

15 15.3

II II

179

11.1 Superconducting Phenomena

Table 11.1 continued. Formula

Tc (K)

Hci (T)

Charge-transfer salts 1.1 (at 6.5 kbar)

(TMTSF)2 PF6

Type

II

(TMTSF)2 ReO4

1.2 (at 9.5 kbar)

II

(TMTTF)2 ClO4

1.4

II

β-(ET)2 I3

1.5

II

β -(ET)2 SF5 CH2 CF2 SO3

5.3

II

10.4

κ-(ET)2 Cu(NCS)2 La1.85 Sr0.15 CuO4

Cuprates (high-Tc ) 38

La2 CuO4.11

43

YBa2 Cu3 O7 (123)

92

Bi2 Sr2 CuO6 (Bi-2201)

20

Bi2 Sr2 CaCu2 O8 (Bi-2212)

92

10

II

45

II

140

II

107

II

II II

Bi2 Sr2 Ca2 Cu3 O10 (Bi-2223)

106

II

Tl2 Ba2 CaCu2 O8 (Tl-2212)

108

II

Tl2 Ba2 Ca2 Cu3O10 (Tl-2223)

125 94

HgBa2 CuO4 (Hg-1201) HgBa2 Ca2 Cu3 O8 (Hg-1223) HgBa2 Ca2 Cu3 O8 (Hg-1223) Nd1.7 Ce0.3 CuO4 LaO0.9 F0.2 FeAs

134 164 (at 300 kbar) 24

Iron-based (pnictide) 28.5

75

II

II 190

II II II II

PrFeAsO0.89 F0.11

52

II

GdFeAsO0.85

53.5

II

BaFe1.8 Co0.2 As2

25.3

II

SmFeAsO0.85

55

II

Ba0.6 K0.4 Fe2 As2

38

II

CaFe0.9 Co0.1 AsF

22

II

Sr0.5 Sm0.5 FeAsF

56

II

FeSe

27

II

in the case of the perfect conductor, Eq. 10.3. Second there is a gap (called 2 for reasons that will become apparent) for excitations, which makes the real part of the conductivity zero for (ﬁnite) frequencies below 2 .∗

∗ The gap energy is in the far infrared, which is why your eyes see no difference between normal and

superconducting states.

180

Superconductors

11.2 Theoretical Background This book is not intended for a course in superconductivity, so I will derive neither BCS theory [210, 211] nor the phenomenological Ginzburg-Landau theory [212–214]. Here I will just list some of the results. The book by Tinkham (Ref. 215) is a good place to start reading about these theories. BCS theory [210, 211] is the microscopic theory of metallic superconductors. These superconductors have the following properties • Below Tc , electrons form Cooper pairs. The Cooper state is a superposition of two electrons of the normal metal into a zero-momentum, spin-singlet state |k ↑ , − k ↓. • The superconducting condensate is a coherent superposition of Cooper pairs, involving all the conduction electrons in the metal. • Because the pairs are made up of two electrons, the number density of Cooper pairs is nc = n/2; the charge is Qc = 2e; and the mass is mc = 2m. • The Cooper pairs exists because of an effective attractive interaction between the two electrons. • In metallic superconductors, this attraction arises through the interaction with the lattice (the phonons). • The attractive interaction reduces the energy of the electrons. In fact, the Fermi surface is unstable towards the formation of a Cooper pair even if there is only an inﬁnitesimal attractive interaction between the electrons. • To break a Cooper pair at the Fermi surface requires energy 2 = 3.5kB Tc

(11.2)

to be supplied. This energy is known as the superconducting energy gap. • In metallic (called “conventional”) superconductors, the gap is small compared to the Fermi energy. The gap scale is a few meV; the Fermi energy several eV. • Thermal energies break Cooper pairs and, because the gap is a collective effect, reduce the gap. It eventually reaches zero at Tc . The behavior (from both experiment and theory) is shown in Fig. 11.5 [216]. • Excitations above the gap are called quasiparticles. They have many of the properties of normal electrons, being spin-half Fermions, but are affected by the BCS coherence factors and have an energy-wave vector dispersion relation that differs signiﬁcantly from that of ordinary electrons in the solid. Ginzburg-Landau theory [212–214] is a phenomenological theory that is based on the Landau theory of second-order phase transitions. The free energy of a superconductor near Tc is written in terms of a complex order parameter, ψ, which is nonzero below Tc and zero above. The theory (when folded into BCS theory [217]) makes the following identiﬁcations, (11.3) ψ = nc (T )eiφ = (T ),

181

Fig. 11.5

11.3 The London Model

Superconducting energy gap measured by tunneling as a function of temperature. (After Ref. 216.)

where ψ represents a coherent superposition of all Cooper pairs, the pair density is nc , φ is the phase of the order parameter, and is the BCS energy gap. The two-ﬂuid model, in which there is a normal ﬂuid (described perhaps by the Drude model) intermixed with the superﬂuid, is consistent with the Ginzburg-Landau theory. As nc is reduced approaching Tc , (Fig. 11.5) nn grows so that n = 2nc + nn .

11.3 The London Model 11.3.1 Heuristic Derivation Dating from 1935, the London model [218] is a mix of electrodynamics and quantum mechanics. Often discussions just start by writing the London equation, but I can derive it in a relatively simple way. I’ll start by reminding myself of the deﬁnition of the electrical current carried by a set of Cooper pairs. Classically it is j = nc Qc v =

nc Qc p, mc

(11.4)

where v (p) is the average velocity (momentum) of the superconducting particles (Cooper pairs), nc is their number density, Qc is their charge, and mc is their mass. Quantum mechanically, I would write something like js =

Qc (ψ ∗ p ψ − ψp ψ ∗ ), 2mc

(11.5)

182

Superconductors

with p the momentum operator and ψ the wave function of the superconducting state, given by Eq. 11.3. In the presence of an electromagnetic ﬁeld, p = −i h∇ ¯ −

Qc A, c

(11.6)

where A is the vector potential. The requirement of charge neutrality in a homogeneous superconductor causes nc to be constant in space. Hence, from Eq. 11.3, √ −i h∇ψ = −i h¯ nc eiφ i∇φ, ¯ and Eq. 11.5 becomes nc Qc js = mc

Qc A . h¯ ∇φ − c

(11.7)

Now, for Cooper pairs, Qc = −2e

mc = 2m

and

nc =

ns , 2

with ns the superﬂuid density in a two-ﬂuid model. At zero temperature in clean metals, ns = n. Thus nc Qc /mc = −ns e/2m and nc Q2c /mc = ns e2 /m. With these replacements I arrive at js = −

ns e ns e2 A. h∇φ − ¯ 2m mc

(11.8)

The two terms in Eq. 11.8 lead to different physics. The ﬁrst term, proportional to the gradient of the phase, governs the Josephson effect, pair tunneling between two superconductors. The second term controls the electromagnetic properties of homogeneous superconductors in which the phase gradient is zero. Constant phase is expected for linear response; however, if there is a supercurrent js then there is a gradient of the phase. For the linear optical conductivity I can neglect as small the current from any phase gradient and write js = −

ns e2 A. mc

(11.9)

Eq. 11.9 is known as the London equation.

11.3.2 London Model Optical Conductivity I’ll subject the superconductor to an electric ﬁeld E = E0 e−iωt , an AC ﬁeld (or plane wave) of frequency ω. Recall that E=−

1 ∂A = E0 e−iωt , c ∂t

meaning that A=−

ic E. w

183

11.3 The London Model

I put this vector potential into Eq. 11.9 to ﬁnd ns e2 E. mω As usual, Ohm’s law is js = σ E. Therefore, the optical conductivity is js = i

(11.10)

ns e2 . (11.11) mω I have seen this before! Look at Eq. 8.25 and 10.1. Equation 11.11 is formally the same as the ﬁnite-frequency conductivity of the perfect metal: the Drude metal, Eq. 4.8, in the limit where τ → ∞. Moreover, I can deﬁne a superconducting plasma frequency 2 /4π ω, and then (using = + 4π iσ /w) get the ωps = 4π ns e2 /m, write σs = iωps s c dielectric function: σs = i

s = c −

2 ωps

, (11.12) ω2 Eq. 11.12 is the dielectric response of perfectly free carriers with no scattering. It has a negative real part and zero imaginary part. At this point I can list four questions that I must answer. They are 1. How do I get the inﬁnite DC conductivity of the superconductor? 2. How does the superconductivity affect electromagnetic wave propagation and reﬂectance? 3. What about the Meissner effect? 4. This is cute, but why do I not take a bunch of Drude-like free carriers and just let their mean free time between collisions go to inﬁnity?

11.3.3 Infinite DC Conductivity I already know the answer to the ﬁrst question; it was part of the introduction to the need for Kramers–Kronig relations. (See Section 10.1.2.) The real part of the conductivity is a delta function at ω = 0. I’ll write it as σ 1 = Aδ(ω) and substitute that into the Kramers–Kronig relation, Eq. 10.20, obtaining ∞ Aδ(ω ) dω 2 . (11.13) 1 (ω) = 1 + 8P ω − ω2 0 The integral is easy to do,∗ and I get 4A , ω2 or, equivalently, the imaginary part of the conductivity is 1 (ω) = 1 −

σ2 (ω) =

A . πω

∗ Because the lower limit of the integral is ω = 0, which is where the delta function is located, the integral only gets half the area, giving −A/2ω2 not −A/ω2 .

184

Superconductors 2 /4 = π n e2 /m. This value I compare this equation with Eq. 11.12 and see that A = ωps s for the weight of the delta function satisﬁes the sum rule, Eq. 10.36 ∞ 2 ωps π ns e2 = . (11.14) dω σ 1 (ω ) = 8 2m 0

So, ﬁnally, the London optical conductivity is ns e2 π ns e2 δ(ω) + i . (11.15) m mω If all the electrons are part of the superconducting condensate, ns = n and ωps = ωp . σ (ω) =

11.3.4 Electromagnetic Wave Propagation and Reflectance The London dielectric function (ω > 0) is purely real and negative. The refractive index in the London model is 2 ωps √ ωps . (11.16) −1≈0+i N = n + iκ = = 0 + i 2 ω ω So the real part of the refractive index∗ n = 0 and κ ≈ ωps /ω. (The approximation in Eq. 11.16 is good. The range of frequencies where the London model describes the superconducting conductivity ends at the superconducting energy gap frequency, say 5 meV or 40 cm−1 , whereas the plasma frequency of a typical metal is, say, 5 eV or 40,000 cm−1 .) The electric ﬁeld in the superconductor decays as E = E0 e−κωx/c = E0 e−x/λL with distance x away from the surface. The decay length is mc2 c c λL ≡ ≡ , (11.17) = κω ωps 4π ns e2 where λL , independent of ω, is known as the London penetration depth.† The London penetration depth plays the role of the skin depth of the metal in the electrodynamics of the superconductor. Typically it is a lot shorter than the normal-state skin depth at frequencies below the superconducting gap, where the model applies. Finally, the reﬂectance, given by Eq. 3.33, is unity. The London superconductor is a perfect reﬂector. Experimentally, superconductors are almost perfect reﬂectors at frequencies below their energy gap.

∗ I use n for both the carrier density and refractive index, here and elsewhere. Symbol duplication is an

unavoidable consequence of the limited number of glyphs in English, the adherence to convention for symbol choice, and in the use of a limited number of fonts. † The units dilemma rears its head here. ω is an angular frequency in radians/s or s−1 . But, like other plasma ps frequencies, it is often reported in cm−1 , making the London length appear to be just the vacuum wavelength of light (λp ) corresponding to this plasma frequency. But if I go through the conversions correctly (Appendix A) I get λL = λp /2π .

185

11.3 The London Model

11.3.5 Meissner Effect I now consider a superconductor with a static magnetic ﬁeld B applied parallel to the surface so as to work out the Meissner effect. I will use the London gauge: ∇ · A = 0. Using the London gauge and the London equation (Eq. 11.9) I can write ∇ ·A∝∇ ·j=−

∂ρ ∂t

where I’ve used the continuity equation on the right-hand side. If I want to think about static ﬁelds, I want no time variation of the charge density. The London gauge enforces this requirement. Before continuing, I must think a bit about Maxwell’s equations. I am about to argue that the superconductor in the presence of an external static magnetic ﬁeld B will have a supercurrent distribution js (r) which serves to make B = 0 in the interior of the superconductor, producing the Meissner effect. Now, js is not a free current in the sense of the current in the macroscopic Amp`ere’s law (Eq. 2.1d). It is a microscopic current that will generate a net magnetization of the superconductor. Therefore, I’ll write Amp`ere’s law in its microscopic form [2]: ∇ ×B=

4π js . c

(11.18)

Because the Meissner effect is a static problem, the time derivative of the electric ﬁeld is zero. Now, I take the curl of Eq. 11.9, ∇ × js = −

ns e2 ns e2 ∇ ×A=− B, mc mc

(11.19)

and take the curl again, ns e2 ∇ ×B mc ns e2 4π =− js mc c = ∇(∇ · js ) − ∇ 2 js

∇ × (∇ × js ) = −

(11.20)

= −∇ 2 js , where I used Amp`ere’s law, Eq. 11.18, to go from the ﬁrst to the second line, the properties of the double cross product to get the third line, and the London gauge condition to go from the third to the fourth line. Thus, ∇ 2 js =

4π ns e2 1 js = 2 js , mc2 λL

186

Superconductors using Eq. 11.17. The physically reasonable solution is that js = 0 deep in the interior of the superconductor and that there are surface currents which decay away from the surface as js (x) = j0 e−x/λL . So the currents are on the surface and js (x) → 0 in the interior. What about the magnetic ﬁeld B? To answer, I return to Eq. 11.18 and take the curl of both sides 4π ∇ × js c 4π ns e2 B =− c mc = ∇(∇ · B) − ∇ 2 B

∇ × (∇ × B) =

(11.21)

= −∇ 2 B, where I used Eq. 11.19 to go from the ﬁrst to the second line, the properties of the double cross product to get the third line, and Eq. 2.4b to go from the third to the fourth line. Thus, ∇ 2B =

4π ns e2 1 B = 2 B, mc2 λL

(11.22)

using Eq. 11.17 for λL . The physically reasonable solution is that B = 0 deep in the interior of the superconductor and that it decays away from the surface as B(x) = B0 e−x/λL ,

(11.23)

as sketched in Fig. 11.6. Both the ﬁeld and the current decay in the same way as a function of depth into the superconductor. The current can be thought of as the current required to generate a ﬁeld of −B0 in the interior, so that the sum of the applied ﬁeld and the generated ﬁeld is zero. Note that B ⊥ js . The current is into the page in Fig. 11.6.

Fig. 11.6

The magnetic field falls from the external value to 1/e at a distance of λL below the surface of the superconductor.

187

11.3 The London Model

11.3.6 Comparison to the Perfect Conductor It is tempting (but not correct) to think of a superconductor as a metal in which (for some reason) scattering processes have stopped happening. The metal would have a Drude conductivity, Eq. 4.10 σ (ω) =

ne2 ωτ 2 /m ne2 τ/m + i , 1 + ω2 τ 2 1 + ω2 τ 2

in which τ → ∞. The real part of the conductivity of this “perfect conductor” is the same as the London model conductivity: a delta function at the origin, inﬁnite at DC and zero at all ﬁnite frequencies. At the same time, σ 2 → ne2 /mω, either by taking the limit or by using the Kramers–Kronig relation for the conductivity. To see what the magnetic ﬁeld looks like in the interior of this perfect conductor, I will write Amp`ere’s law in its microscopic form, Eq. 11.18, take the curl, and then the time derivative 4π dj d ∇ × (∇ × B) = ∇× dt c dt where I have put the ∂E/∂t term into the current. The current can be written j = −nev. Writing out the double curl (as was done above) and using ∇ ·B = 0, this equation becomes dv d 2 4π ∇ B = − ∇ × ne dt c dt But, dv/dt = a, the acceleration, and Newton’s law for these carriers is a = −eE/m, so the right hand side becomes −

4π ne2 d 2 ∇ B= ∇ ×E dt mc Now, I can replace ∇ × E using Maxwell’s equation 2.4c, interchange the operations on the left hand side, and by analogy with Eq. 11.17 deﬁne the penetration length of the perfect conductor as λP = mc2 /4π ne2 , arriving at −

∇2

dB 1 dB = 2 . dt λP dt

(11.24)

The behavior of the time derivative of B for the perfect conductor is of the same form as Eq. 11.22 for the superconductor, except that it is for the derivative rather than for the ﬁeld itself. So for the perfect conductor, a few penetration depths from the surface, the ﬁeld can be present, but dB = 0, dt i.e., it cannot change. This behavior is the ultimate example of Lenz’s law: a current is induced in the conductor by the changing magnetic ﬁeld so directed as to oppose the change in ﬂux. Of course, the decay length of the time-varying ﬁeld is just the skin depth in the ω 1/τ limit.∗ ∗ The perfect conductor has 1/τ = 0 so any ﬁnite frequency is in the high-frequency limit.

188

Superconductors

Table 11.2 London penetration depth of superconductors. Material

˚ λL A

Al Sn Pb Nb YBa2 Cu3 O7

160 340 370 390 1,440

11.4 Length Scales for Superconductors 11.4.1 London Penetration Depth ˚ range. The penetration depth, λL = mc2 /4π ns e2 , is typically in the 100–2,000 A Some values are shown in Table 11.2. Metals with high electron density (Al) have shorter penetration depths than those with lower electron density. I know that as the temperature increases, the superﬂuid density decreases (to zero at Tc ). (See Fig. 11.5.) The penetration depth follows λL (T )∼1/ ns (T ), increasing towards Tc . √ If I use the Ginzburg-Landau temperature dependence (and the identiﬁcation of ns = , I get λL (T ) = Tc /(Tc − T ). The London penetration depth is also the “skin depth” of the superconductor. Light∗ falls off in the interior with characteristic decay length λL . It is interesting to compare the normal-state skin depth and the London length. The latter given in Eq. 11.17, repeated here: mc2 c λL = = . ωps 4π ns e2 Note that this penetration depth is frequency independent. Now, a Drude metal with σdc = ne2 τ/m has a skin depth given by Eqs. 4.38 and 4.39: ⎧ ⎪ ⎪ c2 mc2 ⎪ ω 1/τ ⎨ 2π ωσdc = 2π ne2 ωτ δ= ⎪ ⎪ mc2 ⎪ ⎩ ωc = ω 1/τ p 4π ne2 As long as ns = n (which is the case for pure metals at low temperatures) the London penetration depth is the same as the high-frequency limit of the skin depth of the metal. The low-frequency skin depth of the metal is much longer that the London length and grows as the frequency decreases.

∗ The light must be in the far-infrared range, with photon energy smaller than the energy gap, for the

superconductor to respond as a superconductor.

189

11.5 Excitations in a Superconductor

11.4.2 The Coherence Length In addition to the penetration depth discussed already, a second length scale exists. It is the coherence length, ﬁrst introduced by Pippard [219]. The coherence length also appears in Ginzburg-Landau theory [212, 213] and BCS theory [210, 215]. The three lengths are similar but not identical, either in concept or in value. I’ll give a heuristic argument as follows. The Cooper-pair wave function extends over a ﬁnite distance; at longer distances the amplitude begins to decrease. The wave function ψ thus has an envelope ψ ∼e−r/ξ0 where ξ0 is the coherence length. A consequence of the ﬁnite length is that plane waves can no longer be correct for the wave function. Instead there must be a range of wave vectors, i.e., a q-dependent theory. The range is δksc = kF ± q = kF ±

1 . ξ0

The range of wave vectors must be related to the superconducting binding energy , leading to a spread of kinetic energies, h¯ 2 kF2 h¯ 2 kF h¯ 2 (δksc )2 = ± = EF ± 2 , 2m 2m mξ0 where I have neglected the term containing 1/ξ02 . Note that this argument basically invokes the uncertainty principle: limiting the space part to ξ0 leads to a spread of momenta and corresponding spread of energies. Subtracting EF from both sides gives h¯ 2 kF /mξ0 = 2 or ξ0 =

hv h¯ 2 kF ¯ F = , 2m 2

using h¯ kF = mvF . The BCS theory gives 2 hv ¯ F , (11.25) π 2 close enough. Two materials parameters appear in Eq. 11.25. In the numerator is the Fermi velocity (or Fermi wave vector), which increases with carrier density; the denominator holds the gap (or, equivalently, the transition temperature: 2 = 3.5kTc in BCS theory). Thus high electron density, low Tc materials (think Al) will have long coherence lengths; low electron density, high Tc materials (think YBa2 Cu3 O7 ) will have short coherence lengths. This expectation is in accord with observation. See Table 11.3. ξ0 =

11.5 Excitations in a Superconductor The BCS theory [210, 211, 215] prescribes an energy gap at the Fermi level; no electron may have an energy (measured relative to the Fermi energy – aka the chemical potential)

190

Superconductors

Table 11.3 Coherence length of superconducting materials. Materials

Tc (K)

˚ ξ0 (A)

Aluminum Indium Tin Gallium Lead Niobium PbMo Nb3 Sn C60 K3 C60 Rb3 YBa2 Cu3 O7

1.19 3.40 3.72 5.90 7.22 9.25 15 17 19 31 93

12,000 3,300 2,600 1,600 800 350 25 40 30 23 15

smaller than . Similarly, no hole (the absence of an electron below the Fermi surface) may exist with an energy∗ smaller than . The gap is in the energy spectrum of single-particle excitations of the superconductor. It has an analog in the energy gap of a semiconductor. In the intrinsic (undoped) semiconductor, the Fermi level lies in the middle of the gap (with magnitude Eg ) between valence and conduction bands. The minimum excitation energies are Eg /2. But superconductors are of course not semiconductors. The gap in the latter is due to the static potential of the crystal; it occurs for a crystal momentum k at the Brillouin zone boundary. The gap in the superconductor is tied to the Fermi surface; it occurs at a wave vector k whose magnitude equals the Fermi wave vector, kF . There is no gap in the values of the wave vectors {k}! As in any solid, the wave vectors cover a continuous range, from zero to the Brillouin zone boundary or from zero to inﬁnity depending on the picture one uses. I am writing this paragraph because many discussions of superconducting gaps and gap symmetry present a cartoon where the gap is shown as a shell – with nodes or without them depending on the material – around a Fermi sphere. The picture is wrong for three reasons: (1) The Fermi sphere is a k-space entity and there are no forbidden values of the wave vector k. (2) The gap is most important for states near the Fermi surface, as I will discuss in a minute, but it affects (at least formally) all the quasiparticle states. (3) The gap applies equally to hole states below the Fermi level as to electron states above.

11.5.1 The Excitation Spectrum of a Normal Metal Before discussing the excitation spectrum of a superconductor, let me think about the excitations of a normal metal. The ground state is the T = 0 Fermi sphere shown in ∗ Hole energy is measured downwards from the Fermi level.

191

11.5 Excitations in a Superconductor Fig. 8.2. All single-particle states between zero and EF are occupied; all above are empty. There are two possible kinds of excitations. Electron-like excitations occupy states above EF and hole-like excitations correspond to vacant states below EF . If the excitations are made by (low-energy) optical absorption as intraband transitions or if they are due to ﬁnite temperatures (and the broadening of the Fermi–Dirac function), then they are made by promoting an electron from below to above EF .∗ As I mentioned at the start of Chapter 8, I’ll call the excitations, whether hole-like or electron-like, “quasiparticles.” I can plot the quasiparticle excitation spectrum of the freeelectron normal metal. The electron energies are purely kinetic h¯ 2 k 2 , 2m as in Eq. 8.4. Excitation energies are measured relative to the Fermi energy, so the energy of an electron-like or hole-like excitation h2 k 2 ¯ (11.26) − EF ≡ (k) . En (k) = 2m E(k) =

Here, (k) = h¯ 2 k 2 /2m − EF is the kinetic energy of the electron, measured relative to the Fermi energy. My plot of En (k) vs k will be almost a straight line, because I am interested in excitation energies on the scale of the superconducting energy gap. Superconducting gaps are typically a few meV, whereas the Fermi energy (Table 8.1) is typically more than 10 eV.† For meV variations around the Fermi energy, the curvature in Eq. 8.4 as a function of k is not noticeable. But to be sure that things are absolutely linear, I will plot the quasiparticle energy against the kinetic energy, measured relative to the Fermi energy, i.e., En (k) versus (k). Such a plot is shown in Fig. 11.7 as the red dashed line. The left side shows the hole-like quasiparticles and the right side the electron-like quasiparticles.

11.5.2 The Excitation Spectrum of a Superconductor The excitation spectrum of a superconductor is modiﬁed from that of the normal metal by the presence of the energy gap. In BCS theory [210, 211, 215] (11.27) Es (k) = (k)2 + 2 . The quantity Es (k) is shown in Fig. 11.7 as the blue solid line. The minimum quasiparticle energy is the gap . Because optical absorption breaks a Cooper pair and produces a pair of quasiparticles, the corresponding threshold for optical absorption is 2 . I only need a potential difference of if I tunnel electrons in‡ from a normal metal into the superconductor. ∗ There are other options. I may inject electrons by tunneling through a barrier. Unless I withdraw them

somewhere else, the metal will become charged. In small structures, this process can be observed as single electron tunneling and leads to the Coulomb blockade [220]. † There are exceptions, including the cuprate superconductors and organic superconductors. ‡ Or out; tunneling electrons out corresponds to putting a hole in. This single-particle tunneling differs from the pair tunneling of the Josephson effect. In single-particle tunneling, I must have a potential of ± between

192

Superconductors

Fig. 11.7

The excitation spectrum of a normal metal (dashes) and a superconductor (solid). The superconducting gap was taken to be = 1.2 meV (10 cm−1 ). It is remarkable that the phenomenon of superconductivity, with such a dramatic effect on electrical transport and optical properties, affects the energy spectrum of the electrons in such a modest way. Once one moves several times the gap energy away from the Fermi surface, the energy spectrum is indistinguishable, and one might say that those deeply buried (and highly excited) states are indistinguishable from the normal metal. Yet, the London penetration depth, Eq. 11.17, involves all the conduction electrons.∗ The heat capacity also suggests that all the electrons participate in the superconducting condensation. Of course, I can take the same point of view about the conduction by a normal metal, shown in Fig. 8.4. Instead of thinking that the entire Fermi sphere is displaced, I could say that a number of electrons are excited above the Fermi surface in the direction of the electron ﬂow, and an equal number of holes exist on the opposite side, where occupied electron states once existed.† For electrons far below EF , the states |k, ↑ and |−k, ↓ are both occupied with 100% probability. Are these Cooper pairs in the normal metal? Not really, because the BCS state is a coherent combination of Cooper pairs. I can also represent the excitation energy in a semiconductor picture. In such a picture, the kinetic energy is just that of the electrons, so states below EF have negative energies. I get the picture shown in Fig. 11.8. The electron-like excitations have positive energies and the hole-like ones have negative energies. That the superconducting gap is 2 is obvious

normal metal and superconductor, or I must have a potential of ±2 between two superconductors, in order to have a tunneling current. The DC Josephson effect is the tunneling of Cooper pairs between two superconductors at zero bias. ∗ In clean metals. † This is in fact what the Boltzmann equation suggests.

193

Fig. 11.8

11.5 Excitations in a Superconductor

The “semiconductor picture”of the excitation spectrum of a normal metal (dashes) and a superconductor (solid). The superconducting gap was taken to be = 1.2 meV (10 cm−1 ). The Fermi energy is at E = 0. here, because I must promote an electron from the highest-energy state below E = 0 (the Fermi energy) to the lowest energy state above E = 0. I like the excitation picture, Fig. 11.7, better. Many people do use the semiconductor picture, however.

11.5.3 The Density of States There is a one-to-one correspondence between the states of the superconductor and those of the normal metal, indexed by the quantum numbers k and spin. Thus every superconducting state with energy E(k) is in correspondence with a normal-metal state with energy k . The relation is of course given by Eq. 11.27. Thus, I have Ns (E)dE = Nn ()d where Ns is the density of states of the superconductor and Nn the same for the normal √ metal. The free-electron density of states is Nn ∼ EF + , slowly varying for small around EF . The range of in Fig. 11.7 is 10 meV: the Fermi energy is 10 eV. I can without worrying about error take Nn as constant, equal to the value at the Fermi level, N0 . so that, Ns (E) = N0 From Eq. 11.27, (k) =

d . dE

E(k)2 − 2 and then E d =√ . 2 dE E − 2

194

Fig. 11.9

Superconductors

The density of states Ns of a superconductor versus the energy E. Ns (E) is normalized by the Fermi surface density of states of the normal metal, N0 . The gap was taken as 1.2 meV. The superconductor has no states below and a square root singularity located at : ⎧ ⎨ 0 E < Ns (E) = (11.28) EN 0 ⎩√ E > . E 2 − 2 This function is plotted in Fig. 11.9. Generally, when there is a peak in the density of states for excitations, I would expect a peak in the optical conductivity at that energy. However, experiment [84, 85, 88, 221] shows that this peak is absent in a superconductor; indeed, the conductivity is zero exactly where the density of states diverges. See Fig. 11.12 for an example. It is worth asking why the conductivity does not follow the density of states. The answer is in the BCS coherence factors.

11.5.4 The Coherence Factors The ground state of the superconductor is a linear combination of Cooper pair states where ¯ the pairs |k ↑ , − k ↓ are either full [state O(k)] or empty [state O(k)], ¯ ψ0 = vk O(k) + uk O(k) where vk is the amplitude (square root of the probability) for the state |k ↑ , − k ↓ to be full and uk is the amplitude for the state |k ↑ , − k ↓ to be empty. Normalization requires that |u|2 + |v|2 = 1. BCS [210, 215] ﬁnd that 1 1− vk = 2 E

(11.29)

195

Fig. 11.10

11.6 The Optical Conductivity of a Superconductor

The amplitude vk for the state |k ↑ , − k ↓ to be full and uk for the state |k ↑ , − k ↓ to be empty as a function of (k). The gap was taken as 1.2 meV. and

1 1+ uk = 2 E

(11.30)

with (k) deﬁned in Eq. 11.26 and E(k) deﬁned in Eq. 11.27. These functions are shown in Fig. 11.10. The ﬁgures show that the superconductor (at T = 0) has a ﬁnite probability for Cooperpair states with k > kF to be occupied and a ﬁnite probability for those with k < kF to be unoccupied.∗ This result should be contrasted with the Fermi–Dirac function of Eq. 8.11 which is perfectly sharp at T = 0. In fact, vk qualitatively resembles f (E) for T ≈ Tc . For states with k = kF , the probability that the Cooper-pair state is empty and the probability that it is full are equal; I can think of this situation as implying that these Cooper pairs have 50% electron-like character and 50% hole-like character. The mixed character has important consequences for the optical properties, explaining why the conductivity at the gap is zero rather than maximum.

11.6 The Optical Conductivity of a Superconductor 11.6.1 Mattis-Bardeen Theory The optical conductivity of a superconductor was ﬁrst worked out by Mattis and Bardeen [222] and has been extended by Nam [223, 224] and others [225–227]. The Mattis-Bardeen calculation took the scattering of photoexcited quasiparticles in the superconductor and of ∗ (k) = 0 for states at the Fermi energy.

196

Superconductors

normal carriers in the metal to be the same, calculating σ 1s (ω)/σ n and σ 2s (ω)/σ n in the dirty limit (1/τ 2 ) and the extreme anomalous limit ( δ). The result (at T = 0) is expressed in terms of complete elliptic integrals. The results at ﬁnite temperature may be written ( ' − E(E + hω) 1 σ1 (ω) ¯ + 2 = θ (hω dE √ × [1 − 2f (E + hω)] ¯ − 2 ) ¯ σn hω ¯ E 2 − 2 (E + h¯ ω)2 − 2

−h¯ ω ∞ 2 E(E + hω) ¯ + 2 + dE √ [f (E) − f (E + h¯ ω)] (11.31) hω ¯ ( E 2 − 2 (E + hω)

¯ 2 − 2 and

σ2 (ω) 1 E(E + hω) ¯ + 2 = dE √ [1 − 2f (E + h¯ ω)] σn hω ¯

2 − E 2 (E + hω) max (− , −h¯ ω) ¯ 2 − 2 (11.32)

where ≡ (T ) is the temperature-dependent gap function, shown in Fig. 11.5, and f (E) is the Fermi function at temperature T , enforcing the requirement that (in the semiconductor picture) the excitation is from occupied to unoccupied state. Note that I’ve written Eq. 11.31 as two integrals and in the order opposite to the way they are usually written [222]. The ﬁrst integral only contributes for hω ¯ > 2 and represents the contribution from photoexcited quasiparticles. The second integral represents the contribution from thermally excited quasiparticles. According to Eq. 11.27, the BCS excitation spectrum has a gap, 2 2 Es (k) = (k) + . The second integral therefore starts at . The limits on the integral for σ 2 (ω) seem perverse but it does all work out. Figure 11.11 shows the Mattis-Bardeen conductivity for a “dirty-limit” superconductor. (I’ll discuss what “dirty limit” means in the next section.) The real (σ1 ) and imaginary (σ2 ) parts of the conductivity are shown in the left panel. The real part is zero up to the

Fig. 11.11

Left: real (solid line) and imaginary (dashed line) parts of the optical conductivity at T = 0 K from Mattis-Bardeen theory. Right: the imaginary part of the optical conductivity (solid line), with one part related to the delta function in σ1 (dashed line), and the other part related to the finite frequency part of σ1 (dotted line). The inset shows the same quantities plotted on 1/ω scale.

197

11.6 The Optical Conductivity of a Superconductor

superconducting energy gap 2 and then rises smoothly to reach the normal-state value at a frequency that is several times the gap. The imaginary part looks very London-like at low frequency and falls as 1/ω with increasing frequency. There is a little bit of structure near the gap but σ2 continues to fall as frequency increases. The right panel compares the BCS (Mattis-Bardeen) curve for σ2 with the London-model curve.

11.6.2 The Dirty Limit Dirty metals, alloys, and thin ﬁlms often have short mean free paths. The mean free path can be of order 1–2 nm, compared to perhaps micrometers in pure materials at low temperatures. When the mean free path is shorter than the coherence length, the coherence length itself is shortened, to [215, 228] 1 1 1 + = ξ ξ0 with limits of ξ0 in the clean limit and in the dirty limit. The short mean free path of the dirty metal means a broad spectrum for σ 1 (ω). (See Eq. 4.10a and Fig. 4.1.) It also has an effect on the penetration depth and optical conductivity. To see how, let me start with a series of inequalities: < ξ0 h¯ vF vF τ < 2 h¯ 2 < τ

(11.33)

indicating that the Drude spectrum extends beyond (often well beyond) the gap in the conductivity spectrum. Now, I invoke the conductivity sum rule, Eq. 9.29: ωmax 1 dω σ 1 (ω) = ωp2 8 0 where I’ll stop the integral at a frequency well above 1/τ but below the onset of interband transitions, so that ωp is the free-carrier plasma frequency of the metal. The sum rule tells me that the integral gives the same answer for the plasma frequency in normal and superconducting states. The normal state has the Drude free-carrier response. The superconducting state has an inﬁnite DC conductivity [a delta function Aδ(ω) at ω = 0], a gap of 2 , and a conductivity that increases from zero at the gap to approach the normal state at high frequencies. An example of the conductivity of a dirty-limit superconductor at four temperatures is shown in Fig. 11.12 [221]. (The circles and triangles are data for σ 1 and σ 2 respectively, while the solid lines are a dirty-limit BCS theory calculation [222].) The conductivity is normalized by the normal-state conductivity, which is essentially equal to the DC conductivity, σdc , at all frequencies shown. The superconducting state conductivity is zero up to the gap, 2 , after which it rises slowly to join the normal-state conductivity. The sum rule says that the “missing area” in

198

Fig. 11.12

Superconductors

Conductivity of a superconducting NbTiN film (Tc ≈ 10 K) at four temperatures. The data are normalized to the (approximately constant) normal-state conductivity (σN = 6,800 −1 cm−1 ) [221]. σ 1s appears in the delta function DC conductivity.∗ I can estimate the strength of this delta function from the sum rule by calculating ωmax 1 2 1 dω [σ 1n (ω) − σ 1s (ω)] = A = ωps 2 8 0+ where I start the integral at 0+ to miss the delta function and end it when the difference between normal and superconducting conductivities has become negligible. The sum rule tells me that the missing area in the ﬁnite frequency part of σ 1s (ω) is equal to A/2, the integral of the delta function from 0 to 0+ . (The factor of 1/2 also can be seen earlier in this chapter, in Secton 11.3.3; it arises because the integral starting at ω = 0 only picks up half 2 /4π ω. of the area of the delta function.) The weight of the delta function gives σ2 = ωps The missing area in Fig. 11.12 is proportional to σdc = ne2 τ/m, to 2 , the width of the gap, and to a factor I will call Z that represents the way the conductivity rises to reach the normal-state value. If the conductivity stepped up to 1.0 at ω = 2 , I would have Z = 1. Because the conductivity rises slowly, Z is larger than one. Thus, ne2 τ 1 2 ωps = · 2 · Z 8 m ∗ The missing area in Fig. 11.12 is the area between a horizontal straight line at σ /σ = 1.0 and actual the 1 N σ1 /σN curve.

199

11.6 The Optical Conductivity of a Superconductor

and hence,

ωps 1 = = λL c

8ne2 τ 2 Z. m

√ The penetration depth increases as τ gets shorter, following λL ∼1/ τ .

11.6.3 The Clean Limit It is easy to guess that the clean limit is the case opposite to that just discussed. The clean metal has a long mean free path, so that ξ0 . Then the coherence length is what it is, with examples in Table 11.3. The inequalities in Eq. 11.33 point in the opposite direction, and 1 (11.34) 2 . τ The full width at half-maximum of the Drude function, Eq. 4.10a is equal to 1/τ , so that all of the Drude spectral weight is below the gap and condenses to form the superconducting delta-function DC conductivity. The normal state conductivity evaluated at the gap frequency∗ ω = 2 is σD =

ne2 ne2 /m +i , 2 2m (2 ) τ

making σ 2 larger than σ 1 by a factor of 2 τ . If the normal metal is a really good conductor, then the anomalous skin effect applies in the normal metal (to be discussed in Chapter 14). Similar physics dominates the optical conductivity in the superconducting state. The conductivity is wave-vector dependent, with the q value in the range of 1/λL . The anomalous limit has been described by Mattis and Bardeen [222] and Tinkham [215]. Other materials, especially those with lower electron density such as the cuprate superconductors and organic superconductors, have normal skin depth while being in the clean limit. Then, ωps = ωp and the conductivity will be σ =

ne2 π ne2 δ(ω) + i . m mω

(11.35)

11.6.4 A Hand-Waving Calculation Here I will make a simple-minded calculation based on the ideas of the coherence factors and the mixing of electron-like and hole-like states near the gap energy. At high frequencies the mixing is minimal and the normal-state conductivity and the superconducting-state conductivity are essentially indistinguishable. This statement agrees with observation: there is no change in the color (as seen by humans) of the metal on making the transition from normal to superconducting. ∗ I will be cavalier in this chapter and use 2 either as an energy or as a frequency. I think it will be obvious from

context. (I am no theorist, but setting h¯ = 1 is often convenient.)

200

Superconductors

For frequencies near the gap, I will use a Drude-like model for the quasiparticle scattering.∗ Note that the scattering is essential to give a dominant real part to the conductivity; if ω 1/τ the conductivity is mostly imaginary. So, I write σ 1s (ω) =

nQ2k τ/m , 1 + ω2 τ 2

(11.36)

where Qk ≡ Q E(k) is the effective charge of an excitation at energy E(k), given by Eq. 11.27. This equation should be compared to the ordinary Drude conductivity of Eq. 4.10a, σ 1n (ω) =

ne2 τ/m , 1 + ω2 τ 2

so that Q2 σ 1s (ω) = 2k . σ 1n (ω) e What does Q(E) look like? Well, remember the coherence factors, Eqs. 11.29 and 11.30 (Fig. 11.10), where vk is the amplitude for a state to be full (electron-like) and uk is the amplitude for a state to be empty (hole-like). Their squares are the probabilities, of course. Holes and electrons have opposite charges, so the effective charge is the difference between the probabilities. I’ll write it as Qk = −e(vk2 − u2k ). Using Eqs. 11.29 and 11.30, I get vk2 − u2k = −

E

so that so long as the energies of both excitations† exceed the gap, 2 E 2 − 2 Q2k = e2 2 = e2 . E E2 Now, the energy of the excitations is delivered by the photon energy h¯ ω. I’ll take the energy of each excitation as half of this energy.‡ The conductivity is then ⎧ Aδ(ω) ω=0 ⎪ ⎪ ⎨ 0 0 < ω ≤ 2 ω , σ 1s (ω) = (11.37) ⎪ 2 2 ⎪ ⎩σ (ω) ω − (2 ω ) ω ≥ 2 ω 1n ω2 where 2 ω is the energy gap (for pairbreaking) in frequency units. This conductivity is shown in Fig. 11.13. ∗ As did Mattis and Bardeen. † Remember that the excitations are created in pairs. ‡ This division of energy is where I am waving hands the most; in principle, I should integrate over a range of

excitation energies, allowing one excitation to have an energy ranging from to hω ¯ − while the other ranges from h¯ ω − to , keeping the total energy absorbed equal to hω. ¯

201

Fig. 11.13

11.7 Thin Film Superconductors

The optical conductivity according to Eq. 11.37. The gap was taken to be 2 = 3 meV (2 ω = 24 cm−1 ). The conductivity is zero right at the gap (despite the divergence of the density of states there). The reason is that the effective charge of the gap-edge excitation is zero. The conductivity then rises smoothly until it becomes equal to the normal-state conductivity at ω 2 ω . By the sum rule, A, the weight of the delta function, is twice the missing area in the superconducting-state conductivity. I can do the integral to ﬁnd the missing area. In the dirty limit, where 2 τ 1, A = 4σ1n (0)(2 ). I look back at section 11.6.2 and see that Z = 2.

11.7 Thin Film Superconductors Many infrared studies of superconductors have used thin ﬁlms [84, 85, 88, 221]. The transmittance spectrum of a thin-ﬁlm superconductor is quite distinctive. The ﬁlms are thin enough that the Glover-Tinkham formulas are appropriate. (See Chapter 7, Section 7.4.1.) The transmittance through the ﬁlm is given by Eq. 7.30: T

f

=

4n , (n + 1 + Z0 σ1 d)2 + (Z0 σ2 d)2

where n is the refractive index of the substrate, Z0 = 377 is the impedance of free space, and d the ﬁlm thickness. I look at Figs. 11.11 and 11.13 and expect small transmittance at low frequencies because σ2 is so large. (σ1 is zero below the gap.) The transmittance increases with increasing frequency because σ2 falls. This behavior continues until ω = 2 ; here, σ1 becomes ﬁnite and rises towards the normal state value and so the transmittance decreases. Eventually the frequency is high enough that the conductivity and

202

Fig. 11.14

Superconductors

The transmission through and reflectance from a thin superconducting and normal film on a transparent substrate. The gap has been taken to be 2 = 3 meV (24 cm−1 ). The normal-state sheet resistance used in the calculation is R = 1/σdc d = 377 . The substrate refractive index is n = 2.1. transmittance are indistinguishable from the normal-state values. Calculated transmittance and reﬂectance curves are shown in Fig. 11.14 for both the superconducting and normal states. The normal-state curves are ﬂat, because the calculations were done in the dirty limit, ωτ 1. The superconducting state transmittance is larger than the normal state transmittance in the vicinity of the gap and T s has a maximum at ω = 2 . The reﬂectance is 100% at the lowest frequencies and falls as frequency increases towards the gap. Rs + T s = 1 below the gap, whereas above the gap and in the normal state R + T = 1 − A < 1. Measurements of superconducting thin ﬁlms often yield the ratio of superconducting to normal state transmissions rather than the absolute transmission. There are two motivations for this approach: (1) One can leave the sample in place and change temperature or magnetic ﬁeld, reducing the effects of alignment, standing waves in the apparatus, and other effects which can bother sample-in/sample-out measurements. (2) The effects of the substrate (mostly) divide out. According to Eq. 7.30: (n + 1 + Z0 σN d)2 Ts = . Tn (n + 1 + Z0 σ1 d)2 + (Z0 σ2 d)2 An example is shown in Fig. 11.15. This plot show the transmission ratio, T s /T n , for a NbTiN thin ﬁlm at T = 2 K along with a ﬁt to Mattis-Bardeen theory [229]. The ﬁlm had a transition temperature of Tc = 10 K. The maximum transmittance occurs at the gap frequency, which for this sample is 2 = 25 cm−1 . The normal-state sheet resistance of the ﬁlm is R = 1/σdc d = 130 . The ﬁlm is deposited on a crystal quartz substrate with refractive index n = 2.12. These parameters were used in the calculation.

203

Fig. 11.15

11.8 Unconventional Superconductors

The ratio of superconducting-state to normal state transmittance of a NbTiN thin film. From Ref. 229.

11.8 Unconventional Superconductors At the center of superconducting research these days are the so-called “unconventional” superconductors [230–232]. The interest in these materials exploded at the discovery [190, 233] thirty years ago of superconductivity with Tc > 90 K in layered copper-oxide (cuprate) materials. See Fig. 11.2 and Table 11.1. Many experimenters and theorists caught the “high-Tc fever” and work continues almost unabated today. Examples of such materials include the heavy Fermions (UPt3 ), organics [(TMTSF)2 PF6 ], ruthenates (Sr2 RuO4 ), charge-density-wave materials (2H -NbSe2 ), cuprates (YBa2 Cu3 O7−δ ), and ferropnictides (LaOFeAs). These materials differ in fundamental ways from the metallic (conventional) materials that I have addressed up to this point in this chapter. Among the unconventional properties are anisotropic crystal and electronic structure, strong correlations among the charge carriers, the presence of magnetism, charge ordering, and observations of an unusual linear resistivity in some cases. Among the conventional properties still remaining are inﬁnite DC conductivity, the Meissner effect,∗ ﬂux quantization with the conventional ﬂux quantum, Josephson tunneling, and Cooper pairs. Many unconventional superconductors have anisotropic superconducting gaps. When I showed the excitation spectrum of a conventional superconductor in Fig. 11.7, I did not need to specify the direction of k because the value of is the same everywhere on the Fermi surface. In contrast, the value of the excitation energy in unconventional superconductors often varies with k; there are values where = 0 (nodal values) and others where it is a maximum (anti-nodal). The gap in the cuprates is believed to be of d-wave form, with four nodes equally spaced around the two-dimensional Fermi surface. ∗ Most unconventional superconductors are type-II materials.

204

Superconductors

The optical properties of unconventional superconductors have been widely studied. I’ll give one example, the optical conductivity of Bi2 Sr2 CaCu2 O8 . There are a number of review articles that cover the optical properties of cuprates [234–237] and of other unconventional superconductors [238–243] for those who want more details. The key structural element in Bi2 Sr2 CaCu2 O8 and in the other cuprate superconductors are the two-dimensional CuO2 (ab) planes. The layered structure (orthorhombic or occasionally tetragonal) leads to highly anisotropic properties, including electrical and optical conductivity. The mobile carriers (and the Cooper pairs) reside on the ab plane. Although the superconductivity is three dimensional, the superconducting properties (London penetration depth, coherence length, and critical current) are quite anisotropic. Anisotropy is large in the normal state conductivity too. The ab plane is metallic whereas the c axis appears almost insulating. With this brief introduction complete, I’ll discuss the optical conductivity of Bi2 Sr2 CaCu2 O8 , a cuprate superconductor with Tc = 85 K. The ﬁrst single-crystal reﬂectance spectra of Bi2 Sr2 CaCu2 O8 were reported by Reedyk et al.[244] Similar spectra were found by other workers [138, 177, 245–247]. The optical properties display marked anisotropy. The spectra for the c polarization (perpendicular to the CuO2 planes) are typically those of an insulator. The ab-plane spectra appear metallic at ﬁrst look: the reﬂectance is high in the far infrared and drops steadily throughout the infrared to a minimum around 10,000 cm−1 (1.3 eV). Very little temperature dependence is observed above 3,000 cm−1 . The reﬂectance is low in the visible; all the cuprates are black crystals. Kramers–Kronig analysis of reﬂectance gives the optical conductivity (and other optical “constants”) of Bi2 Sr2 CaCu2 O8 . The temperature evolution of the Ea optical conductivity is shown in Fig. 11.16, after Ref. 138. There are several features to these

Fig. 11.16

Bi2 Sr2 CaCu2 O8 optical conductivity for Ea at temperatures between 20 and 300 K. The dashed line shows a Drude-model fit to the low-frequency, 100 K data. From Ref. 138.

205

11.8 Unconventional Superconductors

spectra, features that occur in all the cuprate superconductors. First, in the normal state (100–300 K), the low-frequency optical conductivity extrapolates reasonably well to the DC conductivity. Second, with decreasing temperature, the low frequency conductivity increases in agreement with the T -linear resistivity. There is a characteristic narrowing of this far-infrared portion of the spectrum. This narrowing can be seen most easily by noting that the 300 K data is larger than the lower temperature data above about 500 cm−1 but then crosses through each of the lower temperature curves at progressively lower frequencies, becoming the smallest conductivity near 100 cm−1 . Third, at high frequencies, σ 1 (ω) does not show much temperature variation; all the curves draw together around 3,000 cm−1 . Fourth, below Tc , the low-frequency conductivity is considerably reduced, so that the 20 K conductivity is smallest at all frequencies measured. The “missing area” in the far-infrared conductivity appears as the zero-frequency delta-function response of the superﬂuid. Two approaches have been used to discuss the optical properties of the cuprate superconductors, called the “one-component” and the “two-component” pictures. In the ﬁrst, there is only a single band or type of carrier, and the unusual frequency dependence in the midinfrared is attributed to interaction with a spectrum of (optically inactive) excitations. This interaction causes a frequency dependence to the carrier scattering rate and enhances the low-frequency effective mass. This approach, appropriate for stronglyinteracting materials, is discussed in Chapter 13. In the two-component approach, two different contributions are assumed: the DC conductivity comes from a set of free carriers, described by a Drude model; the midinfrared conductivity, nearly temperature independent, is due to one or more bands of “midinfrared” carriers. The properties of the free carriers determine the DC conductivity, including its temperature dependence, while the midinfrared carriers dominate the higher frequency conductivity. The superconductivity results from condensation of the free carriers below Tc . The dashed line in Fig. 11.16 shows the Drude conductivity at 100 K, given by f it

σ 1D =

1 ωpD 2 τ , 4π 1 + ω2 τ 2

(11.38)

with ωpD = 9,040 cm−1 (1.12 eV) and 1/τ = 128 cm−1 (16 meV). The Drude contributions at other temperature have essentially the same plasma frequency and scattering rates that are linear in temperature. The two approaches are still discussed, though the majority opinion favors the onecomponent approach. Fortunately, the issue does not need to be settled in order to address the phenomenology of the superconducting-state. If the 100 K 1/τ is used together with estimates [248] for the Fermi velocity vf to compute the ab-plane mean free path , I ˚ ∗ This number is considerably larger than the typical ab-plane get = vf τ ∼ 100 A. ˚ This comparison suggests that the cuprates are in the coherence length [249], ξ ∼ 15 A. clean limit [250], i.e., > ξ . In this limit, absorption associated with the superconducting gap is not observable because in the superconducting state most of the spectral weight moves to the zero frequency delta function. Thus the only signature of the condensate is ∗ The DC mean free path is essentially the same in the one- and two-component pictures.

206

Superconductors

its inductive response, seen in the imaginary part of the conductivity, σ 2 (ω). The delta function conductivity gives, via the Kramers–Kronig relations, σ2 =

ωps 2 , 4π ω

(11.39)

where ωps is the plasma frequency of the superconducting condensate, ωps = 4π ns e2 /m, with ns the density of superﬂuid carriers. From the low-frequency behavior at T = 20 K, (or, equivalently, from the missing area under σ 1 (ω) in the superconducting state) ωps = 9,000 cm−1 (1.11 eV), about the same as the plasma frequency of the free carriers in the two-component analysis. The same analysis gives the a-axis London penetration length ˚ in agreement with measurements by other means. The London model, λaL ∼ 1,800 A, Eq. 11.15, is a good model for the low-frequency conductivity of superconducting cuprates, with nearly all of the Drude-like conductivity spectrum condensing.

12

Semiconductors and Insulators

I will address in this chapter interband transitions in semiconductors and insulators [54, 73, 98, 251, 252]. All solids show these interband optical transitions. In many ways they are analogs of the electric-dipole transitions between principal quantum numbers in atoms, such as 1s → 2p in hydrogen. Although I made some progress towards the goal in Chapter 9, I mostly have treated these interband transitions in one of two ways. (1) Accumulate the low-energy contributions of these transitions into c . (2) Include an electronic Lorentz oscillator as representing the transition between two levels separated by hω ¯ e . Neither approach is very satisfactory.∗

12.1 Band Structure Before considering the optical excitations, the so-called interband transitions, I ﬁrst should say something about what these “bands” really are. Free electrons do not have bands. The energy is solely the kinetic energy h¯ 2 k 2 /2m; I take the electrons and pour them into these free-electron states until I have run out of electrons. In reality of course, no electron is actually free. All interact with the atomic nuclei and with other electrons. The innermost ones are deeply bound in atomic-like very low-energy states. The most energetic electrons may be nearly free, with the details determined by the chemical and crystallographic structure of the solid. Even states above the Fermi energy (which are unoccupied – or empty – at low temperatures) will be affected by the band structure. The electron energies turn out to be organized into a range of quasi-continuous energies, called “bands,” separated by forbidden energy gaps where no states exist [19, 24, 98–100].

12.1.1 Some Qualitative Arguments Let me start by considering an isolated atom. I know that the energies of electrons bound to this atom are quantized into discrete levels and that electromagnetic absorption (photons) will promote electrons from one level to another. Consider the ground state wave function of a simple atom, such as hydrogen. Two H atoms and their 1s orbitals are shown in the upper panel of Fig. 12.1. The wave function falls off quickly away from the central nucleus. When the two hydrogens are allowed to interact, the two wave functions can add ∗ Although if all I am interested in is the dielectric function at low frequencies – well below the energy of

interband effects – they may prove adequate.

207

208

Semiconductors and Insulators

Fig. 12.1

Upper panel: Hydrogen ground-state wave function for two atoms: A and B. Lower panel: the two wave functions can either be added or subtracted. Addition (purple) leads to the bonding orbital; subtraction (green) to the antibonding orbital.

Fig. 12.2

Splitting of the bonding and antibonding levels in H2 . either constructively or destructively. Constructive addition leads to the bonding orbital; destructive to the antibonding orbital.∗ It is evident that the bonding orbital has much more electronic amplitude in the space between the two protons. This counteracts the repulsion felt by the two protons and lowers the energy of the H2 molecule. The antibonding orbital has small amplitude in the space between, which leads to a signiﬁcant increase in the energy. These effects are sketched in the bottom panels of Fig. 12.1. The energy levels are shown in Fig. 12.2. The bonding level holds the two electrons and the antibonding level – which could hold two more – is empty. Now consider a long chain of such atoms, containing N atoms, all separated by lattice constant a. There will be many ways to form linear combinations of the wave functions and so there will be many levels, ranging from one where all are added, so all in phase, to one where each is 180◦ out of phase with its two neighbors. Indeed there will be N such levels. If there is one electron/atom, half will be full and half empty. I claim that this linear chain would be a metal.† ∗ In this discussion I am leaving out the beautiful physics that comes from the spin states of the electrons and

the symmetry that the two-electron wave function must have under exchange. The bonding orbital is a singlet, S = 0, and the antibonding orbital a triplet, S = 1. † One-dimensional metallic chains are susceptible to a Peierls [253] or charge-density-wave transition, where the bond lengths become alternating, short, a − u, and long, a + u. This doubles the unit cell to 2a, and gives two electrons per dimer, e.g., a chain of H2 molecules. This dimerized state is an insulator.

209

12.2 Nearly Free Electrons

If there were two electrons per atom, the uniform chain would have every level ﬁlled with two electrons, one spin up and one spin down. It seems natural to claim that this chain would be an insulator. I have gone about as far as I can without doing some calculations. I could follow the ideas above and do a tight-binding model. But instead, let me return to my free electron model and add, as a perturbation, a periodic potential.

12.2 Nearly Free Electrons The nuclei in the solid form a periodic lattice, so that the potential satisﬁes V (r) = V (r + T)

(12.1)

where T is the translation vector of the crystal. In the one-dimensional case I will consider, T = j a xˆ where the lattice constant is a and j is an integer.∗ Now if V = 0, E = h¯ 2 k 2 /2m (free electrons) with k = 2πj/L (periodic boundary conditions). What is the effect √ of the periodic potential? Well, the free electron states are plane waves, ψ = eikx / L, and plane waves traveling in a periodic medium are diffracted. In one dimension, the incident wave and the diffracted wave must both travel ˆ Diffraction effects thus produce waves traveling in both directions along the chain along x. of atoms.† In general these waves just continue along forever. (There is no absorption.) But for certain values of k, I can get strong interference effects.‡ Consider a partial wave which travels forward for distance a, is reﬂected and travels backward for distance a, and is reﬂected again. If the total distance traveled is an integer times the wavelength, there will be constructive interference. So the condition for diffraction is 2a = λ. But of course k = 2π/λ so the condition is also π k=m a where m, the diffraction order, is a positive or negative integer. Look at the case where m = ±1. (Other orders have higher energies.) Because of diffraction and constructive interference, the wave functions become standing waves: πx 2 eiπ x/a + e−iπ x/a cos = ψ1 = √ L a 2L and eiπ x/a − e−iπ x/a =i ψ2 = √ 2L

πx 2 sin L a

∗ I’ll use j to index the sites just as I did in Chapter 8 (Section 8.2). The one-dimensional chain has length L = J a. If I want to extend to a three-dimensional crystal, then the number of atoms is N = J 3 . † I can also consider this as specular reﬂection by each atom. Note that if there are very many atoms, the effect

of very many scattering events, even very weak ones, is to have equal amplitudes ﬂowing in both directions.

‡ Interference is of course the basis of diffraction.

210

Semiconductors and Insulators

where I have done a side calculation for the normalization. The standing waves lead to a nonuniform density, πx 2 |ψ1 |2 = cos2 L a and πx 2 . |ψ2 |2 = sin2 L a One probability density has crests at x = 0, ± a, ± 2a, . . . and the other has crests half a lattice constant away. Because the potential V (x) is periodic, it can be written as a Fourier series; because the period is a, the longest wavelength component is a, making the lowest Fourier component 2π/a. Let me consider that component∗ alone, x V (x) = −V0 cos 2π a with a minimum at the lattice sites 0, ±a, etc. and a maximum between the atoms. I treat this as a perturbation, (1)

= ψ1 |V |ψ1 L x x 2 cos2 π dx cos 2π = − V0 L a a 0 2 but cos (φ) = [1 + cos(2φ)]/2 and so L x x 1 + cos2 2π = − V0 dx[cos 2π L a a 0 The ﬁrst term in the integral is zero and the second is L/2, so that V0 (1) E1 = − 2 and, for ψ2 ∼ sin(kx) L x x 2 (1) sin2 π E2 = − V0 dx cos 2π L a a 0 V0 = 2. For the states with k = ±π/a, there is an energy difference between the two wave functions. One (the one that goes as sin(kx)) is raised and the other (that goes as cos(kx)) is lowered. That it goes like this is what one might have expected: the cos(kx) function has the electron most likely to be at the nucleii of the atoms, where the potential is a minimum while the sin(kx) function has the electron between the nucleii, where the potential is maximum. The jump in energy of magnitude V0 at k = ±π/a means that there is a range of energies for which there are no solutions to the Schr¨odinger equation [19, 24, 254]. Note E1

∗ There is a DC component of course, but I can suppress that by choosing the zero of energy equal to the DC

component.

211

Fig. 12.3

12.2 Nearly Free Electrons

Energy as a function of the wave vector for a solid with a periodic lattice potential. There are three bands shown completely, plus part of a fourth. There are gaps between the bands where no allowed energies exist. The free-electron parabola, E = h¯ 2 k 2 /2m, is shown as a dashed line. π/a = 2N that the number of k states is unchanged, for spin-1/2 electrons there are 2 22π/L ∗ states between k = −π/a and k = +π/a. Moreover, there are no disallowed values of k – only disallowed values of E(k). These disallowed energies are call forbidden energy gaps. Additional gaps appear at k = ±2π/a, ± 3π/a, . . . . The interference/diffraction effect affects ψ(k = ±π/a), which has λ = 2a, the most but states with nearby wave vectors are also affected. A calculated dispersion relation is shown in Fig. 12.3. Three bands and part of a fourth are shown; there are gaps between the bands. The underlying parabolic free-electron curve is also shown; it is close to these curves in the middle of the bands, but passes below or above them near the band edges. I can now understand the reason why some materials are metals and some insulators. Suppose the linear chain is made up of hydrogen, which has 1 electron per atom. Or suppose it is potassium or silver, with effectively one valence electron per atom. Then there are N electrons and 2N valid k values, so the Fermi wave vector is kF = ±π/2a; half the states in the lowest-energy band are occupied at T = 0 and half unoccupied. If there are two electrons per atom (helium), this one-dimensional solid would have the ﬁrst band full and a gap in energy between the highest occupied state (the most energetic state in the ﬁrst band) and the lowest unoccupied state (the least energetic state in the second band). Then kF = ±π/a and the electrons cannot be accelerated (with a corresponding increase in momentum) without acquiring additional energy. The solid would be an insulator.† ∗ Plus one. The range is more properly stated as −π/a < k ≤ π/a. † On ﬁrst hearing this, it is natural to ask why the divalent alkaline earth elements (beryllium, magnesium,

ˆ y, ˆ and zˆ directions. calcium, . . . ) are in fact metals. The reason is that the electrons have dispersion in the x, Suppose I say that the symmetry of the periodic lattice is such that the diffraction occurs when {kx , ky , kz } = ±π/a, so that the surface in k-space where the gaps occur is a cube. For electrons with kxˆ there is a gap at {kx = π/a,ky = 0, kz = 0} at a free-electron energy of h¯ 2 π 2 /2ma 2 . But if I think about electrons whose wave vector is such that kx = ky = kz , I reach the cube corner where the free electron energy is 3h¯ 2 π 2 /2ma 2 , three times higher. In many materials, this energy exceeds h¯ 2 π 2 /2ma 2 + V0 , so that the Fermi surface, a

212

Semiconductors and Insulators

If there are 3 valence electrons per atom (aluminum), the one-dimensional Fermi wave vector is kF = ±3π/2a. The ﬁrst band is full but the second is half-full. Metal. If 4 (silicon, germanium), then kF = ±2π/a and the ﬁrst and second bands are both full. The material would be an insulator.∗

12.3 Bloch’s Theorem Bloch’s theorem is the basis for much of the picture solid-state physics has for electrons, phonons, and other quantum-mechanical objects in a crystal with translational invariance.† It states that the wave functions are of the form of a product of plane waves and a periodic function that respects the symmetry of the lattice. A statement of the theorem is ψk (r) = eik·r uk (r),

(12.2)

where uk (r) is periodic in T, as in Eq. 12.1. So uk (r) describes the variation of the wave function within the unit cell and the plane-wave exponential function gives the phase between unit cells. If uk = constant, then Eq. 12.2 is the wave function for free electrons. Equation 12.2 is stated for three-dimensional crystals, but for simplicity I’ll discuss it only in one dimension. The Schr¨odinger equation is −

h¯ 2 ∂ 2 ψ(x) + V (x)ψ(x) = Eψ(x), 2m ∂x 2

(12.3)

where the potential energy function is periodic: V (x + j a) = V (x) for j any integer and a the lattice constant. I use periodic boundary conditions, so that ψ(x + L) = ψ(x) with L = J a. Translational symmetry implies that the probability density satisﬁes |ψ(x + j a)|2 = |ψ(x)|2 .

(12.4)

Now let me translate from one unit cell to the next (j = 1). The points x and x + a are equivalent, making the wave functions differ at most by a factor A, the eigenvalue of the translation operator: ψ(x + a) = Aψ(x),

(12.5)

where Eq. 12.4 requires that A∗ A = 1, so A has unit length and some phase. If I translate to the next neighbor along the chain, ψ(x + 2a) = Aψ(x + a) = A2 ψ(x). surface of constant energy, lies in the second band for kxˆ and in the ﬁrst band for k along the diagonal. The material would then be a metal. ∗ As indeed are Si and Ge. They are called semiconductors for historical reasons. The band gap is not so large in these materials as in, for example, Al2 O3 or diamond. So at room temperature the Fermi–Dirac distribution function is not zero in the third band, so there are thermally excited electrons that can conduct in a semi-efﬁcient way. There are also vacancies in the second band, so that there are also holes to contribute to the conductivity. † Here, translational invariance means that the structure repeats periodically and for ever and ever as I move through space.

213

12.4 The Brillouin Zone

Here comes the big step: translate by J lattice constants. Then ψ(x + J a) = AJ ψ(x) = ψ(x)

(12.6)

where the second equality comes from the periodic boundary conditions; the wave function must be single valued when I translate by L = J a. This requirement means that AJ = 1 or A = e2π ij/J so that the J th power of A is unity. I then rewrite Eq. 12.5 as ψ(x + a) = e

2π ij J

(12.7)

ψ(x).

Let me try the following wave function ψ(x) = eikx uk (x).

(12.8)

I make no assumptions about the values of k or the nature of the function u(x). A translation by one lattice constant gives ψ(x + a) = eik (x+a ) u(x + a) = e

2π ij J

eikx u(x)

where the ﬁrst equality comes from Eq. 12.8 and the second from Eq. 12.7. I cancel eikx in the middle part and right side. Then, using quantization of k by the periodic boundary conditions, I ﬁnd that k=

2πj 2πj = , L Ja

with j = 0, ±1, ±2, . . .. This value of k allows me to cancel the other complex exponential, leaving only u(x + a) = u(x), completing the proof of Bloch’s theorem.

12.4 The Brillouin Zone Bloch’s theorem, the periodic lattice, and the boundary conditions all conspire to limit what values k can take. I began with it as a real number (a quantity along a continuous line) taking any value from negative to positive inﬁnity. Then, periodic boundary conditions restricted it to a countable inﬁnity, represented by integers. Now I will show that only a ﬁnite range of these integer-based k values has distinct physical signiﬁcance. I start by once again translating by a single lattice constant ψ(x + a) = uk (x + a)eik (x+a ) = uk (x)eikx eika = eika ψ(x).

(12.9)

Now, deﬁne a wave vector k by k = k +

2π m , a

214

Semiconductors and Insulators

with m an integer. Substitute into Eq. 12.9 to ﬁnd

eika ψ(x) = eik a e2π im ψ(x). But e2π im = 1 so

eika ψ(x) = eik a ψ(x). The state with wave vector k and wave vector k + 2π m/a, with m an integer, are the same. The wave function is the same as is the energy eigenvalue. k is periodic with period 2π/a. Values of k in the range −

π π 0

I’ll need to include in my perturbation interactions of the electrons with both photons (as V eγ ) and phonons (as V ep ). The perturbation Hamiltonian then looks like 1 1 (12.26) H1 = V eγ e−iωt + eiωt + V ep e−ik t + eik t , 2 2 where I have pulled out the time dependent parts of the perturbation to show that one term depends on the photon frequency and one on the phonon frequency. I have hidden everything else (the dipole moment, the Coulomb interaction between electron and ion cores, interatomic springs, etc.) in V eγ and V ep . The frequencies in Eq. 12.26 are ω the frequency of the photon and k , the frequency of a phonon with wave vector k. (1) So now I have to calculate the ﬁrst-order coefﬁcients am that go into Eq. 12.26. The eγ ep matrix elements that I need are Vm0 = m|V eγ |0 and Vm0 = m|V ep |0. Then Eq. 12.24 for the ﬁrst order time derivative becomes (1) eγ ep i h¯ a˙ m = Vm0 ei (ωm0 −ω)t + ei (ωm0 +ω)t + Vm0 ei (ωm0 −k )t + ei (ωm0 +k )t . (12.27) The four terms represent photon absorption (ωm0 −ω), photon emission (ωm0 +ω), phonon absorption (ωm0 − k ), and phonon emission (ωm0 + k ). Photon emission is needed to study photoluminescence, electroluminescence, LEDs, lasers, and other process where the semiconductor emits light. But for absorption, I can omit it. In contrast, I need to allow for phonon emission and phonon absorption to understand the temperature dependence of the absorption. So the time derivative integrates† to become eγ ep Vm0 1 − ei (ωm0 −ω)t Vm0 1 − ei (ωm0 −k )t 1 − ei (ωm0 +k )t (1) am = + . + ωm0 − ω ωm0 − k ωm0 + k h¯ h¯ (12.28) ∗ If the m = 0 term did give a ﬁnite transition rate, I could and would have stopped there. " † Change t to t in Eq. 12.27 and calculate t dt a˙ (1) (t ). m 0

228

Fig. 12.10

Semiconductors and Insulators

Transitions from valence band maximum (marked with 0) to conduction band minimum (marked with f ) via two intermediate states v (in the valence band) and c (in the conduction band). In one case the photon goes first, a direct transition from valence band to conduction band, and then the phonon takes the excited electron to the conduction band minimum. In the second case, the phonon goes first and the photon second. (1)

Now I could substitute Eq. 12.28 for am into Eq. 12.25 right now. Equation 12.25 has a sum over m, an inﬁnite number of ways to go from initial to ﬁnal state. It behooves me to think about how many of these actually will contribute. A little thought (and Fig. 12.10) tells me that there are exactly two ways in second order to go from valence-band maximum to conduction-band minimum. Any other path is at least third order. I can make a vertical transition to the conduction-band state at k = 0 and then use a phonon to get to the ﬁnal state, or I can have a phonon take me to a valence-band state under the conduction-band minimum and then make a vertical transition.∗ With this restriction, Eq. 12.25 has only two terms, with m = v, c and n = f . I have to understand that the matrix elements there are those of the perturbation and the frequencies eγ ω are the frequencies of the time dependent perturbation. Thus: H1f v = Vf v with ω; ep H1f c = Vf c with ω = k . Then, continuing to omit the photon emission term, I have (2) (1) eγ (1) ep (12.29) i h¯ a˙ f = av Vf v ei (ωf v −ω)t + ac Vf c ei (ωf c −k )t + ei (ωf c +k )t . I am ready to substitute Eq. 12.28 into Eq. 12.29, but I should do this with some forethought [54]. Both Eq. 12.29 and Eq. 12.28 contain basically two terms, one with ∗ If I get asked about the Pauli principal and the phonon momentum-changing transition using an already occupied

state, I will run the process backwards: take a hole from the conduction band minimum – where there are lots of holes – to the valence band right “above” it in hole speak, and then use a phonon to move the hole to valence-band maximum.

229

12.9 Indirect Band Gap Absorption

the electron–photon matrix element and one with the electron–phonon matrix element. When everything is multiplied out, there will be two terms containing both matrix elements (which I want) and two containing one or the other squared (which I do not want). These will not contribute to the optical absorption, because in one case (two phonons) I do not have enough energy and in the other (two photons) not enough momentum. So I’ll keep only the terms that do contribute, and ﬁnd (2) i h¯ a˙ f

1 − ei (ωv0 −k )t 1 − ei (ωv0 +k )t eγ + Vf v ei (ωf v −ω)t ωv 0 − k ωv 0 + k eγ Vc0 1 − ei (ωc0 −ω)t ep + Vf c ei (ωf c −k )t + ei (ωf c +k )t . ωc0 − ω h¯ ep

V = v0 h¯

(12.30)

I’ll collect terms and simplify as much as I can. One (certainly incorrect) simpliﬁcation is to assume that the two electron–photon and the two electron–phonon matrix elements are the same. For them to be the same, the electric dipole moment c|x|v for valence to conduction band optical transitions is independent of k. An assumption of constant matrix elements is often made to take them outside of integrals and I will do it here. I’ll also assume that the electron–phonon interaction is the same for valence-band and conduction-band carriers despite their different effective masses. Also, I’ll make use of knowing the form of the frequencies ωnm = (En − Em )/h¯ so I can write ωv 0 + ωf v = (Ev − E0 + Ef − Ev )/h¯ = (Ef −E0 )/h¯ = ωg , where ωg = Eg /h¯ is the energy gap frequency of the semiconductor. As well, ωc0 + ωf c = (Ec − E0 + Ef − Ec )/h¯ = (Ef − E0 )/h¯ = ωg . With these simpliﬁcations, Eq. 12.30 becomes (2) i h¯ a˙ f

ei (ωf v −ω)t − ei (ωg +k −ω)t ei (ωf v −ω)t − ei (ωg −k −ω)t + ωv 0 − k ωv 0 + k ei (ωf c −k )t + ei (ωf c +k )t − ei (ωg −k −ω)t − ei (ωg +k −ω)t + . (12.31) ωc0 − ω

V ep V eγ = h¯

Now look at some of the terms in Eq. 12.31. There are three of them that do not contain ωg : ei (ωf v −ω)t and ei (ωf c ±k )t . These do not contribute to the optical conductivity. In the ﬁrst, ωf v > ωg ≈ ω and, hence, the term oscillates rapidly; it will produce on integration something like sin2 [ 12 (ωf v − ω)t]/(ωf v − ω)2 . As time goes on this function becomes a very narrow function of frequency centered at ω = ωf v . But I am calculating the onset of absorption at ω = ωg < ωf v . I can neglect this term. A similar argument applies to ei (ωf c ±k )t , where k ωf c . So I will just take these away before I do the integration. Finally, energy conservation gives ω = ωg ± k = ωf v + ωv 0 ± k , where I use the plus sign for phonon emission and the minus sign for phonon absorption. I can write two of the denominators in Eq. 12.31 as ωv 0 ± k = ω − ωf v . Then after some algebra (2) i h¯ a˙ f

V ep V eγ =− h¯

1 1 ei (ωg −k −ω)t + ei (ωg +k −ω)t . (12.32) + ω − ωf v ωc0 − ω

230

Semiconductors and Insulators

I’m ﬁnally ready to integrate Eq. 12.32 to ﬁnd i (ωg −k −ω)t

e ei (ωg +k −ω)t − 1 −1 V ep V eγ 1 1 (2) × + af = + . ω − ωf v ωc0 − ω ωg − k − ω ωg + k − ω h¯ (12.33) This equation contains two terms of the form sin 2 iβt/2 eiβt/2 − e−iβt/2 iβt/2 eiβt − 1 = e e = 2i . β β β βt

(2)

When I calculate |af |2 , the probability for an electron to appear in the ﬁnal state, the i and the complex exponential go away. I am left with 4 sin2 βt 2 = 2π tδ(β), β2 where I’ve used sinc2 (x) = sin2 (x)/x 2 as a representation of the delta function. The delta function enforces energy conservation in the optical process. In addition, some cross terms will drop out when the amplitude is squared, as they do not grow linearly in time. (2) So I ﬁnally write the transition rate, Wvc = d|af |2 /dt as Wvc =

2π |V ep |2 |V eγ |2

1 1 + × (ωf v − ω)2 (ωc0 − ω)2

h¯ 4 × [δ(ωg − k − ω) + δ(ωg + k − ω)] .

(12.34)

This equation describes the rate at which light, with the help of the phonons, can promote electrons from the valence band maximum to the conduction band minimum. The strength of the absorption depends on the interaction of the electrons with the phonons (via V ep ) and on the interaction of the electrons with the light (via V eγ ). When I compare the ﬁrst half of Eq. 12.27 with Eq. 9.12, I see that V eγ = (e/2) c|x|v E0 , where |v and |c are the relevant valence- and conduction-band wave functions and E0 is the electric ﬁeld amplitude. The matrix element comes in squared, so the transition rate is proportional to the intensity, just as in Eq. 9.16. This proportionality is the behavior I expect: the higher the intensity, the more photons per second arrive at the sample and so the higher the rate of absorption. As in Eq. 9.19 I can convert to optical conductivity using the absorption coefﬁcient as an intermediate step. The result is σ1 =

2hωW ¯ vc . |E0 |2

(12.35)

There are still a number of things left to do, however. I need to discuss the other matrix element in Eq. 12.34, V ep , the coupling of the electrons to the phonons. The two delta functions enforce energy conservation among the electrons, the phonons (emitted or absorbed), and the light. The condition is

231

12.9 Indirect Band Gap Absorption

ω=

! ωg − k ωg + k

phonon absorption phonon emission.

(12.36)

I also have momentum (or wave vector) conservation. (See Fig. 12.10.) kf − k0 = k

(12.37)

where k0 and kf are the initial and ﬁnal electron wave vector and k is the phonon wave vector. The band structure of the semiconductor determines the left side of Eq. 12.37 and then the phonon dispersion determines the phonon frequency. The absorption process occurs a bit below the semiconducting gap, because it uses both the photon energy and the phonon energy to promote the electron. The emission process occurs a bit above the semiconducting gap, because the photon energy must be used both to create the phonon and to promote the electron. Two simple possibilities for the phonon dispersion k are∗ ! cs k Debye, k = 0 Einstein where cs is the speed of sound. (See Fig. 5.4 for the results of a slightly more realistic model.) All phonon branches have k-values from 0 to the zone boundary, so wave vector conservation is always possible. When k is large, the frequency is also relatively large, at least on the scale of the phonon frequencies. It is almost always small on the scale of ωg . Phonons obey Bose–Einstein statistics; in thermal equilibrium the number of phonons in a given state with a given frequency is given by the Bose–Einstein distribution [19, 24]. The probability of phonon absorption is proportional to PA = n(k ,T ) =

e

1 h¯ k kB T

(12.38)

, −1

where the phonon modes are indexed by wave vector k. (A polarization and branch index should also be attached here.) The probability of emission is

e

PE = 1 + n(k ,T ) =

e

h¯ k kB T

h ¯ k kB T

. −1

I’ll need to include these probabilities in the electron–phonon matrix element for each process. At ﬁnite temperatures I can have either absorption or emission of the phonon. Equation 12.36 tells me that the threshold for absorption is lower than that for emission (by 2k ). But the probability of emission dominates for T < h ¯ k /kB . The scale of temperatures is the Debye temperature, which is 370 K for Ge and 645 K for Si. At low temperature, PA = e

h − k¯ Tk B

PE = 1 + e

h − k¯ Tk B

.

∗ Another possibility of course is to use the actual phonon dispersion curves as measured by neutron scattering

or as calculated by some theoretical method.

232

Semiconductors and Insulators

In the following, I use these low-temperature probabilities; it is straightforward to insert the more general probabilities for higher temperature cases. I’ll treat various absorption processes as independent; the optical conductivity will be a sum of all possible processes at the given frequency. As frequency increases from zero, phonon absorption will turn on ﬁrst, then phonon emission, and then direct interband transitions. So now I have all the components needed to assemble the optical conductivity from indirect transitions from the valence-band maximum to the conduction-band minimum. But this is only one of many possible indirect transitions. Suppose I increase the photon energy a bit. Looking at Fig. 12.10, it is obvious that I could go from the valence band maximum to states in the conduction band a bit above the minimum. Of course, I could alternatively start a bit below the valence-band maximum and make a transition to the conduction-band minimum. Considering all directions in k-space, there are many states with energy differences of hω ¯ with ω a bit above ωg . The calculation at this point is very similar to the derivation in Section 12.7, so I will be even more sketchy here than I was earlier in the section. I’ll abandon all the various constants (e, h, ¯ etc.) but keep other terms. First, I’ll deal with the pesky 1/(ωf v − ω)2 + 1/(ωc0 − ω)2 term in Eq. 12.34. This term looks like a resonant denominator but it is not. The frequency ω is near the minimum value, ω ≈ ωg . The two frequencies ωf v and ωc0 are respectively the frequencies of direct interband transitions at the conduction band minimum and at the valence band maximum. These frequencies differ a bit but are much larger than the gap frequency. So I’ll set ωf v ≈ ωdg ≈ ωc0 with hω ¯ dg the direct band gap energy. The other things to do are • Sum over states in both conduction band (cb) and valence band (vb): (k in cb) ·(k in vb) . " • Convert to integrals: k → 2 d 3 k/(2π )3 . • Convert to energy integrals assuming parabolic behavior around the band extremes. If Fig. 12.10 describes the band structure, the valence band follows E = E0 − h¯ 2 k 2 /2m∗h and the conduction band follows E = Ef + h¯ 2 (k − kf )2 /2m∗h . √ • Put in the density of energy states: D(E) = E away from the band extremes. • Replace one factor of ω with ωg because I really am only interested in evaluating things at ω = ωg . • Do one energy integral, consuming the delta functions: E = h(ω ¯ ± k − ωg ). eγ • Use V = (e/2)|xvc |E0 . After these steps, the conductivity is proportional to σ 1 ∝ |V ep |2 |xvc |2

h¯ ω±h¯ k −Eg √ ωg hω ± h ωP − E EdE ¯ ¯ {A,E} k g (ωd − ωg )2 0

where the + sign is for the case of phonon absorption and the − for phonon emission. I choose the appropriate probability when I pick which sign I want. The integral is straightforward and the result gives the following regimes. First, transparent: σ 1 = 0,

(12.39)

233

12.10 Excitons for ω ≤ ωg − k . Second, phonon absorption:

σ 1 ∝ |V

ωg − | |xvc | e 2 (ωd − ωg )

ep 2

2

h ¯ k kB T

(ω + k − ωg )2 ≡ σ1A,

(12.40)

for ωg − k ≤ ω ≤ ωg + k . Third, phonon emission and phonon absorption: h ωg − k¯ Tk ep 2 2 B σ 1 ∝ |V | |xvc | 1+e (ω − k − ωg )2 + σ1A ≡ σ1E + σ1A (ωd − ωg )2 (12.41) for ωg + k ≤ ω ≤ ωdg , where ωdg is the direct band gap. Finally, (Eq. 12.20) σ 1 ∝ f ω − ωdg + σ1E + σ1A

(12.42)

for ω ≥ ωdg . Once the absorption turns on, there are two regions where the absorption increases quadratically in the frequency (or energy) difference above their threshold. The ﬁrst, phonon absorption, is exponentially small at low temperatures. The second, phonon emission, is weakly temperature-dependent at low temperatures. At high temperatures, both terms are strong. Both are negligible once the direct absorption turns on at ωdg .

12.10 Excitons The picture of interband transitions that began with Section 12.7 puts the electron–hole pair produced by optical absorption into delocalized states, extending in principal throughout the crystal. This point of view, energy band theory, is justiﬁed in ignoring the Coulomb interaction between electron and hole, inasmuch as this may well have been left out or approximated in deriving the band structure (H0 ) in the ﬁrst place. If, in contrast one begins with a localized tight-binding theory using linear combinations of atomic orbitals, the electron and hole might be located on a single atomic site. In this second case, it is likely that the Coulomb energy between electron (negative) and hole (positive) must be included. Reality is as ever somewhere between these two extremes. Effects of the Coulomb interaction are observed in many solids and go by the name of excitons. The exciton is a bound electron–hole pair. A photon may create an exciton if the photon energy equals the semiconductor’s energy gap minus the exciton binding energy Eex : h¯ ω = Eg −Eex . Because the exciton is neutral (one electron plus one hole) it does not carry electrical current. The exciton can migrate through the crystal, hopping from site to site, and carrying therefore an energy current. Many authors [54, 105, 252] distinguish two exciton types: Frenkel excitons are small (one atomic site) and tightly bound. Wannier excitons are large (with a radius considerably larger than the lattice spacing) and have a corresponding smaller binding energy. A third type, similar to Frenkel excitons, is the charge-transfer exciton where the electron and hole occupy neighboring molecules. Unlike Frenkel and Wannier excitons, charge-transfer excitons have a net dipole moment.

234

Semiconductors and Insulators

Excitons are observed in many solids. The excitons in KCl (and other ionic crystals), anthracene (and other organic materials), and other large band gap solids are interpreted as Frenkel excitons. Charge-transfer excitons occur in low-dimensional organic conductors, La2 CuO4 , and other cuprate materials. Wannier excitons occur in many semiconductors including Ge, GaAs, CuO2 , Xe, and ZnTe. I’ll work out an extremely simple model for Wannier excitons, based on the Coulomb interaction in the crystal. To start, I’ll consider that the electron and hole are in band states with little relative difference in their group velocities. In vacuum their potential energy would be V (r) = −ee/r. Using either the Bohr model or the Schr¨odinger equation they would be bound with energy En = −R/n2 with n = 1,2,3 . . . the principal quantum numbers and R = μe2 /2h¯ 2 the Rydberg of positronium, about 6.8 eV. (μ = me /2 is the reduced ˚ mass.) The radius of the n = 1 wave function (the Bohr radius) is a = h¯ 2 /μe2 ≈ 1 A. Two changes need to be made on account of the crystal. First, the dielectric medium screens the electric ﬁeld, so I need to make the substitution e2 → e2 /1 (0), with 1 (0) the static dielectric constant.∗ Second, the effective mass of the electron and hole are not the free electron mass but instead the band mass at the band edges, m∗e and m∗h respectively. The Hamiltonian for the excited electron hole pair is H=−

h¯ 2 2 h¯ 2 2 e2 . ∇ − ∇ − e h ∗ 2m∗e 2mh e1 (0)|re − rh |

(12.43)

The solution is easy.† E = Eg +

R μ∗ hK ¯ 2 − , ∗ 2(m∗e + mh ) n2 m[1 (0)]2

(12.44)

where μ∗ is the reduced mass, 1/μ∗ = 1/m∗e + 1/m∗h , and K = ke + kh is the total wave vector of the two particles. The second term is the kinetic energy of the center of mass of the electron–hole pair and the third is their binding energy. The exciton “Rydberg” is Rex = R

μ∗ . m[1 (0)]2

Because the dielectric constant is big (of order 10) and the reduced mass is small (perhaps 0.05m) the exciton Rydberg is Rex ≈ 7 meV ∼ 50 cm−1 . At the same time, the exciton ˚ This size is much larger than the 2–3 A ˚ radius for n = 1 is aex = a0 m1 (0)/μ∗ ≈ 100 A. interatomic spacing of most semiconductors. The large size justiﬁes the use of the Wannier picture. Some values [277, 278] are shown in Table 12.4. There are some evident trends. As the band gaps increase, so do the exciton binding energies; the exciton dimensions decrease with increasing gap. It is not uncommon to see plotted on a diagram like Fig. 12.4 or Fig. 12.5 exciton dispersion relations that follow Eq. 12.44. The dispersion curves appear just below the conduction band, offset by Rex /n2 . Such a diagram can be helpful in visualizing the situation but is in fact incorrect. The band diagrams show the energies of single electrons ∗ I use the static dielectric constant because I am seeking a stationary state for the exciton wave function. † Because I know how to solve the hydrogen atom!

235

12.10 Excitons

Table 12.4 Exciton binding energy and size for certain semiconductors. Material InSb Cd0.3 Hg0.7 Te Ge InP GaAs CdTe Cu2 O CdS ZnSe GaN

Fig. 12.11

Eg eV

Rex meV

aex ˚ A

0.237 0.26 0.89 1.42 1.52 1.61 2.17 2.6 2.82 3.51

0.5 0.7 1.4 5.0 4.1 10.6 97.2 28 20.4 22.7

860 640 360 140 150 80 38 27 60 40

Excitation energy in a semiconductor. Three exciton levels are shown as well as the continuum of excitations above these.

in valence and conduction bands. I can put an electron in the conduction band by marking the energy Ee and wave vector ke . I can indicate a hole by marking the energy Ev and wave vector kv of the valence band state from whence it came, understanding that the hole energy Eh = −Ev and the hole wave vector kv = −kv . I cannot put the energy of an electron–hole pair on such a diagram. A better way to approach such a diagram is to make an excitation spectrum, just as I did for a superconductor, in Chapter 11 (Section 11.5). Such a diagram is shown in Fig. 12.11 The ground state, E = 0, is the semiconductor with full valence band and empty conduction band. A photon of frequency ω and essentially zero wave vector is absorbed. If

236

Fig. 12.12

Semiconductors and Insulators

Sketch of the optical conductivity of a semiconductor with several exciton lines below the onset of interband transitions. there is no Coulomb interaction, assuming parabolic dispersion, and if hω ¯ ≥ Eg , then an electron–hole pair is created with energy Eg +

h¯ 2 kh2 h¯ 2 ke2 + = hω. ¯ 2me 2mh

(12.45)

The wave vector selection rule is satisﬁed by requiring ke + kh = 0 which will be true if the valence band state and conduction band state have the same wave vector. If now I turn on the Coulomb interaction, there is an attraction of electrons and holes. I create excitons, electron–hole pairs with energies given by Eq. 12.44. Three such levels are shown in Fig. 12.11. Excitons contribute to the optical conductivity when photons create excitons with one or another value of n. Now the photon has q = 0 so cannot give the exciton center of mass any momentum. Consequently there is a peak in σ 1 (ω) when ω = ωg − Rex /hn ¯ 2 for a number of values of n. Just above the exciton lines, which can carry considerable oscillator strength, the continuum of electron–hole excitations (interband transitions) begins. A cartoon of the spectrum is in Fig. 12.12 and an example of exciton peaks in Cu2 O is in Fig. 12.13.

12.11 Impurity-Induced Absorption Silicon, GaAs, Ge, and other semiconductors are a dominant force in the world economy for one reason: their electrical properties may be determined by incorporating controlled amounts of other atoms. These atoms are called “impurities” and the process is called

237

Fig. 12.13

12.11 Impurity-Induced Absorption

Absorption coefficient [− ln(T ) actually] of Cu2 O showing a series of exciton lines. From Ref. 279. “doping.” Neither term is particularly well chosen; in particular the dopants are not undesirable impurities but instead are carefully controlled as to type, concentration, and location. Si is typically doped with atoms from periodic table columns on either side of Si itself. Si (group IV A) has four valence electrons (3s2 3p2 ) which bond covalently to four neighboring Si atoms, forming a tetrahedrally coordinated cubic crystal structure. Atoms from the neighboring columns have one more or one less valence electron. B, to the left (group III A), has three and P, to the right (group V A), has ﬁve. When a B atom substitutes for Si, it accepts an electron from the valence band to complete the bonding, leaving a hole behind. When a P atom is substituted, it uses four of its electrons for the covalent bonds and donates the ﬁfth to the conduction band. Thus doping controls the free-carrier density, and hence the electrical conductivity. It also controls the energy location of the chemical potential. And ﬁnally it controls the sign of the charge carriers. Hole doped Si (e.g., with B) has positive carriers and is called p-type silicon. Ga, In, N, and Al also can be used to produce p-type Si for special applications. Electron doped Si (e.g., with P) is called n-type silicon. As and Sb are also used to make n-type Si. If the above were the whole story, I would be almost done with this section. I would just say that the free carriers give a Drude-like conductivity with carrier density that depends on doping and with a scattering rate determined by a number of processes, some of which could be doping dependent. But this is not the whole story. It is correct at very high doping, where the doped Si is actually a metal. (The Fermi level is in either the conduction or valence band.) It is approximately true at very high temperatures, although in that case there are also free carriers thermally populated in both conduction and valence bands. But the dopant atoms have a net charge. P and other donors have given up one electron and so have a charge +e. B, and other acceptors, have accepted one, and have a charge −e. There is a Coulomb

238

Semiconductors and Insulators

interaction between the dopant ions and an electron or hole in the solid. The result is another hydrogen atom problem. I’ll start by looking at the quantum problem at T = 0. The Hamiltonian is H=−

e2 h¯ 2 2 , ∇ − 2m∗ 1 (0)|r|

(12.46)

where m∗ is the effective mass, either hole or electron depending on which case is in play, r is the separation of the electron or hole from the impurity, and 1 (0) is the static dielectric constant. Like the exciton, Eq. 12.46 is a scaled version of the Hamiltonian for the hydrogen atom, which I know how to solve. In fact, shallow impurities are an interesting analog to the hydrogen atom. The energy levels for electrons in the conduction band at the level of the Bohr model are m∗e R Re = − 2. Ee = − 2 2 n m[1 (0)] n

(12.47)

Here R = me4 /4π h¯ 3 c = 13.6 eV is the Rydberg energy, n = 1, 2, 3 . . . is the principal quantum number, and m∗e (= 0.26m for Si) is the effective mass. This mass is an average of transverse and longitudinal effective masses for the Si conduction band minima. If I use 1 (0) = 11.7 as the Si dielectric constant, then Re = 25.8 meV. The energy is measured from the bottom of the conduction band, so the donor level is about 26 meV below the conduction band edge. At the same time, the radius for n = 1 is ae = a0 m1 (0)/m∗e ≈ ˚ The electron wave function extends over many lattice constants. 22 A. A full quantum-mechanical picture of the energy levels of the donor atom includes many effects [252, 280]. The bound electron wave function is expanded in terms of Bloch functions for the crystal and the anisotropy of the conduction band and valley-orbit coupling are included. The results of a calculation along with experimental values for the levels are shown in Fig. 12.14. The values of the ground state energy splitting from the conduction-band minimum are given in Table 12.5. For holes in the valence band, Eq. 12.46 gives m∗h R . Ev = − 2 n m[1 (0)]2

(12.48)

Here m∗h (= 0.39m for Si) is an effective average of light-hole and heavy-hole masses (a detail of the band structure of Si). Using these numbers then Rh = 38.7 meV. The energy of the hole states are measured downward from the valence-band maximum, so this

Table 12.5 Ionization energy (Ec − Ed or Ea − Ev , in meV) of donors and acceptors in silicon [252, 280–282]. Donors Dopant Ionization energy

P 46

As 54

Acceptors Sb 43

B 45

Al 57

In 160

239

12.11 Impurity-Induced Absorption

Fig. 12.14

Calculated and measured donor levels in Si [280].

Fig. 12.15

Optical conductivity of lightly doped Si at five temperatures.

negative energy level is about 39 meV above the top of the valence band. Measurements put it a bit further away [252, 281, 282]. The low-temperature spectra of lightly doped Si (and other semiconductors) resembles that of hydrogen, after accounting for the scaling by dielectric constant and effective mass discussed above. An example is shown in Fig. 12.15. This diagram shows the optical conductivity measured at a number of temperatures on a Si sample with about 6 × 1013 P atoms/cm3 (a dopant concentration of 1.2 parts per billion). The lines tagged in black correspond to transitions from the ground state 1S(A1 ) to higher nP states. Transitions up to n = 6 are identiﬁed.

240

Semiconductors and Insulators

As temperature is increased, the intensity of these narrow conductivity peaks decreases, because carriers are being excited thermally to the conduction band. (And in fact at higher temperatures a Drude-like free-carrier peak is seen below 50 cm−1 or 6 meV.) Another effect that is seen is the appearance of new lines (tagged in red) at intermediate temperatures. These lines are strongest around 50 K. They are due to carriers thermally promoted above the ground state being excited to higher levels. The analogy to the behavior of hydrogen is good. The features seen at the lowest temperature are comparable to the Lyman series, where the starting point is the ground state. The features that appear as temperature is increased are like the Balmer series, where the starting point is the ﬁrst level above the ground state.

13

Strongly Interacting Solids

Much of the richness of solid-state physics arises from the interactions among electrons, phonons, magnons, and other entities in the solid. These interactions are responsible for superconductivity, magnetism, metal–insulator transitions, and many other effects. They are also responsible for temperature-dependent transport properties and for frequencydependent optical properties. I have worked out the dielectric function and optical conductivity of a Drude metal already. I ﬁrst did it classically (Chapter 4), then quantum mechanically, and then quantum mechanically again using the Boltzmann equation (Chapter 8). All three times I got the same results for the conductivity (Eqs. 4.8, 8.21, and 8.39) and also for the dielectric function (Eqs. 4.11 and 8.22). The scattering rate 1/τ appears as a parameter in these equations. The charge carriers are assumed to scatter off of something at a rate given by 1/τ . There are many such somethings; two that are important for simple metals are impurities and phonons, both of which break the translational symmetry of the crystal. Many other possibilities exist. The assumption implicit (if unstated at the time) is that 1/τ is just a constant and the same value should be used at zero frequency and at petahertz frequencies. Now, I know that 1/τ is a function of temperature. I showed as an example the resistivity of the good metal silver in Fig. 8.6. I write here the Drude formula for the DC resistivity: ρdc = 1/σdc = (m/ne2 )(1/τ ), where the mass m, density n, and charge e of the carriers are essentially constant in temperature.∗ The strongly temperature-dependent ρ is then caused by a strongly temperature-dependent 1/τ . In pure ordinary metals, such as Ag, the temperature-dependent transport is attributed to the temperature dependence of the phonons. It is worth asking this: Can the scattering rate be temperature dependent without also being frequency dependent? I think that the answer is no, although I cannot provide a proof. I can give an example of a case where I do expect both temperature and frequency dependences. The example is the interaction of electrons and phonons. The phonons have a range of energies or frequencies, from zero to the Debye frequency in the simplest case; more complicated phonon spectra exist in multi-atom solids. The occupied energies, however, are determined by the temperature and the distribution function. Roughly speaking, the range is from zero to h¯ ω ≈ kB T where kB is Boltzmann’s constant and T the temperature. The zero-frequency (DC) transport involves scattering by these ∗ This statement is not true for a semiconductor, where the carrier density n is thermally activated and thus varies

exponentially with 1/T . It is also not true for quasiparticles in a superconductor, whose charge q consists of a mixture of electron-like and hole-like states.

241

242

Strongly Interacting Solids

thermal excitations and varies with temperature because the number of thermally-generated phonons varies with temperature. There is another allowed phonon–electron interaction at ﬁnite photon frequencies. The electrons, driven at the frequency of the electric ﬁeld, may emit (rather than absorb) a phonon.∗ The emission process may occur at zero temperature, but clearly the energy of the emitted excitation must come from the electromagnetic ﬁeld – the photon. Phonon emission is therefore a ﬁnite frequency effect and should be largest at frequencies at and above the maximum frequency of the phonons. Emission leads to scattering – and current relaxation – because the emitted phonon has a momentum, requiring that the electron change its momentum. Phonon energies are much less than Fermi energies, so that the change of energy is typically small but the change of momentum can be large. A consequence of the emission process is a frequency dependence to the scattering rate and conductivity that is not captured by the Drude model with scattering rate 1/τ (T ) as obtained from DC resistance. I will cover brieﬂy in this chapter this and another of other optical effects in interacting electron systems. The interactions may be between (or among) the charge carriers themselves or may be with the phonons or other bosonic spectra. This topic is the realm of quantum many-body theory and of numerical approaches. This fact leads to a somewhat unsatisfactory approach: I’ll present results from workers in the ﬁeld, cite their papers, try to give a discussion of the underlying physics, work out in a couple of cases simple toy models, and then say what optical effects are obtained from these concepts. But derivations from ﬁrst principles will be lacking.

13.1 Notation: The Generalized Drude Model I need to deﬁne the notation used before I can address the ways in which interactions can affect optical properties. It is not as straightforward as it might seem. I cannot simply replace 1/τ with 1/τ (ω) and put this function into Eqs. 4.11 and 4.8. The real and imaginary parts of the dielectric function and conductivity satisfy Kramers–Kronig relations and the scattering rate appears in different ways in the real and the imaginary parts. (See Eqs. 4.10a and 4.10b or Eqs. 4.14a and 4.14b.) This substitution would violate causality and I don’t want to do that. There are in reality two (equivalent) way to resolve this violation but there are a bewildering number of variations on these two. The two are: (1) I make another quantity (the plasma frequency or the effective mass) also frequency dependent [283], choosing the frequency dependence so that Kramers–Kronig is satisﬁed. (2) I make the scattering rate a complex quantity [284], and relate the real and imaginary parts of this quantity so that the conductivity or dielectric function obey Kramers–Kronig.† A related variation is to deﬁne an optical self energy, the usual self energy averaged over the Fermi surface [285]. ∗ Emission of other other kinds of excitations is also possible. † Perhaps not surprisingly, this obedience is achieved by making the complex scattering rate itself obey a

Kramers–Kronig relation.

243

13.1 Notation: The Generalized Drude Model

13.1.1 Frequency-Dependent Mass (Or Plasma Frequency) To make the plasma frequency or the effective mass also frequency dependent, I’ll rewrite Eq. 4.13 as (ω) = ni (ω) −

[ωeff (ω)]2 ω2 + iω/τ ∗ (ω)

(13.1)

where 1/τ ∗ is the frequency dependent scattering rate (written with an asterisk because the effective mass will be starred too), ωeff (ω) is the effective plasma frequency, and I have gathered all the other contributors to the dielectric function (core electrons, interband transitions, optical phonons – the noninteracting parts) into ni . The plasma frequency of the metal in the noninteracting case is ωpb = 4π ne2 /mb (Eq. 4.12). I’ve added the subscript b to the plasma frequency and to the mass to stand for “bare” or “band,” the mass in the absence of interactions but allowing for band structure effects.∗ It thus makes good sense to deﬁne ωeff (ω) as containing a frequency-dependent effective mass m∗ (ω) via 4π ne2 (13.2) ωeff (ω) = m∗ (ω) and writing the equivalent of Eq. 4.11 for the interacting case as (ω) = ni (ω) −

4π ne2 /m∗ (ω) ω2 + iω/τ ∗ (ω)

(13.3)

where n and e, the carrier density and electronic charge respectively, are not functions of frequency.† Another variation is to deﬁne a dimensionless mass enhancement factor λ(ω) and write m∗ (ω) = mb [1 + λ(ω)].

(13.4)

Of the three conceptually identical equations, I like Eq. 13.3 the best and will adopt it as a standard. I like Eq. 13.1 the least and won’t use it any more. Papers discussing optical effects in correlated or interacting electrons often show or calculate the real part of the optical conductivity. One advantage of using the conductivity is that various processes generally add in parallel; I can write σ = σni + σi where the subscript i means “interacting” and then only write the interacting term. I may even drop the subscript. A disadvantage is that I have to get the units right. Note that the contributions of the noninteracting electrons (e.g., interband transitions) may occur at high frequencies and thus may be ignored for the real part of the conductivity. However, the lowfrequency limiting behavior generates a linear-in-frequency addition to the imaginary part: σni 2 = −ω(ni 1 − 1)/4π . (See Eq. 3.8.) This additional term rarely can be neglected. To do so is equivalent to neglecting c in Eq. 4.11. The result is the loss of the plasma minimum in ∗ In the simple case it of course is just the free electron mass. † The density and charge may also depend on the frequency. Indeed, I discussed in Section 11.6.4 the excitation

spectrum of a superconductor in terms of an effective charge for the quasiparticles, interpreted as mixing of electrons and holes. I kept the mass constant, equal to mb .

244

Strongly Interacting Solids

reﬂectance that I plotted in Fig. 4.7; the reﬂectance simply decreases monotonically starting at the frequency where 1 (ω) becomes positive. With frequency-dependent effective mass and scattering rate, the Drude conductivity becomes σi = i

ne2 /m∗ (ω) , ω + i/τ ∗ (ω)

(13.5)

where I’ve relocated τ ∗ and i from where they are in the standard expression, Eq. 4.8, so that τ ∗ only appears once, and as a rate. If I have the complex dielectric function or complex conductivity for some material, and I have properly subtracted ni or σ ni , then I can see what the complex scattering rate and effective mass (or λ(ω) or ωeff ) look like by inverting the real and imaginary part of Eqs. 13.5 or 13.3. The result is σi 1 (13.6) 1/τ ∗ = ω σi 2 and 2 ωpb m∗ = mb 4π ω

σi 2 2 σi 1 + σi22

.

(13.7)

I need to know ωpb in order to evaluate Eq. 13.7. I use the sum rule on the conductivity, Eq. 9.30, ∞ 1 2 π ne2 dω σ i 1 (ω) = ωpb = . 8 2 mb 0 The idea of the sum rule is that interactions (including phonon scattering or superconductivity or any other) can change the functional form of the optical conductivity and can move spectral weight from one frequency location to another, but that the overall area under the curve is unchanged. Its result can be interpreted as giving the plasma frequency of the bare or band carriers, before turning on the interactions.

13.1.2 Complex Scattering Rate An alternate approach is to make the scattering rate a complex number and leave the plasma frequency as the bare plasma frequency [284]. The dielectric function then looks like (ω) = ni (ω) −

2 ωpb

ω2 + ωM(ω)

.

(13.8)

The complex function M(ω) is known as the “memory function” and contains the information about the interactions. If there is only scattering from impurities, one ﬁnds M1 = 0 and M2 = 1/τi∗ . I actually see a variation on this notation more than the original. The variation is to deﬁne M = i and write the dielectric function as (ω) = ni (ω) −

2 ωpb

ω2 + iω(ω)

,

(13.9)

245

13.1 Notation: The Generalized Drude Model

and the conductivity as σi = i

ne2 /mb . ω + i(ω)

(13.10)

The quantity is also known as the memory function. Many authors [237, 246, 286, 287] use a different notation, writing σi = i

ne2 /mb ω(1 + λop ) + i/τ op

(13.11)

where 1/τ op = 1 is the optical (or “unrenormalized”) scattering rate and λop = −2 /ω is the mass enhancement factor. Note that although λop is the same quantity that appears in Eq. 13.4, 1/τ op differs from 1/τ ∗ . I’ll discuss the differences below. I started this section by asserting that the Kramers–Kronig relations for the conductivity or the dielectric function required a complex scattering rate.∗ Let me write Ohm’s law in a way closer to the way it is done in circuits. Instead of j(ω) = σ (ω)E(ω) I’ll use E(ω) = ρ(ω)j(ω). The resistivity ρ is a response function relating the ﬁeld to the current and must satisfy Kramers–Kronig. But according to Eq. 13.10, mb (13.12) ρ1 + iρ2 = 2 [1 + i(2 − ω)] ne so 1 and 2 − ω satisfy the same Kramers–Kronig relations as ρ1 and ρ2 . The real and imaginary parts of are easy to obtain from Eq. 13.12 1 =

σi 1 ne2 ne2 ρ1 = mb mb σi21 + σi22

and σi 2 ne2 ne2 ρ2 = ω − . 2 mb mb σi 1 + σi22 To extract the complex scattering rate (or memory function) from optical conductivity data, I need to know the ratio of carrier density n to bare mass mb . This ratio appears in the saturation value of the oscillator strength sum rule on the conductivity, and many workers use the value it reaches at the onset of interband transitions to estimate the ratio. Of course, considerations of crystal chemistry and electronic structure calculations also can give insight into these quantities. 2 = ω +

13.1.3 Optical Self Energy Littlewood and Varma [285] have written the dielectric function in the following form (ω) ≈ ni −

2 ωpb

[ω2 − 2ωop (ω/2)]

,

(13.13)

where op is the optical self energy governing quasiparticle excitations. The factors of two appear because quasiparticle excitations (as in superconductors or electron–hole pairs in ∗ Or a frequency-dependent plasma frequency.

246

Strongly Interacting Solids

semiconductors) are made in pairs. The division of the photon frequency by two in the argument of op assumes equal energy supplied to each of the excitations and is often not explicitly included. Sometimes it is explicitly excluded. A discussion of the relation between the self energy and the memory function, including how to average over the Fermi surface, has been given by Allen [288]. I compare Eq. 13.13 with Eqs. 13.8 and 13.10 and ﬁnd that M(ω) = i(ω) = −2op (ω/2).

13.1.4 Relations among These Approaches The ﬁrst comment I can make is that I cannot see a fundamental reason to use one or another of these approaches. All accomplish the goal of considering frequency-dependent or energy-dependent effects in the optical conductivity of correlated electron systems. Moreover, it is easy to translate among them. Thus, with a bit of algebra I get m∗ 1 , mb τ ∗

m∗ , 2 = ω 1 − mb

1 =

and 1 ω1 = , τ∗ ω − 2 m∗ ω − 2 . = mb ω

(13.14)

The terms “renormalized” and “unrenormalized” modify “scattering rates” in many papers. Let me see how the two rates appear. I start with Eq. 13.4 where I’ve written the effective mass of the charge carriers as m∗ = mb (1 + λ). Here, m∗ is a mass that has been renormalized from the bare/band value by the interactions of the carriers with other excitations in the solid. I think the term comes from Landau’s Fermi liquid theory, where he showed that the states in strongly-interacting systems are one-to-one with those in the noninteracting Fermi gas as long as one renormalizes the parameters. Now, I substitute m∗ into Eq. 13.5, and multiply top and bottom by 1 + λ to get σi = i

ne2 /mb . ω(1 + λ(ω)) + i(1 + λ(ω))/τ ∗ (ω)

(13.15)

I’ll now write Eq. 13.10 again, but expanding = 1 + i2 : σi = i

ne2 /mb . ω − 2 (ω) + i1 (ω)

(13.16)

When I compare the real parts of the denominators of Eqs. 13.15 and 13.16 I learn nothing that is not in Eq. 13.14. But the imaginary parts show that 1 τ ∗ (ω)

=

1 (ω) . 1 + λ(ω)

(13.17)

The quantity 1/τ ∗ is called the renormalized scattering rate and 1 the unrenormalized rate.

247

13.2 Electron–Electron Interactions

Note that the distinction between renormalized and unrenormalized rates evaporates at zero frequency. The DC limit of Eq. 13.5 is σdc =

ne2 τ ∗ ne2 = . m∗ 1 m b

The enhanced mass is canceled by the smaller scattering rate. Finally, let me comment that I have seen 1 and gG2 described as causal and m∗ and 1/τ ∗ described as non causal. Do not be deceived by this. The equations using m∗ and 1/τ ∗ do not violate causality. What is meant is that the two functions are not Kramers– Kronig pairs.

13.2 Electron–Electron Interactions Electrons are charged particles and interact via the Coulomb interaction. An electron that is separated by the Bohr radius from another electron sees an electrostatic potential of 27 eV. Of course the average separation in a solid of the conduction electrons one from another is a bit more than this, but still I might expect to see eV scale Coulomb energies. These energies are not too different from the Fermi energy. Given this large energy, it seems surprising that the free-electron gas, neglecting completely interactions among the electrons, describes well the electrical, thermal, magnetic, and optical properties of metals. The answer lies in Fermi liquid theory. In this picture, interactions between electrons are turned on adiabatically in a way that there is a one-toone mapping between electron states in the noninteracting picture and electron-states in the interacting picture. The free-electron states are mapped into Fermionic quasiparticle states in the interacting system. The quantum numbers of the quasiparticle (charge, momentum, and spin) remain the same as they were before interactions were turned on. The interacting system also has a Fermi surface with the same volume (number of states) but the energy, the effective mass, and the scattering rate differ from those of the free particles. Despite the different parameters, Fermi liquid theory allows the strongly interacting system to be described in a noninteracting picture.

13.2.1 The Fermi Liquid The transport processes in the Fermi liquid should be affected by electron–electron scattering. Here, I’ll try to estimate the rate of such scattering.∗ The qualitative argument is that at temperature T two electrons can interact effectively only if their energies are within the kB T energy range around the Fermi energy EF where the Fermi–Dirac distribution function is neither one nor zero. The probability that one electron has an such an energy is of order kB T /EF . The probability that the other also

∗ I’ll do this in a free-electron picture. I actually do not need any of the Fermi-liquid machinery to do the

calculation at the level at which I’ll do it.

248

Strongly Interacting Solids

Fig. 13.1

Electron 1 (above the Fermi level) scatters with electron 2 (below it) and relaxes towards the Fermi level. A hole is left in the Fermi sphere and there are two electrons above the Fermi surface. Momentum and energy are conserved in the process. is within this range is the same. Because the particles are independent, the scattering probability is proportional to (kB T /EF )2 . I can ﬂesh this idea out a bit more by considering the zero temperature Fermi sphere with an electron in a state close to but just above the Fermi surface. This electron has energy E1 > EF . (I’ll suppose in a moment that the electron acquired this extra energy by absorbing a photon with energy hω ¯ = E1 − EF .) As indicated in Fig. 13.1, this electron can scatter from a second electron with energy E2 < EF (just below the Fermi energy). The discussion is simpliﬁed if I consider the energies of the initial and ﬁnal states relative to the Fermi level: i = Ei − EF . Electron 1 has relative energy 1 > 0 and electron 2 has relative energy 2 < 0. The scattered electrons have relative energies 3 and 4 ; the Pauli principle requires both energies to be just above the Fermi energy. Moreover, energy conservation requires the distance electron 2 is below the Fermi surface to be less than the distance electron 1 was above it: |2 | < 1 . Therefore, the fraction fi of electrons in the Fermi sphere that actually can interact with electron 1 is the ratio of the volume a shell of thickness 1 to the volume of the whole Fermi sphere:

EF − 1 3/2 V (EF ) − V (EF − 1 ) 1 ≈1− ≈ , (12.5) fi ≈ V (EF ) EF EF √ where I have used 4π kF3 /3 with kF = 2mEF /h¯ for the volume of the sphere. The fraction fi is small. Now I look at the ﬁnal states after the interaction process. Energy conservation requires that the sum of ﬁnal relative energies satisﬁes 0 ≤ 3 + 4 ≤ 1 . I’ll assume upper limits of 1 , and see that the fraction ff of states above the Fermi level that are accessible to the scattered electrons is of order 1 ff ≈ . (12.6) EF

249

13.2 Electron–Electron Interactions

Consequently the phase space f for an electron–electron scattering event becomes

2 1 f ≈ . (13.18) EF If I include ﬁnite temperatures, there is a width of energies of order kB T around the Fermi energy to include in this phase-space argument. I also set 1 ≈ hω, ¯ the energy available from a photon, to get

2

kB T 2 h¯ ω f ≈ + . (13.19) EF EF This is a very small number, say 10−8 at 10 K or 10 cm−1 . The scattering rate will be proportional to f , so that it follows that 1/τ ∝ T 2 at low frequencies and 1/τ ∝ ω2 at low temperatures. There is however, an annoying ﬂaw in this argument: The scattering process conserves momentum, which means that k1 +k2 = k3 +k4 . I suppose that before the scattering event the current was given by Eq. 8.20, j = −(neh/m)δk ¯ i , with n the electronic density, e the electronic charge, m the effective mass of the charge carriers, and δki the displacement of the Fermi sphere from its equilibrium position. Then, after the scattering has taken place I have a new δkf = δki + (k3 + k4 − k1 − k2 )/N = δki where N is the total number of electrons. So the current is unchanged because the scattering is within the electron system alone and the total momentum is unchanged. For electron–electron scattering to affect the conductivity, it must involve “umklapp scattering,” a process where at least one of the two scattering wave vectors lies outside the Brillouin zone. By the arguments surrounding Fig. 12.4, I can reduce this vector to the ﬁrst zone by the addition of whatever reciprocal lattice vector G that accomplishes this task. This umklapp scattering process does change the total momentum of the electron system and contribute to the optical conductivity. As an illustration, consider a one-dimensional example so that k is a scalar. As in the left panel of Fig. 12.4, k has a range of −π/a < k ≤ π/a. Suppose k3 = (1 + δ)π/a, placing it a small amount δ past the zone boundary, which is at +π/a. I can equally well represent it as k3 = (1 + δ)π/a − 2π/a, using G = 2π/a. Then k3 = −(1 − δ)π/a, close to the zone boundary on the opposite side of the Brillouin zone. Umklapp scattering has signiﬁcantly affected the electron’s momentum. Electron–electron interactions plus umklapp scattering will lead to ω2 and T 2 terms in the scattering rate. Many-body calculations of the scattering rate due to electron–electron scattering have been done by a number of workers [289–295]. The scattering rate is ( 2 ' 1 2 = (hω) + (2π kB T )2 , ¯ τ 3π hE ¯ F

(13.20)

' ( 1 2 = a (hω) + b(π kB T )2 . ¯ τ

(13.21)

or in more generic form

250

Fig. 13.2

Strongly Interacting Solids

Optical conductivity of a Fermi-liquid metal. A Drude spectrum is shown for comparison. The factor b should be b = 4 but experiments ﬁnd it varying from below 1 to almost 6 [295]. These discrepancies are an active area of research. In principal, the ω2 behavior continues up to photon energies of order the Fermi energy, above which 1/τ should become constant.∗ The real part of the Fermi-liquid conductivity [289, 295] is then ω2 + (2π kB T /h) ¯ 2 . ω2 When hω ¯ 2π kB T the conductivity is constant, called the “Fermi foot.” In this it differs from the high-frequency part of the Drude formula, where σ 1D ∼ 1/ω2 . A plot of the conductivity is in Fig. 13.2. The conductivity spectrum has a low frequency part which is equal to the DC conductivity, a Drude rolloff, and then a long foot beginning when hω ¯ > EF ¯ ≈ 2π kB T (about 190 cm−1 in this calculation, which is for T = 50 K). Once hω (about 5,000 cm−1 ), the Drude spectrum is regained but with a much larger scattering rate. A Drude spectrum, having the same DC conductivity and low-frequency scattering rate is also shown in Fig. 13.2. σ 1 (ω) = σ 0

13.2.2 The Marginal Fermi Liquid Varma et al. [296] proposed a phenomenological model for the oxide superconductors that they call a “marginal Fermi liquid.” This model assumes that excited charge carriers interact with a spectrum of (optically inactive) excitations which is ﬂat over T < ω < ωc , where ωc is a high energy scale (the bandwidth, for example) that cuts off the spectrum. Evidence advanced in support of this hypothesis describing the cuprates includes the Raman spectrum [297], where a broad continuum of electronic excitations extending to ∗ At such frequencies, usually, many other optical processes have also turned on and the detailed Fermi-liquid

behavior would be masked anyway.

251

13.2 Electron–Electron Interactions 1 eV (8,000 cm−1 ) is observed, and the angle-resolved photoemission [298, 299], where a broad, asymmetric peak at the Fermi energy is seen. According to Varma et al. [296] and Littlewood and Varma [285] the quasiparticle self energy of the marginal Fermi liquid has an imaginary part which qualitatively goes as ! π 2 λT , ω < T (13.22) − Im (ω)∼ π λω, ω>T where λ is the strength of the interaction, an integral of square of a matrix element and a density of states. There is a corresponding logarithmic (in ω/ωc or T /ωc , whichever is greater) behavior in the effective mass, with the mass enhancement proportional to λ. The inverse lifetime (or scattering rate) of the charge carriers is given by the imaginary part of the self energy, which at zero frequency is linear in T . This result is in accord with the measured resistivity of optimally-doped cuprate superconductors [300, 301]. At high frequencies, there is no temperature dependence in Eq. 13.22 and the scattering rate is proportional to ω; the lifetime to 1/ω. Thus, at high frequencies the conductivity becomes σ1 (ω) = ωp2 τ/4π (1+ω2 τ 2 )∼ωp2 /4π ω. It goes like 1/ω in contrast to the 1/ω2 dependence of an ordinary metal with frequency-independent scattering. This behavior is reasonably in accord with the conductivity spectrum of Fig. 11.16.

13.2.3 The Hubbard Model In both the Fermi liquid and the marginal Fermi liquid, the transport and optics are basically metallic in the qualitative sense. The DC conductivity decreases as temperature is raised from the lowest T . Analysis discloses that the carrier density is roughly constant over a wide temperature range. The optical conductivity has a maximum at ω = 0 and falls with increasing frequency. (The frequency dependence differs from the Drude metal, but has a superﬁcial resemblance and often may be ﬁt by a Drude–Lorentz model.) In contrast, the Hubbard model [302] allows for strong Coulomb repulsion between electrons. If this repulsion is sufﬁciently strong, and if the electron occupancy is right (about one per site), the Hubbard model gives an insulating ground state in a system that otherwise would be a metal. This insulating state is a speciﬁc example of a Mott transition – an insulating state driven by correlations of the electrons [303]. Thus there are two different mechanisms that can affect solids which otherwise would be free-electron metals and make them insulators. In band insulators, the electron interacts with the periodic potential of the ions, giving a gap in the single-particle spectrum when the Fermi surface coincides with the Brillouin-zone boundary. Mott Insulators are insulators due to the electron–electron interaction. Many-body physics leads in Mott systems to a gap in the charge excitation spectrum. The system has to pay too high a price to have electrons be mobile and thereby approach each other too closely. In it’s simplest form, the Hubbard Hamiltonian is written in second-quantized notation as ci†σ cj σ + U ni↓ ni↑ (13.23) H=t ij σ

i

252

Strongly Interacting Solids where t is a transfer or hopping integral, ci†σ creates an electron on site i with spin σ , cj σ destroys an electron on site j with spin σ (so that in concert they transfer an electron from site j to site i). The ﬁrst sum is a restricted sum over sites and their neighbors, organized so that the electron can transfer between j and any neighbor. The second sum (on σ ) is a sum on spin. In the second term, U is the strength of the Coulomb repulsion between two electrons on the same site and ni σ = ci†σ ci σ counts the number of electrons on site i with spin σ . The Pauli principal ensures that the count is either 0 or 1. The second term is summed over sites, adding U to the energy eigenvalue every time two electrons occupy the same site. If U = 0, then Eq. 13.23 is the Hamiltonian of a tight-binding metal. It is easy to solve by writing the Fourier transform of the creation/annihilation operators 1 −ik·a e ci†σ = √ N k where N is the number of sites, k is the wave vector, proportional to (integer)·2π/L, and the sum would be over these integers. Using this operator and its Hermitian conjugate, it is easy to show that the energy is Ek = −2t cos(ka).

(13.24)

The larger is the transfer integral, the greater the width of the band. This relationship makes sense: strong overlap between sites leads to large bandwidth. Here, the width is W = 4t. The nonlinear behavior of the Hubbard model make it intractable in general. An exact solution has been made for the case of half ﬁlling (exactly one electron per site) in one space dimension [304]. The result is that the one dimensional chain is an insulator for all ﬁnite U . (However the charge gap is quite small for U < 2t.) Other results come from numerical solutions of clusters and from various approximations. There are lots of these, done in all space dimensions (from one to inﬁnity) and sometimes for more than a single band. Almost all results do show a Mott–Hubbard metal–insulator transition as U is increased from zero. ∗ Typically, U > ∼ 4t is needed in order to render the solid an insulator. The picture that emerges is sketched in Fig. 13.3. On the left is the metal (U = 0), with bandwidth W . The metallic band is half ﬁlled. Because a single band can generally hold two electrons per site and still make the Pauli principal satisﬁed, the half-ﬁlled metal has one electron per site. On the right is the insulator, with U large enough to make it so. There are now two bands: the “lower Hubbard band,” which is completely ﬁlled and the “upper Hubbard band,” completely empty. Both bands are narrower than the single band of the metal. There is an energy gap between the two bands; the system is an insulator. It is relatively simple to imagine the optical properties of such a system. The metal would have a Drude spectrum although probably with a frequency-dependant scattering rate and effective mass. The insulator would have the spectrum of a semiconductor or insulator with a gap Eg ∼ U . ∗ A band ﬁlling near 1/2 is also needed. The Hubbard model can be extended with next-nearest-neighbor Coulomb

repulsion V If U and V are both large enough, the 1/4 ﬁlled chain is insulating. Extension to even longer-ranged Coulomb terms are possible too. A number of interesting cases are discussed is in Ref. 305.

253

13.2 Electron–Electron Interactions

Fig. 13.3

Cartoon of energy band densities of states in (left) half-filled-band metal and (right) highly correlated “metal”with large Coulomb energy U .)

Fig. 13.4

Optical conductivity of K-TCNQ at 300 K. The dotted line shows the a-axis (stacking axis) spectrum. The spectrum perpendicular to the stacking axis (b or c) is dashed and a fit to Lorentzian oscillators is the solid line. An example is shown in Fig. 13.4. This ﬁgure shows the optical conductivity of potassium-tetracyanoquinodimethane (K-TCNQ or K-(NC)2 CC6 H4 C(CN)2 ), a quasi one dimensional organic solid [306]. The material is highly anisotropic, with a nearly tetragonal crystal structure. (See Chapter 15.) This material is a charge-transfer salt, in which an electron is removed from the K atom, rendering it a closed-shell K+ ion, and transferred to the TCNQ molecule, making it a singly-charged ion. TCNQ is a planar molecule and stacks face-to-face, with the stacking axis (also called the chain axis) along the a crystal axis. With one electron per molecule, K-TCNQ would be expected to be an organic metal. Instead. it is an insulator, and the insulating behavior is generally interpreted as due to a strong Coulomb interaction, exactly as in the Hubbard model.

254

Strongly Interacting Solids

The dotted line in Fig. 13.4 shows the a-axis (stacking axis) spectrum. The most prominent feature is a strong peak at about 7,000 cm−1 (0.9 eV). This peak is attributed to transitions across a Mott–Hubbard gap, with U ≈ 0.9 eV. There are a number of sharp peaks at lower frequencies, where the vibrational modes of the molecule occur. These are due to the Rice effect; see Section 13.3.2. To see how the Hubbard model works, I will work through the simple problem of two electrons on two sites. This is the “half-ﬁlled” case and actually contains much of the physics [307–309]. My system consists of two sites, each with a single molecular orbital. Because the electrons have spin, the two sites may be occupied with 0–4 electrons, subject to obeying the Pauli principal. The only interesting case is the one with two electrons. Applied to two sites, numbered 1 and 2, Eq. 13.23 is

c1†σ c2σ + c2†σ c1σ + U n1↑ n2↓ + n2↑ n1↓ . (13.25) H=t σ

The ﬁrst term allows an electron to hop from site 1 to 2 and from 2 to 1. The second term represents the cost of having the two electrons on the same site. There can also be a site energy En which I’ll take to be zero. I have two electrons and I can place them on either of the two sites and with either spin up or spin down. (I of course cannot place them both on the same site with the same spin.) An example basis state is |↑↓,00, where both electrons are on site 1, none on site 2. Another example, |↑ 0,0 ↓, has an up-spin electron on site 1 and a down-spin electron on site 2. There are a total of six possibilities: (a) two for double occupancy of one or the other site; (b) two with spins antiparallel and with one on each site; and (c) two for spins parallel and with one on each site. I could start with these, but it helps to form linear combinations that respect the symmetry of the system [307, 308]. So I write the following six basis states: 1 |a+ = √ (|↑↓,00 + |00,↑↓) 2 1 |a− = √ (|↑↓,00 − |00,↑↓) 2 1 |b+ = √ (|↑ 0,0 ↓ + |0 ↓,↑ 0) 2 1 |b− = √ (|↑ 0,0 ↓ − |0 ↓,↑ 0) 2 |cu = |↑ 0,↑ 0 |cd = |0 ↓,0 ↓ The states are normalized and orthogonal. I operate with the Hamiltonian of Eq. 13.25 on |a+ |a− , and |b+ : 1 H |a+ = √ t (|↑ 0,0 ↓ + |↑ 0,0 ↓ + |0 ↓,↑ 0 + |0 ↓,↑ 0) 2 1 + √ U (|↑↓,00 + |00,↑↓) 2 = 2t |b+ + U |a+ .

(13.26)

255

13.2 Electron–Electron Interactions 1 H |a− = √ t (|↑ 0,0 ↓ − |↑ 0,0 ↓ + |0 ↓,↑ 0 − |0 ↓,↑ 0) 2 1 + √ U (|↑↓,00 − |00,↑↓) 2 = U |a− . 1 t (|↑↓,00 + |00,↑↓ |↑↓,00 + |00,↑↓) H |b+ = + √ |b+ 2 = 2t |a+ . The remaining wave functions in Eq. 13.26 are already eigenfuctions, with energy E = 0. (If I had included the site energy, every diagonal term would have an additional 2En .) The Hamiltonian matrix is ⎛

a+ b+⎜ ⎜ a−⎜ ⎜ H= ⎜ b−⎜ ⎜ cu ⎝ cd

a+

b+

a−

b−

cu

cd

U 2t 0 0 0 0

2t 0 0 0 0 0

0 0 U 0 0 0

0 0 0 0 0 0

0 0 0 0 0 0

0 0 0 0 0 0

⎞ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎠

(13.27)

Thanks to the fact that I wrote linear combinations of the basic wave functions in Eq. 13.26, it is trivial to diagonalize Eq. 13.27. I have only the 2×2 part at the upper right to address, a result of mixing of the |a+ and |b+ states. The characteristic equation is U − E 2t = E 2 − U E − 4t 2 = 0 2t −E and the eigenvalues are E=

U 1 2 ± U + 16t 2 . 2 2

(13.28)

The negative sign corresponds to the energy of the ground state and the positive sign the energy of one (out of ﬁve) of the excited states. It is straightforward to ﬁnd the wave functions corresponding to these energies. The 2 2 ground-state wave function, with energy Eg = U/2 − U /4 + 4t , is |g =

1 4t 2 + Eg2

2t |b+ + Eg |a+ .

For the upper level, with high energy Eh = U/2 + |h =

1 4t 2 + Eh2

I leave it to you to show that g|h = 0.

(13.29)

U 2 /4 + 4t 2 , the wave function is

(Eh |a+ + 2t |b+ ) .

(13.30)

256

Strongly Interacting Solids

Both solutions contain an admixture of the two initial basis states. Their relative weights depend on the ratio of t to U . For U t, the ground-state energy is Eg = −4t 2 /U, slightly negative. The corresponding wave function is

2t |g = Cg |b+ − |a+ , U where Cg is for normalization.∗ The amplitude of the double-occupied term |a+ is small. The highest-energy excited-state in the large U limit has Eh = U + while

4t 2 U

2t |h = Ch |a+ + |b+ . U

with Ch another normalization factor. There is also a high-energy state with energy U and wave function |a− . I’ll return to this state in a moment. In the other limit, t U , Eg = −2t + U/2 and Eh = 2t + U/2. The wave functions become – in the case where U = 0 – just the bonding and antibonding states of the two-site molecule. The states |b− , |cu , and |cd all have total spin S = 1. These are the triplets, with energies ET = 0; their energy is between the singlet S = 0 ground state and the excited state energies Eh and U of the two other singlet states. I have not yet said much about the state |a− . This state is the one that is connected to the ground state by the electric-dipole matrix element, and hence the state that governs the dielectric function. If the vector joining site 1 to site 2 is a, then I write the dipole moment as ea ea p = − (n1 − n2 ) ≡ − δn 2 2 where ni = ni↑ + ni↓ is the number operator for site i. Now, δn |b+ = 0, because the two electrons are with equal amplitude on each site. However δn |a+ = 2 |a− , because |a+ is made up of states where there is double occupancy. Thus the dipole matrix element couples the ground state to state |a− . It is a charge-transfer excitation where an electron is transferred from one site to another; the energy of the excited state is U and the photon energy required to make the transition is (13.31) hω ¯ ct = U − Eg = U/2 + U 2 /4 + 4t 2 . ∗ I get C from requiring that g|g = 1. g

257

13.3 Electron–Phonon Interactions If U t, the energy difference is hω ¯ ct ≈ U , which is what I would expect in the strongly interacting case. For large U the dipole matrix element is 2t , U so that charge-transfer transitions are suppressed by the energy cost of double occupancy. The optical conductivity (or − c , with c the high-frequency “core” part of the dielectric function) is proportional to the square of this matrix element. Following Rice [307], I write it as a− |p|g ≈ ea

= c +

1 4π ne2 a 2 4t 2 , 2 h¯ U ωct − ω2 + iωγ

(13.32)

where n is the number density of molecules (not dimers), I took ωct = U/h, ¯ and I added by hand a ﬁnite line width γ to the charge transfer excitation.

13.3 Electron–Phonon Interactions 13.3.1 The Holstein Effect The temperature-dependence of the resistivity of simple metals is well understood as arising from electron scattering by thermally-generated phonons. In pure metals, the mean free path and scattering time τ can decrease by several orders of magnitude on warming from near zero Kelvin to room temperature. At ﬁrst, it is easy to imagine that the same decrease would be observed in the optical regime, at least for photon energies below the onset of interband transitions, say at midinfrared frequencies of a thousand cm−1 or 0.1 eV. This strong temperature dependence is not observed; instead, the optical measure of electron scattering ﬁnds a time τ considerably shorter than what one infers from DC resistance [310, 311]. The cause of the difference between DC and optical measures is explained by the Holstein model [92, 312–316]. In fact, both the frequency and temperature dependence of the optical conductivity can be described in this model. The interaction of the electrons with the phonons can be shown to depend on α 2 F (), the electron–phonon spectral density, a function of , the phonon frequency.∗ The overall electron–phonon coupling constant λ is given by ∞ 2 α F () d. (13.33) λ=2 0 Now, at DC (and very low frequencies) the only scattering processes available are the absorption of or scattering by a phonon, with a change of electron momentum and energy removed from the electric current density. The temperature dependence of the ∗ This spectral density is in fact the product of two things: a coupling constant α (which enters through its square)

and a density of states for the phonons F ().

258

Strongly Interacting Solids

resistance, therefore, is set by the number of thermally generated phonons (a Bose–Einstein distribution) combined with their momentum. Phonons with small momentum do not scatter electrons by very large angles. Above the Debye temperature, the entire acoustic branch is excited and [19, 98, 101] h/τ ¯ = 2π λkB T . At temperatures well below the Debye temperature, only low energy (and small momentum) phonons exist, and the resistivity is expected to follow T 5 . If, however, I turn the frequency up, another process can come into play: the electrons may also emit phonons. In this Holstein emission process, a charge carrier absorbs a photon of energy ω, emits an excitation of energy and momentum hk ¯ and scatters, giving rise to absorption. (The excitation is generally a phonon but in fact could be any boson that couples linearly to the charge carriers.) Momentum is conserved in the electron–phonon system; energy largely in the photon–phonon system. Only phonons with energy less than the photon energy play a role. These considerations lead to the following expression for the T = 0 electron–phonon scattering rate due to Holstein phonon emission [312], 2π ω 2 α F ()(ω − )d. (13.34) 1/τh (ω) = ω 0 A Holstein sideband due to electron–phonon coupling has been observed in the infrared spectra of conventional strong-coupling metals, such as lead [313–316]. Figure 13.5 shows an example of the effect in Pb. The ﬁgure shows the difference between the surface resistance in the superconducting state and the surface resistance in the normal state, Rs − Rn . There is a three times smaller scale below 26 cm−1 . The measurements are on an absolute scale and agree very well with the calculations by Shaw and Swihart [317], which are shown in the ﬁgure, and also with calculations by Scher [318] and Allen [312]. When the metal becomes superconducting and an energy gap appears in the excitation spectrum (shown in Fig. 11.7), the process also includes breaking a Cooper pair into its

Fig. 13.5

Holstein sidebands in Pb. After Ref. 314.

259

13.3 Electron–Phonon Interactions component electrons. Thus energy balance requires ω ≥ + 2 /h. ¯ All the phonon-related features are shifted up by the gap frequency. Such a shift is a pretty unambiguous proof that the Holstein effect is observed. The features in Fig. 13.5 are in accord with this picture. The step upward in Rs − Rn at 21 cm−1 occurs at the superconducting gap 2 . The smaller upward steps at about 55 and 90 cm−1 are respectively from the Holstein emission at the transverse and longitudinal phonon density of states maxima, shifted by 2 . The downward steps at 35 and 65 cm−1 are the Holstein emission in the normal state, which of course are unshifted. I’ll use a simple toy model to illustrate the phenomenon. Suppose my phonon spectrum consists of a single Einstein mode: F () = Dδ( − 0 ). I evaluate Eq. 13.33 ﬁrst to ﬁnd that λ = 2Dα 2 / 0 . Then Eq. 13.34 gives ! 0 ω ≤ 0 1/τh (ω) = (13.35) ω − π λ0 ω 0 ω ≥ 0 The scattering rate is strongly frequency dependent. I show a plot in Fig. 13.6. I used 0 = 200 cm−1 and λ = 0.5 or 2 for the calculations. The scattering rate turns on at the phonon frequency, rises smoothly and then ﬂattens out. The limiting high frequency value is 1/τh = π λ0 , comparable to the DC scattering rate at T = h ¯ 0 /2kB . In accord with the discussion in Section 13.1 of this chapter, the frequency-dependent scattering rate is accompanied by a frequency-dependent mass enhancement factor λ(ω); both must be included in calculating via Eq. 13.11 the conductivity [286]. Figure 13.7 shows the optical conductivity at low temperatures of a metal due to the Holstein emission process. I included a modest impurity scattering here, 1/τi = 10 cm−1 , and employed Matthiessen’s law: 1/τ = 1/τH (ω) + 1/τi . The inset shows the conductivity on a logarithmic scale. Below 0 , the conductivity has Drude form, falling to half its DC value at 10 cm−1 and falling like 1/ω2 above this frequency. Then, at 200 cm−1 , the phonon

Fig. 13.6

Phonon emission scattering rate due to coupling to an Einstein phonon at 200 cm−1 .

260

Fig. 13.7

Strongly Interacting Solids

Real part of the optical conductivity (normalized by the DC value) of a metal due to the Holstein emission process. emission processes begin. The scattering rate increases, but so does the conductivity. The reason is that the metal is in the high frequency limit, where σ1 ≈ ne2 /mw 2 τ , so an increase in 1/τ , or a decrease in τ , makes the conductivity bigger. As the frequency continues to increase and the scattering rate approaches its limiting high-frequency value, the conductivity begins to fall as 1/ω2 again, but now the width of the Drude-like spectrum is 314 cm−1 rather than 10 cm−1 . There are differences in details if I were to use a more realistic phonon spectrum. Typical metals have F () ∼ ω2 at low frequencies. There are two maxima in the density of states, one at the transverse zone-boundary frequency and one at the longitudinal zone-boundary frequency. The width of the F () softens the onset of the increase in 1/τ (ω) but the basic behavior is the same as in Fig. 13.7.

13.3.2 The Rice Effect Many materials, including linear-chain organic and inorganic conductors, electro-active polymers, fullerenes, and cuprates exhibit charge ordering, charge-density waves, or dimerized ground states.∗ The charge density wave is generally understood as being a Peierls transition [253]. The Peierls transition occurs on account of the electron–phonon interaction. A variation of charge occurs along the chain of molecules with a wave vector of 2kF . This charge density wave causes (or is caused by) a lattice distortion with the same wave vector. In consequence, the electron states get a zone boundary at ±kF , causing occupied states just below the Fermi wave vector to have their energies lowered (and empty states just above to have their energy raised). The empty states do not contribute to the total ∗ By “dimerized” I mean a system where two identical molecular units are in some way bonded to each other

more strongly than to other units in the solid. Other systems occur as trimers (three molecules) or tetramers (four); the Rice effect can occur in all these materials.

261

13.3 Electron–Phonon Interactions

energy but the ﬁlled states do; consequently the overall system energy is lowered. A gap occurs at the Fermi surface, rendering the material an insulator. If the molecules making up the solid have internal degrees of freedom or if there is a basis of atoms for the un-dimerized solid, then the infrared spectrum can display unusual phonon features that I like to call the “Rice effect” [307, 319–322]. Other names used for this effect are phase phonons, charged phonons, electron-molecular vibration (EMV) interactions, and infrared active vibrations (IRAV). The Rice effect is observed in organic linear-chain conductors [306, 323–326], polyacetylene [126, 327–330], doped C60 [331, 332], and possibly cuprate superconductors [333, 334]. I’ll discuss this in the context of the organic linear-chain conductors, where linear coupling of charge carriers to the totally symmetric (Ag ) phonons of the molecules leads to structure in the conductivity spectrum at the phonon frequencies. This mechanism occurs because the electron energies depend on the bond lengths while at the same time the bond lengths depend on the local charge density. Infrared radiation at the Ag phonon frequencies can pump charge over long distances, giving rise to absorption that can approach electronic oscillator strength and that is polarized in the direction of easy electronic motion. This direction is in the quasi-one-dimensional stacking axis in the organics, which nearly is perpendicular to the planes of the molecules. (The Ag modes are normally infrared inactive and their normal modes are in the plane of the molecule. Thus, the Rice effect causes infrared features from the “wrong” modes, with the “wrong” polarization, and with the “wrong” oscillator strength.) The Rice effect is responsible for the narrow peaks in the spectrum of Fig. 13.4. When the electronic continuum overlies the phonon frequencies, characteristic Fano lineshape antiresonances occur in the continuum spectrum. As an example, Fig. 13.8 shows the optical conductivity [326] of the quasi-onedimensional organic semiconductor N-dimethyl thiomorpholinium(TCNQ)2 . This spectrum was measured with the electric ﬁeld vector polarized along the c crystallographic axis, which is the stacking axis or the chain axis of the TCNQ molecule and also the most highly conducting direction. The spectrum has an electronic excitation at ωe ≈ 3,200 cm−1 and a second (not shown at ≈ 10,500 cm−1 . The mid-infrared band contains a majority of

Fig. 13.8

Optical conductivity of semiconducting N-dimethyl thiomorpholinium(TCNQ)2 .

262

Strongly Interacting Solids

the oscillator strength. These charge-transfer absorptions are attributed to the transfer of charge between TCNQ molecules in the stack [335–337] and can be understood in terms of strong Coulomb interactions using an extended Hubbard model with both a large on-site interaction U and a only somewhat weaker next-nearest-neighbor interaction V . At low frequency, the spectrum displays many sharp vibrational features. Ten of these modes are Ag vibrations of the TCNQ molecule, activated by coupling to the charge transfer excitations [319,320,326,335]. These phonon features in the conductivity generally take on the appearance of a derivative of the ordinary Lorentz oscillator phonon absorption, known as a Fano lineshape. The Rice effect leads to the following dielectric function: (ω) = c + · · · +

4π χ e (ω) , 1 − D0 (ω)χ e (ω)/χ 0

(13.36)

where c is the high frequency dielectric constant, · · · represents other contributions (interband transitions, ordinary optical phonons, and non-interacting free carriers, for example), and the last term is the effect of the Rice effect phonons. In it, χ e is the electronic susceptibility of the carriers in the absence of coupling, χ 0 is the zero-frequency susceptibility, and D0 is the phonon propagator: D0 (ω) =

α

λα ωα2 , ωα2 − ω2 − iωγα

(13.37)

with λα the dimensionless electron–phonon coupling constant, ωα the unperturbed frequency, and γα the width of the αth phonon mode. The total dimensionless electron–phonon coupling constant is λ = α λα and the usual electron–phonon coupling function α 2 F (ω) is related to D0 by α 2 F (ω) = π −1 Im D0 (ω).

14

Nonlocal Effects

Ohm’s law is local: the current j at location r depends on the electric ﬁeld at location r and not on the ﬁeld anywhere else. In pure metals at low temperatures the response to the ﬁeld becomes nonlocal. The current at location r depends on ﬁelds at other locations r . This nonlocal response is not unusual. Anyone who has played shufﬂeboard (or hockey) knows that the puck will slide considerable distance away from the location where the force was applied to it. The principal optical consequence of nonlocality is the anomalous skin effect. I’ll ﬁrst review the normal skin effect, already introduced in Chapter 4 (Section 4.5.2). Then I’ll discuss the conditions necessary for the appearance of nonlocal effects and make a simple argument of how to calculate the skin depth in the nonlocal regime.

14.1 The Normal Skin Effect Recall Eqs. 4.38 and 4.39, which specify the penetration depth of a metal. The amplitude of the ﬁeld decays with distance along the path of the light as e−x/δ , with κω/c = 1/δ. At low frequencies, ωτ 1, I found c2 2 c c ≈ , δ= = ωκ 2π ωσdc ωp ωτ where σdc = ωp2 τ/4π . In the other limit, high frequencies, ωτ 1, and the penetration depth becomes c . δ≈ ωp This length, c/ωp , is as short as the penetration depth gets. The skin effect is not only an optical effect. It also affects electrical currents in wires carrying high-frequency∗ signals. Figure 14.1 shows the ﬁeld or current distribution ﬂowing in a wire with circular cross section. The current density is high near the surface and falls exponentially to near zero in the center. Figure 14.2 shows the room temperature skin depth for several metals at frequencies from 1 Hz to 10 THz. Lines are shown for metals with a range of conductivities: good metals (Ag, Cu, Au), fair metals (Pd, Pt, Ta), ∗ Or any frequency. Even at 60 Hz, good conductors have a ﬁnite penetration of ﬁelds and currents. The skin

depth in copper is about 1 cm at 60 Hz and 300 K.

263

264

Nonlocal Effects

Fig. 14.1

The current in a conductor carrying an alternating current. The current flows only near the surface, dying out exponentially towards the center.

Fig. 14.2

Room-temperature classical skin depth as a function of frequency for metals with a range of conductivities or resistivities, varying from 300 μ-cm (YBa2 Cu3 O7 ) to around 2 μ-cm (Ag, Cu, Au) with Pd, Pt, and Ta (ρ ≈ 10 μ-cm) in the middle. The frequency range is 1 Hz–10 THz. Note that 10 THz == 333 cm−1 . and a “bad metal” (YBa2 Cu3 O7 ). The skin depth decreases (very approximately) from 10 cm to 100 nm over these frequencies. Note that 1 THz is 33 cm−1 or about 4 meV. On this many-decades plot, the differences among metals whose conductivity varies by less than ±50% is not large. The classical skin depth formula, Eq. 4.38, is valid at low frequencies (ω 1/τ ). As frequency increases, one must use the exact expression, δ = c/ωκ, which is easy enough if one knows the complex dielectric function. Figure 14.3 shows the skin depth for silver in the radio-frequency to ultraviolet range, 3 MHz to 1.2 PHz, 10−4 cm−1 to 40,000 cm−1 , or just over 10−8 eV to 5 eV.∗ This range includes ωτ = 1, so the skin depth initially ∗ The calculation does not make an approximation for δ. The dielectric function model consists of a Drude

free-carrier part, plus Lorentz oscillators above 4 eV to account for the contribution of the d electrons. I then √ calculated , followed by N = n + iκ = and δ = c/ωκ.

265

Fig. 14.3

14.1 The Normal Skin Effect

Classical skin depth for silver from RF to uv frequencies at 5 temperatures. Three frequency/energy scales are given. The curves shown with dashed lines are not realistic; silver would be in the anomalous skin effect regime and not the classical regime over much of the frequency range.

√ falls as 1/ω before ﬂattening out in the high frequency limit, at δ ≈ c/ωp according to Eq. 4.39. There is a signiﬁcant increase in the skin depth near the plasma minimum. This rise is due to the sign change of at this frequency and a corresponding decrease in κ. Then, for silver, the interband transition from the d levels turn on, and the classical penetration depth decreases again. At room temperature, the high frequency skin depth is comparable to the 40 nm mean free path. It is much larger that the mean free path at frequencies below 1/τ . However, as temperature is reduced, the conductivity increases (because the mean free path is getting longer and longer), making the skin depth (Eq. 4.38) shorter and shorter. I have included in Fig. 14.3 the classical skin depth for silver assuming the conductivity varies as in Fig. 8.6. It does not take long in the case of silver and other good conductors to get into a situation where the mean free path is much larger than the skin depth. The mean free path is the length scale (just as the relaxation time is the time scale) for relaxation of the current. But if the mean free path is larger than the skin depth, then those electrons moving at angles to the surface see an electric ﬁeld which varies enormously over the trajectory. Electrons moving parallel to the surface see a constant ﬁeld. This situation is illustrated in Fig. 14.4. The current is a complicated and nonlocal response to the ﬁeld. The dashed curves for temperatures in the 10–100 K range in Fig. 14.3 do not apply to this physical situation.

266

Fig. 14.4

Nonlocal Effects

The electric field of light which is incident on the surface of a clean metal accelerates the electrons that are within the skin depth. Two electron trajectories are shown. One has the electron staying within the skin and seeing the external field over its entire mean free path. The second shows the electron going into the depths of the metal. Each mean free path starts and ends with a momentum-changing collision.

14.2 The Anomalous Skin Effect This anomalous skin effect was studied in the 1950s by Pippard [338], Chambers [339], and many others. As I will discuss, the physical situation is: 1. δ = δcl . 2. δASE > δcl . 3. The current is nonlocal, so Ohm’s law becomes a convolution of the form j(r) = (r − r )E(r )d 3 r V

(r − r )

where is the Fourier transform of σ (q,ω) with hq ¯ a momentum. 4. The ﬁelds are q dependent with q ≈ 1/δASE . In the anomalous skin effect regime, the effect of an external ﬁeld on a speciﬁc electron state k depends on how k is oriented relative to the surface. Two distinct electron trajectories are shown in Fig. 14.4. Each electron starts off immediately after a collision and travels for the mean free path before another collision occurs. The electrons are accelerated by any electric ﬁeld as they move along their trajectories. The electron whose path is entirely within the skin feels this force over its entire trajectory. (The ﬁeld does work during the entire time that the electron is ﬂying free between collisions; the work gives energy to the electron and causes it to contribute to the electric current. At the collision, the electron motion is randomized and no longer contributes to the current.) In contrast, the electron that departs deep into the metal only sees the ﬁeld for part of its total free path. The ﬁeld therefore does less work on this second electron.

267

14.3 The Extreme Anomalous Limit

14.3 The Extreme Anomalous Limit The concepts in the previous paragraph form the basis of Pippard’s effectiveness concept for the skin effect. The electric ﬁeld amplitude decays from the surface with a length δ. The decay occurs because energy is absorbed by the electrons. To be most effective, the entire trajectory must be where the ﬁeld is ﬁnite, i.e., within the skin. The path length is the mean free path . When δ, this requirement restricts the angle of the k to a small value relative to the surface. The “effective” number of electrons is smaller than the total number: δ (14.1) neff = n. The metal then acts as if the current is only carried by the effective electrons∗ neff e2 neff e2 τ = m mvF where I have used τ = /vF . Now replace neff using Eq. 14.1: σ eff =

ne2 δ . mvF I now calculate the skin depth self consistently: c c = δ ASE = √ 2π σeff ω 2 ω 2π nemvδASE F σ eff =

(14.2)

where I have substituted using Eq. 14.2. Square both sides, multiply by δASE , and take cube root to ﬁnd 1/3

2 c mvF δ ASE = . (14.3) 2π ne2 ω The skin depth in the extreme anomalous regime goes as ω−1/3 compared to ω−1/2 in the normal skin regime. If I use the deﬁnition of the plasma frequency, Eq. 8.23, I can recast this for comparison with Eqs. 4.38 and 4.39:

c 2vF 1/3 ωp 1/3 . (14.4) δ ASE = ωp c ω The plasma frequency, ωp , appears twice in Eq. 14.4; I put the c/ωp factor in front to allow comparison to the normal skin effect formulae. Two cube roots follow this scale factor. The ﬁrst cube root is smaller than unity† but the second is much larger than unity. The plasma frequency is 70,000 cm−1 or 9 eV whereas the frequency is smaller than 1/τ = 0.1 cm−1 or 10 μeV in pure metals‡ at low temperatures. ∗ I write the conductivity as a DC conductivity. Hence, this picture is a low frequency, ω 1/τ , picture. The

high frequency penetration length c/ωp is a kinetic inductance or inertial effect and does not depend on the mean free path. † Recall: v = c/200. F ‡ The anomalous skin effect only occurs in pure metals at low temperatures.

268

Fig. 14.5

Nonlocal Effects

Skin depth for silver from RF to uv frequencies at 5 temperatures. Three frequency/energy scales are given. The extreme anomalous limit is shown as a solid line. The skin depth calculated from the classical equation is shown with dashed lines where it is incorrect. Below the frequency where the classical and anomalous skin effect curves cross, silver is in the classical regime. None of the terms in Eq. 14.3 have any signiﬁcant temperature dependence; consequently, neither does δASE . The temperature-dependent family of curves calculated for the normal skin effect will all merge into a single, frequency-dependent curve at low temperatures. This behavior is illustrated in Fig. 14.5, where I show the classical skin depth for silver in the optical range, 3 MHz to 1.2 PHz, 10−4 cm−1 to 40,000 cm−1 , or just over 10−8 eV to 5 eV. The anomalous limit (which is temperature independent) is shown as a black solid line. With increasing frequency the skin depth passes from classical to anomalous and then back to a high-frequency relaxation regime as ω∼1/τ . At the lowest temperatures, the crossover is at 70 kHz.

14.4 ω–τ Plot The anomalous regime has both a high-frequency and a low-frequency boundary. The lowfrequency boundary occurs where the anomalous skin depth equals the normal skin depth and also equals the mean free path: δASE = δcl = . If δ = , then all electrons are effective. I can calculate the frequency where the transition occurs by setting = δcl to ﬁnd 1/2 c2 2 = vF τ = ωp2 ωτ

14.4 ω–τ Plot

269

or ω=

2c2 2c2 vF = . 3 ωp2 τ 3 vF2 ωp2

(14.5)

This is also the frequency where δcl = δASE . Equation 14.5 represents a boundary between the normal skin effect (low ω or short τ ) and the anomalous skin effect (higher ω or long τ ). Both of these boundaries are computed in the low-frequency limit, ω 1/τ . Once the frequency increases enough that ω 1/τ , both normal and anomalous skin effects are modiﬁed. In this high frequency region, the ﬁeld oscillates many times, accelerating and decelerating the electron each cycle until it has a collision. This relaxation regime in the local limit is where ω 1/τ , σ1 σ2 , and δcl = c/ωp , (Eq. 4.39). As the mean free path becomes longer than the skin depth, many electrons will enter the skin, be accelerated and decelerated each cycle of the ﬁeld, collide once with an impurity or the surface, and exit the skin. The dissipation in this “anomalous relaxation” regime is less than when the mean free path is short, but the differences in the values of the skin depth in the local relaxation and anomalous relaxation regimes are small.

Fig. 14.6

Roadmap [340] of the skin effects in the ω–τ plane. The materials parameters used are those of silver or copper. The roadmap frequency scales are THz and cm−1 (bottom) and meV (top); the interesting range is 1–1,000 cm−1 , .03–30 THz, or 0.1–100 meV. Note that the angular frequency ω is found by multiplying the frequency in Hz by 2π or the frequency in cm−1 by 2π c.

270

Fig. 14.7

Nonlocal Effects

Sketch [340] of electron trajectories in region A (normal skin effect), region B (relaxation regime), region D (anomalous skin effect), and region E (anomalous relaxation). Figure 14.6 shows a roadmap [340] of the skin effects in the ω–τ plane. The horizontal axis is the frequency ω while the vertical axis is the scattering time τ . The materials parameters used are those of silver or copper. For low frequencies and short mean free paths (high temperatures), one is in the normal skin regime (Region A). If the mean free path (and relaxation time) get longer and longer, one eventually crosses the boundary given by Eq. 14.5 and is in the anomalous skin regime (Region D). If instead, I keep τ short but increase the frequency, I enter the relaxation regime, (Region B) unless τ is really short, in which case the metal becomes partially transparent (Region C), because 1 is positive.∗ At high frequencies and in clean metals the relaxation regime and the anomalous skin effect regimes cross the boundary into the anomalous relaxation regime (Region E). Finally, once ω > ωp /c , the metal is partially transparent. Figure 14.7 shows [340] electron trajectories in four of the ﬁve regimes. (In Region C the skin depth is very large, so that the trajectories are as in A.)

14.5 The Surface Impedance I want to ﬁnd a material-related function to describe the optical properties of a nonlocal system. Of course, it should be also deﬁned and reasonable for the local limit where Ohm’s law is valid. Moreover, it should be related to observables such as the absorption or reﬂectance. The skin depth is such a quantity but it speciﬁes the behavior of the ﬁelds inside the metal. I would like something that can be related to measured quantities outside ∗ Write = − ω2 /(ω2 + 1/τ 2 ) = 0. If 1/τ is a large frequency, the zero of is well below the usual c 1 1 p 2 τ 2 can be everywhere positive. ω = ωp /c . In fact, it may not exist at all; for a really dirty metal, 1 = c − ωp

271

14.5 The Surface Impedance the metal. The surface impedance Z = R + iX is one such measure. As I will discuss, its real part, the surface resistance R, is related to loss in the metal and the surface reactance, X, to dispersion. I’ll start by reminding myself of the resistance and reactance of an electrical circuit. At zero frequency (DC currents), the resistance is given by freshman physics (Ohm’s law No. 2): R = V /I where V is the voltage drop of the circuit and I is the current passing through it.∗ At ﬁnite frequencies, I must replace the real R with a complex Z. Now, if the current is organized into a surface sheet, with surface current K, then the same law is [2] Z = E/K. The skin is such a sheet, except that the current is not in an inﬁnitesimally thick layer but in a layer a few times the skin depth thick. Then† ∞ K= j (x)dx 0

and E(0) , Z = "∞ 0 j (x)dx

(14.6)

where E(0) is the ﬁeld at the surface. Wherever the normal skin effect is in effect, I can use Ohm’s law j = σ E. I also know that the ﬁeld goes as E = E(0)e−x/δ . Then Z=

E(0) "∞ . σ E(0) 0 e−x/δ dx

(14.7)

The integral is easy to do; it integrates to −(δ)e−x/δ . This contributes zero at the upper limit and δ at the lower limit. Hence 1 . (14.8) Z= σδ At low frequencies, σ = σ 1 = σdc and the surface impedance is real: R = 1/σ dc δ is the resistance of a slab of metal with thickness δ and equal length and width. This is often called the square resistance or the sheet resistance R . At higher frequencies, both σ and δ are complex, and thus so is Z. Using Eq. 4.38 I ﬁnd (low frequencies!) 2π ω when ω 1/τ . (14.9) Z= σ dc c2 The surface impedance grows as ω1/2 and decreases if the conductivity increases.‡

.. ∗ #1: V = I R; #3: I = V /R. † Fields and currents are vectors, but if I take the ratio of two of these, I must take the magnitudes. For isotropic and homogeneous materials, the current and electric ﬁeld are in the same direction so I just take ratios of the amplitudes. ‡ But only as the square root of the conductivity. At DC the resistance decreases linearly in the conductivity.

272

Fig. 14.8

Nonlocal Effects

Geometry for calculating the surface impedance. The four numbered line segments will be where I convert a surface integral to a line integral. Segment 3 is deep enough that the field is zero at its location. The yˆ axis, E, and j are into the plane of the figure.

14.5.1 The General Case (At Low Frequencies) At frequencies low enough that I can neglect the inductive response (because σ 1 σ 2 ) and the displacement current, Maxwell’s fourth equation (Eq. 2.4d), is ∇ ×H=

4π j. c

(14.10)

Now look at the geometry of Fig. 14.8. The electromagnetic wave of frequency ω is incident from the left, with q normal to the surface, H in the plane of the paper, and E into ˆ and hˆ respectively along the x, y, and z Cartesian the paper. As usual, I will take q, ˆ e, axes. After the wave crosses the surface, it will decay with a skin depth δ (equation for and magnitude of to be speciﬁed). The current j (which also decays with decay length δ) is into the plane of the paper, parallel to E. A rectangular surface is shown outlined in red. It is bounded by 4 line segments: 1 , 2 , 3 , and 4 . 3 is very many skin depths below the surface, where ﬁelds are zero. ˆ dx So I will integrate Eq. 14.10 over the area of this surface using dS = ydz 4π dS · j. c S 4π = dz dx yˆ · j. c

dS · ∇ × H = S

Using the deﬁnition of Z, Eq. 14.7, I can evaluate easily the right-hand side:

4π E(0) dz c Z 4π E(0) L1, = c Z

dS · ∇ × H = S

273

14.5 The Surface Impedance

where L 1 is the length of line segment 1 . But also I can transform the surface integral on the left side to a line integral around the perimeter of the surface S using Stokes theorem! It becomes ) dS · ∇ × H = H · dl S dz H (0) + dx H · xˆ = 1 2 dz H(x→∞) − dx H · xˆ − 3

4

= H (0)L 1 . Here, the differential vector dl runs clockwise around the perimeter, following 1 . . . 4 . The dot product of H and dl makes the integrals 2 and 4 zero; the magnetic ﬁeld H is zero along 3 . Hence, the surface impedance is Z=

4π E(0) , c H (0)

(14.11)

the ratio of the electric ﬁeld at the surface to the magnetic ﬁeld at the surface.

14.5.2 Impedance of Free Space Suppose I replace the metal with vacuum. The ﬁelds are still deﬁned in any y–z plane. In vacuum E = H so the impedance of free space is∗ Z0 =

4π = 377 . c

(14.12)

14.5.3 Fields at the Surface I’ll start by looking back at the discussion of normal-incidence reﬂection in Chapter 3, Section 3.6. I know that the electric ﬁeld is reversed on reﬂection (because the metal is ˆ the reﬂected ﬁeld is along the more dense medium). Thus, with the incident ﬁeld along y, ˆ The reﬂectance is nearly 100% in good metals, so the resultant ﬁeld is 1 − (−r) with −y. the amplitude reﬂectivity r given in Eq. 3.32.† Because the E ﬁelds are antiparallel, the H ﬁelds are parallel, adding to 1 + (−r), larger than then incident H ﬁeld by almost a factor of two. Thus the surface impedance is much smaller than 377 . Indeed, from above I get Z=

4π 1 + r c 1−r

with r = (1 − N )/(1 + N ). (r < 0.) Substituting, I ﬁnd Z=

4π 1 . c N

(14.13)

∗ See Appendix A. † r is negative (the ﬁeld is reversed) so I write it as 1 − (−r) to indicate a difference between unity and a number

just above −1, e.g., −0.99. The difference is 0.01.

274

Nonlocal Effects

But I knew this! The magnitude of the magnetic ﬁeld inside the metal (or any local, nonmagnetic, linear, homogeneous, and isotropic material) is H = N E. The tangential components are continuous at the interface, so the ﬁelds at the surface are the same as the ﬁelds just inside the metal.

14.5.4 Back to the Dielectric Function √ √ Because N = , I can write Z = (4π/c) 1/. Moreover, I can write = c + 4π iσ /ω and at low frequencies (compared to ωp ) neglect c and obtain ω 4π Z= . (14.14) c 4π iσ √ √ Now 1/ i = (1 − i)/ 2, so I can also write 2π ω Z = R + iX = (1 − i) . (14.15) c2 σ At low frequencies σ ≈ σdc and δ = δcl and∗ R = −X =

1 . σdc δcl

14.5.5 The Surface Impedance in the Anomalous Regime The same approach works for the anomalous skin effect: R=

1 , σ eff δASE

with σ eff = ne2 δASE /mvF and δASE = (c2 mvF /2π ne2 ω)1/3 . Note that δASE comes in twice, once directly and once replacing the mean free path in σ eff . Then

2/3 mvF 2π ne2 ω R= , ne2 c2 mvF or, after some algebra

R=

(2π )2 mvF ω2 ne2 c4

1/3 .

So the anomalous-limit surface impedance goes as ω2/3 . It can be rewritten as: v 1/3 ω 2/3 F , R = Z0 4c ωp

(14.16)

(14.17)

with Z0 = 4π/c = 377 , according to whether you want cgs or SI units. ∗ Consider a thin ﬁlm with thickness d δ. Then the currents are conﬁned to a distance d not a distance δ, and

Z=

ρ 1 = ≡ Z . σd d

275

14.5 The Surface Impedance

14.5.6 Reflectance in Terms of the Surface Impedance According to Eq. 3.33 the reﬂectance is 1 − N 2 . R = 1+N Now N = Z0 /Z so

Z − Z0 2 . R= Z + Z0

(14.18)

Eq. 14.18 is very familiar to the discussion of energy ﬂow in waveguides and coaxial transmission lines. It says that a discontinuity in the line impedance causes a reﬂection in the line. The most extreme discontinuity is a short circuit (Z = 0) or an open circuit Z = ∞); both give 100% reﬂection.

14.5.7 Numerical Values I use as an example the classical surface impedance (Eq. 14.15) with σdc = 6 × 105 −1 cm−1 at 300 K. If the frequency is ω = 1010 s−1 (0.05 cm−1 ), then R = 4 m . Compare this very low value with the impedance of free space, Z0 = 377 . The metal looks like a short circuit. Just as a shorted transmission line reﬂects the signals sent down it, the metallic surface is an excellent reﬂector.∗ Indeed, I can rewrite Eq. 14.18 as R = 1 − 4Z/Z0 ∼ 1 − 10−5 .

∗ I ﬁnd this transmission line analogy very useful in understanding why a high absorber is also a high reﬂector.

The short circuit ought to draw very large currents and dissipate lots of power. It does not. Instead, it returns the electromagnetic energy back toward the source.

15

Anisotropic Crystals

15.1 Optics of Crystals The study of anisotropic materials, the subject of this chapter, is often called “crystal optics,” because many crystalline solids exhibit anisotropic properties. In fact, only one of the seven systems known to crystallography, the cubic crystal system, has isotropic optical properties. I’ll deﬁne an anisotropic material as one having properties that depend on direction. “Direction of what?” is a fair question when faced with the deﬁnition I just gave. The answer: it is essentially always the direction of the electric ﬁeld which controls wave propagation, charge transport, and optical absorption. Despite the large numbers of anisotropic crystals, anisotropic materials are not widely experienced in everyday life. Many persons have seen or used “polaroid,” plastic polarizing ﬁlms [341]. These polarizing ﬁlms are used as sunglasses and in photography; these devices are not single crystals but they are anisotropic. Polaroid sheet contains linear chains of absorbing molecules in a transparent polymer host. It absorbs light with linear polarization parallel to the chains and has maximum transmission for light with polarization rotated by 90◦ . Research life differs from everyday life. Many of the solids that have attracted the most attention in condensed-matter physics over the past several decades are anisotropic. The list includes cuprate superconductors, Fe-based superconductors, certain topological insulators, organic linear-chain conductors, electroactive polymers, graphene, graphite, carbon nanotubes, and others.

15.2 Polarized Light Looking around in textbooks or on the Internet, I sometimes encounter statements like the following: “A polarizer is an optical device that passes light of a speciﬁc polarization and blocks waves of other polarizations.” This statement is (at best) incomplete: the polarizer will block (by absorption, by refraction out of the beam, or by reﬂection) light with its electric ﬁeld directed along one speciﬁc axis.∗ It will transmit more or less of the light in all other polarizations, with maximum transmission for light polarized perpendicular to the ∗ In real polarizers the blockage is rarely 100%; however, the leakage can in the best cases be only a few parts

per million.

276

277

15.2 Polarized Light

direction of blockage. Because the superposition principle applies to these ﬁelds, the light incident on the device can be treated as a superposition of two orthogonal ﬁeld directions: one is parallel to the blocking direction and the other is perpendicular to it. The transmitted beam is this second component.

15.2.1 Linear Polarization It should come as no surprise that I now assert that the electromagnetic waves I introduced in Chapter 2 are linearly polarized waves. The ﬁelds point in speciﬁc directions, unchanged as the waves propagate. I’ll take the electric ﬁeld direction as representing the plane of polarization. The plane-wave solutions are given by Eqs. 2.5 and 2.6; the direction of the electric ﬁeld for waves in vacuum was deﬁned right after Eq. 2.9 as eˆ for the electric ﬁeld and hˆ for the magnetic ﬁeld, with eˆ · hˆ = 0. A cartoon of the ﬁelds may be seen in Fig. 2.1. The ﬁelds for waves in local, nonmagnetic, linear, isotropic, and homogeneous media are the solutions to Eqs. 3.3a–3.3d, written as a polarized plane wave in Eq. 3.11. To be speciﬁc, let me orient the propagation vector q along the x axis and the electric ﬁeld along the y axis. My linearly-polarized plane wave is then ˆ i (qx−ωt ), E = E0 ye

(15.1)

where E0 is the (complex) amplitude of the ﬁeld.

15.2.2 Unpolarized Light It is easy to write a formula for linearly polarized light. It is not so easy to write one for unpolarized light. Suppose I try to add a second ﬁeld, at right angles to the ﬁeld in Eq. 15.1, thinking that I will then have the ﬁeld along both y and z, which would seem to ﬁll the bill of having the ﬁeld along no single axis. The second ﬁeld is E2 = E0 zˆ ei (qx−ωt ) .

(15.2)

If I add the ﬁelds in Eqs. 15.1 and 15.2 I get the sum to be √ ˆ i (qx−ωt ), (15.3) Es = E0 (yˆ + zˆ )ei (qx−ωt ) = 2E0 ee √ ˆ with eˆ = (yˆ + zˆ )/ 2. The sum is still linearly polarized; the direction of polarization (e) ◦ is at 45 to the y and z axes. The superposition of the two linearly polarized beams has produced another linearly polarized beam. So what is “unpolarized light” and how do I write the ﬁelds for it? Let me start the answer by saying that the linearly polarized ﬁelds in Eqs. 15.1–15.3 are perfectly coherent. I can delay one or the other by seconds or years or even the age of the Universe and still ﬁnd coherent superposition because the frequency and wavelength are unvarying.∗ Unpolarized light consists of the superposition of uncorrelated ﬁelds oriented in random directions. (The ∗ No actual source exists with coherence times of years, much less the age of the Universe. The initial LIGO laser interferometer had coherence times of 2×105 s, about two days [342]. More typical values for very stable

lasers are a few milliseconds.

278

Anisotropic Crystals

Fig. 15.1

Right circular polarized waves. The red cosine wave is the yˆ component while the blue sine wave is the zˆ component. The resultant is a green helix that rotates once per wavelength. ﬁelds are perpendicular to the propagation direction, of course.) There is enough variation in frequency that there is no coherent superposition of the constituent ﬁelds. The ﬁelds may also be partially polarized, in which case a polarizer ﬁnds power variations as it is rotated through 180◦ but not to zero at any orientation. I can represent partially polarized light as a superposition of unpolarized light and perfectly polarized light. The method of writing unpolarized and partially polarized light uses Stokes vectors and Mueller matrices [2, 343, 344], 4×4 matrices acting on 4-element vectors. This approach does the job, but is more than needed here. From the point of view of understanding, measuring, and interpreting the optical properties of solids, I can employ the perfectly polarized light introduced above.

15.2.3 Circular Polarization Photons have helicity; the two possible states are ±h¯ and correspond to circularly polarized light. Circular polarization is the sum of two linearly polarized ﬁelds shifted in phase by 90◦ . See Fig. 15.1. I write E± = E0 (yˆ ± i zˆ )ei (qx−ωt ),

(15.4)

where the minus sign is for right circular polarization and the plus is for left circular polarization.∗ I’ve said that the observable is the real part of the complex ﬁeld. It is worth writing the real part of Eq. 15.4: E± = E0 [yˆ cos(qx − ωt) ∓ zˆ sin(qx − ωt)].

∗ There are two conventions in use. These are generally described by saying that you put your right or left thumb

along the direction of the wave the ﬁngers then point in the direction of rotation of the corresponding circular polarization (right or left). The problem is that sometimes the thumb points towards the source of the radiation and sometimes away. I have used the second convention.

279

15.3 Crystal Symmetry

The electric ﬁeld vector of the circular polarized wave at ﬁxed time follows a helical path along the direction of propagation. circular polarization Plane polarized light can be written as a sum of equal amplitudes of right and left circularly polarized light at various relative phases. If the relative phase is zero, I add them as 1/2(yˆ

ˆ + i zˆ ) + 1/2(yˆ − i zˆ ) = y,

to get polarization along the x axis with unit amplitude. If the relative phase is π , 180◦ , then I add them as 1/2(yˆ

+ i zˆ ) + 1/2(yˆ − i zˆ )eiπ = 1/2(yˆ + i zˆ ) − 1/2(yˆ − i zˆ ) = i zˆ .

(To avoid shifting the phase of the plane polarized light, I would need to retard the phase of the left circular polarization by 90◦ and advance the right by the same amount.) In general, a phase difference of φ rotates the plane of polarization by θ = φ/2.

15.2.4 Elliptical Polarization Looking up or down the beam, the E ﬁeld of plane polarized light is a line along the polarization direction. The E ﬁeld of circular polarized light is a circle. Elliptical polarized light is a linear combination of plane and circular polarizations. Looking along the beam, the E ﬁeld of elliptical polarized light traces an ellipse. The ratio of major to minor axis of the ellipse is set by the ﬁeld strengths of the plane and circular constituents.

15.3 Crystal Symmetry Symmetry is a fundamental concept in physics. The basic idea is that any physical system which is unchanged – the correct word is “invariant” – under some operation will have observables that must respect the symmetry. Mathematically, the symmetry operations deﬁne a mathematical group; group theory [28, 29] is the mathematical theory of these groups and their manipulation. Most books on solid-state physics cover crystal symmetry. I particularly like the discussion by Burns [23] but Kittel [24] and Ashcroft and Mermin [19] are also good.

15.3.1 Translational Symmetry Translational symmetry is the basic symmetry that deﬁnes a crystal. Each crystal structure can be constructed by starting at some point in space and moving by the translation vector (actually a set of vectors) that deﬁnes the crystal to generate all the points of the crystal lattice. For example, I can deﬁne the NaCl lattice by starting at the center of an Na atom and then moving by a translation vector to the center of a neighboring Na atom, then by a translation vector to the center of another Na atom, and so on. Now, if I move to the nearest Cl atom, the same set of translation vectors will trace out all the Cl atoms in the crystal.

280

Fig. 15.2

Anisotropic Crystals

A sketch of a face centered cubic lattice (for a monatomic crystal), showing the primitive translation vectors (red) and the conventional translation vectors (blue). The translation vector is usually written as T = na + mb + pc where n, m, and p are (positive and negative) integers and the vectors a, b, and c deﬁne the unit cell of the crystal. The set of points deﬁned by T as the integers run over the range from minus to plus inﬁnity is known as a Bravais lattice. The name is that of French crystallographer Auguste Bravais (1811–1863), who proved that in three-dimensional space only fourteen distinct lattices may be constructed. To each point of the Bravais lattice one attaches a basis of atoms. (The attachments is done in an identical fashion for each point in order to preserve translational symmetry.) The basis in the example above is one Na and one Cl atom. Note that there are usually two ways to set up the vectors a, b, and c. In one, they are the “primitive vectors,” the smallest vectors possible; therefore, they reach every point in the Bravais lattice. The second way uses the conventional vectors. These deﬁne a unit cell which is larger than the primitive cell; however, the conventional cell generally clearly exhibits the symmetry of the lattice. The difference is perhaps best illustrated with an example. Figure 15.2 shows a face-centered cubic (fcc) lattice. The primitive vectors go from the origin at the front bottom corner of the cube across the three adjacent faces to the atoms – nearest neighbors all – in the centers of the faces. The conventional vectors go from the origin along the cube edges to the second-neighbor atoms at the adjacent corners. If the primitive vectors are used, all the points of the Bravais lattice will be reached. If the conventional vectors are used, only a fraction are reached by movements by T; the other points are assigned to the basis of the structure. There are four atoms in the basis in the conventional fcc cell. Although the need to deﬁne a basis even in monatomic crystals seems like an added complication, the conventional cell is much easier to visualize and to use to illustrate the crystal symmetry; consequently, I’ll use the conventional cell. The vectors a, b, and c deﬁne a rectangular prism with edges of length a, b, and c; there are angles α, β, and γ deﬁned respectively in the following way. α is the angle between b and c. β is the angle between c and a. γ is the angle between a and b.

281

Fig. 15.3

15.3 Crystal Symmetry

The seven crystal systems.

15.3.2 Seven Crystal Systems Every crystal belongs to one of seven crystal systems. Each system is deﬁned in terms of the relative lengths of the unit vectors a, b, and c of the lattice unit cell, as well as the angles between these vectors. The seven crystal systems are cubic, tetragonal, orthorhombic, monoclinic, triclinic, hexagonal, and trigonal. They are illustrated in Fig. 15.3. Cubic. I start with the system with the highest symmetry: cubic. The cubic crystal has all axes equal (a = b = c) and all angles 90◦ . The rectangular prism of the cubic system is, not surprisingly, a cube. Tetragonal. If I take the cubic crystal and expand (or compress) it along one axis, I get a tetragonal crystal. Here, a = b = c; all angles are 90◦ . Orthorhombic. If I take the tetragonal crystal and expand (or compress) it along a second axis, I get an orthorhombic crystal. Here, a = b = c; all angles are 90◦ . Monoclinic. If now I take the orthorhombic crystal and tip one axis away from the normal to the plane deﬁned by the other two in a way that preserves two right angles, I get a monoclinic crystal. For the monoclinic crystal, a = b = c; the angle β = 90◦ while the other two are 90◦ . Triclinic. To make triclinic, I take monoclinic and tip the other axes so that none are perpendicular to any other, making α = β = γ = 90◦ . It remains true that a = b = c also. I’ve now made the lattice as low in symmetry as I can.

282

Anisotropic Crystals Hexagonal. I return to the tetragonal system and open the angle γ to 120◦ . The formerly square ab plane is now a hexagonal ﬁgure. The hexagonal crystal has a = b = c and α = β = 90◦ ; γ = 120◦ . Trigonal. Finally, I return to the cube and pull it along one body diagonal, rendering all angles different from 90◦ but all still equal. The axes also remain equal, a = b = c. Trigonal sometimes called rhombohedral. The seven crystal systems contain the fourteen Bravais lattices.∗ The criterion for deﬁning a Bravais lattice is that the surroundings of the lattice points be identical. The Bravais lattices are shown in many books on solid-state physics and crystallography [19, 23, 24]. All of the Bravais lattices have lattice points located at the corners of the prism and some have other lattice points located at symmetric locations, in the middle of a face or at the body center. For example, the cubic system has simple cubic (sc), body-centered cubic (bcc), and face-centered cubic (fcc) Bravais lattices. It is worth noting that the hexagonal Bravais lattice (the only member of that crystal system) requires that there be a lattice point at the center of the hexagon, so that the lattice points on the ab plane form a triangular mesh.

15.4 The Dielectric Tensor Crystal symmetry has a dominant effect on the dielectric function. In a general crystal, the relation between D and E is a 3×3 tensor† as I wrote already in Eq. 2.11: ↔

D= ·E where (still in general)

⎛

xx = ⎝ yx zx

↔

xy yy zy

⎞ xz yz ⎠ . zz

(15.5)

The off-diagonal terms allow an electric ﬁeld along xˆ to produce a response (polarization ˆ or current) along yˆ or zˆ as well as x.

15.4.1 The Principal Axes This dielectric tensor is a symmetric tensor;‡ hence, it is possible to ﬁnd a Cartesian coordinate system in which it can be rendered diagonal. In this coordinate system, I have ∗ When I take into account reﬂection, rotation, inversion, and “improper rotation” symmetry operations, I will

ﬁnd that there are thirty-two different crystal classes. Furthermore, the combination of all possible symmetry operations results in a total of 230 different space groups. Fortunately, for considering optical anisotropy, I only need to think about the seven crystal systems. If I want to consider selection rules, such as which vibrational modes appear in an infrared spectrum, then I would need to dig deeper. † It is a 3×3 tensor because there are three directions in space. ‡ The symmetry may be proved in a number of ways: from thermodynamics, using Onsager’s reciprocity relation, by energy conservation [23].

283

15.4 The Dielectric Tensor ⎛

0 y 0

x ↔ =⎝0 0

⎞ 0 0⎠. z

(15.6)

↔

The axes of the coordinate system in which is diagonal are known as the principal axes. The diagonal components are the principal components. I will write diagonal component with a single subscript, as x rather than xx . An alert reader might ask at this point: Does the fact that the dielectric function is diagonal in its principal axes mean that I have removed the situation where polarization or current are not in the same direction as the electric ﬁeld? The answer is “yes” in the special case where the ﬁeld is along one of the principal axes; in this case the polarization and current are also along the principal axis. However, if the ﬁeld is in an arbitrary direction, then the answer is deﬁnitely “no!” Polarization and current will be in directions different from the electric√ﬁeld. As an example, let me take E = (E0 / 2)(yˆ + zˆ ), a ﬁeld of amplitude E0 at 45◦ to the ↔ y and z principal axes. The displacement vector is the dot product of and E, i.e.,∗ E0 ↔ D = · E = √ (y yˆ + z zˆ ), 2 making D not parallel to E if y = z , i.e., if the y–z plane is not isotropic.

15.4.2 Complex Dielectric Tensor That the dielectric function is a tensor does not stop it from being a complex function, and I’ll write it the same way I typically did when it was a scalar: ↔

↔

= 1 +

↔

4π i ↔ σ 1, ω

(15.7)

↔

where both 1 and σ 1 are 3×3 diagonalizable tensors with real elements. For example the conductivity (in its principal axes) is ⎛ ⎞ σ 1x 0 0 ↔ σ1 = ⎝ 0 (15.8) 0 ⎠. σ 1y 0 0 σ 1z

15.4.3 Crystal Symmetry Restricts the Dielectric Tensor The dielectric tensor must respect the symmetry of the crystal. If the crystal is indistinguishˆ then a ﬁeld in those two directions will induce identical polarizations able along xˆ and y, ↔ and currents; the corresponding elements in must be identical. ∗ The process for multiplying the dielectric tensor ↔ and the (column vector) electric ﬁeld E is as follows:

⎛ xx · E = ⎝ yx zx

↔

xy yy zy

⎞ ⎛ ⎞ Ex xz yz ⎠ · ⎝Ey ⎠ zz Ez

ˆ yx Ex + yy Ey + yz Ez ) ˆ xx Ex + xy Ey + xz Ez ) + y( = x( + zˆ (zx Ex + zy Ey + zz Ez ).

284

Anisotropic Crystals

There are a number of ways I could understand why for example the dielectric tensor of an orthorhombic crystal has three different elements and where the principal axes point. I can use group theory. I can consider the properties of tensors. What I will do here is make a (perhaps somewhat hand-waving) argument based on things I can do to the crystal that leave it unchanged. The operations I need are rotation and reﬂection. I’ll state a sort of Murphy’s law for the optics of crystals: if the dielectric tensor can possibly display anisotropy, it will do so. Murphy affects the principal-axis values: if they can be different, they will be different.∗ Moreover, if the symmetry does not ﬁx the directions of the principal axes, the axes will change direction as the wavelength varies. Cubic. I start again with the cubic crystal system. The cubic system has three orthogonal four-fold (90◦ ) rotation axes along the a, b, and c crystal axes. (There are also three orthogonal mirror planes, all normal to the crystal axes, four 120◦ axes along the body diagonals, a center of inversion, and others, making a total of 36 cubic space groups [23]. The amount of detail can become quite large.) The three four-fold axes mean that the crystal properties are unchanged for 90◦ rotations; the diagonal components of the dielectric tensor must be the same. The tensor can then be written as ⎛ ⎞ 1 0 0 ↔ ↔ = ⎝ 0 1 0⎠ = 1 , Cubic. (15.9) 0 0 1 ↔

where is a complex scalar and 1 is the identity tensor. But the dot product of the identity ↔ ↔ tensor and a vector is just the vector, so I have D = · E = 1 · E = E. The dielectric function of a cubic crystal is a scalar; the material is isotropic. Tetragonal. The tetragonal lattice has mirror planes in the a–b, a–c, and b–c planes. A reﬂection leaves unchanged a vector lying in the plane of the mirror but reverses one perpendicular to the mirror. To be unchanged under reﬂection, the axes must lie in the mirror or be perpendicular to it. Hence the principal axes are along the crystallographic axes. The structure has one fourfold rotation axis along the c axis. The components of the dielectric tensor for a and b are therefore identical; the c axis component is different. I then have ⎛ ⎞ a 0 0 ↔ = ⎝ 0 a 0 ⎠ . Tetragonal. (15.10) 0 0 c The dielectric tensor is said to be uniaxial: there is an optic axis along c and if the electric ﬁeld is along c, then D = c ˆ c E. For electric ﬁeld direction eˆ in the a–b plane, D = e ˆ a E. Orthorhombic. The orthorhombic lattice has mirror planes in the a–b, a–c, and b–c planes. Hence the principal axes are along the crystallographic axes. There are only twofold axes, which take an axis into itself. So the three components are different, ∗ There are of course counterexamples; Murphy’s laws are not theorems. For example, the components of the

dielectric function vary with frequency and it is possible that if I graph them over a wide frequency range they will cross one or more times. At the frequencies where they cross, the anisotropy does not exist. However, as the mathematicians say, this is a set of measure zero.

285

15.5 Plane-Wave Propagation in Anisotropic Materials ⎛ a ↔ =⎝0 0

0 b 0

⎞ 0 0⎠. c

Orthorhombic.

(15.11)

The orthorhombic system is biaxial. Monoclinic. Monoclinic crystals are also biaxial. The b axis is at right angles to both a and c, making one of the principal axes parallel to b. The other two axes are not ﬁxed relative to the crystal axes and will change directions as the frequency of the electromagnetic ﬁeld changes. I must re-diagonalize the tensor for each frequency of the light that encounters the crystal. ⎛ ⎞ x 0 0 ↔ = ⎝ 0 y 0 ⎠ , Monoclinic. (15.12) 0 0 z with y = b . Triclinic. The only symmetry operations are identity and inversion. The crystal is biaxial with axes all changing direction with frequency. ⎛ ⎞ x 0 0 ↔ = ⎝ 0 y 0 ⎠ . Triclinic. (15.13) 0 0 z Hexagonal. The hexagonal class has a six-fold axis perpendicular to the hexagonal or basal plane. This is as good as a four-fold axis for forcing the response of the plane to be independent of the direction of the in-plane ﬁeld. Hexagonal crystals are uniaxial with the optic axis perpendicular to the basal plane ⎛ ⎞ a 0 0 ↔ = ⎝ 0 a 0 ⎠ . Hexagonal. (15.14) 0 0 c Trigonal. The optic axis is ﬁxed to the direction the cube was pulled or pushed. Trigonal (rhombohedral) crystals are uniaxial. ⎛ ⎞ x 0 0 ↔ = ⎝ 0 x 0 ⎠ . Trigonal. (15.15) 0 0 z

15.5 Plane-Wave Propagation in Anisotropic Materials 15.5.1 Coordinates I need to deﬁne a coordinate system in which to describe electromagnetic wave propagation in a crystal. It may seem that I have a choice in how to align the axes of my coordinate system. On the one hand, I could, as I did in Section 2.8 for electromagnetic waves in

286

Anisotropic Crystals

vacuum, align the wave vector q and the ﬁelds D and H along the Cartesian axes and let the dielectric tensor be in nondiagonal form. On the other hand, I can choose as my Cartesian system the principal axes and let the ﬁelds fall on the crystal as they may, with the wave vector and ﬁeld vectors of the electromagnetic wave possibly having components along two or three axes. In practice, the choice is not there. I will have to use the principal axes as my coordinate axes.

15.5.2 Maxwell’s Equations Revisited I will continue to write the electric ﬁeld E and the magnetic ﬁeld H of the light as complex plane waves, as in Eqs. 2.5 and 2.6. I will also write D(r,t) = D0 ei (q·r−ωt ) .

(15.16)

I can start with Maxwell’s equations given in Eqs. 2.4a–2.4d and then make use of the simpliﬁcations of local, nonmagnetic, linear, and homogeneous materials, leaving out only ↔ ↔ ↔ ↔ the assumption of isotropy. I will plan to use D = · E with = 1 + (4π i/ω) σ 1 , so that, after substituting the plane-wave ﬁelds into Maxwell’s equations, I have q·D=0 q·H=0 ω q×E= H c ω q × H = − D. c

(15.17a) (15.17b) (15.17c) (15.17d)

These Maxwell’s equations for anisotropic materials tell me that it is q, D, and H that determine my right-handed coordinate system. The electric ﬁeld E is not in general parallel to D, so the electric ﬁeld will not in general be perpendicular to q. Equation 15.17c tells me that the ﬁeld E is perpendicular to H.

15.5.3 Field Directions From Maxwell’s equations, Eqs. 15.17a–15.17d, I can construct the picture of the ﬁeld directions shown in Fig. 15.4. The coordinates here are those of the ﬁelds, q, D, and H, so that in general the dielectric tensor is not diagonal. The E ﬁeld is inclined to these axes and has a component along either ±q as shown in the left or right sides of the ﬁgure. The direction of energy ﬂow is determined by the Poynting vector S, given (as I have said before) by S = (c/8π ) Re E × H∗ . In vacuum and in isotropic materials, the wave vector and Poynting vector point in the same direction. This is not the case in anisotropic crystals. The wave vector q is related to the complex refractive index in the usual way: q=N

ω q. ˆ c

(15.18)

287

Fig. 15.4

15.5 Plane-Wave Propagation in Anisotropic Materials

Fields for a wave propagating along x in an anisotropic medium with principal axes at an arbitrary angle with respect to the fields. The vectors q, D, and H form a right handed set and determine the primed coordinate system. I combine Eqs. 15.17c and 15.18 to write H = N qˆ × E. With this, and using the identity for the triple cross product, the Poynting vector is c ˆ qˆ · e)]. ˆ (15.19) S = (Re N ) |E|2 [qˆ − e( 8π Thus S, E, and H form a right-handed set and S points away from q by the same angle that E points away from D. Energy ﬂow and the ray direction directions differ, as shown in Fig. 15.4.

15.5.4 The Refractive Index Now, I ﬁnd a formal solution for the refractive index (and, hence, for the wave vector) of plane-polarized light in anisotropic crystals. The easiest way to continue is to take the cross product of q with Eq. 15.17c and use the vector identity for the triple cross product on the left side and Eq. 15.17d on the right side:∗ ω q × (q × E) = q × H c ω2 q(q · E) − q 2 E = − 2 D. c ↔

I then obtain (after using Eq. 15.18, canceling ω2 /c2 , using D = · E, changing signs, and swapping left and right sides): ↔

· E = N 2 [E − q( ˆ qˆ · E)] .

(15.20)

∗ An equally valid approach would be to take the curl of Eqs. 2.4c and 2.4d, use some vector identities, and obtain

a wave equation for E. The use of plane waves form for the ﬁelds leads to the same equation for the refractive index that I get here.

288

Anisotropic Crystals As a comment, the amplitude and the ei (q·r−ωt ) terms in the electric ﬁeld E will divide out; I could replace E with eˆ in Eq. 15.20 if I wanted to do so. The refractive index N is ˆ and by the electric determined by the dielectric tensor, by the wave propagation direction q, ˆ Before outlining the solution for the most general anisotropic crystal, I’ll ﬁeld direction e. look at the important case of the uniaxial crystal.

15.6 The Uniaxial Crystal The tetragonal, hexagonal, or trigonal systems are uniaxial: there is a single “optic axis,” typically taken as being in the z direction.∗ The dielectric tensor is given by one of Eqs. 15.10, 15.14, or 15.15. I’ll use the notation of the ﬁrst two of these. Two of the diagonal components are the same ( a ) and one is different ( c ). ↔ My goal is to obtain an equation for N in terms of the components of for a given ray ˆ My second goal is to ﬁnd the electric ﬁeld (to within an arbitrary constant). direction q. My third goal is to calculate the Poynting vector and to determine its direction relative to ˆ The equation for N will be the equivalent for anisotropic materials of Eq. 3.10, which q. √ reads N = . It is equivalent but in no way as simple.† The a–b plane of the uniaxial crystal is isotropic; the properties of the crystal do not change as it is rotated around the optic (z) axis. So I can set qˆ in the x–z plane and at an angle θ to the optic axis, so that qˆ · yˆ = 0 while qˆ · zˆ = cos θ and qˆ · xˆ = sin θ , making qˆ = sin θ xˆ + cos θ zˆ

(15.21)

If I think now about the electric ﬁeld direction, there seem to be two possibly distinct cases: ˆ and (2) the ﬁeld lies in the x–z (1) the ﬁeld is perpendicular to the x–z direction (along y) plane and hence has no yˆ component. In case (1) the waves are transverse whereas in case ˆ (2) they may have an E-ﬁeld component parallel to q.

15.6.1 The Refractive Index 15.6.1.1 Case 1: E Perpendicular to the Optic Axis ˆ then it is perpendicular to q also. Equation If E is perpendicular to the optic axis (along y) 15.20 becomes a Ey = N 2 Ey , √ ˆ e, ˆ and hˆ form a rightso that N = a . The magnetic ﬁeld is given by Eq. 15.17c; q, handed set just as in the isotropic case, Eq. 3.3. Moreover D(= a E) points in the same ∗ It is not the “optical axis.” The optical axis is the axis about which an optical system, such as a lens, has a

certain degree of symmetry.

† It is complicated enough for uniaxial materials; for biaxial crystals it is more so.

289

15.6 The Uniaxial Crystal

direction as E. This polarization sees no hint of the anisotropy. It is known as the “ordinary” ray or “ordinary” wave propagation: √ (15.22) No = a .

15.6.1.2 Case 2: E in the Plane Containing the Optic Axis and q For the “extraordinary” wave, q and E both have xˆ and zˆ components; neither has yˆ components. Equation 15.20 thus becomes two equations: a Ex = N 2 Ex − N 2 sin θ (qˆ · E) c Ez = N 2 Ez − N 2 cos θ (qˆ · E). I can rewrite these in the following way (where I’ve multiplied the ﬁrst by sin θ and the second by cos θ ): N 2 sin2 θ (qˆ · E) N 2 − a N 2 cos2 θ (qˆ · E) Ez cos θ = N 2 − c Ex sin θ =

I can add these, and then qˆ · E = Ex sin θ + Ez cos θ cancels out, leaving 1 sin2 θ cos2 θ = + . N2 N 2 − a N 2 − c This equation appears to be quadratic in N 2 , but, when fractions are cleared, the N 4 terms cancel, leaving only the quadratic term. After a minute amount of algebra I get √ a c , (15.23) N (θ ) = 2 c cos θ + a sin2 θ where I have written explicitly that the refractive index is a function of the angle the ray makes to the optic axis. The refractive index moves smoothly between two extremes, !√ a ≡ No θ = 0◦ N (θ ) = √ c ≡ Ne θ = 90◦, where Ne is known as the “extraordinary” refractive index. Note that in fact the extraordinary wave has a refractive index N (θ ) and a propagation velocity that depends on the direction of q. N(θ ) equals what one sees in the literature and in tables of materials properties for Ne when θ = 90◦ . This is the propagation direction for which N (θ ) differs the most from No .

15.6.2 “Ray Surfaces” As I have just shown, the refractive index of a uniaxial crystal has two values; the electric ﬁeld directions (or polarizations) that correspond to these two values are orthogonal. One

290

Anisotropic Crystals

polarization, the extraordinary ray, has a refractive index that varies with the direction of q. Consequently, light traveling in the crystal moves with a speed that depends on polarization and on direction of travel. Imagine that there is a point source of light at the center of the crystal capable of emitting in all directions a short ﬂash of unpolarized light. The ﬂash expands out from the point with a speed set by c/n where n is the real part of the refractive index N . In an isotropic medium, the light will be located in an expanding spherical shell. In an anisotropic material, there are two shells of light. One, generated by ordinary rays, travels in a spherical shell at c/no and with electric ﬁeld direction perpendicular to the optic axis. The other set of rays, the extraordinary ones, give an ellipsoid of revolution about the optic axis. The distance from the origin of this ellipsoid is c/n(θ ), where θ is the angle of the ray to the optic axis. The √ sphere and ellipsoid touch along the optic axis (θ = 0) where n(θ ) = no = a . They √ have a maximum separation for propagation in the ab plane, where no still equals a and √ n(θ ) = ne = c . There are two possibilities for the ellipsoidal shell. If ne > no (a positive uniaxial crystal), the extraordinary waves travel more slowly than the ordinary, and the extraordinary surface is a prolate ellipsoid inside the ordinary sphere. If, in contrast, ne < no (a negative uniaxial crystal), the extraordinary waves travel more quickly than the ordinary, and the extraordinary surface is an oblate ellipsoid surrounding the ordinary sphere. These surfaces are illustrated in Fig. 15.5 for both negative and positive uniaxial materials. The electric ﬁeld for the ordinary waves are everywhere perpendicular to the optic axis. The electric ﬁeld for the extraordinary wave is parallel to the optic axis when this wave is

Fig. 15.5

Ray surfaces for negative (top) and positive (bottom) uniaxial materials. The polarization vectors are indicated on the surfaces. The surfaces are shown looking down the optic axis (O.A.) (left side) and with the optic axis lying in the plane of the figure (right side). Field directions are also shown; dots indicate fields perpendicular to the drawing; arrows show fields in the plane of the drawing.

291

15.6 The Uniaxial Crystal

propagating ab plane but rotates to remain tangent to the ellipse as the propagation direction moves out of this plane.

15.6.3 The Fields Now I’ll address the electric ﬁeld, magnetic ﬁeld, and Poynting vector in the uniaxial crystal. I used Faraday’s law, Eq. 15.17c, and Amp`ere’s law, Eq. 15.17d, to obtain the equation for N (θ ) and will use one of these again to ﬁnd the relationship between magnetic and electric ﬁelds. What I need now is Gauss’ law, Eq. 15.17a. I will write ∇ ·D=0=q·D

or

↔

qˆ · · E = 0

↔

where I have used that D = · E and divided out either No ω/c or N (θ )ω/c depending on whether the E direction is for the ordinary or extraordinary direction. The ray direction is qˆ = sin θ xˆ + cos θ zˆ .

15.6.3.1 Case 1: E Perpendicular to the Optic Axis: Electric and Magnetic Fields √ The E ﬁeld is the yˆ direction by construction. The refractive index is No = a as given in Eq. 15.22. Then, I can ﬁnd the H ﬁeld using Eq. 15.17c, which I write as H = No qˆ × E. The cross product is xˆ yˆ zˆ H = No qˆ × E = No sin θ 0 cos θ = −No Ey cos θ xˆ + No Ey sin θ zˆ . 0 Ey 0 The magnitude of this ﬁeld is

H = No Ey cos2 θ + sin2 θ = No Ey .

So the ﬁelds are in every way ordinary. The wave is a transverse electromagnetic wave with the same relation between q, E, and H as in an isotropic materials. The refractive index is N = No . The Poynting vector is parallel to the wave vector, so the waves and energy ﬂow in the same direction.

15.6.3.2 Case 2: E in the Plane Containing the Optic Axis and q: Electric Field Light with this polarization is called the “extraordinary” wave. I’ll start by writing a general electric ﬁeld vector in the x–z plane: E = Ex xˆ + Ez zˆ .

(15.24)

What I want to know is the direction of E as a function of θ ; to know this ﬁeld requires me to ﬁnd Ex and Ez in terms of the overall magnitude of the electric ﬁeld∗ E. Now the displacement vector D is ∗ There is no constraint on the magnitude of the ﬁeld. I can always make the overall electric ﬁeld larger or smaller

by turning up or down my lamp, or my laser, or my RF generator.

292

Anisotropic Crystals ↔

D = · E = a Ex xˆ + c Ez zˆ, and then Gauss’ law is qˆ · D = 0 = a Ex sin θ + c Ez cos θ . After a couple of lines of algebra I get Ez = −Ex

a tan θ . c

(15.25)

Although Eq. 15.25 describes the ratio of the two components of the electric ﬁeld, it is not very illuminating. So I’ll write a tan θ zˆ c √ and write the magnitude of the electric ﬁeld E = E · E. Several lines of algebra later I arrive at E = Ex xˆ − Ex

Ex =

c cos θ

E.

(15.26)

a2 sin2 θ + c2 cos2 θ

I now put this into Eq. 15.25 and ﬁnd Ez = −

a sin θ

E.

(15.27)

a2 sin2 θ + c2 cos2 θ

I said that the electric ﬁeld is not perpendicular to the wave vector. Let me check that by calculating the dot product of qˆ and E, which I’ll call E : E = qˆ · E = Ex sin θ + Ez cos θ . I substitute Eqs. 15.26 and 15.27 to ﬁnd (c − a ) sin θ cos θ E. E = a2 sin2 θ + c2 cos2 θ

(15.28)

ˆ I like Eq. 15.28 very much indeed. It shows that the q-parallel (extraordinary) part of the electric ﬁeld in uniaxial crystals is zero if (1) c = a (the material is not anisotropic) or (2) θ = 0 (the wave is propagating along the optic axis) or (3) θ = 90◦ (the wave is propagating perpendicular to the optic axis). In all other cases, there is a component parallel ˆ to q.

15.6.3.3 Case 2: E in the Plane Containing the Optic Axis and q: Magnetic Field Now that I have an equation for E, I can calculate H from Amp`ere’s law: H = N (θ )qˆ × E. ˆ and (to start) 15.24 (for E): I do this calculation, using Eqs. 15.21 (for q), ˆ H = N (θ )(Ex cos θ − Ez sin θ )y.

293

15.6 The Uniaxial Crystal Now, Ez is negative for θ in the range 0–90◦ . (See Eq. 15.27.) Thus, H is deﬁnitely in the plus yˆ direction. I substitute Eqs. 15.26, 15.27 (for ﬁelds), and 15.23 (for N (θ )) to obtain a c (a sin2 θ + c cos2 θ ) ˆ E y. (15.29) H= a2 sin2 θ + c2 cos2 θ I do not like Eq. 15.29 very much but see no way to clean it up. It has the advantage of being dimensionally correct and of giving ! No E yˆ θ = 0 (15.30) H= Ne E yˆ θ = 90◦ √ √ where No = a is the ordinary refractive index and Ne = c is the extraordinary refractive index. As ever, it is the E-ﬁeld direction that determines which refractive index is employed.

15.6.3.4 Case 2: E in the Plane Containing the Optic Axis and q: Poynting Vector The next (and last) step in the treatment of wave propagation in uniaxial materials is to calculate the time-average Poynting vector, S = (c/8π )E × H∗ . I’ll use E = Ex xˆ + Ez zˆ ˆ Then (Eq. 15.24) and H = H y. S=

c (−Ez H ∗ xˆ + Ex H ∗ zˆ ) 8π

and, using Eqs. 15.26, 15.27, S=

c a sin θ xˆ + c cos θ zˆ EH ∗ . 8π 2 sin2 θ + 2 cos2 θ a c

(15.31)

∗ The √ magnitude of the Poynting vector is S = (c/8π )EH (which I get either by calculating S · S or by noting that the angle between the electric and magnetic ﬁelds is 90◦ ). The direction of the Poynting vector is more interesting than the magnitude; the unit vector in the direction of S is

a sin θ xˆ + c cos θ zˆ sˆ = a2 sin2 θ + c2 cos2 θ

(15.32)

and a sin2 θ + c cos2 θ qˆ · sˆ ≡ cos φ = a2 sin2 θ + c2 cos2 θ where φ is the angle between qˆ and sˆ . The angle is zero for θ = 0 and 90◦ and not zero for other values. As sketched in Fig. 15.4, the Poynting vector can lie either between q and D or on the other side of q from D, depending on whether E = qˆ · E is negative or positive.

294

Anisotropic Crystals

(See Eq. 15.28.) So I’ll also specify the angle α between S and the optic axis, given by cos α = zˆ · sˆ . The result is cos α =

cos θ a c

2

sin2 θ

. + cos2 θ

15.6.4 Some Uniaxial Materials Many materials (quartz, sapphire, ice) are uniaxial crystals. The refractive indices of a number of these materials are in Table 15.1, from Ref. 345. The refractive index is for a frequency in the yellow (590 nm, 16,950 cm−1 , 2.10 eV), close to the wavelength of low-pressure sodium lamps, like those used in some street lamps. Most of these materials are reasonably transparent at this wavelength. The table gives the name, chemical formula, crystal system, no , ne , and δn = ne − no . All three of the uniaxial crystal systems are represented. Calcite has a reasonably large δn and good optical transparency, a reason why calcite is used in many polarizers supplied by commercial vendors.

Table 15.1 Uniaxial crystals, at 590 nm. Material

Formula

Crystal system

no

ne

n

Barium borate

BaB2 O4

Tri

1.678

1.553

−0.124

Beryl

Be3 Al2 (SiO3 )6

Hex

1.602

1.557

−0.045

Calcite

CaCO3

Tri

1.658

1.486

−0.172

Calomel

Hg2 Cl2

Tet

1.973

2.656

+0.683

Cinnabar

HgS

Tri

2.905

3.256

+0.351

Hematite

Fe2 O3

Tri

2.940

3.220

+0.287

Ice

H2 O

Hex

1.309

1.313

+0.004

Lithium niobate

LiNbO3

Tri

2.272

2.187

−0.085

Magnesium ﬂuoride

MgF2

Tet

1.380

1.385

+0.006

Quartz

SiO2

Tri

1.544

1.553

+0.009

Rutile

TiO2

Tet

2.616

2.903

+0.287

Sapphire

Al2 O3

Tri

1.768

1.760

−0.008

Sodium nitrate

NaNO3

Tri

1.587

1.336

−0.251

Silicon carbide

SiC

Hex

2.647

2.693

+0.046

Tourmaline

(a silicate)

Tri

1.669

1.638

−0.031

Zircon, high

ZrSiO4

Tet

1.960

2.015

+0.055

Zircon, low

ZrSiO4

Tet

1.920

1.967

+0.047

Tri = trigonal; Hex = hexagonal; Tet = tetragonal.

295

15.7 The Biaxial Crystal

15.7 The Biaxial Crystal ↔

My goal now is to obtain a general equation for N in terms of the components of without restricting the symmetry. The algebra is similar to what I did for the uniaxial crystal. First, I write Eq. 15.20 in components, using the form in Eq. 15.6 for the dielectric tensor and dotting from the left with the appropriate unit vector: ˆ qˆ · E) x Ex = N 2 Ex − N 2 (xˆ · q)( ˆ qˆ · E) y Ey = N 2 Ey − N 2 (yˆ · q)( 2

(15.33)

2

ˆ qˆ · E) z Ez = N Ez − N (ˆz · q)( ˆ is a clumsy way to write “the x component of the unit vector q.” ˆ (qx is already where (xˆ · q) taken as the x component of the wave vector q.) In order to be slightly less clumsy,∗ I will deﬁne xˆ · qˆ ≡ α, yˆ · qˆ ≡ β, and zˆ · qˆ ≡ γ , noting that the dot product of two unit vectors is just the cosine of the angle between them.† These three equations can be reorganized (solve for Ei and then multiply by α, β, and γ respectively) to give N 2α2 (qˆ · E) N 2 − x N 2β 2 (qˆ · E) βEy = 2 N − y αEx =

γ Ez =

N 2γ 2 (qˆ · E). N 2 − z

Now, I sum these three equations. I recognize the sum of the terms on the left as qˆ · E = αEx + βEy + γ Ez , so that the sum is α2 β2 γ2 2 qˆ · E. qˆ · E = N + 2 + 2 N 2 − x N − y N − z If I were working with isotropic systems, I would be in trouble because qˆ · E would be zero and N 2 would equal . But this trouble does not arise for anisotropic materials. I can cancel ↔ qˆ · E from both sides and obtain the desired equation for N 2 in terms of : 1 α2 β2 γ2 = 2 + 2 + 2 . 2 N N − x N − y N − z

(15.34)

Eq. 15.34 appears to be a cubic‡ equation for N 2 . Fortunately the N 6 term cancels on both sides because α 2 + β 2 + γ 2 = 1. The quadratic equation for N 2 is

∗ But maybe a bit more obscure. † I’m using the conventional notation for direction cosines and hoping that the use of α, β, and γ earlier for

the angles in the unit cell prism does not lead to too much confusion. In my discussion of uniaxial crystals, cos θ = γ . ‡ Or a sixth-order equation for N . But it is N 2 I want.

296

Anisotropic Crystals ' ( ' % & N 4 x α 2 + y β 2 + z γ 2 − N 2 x y α 2 + β 2 % & % &( + y z β 2 + γ 2 + z x γ 2 + α 2 + x y z = 0.

(15.35)

Equation 15.35 is of the form a(N 2 )2 + b(N 2 ) + c = 0. I know the solution because I learned the quadratic equation some years ago.∗ The three terms that go into the quadratic formula are a = x α 2 + y β 2 + z γ 2 % & % & % & b = −x y α 2 + β 2 − y z β 2 + γ 2 − z x γ 2 + α 2

(15.36)

c = x y z . If ever I need it, I can write several pages of algebra and have a result. There will in fact be two results and, when they are plugged back into Eq. 15.20, I will ﬁnd that the two results correspond to orthogonal directions of E. The solutions depend also on direction of propagation, so that there are two ellipsoidal ray surfaces. These surfaces intersect at four points in pairs along a line joining the intersection points and the origin. At these points the two refractive indices are equal. The two lines are the two optic axes of the biaxial crystal.

15.7.1 Rays and Fields along Principal Axes Optical effects in the biaxial crystal are considerably simpliﬁed if q and E are along principal axes. Let me set Exˆ but allow (for the moment) q to be arbitrary. With this direction for the electric ﬁeld, the dot product qˆ · E = αEx where α is the cosine of the ˆ I can then rewrite Eq. 15.33 as angle between q and x. x Ex = N 2 Ex − N 2 α 2 Ex 0 = N 2 βαEx 0 = N 2 γ αEx . If I suppose that α = 0, then the second and third of these require β = γ = 0. But then ˆ α = 1 and the ﬁrst equation leads to Ex = 0, contradicting my starting with E = Ex x. Thus, I have to take α = 0, putting q in the y–z plane, perpendicular to E. Then, Eq. 15.33 become Na2 = x .

(15.37)

Similar arguments give Nb2 = y when the ﬁeld is in the yˆ direction and Nc2 = z for ﬁeld in the zˆ direction. The anisotropy is evident in the different values of N affecting wave propagation for the three ﬁeld directions but the wave propagation is purely ordinary. Moreover, the arguments that led to Eq. 15.30 tell me that the magnitudes of the corresponding magnetic ﬁeld are in each case H = Ni E, just as in the ordinary case. ∗ There is a nice discussion at the Wolfran website on the method to preserve numerical accuracy when b2

4ac so one of the roots involves the difference between two almost identical numbers. See http://mathworld .wolfram.com/QuadraticEquation.html.

15.8 Anisotropic Material with Boundaries: R and T

297

15.8 Anisotropic Material with Boundaries: R and T Now let me turn to the case of light incident on the surface of an anisotropic crystal. The general case is quite complicated. The surface may be cut at an arbitrary angle to the principal axes; the angle of incidence may vary, as may the polarization. I’ll discuss some important cases that allow more or less simpliﬁcation. A complete discussion of the general case can be found in Born and Wolf [8]. The transmission and reﬂection of light at an interface are determined by the boundary conditions.∗ As I’ve already shown, the electric ﬁeld in the anisotropic medium generally consists of two orthogonal contributions: the ordinary wave and the extraordinary wave. Each has an associated magnetic ﬁeld and q vector. So I will need to decompose the incident ﬁelds along these two directions and apply the boundary conditions to both.

15.8.1 Normal Incidence with Field along a Principal Axis I will start with a simple case: The ﬁeld is normally incident on a crystal that was grown (or cut and polished) with two principal axes lying in the surface and the third parallel to the normal. For deﬁniteness, let me consider an orthorhombic crystal (biaxial) with the a ˆ and the b and c axes in the surface, parallel to yˆ and axis along the normal, parallel to x, zˆ , respectively. I’ll then have q parallel to xˆ and can polarize the incoming light in the ˆ Continuity of the electric ﬁeld y–z plane. Suppose that the incident ﬁeld is polarized Ey. means that the ﬁeld inside is also along yˆ and that it is traveling in a medium characterized by Nb . (See Eq. 15.37 and what immediately follows that.) The ﬁeld inside is smaller on account of the fact that there is also a reﬂected wave moving out along the normal. The situation is in fact exactly the same as the one I worked out back in Chapter 3 (Section 3.3). See also Fig. 3.2. Using the notation of the current chapter† and letting the incident ﬁeld be in vacuum, I can just write 1 − Nb . (15.38) rb = 1 + Nb What I measure is the reﬂectance,

1 − Nb 2 Rb = 1 + Nb =

(nb − 1)2 + κb2

(15.39)

, (nb + 1)2 + κb2 √ with nb and κb the real and imaginary parts of Nb = b . Now I can rotate the polarizer 90◦ and measure Rc . I can ﬁnd a surface (or cut and polish one) containing the a axis, polarize the light appropriately, and measure Ra ‡ ∗ In the absence of surface charges or currents, the boundary conditions are the continuity of the tangential

component of E, the normal component of D, the normal component of B, and the tangential component of H.

† I used a and b for the two media in Chapter 3; here a and b represent crystal axes. ‡ I can turn the polarizer again and measure one of the other two. In principle, neglecting edge states, this fourth

measurement is redundant.

298

Anisotropic Crystals

These three measurements are done for the cases where the wave propagation is the simplest. But they are exactly what I want if I am interested in the dielectric tensor of the anisotropic material. Causality still applies, and so I can use the Kramers–Kronig method to estimate the principal components of the dielectric tensor in the same way as for isotropic solids. Transmittance is equally straightforward. The transmittance discussion in Chapter 7 applies to the polarized transmittance. The light polarized along the a axis travels at speeds and with absorption governed by Na . I say that it is simple or straightforward but there are subtleties that should be mentioned. For instance, reﬂection measurements are typically made at near normal incidence and not at exactly normal incidence.∗ Normally the reﬂectance from the Fresnel equations does not vary much with angle out to 10◦ or so. (See Appendix E.) In some cases, however, the reﬂectance for anisotropic media can show anomalies, especially with p-polarized light (light where the electric ﬁeld is in the plane of incidence and thus light at nonnormal incidence has a vertical component). If the dielectric function for the principal axis parallel to the surface normal direction has a zero at some frequency, anomalies may appear in the p-polarized spectrum. A good example has been given by Duarte, Sanjurjo, and Katiyar [346]. The ﬁx is to use s-polarized light as much as possible.

15.8.2 Normal Incidence with Field in a Plane Containing an Optic Axis I’ve just seen that reﬂectance and transmittance is pretty simple if the ﬁeld is along a principal axis. What about the case if the ﬁeld direction is between these two directions? Let me suppose that surface contains both the b and c axes, as above. The incident ﬁeld has Ei at an angle φ to the c axis, so that Ei = Ei sin(φ)yˆ + Ei cos(φ)ˆz with Ei the incident electric ﬁeld strength. The reﬂected ﬁeld has Er = Ei rb sin(φ)yˆ + Ei rc cos(φ)ˆz, making the reﬂected intensity be R(φ) = Rb sin2 (φ) + Rc cos2 (φ). One of Rb and Rc is larger than the other. The reﬂectance interpolates smoothly between these two values as φ is varied. The principal axes correspond to the direction where the reﬂectance is a maximum and the (orthogonal) direction where it is a minimum. Note that the outgoing waves will not be polarized at φ. (Consider the case where Rb = 0. The reﬂected ﬁeld will be polarized always along zˆ , increasing in intensity as cos2 (φ) as the incident polarization direction is varied.) I could place an analyzing polarizer in the optical train behind the sample also at angle φ. I would then need to take the dot product eˆ · Er , where e = sin(φ)yˆ + cos(φ)ˆz before squaring to get the intensity.

∗ Angles of incidence of 5◦ –10◦ are common in order that the reﬂected light can take a path distinct from the

incident light. Even if a beamsplitter is used to pick off the reﬂected light, the light is typically focused on the sample; only the central ray in the pencil of incident light is at normal incidence.

299

Fig. 15.6

15.8 Anisotropic Material with Boundaries: R and T

Light is normally incident on a uniaxial crystal with optic axis at an angle θ to the surface normal. The electric field of the incident light is oriented so as to excite the extraordinary wave in the crystal.

15.8.3 Normal Incidence Reflectance with an Inclined Optic Axis I now turn to the case of a uniaxial crystal cut so that the optic axis dips below the surface. I’ve simpliﬁed to a uniaxial crystal (tetragonal, hexagonal, or trigonal) and will make use of the ﬁelds that I calculated in Section 15.6.3 of this chapter. I’ll continue to use a coordinate system in which the optic axis is along zˆ ; consequently, the incoming wave vector and ﬁelds will be inclined relative to the coordinates. A diagram of the geometry is in Fig. 15.6. The optic axis is along the zˆ direction and the normal to the surface lies in the x–z plane, at an angle θ to the optic axis. The normal vector is then nˆ = zˆ cos(θ ) + xˆ sin(θ ). The wave vector direction qˆ will equal nˆ for normal incidence.

15.8.3.1 The Ordinary Wave ˆ not as shown in Fig. 15.6 but instead perpendicular If I orient my electric ﬁeld along y, to the plane of the diagram, I will have ordinary waves inside the crystal, with wave √ propagation and reﬂectance governed by No = a according to Eq. 15.22. The reﬂected ﬁeld and reﬂectance follow as usual.

15.8.3.2 The Extraordinary Wave If I orient my electric ﬁeld in the x–z plane, as shown in Fig. 15.6, I will launch the extraordinary wave in the crystal. For simplicity (and without loss of generality in this linear medium) let me set the amplitude of the incident ﬁeld to unity. Then I have Ei = zˆ sin(θ ) − xˆ cos(θ ). The reﬂected ﬁeld is written ˆ e cos(θ ), Er = zˆ re sin(θ ) − xr where re is the complex amplitude reﬂectivity.

300

Anisotropic Crystals

For the ﬁeld inside, I can write ˆ tx , Et = zˆ Etz + xE ˆ where Etz is the strength of the ﬁeld component along zˆ and Etx is the strength along x. I know these ﬁelds. I worked out the components of the extraordinary wave earlier in this chapter; they are given in Eqs. 15.26 and 15.27. I also know the magnetic ﬁeld (along yˆ in this geometry); it is in Eq. 15.29. The electric ﬁeld and magnetic ﬁelds are continuous across the boundary, so of course all I now need to do is to equate the ﬁelds on the two sides of the boundary. After a moderate amount of algebra I obtain re =

1 − N (θ ) 1 + N (θ )

(15.40)

√ where N(θ ) = a c / c cos2 θ + a sin2 θ, as given in Eq. 15.23. I think that Eq. 15.40 is both surprising and not surprising. It is surprising that things worked out so nicely to give a solution formally like the isotropic case. It is not surprising in that I’d expect a wave in the medium characterized by a particular value N (θ ) of the refractive index to have a reﬂectance 1 − N (θ ) 2 Re = 1 + N (θ ) (15.41) [n(θ ) − 1]2 + κ(θ )2 = , [n(θ ) + 1]2 + κ(θ )2 with n(θ ) and κ(θ ) the real and imaginary parts of N (θ ).

15.9 Polarizers and Waveplates Anisotropic materials are needed to produce or manipulate polarized light. There are a variety of devices, but the basics are linear polarizers, quarter-wave plates, and half-wave plates. I’ll discuss each of these brieﬂy.

15.9.1 Polarizers A linear polarizer is a device which is opaque (or reﬂecting) for one speciﬁc polarization direction and transparent for the orthogonal polarization. (See Section 15.2 earlier in this chapter.) The simplest way to achieve this property is to have a slab geometry made from a uniaxial material with the optic axis (ˆz) in the plane of the slab. Suppose the corresponding component of the dielectric tensor, c , has a relatively large imaginary part while the other two diagonal components have zero imaginary parts. Then a light ﬁeld polarized along zˆ sees an absorption coefﬁcient αc = ωc2 /nc and as long as the slab’s thickness d is large enough, the transmittance, which – if reﬂection can be ignored – will be T = e−αc d → 0. The transmittance for light polarized in the nonabsorbing direction will – neglecting

301

15.9 Polarizers and Waveplates

reﬂection and residual absorption – be nearly 100%. Suppose the incident ﬁeld is of the ˆ having been linearly polarized by an upstream form E = E0 (cos θ yˆ + sin θ zˆ ) with qx, polarizer. Then the component parallel to y is transmitted and that parallel to z is not. The transmitted intensity is then It = Io cos2 θ,

(15.42)

where I0 is the incident intensity. This cos2 behavior is known as the law of Malus. The most common dichroic material of the type described above is known as “polaroid,” a polymeric material containing aligned chains of absorbing molecules. The chains are absorbing for parallel polarization. Other polarizers are made of a parallel grid of wires; these reﬂect light parallel to the wire and transmit the component perpendicular to the wire. The highest-quality polarizers operate on other principles. The refractive indices for ordinary and extraordinary rays differ, and so light incident on a crystal at an oblique angle is refracted according to Snell’s law, with no or ne coming into play depending on polarization. (See Appendix E.) So a prism with the optic axis parallel to the base of the prism will separate polarizations into two beams that will separate after traveling some distance behind the prism. The critical angle for total internal reﬂection also depends on polarization. (See also Appendix E for a discussion of total internal reﬂection.) There are a number of polarizer designs that use total internal reﬂection to reﬂect one polarization while allowing the other polarization to be transmitted. These devices achieve a very high degree of polarization.

15.9.2 Quarter-Wave Plate A quarter-wave plate is a device that converts linearly polarized light to circularly polarized light. It typically comes as a thin transparent slab made of a birefringent crystal. The optic axis lies in the plane of the slab. The user transmits light through the slab at normal incidence. The transmitted light gains phase according to the refractive index and distance traveled in the wave plate. I set the xˆ direction as the normal into the slab and orient q along this normal. The optic axis, with refractive index ne , is along zˆ . Fields in the yˆ direction see refractive index no . I’ll choose a material for which ne > no .∗ The incoming ﬁeld is plane polarized light with the plane of polarization at an angle θ to the optic axis: Ein = E0 [yˆ sin(θ ) + zˆ cos(θ )] ei (qx−ωt ), where E0 is the complex amplitude and I’ll ignore reﬂection at the slab surfaces (or ask that the wave plate be antireﬂection coated). The two components of the electric ﬁeld propagate with wavevectors qe = ne ω/c = 2π ne /λ and qo = no ω/c = 2π no /λ for the components respectively parallel and perpendicular to the optic axis.† The light leaving the wave plate is Eout = E0 yˆ sin(θ )ei 2π no d/λ + zˆ cos(θ )ei 2π ne d/λ ei (qx−ωt ), ∗ This requirement would allow many possible choices of materials; see Table 15.1. † Here, λ is the vacuum wavelength of the light.

302

Anisotropic Crystals where d is the thickness of the plate. Because no = ne the two components have gained different phases on going through the wave plate. The phase difference is what matters; I’ll deﬁne it as

φ =

2π (ne − no )d λ

(15.43)

so that the transmitted light is Eout = E0 eiφo yˆ sin(θ ) + zˆ cos(θ )ei φ ei (qx−ωt ),

(15.44)

where φo = 2π no d/λ. Now let me orient the polarization of the incoming plane polarized light so that θ = 45◦ and at the same time, make the thickness of the wave plate such that (ne − no )d =

λ , 4

(15.45)

making φ = π/2 and ei φ = i. In this case the transmitted ﬁeld is left circularly polarized light: Eout =

E0 eiφo [yˆ + i zˆ ] ei (qx−ωt ) . √ 2

(15.46)

This result is worth a few remarks. First, Eq. 15.45 makes clear the basis of the name “quarter-wave plate.” If I want right circular polarization, I rotate the plate until the optic ˆ I can also use materials with ne < n0 , in which case φ = −π/2 and axis is along y. the analysis following Eq. 15.44 leads to right circular polarization. If I rotate things such that θ = 45◦ , I get elliptically polarized light with an ellipticity that goes to zero when θ = 0 or 90◦ . Finally, if I make the quarter-wave plate from sapphire (ne − no = 0.008 at ˚ the thickness of a zero-order quarter-wave plate is rather thin, of order 18 λ = 5,900 A), μm. Multiple-order wave plates increase the thickness by as many factors of 2π in φ as needed to make a more robust device.

15.9.3 Half-Wave Plate A half-wave plate is a device that rotates the polarization plane of linearly-polarized light. It differs from the quarter-wave plate only in the thickness d. The name even suggests the the difference; the half-wave plate is twice the thickness of the quarter-wave plate. The thickness satisﬁes (ne − no )d =

λ , 2

(15.47)

making φ = π and ei φ = −1. Equation 15.44 then becomes Eout = E0 eiφo [yˆ sin(θ ) − zˆ cos(θ )] ei (qx−ωt ) .

(15.48)

303

15.10 Things Not in This Chapter

The light leaving the half-wave plate is clearly not parallel to the light entering it. I ﬁnd the rotation angle by computing the dot product of the unit vectors of incident and transmitted light: cos( ) = [yˆ sin(θ ) + zˆ cos(θ )] · [yˆ sin(θ ) − zˆ cos(θ )] = sin2 (θ ) − cos2 (θ ) = cos(2θ ). If the incident polarization is at 45◦ to the optic axis, the plane of polarization is 90◦ away from the incident direction. Any other rotation angle may be obtained by adjusting the angle of the optic axis (or the incoming polarization) between 0 and 45◦ .

15.10 Things Not in This Chapter I’ll now conclude the discussion of crystal optics by mentioning a couple of things that I have not covered. I only sketched the solution for biaxial crystals and omitted the extra richness associated with the ray surfaces of these materials. Also, I only brieﬂy discussed the difference between optical waves in crystals and optical rays in crystals. Figure 15.7 illustrates the difference: the Poynting vector S, which points in the direction of energy ﬂow, is not parallel to the wave vector q. Therefore, even for normal incidence, where Snell’s laws tells me that the angle of refraction is zero (regardless of index of refraction), the energy of the extraordinary ray can propagate at an angle to the normal. This effect is usually demonstrated by looking at printed text through a birefringent crystal and observing two images of the text; the images have orthogonal polarizations. I have not mentioned liquid crystals, where an applied electric ﬁeld can induce anisotropy, or the Pockels electro-optic effect, where an electric ﬁeld modiﬁes the refractive index. These are both nonlinear processes of course, but once the ﬁeld is set, the material acts as a linear anisotropic solid.

16

Magneto-Optics

This chapter explores the effect of a strong static magnetic ﬁeld on the optical properties of metals and of insulators. The effects are substantial. One reason is that the static ﬁelds are really large, compared to the ﬁelds from ordinary incoherent light.∗ If for instance I have a 100 W light bulb, emitting in all directions, I can estimate that the magnetic ﬁeld of the light at a distance of 1 m is about 2.6 mG or 2.6×10−7 T. This ﬁeld is much smaller than the 0.5 G ﬁeld at the Earth’s surface.† Earth’s ﬁeld in turn is basically negligible compared to the 8–12 T superconducting solenoids existing at many laboratories or the 45 T hybrid magnet at the National High Magnetic Field Laboratory.‡

16.1 Charged Particle in a Magnetic Field The ﬁeld interacts with the charge motion in the solid through the Lorentz force, q F = v × B0 (16.1) c for a particle with charge q. The charge for electrons is negative, q = −e. B0 is the strength of the (static) magnetic ﬁeld. Note that when I need to be speciﬁc about directions, B0 will be in the zˆ direction, so that I will write B0 = B0 zˆ whenever I need to specify a direction. The velocity v is substantial; remember that the Fermi velocity is of order c/200. Figure 16.1 shows the three vectors when v is in the x–y plane. Among the effects that I can address starting with Eq. 16.1 are the Hall effect, magnetoresistance, Cyclotron resonance, helicons (whistlers), and the Faraday effect. I’ll start by considering free carriers (metals or doped semiconductors). Then, at the end of the chapter, I will work out Faraday rotation in a transparent insulator.

∗ Lasers, especially short-pulsed lasers are a different story. † Wikipedia says 25–65 μT. ‡ Fifty years or so ago, people reported the ﬁelds produced by magnets in their laboratories in G (Gauss) or kG

(thousand Gauss). But at some time in the last few decades, reports of ﬁeld in T (Tesla) became more common. This change may have been due to pressure to use SI units everywhere but may instead be due to the appearance of too many zeros in the cgs numbers; 12 T is easier to say than 120,000 G. In this chapter, I’ll often specify ﬁelds in T, but I (and you) must remember that I am working in cgs-Gaussian units, so whenever I need to compute some quantity containing the ﬁeld, I will need to enter ﬁeld values in Gauss.

304

305

Fig. 16.1

16.1 Charged Particle in a Magnetic Field

Force F on a (positive) charge moving in a magnetic field B with velocity v.

16.1.1 Cyclotron Orbits I’ll start with the motion of a free electron in a metal when a magnetic ﬁeld is applied. As I discussed in Chapter 8, the electrons are speciﬁed by a wave vector k, related to the with m the mass. Thus the Lorentz force is velocity by vk = hk/m ¯ he ¯ (16.1) k × B0 . mc The force is orthogonal to both k and B0 . Now the force leads to an acceleration, which in this case changes the direction of the velocity (or k) vector without changing its magnitude. (Magnetic ﬁelds do no work; the kinetic energy is unchanged.) I use Eq. 8.13 and include the damping force from Eq. 8.14, Fk = −

δk dk = Fk − h¯ dt τ he δk ¯ (16.2) = − k × B0 − h¯ mc τ where τ is the mean free time between collisions. Now, I take (for the moment) τ to be long enough that I can ignore it. The only force is the Lorentz force, h¯

eB0 dk =− k × zˆ . dt mc I’ll write the components of k, deﬁning as I do ωc , the cyclotron frequency,∗ ωc ≡

eB0 mc

(16.3)

(16.4)

∗ I’m making ω a positive quantity. I could equally well have made it negative (for electrons) by bringing c

the minus sign along. I’ll have to remember that I did not do so when the question of the sense of the motion comes up.

306

Magneto-Optics

so that dkz =0 dt dkx = −ωc ky dt dky = ωc kx . dt

(16.5a) (16.5b) (16.5c)

The equations tell the story and some of it is pretty simple. The zˆ component is constant because components of the velocity parallel to the magnetic ﬁeld do not contribute to the Lorentz force. The other two are coupled; I solve them by taking another derivative of Eq. 16.5b to ﬁnd that k¨x = −ωc k˙y = −ωc2 kx . The solution is either a sine or cosine of ωc t. I look at the signs in Eqs. 16.5b and 16.5c and decide that kx = k⊥ cos(ωc t) ky = k⊥ sin(ωc t),

(16.6)

where k⊥ is the magnitude of the component of k perpendicular to zˆ , the ﬁeld direction;

k⊥ = k 2 − kz2 . The in-plane part of the electron wave vector, k⊥ (and, equivalently, the in-plane velocity vector) remains tangent to the electron’s circular orbit as it moves in a counterclockwise sense around the magnetic ﬁeld.∗ The angular frequency of the orbital motion is given by Eq. 16.4. For electrons with a mass equal to me , the free-electron mass, the frequency fc = ωc /2π is B0 B0 B0 = 28.0 GHz = 0.933 cm−1 . 1G 10 kG/1 T 10 kG/1 T If the effective mass of the charge carriers is higher or lower than the free-electron mass, the frequency will be correspondingly lower or higher. But the effect clearly occurs in the radio-frequency to far-infrared spectral region. Fields of 100 kG (10 T) provide cyclotron frequencies of just under 10 cm−1 (300 GHz/1.2 meV) for free electrons. If the effective mass is m = 0.013me , the electron effective mass in InSb, the frequency increases to fc = 720 cm−1 (89 meV). I convert from wave vector to velocity to ﬁnd that vx = v⊥ cos(ωc t) and vy = v⊥ sin(ωc t) with v⊥ = h¯ k⊥ /m. Integrating once gives x = x0 + (v⊥ /ωc ) sin(ωc t) and y = y0 − (v⊥ /ωc ) cos(ωc t). The radius of the orbit is Rc = (v⊥ /ωc ). The velocity varies from zero to the Fermi velocity. So the maximum orbital radius is for electrons moving in the plane perpendicular to the ﬁeld with the Fermi velocity; this radius is vF mvF c = . Rc = ωc eB0 fc = 2.80 MHz

At a ﬁeld of 100 kG, the radius for an orbit for a Fermi surface electron moving in the x–y ˚ This is quite a bit longer than the mean free plane of a metal like silver is Rc = 7,900 A. ˚ for the mean free path at 300 K for path at room temperature. (I usually use = 300 A a good metal like silver or copper. Thus /Rc = ωc τ ≈ 0.04 at 300 K.) However at low ∗ If my charge carrier are holes, with q = +e, the sense is clockwise. All else is the same.

307

16.1 Charged Particle in a Magnetic Field

temperatures, the mean free path of pure metals can be 100–1,000 times longer, allowing many orbits before a scattering event upsets the electron. As I work through the various optical effects in a magnetic ﬁeld, I’ll see that it is the factor ωc τ that determines how heavy the hand of the magnetic ﬁeld is on the properties of the solid. Large ωc τ , big effect; small ωc τ , modest effect.

16.1.2 Quantum Mechanical Picture After the magnetic ﬁeld is applied, the quantum numbers of the free electron metal, which in zero ﬁeld were {kx ,ky ,kz,σ } where σ is the spin, are no longer good. I can see that they no longer represent stationary states of the Schr¨odinger equation because Eqs. 16.5a and 16.5b show that kx and ky are time dependent. Calculating the energy levels and wave functions of the electrons in a magnetic ﬁeld [347] has been of great interest since the excitement surrounding the quantum Hall effect. Most of the interest centers on the two-dimensional, low-density electron gas, where the quantum Hall effect is observed. But of course the physics is the same in metals, with their much larger Fermi energies.∗ I’ll consider completely free electrons, as in Chapter 8. But the momentum operator differs from that in Eq. 8.1, becoming p = −i h∇ ¯ − (e/c)A, where A is the magnetic vector potential. The Hamiltonin is H = p2 /2m so that the Schr¨odinger equation is 1 e 2 −i h∇ (16.7) ¯ − A ψ = Eψ. 2m c Once I have a vector potential, I have the enjoyment of specifying a gauge. This problem is most simply approached in the Landau gauge, where the vector potential is oriented along ˆ If I take the curl, I ﬁnd ∇ × A = B0 zˆ , which is what I want. ˆ A = B0 x y. y: In Cartesian coordinates, Eq. 16.7 becomes

h¯ 2 h¯ 2 ∂ 2 ψ ∂ eB0 2 h¯ 2 ∂ 2 ψ − i x − ψ − = Eψ. (16.8) − 2m ∂x 2 2m ∂y 2m ∂z2 hc ¯ I separate variables. Try ψ = u(x)eiβy eikz z where the z dependence gives plane-wave solutions along z, with contribution to energy h¯ 2 kz2 /2m. This result is no surprise; the magnetic ﬁeld exerts no force on particles moving in the ﬁeld direction I substitute, cancel the complex exponentials, do a little arrangement of constants in the middle term, and arrive at

h¯ β 2 h¯ 2 ∂ 2 u(x) m eB0 x− + u(x) = E u(x), (16.9) − 2m ∂x 2 2 mc m

∗ The energies in question are the Fermi energy, of order eV in metals but meV in doped semiconductors, and

hω ¯ c , of order meV to perhaps 100 meV, depending on the effective mass and the magnetic ﬁeld.

308

Magneto-Optics with E = E − h¯ 2 kz2 /2m. I’m glad to see ωc = eB0 /mc appearing in Eq. 16.9. This equation is that of a simple harmonic oscillator. I can write it in the conventional form using ωc and by deﬁning x0 = hβ/mω ¯ c as the equilibrium point of the oscillator. Then h¯ 2 ∂ 2 u(x) mωc2 (x − x0 )2 u(x) = E u(x). + 2m ∂x 2 2 The function u(x) is a product of a Gaussian centered at x0 and Hermite polynomials. The energy eigenvalues are

h¯ 2 kz2 1 , (16.10) E = hω n + + ¯ c 2 2m −

with n = 1, 2, 3, . . . the Landau level index. I can view the radius of a Landau orbit as being the classical turning point n = xmax −x0 of the harmonic oscillator. The turning points are found by equating the total energy to the potential energy function.∗ I have h¯ ωc (n + 1/2) = (mωc2 /2)2n or

1 1 2hc 20 ¯ n+ n+ n = = , eB0 2 π B0 2 with 0 = hc/2e the ﬂux quantum. I see that the ﬂux through the lowest Landau level (n = 0), = B0 (π 20 ) is = 0 . In fact there is a single ﬂux quantum through the annulus between level n − 1 and level n for all n. Each Landau orbit n collects all the allowed {kx ,ky } points in the zero-ﬁeld case that exist between it and the one below it in energy. (See Chapter 8.) Because each annulus has the same area, each has the same occupancy. The highest occupied level is that for which hω ¯ c (n + 1/2) = EF . There are orbits in k-space as well; see Eq. 16.6. These are oriented in a plane perpendicular to the ﬁeld, i.e., in the x–y plane. The radius of the orbit with perpendicular 2 /2m = hω (n + 1/2). The orbital radius in k-space is wave vector k⊥n is given by h¯ 2 k⊥n ¯ c then

1 1 2eB0 2π B0 n+ n+ = k⊥n = hc 2 0 2 ¯ with 0 again the ﬂux quantum. Note that k⊥n n = 2(n + 12 ). The Fermi sphere reconstructs into a series of cylindrical shells, separated in energy by hω ¯ c . The energy separation increases as the magnetic ﬁeld becomes larger; the number of Landau levels with energy below the Fermi energy becomes correspondingly smaller. As ﬁeld is increased, a given Landau level’s energy increases from below EF to above EF . The passing of Landau levels through the Fermi energy is responsible for oscillations in susceptibility (de Haas-van Alphen effect) and transport properties (Shubnikov-de Haas effect) as a function of ﬁeld.† Spin adds another magnetic energy, a Zeeman term, Eσ = gμB B0 ms where g is the Land´e g-factor of the electron (just over 2 for free electrons but quite different from 2 in ∗ There are better ways to do this based on correspondence principle or on ﬁnding the maxima of the quantum

mechanical probability.

† Actually the oscillations are periodic in 1/B . 0

309

16.2 Magneto-Conductivity Tensor of a Metal multi-electron atoms), μB = eh/2mc is the Bohr magneton, and ms the z-component of ¯ the electron spin. For free electrons ms = ±1/2 and I take g ≈ 2, making the Zeeman energy become ωc eB0 =± . (16.11) 2mc 2 So the spin down electrons are lowered in energy by an amount equal to the zero-point energy of the Landau levels while the spin up electrons are raised by the same amount. (In solids where there are many electrons in each atom, in cases when spin-orbit interactions are large, and in situations where there are strong crystal ﬁeld effects, g differs very much from the free-electron value.) Eσ = ±h¯

16.2 Magneto-Conductivity Tensor of a Metal Now I want to consider the optical properties of a free-electron metal in a magnetic ﬁeld. I’ll use the concepts of the familiar Drude model as developed in Chapter 8. The metal is subject to an electric ﬁeld, so that I must modify Eq. 16.2 by including E. The three forces to which an electron is subject are the accelerating electric ﬁeld. the deﬂecting magnetic ﬁeld, and the stopping damping force. And this time I cannot neglect damping, characterized by a relaxation time τ . Newton’s law is h¯ e δk dk = −eE − k × B0 − h¯ . (16.12) h¯ dt mc τ I’ll now make a few comments and state a few assumptions: 1. I can’t do what I did in Eq. 8.12 and have the electric ﬁeld along yˆ and the wave traveling ˆ The reason is that the magnetic ﬁeld is ﬁxed to zˆ , and I want to allow for cases along x. where the electric ﬁeld and propagation directions each have components parallel or perpendicular to the magnetic ﬁeld. Hence, I’ll write E = E0 ei (q·r−ωt )

(16.13)

and specify the directions of the electric-ﬁeld vector E0 and wave vector q later. 2. I am operating in the linear∗ regime. As in the case without a magnetic ﬁeld, this assumption means that after any start-up transient decays (requiring time τ ), the time dependence of the electron’s wave vector k follows E, so that dk = −iωk. dt 3. The ﬁeld is along zˆ , so that k × B0 = B0 k × zˆ . 4. I can average over the k values of the occupied states, so that m k = δk = vdrift . h¯ ∗ And isotropic and homogeneous!

310

Magneto-Optics Moreover, δk = k − k0 with k0 the wave vector of the electron in equilibrium and k0 = 0. See the discussion around Eq. 8.14. 5. The current is just the charge density times the average velocity (or the number density n times the electronic charge −e times the drift velocity), j = −nevdrift = −ne

h¯ δk. m

6. As ever, the cyclotron frequency is ωc = eB0 /mc. Equation 16.12 becomes e δk . −iω k = − E − ωc k × zˆ − τ h¯ I can work this problem at least two ways. One is to solve for δk, taking into account assumption 4 and then use assumption 5 to get the current. The other is to use assumption 5 to turn the equation of motion into an equation for the current. I’ll do the latter, substituting δk = k = −(m/neh)j. leave the term containing E ¯ I’ll multiply through by nehτ/m, ¯ on the right, and move all terms containing j to the left, to ﬁnd that my equation of motion has become ne2 τ E. (16.14) m Were it not for the magnetic ﬁeld, this equation would become the Drude formula, Eq. 8.21 or Eq. 4.8. But I do have a magnetic ﬁeld. And I see that Eq. 16.14 tells me that whatever the direction of j (other than along zˆ ), there will be a component of E that is parallel to j and one that is perpendicular to j. Moreover, the factor ωc τ determines (at low frequencies at least) whether the parallel or perpendicular component is the larger. To work out the relation between j and E (the conductivity), it helps to simplify the formulas. I’ll deﬁne as 1 (16.15) ≡ω+i . τ (1 − iωτ )j + ωc τ j × zˆ =

equals ω at high frequencies and i/τ at low frequencies.∗ I’ll also deﬁne σD (ω) as σD (ω) =

ine2 ne2 τ/m = . 1 − iωτ m

(16.16)

σD is just the zero-ﬁeld frequency-dependent Drude conductivity, seen in in Eq. 8.21 or Eq. 4.8. (It was called just σ there.) With these deﬁnitions, I am able to write Eq. 16.14 in a way that resembles Ohm’s law: ωc (16.17) j + i j × zˆ = σD E. ∗ It might seem more direct to deﬁne a complex relaxation time as τ˜ = τ/(1 − iωτ ), making the Drude conductivity be σD = ne2 τ˜ /m. This deﬁnition connects well to the low-frequency conductivity. But shortly I’ll be interested in frequencies near ωc in the case where ωc τ 1 and the use of makes that discussion

easier.

311

16.2 Magneto-Conductivity Tensor of a Metal

The components of Eq. 16.17 are ωc j = σD Ex y ωc jy − i jx = σD Ey

jx + i

(16.18x) (16.18y)

jz = σD Ez,

(16.18z)

where the minus sign in Eq. 16.18y is a consequence of the right-hand rule in the cross product. Equation 16.18 tells me that if I apply an electric ﬁeld in the xˆ direction, I will get currents in both yˆ and xˆ directions. Which current is bigger depends on the value of ωc τ . ↔ I can immediately deﬁne a resistivity tensor ρ which relates electric ﬁeld to current according to ↔

ρ · j = E.

The resistivity tensor is ⎛

1 ρ = ρD ⎝−iωc / 0

↔

iωc / 1 0

⎞ 0 0⎠ 1

(16.19)

where ρD = 1/σD . I must remember that σD is a frequency-dependent complex quantity! ↔ I also want to ﬁnd the conductivity tensor σ , for which ↔

j = σ · E. I could use some matrix inversion method if I want to be sophisticated, but I found it simpler just to go back to the component equations. I can solve Eq. 16.18y for jy , substitute that into Eq. 16.18x, do a bit of algebra, and ﬁnd jx =

σD 2 σD ωc Ex − i 2 Ee y. 2 2 − ωc − ωc2

The coefﬁcient of Ex is σxx and the coefﬁcient of Ey is σxy . Evidently, and not unexpectedly, σxz = 0. Now I go back to Eq. 16.18x and solve for jy and get something very similar. (There is a sign difference in the off-diagonal term.) The zˆ current depends only on the zˆ ﬁeld, so I now know that the conductivity tensor is ⎛

2 2 ⎜ − ωc2 ↔ ⎜ σ = σD ⎜i ωc ⎝ 2 − ω2 c 0

ωc 2 − ωc2 2 2 − ωc2 0

−i

⎞ 0 ⎟ ⎟ , 0⎟ ⎠

(16.20)

1

with σD = ine2 /m = ne2 τ/m(1 − iωτ ). (I remind myself that = ω + i/τ .) Note that the conductivity tensor and the resistivity tensor are explicitly antisymmetric. Thus, there is no way to orient someting to make them diagonal.

312

Magneto-Optics

16.2.1 Hall Effect The Hall effect is a consequence of the off-diagonal terms in the magnetoconductivity tensor [19, 348]. Discovered by Edwin Hall [349] in 1879, the effect is the appearance of an electric ﬁeld in a conductor at right angles to the electrical current in the conductor when there is a magnetic ﬁeld perpendicular to the current. It is the basis of a large number of sensors; Hall devices are used to measure magnetic ﬁelds, make noncontact current measurements, and sense rotational speeds of engines. The Hall effect as it usually is experienced is a low-frequency phenomenon, so I’ll take ωτ 1, making = i/τ and σD = ne2 τ/m. The geometry of a Hall device is simple: it is a rectangular prism of thickness t, width w, and length L, often called a Hall bar. A current ﬂows along the length of the device, in the xˆ direction. (If the charge carriers are electrons, they ﬂow in the −xˆ direction.) A magnetic ﬁeld is oriented along zˆ . The Lorentz force will accelerate the electrons in the −yˆ direction. The electrons cannot escape from the device so they pile up along the −y edge of the device, making that side negatively charged. The other side is depleted of electrons and becomes positively charged. The charge imbalance creates an electric ﬁeld, the Hall ﬁeld, from plus to minus; this ﬁeld exerts a force on the electrons in the +yˆ direction.∗ The charge buildup stops when the Hall electrical force balances the Lorentz magnetic force. The Hall coefﬁcient RH is deﬁned via Ey = RH B0 jx .

(16.21)

With current only in the xˆ direction, the resistivity tensor gives the ﬁelds induced by this current. They are: Ex = −ρD jx Ey = −ρD ωc τjx . Evidently RH B0 = −ρD ωc τ = −

eB0 τ m . · mc ne2 τ

There are some cancellations, after which I ﬁnd 1 . nec RH is negative because electrons are negative. The Hall effect allows measurement of the carrier density. Moreover, if the charge carriers are positive holes instead of negative electrons, RH will be positive. The electric ﬁeld in the direction of current, Ex , is often called the longitudinal ﬁeld. It is independent of magnetic ﬁeld strength in this model.† The electric ﬁeld in the transverse direction, the Hall ﬁeld, grows without limit. Surfaces are not required to have the Hall RH = −

∗ Why, oh why, did Franklin not choose the other signs for vitreous and resinous electricity? † A result contradicted by experiment.

313

Fig. 16.2

16.2 Magneto-Conductivity Tensor of a Metal

The electric current and electric field in a metal (whose charge carriers are negative) with a strong magnetic field along the zˆ axis. ﬁeld or a Hall current. In fact, I only put the surface in to make contact with the Hall bar geometry used to measure the Hall coefﬁcient. Figure 16.2 shows the relation between current and electric ﬁeld inside the material. The external magnetic ﬁeld is (as always) along zˆ . The current j is in the xˆ direction and there is a component of the electric ﬁeld Ex along the current. The Hall ﬁeld in Fig. 16.2, along −yˆ (because electrons are negatively charged), is larger than the longitudinal ﬁeld; the diagram is drawn for ωc τ ≈ 3. The angle between j and E is the Hall angle, θH . The Hall angle satisﬁes tan θH = ωc τ . As ωc τ increases from zero to a large value—by increasing B0 or decreasing temperature∗ —the Hall angle increases from zero to 90◦ . This free electron model does a moderately good job of describing simple metals. For me to take it seriously, I’d like for experiment to observe a Hall coefﬁcient that is independent of magnetic ﬁeld and current, so that EH is linear in B0 . I’d also like for RH to be independent of temperature in metals and to agree with the thermal generation of free carriers for semiconductors. For the elements that are metals, one can list −necRH , which of course should be unity. To test whether it is, I need to know the carrier density n by other means. I can get it from transport (if I know τ ). I can get it from chemistry. I can get it from electronic structure calculations. I can get it from the square of the plasma frequency. Here, I’ll get it from Table 8.1. Then I ﬁnd at high ﬁelds and low temperatures ⎧ ⎪ ⎪ ⎨1.0 ± 0.1 Na,K,Cs,Rb −necRH = 1.4 ± 0.2 Cu,Ag,Au ⎪ ⎪ ⎩−0.3 Al (at high ﬁelds). The alkali metals behave as I expect them to because I know that they lose their single valence electron easily and that their Fermi surfaces are close to spherical. The noble metals appear to have fewer carriers than their reputation as monovalent metals would suggest. To understand this deﬁcit I have to look at their Fermi surfaces [19, 23] and notice the necks and the possibility of a number of “orbits” that the k vector can take in the ﬁeld. Aluminum starts by having the wrong sign, suggesting positive carriers, and only one hole per atom. This result is a surprise to the free-electron picture but actually not uncommon. Many metals have positive Hall coefﬁcients. It is a consequence of their electronic band structure. Another consequence (observed in aluminum among others) is that the Hall ∗ Increasing B will always make ω τ bigger; decreasing temperature may or may not do the trick. It depends c 0

on the cleanliness and the physics of the material.

314

Magneto-Optics

coefﬁcient has different values in low-ﬁeld and high-ﬁeld regimes, where the crossover occurs when ωc τ = 1. Indeed, at high ﬁelds the Landau level spacing begins to dominate and Shubnikov-de Haas oscillations [19, 350] in resistivity and Hall effect can be seen.∗

16.2.2 The Dielectric Tensor Now that I know the conductivity tensor, I can think about how electromagnetic waves propagate in a metal subject to a static magnetic ﬁeld. I’ll keep the static ﬁeld B0 along the zˆ axis and orient the wave vector and electric ﬁeld directions relative to that. The waves are governed by the complex frequency-dependent conductivity tensor, as written in Eq. 16.20, or, equivalently, the dielectric tensor. And, as ever and ever, by Maxwell’s equations. I can use either the conductivity or the dielectric tensor† to develop the solutions for wave propagation. I’ll make the same choice that I did in Chapter 2 and use the dielectric tensor. In terms of the tensor of Eq. 16.20, I write ↔

↔

(ω) = c 1 +

4π i ↔ σ ω

(16.22) ↔

where c is the (scalar) high-frequency contribution,‡ 1 is the unit tensor, one on the diagonals, 0 on the off diagonals. I’ll now write the dielectric tensor explicitly. As before, I deﬁne a plasma frequency ωp = 4π ne2 /m so that σ D = iωp2 /4π . After a bit of algebra I obtain ⎛ ⎞ ωp2 ωp2 ωc −i 0 ⎜ c + ⎟ ω(ωc2 − 2 ) ω(ωc2 − 2 ) ⎜ ⎟ ⎜ ⎟ 2 2 ↔ ωp ωc ωp ⎟. =⎜ (16.23) ⎜ i ⎟ + 0 c ⎜ ω(ωc2 − 2 ) ⎟ ω(ωc2 − 2 ) ⎝ ⎠ ωp2 0 0 c − ω The ﬁrst two diagonal components are equal, xx = yy . If ωc τ 1, these quantities have a sharp resonance at ω = ωc ; their real parts are positive below ωc and negative above √ it. (They will cross zero again at ωp / c .) The third diagonal component, zz , has the dielectric function of a Drude metal, identical to Eq. 4.13. The nonzero off-diagonal components are opposites: xy = −yx . They display the same resonance near ωc as the diagonal terms do. At ﬁrst glance, they may appear to be pure imaginary, but = ω + i/τ is complex, so the off-diagonal terms are also complex.§ ∗ I have neglected up to now to mention the very interesting and very well known quantum Hall effect. I’ll just

say that it is beyond the scope of this book, as are the Shubnikov-de Haas oscillations and related quantum oscillations. † But not both! ‡ In Section 16.5, I’ll show that the dielectric function of an insulator (and is the simplest representation of an c insulator I can think of) is also a tensor when a magnetic ﬁeld is applied. For the time being, I’ll pretend that this is not the case. § Because xy = −yx , the imaginary part of one of the two off-diagonal terms will be negative. Generally, negative imaginary parts of dielectric functions – or negative real parts of conductivities – are forbidden by energy conservation. Here, because for example σxy relates the x component of current to the y component of electric ﬁeld, the corresponding part of j · E = 0.

315

16.3 Electromagnetic Wave Propagation

16.3 Electromagnetic Wave Propagation Now I will think about the propagation of electromagnetic waves in this metal. Making another visit to Maxwell’s equations, I continue to write the electric and magnetic ﬁelds of the light as complex plane waves, as in Eqs. 2.5 and 2.6. I also have ↔

D = · E, so that D is not parallel to E. I start with Maxwell’s equations, Eqs. 2.4a–2.4d, in local, nonmagnetic, homogeneous, and linear materials. After substituting the plane-wave ﬁelds into Maxwell’s equations, I have ↔

q· ·E=0 q·H=0 ω q×E= H c ω↔ q × H = − · E. c

(16.24a) (16.24b) (16.24c) (16.24d)

I look at these equations for a bit and see that H is perpendicular to both E and q but that E and q are not perpendicular to each other. The next step is to combine things in the usual way so as to eliminate H. I take the cross product of q with Eq. 16.24c, use the BAC−CAB rule on the triple cross product, and replace q × H using Eq. 16.24d: ω q×H c ω2 ↔ q(q · E) − q 2 E = − 2 · E. c q × (q × E) =

(16.25)

In principle, there will be components of the propagation vector q and the electric ﬁeld E along all three Cartesian axes. However, the only physics distinction is between zˆ and perpendicular to zˆ . An electron running along yˆ is deﬂected towards xˆ and one running ˆ So, without loss of generality, I can rotate the x–y plane along xˆ is deﬂected toward −y. until q has only components along xˆ and zˆ : q = qx xˆ + qz zˆ = q sin θ xˆ + q cos θ zˆ where θ is the polar angle, as illustrated in Fig. 16.3. Note that I can not do what I did for anisotropic crystals (Section 15.6.3), which was to consider independently the cases of electric ﬁeld parallel and perpendicular to the x–z plane. The dielectric tensor (or conductivity tensor) has intrinsically off-diagonal components, so there is always a component of E parallel to the current and a (Hall) component perpendicular to it. Thus I can only write E = Ex xˆ + Ey yˆ + Ez zˆ .

(16.26)

316

Fig. 16.3

Magneto-Optics

The wave vector q is in the x–z plane, at an angle θ to the zˆ axis. Proceeding, I deﬁne the complex refractive index N via ω ω (16.27) q = N sin θ xˆ + N cos θ zˆ . c c I look at Eq. 16.25 and see that when Eqs. 16.26 and 16.27 are substituted, there will be a common factor of ω2 /c2 everywhere. I do the substitutions, cancel this factor, collect the components, making use of yy = xx and yx = −xy in Eq. 16.23 to obtain 0 = [(xx − N 2 cos2 θ )Ex + xy Ey + N 2 cos θ sin θ Ez ]xˆ + [−xy Ex + (xx − N 2 )Ey ]yˆ 2

(16.28) 2

2

+ [N cos θ sin θ Ex + (zz − N sin θ )Ez ]ˆz. For a vector to be zero, all three components must be zero; thus, Eq. 16.28 is actually three equations. I use the zˆ component to ﬁnd a function representing Ez and the yˆ component to do the same for Ey , substitute these into the xˆ component, cancel Ex , and obtain an equation for N 2 in terms of θ , xx , and xy . At ﬁrst it appears to be a cubic equation, but the N 6 terms add to zero, so it is quadratic: 0 = N 4 (xx sin2 θ + zz cos2 θ ) 2 2 − N 2 [xx zz (1 + cos2 θ ) + (xx + xy ) sin2 θ ]

(16.29)

2 2 + (xx + xy )zz .

Although I know how to solve quadratic equations, I ﬁnd that I gain no insight in writing the general solution for N 2 .∗ Instead, I will consider two special cases.

16.3.1 Faraday Geometry: Wave Vector Parallel to Field First, I set qˆ = zˆ ; θ = 0. In this case, Eq. 16.29 becomes 2 2 + xy 0 = N 4 − 2N 2 xx + xx

↔ ∗ I did check that if there is no magnetic ﬁeld, so that ↔ = 1 , then N 2 = .

317

16.3 Electromagnetic Wave Propagation

the solutions to which are N±2 = xx ± ixy .

(16.30)

I use N± in Eq. 16.28 (the yˆ component) to ﬁnd Ey = ±iEx . The zˆ component gives Ez = 0. Thus I have transverse waves (q · E = q zˆ · E = 0). I can go back to Eqs. 15.17 or 16.25, or even to Maxwell’s equations, and ﬁnd that the solutions are circular polarized ˆ (qz−ωt ) E± = E0 (xˆ ± i y)e with q = (ω/c)N± . See Eq. 15.4; the minus sign is for right circular polarization and the plus is for left circular polarization.∗

16.3.2 Cyclotron Resonance and Helicons The normal modes of the metal in a magnetic ﬁeld and with propagation along the ﬁeld direction are circularly polarized light. I’ll deﬁne the dielectric functions of the circular polarized modes as ± ≡ N±2 = xx ± ixy , where the components are given in Eq. 16.23. Writing these out, ± = c +

ωp2 ( ± ωc ) ω(ωc2 − 2 )

.

This formula looks ﬁne and has a nice resonant denominator, but I notice that ωc2 − 2 = (ωc + )(ωc − ), allowing me to write the dielectric function for the left circular polarization as + = c +

ωp2 ω(ωc − )

= c +

ωp2 ω(ωc − ω) − iω/τ

,

(16.31)

.

(16.32)

while that for the right circular polarization is − = c −

ωp2 ω(ωc + )

= c −

ωp2 ω(ωc + ω) + iω/τ

I have inserted in the rightmost formulas the deﬁnition = ω + i/τ . There are big differences in the behavior of + and − , especially in the case where ωc τ 1. + is positive from ω = 0 to ω = ωc . Above ωc it is negative and remains negative up to the screened plasma frequency. − is negative at all frequencies up to the screened plasma frequency, just as in the case of zero magnetic ﬁeld. Figure 16.4 shows the real parts of the conductivity, σ 1+ , and dielectric function, 1+ , for a pure metal in zero ﬁeld and in ﬁelds of 10, 30, 100, and 300 kG (1, 3, 10, and 30 T). ∗ See footnote in Section 15.2.3 about the conventions in use.

318

Fig. 16.4

Magneto-Optics

(a) Faraday geometry conductivity for the + polarization (left circular polarization) of a pure metal with zˆ -axis magnetic field. (b) Real part of the dielectric function in the same configuration. Note that the dielectric function values have been divided by 109 before plotting.

The metal is described by Eq. 16.31 with parameters chosen to represent silver or copper at low temperatures: ωp = 70,000 cm−1 (8.5 eV) and 1/τ = 0.1 cm−1 . The corresponding scattering time, τ = 50 ps, gives a mean free path = 80 μm and a resistivity ratio RRR = 1,300. The cyclotron frequencies of the conduction electrons are 0.93, 2.8, 9.3, and 28 cm−1 at the four ﬁelds so that the product ωc τ increases from 10 at 10 kG to 300 at 300 kG. The zero-ﬁeld conductivity and the zero-ﬁeld 1 (ω) follow the Drude form (shown in Fig. 4.4). The conductivity rolls off as frequency increases, following σ1 ∼ 1/ω2 at high frequencies. The dielectric function is negative, also going as 1 ∼ −1/ω2 . Things change dramatically when the ﬁeld is applied. The low frequency conductivity is suppressed, more and more with increasing ﬁeld. The suppression is consistent with the tensor conductivity of Eq. 16.20, although I need to remember that I am plotting only the real part of σ+ = σxx + iσxy . There is a strong resonance at ω = ωc . This cyclotron resonance carries most of the spectral weight originally associated with the DC conductivity. The maximum conductivity is σ1 (ωc ) = ωp2 τ/4π , the same as the DC conductivity. The resonance becomes sharper as ﬁeld increases, because ωc τ is linear in the ﬁeld. The conductivity in ﬁeld is close to that in zero ﬁeld for ω ωc ; this behavior continues to high frequencies. The real part of the dielectric function, 1+ , has even more dramatic changes when the ﬁeld is applied. It is positive for all ω < ωc . A positive 1+ , along with an 2+ that is not too large, implies a region of transparency in the metal.

319

16.3 Electromagnetic Wave Propagation

(a) Fig. 16.5

(b)

(a) Refractive index for the + polarization (left circular polarization) of a pure metal in with zˆ -axis magnetic fields in the Faraday geometry. (b) Absorption coefficient in the same configuration. Note that the absorption coefficient values have been divided by 106 before plotting. The optical constants that govern wave propagation are shown in Fig. 16.5. The left panel shows the real part of the refractive index and the right shows the absorption coefﬁcient of a metal in a strong ﬁeld. The zero-ﬁeld curve is the same as in the Drude model discussion. √ (See Fig. 4.5. The zero-ﬁeld absorption coefﬁcient starts off as ω and then ﬂattens out when ωτ 1.) In a strong ﬁeld, the refractive index is large, of order n ≈ 104 –105 . Consequently, electromagnetic wave propagation is slow, v = c/n ≈ 105 –106 cm/s. The absorption coefﬁcient is small for frequencies below the cyclotron frequency. There is a strong and narrow peak when ω = ωc (the cyclotron resonance absorption) and then a decrease to the zero ﬁeld value.∗ The transmission of circularly polarized electromagnetic radiation at frequencies below the cyclotron resonance goes under several names: helicons, Alfv´en waves, and whistlers [351]. Helicons have been seen in many clean metals, including potassium, sodium, indium, aluminum, and bismuth [352, 353]. Cyclotron resonance requires ωc τ > 1 to give the appearance of a resonance in the spectrum. Figure 16.6 shows the effect of changing the scattering time τ from ωc τ = 30 to ωc τ = 0.2. If ωc τ ≈ 1, the resonance is not observed. If I wanted to take the maximum in α when ωc τ = 1 as corresponding to the cyclotron frequency, I would obtain too large a value for the resonance frequency. The absorption curve sharpens for higher values of ωc τ . (I observe the same thing in Fig. 16.5b, where I am varying ωc and keeping τ constant.) ∗ Note that Fig. 16.5 shows a small absorption coefﬁcient below the cyclotron frequency, but it is only small relative to zero ﬁeld value. The parameters that I used give α(ω = 1 cm−1 ) = 300 cm−1 . The transparency

is relative; a slab of a 100 μm thickness might transmit 5% of the light that enters on the incident side to the far side. The reﬂection losses will be pretty impressive as well, given that n ≈ 105 !

320

Fig. 16.6

Magneto-Optics

Absorption coefficient of a metal for four values of the scattering time τ . The cyclotron frequency is ωc = 28 cm−1 .

16.3.3 Cyclotron Resonance in Semiconductors So far in this chapter, I have worked out and discussed the magneto-optics of metals. In actuality, the magneto-optics of semiconductors are equally if not more interesting and are more commonly measured [354, 355]. There are a number of reasons for this: 1. An important parameter of a semiconductor is the effective mass of the charge carriers, and measuring the cyclotron frequency, ωc = eB/m∗ c, gives this unambiguously. 2. It is common for m∗ to be smaller than the free electron mass, making the resonance frequency somewhat higher than for free electron metals and in a more accessible spectral region.∗ 3. The carrier density is three to four orders of magnitude smaller, making ωp = 4π ne2 /m∗ quite a bit smaller. The dielectric function and conductivity scale as ωp2 so the lower carrier density leads to smaller absorption, an effect somewhat counteracted by the smaller effective mass.† 4. Semiconductors may have carriers in several bands (electrons in the conduction band, light, heavy, and split-off holes in the valence band) and with anisotropic effective mass ellipsoids. Each has its own effective mass, adding richness to the cyclotron resonance spectra. 5. Although the doping process introduces impurities into the crystal lattice, semiconductors can have high mobilities, so that ωc τ > 1 can be achieved.

∗ For example, the conduction-band effective mass in GaAs is m∗ /m = 0.067, making the 100 kG (10 T) e cyclotron frequency ωc = 139 cm−1 . Measurements at this frequency with commercial infrared spectrometers is easier than at 9.3 cm−1 , the resonant frequency for free-electron metals at this ﬁeld. † It is the ratio n/m∗ that matters.

321

Fig. 16.7

16.3 Electromagnetic Wave Propagation

(a) Faraday geometry conductivity for the − polarization (right circular polarization) of a hole-doped semiconductor with a 100 kG zˆ -axis magnetic field and with zero field. (b) Real part of the dielectric function in the same configuration. There are two peaks because the model includes holes with two different effective masses. The DC conductivity of a semiconductor is often written in terms of the mobility. Suppose there are both electrons (number density n and mobility μe ) and holes (number density p and mobility μh ). Then the DC conductivity is σ = neμe + peμh .

(16.33)

If I compare Eq. 16.33 with the Drude DC conductivity, Eq. 4.9, I see that μ = eτ/m∗ , with subscript for electron or hole, as appropriate. Then, looking at Eq. 16.4, I notice that the product of cyclotron frequency and scattering time, ωc τ , can be written μB0 eB0 τ = , (16.34) ∗ m c c for each electron band and for each hole band in the semiconductor. The mass m∗ written here and m in Eq. 16.4 both represent the effective mass of the charge carriers. Equation 16.34 then speciﬁes μB0 /c 1 as the requirement to see cyclotron resonance.∗ To illustrate cyclotron resonance, I’ll take the carrier density n = 5 × 1017 cm−3 , about 100,000 times lower than in a metal and about ten times lower than the concentration for the metal–insulator transition in doped silicon [356–358]. Effective masses in semiconductors range from 0.01 to nearly 1; I’ll assume that the carriers live in two bands, one with m∗ = 0.1me and the other with m∗ = 0.5me . These are representative values for the case where there are light and heavy holes bands at the top of the valence band. Finally, I’ll do the calculation for a ﬁeld of 100 kg (10 T) and for μ = 3 × 104 cm2 /volt-sec = 1 ×107 cm2 /statvolt-sec. The results are shown in Fig. 16.7. The optical conductivity has peaks at each of the two cyclotron resonance frequencies. The frequencies are set by the carrier effective mass. The lower peak is broader (because the cyclotron frequency is lower and I took identical scattering rates of 1/τ = 3 cm−1 for both carrier types) and has lower oscillator strength (because the carrier densities are identical but the effective masses are not). The real part of the dielectric function is positive below the ωc τ =

∗ See Appendix A for a discussion of units. The mobility here is expressed in cm2 /statvolt-sec, 300 times larger than mobility reported in cm2 /volt-sec in most handbooks. (And, the ﬁeld is in Gauss!)

322

Magneto-Optics

Electrons

Electrons

Holes

Fig. 16.8

Holes

Swept-frequency cyclotron resonance data for silicon. (After Ref. 354.) lower resonance (and for some frequencies between the resonances). The semiconductor will be transparent (for thickness of a few millimeters) below the lower resonances as well as between the resonances and above the screened plasma frequency. Wave velocities in the semiconductor are smaller than in vacuum but not so small as in a metal. At ω = 1 cm−1 , the parameters used give n = 70. I’ve calculated spectra at (several) ﬁxed ﬁeld values. One way to study cyclotron resonance is to measure the absorption∗ spectrum at ﬁxed ﬁeld. In principal this method is best, because many quantities which affect the resonances could be ﬁeld dependent, and the spectra can be measured at ﬁeld up to the maximum available in the laboratory. Another method is to shine a monochromatic electromagnetic wave on the sample and sweep the magnetic ﬁeld. There will be absorption as each and every type of charge carrier comes into resonance. An example [354] of such an experiment is shown in Fig. 16.8. If the incident radiation has left or right circular polarization, then only orbits due to electrons or holes will be seen. If it is linearly polarized,† then both will be seen, as I can decompose linear polarization into the sum of left and right circular polarizations. Figure 16.8 was measured with linear polarization. Four absorption peaks are shown in Fig. 16.8. Two (the lowest ﬁeld and the highest ﬁeld) are associated with the light holes and heavy holes, respectively. The other two are for electrons. There are two frequencies for electrons because the conduction band has an anisotropic effective mass tensor. Cyclotron resonance played a big part in determining silicon’s band structure.

16.3.4 Voigt Geometry To use Voigt geometry I orient q perpendicular to the magnetic ﬁeld. I look at Fig. 16.3 and ˆ ω/c, making θ = 90◦ . Then, Eq. 16.28 becomes Eq. 16.27, write q = xN 0 = [xx Ex + xy Ey ]xˆ + [−xy Ex + (xx − N 2 )Ey ]yˆ + [(zz − N 2 )Ez ]ˆz. ∗ Or transmission, or reﬂection, or conductivity. † Or unpolarized, but see the discussion in Section 15.2.2.

(16.35)

323

16.3 Electromagnetic Wave Propagation Here, I can put the electric ﬁeld either parallel or perpendicular to the zˆ axis (the ﬁeld direction). In the ﬁrst case, Ez = 0 and Ex = Ey = 0, I get N 2 = zz . This is the same result I would get if there were no magnetic ﬁeld. So, the wave with this polarization is insensitive to the magnetic ﬁeld. Of course, I expect this result on physics grounds: the electric ﬁeld Ez gives currents along zˆ and the Lorentz force, proportional to v×B, is zero.∗ The case when the electric ﬁeld is in the x–y plane is more interesting. I use the xˆ component of Eq. 16.35 to ﬁnd that the longitudinal ﬁeld is related to the transverse ﬁeld by Ex = −(xy /xx )Ey . Next, I substitute Ex into the yˆ component and obtain N 2 ≡ ⊥ = xx +

2 xy

xx

,

where ⊥ is meant to indicate that this is the dielectric function for a wave traveling in the plane perpendicular to the static magnetic ﬁeld. Now, the off-diagonal component is linear in ωc , so the Voigt geometry gives an effect which is quadratic in the ﬁeld. I insert the components from Eq. 16.23 and, after a bit of algebra, arrive at ωp2 ω˜ p2 − 2 , ⊥ = c − ω2 ω˜ p2 ( /ω) + ωc2 − ω √ where ω˜ p = ωp / c is the screened plasma frequency. 2 There is a resonance near ω˜ p + ωc2 but a zero just below that, near ω˜ p . To see the behavior a bit more clearly, I’ll take the high frequency limit.† I set ωτ 1, making ≈ ω. After further algebra, the dielectric function becomes: ⊥ = c −

ωp2

ωc2 ωp2 + . ω2 (ω˜ p2 + ωc2 − ω2 )ω2

(16.36)

The ﬁrst two terms in Eq. 16.36 are the dielectric function of free electrons (or the Drude model when ωτ 1). The third term is a consequence of the magnetic ﬁeld. It is 2 proportional to B0 through ωc and has a resonance at ω = ω˜ p2 + ωc2 . The wave in Voigt geometry has components parallel and perpendicular to the propagation direction. Taking qˆ = xˆ I ﬁnd ω˜ p2 (ωc /ω) xy Ex =− =i 2 . Ey xx ω˜ p ( /ω) + ωc2 − ω2 This ratio has a maximum near ωp2 + ωc2 . At frequencies below the plasma frequency, I can simplify in one of two ways: ⎧ ω ⎪ 1/τ ω ω˜ p, ⎨i ωc Ex = ⎪ Ey ⎩ω τ ω 1/τ . c and I’d want ωc τ 1 as usual. ∗ Remember: j = nev. † The plasma frequency is the highest frequency in the problem, followed by the cyclotron frequency, and then

by the scattering rate.

324

Magneto-Optics

16.4 Other Magneto-Optical Effects Here I will mention brieﬂy some of the variety of magneto-optical effects that one may observe. There are a number of these; in the main they are consequences of off-diagonal tensor components as seen in Eqs. 16.20 and 16.23. In turn, such components arise in magnetized material, either from an applied ﬁeld or from intrinsic magnetization. Faraday rotation. There is a rotation of the plane of polarization for linearly polarized light transmitted through transparent materials with qˆ along the magnetic ﬁeld direction.∗ The refractive indices for the two circular polarizations differ, and therefore so do the velocities. I will work out Faraday rotation in the next section. Magnetic circular dichroism. The absorption coefﬁcient for right and left circular polarization in the Faraday geometry differ. The dielectric function for cyclotron resonance and for helicons (Eqs. 16.31 and 16.32) is an extreme example of magnetic circular dichroism. See Fig. 16.5. Linear magnetic birefringence. In the Voigt geometry, the material exhibits different refractive indices for polarizations parallel and perpendicular to the magnetic ﬁeld. Magnetic linear dichroism. The absorption differs for electric ﬁeld parallel and perpendicular to the external ﬁeld (in the Voigt geometry). Magneto-optic Kerr effect. There is a change of polarization state when light is reﬂected from a material subject to a magnetic ﬁeld. If I send in linearly polarized light, I may receive elliptically polarized light. But I may also observe linear polarization with the plane of polarization rotated. The experimental conﬁgurations may vary: one needs to distinguish the direction of the magnetization vector with respect to the reﬂecting surface, the direction of the magnetization vector with respect to the plane of incidence,† and the polarization direction of the incident light. The Kerr rotation is linear in the strength of the applied magnetic ﬁeld. Voigt effect. This effect is like the Kerr effect except that the rotation is quadratic in ﬁeld strength. Because all these magneto-optical effects are small, the quadratic ones are very weak compared to the linear ones. The Voigt effect is sometimes called the Cotton-Mouton effect, but I think the Cotton-Mouton effect is really an effect of alignment of magnetic nanoparticles in a ﬂuid. Magnetic resonance. Electrons and nuclei have spin, and a magnetic dipole moment due to that spin degree of freedom. In a magnetic ﬁeld, an electromagnetic ﬁeld of the right frequency will induce a transition from a lower to a higher quantized energy level of the dipole. Among the possibilities are nuclear magnetic resonance [359], electron spin resonance (or electron paramagnetic resonance) [360, 361], ferromagnetic resonance [362, 363], and antiferromagnetic resonance [364]. In the latter two, the internal order of the spin system plays a big role.

∗ The geometry is the “Faraday geometry” that I used in Section 16.3.1. † The plane of incidence is a plane containing the surface normal and the (non-normal) incident and reﬂected

wave vectors. The electric ﬁeld may be parallel or perpendicular to this plane.

325

16.5 Faraday Rotation in an Insulator

Magnetoelectric effect. In the class of materials now called “multiferroics,” there is coupling of ferroelectric and ferromagnetic degrees of freedom. An electric ﬁeld will affect the magnetization and a magnetic ﬁeld. Moreover, exotic spin excitations exist: electroactive magnons (or electromagnons), spin waves that are excited by electromagnetic ﬁelds and observed in the infrared spectrum [365–367]. These are all very interesting topics, but, except for Faraday rotation, I’ll not discuss these (or other magneto-optical effects) further.

16.5 Faraday Rotation in an Insulator Faraday rotation was discovered in 1845 when Michael Faraday observed the rotation of the polarization direction in plane-polarized light it traversed a glass rod in a magnetic ﬁeld. The geometry had the light propagation direction parallel to the magnetic ﬁeld direction. The amount of rotation increased with the ﬁeld and with the length of the rod. I can see three approaches to this problem. (1) I can say that the difference between a metal, which has at zero-ﬁeld the Drude dielectric function given by Eq. 4.13, and an insulator, with the Lorentz dielectric function of Eq. 4.31, is the restoring force of the bound electrons. This restoring force leads to a resonant frequency at ωe in the Lorentz oscillator. The metal has a pole at the origin and the insulator has one at the resonant frequency. So all I need to do is to shift the origin and put the resonant frequency into Eqs. 16.31 and 16.32. (2) A second approach would be essentially to duplicate the earlier sections of this chapter. Start with an equation of motion that includes the restoring force; ﬁnd the dielectric tensor; use that tensor in Maxwell’s equations for arbitrary qˆ and eˆ directions; and ﬁnally simplify to the geometry of the Faraday effect. (3) The third approach, which I will adopt, is to solve the equation of motion for the bound carriers to obtain the dielectric (or susceptibility) tensor, form the left and right circular combinations, and then consider the propagation of circularly-polarized light in the material.

16.5.1 The Susceptibility Tensor I start with the equation of motion I used for bound electrons, Eq. 4.20, and include the Lorentz force from the static magnetic ﬁeld B0 in the sum of forces on the right, e m¨r = −mω02 r − mγ r˙ − eE − r˙ × B0 . (16.37) c As usual, I’ll take an e−iωt time dependence for r and for E, so that r˙ = −iωr and r¨ = −ω2 r. Next, I will write the dipole moment/unit volume as P = −ner, with n the number density of the bound electrons, as usual. Third, I will make the local ﬁeld correction as done in Chapter 4 (Section 4.4). Here, this correction consists of replacing ω0 with ωe . With these three things done, I have this equation for the dipole moment/unit volume: (ωe2 − ω2 − iωγ )P −

iωe ne2 P × B0 = E. mc m

(16.38)

326

Magneto-Optics Alertly, I recognize in Eq. 16.38 a cyclotron frequency ωc = eB0 /mc and a plasma 2 4π ne /m. It helps to write the components of frequency (as in Eq. 4.31) ωpe = Eq. 16.38. I’ll take, as I did earlier, B0 = B0 zˆ . Then the z component does not contain the magnetic ﬁeld; in fact, it is identical with what I would get in the zero-ﬁeld situation. The other two components do contain the ﬁeld.∗ (ωe2 − ω2 − iωγ )Px − iωωc Py = (ωe2 − ω2 − iωγ )Py + iωωc Px = (ωe2 − ω2 − iωγ )Pz = ↔

2 ωpe

4π 2 ωpe 4π 2 ωpe 4π

Ex Ey

(16.39)

Ez .

↔

It is clear that I must write P = χ · E, with χ the electric susceptibility tensor. This tensor has the same format as Eqs. 16.20 and 16.23. There are four distinct elements; the diagonal elements satisfy χ xx = χ yy = χ zz while the nonzero off-diagonal components obey χ yx = −χ xy .

16.5.2 The Refractive Index for Circular Polarization Here, I want to consider the case where qˆ is along zˆ , i.e., waves propagating along the magnetic ﬁeld. This situation is the Faraday geometry, which I discussed for metals in Section 16.3.1. The analysis of ﬁeld there applies here too: Maxwell’s equations will give transverse plane waves, with E in the x–y plane. However, instead of solving for Px and Py , I note that I see a sort of symmetry in Eq. 16.39, with Px − iF (ω)Py ∝ Ex and Py + iF (ω)Px ∝ Ey , where F is the function F (ω) = iωωc /(ωe2 − ω2 − iωγ ). Instead of plane polarized ﬁelds, let me take circular polarized ﬁelds. I will write the electric ﬁeld and the polarization vector in the plane perpendicular to the magnetic ﬁeld as E⊥ = E+ + E− and P⊥ = P+ + P− where ˆ + E+ = (xˆ + i y)E ˆ − E− = (xˆ − i y)E ˆ + P+ = (xˆ + i y)P ˆ −, P− = (xˆ − i y)P where E+ , E− , P+ , and P− are the complex amplitudes of the four ﬁelds. By choice of these amplitudes and their phases, I can construct any speciﬁc xy-plane ﬁeld. The components of these ﬁelds are Ex = xˆ · (E+ + E− ) = E+ + E− Ey = i(E+ − E− ) Px = P+ + P− Py = i(P+ − P− ). ∗ Actually they contain the cyclotron frequency.

327

16.5 Faraday Rotation in an Insulator

Now, I substitute these components into the ﬁrst two lines of Eq. 16.39, multiplying as I do the second by −i, to ﬁnd (ωe2 − ω2 − iωγ )(P+ + P− ) + ωωc (P+ − P− ) = (ωe2 − ω2 − iωγ )(P+ − P− ) + ωωc (P+ + P− ) =

2 ωpe

4π 2 ωpe

(E+ + E− )

(E+ − E− ). 4π First I add these and then subtract them. A small amount of algebra leads me to P+ = P− =

2 /4π ωpe

ωe2 + ωωc − ω2 − iωγ 2 /4π ωpe

ωe2 − ωωc − ω2 − iωγ

E+ ≡ χ + E+ E− ≡ χ − E− .

I will deﬁne as usual the dielectric function as = c + 4π χ with c the high frequency value of . Then, 2 ωpe . (16.40) + = c + 2 ωe + ωωc − ω2 − iωγ − = c +

2 ωpe

ωe2 − ωωc − ω2 − iωγ

.

(16.41)

The effect of the ﬁeld is to shift the resonance to higher frequencies for the E+ circular polarization and to lower frequencies for the E− circular polarization. One almost always has ωe ωc ; the energy gap is probably in the near infrared or visible (0.5–5 eV) while the cyclotron frequency is in the far infrared (1 meV). One also wants ωpe to be large enough to give a reasonable infrared refractive index.∗ Finally, ωc γ makes the absorption small at frequencies where the Faraday effect is important.† The optical frequency ω must clearly be below ωe for small absorption. For simplicity, I can set γ = 0 and consider that ± is a real function representing the dispersion of the material for frequencies below ωe , the electronic absorption edge.‡ With γ = 0, the dielectric function and refractive index are real. These functions differ for the two circular polarizations. The refractive indices are 2 ωpe √ (16.42) n+ = + = c + 2 ωe + ωωc − ω2 for the left circular polarization (E+ ) and √ n− = − = c +

2 ωpe

ωe2 − ωωc − ω2

(16.43)

for the right circular polarization (E− ). Clearly, n− > n+ . ∗ As far as desirable values for the ratio of ω to ω go, I’d look for anything from 1.1 to 2 or more. pe e † The restriction ω γ is the same as ω τ 1 in the metals case. c c ‡ For a realistic model I should include one or more infrared oscillators representing optical phonons. These cause

far-infrared absorption up to the highest longitudinal optical phonon frequency. There is transmission from there up to ωe . They also have a small effect on numerical results but do not change the physics.

328

Magneto-Optics

The refractive indices in Eqs. 16.42 and 16.43 are perfectly good for calculating wave propagation, but how they vary with the ﬁeld strength B0 (or ωc ) is not obvious. So I will use the fact that ωc ωe and expand the refractive index to ﬁrst order in ωc . I’ll start by writing the expansion of ± and then notice that the leading term contains the zeroﬁeld frequency-dependent dielectric function, which I’ll call o for “ordinary:” o (ω) = 2 /ω2 − ω2 . c + ωpe e

2 ωpe ωωc o − c ωωc 1∓ 2 = o 1 ∓ . ± = c + 2 o ωe − ω2 ωe − ω2 ωe2 − ω2 The refractive index is easy: take square root and expand:

o − c ωωc n± = no 1 ∓ , (16.44) 2o ωe2 − ω2 where no (ω) = o (ω) is the frequency dependent refractive index in zero ﬁeld.

16.5.3 Proof that the Plane of Polarization Is Rotated I’ll now work it out explicitly how the electric ﬁeld direction changes as light travels through the material in the Faraday geometry. A sketch is in Fig. 16.9. I start with an ˆ x-polarized electric ﬁeld incident from the left on the crystal surface (located at z = 0) of the form ˆ 0 ei (qz−ωt ) . El = xE Here, q = nω/c, with n the appropriate refractive index. As discussed in Section 15.2.3, plane-polarized light can be written as a sum of equal amplitudes of right and left circularly polarized light at some speciﬁc relative phase.∗ Thus the ﬁeld (at z = 0 and t = 0) is ˆ 0= El = xE

Fig. 16.9

E0 E0 ˆ + ˆ (xˆ − i y) (xˆ + i y). 2 2

The Faraday effect is the rotation of the plane of polarization of light as it passes through a crystal subjected to a static magnetic field B0 = B0 zˆ . The direction of propagation is along the magnetic field direction. The incident light, on the left, has its electric field parallel to xˆ and the transmitted field has E rotated in the x–y plane.

∗ If the relative phase is zero, I get polarization along the x axis.

329

16.5 Faraday Rotation in an Insulator

The two circular polarizations have different velocities in the material because they have different refractive indices; there will be a phase difference between right and left circular polarizations that develops as the wave travels onward. At z = +d, Et =

ω ω E0 E0 ˆ i (n − ) c d + ˆ i (n + ) c d . (xˆ − i y)e (xˆ + i y)e 2 2

(16.45)

ω

I factor the E0 ei (n+ ) c d term and collect together the xˆ and yˆ components: ω ω E0 i (n+ ) ω d c Et = e xˆ 1 + ei (n− −n+ ) c d + i yˆ 1 − ei (n− −n+ ) c d . 2

(16.46)

Next, I deﬁne an overall phase δ ≡ (n+ )ωd/c and a phase difference ω φ ≡ (n− − n+ ) d. c Note that n− > n+ making φ a positive angle. The ﬁeld can be simpliﬁed E0 iδ Et = e xˆ 1 + eiφ + i yˆ 1 − eiφ 2 E0 i (δ+φ/2) −iφ/2 xˆ e = + eiφ/2 + i yˆ e−iφ/2 − eiφ/2 , e 2

(16.47)

(16.48)

where I factored out another phase term. I could have done this back in Eq. 16.46 but it was not obvious that I needed to do so then. I recognize the complex exponential representation of cosine and sine in Eq. 16.48, so that I can write Et = E0 ei (δ+φ/2) [xˆ cos(φ/2) + yˆ sin(φ/2)] .

(16.49)

The electric ﬁeld started with only an xˆ component and after a distance d has both xˆ and yˆ components. But it is still linearly polarized light, at an angle θF to the x axis:

φ sin(φ/2) tan θF = = tan . cos(φ/2) 2 The rotation angle is half the phase difference for the two circular polarizations: θF = φ/2. The Faraday rotator is said to be a “nonreciprocal” device: Sending the transmitted light back through in the opposite direction does not undo the change the beam suffered in the forward pass. To see how this works, let me imagine that the transmitted beam in Fig. 16.9 is reﬂected and returned to the rotator, incident from the right. This light is moving to the left, so the ﬁeld is of the form ˆ 0 e−i (qz+ωt ) . Er = xE It is convenient to shift the coordinate system, putting the origin of the z axis at right edge of the crystal and the left edge at z = −d. The light incident from the right can have both xˆ and yˆ components. I write the xˆ component at the new origin (and t = 0) as a sum of equal-amplitude right and left circular polarizations: ˆ 0x = Erx = xE

E0x E0x ˆ + ˆ (xˆ − i y) (xˆ + i y). 2 2

330

Magneto-Optics

The two circular polarizations have different refractive indices and the light reaches the left side of the crystal (at z = −d) as ω ω E0x E0x ˆ −i (n− ) c (−d ) + ˆ −i (n+ ) c (−d ) . (16.50) (xˆ − i y)e (xˆ + i y)e 2 2 Other than amplitude, Eq. 16.50 is identical to Eq. 16.45. Thus the rest of the algebra is also identical, and

Ebx =

Ebx = E0x ei (δ+φ/2) [xˆ cos(φ/2) + yˆ sin(φ/2)] .

(16.51)

The x-component of the backward-going light leaving the Faraday rotator is plane polarized, pointing in the x–y plane at an angle θF = φ/2, with φ deﬁned by Eq. 16.47. If the backward-going incident ﬁeld also has a y component, amplitude E0y , I can follow it through as I did for the x component to ﬁnd that this ﬁeld is linearly polarized but with xˆ as well as yˆ components: Eby = E0y ei (δ+φ/2) [−xˆ sin(φ/2) + yˆ cos(φ/2)] .

(16.52)

The total backward-going light beam is the sum Ebx + Eby . The important case is when the incident backward-going light is reﬂected forward-going light. In this case,∗ Eq. 16.49 tells me that E0x = cos(φ/2) and E0y = sin(φ/2). With these as the components of Er , I get Eb = E0 e2i (δ+φ/2) xˆ cos2 (φ/2) − sin2 (φ/2) + 2yˆ cos(φ/2) sin(φ/2) . ˆ − φ 2 /r) + √ ˆ Suppose φ/2 is small. Then (ignoring phase) Eb = E0 [x(1 yφ]. The more ◦ interesting case is when φ/2 = π/4 (45 ). Then sin(φ/2) = cos(φ/2) = 1 2 and ˆ Eb = E0 e2i (δ+φ/2) y. The light which has passed through the Faraday rotator twice leaves with polarization at right angles to the incident light.

16.5.4 The Verdet Constant Using Eq. 16.44 for n± , the phase difference between right and left circular polarizations becomes

ωc d o − c ω2 e ω 2 o − c = B0 d, (16.53) φ= 2 2 2 2 o o ωe − ω mc ωe − ω2 c where the cyclotron frequency ωc = eB0 /mc has been used in the righthand quantity. The plane of polarization rotates through an angle θF = φ/2. The ability of a material to rotate polarization depends on a number of its properties. It is characterized by the Verdet constant V of the substance, deﬁned by θF ≡ VB0 d. ∗ I take the reﬂection coefﬁcient to be 100%.

(16.54)

331

Fig. 16.10

16.5 Faraday Rotation in an Insulator

Faraday isolator. The device consists of an input polarizer (Pol), a Faraday rotator, a half-wave plate (HWP), and an output polarizer. Light is incident from the left to right (red) and a return beam goes from right to left (blue). The arrows indicate the polarization direction in the plane perpendicular to the beam. Comparison of Eq. 16.54 and Eq. 16.53 causes me to write

o − c ω2 e V= o 2mc2 ωe2 − ω2 Even in the most effective Faraday materials, the Verdet constant is quite small. The mechanism discussed above, which is from the v×B0 term in the equation of motion of the bound electrons, gives a strong frequency dependence to V. The Verdet constant increases as V ∼ ω2 . It has only weak dependence on temperature. Another mechanism exists in crystals and glasses with paramagnetic ions. These materials have a Verdet constant that is proportional to the paramagnetic susceptibility, χ p , which follows a Curie law, χ p = C/T . The Verdet constant therefore follows 1/T . The frequency dependence is as above. As an example, the Verdet constant for terbium gallium garnet (Tb3 Ga5 O12 or TGG), a paramagnetic material commonly used in near-infrared/visible Faraday isolators, at ω = 9,400 cm−1 (the 1,064 nm wavelength of a Nd:YAG laser) is V = −40 μrad/G·cm (−40 rad/T·m). At ω = 15,800 cm−1 (the 633 nm wavelength of a HeNe laser) it increases to V = −134 μrad/·cm. To achieve a rotation at Nd:YAG wavelength of −45◦ (which is what I want for a Faraday isolator; see below) in a ﬁeld of 10 kG (1 T) (which I can get from strong permanent magnets) the crystal needs to be 2 cm long. It could be about 30% of that length at the He–Ne wavelength. The TGG Verdet constant increases by a factor of 30 on cooling from 300 K to 10 K.

16.5.5 A Faraday Isolator The Faraday effect allows the construction of a device where one observer can see a second observer while at the same time the second observer cannot see the ﬁrst. The Faraday isolator, consisting of an input polarizer, the Faraday rotator, a half wave plate, and an output polarizer, is sketched in Fig. 16.10. The Faraday rotator consists of a magnet, with magnetic ﬁeld along the axis of the device, and a crystal (Verdet) with Verdet constant times length times magnetic ﬁeld

332

Magneto-Optics strength set to provide a 45◦ rotation of the plane of polarization. The half-wave plate is a reciprocal device that rotates the plane by −45◦ to align the polarization with the axes of the output polarizer. The half-wave plate is typically done for convenience, to make the output polarization in the same direction as the input polarization. The beam (in red) is incident from the left side. If it is vertically polarized, it is transmitted by the input polarizer,∗ rotated to 45◦ by the Faraday rotator, rotated back to the vertical by the half-wave plate, and transmitted through the output polarizer. Any light incident from the right (in blue, due for example to reﬂections of the beam behind the isolator) is transmitted as vertically polarized light by the output polarizer, rotated to 45◦ by the half-wave plate, rotated further to 90◦ by the Faraday rotator, and diverted away from the path of the incident beam by the input polarizer, as shown. Betsy, on the right, can see Alan, on the left, but Alan cannot see Betsy.

∗ If it is not vertically polarized, some fraction is rejected by this polarizer; if it is unpolarized, that fraction is

half of the incident power.

17

Inhomogeneous Materials

Many materials seen in everyday life are inhomogeneous: inks, paint, cement, ceramics, stained glass, etc. An example is shown in Fig. 17.1. These materials are mixtures or composites of two or more materials with different dielectric response functions. Some of these composite materials appear to be inhomogeneous to the human eye; the appearance (tint, brightness, saturation) varies from point to point. But others appear completely uniform. One of my goals here is to understand the ways in which the effective properties of an inhomogeneous medium depend upon the properties of its constituents and their geometric arrangement in the medium. I am mostly interested in materials in which the scale of the inhomogeneity is smaller than the wavelength, so that they appear to be uniform.∗ To understand the optical properties of such materials, I’ll try to calculate the average or effective response of the mixture from knowledge (or assumptions) about the properties of the constituents, their dielectric functions, their size, their concentration, and perhaps some little knowledge of how they are arranged in the composite. The ﬁeld of inhomogeneous materials has been an active area of research for many years, both because of the intrinsic interest of the subject and due to possible technological applications of these materials. An area of basic interest is the insulator-to-conductor transition or “percolation transition” which occurs in these materials as a function of the concentrations of the constituents and which resembles in many ways a secondorder thermodynamic phase transition. A possible important application is in the design of materials with useful infrared properties, such as efﬁcient photothermal solar energy collectors. I’ve identiﬁed the dielectric function (and permeability μ if magnetic) as specifying the optical properties of a material. In the homogeneous material, is the same at every point in the material. The situation is greatly complicated if the medium is not spatially homogeneous but instead has physical properties which vary throughout the material. The manner of the variation may be random, may be periodic, or may be ordered in some other way; in all cases the dielectric function and permeability become functions of position as well as of the frequency: = (r,ω)

(17.1)

∗ The other extreme, materials which obviously differ as one looks here and there at them, is either trivial – just

average the reﬂectance or transmittance of the components – or very difﬁcult – the response is determined by scattering, diffraction, and interference of light striking the different parts and depends on the details of the organization of the composite.

333

334

Inhomogeneous Materials

Fig. 17.1

Detail of a stained-glass window at the University of Virginia chapel. The red panels are “gold ruby”glass, a red glass made by adding gold salts or colloidal gold to molten glass. The process precipitates small (10 nm scale) gold particles in the glass. The blues come from cobalt and the other colors from the addition of a variety of metallic salts. and μ = μ(r,ω).

(17.2)

As an example of an inhomogeneous medium, I will consider a composite made from metal small particles and insulating grains. The dielectric response function of each constituent is assumed to be well understood. The metal could well be described by a Drude dielectric function Eq. 4.13 while the insulator has a dielectric function ins that is mostly real and nearly constant.∗ Thus, the spatially varying dielectric function has two possible values: ⎧ ⎪ ωp2 ⎨ − , r in metal. c (r,ω) = ω2 + iω/τ ⎪ ⎩ , r in insulator. ins The local properties of this material vary dramatically depending upon whether r is in the metallic or insulating component of the composite. Although it is true that the functions (r,ω) and μ(r,ω) completely describe the electromagnetic response of the medium, this description is not very useful because to employ it would require a knowledge of the exact geometric location of the constituents. Generally, this information is unavailable; in addition, the interesting quantity is the average response of the inhomogeneous medium to external ﬁelds, not the local response. Fortunately, so long as the scale on which measurements are made (the wavelength) is large compared to the scale of the ﬂuctuations of the dielectric function (the particle size), the ∗ It could be vacuum, with = 1.

335

17.1 The Effective Medium

inhomogeneous medium appears to be uniform in its response to external ﬁelds and can thus be described by an effective dielectric function eff (ω) and permeability μeff (ω). The problem with which I am confronted, therefore, is in its most general terms the following: given an inhomogeneous medium that has a well-deﬁned local dielectric function (r,ω) and permeability μ(r,ω), how can the effective response functions of the entire medium be determined?

17.1 The Effective Medium Historically, the problem of calculating eff (ω) and μeff (ω) has been addressed from two rather different points of view. The ﬁrst is a molecular ﬁeld model originally developed by Clausius, Mossotti, Lorentz, and Lorenz to calculate the local ﬁeld in a crystal and later applied to the optical properties of an inhomogeneous medium by Garnett [368, 369]. Garnett wrote about the colors of stained glasses containing metallic inclusions. (See Fig. 17.1.) Because his full name was James Clerk Maxwell Garnett, this model has become known as the Maxwell-Garnett theory (MGT). The second point of view is a symmetrical effective medium approach, initially developed by Bruggeman [370] and rediscovered by Landauer [371]. The application of this model to optical properties was ﬁrst suggested by Springett [372] and by Stroud [373]. This model is generally called the effective medium approximation (EMA), although both it and the MGT are in fact effective medium theories. Each provides an expression for the effective dielectric function of a homogeneous medium which has properties effectively identical to those of the inhomogeneous medium. Each theory (and most subsequent developments) begins with a major simpliﬁcation. The local dielectric function (r,ω) of the inhomogeneous medium is assumed to take on a limited number of discrete values (perhaps as small as two) rather than being allowed

Fig. 17.2

The upper panels show a composite made of two types of materials, white grains and black grains. In the MGT, the composite is viewed as consisting of black grains embedded in an host of the white material. In the EMA, both white and black grains are viewed as surrounded by the effective medium and combined in a weighted average way.

336

Inhomogeneous Materials

to vary over a continuous range. This simpliﬁcation corresponds to the example already discussed: the system is a disordered composite, a random mixture of many grains each of which by itself has spatially uniform properties. The composite is characterized by specifying the volume fraction, dielectric function, shape, and size of each grain type. Each grain is then taken to be a polarizable entity, with electric (and magnetic) dipole moment induced by electric (and magnetic) ﬁelds from external sources as well as from the ﬁelds of the polarized grains in the outside medium. The principal difference between the MGT and the EMA is the way in which the medium surrounding the grain under consideration is treated. This difference is illustrated in Fig. 17.2. In the MGT it is assumed that the medium surrounding the grains is one of the constituents of the mixture (for example, the one with the largest volume fraction) while in the EMA it is assumed that the surrounding medium is characterized by the effective properties of the inhomogeneous medium.

17.2 Response of a Single Grain 17.2.1 Quasistatic Model: Electric Dipole Moment The initial step in the solution for the effective properties of an inhomogeneous medium is to ﬁnd the electromagnetic ﬁelds inside and outside of a single particle of radius a when that particle is subjected to a plane wave ﬁeld. For simplicity I will assume that the particle is spherical and that I am in the long-wavelength limit, λ a. Then, the applied ﬁelds appear to be spatially uniform, time varying ﬁelds. The particle in this quasistatic limit has only dipole moments; these moments are time varying so that electric current ﬂows and energy can be absorbed. I’ll deﬁne the dipole moment in terms of the polarizability in a way similar to what I did for atoms in Eq. 4.1: p = γe E0 e−iωt

(17.3)

where is the volume and γ e is the electric polarizability per unit volume of the particle, given by the solution to the static boundary value problem of a dielectric sphere in a uniform far ﬁeld [2]. Deﬁning the dipole moment does not tell me what it is. What I have to do (in this quasistatic limit) is to solve a boundary value problem: that of a sphere with dielectric function in a uniform far ﬁeld.∗ Actually, I do not have to solve the problem; it is a standard problem in many textbooks [2]. I just need to write down the solution. The polarizability is γe =

3o p − o , 4π p + 2o

(17.4)

∗ I can think of this problem as the task of ﬁnding the polarization in a small dielectric sphere located between

the plates of a large capacitor. The capacitor plates are attached to a voltage source, producing far away from the sphere a ﬁeld E between the plates.

337

17.3 Effective Medium Theories

where p is the complex dielectric function of the particle and o is the complex dielectric function of the medium outside the particle. The electric ﬁeld outside the particle is that of a dipole with moment p. This electric dipole moment is the ﬁrst term in the Mie [8, 374–376] solution for the multipole moments of the sphere. The same solution ﬁnds that the electric ﬁeld is 3o Eo e−iωt . (17.5) Ep = p + 2o Note that this ﬁeld is uniform and parallel to the external ﬁeld. The difference between Eo and Ep is called the depolarizing ﬁeld.

17.3 Effective Medium Theories To ﬁnd the effective dielectric function of a composite material, I have to do some sort of averaging. It helps to use resistor networks as model systems in thinking about inhomogeneous systems. I suppose that the network contains a large number of resistors, with values varying over a wide range. The resistors are connected in a series/parallel conﬁguration. The values of a particular resistor as well as how it is wired into the network are chosen at random. I inject current into the network and measure the voltage developed across it. If I probe around inside, I’ll ﬁnd that some resistors will carry a lot of current; some a small amount or even zero current. Similarly, there will be parts of the network with big voltage drops and other parts with small voltage drops. But the ratio of voltage across the network to the current ﬂowing into or out of it is the effective resistance of the network. A picture of the composite for which I will calculate the optical properties considers it to be composed of small grains of two or more materials. The grains are smaller than the wavelength of the light being used to examine them; consequently they are not resolved. All the grains are not the same (else the material would be homogeneous) but they are not all different either. I suppose that there are Ni grains of type i, each with average volume i . Then I can deﬁne the volume fraction fi of type i grains as fi = where V is the sample volume. Clearly∗

Ni i V

(17.6)

fi = 1.

i

17.3.1 Average Fields I will deﬁne the effective dielectric function and permeability of the inhomogeneous medium in terms of volume-averaged ﬁelds, E, and responses, D. (It is also possible to work with the volume averaged dipole moment per unit volume, P, or current, j; the ∗ If there is empty (void) space in the composite, I will consider this to be one of the components of the

inhomogeneous system.

338

Inhomogeneous Materials

choice is entirely a matter of individual preference.) If fi is the volume fraction of the ith component of the medium, then the average electric ﬁeld is fi Ei E = i

deﬁnition∗

with an analogous for D. For simplicity I will assume a two-component composite and label these constituents as type a and type b materials. If f is the volume fraction of type a, then (1 − f ) will be the volume fraction of type b, so that the average ﬁelds are: E = f Ea + (l − f )Eb D = f a Ea + (l − f )b Eb,

(17.7)

where I have used a local relationship Di = i Ei . The effective dielectric function is deﬁned in terms of the average ﬁelds: D = eff E.

(17.8)

When I write Eq. 17.8, I take the point of view that the interesting property of the medium is the average response to external ﬁelds; the external ﬁeld is just E while D is the response to those ﬁelds.

17.3.2 Maxwell-Garnett Dielectric Function The Garnett theory (MGT) is implicitly a model for a dilute system. According to the MGT, a single grain of dielectric function a is assumed to lie at the center of a cavity (the Lorentz cavity) carved out of the interior of the inhomogeneous medium. There may be other type a grains in this cavity; the remaining space is assumed to be ﬁlled with a medium with dielectric function eb . Thus the local ﬁeld at the grain is the superposition of the uniform applied ﬁeld, the uniform ﬁeld from the charge (polarization charge) located on the cavity surface, and the dipolar ﬁelds from the neighboring particles. As discussed by Landauer [21] in his review of inhomogeneous materials, I can exclude other grains from the cavity by making the cavity tightly to jacket the central grain. A more common approach is to argue that the dipolar ﬁelds from those neighboring grains which are inside a large cavity sum to zero in the vicinity of the central grain.† With this assumption, the electric ﬁeld inside the grain is uniform and found by substitution of p = a and o = b into Eq. 17.5: Ea =

3b Eb e−iωt . a + 2b

(17.9)

∗ If I want to calculate the magnetic response, then I will also deﬁne H, and B. The derivations for effective

permeability are perfectly analogous to those for effective dielectric function.

† If the arrangement is periodic, the contribution can be calculated; it often is zero. If the arrangement is random,

one can argue that the ﬁeld direction and magnitude at the cavity center will be random, and the random orientations of many contributions will tend to zero.

339

17.3 Effective Medium Theories

Combining Eqs. 17.7 and 17.9 gives, after some algebra, Garnett’s expression for eff which I label mgt : mgt = b + b

3f (a − b ) . (1 − f )(a − b ) + 3b

(17.10)

Eq. 17.10 illustrates two properties which are characteristic of the MGT approach to inhomogeneous media. First, the equation is inherently asymmetric in its treatment of the two constituents: different values are obtained for mgt depending on whether, for example, I regard the composite as consisting of metal grains embedded in insulator or the other way around. Second, the equation gives a smooth variation of mgt with volume fraction, from b when f = 0 to a when f = 1. That real physical systems do not always behave in this fashion may be seen by considering the low-frequency behavior of an inhomogeneous medium for which a = 1 and b = 4π iσ b /ω, i.e., material a is vacuum, with zero conductivity, and material b is a metal with DC conductivity σ b . At f = 0 the MGT conductivity is just σ b . Now I start carving or drilling holes in the material, increasing f . The presence of these holes cause the effective conductivity to decrease. According to the MGT, the conductivity will remain ﬁnite all the way to f = 1, when no conducting component remains. In reality, however, the medium is likely to stop conducting at a lower value of f , when the nonconducting regions occupy enough space to prevent current ﬂow in the sample. This “percolation threshold” is not predicted by the MGT; it is, in fact, speciﬁcally excluded by the assumption that the embedded grains do not contact one another. In applications of the MGT the asymmetry and the absence of a percolation transition can be handled in an ad hoc fashion by assuming that as the volume fraction of one constituent increases from zero to unity, its role changes from that of inclusion to that of host. Despite its shortcomings, the MGT is generally believed to work reasonably well in dilute mixtures, where the grains of the minority constituent are well separated. More generally, Hashin and Shtrikman [377] have shown that the MGT expression represents bounds to the actual conductivity of a two-component heterogeneous medium, an upper bound if σ a < σ b and a lower bound if σ a > σ b . The MGT approach to the properties of inhomogeneous media has been rediscovered and elaborated numerous times over the past 100 years [378–389]. As an example, let us consider the case of small metal particles embedded in a medium with dielectric constant eb = 1. For the metal I assume a simple Drude dielectric function, Eq. 4.13, with c = 1: a = 1 −

ωp2 ω2 + iω/τ

.

Under these assumptions, the MGT dielectric function becomes mgt = 1 +

f ωp2 2 − ω2 − iω/τ ωmgt

.

(17.11)

340

Inhomogeneous Materials

The effective dielectric function will exhibit a resonant absorption when the frequency of the light equals the Maxwell-Garnett resonant frequency, ωmgt , equal to 1−f . ωmgt = ωp 3 This Maxwell-Garnett resonance arises physically from the fact that the Drude dielectric function of a metal, Eq. 4.13, is negative below the plasma frequency and can thus cancel in the electric polarizability, Eq. 17.4, the positive dielectric constant of the surrounding medium. In the example above, the cancellation occurs when a = −2. More sophisticated models, in which the outside medium has dielectric constant b and the metal has a core contribution c in its dielectric function, become algebraically more complex but retain the Lorentzian form of Eq. 17.11. The resonance frequency is shifted in this more general case to 1−f . (17.12) ωmgt = ωp (1 − f )c + (2 + f )b Figure 17.3 shows the MGT frequency-dependent conductivity. I have taken the metallic portion of the composite to have a Drude dielectric function, Eq. 4.13, and the insulating portion to have a real, constant dielectric function. The conductivity is shown over the entire frequency range from DC to UV for metal volume fractions of 0.1, 0.3, 0.5, 0.7, and 0.9. A curve is also shown where the MGT is inverted, i.e., the metal was taken as host and

Fig. 17.3

Frequency-dependent conductivity calculated from the Garnett theory. The calculation used a Drude dielectric function for the inclusion (a = Drude ) with parameters meant to represent silver [c = 4.0, ωp = 70,100 cm−1 (8.7 eV) and 1/τ = 1,300 cm−1 (0.16 eV)]. The scattering rate is about 10× that of pure silver, under an assumption that scattering from the surface of the particle determines the mean free path. For the insulator, b = ins = 4.

341

17.3 Effective Medium Theories

the insulator as inclusion, both with volume fractions of 0.5. Relatively short mean free ˚ were taken in calculating these plots; this choice leads to a rather broad paths (about 30 A) MGT resonance. There are several points to make about Fig. 17.3. There is no DC conductivity in the MGT when the metal is taken as inclusion so long as f < 1; there is always a ﬁnite DC conductivity when the metal is host. The low-frequency spectrum of the metal–host mixture is of Drude form. The MGT resonant frequency (given by Eq. 17.12), moves to lower frequencies as the concentration increases. The low-concentration value for the resonant √ frequency is ωmgt = ωp / c + 2b .

17.3.3 The Effective Medium Approximation The second approach to the theory of inhomogeneous media, due to Bruggeman [370] and Landauer [371], is generally called the effective medium approximation (EMA). In this discussion I will again restrict myself to a two-component medium made up of spherical grains. The ﬁrst component has dielectric function a and is present with volume fraction f while the second has b and the remaining volume fraction, 1 − f . In contrast to the MGT, the EMA has the attractive feature of treating all constituents of the medium in an equivalent way. It achieves this symmetry by regarding an individual grain (which may be either type of material) as being embedded in an otherwise homogeneous “effective” medium which is assumed to possess the average properties of the medium. When placed in an external ﬁeld, the grain in question will be polarized; the ﬁeld inside is given by Eq. 17.5, with o equal to the effective dielectric function EMA Ep =

3EMA Eeff e−iωt p + 2EMA

(17.13)

where Eeff is the effective ﬁeld in the surrounding medium. This ﬁeld is chosen in a selfconsistent way so that the electric ﬁeld in the medium, when summed over all the grains in the medium, equals Eeff . This self-consistency condition may be incorporated in a number of ways; the simplest is to set Eeff equal to the deﬁnition of the average ﬁeld, Eq. 17.7, Eeff = f Ea + (l − f )Eb and then substitute Eq. 17.13 evaluated for the ﬁelds inside the two kinds of grains. After minimal algebra, this procedure yields a quadratic equation for EMA , which is conventionally written f

a − EMA b − EMA + (1 − f ) = 0. a + 2EMA b + 2EMA

(17.14)

This quadratic equation may also be obtained by using Deff = EMA Eeff , with Deff = D. The solution to Eq. 17.14 EMA =

1 2 B ± B + 8a b, 4 4

342

Fig. 17.4

Inhomogeneous Materials

Frequency-dependent conductivity calculated from the effective medium approximation (EMA). where the sign of the square root is chosen such that Im EMA ≥ 0 and where B = a (3f − 1) + b (2 − 3f ). The EMA differs from the MGT in two important ways. First, the equations treat each of the constituents of the medium on an equal basis. The EMA is thus a symmetric theory and is not restricted to a particular range of concentrations. Second, the EMA predicts a metal–insulator transition at a critical volume fraction (for spherical grains) of fc = 1/3. If I reconsider the example of the metal into which I carve or drill holes (in Section 17.3.2 of this chapter), then the composite stops conducting when 67% of it is void and 33% is metal.∗ To demonstrate this second point, I assume that the imaginary part of the complex dielectric function dominates the real part as ω → 0, so that a = 4π iσ 1a /ω 1a . If, in addition, σ 1b = 0, Eq. 17.14 may be solved to ﬁnd ! 0 f ≤ 1/3 σ 1EMA = 3f − 1 (17.15) 2 σ 1a f > 1/3. The EMA may readily be extended to systems more complicated than the one considered here. For metal–insulator composites with low metal volume fraction, the theory gives a broad absorption peak centered near the Maxwell-Garnett resonance frequency. Figure 17.4 shows the EMA frequency-dependent conductivity over the entire frequency range from DC to UV for a metal–insulator composite. I have taken the metallic portion ∗ There are still metal grains touching other metal grains, but the chance of an inﬁnite cluster of such grains

spanning the entire sample is – within the EMA – zero.

343

17.3 Effective Medium Theories

of the composite to have a Drude dielectric function, Eq. 4.13, and the insulating portion to have a real, constant dielectric function with b = 4. The calculation was done for ˚ volume fractions f of 0.1, 0.3, 0.6, and 0.7. Relatively short mean free paths (about 30 A) were taken in calculating this plot but the Drude width does not determine the width of the infrared band; the width of the EMA resonance is intrinsic to the theory. There are several points to make about this ﬁgure. The symmetric EMA has a insulator– conductor transition when the metal volume fraction reaches 1/3, the critical concentration for percolation. Second, although the EMA does give a broad resonance centered near the MGT resonant frequency (a frequency given by Eq. 17.12), this resonance has much greater width than in the MGT. (See Fig. 17.3.) The low frequency edge of the EMA resonance moves to zero frequency at the percolation transition [390]; this behavior is seen in the curve for the f = 0.3 sample in Fig. 17.4. Third (although this point is hard to see from Fig. 17.4), the MGT and the EMA at small concentrations give nearly identical results for the low-frequency conductivity. The concentration dependence of various characteristic frequencies in the EMA has been discussed by Stroud [390]. A plot is seen in Fig. 17.5. The frequencies ω+ and ω− are the impurity band limits as calculated in the EMA. ω˜ imp and ωimp are the impurity band centroids. There are two percolation concentrators marked. The ﬁrst, f = 1/3, is where the metal component ﬁrst forms a continuous path throughout the sample. The second, f = 2/3, marks where the insulating component ﬁrst becomes discontinuous. Figure 17.5 shows that the low-frequency and high-frequency limits move apart as f increases from zero to the metal percolation transition. At the transition, ω− reaches zero frequency. At higher concentrations ω− increases, leaving a gap between DC and the impurity band. The upper limit, ω+ reaches ωp at f = 2/3. As f → 1 the width of the impurity band shrinks to zero. There is a percolating mode at zero frequency once f > fc ;

Volume Fraction

Fig. 17.5

Concentration (f ) dependence of the characteristic frequencies of a metal–insulator composite. ω+ and ω− are the impurity band limits as calculated in the EMA. The concentrations where the metal and insulator components have their percolation transitions are shown by arrows. ω˜ imp and ωimp are the impurity band centroids. (From Ref. 390.)

344

Inhomogeneous Materials

it clearly can be seen in Fig. 17.4. The DC conductivity is zero for f < 1/3 and ﬁnite for f > 1/3. It grows with increasing metal concentration.

17.4 Other Approaches 17.4.1 Percolation Theory Percolation theory addresses the properties of inhomogeneous materials by investigating an ordered lattice in which each site (or bond) is occupied with probability p or vacant with probability 1 − p and in which adjacent occupied sites (or bonds) are regarded as being electrically connected. The probability p in this model plays the role of volume fraction for a continuous medium. A computer is used to generate the lattices and to solve Kirchoff’s laws for the conductivity of the lattice as a function of the occupation probability, the dimensionality, the nature of the interconnection, and the type of lattice employed. Percolation theories always give a percolation transition, but the occupation probability pc at which this transition occurs (the critical probability) varies from as low as 0.2 to as high as 0.7 depending on the coordination number and dimensionality. Several authors [391–393] have argued, however, that when the amount of space that can be ﬁlled by spheres (of equal size) in a particular lattice is taken into account, the critical volume fraction in three dimensions is always in the range 0.16 ≤ fc ≤ 0.18, a value which is in accord with experiment [394]. The electrical resistance of a percolating system has been widely addressed [395–405]. An important concept [406–412] relates the percolation transition to a second-order thermodynamic phase transition, leading to a scaling theory of the transition. The main predictions of this idea are that the critical probability pc plays the role of the thermodynamic critical temperature Tc and that many properties of the inhomogeneous medium obey power-law dependences on the quantity p−pc . For instance, the conductivity of the network, σ e , goes to zero as p → pc from above according to σ e ∼ (p − pc )t

p > pc

(17.16)

while the static dielectric constant e diverges below pc as e ∼ (pc − p)−s

p < pc .

(17.17)

According to the scaling theory, quantities such as the percolation threshold and the proportionality constants in Eqs. 17.16 and 17.17 may vary from system to system depending upon the details of material and sample preparation, but the exponents s and t are universal; they depend only on the dimensionality. In three dimensions [413] t ≈ 1.7 and s ≈ 0.6. The latter estimate in particular is in remarkably good agreement with experiment [313, 414]. Note that both scaling exponents differ from those of the EMA, for which s = t = 1. All I have done up to now is to write about the DC conductivity of a percolating system; I have not addressed the frequency dependence of this conductivity. Now, once I make a material inhomogeneous, it will contain both inductive and capacitive elements.

345

17.4 Other Approaches

The inductive elements are there because currents will have to circulate around the nonconducting parts of the composite. Capacitive elements are there because charges will appear on the surfaces of these nonconducting parts. These elements will contribute to deviations from the Drude conductivity of the metal (at high metal concentrations) or the insulating dielectric response of the insulator (at low metal concentrations). The low-frequency conductivity within the EMA varies as ω2 for f fc and as (ω) for f > f c. Bergman and Imry [412] have suggested that the conductivity at p = pc obeys σ 2 ∼ ωβ with β = 0.73. A close result was obtained by Stroud and Bergman [415], who found that σ 2 ∼ ωt/(t+s ) . The exponent t/(t + s) = 0.75.

17.4.2 Eddy Currents: Magnetic Dipole Absorption A conducting spherical particle in a time-varying magnetic ﬁeld will have currents, commonly called eddy currents, induced in it. The magnetic ﬁeld of an electromagnetic wave is such a time-varying ﬁeld. If the diameter is small compared to the wavelength, these currents give the particle a time-varying magnetic dipole moment, m = γm H0 e−iωt , where is the volume of the sphere, H0 the amplitude of the ﬁeld, and γm the magnetic polarizability. The solution for the latter may be found in Landau and Lifshitz [3] and Smythe [6]: 3 3 3 j2 (ka) 3 = cot(ka) (17.18) − 1 − γm = 8π j0 (ka) 8π (ka)2 ka where j0 and j2 are spherical Bessel functions, a is the radius, and k is the wave vector for light propagating inside the material making up the sphere.∗ This wave vector is ω√ ω 1 N= = (1 + i) c c δ where the last equality is true for a metal in the low-frequency limit. δ is the skin depth. The eddy currents are a consequence of the ﬁnite skin depth of the particle and are signiﬁcant for the electromagnetic response of the inhomogeneous medium in the case where the radius is of the same order as the skin depth [416–419]. When light is traveling in a composite material composed of conducting metal spheres, there will be a bunch of magnetic dipoles in the composite; there is no magnetic dipole moment in the insulating regions. So I could carry through a Maxwell-Garnett or effective medium calculation for the effective magnetic permeability of the composite. I refer the reader to a few papers to see how this goes [417, 418, 420]. k=

∗ I cannot say “propagating inside the sphere” because the sphere is small compared to the wavelength, making

propagation not possible.

346

Inhomogeneous Materials

17.4.3 Mie Scattering I have considered in this chapter only inhomogeneous media made up of particles whose size is smaller than the wavelength and skin depth. The case where the particles are comparable to the wavelength is the domain of Mie theory [374]. This theory, also developed by Debye [375], calculates the scattering by a spherical particle, essentially as a multipole expansion for the scattered electric and magnetic ﬁelds. The polarizabilities given by Eqs. 17.4 and 17.18 are related to the ﬁrst two (dipolar) terms in this series. When the particle is nearly the same size as the wavelength, all terms are important. Stroud and Pan [421] applied the theory to the speciﬁc problem of electromagnetic wave propagation in composite media. A good discussion is in the book by van de Hulst [376].

Appendix A Notes about Units

First, let me start with common units used to measure frequency, photon energy,∗ and related quantities. ω, angular frequency, in s−1 (radian/s) f , frequency, in Hz (f = ω/2π ) λ0 , vacuum wavelength† (λ0 f = c) ν, wavenumber (or “frequency”), in cm−1 (ν = f/c = 1/λ0 = ω/2π c) with λ0 in cm. E, photon energy, in eV (E = hf = hω ¯ = hcν) T , temperature, in K (T = E/kB ) To convert: 1 cm−1 = 1.44 K = 1/8,066 eV = 0.124 meV = 30 GHz = 1.88×1011 s−1 1 eV = 8,066 cm−1 = 11,600 K = 242 THz = 1.52×1015 s−1 = 1/(1.24 μm) red = 2 eV= 16,000 cm−1 = 1/(620 nm) I am using cgs-Gaussian units for electromagnetic, quantum mechanical, and solid-state quantities. t, time, in seconds (s) , length, in cm c = 3 × 1010 cm/s (more or less) E ﬁeld in statvolts/cm (but irrelevant, usually) H ﬁeld in gauss or oersted (but irrelevant, usually) m, mass, in grams (g) h and h, ¯ Planck’s constants, in erg-s‡ e, charge, in esu The dielectric function, , permeability, μ, and refractive index, N , are dimensionless, a notable advantage.§ The principal measured quantities that have units are the absorption coefﬁcient, α, penetration depth, δ, and conductivity, σ .

∗ † ‡ §

347

If, like the particle physicists, I set h¯ = 1, then (angular) frequency and energy are identical. The wavelength in a medium – even air – is of course different: λ = λ0 /n. But it even more common to use electron volts, so that h¯ = 6.58 × 10−16 eV-s. In SI, it is the relative version, e.g., r that has no dimensions; the dielectric constant has the units of the vacuum permittivity.

348

Appendix A α, absorption coefﬁcient, in cm−1 (even in SI, usually) ˚ or even meters δ, penetration depth, in cm or μm or A − 1 σ , conductivity, is in s , i.e., it is a frequency In practical units, σ is measured in −1 cm−1 ,∗ and ρ = 1/σ is in Ohm-cm or -cm To convert: σprac = σesu /30c ≈ σesu /9 × 1011 For copper at 300 K, ρ ≈ 1.6 μ-cm, so σ ≈ 6 × 105 −1 cm−1 ≈ 6 × 1017 s−1 . Note that the equation for conductivity is the same in both systems; in the Drude model at zero frequency it is given by Eq. 4.9: σdc = ne2 τ/m. The factor of 9 × 1011 comes from using in cgs (SI) the following: esu (Coulombs) for the charge, grams (kg) for the mass, cm−3 (m−3 ) for the carrier density, and then using the factor of 100 between between −1 m−1 and −1 cm−1 . The equations for the plasma frequency are not the same in the two systems, although the units for it (s−1 ) are the same. In cgs (see Eq. 4.12) it is 4π ne2 , ωp = m whereas in SI it is

ωp =

ne2 , 0 m

where 0 = 8.854 × 10−12 Farad/m is the permittivity of the vacuum.† The impedance of free space, Z0 is different both in equation and units in the two systems. It’s deﬁned by Z0 = (4π/c)(E/H ) = 4π/c in cgs. Here E and H are respectively the amplitudes of the electric and magnetic ﬁelds, equal in vacuum. In SI, Z0 = E/H = μ0 c = 376.7 . See Eq. 14.12. It is often reported as 120π , which it would be were c = 3 × 108 m/s. The cgs value, 4π/c = 4.189 × 10−10 sec/cm. The ratio of the two is 30c. (Surprise!) The absorption coefﬁcient α and the optical conductivity σ1 are similar quantities. It is often nice to go back and forth, especially in cases of weak absorption bands that do not affect the refractive index very much. Now, α=

2ω κ c

and

2 = 2nκ

∗ To be fully SI-ized, one should report σ in Ohm−1 m−1 , and some do. There is a factor of 100 between −1 cm−1 and −1 m−1 . I’ll let the reader ﬁgure out which way it goes. † Persons who wonder about the reasons why the vacuum has a permittivity (and permeability) that differs from

unity might want to read Casimir’s discussion of the volumetric constant of empty space [422].

349

Appendix A

where n and κ are respectively the real and imaginary parts of the refractive index. The factor of two on the left comes because the absorption coefﬁcient is deﬁned in terms of the exponential decay of intensity as light passes through the material and the one on the right comes from writing the imaginary part of = N 2 . Then, because 4π σ1 /ω = 2 , I can write σ1 = ncα/4π . This equation gives esu values for the conductivity. To convert to SI, I (as usual) divide by 30c. But then I notice the 120π in the denominator and recognize it as the impedance of free space. So, I write nα σ1 = Z0 with n the refractive index, α the absorption coefﬁcient, and Z0 = 376.7 the impedance of free space. σ1 appears in −1 cm−1 if α is in cm−1 . The equations for the classical skin depth differ in the two systems. According to Eq. 4.38 and the discussion at the beginning of Chapter 14 (in Section 14.1), the classical skin depth is c2 2c2 , = δ= 2π ωσdc ωp2 ωτ where σdc is the DC conductivity, measured (esu) in sec−1 . The calculation will yield δ in cm. In SI, with the conductivity σdc in −1 m−1 , the skin depth is 20 c2 2c2 δ= , = ωσdc ωp2 ωτ where you would use c = 3 × 108 m/s so that δ emerges in m. I may also use √ δ = 2/ωσdc μ0 with μ0 = 4π × 10−7 N/A, the permeability of free space, again with σdc in −1 m−1 and δ in m. The mobility is also an optical/electrical materials property with units. The conductivity σ is written in terms of mobility as σ = neμ where n is the carrier concentration, e the electronic charge, and μ the mobility. If the semiconductor is in the regime where a Drude model applies, one has μ = eτ/m∗ . Here τ is the mean time before the next collision and m∗ is the effective mass. The units in which mobilities are usually reported are cm2 /V·s. This set is neither-ﬁsh-nor-foul; in pure SI, the units should be m2 /V·s. If the mobility is μ = 1,000 cm2 /V·, it is μ = 0.1 m2 /V·s. To convert to cgs-Gaussian, where the units are cm2 /statV·s, multiply the mobility in cm2 /V·s by 300. (Or multiply the mobility in m2 /V·s by 3×106 .)

Appendix B Maxwell’s Equations in SI

Maxwell’s equations look a bit different in SI. For example, Eq. 2.1 is simpler looking in SI:∗ ∇ · D = ρext

(B.1a)

∇ ·B=0

(B.1b)

∇ ×E=−

∂B ∂t

∇ × H = j free +

(B.1c) ∂D . ∂t

(B.1d)

The Lorentz law (Eq. 2.2) is F = q(E + v × B),

(B.2)

where v is the particle’s velocity.† In vacuum, the SI version of Eq. 2.3 becomes D = 0 E and B = μ0 H, where 0 and μ0 are the permittivity and permeability of vacuum, with values 0 = 8.854 × 10−12 −7

μ0 = 4π × 10

Farad/m

Henry/m.

In vacuum, one ﬁnds plane-wave solutions, with velocity 1 ≡ c. √ 0 μ0 In macroscopic media, the auxiliary ﬁelds are D = 0 E + P 1 B−M H= μ0

(B.3)

which, in local, linear, isotropic, and homogeneous media, become D = r 0 E B H= μr μ0

∗ Although I think that it is nice to see the speed of light appearing in the equations of electromagnetism. † This one gives no indication that speeds need to approach lightspeed before magnetic forces and electric forces

become comparable (for, say, ﬁelds with the same electric and magnetic energy densities).

350

351

Appendix B

with r and μr dimensionless numbers, called respectively the relative permittivity and relative permeability, identical to the dielectric constant and permeability μ in cgsGaussian units. The SI energy density is u = 1/2(E · D + B · H). (In vacuum, u = 1/2(0 E 2 + B 2 /μ0 ).) The Poynting vector is S = E × H. SI units for S are particularly easy (and, I must admit, easier than in cgs) because the electric ﬁeld is in V/m and the magnetic ﬁeld is in A/m, making the units of the Poynting vector (and of the intensity, equal to the magnitude of time-averaged S) be W/m2 .

Appendix C Partial Derivatives and Vector Operators Acting on Plane Waves Let’s write a complex plane wave A as A = A0 ei (q·r−ωt ) = (A0x xˆ + A0y yˆ + A0z zˆ ) eiqx x eiqy y eiqz z e−iωt where A0 is a constant vector specifying the direction, magnitude, and phase of A, and the wave vector q = qx xˆ + qy yˆ + qz zˆ is normal to the planes of constant phase. Now take the partial with respect to time of A. The only term containing the time in the vector is e−iωt and ∂ −iωt e = −iωe−iωt ∂t so that ∂ A = −iωA. ∂t Now, I want to act on A with the vector operator ∇ where ∇ = xˆ

∂ ∂ ∂ + yˆ + zˆ . ∂x ∂y ∂z

First, I’ll compute the divergence ∇ · A. If I do this, and write out the dot product of ∇ with A0 , I get

∂ ∂ ∂ + A0y + A0z eiqx x eiqy y eiqz z e−iωt . ∇ · A = A0x ∂x ∂y ∂z Each partial derivative only acts on one of the complex exponentials in A, so that ∇ · A = (iqx A0x + iqy A0y + iqz A0z ) eiqx x eiqy y eiqz z e−iωt or ∇ · A = iq · A. In a similar way, I can show that ∇ × A = iq × A, ∇ 2 A = −q 2 · A, and ∇A = iqA. In the last of these A is a scalar. The great thing about the complex exponential solutions to Maxwell’s equations is that they allow me to replace differential equations with algebraic ones. 352

Appendix D The Wave Equation

It is not surprising that electromagnetic waves satisfy a wave equation. Many textbooks derive a wave equation from Maxwell’s equations and use that to ﬁnd the wave-like ﬁelds of propagating electromagnetic waves. Instead, in Chapter 2 I showed that the wavelike solutions satisﬁed directly Maxwell’s equations. The wave equation approach is certainly worth mentioning, so I do that here. I’ll start with Eqs. 2.4a–b. I’ll take the medium to be uncharged, linear, isotropic, and homogeneous, so that D = 1 E, j = σ1 E, and B = μH. With these deﬁnitions, I have ∇ ·E=0

(D.1a)

∇ ·H=0

(D.1b) μ ∂H ∇ ×E=− (D.1c) c ∂t 1 ∂E 4π ∇ ×H= σ1 E + . (D.1d) c c ∂t Now, I take the curl of Eq. D.1c, interchanging the order of derivatives on the right: μ ∂∇ × H . c ∂t I use a vector identity on the left and replace ∇ × H on the right with the right side of Eq. D.1d ∇ × (∇ × E) = −

4π ∂E 1 μ ∂ 2 E − 2 ∇(∇ · E) − ∇ 2 E = − 2 σ1 μ . ∂t c c ∂t 2 Now ∇ · E = 0. Rearranging slightly the rest, I ﬁnd 4π ∂E 1 μ ∂ 2 E ∇ 2 E − 2 σ1 μ − 2 = 0. (D.2) ∂t c c ∂t 2 Eq. D.2 is the wave equation for the electric ﬁeld in a conducting and magnetic solid. If I take the curl of Eq. D.1d and follow exactly the same procedure, I obtain a wave equation for the magnetic ﬁeld: 4π ∂H 1 μ ∂ 2 H = 0. ∇ 2 H − 2 σ1 μ − 2 ∂t c c ∂t 2 I can employ either Eq. 2.5 or Eq. 2.6 in these to show that ω2 4π i ω2 q 2 = 2 1 μ + 2 ωσ1 μ = 2 μ, c c c exactly as in Eq. 3.35. 353

(D.3)

Appendix E Reflection and Transmission at Oblique Incidence I derived a formula for the reﬂectance at normal incidence in Chapter 3 (Section 3.6). (See Eq. 3.33.) Here, I’ll consider the reﬂectance at nonnormal incidence. Two neat effects will appear: zero reﬂectance at Brewster’s angle and zero transmittance in the regime of total internal reﬂection. I’ll ﬁrst discuss the relations amongst the angles of incident, reﬂected, and transmitted rays and then go on to obtain the transmission and reﬂection coefﬁcients. I’ll work out the angle relations in two ways: ﬁrst using Fermat’s principle and second by the boundary conditions. Fermat’s Principle of Least Time may be stated as “light travels between two given points along the path of shortest time.” In a single medium, this statement is equivalent to saying that light travels in straight lines.∗ Fermat’s principle may be regarded as an axiom, as an experimental observation, or as the results of solutions to Maxwell’s equations.

Reflection and Refraction In Fig. E.1, an incident light ray IO strikes (at point O) the interface between two media of complex refractive indices Na = na + iκa and Nb = nb + iκb . Part of the ray is reﬂected as ray OR and part transmitted as ray OT. The angles that the incident, reﬂected, and transmitted rays make to the normals of the interface are θi , θr , and θt , respectively. Light in medium a travels with speed va = c/na . The time it takes for the light to go from point I to point R via point O is the length of the path taken divided by the speed: y 2 + h2i ( − y)2 + h2r + T = Ti + T r = va va with the lengths deﬁned in Fig. E.1. Now the light could in principal take any path that starts at I, ends at O, and includes the interface.† For instance, it could go horizontally to the right to the interface and then slant up to R, so that y = 0. There are an inﬁnite number of such paths and Fermat tells me that the one taken has the minimum value of T . If so, y −y dT =0= − . 2 2 dy va y + hi va ( − y)2 + h2r ∗ I ignore the lensing of light by strong gravitational ﬁelds. But see Ref. 423. † Although I did not specify it, the interface must be smooth on the scale if the wavelength; this is the case of

specular reﬂection. If the surface is rough, light can travel from point I to point R via many spots on the interface. This second case is called diffuse reﬂectivity (or transmissivity) and is what you want for illumination. Metal mirrors are specular; white paper is diffuse.

354

355

Appendix E

Fig. E.1

Non-normal incidence at the interface between two media. The wave vectors qi , qr , and qt for the incident, reflected and transmitted waves are shown. The points I and R are separated along the interface (vertically here) by distance and are distances hi and hr above the interface. The point T has the same vertical distance from O as does R, but is ht below the interface. I look atthe triangles in the ﬁgure and see that sin θi = y/ y 2 + h2i and sin θr = ( − y)/ ( − y)2 + h2r . Hence, after substitution and a modest amount of algebra, I ﬁnd that the angle of the light leaving the surface is the same as the arrival angle. This result is the law of reﬂection,∗ θi = θr .

(E.1)

I drew Fig. E.1 with points I, O, R in the plane containing also the normal to the surface. I should consider whether the light could take some skewed path and reach R by going out of the plane deﬁned by I, O, R and the normal. But a little thought convinces me that such a path, which would go via a point on the interface O that is above or below point O, is longer than the one shown and so does not satisfy Fermat’s Principle of Least Time. The plane containing the wave vector of the incident light (qi ) and the surface normal is called the plane of incidence and the law of reﬂection says that this plane also contains the reﬂected wave vector qr . By the same argument, the transmitted wave vector qt is also in this plane. When light is transmitted across the interface, its speed changes to vb = c/nb . The time taken for light to travel from I to T is now 2 2 ( − y)2 + h2t y + hi + . T = Ti + T t = va vb

∗ I understand the diffuse reﬂection from a rough surface as satisfying the law of reﬂection locally, but the

roughness makes the local normal, when averaged over the surface, point in many of the possible directions.

356

Appendix E I set the derivative to zero and note that sin θt = ( − y)/ ( − y)2 + h2t . So after a modicum of algebra, including substituting for the velocities, I get Snell’s law: na sin θi = nb sin θt .

(E.2)

Let me now consider what the boundary conditions on the ﬁelds tell me. I’ll orient the coordinates so that the x axis is along the interface normal, into medium b. I’ll put the y axis in the interface and in the plane of incidence and the z axis in the interface perpendicular to the plane of incidence. For these coordinates, the real parts of the three wave vectors are ˆ Re qr = (ω/c)na (− cos θr xˆ + sin θr y), ˆ and Re qt = Re qi = (ω/c)na (cos θi xˆ + sin θi y), ˆ The ﬁelds in medium a are the superposition of incident ﬁeld (ω/c)nb (cos θt xˆ + sin θt y). and reﬂected ﬁeld; in medium b the transmitted ﬁeld. The boundary conditions to consider now are the continuity of tangential electric ﬁeld and tangential magnetic ﬁeld, written in the forms of Eqs. 2.5 and 2.6. These generically may be written (at x = 0) as Fi ei (

ωi c

na y sin θi −ωi t )

+ Fr ei (

ωr c

na y sin θr −ωr t )

= Ft ei (

ωt c

nb y sin θt −ωt t )

,

(E.3)

where F is either the electric or magnetic ﬁeld of the light wave. I have put subscripts on the frequency to allow me to think whether the frequencies of all three waves need to be the same. I can address the frequency issue quickly. So that the boundary conditions remain satisﬁed at all times, given that they are satisﬁed at one instant of time, the three harmonic terms must vary in time at the same rate. This conclusion follows from the linear nature of Maxwell’s equations. Hence, all ﬁelds vary in time as e−iωt . Now, the boundary conditions must be satisﬁed at all points on the interface as well. Suppose that they are satisﬁed at one particular point, such as y = z = 0. Then, in order that they remain true for other points on the interface, each term in Eq. E.3 must vary in the same fashion I move along the y axis and in the plane of the interface. This requirement means that the coefﬁcients of y must be equal. I get ω ω ω na sin θi = na sin θr = nb sin θt . c c c The ﬁrst pair reduce to the law of reﬂection θi = θr and the ﬁrst and third give Snell’s law na sin θi = nb sin θt .

Absorbing Media The propagation in strongly absorbing materials of waves incident at oblique angles to interfaces is complicated. Let me pose the problem and discuss it qualitatively. For the moment, I’ll take the material in which the incident and reﬂected waves are traveling as nonabsorbing.∗ ∗ A semi-inﬁnite absorbing medium poses conceptual dissonance. For a ﬁnite amount of energy to arrive at the

interface, it must have started with inﬁnite energy.

357

Appendix E

y

d

t

r

x

i

na

Fig. E.2

Nb

Nonnormal incidence at the interface between two media, one with refractive index na and the other with complex index Nb . The wave vectors for the incident, reflected and transmitted waves are shown. Also shown are the plane of incidence, the plane of constant phase for the incident wave, and the plane of constant amplitude for the transmitted wave.

The geometry is shown in Fig. E.2. The incident wave arrives at the interface at an angle to the normal. The planes of constant phase, to which the incident wave vector qi are normal, are also inclined. Because medium a is nonabsorbing, the intensity at the interface (or just before the interface) is everywhere the same. Light reaching the interface is refracted to continue as the transmitted wave. The planes of constant phase for the refracted wave, perpendicular to qt , are also inclined to the interface. What about the planes of constant amplitude? If the ﬁelds were to be written as eiqt ·r−ωt (Eqs. 3.11 and 3.12), the planes of constant amplitude would also be orthogonal to qt . But this claim is not correct. I see where the misconception comes from by looking at the four rays shown as dashed lines in Fig. E.2. When they arrive at a plane perpendicular to qt , the rays will have gone different distances in the absorbing medium, with the one at the bottom of the diagram having gone the farthest and the one at the top the shortest distance. Now, after crossing the interface, each ray or pencil of light does follow Eqs. 3.11 and 3.12 and, after reaching a depth d in medium b, has amplitude e−κb ωd/c cos θt . The planes of constant amplitude are parallel to the interface, as indicated in the ﬁgure. A wave where the planes of constant phase and the planes of constant amplitude are not the same is an inhomogeneous wave [8, 424, 425]. The details are worked out in Born and Wolf [8]. To evade this complication, I will take the refractive indices as real. The interesting phenomena and physics are in transparent media anyway.

358

Appendix E For further ease, I’ll take the materials to have μ = 1. The equations with different values of permeability may be seen in Jackson [2].

Amplitude Equations It turns out that the oblique-angle reﬂection depends both on the angle of incidence of the light and on its polarization (E-vector direction). The equations are called the “Fresnel equations” and it is conventional (and correct) to work them out separately for the electric ﬁeld parallel and perpendicular to the plane of incidence. Any other polarization direction can be worked out by superposition. The terminology is diverse and often used without explanation. If the electric ﬁeld lies in (is parallel to) the plane of incidence, I’ll call it p polarization, for “parallel.” The English word for perpendicular starts with same letter∗ so the polarization perpendicular to the plane of incidence is called s polarization (from “senkrecht,” German for perpendicular). Other terms used for p polarization are transverse-magnetic (TM), pipolarized, π -polarized, tangential-plane-polarized, and -polarized; s polarization can be called transverse-electric (TE), sigma-polarized σ -polarized, sagittal-plane-polarized, or ⊥-polarized. Finally, the plane of incidence, to which the ﬁeld is either perpendicular or parallel, is the plane deﬁned by the normal to the ﬂat interface and the incident wave vector, qi .† The boundary conditions are that the normal components of D and B and the tangential components of E and H are continuous across the interface. (With μ = 1, B = H.) I’ll use the coordinate system of Fig. E.2, with the x axis perpendicular to the interface. The y and z directions lie in the interface, with y also in the plane of incidence and z perpendicular to it.

Electric Field Perpendicular to the Plane of Incidence (s) The coordinate system and ﬁeld directions are shown in Fig. E.3. I write the ﬁelds (at the origin and at t = 0) as Ei = zˆ Er = rs zˆ Et = ts zˆ

(E.4)

Hi = na (xˆ sin θi − yˆ cos θi ) Hr = na rs (xˆ sin θi + yˆ cos θi ) Ht = nb ts (xˆ sin θt − yˆ cos θt )

∗ One source of confusion. † It is not the plane of the interface. Also, normal incidence has no plane of incidence (or has all planes as the

plane of incidence) and the subscripts p and s need not be used.

359

Fig. E.3

Appendix E

Geometry of transmission and reflection for s-polarized light. The interface between the two media (with refractive indices na and nb ) is the y–z plane. The plane of the paper is the plane of incidence. where I took the amplitude of the incident ﬁeld as unity, rs is the amplitude of the reﬂected ﬁeld, and ts is the amplitude of the transmitted ﬁeld. For the magnetic ﬁelds, I used qˆ × eˆ for the direction and Eq. 3.14 (H = N E) for the magnitudes. Now, I apply the boundary conditions. Tangential E is continuous. I dot the E ﬁeld with zˆ and equate the ﬁelds on left and right side of the interface: 1 + r s = ts ,

(E.5)

because the electric ﬁeld is purely tangential. Tangential H is continuous. The magnetic ﬁeld has both tangential and normal components. For the former, I dot with yˆ yielding −na cos θi + na rs cos θi = −nb ts cos θt .

(E.6)

I substitute ts from Eq. E.5 into Eq. E.6, and solve for the reﬂectivity rs =

na cos θi − nb cos θt . na cos θi + nb cos θt

(E.7)

Now, I put rs from Eq. E.7 back into Eq. E.5. It cleans up nicely: ts =

2na cos θi . na cos θi + nb cos θt

(E.8)

The angle θi = 0 at normal incidence as is θt = 0, by Snell’s law. Equations E.7 and E.8 reduce to Eqs. 3.30 and 3.31 at normal incidence, as they should. The other limit, θi = 90◦ , requires∗ me to specify that na < nb , in which case rs = 1 and ts = 0. I used two of the four boundary conditions. What about the other two? Well, D · xˆ = 0 for all three ﬁelds, so the normal D condition is trivially satisﬁed. As to normal B, I use

∗ Otherwise Snell’s law requires an angle for which the sine is greater than 1.

360

Fig. E.4

Appendix E

Geometry of transmission and reflection for p-polarized light. The interface between the two media (with refractive indices na and nb ) is the y–z plane. μ = 1 for both materials, so taking the dot product of the magnetic ﬁelds in Eq. E.4 with xˆ gives na sin θi + rs na sin θi = ts nb sin θt . But, Eq. E.5 gives 1 + rs = ts . By use of this boundary condition, I rederive Snell’s law.

Electric Field Parallel to the Plane of Incidence (p) The coordinate system and ﬁeld directions are shown in Fig. E.4. I’ve set the ﬁeld directions so that the case where θi = θr = 0 in Fig. E.4 uses the same convention as in Fig. 3.2: the electric ﬁelds are parallel and the magnetic ﬁelds antiparallel. I should warn you that about half the time I see a different convention. Some books [3, 5] use this convention; others [2, 4, 8] use the opposite one. I write the ﬁelds (at the origin and at t = 0) as Ei = −xˆ sin θi + yˆ cos θi Er = rp (xˆ sin θi + yˆ cos θi ) Et = tp (−xˆ sin θt + yˆ cos θt )

(E.9)

Hi = na zˆ Hr = −na rp zˆ Ht = nb tp zˆ where I took the amplitude of the incident ﬁeld as unity, rp is the amplitude of the reﬂected ﬁeld, and tp is the amplitude of the transmitted ﬁeld. I used qˆ × eˆ for the direction of the magnetic ﬁelds and Eq. 3.14 (H = N E) for their magnitudes.

361

Appendix E

Now, I apply the boundary conditions. Tangential E is continuous. I dot the E ﬁeld with yˆ and equate the ﬁelds on left and right side of the interface: cos θi + rp cos θi = tp cos θt .

(E.10)

Tangential H is continuous. The magnetic ﬁeld has only tangential components. I dot with zˆ yielding na − na rp = nb tp .

(E.11)

I substitute tp from Eq. E.11 into Eq. E.10, and solve for the reﬂectivity rp =

na cos θt − nb cos θi . na cos θt + nb cos θi

(E.12)

Now, I put rp from Eq. E.12 back into Eq. E.11. It cleans up nicely: tp =

2na cos θi . na cos θt + nb cos θi

(E.13)

Eqs. E.12 and E.13 reduce to Eq. 3.30 and 3.31 at normal incidence, as they should. The other limit, θi = 90◦ , again requires me to specify that na < nb , in which case rp = 1 and tp = 0. As far as the other two boundary conditions go, the condition on Bn is trivially satisﬁed and the condition on Dn gives Snell’s law. Equations E.7, E.8, E.12, and E.13 all contain both cos θi and cos θt . These quantities are not independent; Snell’s law (na sin θi = nb sin θt ) relates them. When I need to, I can use n2 (E.14) cos θt = 1 − a2 sin2 θi nb to eliminate cos θt . Meantime, however, I’ll calculate the reﬂected amplitudes in 4 cases: both polarizations with nb > na and both polarizations with nb < na . The results are in Fig. E.5. The left panel shows the results for the case where the light is incident from the “less dense” (smaller n) material onto the “more dense” (larger n) material. At normal incidence θi = 0, the reﬂectivity is negative, r = −1/3 (for na = 1 and nb = 2) in both the s and p cases∗ The reﬂectivity is basically ﬂat for the ﬁrst 5◦ or so but the two curves separate at larger angles. The s-polarized reﬂectivity becomes more negative (and hence larger in magnitude) eventually reaching rs = −1 at 90◦ incident angle. The p-polarized reﬂectivity becomes smaller in magnitude and crosses zero at an incident angle (for the refractive indices used) just above 60◦ . Then it grows in magnitude, reaching rp = +1 at 90◦ incident angle. Thus both polarizations have identical reﬂectivities at normal and at grazing incidence but nowhere in between. There are differences and similarities when the light is incident from the “more dense” (larger n) material onto the “less dense” (smaller n) material. The normal incidence reﬂectivity is positive rather than negative, with the same magnitude as the case I discussed above. The p-polarized reﬂectivity crosses zero at a smaller incident angle, just above ∗ As it should be. There is no plane of incidence when θ = 0. (Or,there is an inﬁnite number of them.) i

Appendix E

R

362

I

Fig. E.5

D

Amplitude reflectivity for p- and s-polarized light as a function of angle of incidence. Left panel: The media have na = 1 and nb = 2. Right panel: The media have na = 2 and nb = 1. 25◦ for the parameters used. The reﬂectivity reaches ±1, but at angles well below grazing incidence. Both s-polarized and p-polarized reﬂectivities reach rs = +1 and rp = −1 at 30◦ incident angle.

Special Angles There is one angle for a given na and nb when the value of rp goes to zero.∗ All the p-polarized incident light is purely refracted into the second medium. To ﬁnd the angle, I set rp = 0 in Eq. E.12 to ﬁnd n2 nb cos θi = na cos θt = na 1 − a2 sin2 θi , nb where I’ve used Eq. E.14 on the right to eliminate θt . I square both sides, use 1 = sin2 θi + cos2 θi , collect terms, take a square root, use tan = sin / cos, and ﬁnd that the angle of zero reﬂectivity, θB obeys nb tan θB = . (E.15) na

∗ The angle at which r changes sign! This statement is true for nonabsorbing media. In contrast, if there is p

absorption, there is a complex refractive index and the amplitude reﬂectivity is complex in turn. The magnitude of the complex reﬂectivity is always positive. It can get small at some angle, but will not be zero.

363

Appendix E This angle is known as Brewster’s angle. It is 63.4◦ for the left panel of Fig. E.5 and 26.6◦ for the right panel. It is 56◦ for an interface between glass (n = 1.5) and vacuum or air (n = 1). Finally for a silicon (n = 3.48)/vacuum interface, θB = 74◦ . When I calculate the angle between the reﬂected wave and the transmitted wave (the angle π − θr − θt in Fig. E.4 when θr = θi = θB ), I ﬁnd that the angle is 90◦ . I can see this in several ways: I can compute the angle using Eqs. E.2 and E.14 as well as some trigonometric identities and ﬁnd that the angle is π/2. An alternate way is to compute the angle for which qr · qt = 0 and ﬁnd that it is indeed θB . There is some physics in the fact that the reﬂectance is zero when the reﬂected and transmitted rays are at right angles to each other. I can ask “why is there light reﬂected from a surface and what are the sources of this light?” Electromagnetic radiation has as its sources accelerated charges. The transmitted ﬁeld in medium b induces a time-varying electric dipole moment/unit volume Pb = χ b Et = (b − 1)Et /4π where χ b is the complex susceptibility and b is the complex dielectric function. The dipole moment/unit volume is composed of a very large number of oscillating dipoles, each of which emits dipole radiation. The reﬂected light is the superposition of the emitted ﬁelds from all these dipoles. The dipoles are oriented along Et , which is perpendicular to qt and hence is, for p-polarized light, parallel to qr . But the radiated power is zero along the axis of the dipole; hence, the reﬂectivity is zero. At Brewster’s angle, reﬂected light is 100% s-polarized and transmitted light is preferentially p-polarized. A variety of devices take advantage of this selectivity. One of the simplest is a polarizer oriented for p polarization, and therefore suppressing reﬂected light from windows in photographs or optical instruments. A “pile of plates,” at Brewster’s angle, each reﬂecting a few percent of the s-polarized light, may be used to provide highly polarized transmitted light over a broad range of wavelengths. The other interesting angle, known as the critical angle, appears in the right panel of Fig. E.5; it is the angle of incidence at and beyond which the reﬂectivity is ±1. The phenomenon is known as “total internal reﬂection.” Whereas Brewster’s angle occurs only for p-polarized light and is found independent of which index is larger, the critical angle is found only if nb > na and occurs for both polarizations. Snell’s law, Eq. E.2, can be written sin θt = (na /nb ) sin θi . If na > nb , then θt > θi . There is then some incident angle for which θt = 90◦ . This, the critical angle, is then given by

nb . θ c = arcsin na All light is reﬂected and |rs | = |rp | = 1. The critical angle is 41.8◦ for a glass (na = 1.5) to air or vacuum (nb = 1) interface. For silicon (n = 3.48) to vacuum, θc = 16.7◦ . Recall that the angles are measured with respect to the normal, so light does not need to be sent to the interface at near grazing incidence to have total internal reﬂection. The effect of total internal reﬂection is to contain the light inside the medium. It is the basis of ﬁber optics and other dielectric wave guides or light pipes. That there is no transmitted light does not mean that the ﬁelds are zero in medium b. In fact, there are exponentially decaying evanescent ﬁelds in the second medium [2, 8].

364

Appendix E

Reflectance and Transmittance The Poynting vectors of incident, reﬂected, and transmitted waves tell me the intensities of the light in these beams. The reﬂectance R and transmittance T represent the fraction of the incident energy that is reﬂected or transmitted by the interface. Because intensity is energy/area, I’ll have to consider the change of area of the beams. For reﬂectance it is easy: the incident and reﬂected waves propagate in the same medium and make the same angle with the normal to the surface. Consequently the reﬂectance is R = |r|2 . The transmittance T is generally not equal to |t|2 for two reasons. First, the Poynting vector includes a factor of the refractive index n, just at it did in Chapter 3 (Section 3.5). Second, because the light is refracted into a different direction, the cross-sectional areas of a pencil or rays is different in the two media. The transmittance is T =

nb cos θt 2 |t| . na cos θi

(E.16)

The factor of nb /na comes from the ratio of Poynting vectors. The factor of cos θt / cos θi represents the change in area of the pencil of rays. The reﬂectance for s-polarized light is 2 2 2 na cos θi − nb 1 − na2 sin2 θi nb na cos θi − nb cos θt , = Rs = na cos θi + nb cos θt n cos θ + n 1 − n2a sin2 θ a i b i 2 n b

while the reﬂectance for p-polarized light is 2 na 1 − na cos θt − nb cos θi = Rp = na cos θt + nb cos θi n 1 − a

n2a n2b n2a n2b

2 sin2 θi − nb cos θi . 2 sin θi + nb cos θi

To obtain the second form of each equation I eliminated cos θt using Eq. E.14. I can calculate the transmittances for the two polarizations from Eqs. E.16, E.8, and E.13. As an alternative, I can invoke the conservation of energy and then the transmission coefﬁcients are given by T s = 1 − Rs ,

(E.17)

T p = 1 − Rp .

(E.18)

and

Appendix F A Field Guide to Optical “Constants”

What follows is a list and brief discussion of the optical functions used in studying the optical properties of solids.

Basic Functions I’ll start with the idea that I have measured the reﬂectance R and the phase shift on reﬂection φ (by Kramkers-Kronig, ellipsometry, analysis of thin ﬁlm data, or other means. Then, the complex refractive index N comes from the inversion of Eq. 3.32. (See also Eq. 10.24.) √ 1 − Reiφ . (F.1) N= √ 1 + Reiφ 1. Refractive index. The real part of N is n = Re(N ).

(F.2)

2. Extinction coefﬁcient. The imaginary part of N is κ = Im(N ).

(F.3)

Continuing, the complex dielectric function according to Eq. 3.10 is = N 2 . 3. Real dielectric function. 1 = Re().

(F.4)

2 = Im().

(F.5)

4. Imaginary dielectric function.

Equation 3.6 relates the complex dielectric function and complex conductivity. In cgs the conductivity and frequency are both measured in sec−1 and the relation is =1+

4π iσ , ω

(F.6)

whereas in SI the conductivity is in −1 m−1 , and it is =1+ 365

iσ , ω0

(F.7)

366

Appendix F with 0 the dielectric function of empty space. In lab units, frequencies are in cm−1 and conductivities are in −1 cm−1 , and the relation becomes =1+

60iσ . ω

(F.8)

5. Conductivity (real part). The real part of the conductivity (in −1 cm−1 ) is then ω2 σ1 = , (F.9) 60 with ω in cm−1 . This equation∗ can be compared to the expression in cgs: ω2 , σ1 = 4π

(F.10)

with ω in sec−1 and σ1 also in sec−1 . The cgs conductivity is 9×1011 times larger than the SI conductivity. 6. Conductivity (imaginary part). The imaginary part of the conductivity (in −1 cm−1 ) is ω(1 − 1) . (F.11) 60 Sometimes it is helpful to employ a partial dielectric function to eliminate c (including Maxwell’s displacement current) and/or other contributions: σ2 = −

σ2 = −

ω( 1 ) , 60

(F.12)

where 1 = 1 − c . 7. Absorption coefﬁcient. The absorption coefﬁcient (in cm−1 ) is α = 4π ωκ,

(F.13)

correct for ω in cm−1 . In cgs, this is α = 2ωκ/c,

(F.14)

where ω is in sec−1 . 8. Skin depth. In the skin effect the electric ﬁeld goes as e−x/δ but of course the wave governed by a refractive index N has a ﬁeld which decays as e−κωx/c (ω in rad/s). Hence: δ=

108 , 2π ωκ

(F.15)

˚ with ω in cm−1 . The factor of 108 makes the units of δ be A. ∗ The same factor of 60 appears if I calculate σ from the plasma frequency and relaxation rate, dc

σdc =

2 ωp

60(1/τ )

,

with ωp and 1/τ in cm−1 and σdc in −1 cm−1 . In reality, 60 = 377 /2π . If I want more accuracy, I √ have to use Z0 = 376.73 = μo /0 with μo and 0 respectively the magnetic permeability and electric permittivity of the vacuum. The factor changes a small amount: 60 → 59.958.

367

Appendix F

9. Loss function. The energy loss function governs the transmission of fast electrons through the material. These depend on the longitudinal response of the dielectric. It is typically written as − Im(1/); here I use L. L=

(12

1 2 = − Im . 2 + 2 )

(F.16)

10. Surface loss function. The “surface” energy loss function is Ls =

1 2 . = − Im 2 2 −1 ((1 − 1) + 2 )

(F.17)

Sum Rules 11. Conductivity sum rule. This is the most important sum rule function. The f-sum rule for solids can be written ∞ 2 ωp,tot σ1 (ω )dω = , (F.18) 8 0 where ωp,tot = 4π ntot e2 /m is the plasma frequency for all the electrons in the solid. I may write a partial sum rule (for the conduction band, say) as ω π ne2 σ1 (ω )dω = , (F.19) 2m∗ 0 where m∗ is the average effective mass of the band. If the upper limit is above the freecarrier contribution and below the onset of the interband transitions, the right hand side becomes ωp2 /8 with ωp the conduction band plasma frequency. Next, write n = Neff /Vc and let m be the free electron mass. The density n is in the number of effective electrons per unit cell volume (or formula volume). Then, calculate m 2mVc ω σ1 (ω )dω , (F.20) Neff ∗ = m π e2 0 with m the mass of an electron and m∗ the effective mass of the charge carriers. 12. Energy loss function sum rule. I may write a partial sum rule (for the conduction band, say) of the loss function as ω π ne2 1 ω L(ω )dω = , (F.21) 4π 0 2m∗ where m∗ is the average effective mass of the band. If the upper limit is above the freecarrier contribution and below the onset of the interband transitions, the right hand side becomes ωp2 /8 with ωp the conduction band plasma frequency. (The factor of 1/4π is the same as appears in ω2 /4π = σ1 .) Thus, ω m mVc Neff ∗ = ω L(ω )dω . (F.22) m 2π 2 e2 0 13. Surface loss function sum rule. It is the same as Eqs. F.21 and F.22, but for Ls .

368

Appendix F

Frequency-Dependent Scattering, Self-Energy, and Effective Mass The dielectric function of perfectly free (noninteracting) carriers with density n, charge ±e, and mass m is given by (ω) = c − with ωp , the plasma frequency, (in cgs)

ωp2

,

(F.23)

4π ne2 . m

(F.24)

ω2

ωp =

If I allow scattering of free carriers from impurities, defects, and surfaces with a mean free time τ or scattering rate 1/τ , independent of the frequency, the dielectric function has the Drude form: (ω) = c −

ωp2 ω2 + iω/τ

.

(F.25)

As discussed in Section 13.1, interactions make the scattering rate 1/τ a function of frequency (and probably also of temperature). However, to respect the Kramers– Kronig relations, one must consider the scattering rate to be a complex function or to have the effective mass m∗ also vary with frequency. Theorists have devised a number of such functions: a complex scattering (or memory) function , a complex scattering rate 1/τ ∗ and effective mass m∗ , a complex scattering rate 1/τ ∗ and mass enhancement factor λ, and a complex self-energy function .∗ Each and all of these quantities are calculable from the complex dielectric function. It is necessary to know the unrenormalized plasma frequency and c . (See below.) 14. Damping via memory function. The frequency dependent and complex damping is often written in an extended Drude model by replacing 1/τ by a “memory function” . I write = c −

ωp2 ω(ω + i)

,

(F.26)

with = 1 + i2 , = − c then ωp2

1 Im . ω

15. Imaginary part of the memory function. The imaginary part of is 1 = −

2 =

∗ There are actually two of these.

ωp2 ω

Re

1 + ω.

(F.27)

(F.28)

369

Appendix F 16. Scattering rate, 1/τ ∗. 1/τ ∗ = −ω

Im( ) . Re( )

(F.29)

17. Effective mass.

ωp2 m∗ 1 . = − 2 Re m

ω

(F.30)

18. Mass enhancement factor λ(ω). The effective mass may be written in terms of a mass enhancement factor λ(ω): m∗ = 1 + λ(ω). m

(F.31)

ωp2 1 λ(ω) = − 2 Re − 1.

ω

(F.32)

Hence,

19. Imaginary part of the (one-particle) self-energy. In some theories (such as the marginal Fermi liquid) the imaginary part of the self energy plays the role of a scattering rate, with the dielectric function (ω) = c −

ωp2 ω[ω − (ω)]

.

(F.33)

Here, ωp is the (unrenormalized)∗ plasma frequency and c the limiting high frequency value of the dielectric function. The imaginary part of is related to the quasiparticle lifetime through 1/τ ∗ (ω) = − Im (ω)(mb /m∗ (ω)) with m∗ the effective mass and mb the band mass. Note that 2 = −1 . Compute − Im via ωp2

1 Im , (F.34) ω

with = − c . One must know the plasma frequency and c . Or, one may subtract a model dielectric function that describes the noninteracting components to remove optical phonons and interband transitions. 20. Real (one-particle) self-energy. The real part of is related to the effective mass m∗ of the interacting carriers by − Im (ω) = −

m∗ (ω)/mb = 1 − Re (ω)/ω.

(F.35)

Hence, compute Re (ω) =

ωp2 ω

Re

1 + ω.

Note that 1 = +2 . ∗ Unrenormalized means “what it would be if there were no interactions.”

(F.36)

370

Appendix F

21. Imaginary part of the (two-particle) self-energy. A slightly different approach recognizes that optical excitations are created in pairs (electron and hole) and that the selfenergy should be a two-particle process. Still, the imaginary part of the self energy plays the role of a scattering rate, with the dielectric function written as (ω) = c −

ωp2 ω[ω − 2(ω/2)]

(F.37)

with ωp the (unrenormalized) plasma frequency and c the limiting high frequency value. The factors of 2 occur because the excitations are created in pairs (electronhole pairs or quasiparticle pairs). (These factors do not appear in all theoretical treatments. Indeed the “one-particle” versions are much more commonly seen.) The imaginary part of is related to the quasiparticle lifetime through 1/τ ∗ (ω) = −2 Im (ω/2)(mb /m∗ (ω)) with m∗ the effective mass and mb the band mass. Compute − Im via ωp2

1 (F.38) 2ω

with = −c . The (unrenormalized) plasma frequency and c must be known. Note that optical phonons and interband transitions may occur; one is allowed to subtract these from . After computing the right hand side of the above equation, one should divide the frequencies by 2, so that the dielectric function value at 400 cm−1 (for example) generates the − Im value at 200 cm−1 . 22. Real part of the (two-particle) self-energy. The real part of is related to the effective mass m∗ of the interacting carriers by − Im = −

Im

m∗ (ω)/mb = 1 − 2 Re (ω/2)/ω.

(F.39)

Hence, compute ωp2

1 + ω/2. (F.40) 2ω

After computing the right hand side of the above equation, divide the frequencies by 2, so that the dielectric function value at 400 cm−1 (for example) generates the Re value at 200 cm−1 . Re (ω/2) =

Re

Specialized Functions, Mostly for Superfluids 23. Superﬂuid plasma frequency. A superﬂuid has a dielectric function that is = c −

with ωps

2 ωps

, ω2 the superﬂuid plasma frequency. Calculate ωps = ω2 | Re( )|,

(F.41)

(F.42)

371

Appendix F

where the absolute value is used instead of a minus sign to avoid numerical problems. I have to be sure that is negative when invokeing this function! If ωps is (nearly) constant in frequency, the behavior is that of a superﬂuid. 24. Number of “free carriers.” Again, writing 2 ωps (F.43) = c − 2 , ω 2 = 4π N (ω)e2 /V m so with ωps the superﬂuid plasma frequency. Then, write ωps s c that:

Ns (ω) = ω2 Vc (m/4π e2 )| Re( )|,

(F.44)

Ns (ω) should be nearly constant as a function of frequency for the concept to be valid. 25. London penetration depth. The dielectric function in Eqs. F.41 or F.43 is that of a London superconductor, so one may also calculate λL as 108 , (F.45) λL = 2π ω | Re( )| ˚ λL (ω) should be with ω in cm−1 . The factor of 108 makes the units of λL (ω) in A. nearly constant as a function of frequency for the concept to be valid.

Other Specialized Functions 28. Optical resistivity (real part). The optical resistivity is just the inverse of the optical conductivity, so the real part is

1 . (F.46) ρ1 = Re σ

Because σ is complex, ρ1 = σ1 / σ12 + σ22 . 29. Optical resistivity (imaginary part). The imaginary part of the optical resistivity is

1 . (F.47) ρ2 = Im σ 30. Absolute value of the dielectric function. There are examples where the magnitude of the complex dielectric function || displays power law behavior. Hence, calculate || = 12 + 22 . (F.48) Note that this should be the entire function, so c is not generally subtracted. 31. Absolute value of the conductivity. This quantity is |σ | = σ12 + σ22 .

(F.49)

32. Tan(δ). The loss tangent is commonly used in the analysis of RF and microwave experiments. It is 2 (F.50) tan δ = . 1 This calculation uses the entire function, so c is not generally subtracted.

Appendix G Software

Data analysis programs for working with optical spectra are available at www.cambridge.org/tanner. These run in Windows (7 through 10 at least). They are not true Windows applications, though, lacking the message boxes, drop-down menus, radio buttons, tool tips, animated paper clips, etc. that we’ve come to know and love. Installation is accomplished by extracting the zip ﬁle into a directory on your path. Then read “man.pdf,” the manual. Run the programs from a command window. You can also add links on the desktop; most will accept drag/drop from Windows Explorer. The zip ﬁle includes the following programs: Data manipulation cmp.exe Compute with spectra: +, −, ∗, / and more. interp.exe Interpolate at evenly spaced points. fts.exe Fourier-transform smoothing of data. gtf.exe Glover–Tinkham conductivity of a ﬁlm from R/T . mav.exe Merge and average overlapping data sets. pik.exe Pick sections out of a data ﬁle. q.exe Quickly make plot on the screen. t2a.exe T to α. Allows for reﬂections at the surfaces. Kramers–Kronig analysis kk.exe Kramers–Kronig analysis of R or T . Requires xro for extrapolation. op.exe Optical properties from Kramers–Kronig results. xro.exe Compute extrapolated x-ray reﬂectance from atomic scattering data. Fitting dff.exe Dielectric function ﬁt. Least square to models. dfc.exe Dielectric function calculate. Companion to dff/tff. pfit.exe Power series ﬁt, to up to x 8 . tff.exe Thin ﬁlm ﬁt. Least-square to R or T . Many models. Utilities j2w.exe Converts JCAMP ﬁles to two column data. w2l.exe Convert from wavenumber to wavelength. And others Read the manual. The Kramers–Kronig (reﬂectance) code was written by Claus Jacobsen. The leastsquares minimization uses a routine by Bevington. Most of the other important routines were written by Charles Porter; the rest is by David Tanner. The programs are free to all to use and to redistribute, subject only to a request that users acknowledge the principal author, Charles Porter. 372

References

[1] J. Clerk Maxwell, “A dynamical theory of the electromagnetic ﬁeld,” Phil. Trans. Royal Soc. (London) 155, 459–512 (1865). [2] J.D. Jackson, Classical Electrodynamics (John Wiley & Sons, New York, 1975). [3] L.D. Landau and E.M. Lifshitz, Electrodynamics of Continuous Media (Pergamon, New York, 1960). [4] M.A. Heald and J.B. Marion, Classical Electromagnetic Radiation (Saunders College Publishing, Philadelphia, 1995). [5] D.J. Grifﬁths, Introduction to Electrodynamics (Prentice Hall, Upper Saddle River, New Jersey, 1999). [6] W.R. Smythe, Static and Dynamic Electricity (McGraw-Hill, New York, 1950). [7] M.V. Klein and T.E. Furtak, Optics (Wiley, New York, 1986). [8] M. Born and E. Wolf, Principles of Optics (Pergamon, Oxford, 1970). [9] V.G. Veselago, “The electrodynamics of substances with simultaneously negative values of and μ,” Soviet Physics Uspekhi 10, 509–514 (1968). [10] M.W. McCall, A. Lakhtakia, and W.S. Weiglhofer, “The negative index of refraction demystiﬁed,” Eur. J. Phys. 23, 353–359 (2002). [11] J. Pendry, “Optics: Positively negative,” Nature 423, 22–23 (2003). [12] S.A. Ramakrishna, “Physics of negative refractive index materials,” Rep. Prog. Phys. 68, 449–521 (2005). [13] V.M. Shalaev, “Optical negative-index metamaterials,” Nat. Photon. 1, 41–48 (2007). [14] R.A. Shelby, D.R. Smith, and S. Schultz, “Experimental veriﬁcation of a negative index of refraction,” Science 292 77–79 (2001). [15] L.I. Schiff, Quantum Mechanics (McGraw-Hill, New York, 1968). [16] P. Drude, “Zur Elektronentheorie der Metalle” (“The electron theory of metals”), Ann. Phys. (Leipzig) 1, 566 (1900). [17] www.pdi-berlin.de/outreach/paul-drude. His important papers and books published in German in 1890, 1894, 1900, 1902, and 1904 are listed here. See also Paul Drude, The Theory of Optics (Dover, Mineola, 2005). [18] D.C. Johnston, “The puzzle of high temperature superconductivity in layered iron pnictides and chalcogenides,” Adv. Phys., 59, 803–1061 (2010). [19] N.W. Ashcroft and N.D. Mermin, Solid State Physics (Holt, Rinehart and Winston, Philadelphia, 1976). ¨ [20] E. Hagen and H. Rubens, “Uber die Beziehung des Reﬂexions- und Emissionsverm¨ogens der Metalle zu ihrem elektrischen Leitverm¨ogen” (“On the relation 373

374

References

[21]

[22]

[23] [24] [25] [26] [27]

[28] [29] [30] [31] [32] [33] [34] [35] [36] [37]

[38]

of reﬂectivity and emissivity of metals with their electrical conductivity”), Ann. Phys. (Leipzig) 4, 873 (1903). R. Landauer, in Electrical Transport and Optical Properties of Inhomogeneous Media, edited by J.C. Garland and D.B. Tanner (The American Institute of Physics, New York, 1978), p. 1. B.L. Henke, E.M. Gullikson, and J.C. Davis, “X-ray interactions: Photoabsorption, scattering, transmission, and reﬂection at E = 50–30000 eV, Z = 1–92,” Atom. Data Nucl. Data Tables 54, 181–342 (1993). G. Burns, Solid State Physics (Academic Press, San Diego, 1985). C. Kittel, Introduction to Solid State Physics (Wiley, New York, November 2004). The 3rd and 5th editions are worth looking at also. N.A. Spaldin, “A beginner’s guide to the modern theory of polarization,” J. Solid State Chem. 195, 2–10 (2012). D. Vanderbilt, “Soft self-consistent pseudopotentials in a generalized eigenvalue formalism,” Phys. Rev. B, 41, 7892 (1990). K. Laasonen, A. Pasquarello, R. Car, C. Lee, and D. Vanderbilt, “Car-Parrinello molecular dynamics with Vanderbilt ultrasoft pseudopotentials,” Phys. Rev. B, 47, 10142 (1993). M. Tinkham, Group Theory and Quantum Mechanics (Dover, Mineola, New York, 2003). G. Burns, Introduction to Group Theory with Applications (Academic Press, New York, 1977). M.S. Dresselhaus, “Applications of Group Theory to the Physics of Solids,” MIT (2002). web.mit.edu/course/6/6.734j/www/group-full02.pdf. Wikipedia, the free encyclopedia, “Pole–zero plot,” (2018). http://en.wikipedia.org/ wiki/Pole-zero plot. R. Lyddane, R. Sachs, and E. Teller, “On the polar vibrations of alkali halides,” Phys. Rev. 59, 673–676 (1941). W. Cochran and R.A. Cowley, “Dielectric constants and lattice vibrations,” J. Phys. Chem. Solids 23, 447–450 (1962). A.S. Barker, Jr., “Long-wavelength soft modes, central peaks, and the LyddaneSachs-Teller relation,” Phys. Rev. B 12, 4071–4084 (1975). A.J. Sievers and J.B. Page, “Generalized Lyddane-Sachs-Teller relation and disordered solids,” Phys. Rev. B 41, 3455–3459 1990. A.S. Barker and M. Tinkham, “Far-infrared ferroelectric vibration mode in SrTiO3 ,” Phys. Rev. 125, 1527–1530 (1962). W.G. Spitzer, R.C. Miller, D.A. Kleinmann, and L.E. Howarth, “Far infrared dielectric dispersion in BaTiO3 , SrTiO3 , and TiO2 ,” Phys. Rev. 126, 1710–1721 (1962). 20 K. Kamar´as, K.-L. Barth, F. Keilmann, R. Henn, M. Reedyk, C. Thomsen, M. Cardona, J. Kircher, P.L. Richards, and J.-L. Stehl´e, “The low-temperature infrared optical functions of SrTiO3 determined by reﬂectance spectroscopy and spectroscopic ellipsometry,” J. Appl. Phys. 78, 1235–1240 (1995).

375

References

[39] R. Henn, A. Wittlin, M. Cardona, and S. Uchida, “Dynamics of the c-polarized infrared-active modes in La2−x Srx CuO4 ,” Phys. Rev. B 56, 6295–6301 1997. [40] R.B. Sanderson, “Far infrared optical properties of indium antimonide,” J. Phys. Chem. Solids 26, 803–810 (1965). [41] A.G. Shenstone, “The arc spectrum of silver,” Phys. Rev. 57, 894 (1940). [42] J.C. Pickering and V. Zilio, “New accurate data for the spectrum of neutral silver,” Eur. Phys. J. D 13, 181 (2001). [43] E.D. Palik, Handbook of Optical Constants of Solids I and II (Academic Press, Orlando, Florida, 1985 and 1991). [44] E.A. Taft and H.R. Philipp, “Optical constants of silver,” Phys. Rev. 121, 1100–1103 1961. [45] H. Ehrenreich and H.R. Philipp, “Optical properties of Ag and Cu,” Phys. Rev. 128, 1622 (1962). [46] H. Bennett, M. Silver, and E. Ashley, “Infrared reﬂectance of aluminum evaporated in ultra-high vacuum,” J. Opt. Soc. Am. 53, 1089–1095 (1963). [47] J.M. Bennett, E.J. Ashley, “Infrared reﬂectance and emittance of silver and gold evaporated in ultrahigh vacuum,” Appl. Optics 4, 221–224 (1965). ¨ [48] B. Dold and R. Mecke, “Uber Gangsmetallen und deren Legierungen im Infrarot” (“About transition metals and their alloys in the infrared”), Optik 22, 435 (1965). [49] G. Irani, T. Huen, and F. Wooten, “Optical constants of silver and gold in the visible and vacuum ultraviolet,” J. Opt. Soc. Am. 61, 128–129 (1971). [50] H.J. Hagemann, W. Gudat, and C. Kunz, “Optical constants from the far infrared to the x-ray region: Mg, Al, Cu, Ag, Au, Bi, C, and Al2O3,” J. Opt. Soc. Am. 65, 742 (1975). See also DESY Report SR-74/7, Hamburg, 1974. [51] P. Winsemius, F.F. van Kampen, H.P. Lengkeek, and C.G. van Went, “Temperature dependence of the optical properties of Au, Ag, and Cu,” J. Phys. F, 6, 1583 (1976). [52] G. Leveque, C.G. Olson, and D.W. Lynch, “Reﬂectance spectra and dielectric functions for Ag in the region of interband transitions,” Phys. Rev. B 27, 4654 (1983). [53] H.U. Yang, J. D’Archangel, M.L. Sundheimer, E. Tucker, G.D. Boreman, and M.B. Raschke, “Optical dielectric function of silver,” Phys. Rev. B 91, 235137 (2015). [54] F. Wooten, Optical Properties of Solids (Academic Press, New York, 1972). [55] S. Roberts, “Optical properties of copper,” Phys. Rev. 118, 1509 (1960). [56] A.D. Raki´c, A.B. Djuriˇsic, J.M. Elazar, and M.L. Majewski, “Optical properties of metallic ﬁlms for vertical-cavity optoelectronic devices,” Appl. Opt. 37, 5271–5283 (1998). [57] “Optical constants of Cu, Ag, and Au revisited,” S. Babar and J. H. Weaver, Appl. Opt. 54, 477–481 (2015). [58] L.R. Canﬁeld, G. Hass, and W.R. Hunter, “The optical properties of evaporated gold ˚ to 2000 A ˚ ,” J. de Physique 25, 124 (1964). in the vacuum ultraviolet from 300 A [59] H. Ehrenreich, H.R. Philipp, and B. Segall, “Optical properties of aluminum,” Phys. Rev. 132, 1918–1928 (1963).

376

References

[60] E. Shiles, T. Sasaki, M. Inokuti, and D.Y. Smith, “Self-consistency and sum-rule tests in the Kramers-Kronig analysis of optical data: Applications to aluminum,” Phys. Rev. B 22, 1612 (1980). [61] D.Y. Smith and B. Segall, “Intraband and interband processes in the infrared spectrum of metallic aluminum,” Phys. Rev. B 34, 5191–5198 (1986). [62] D. Brust, “Electronic structure effects in the Drude and interband absorption of aluminum,” Phys. Rev. B 2, 818–825 (1970). [63] H.H. Li, “Refractive index of silicon and germanium and its wavelength and temperature derivatives,” J. Phys. Chem. Ref. Data 9, 561–658 (1980). [64] D.F. Edwards and E. Ochoa, “Infrared refractive index of silicon,” Appl. Optics 19, 4130–4131 (1980). [65] W.R. Thurber, R.L. Mattis, Y.M. Liu, and J. J. Filliben, “Resistivity-dopant density relationship for phosphorus-doped silicon,” J. Electrochem. Soc. 127, 1807–1812 (1980). [66] H.R. Philipp and E.A. Taft, “Optical constants of silicon in the region 1 to 10 eV,” Phys. Rev. 120, 37–38 (1960). [67] H.R. Philipp and H. Ehrenreich. “Optical properties of semiconductors,” Phys. Rev. 129, 1550–1560 (1963). [68] D.E. Aspnes and A.A. Studna, “Dielectric functions and optical parameters of Si, Ge, GaP, GaAs, GaSb, InP, InAs, and InSb from 1.5 to 6.0 eV,” Phys. Rev. B 27, 985–1009 (1983). [69] G.E. Jellison Jr., “Optical functions of silicon determined by two-channel polarization modulation ellipsometry,” Opt. Mat. 1, 41–47 (1992). [70] C.M. Herzinger, B. Johs, W.A. McGahan, J.A. Woollam, and W. Paulson, “Ellipsometric determination of optical constants for silicon and thermally grown silicon dioxide via a multi-sample, multi-wavelength, multi-angle investigation,” J. Appl. Phys. 83, 3323–3336 (1998). [71] D. Chandler-Horowitz and P.M. Amirtharaj, “High-accuracy, midinfrared (450 cm−1 ≤ ω ≤ 4000 cm−1 ) refractive index values of silicon,” J. Appl. Phys. 97, 123526/ 1–8 (2005). [72] H. Ehrenreich, H.R. Philipp, and J.C. Phillips, “Interband transitions in groups 4, 3-5, and 2-6 semiconductors,” Phys. Rev. Lett. 8, 59–61 (1962). [73] J.C. Phillips, “Band structure of silicon, germanium, and related semiconductors,” Phys. Rev. 125, 1931–1936 (1962). [74] D. Brust, “Electronic spectra of crystalline germanium and silicon,” Phys. Rev. 134, A1337–A1353 (1964). [75] J.P. Walter and M.L. Cohen “Frequency- and wave-vector-dependent dielectric function for silicon,” Phys. Rev. B 5, 3101–3110 (1972). [76] J.R. Chelikowsky and M.L. Cohen, “Electronic structure of silicon,” Phys. Rev. B 10, 5095–5107 (1974). [77] O.S. Heavens, Optical Properties of Thin Solid Films (Dover, Mineola, NY, 1955). [78] K.B. Blodgett, “Interference colors in oil ﬁlms on water,” J. Opt. Soc. Am. 24, 313–315 (1934).

377

References

[79] E. Shevtsova, C. Hansson, D.H. Janzen, and J. Kjærandsen, “Stable structural color patterns displayed on transparent insect wings,” Proc. Nat. Acad. Sci. 108, 668–673 (2011). [80] B.P. Abbott et al. (LIGO Scientiﬁc Collaboration), “LIGO: The Laser Interferometer Gravitational-wave Observatory,” Rep. Prog. Phys. 72, 076901/1–25 (2009). [81] H. Kogelnik and T. Li, “Laser beams and resonators,” Appl. Optics, 5, 1550–1567 (1966). [82] A.E. Siegman, Lasers (University Science Books, Mill Valley, Calif., 1986). [83] F. Abel´es, “La th´eorie g´en´erale des couches minces,” (“The general theory of thin ﬁlms,”), J. Phys. Radium 11, 307–310 (1950). [84] R.E. Glover and M. Tinkham, Phys. Rev., 107, 844 (1956); ibid., Phys. Rev. B 108, 1175 (1957). [85] L.H. Palmer and M. Tinkham, Phys. Rev. 165, 588 (1968). [86] D.R. Karecki, G.L. Carr, S. Perkowitz, D.U. Gubser, and S.A. Wolf, Phys. Rev. B 27, 5460 (1983). [87] F. Gao, G.L. Carr, C.D. Porter, D.B. Tanner, G.P. Williams, C.J. Hirschmugl, B. Dutta, X.D. Wu, and S. Etemad, “Quasiparticle damping and the coherence peak in YBa2 Cu3 O7−δ ,” Phys. Rev. B 54, 700–710 (1996). [88] H. Tashiro, J.M. Graybeal, D.B. Tanner, E.J. Nicol, J.P. Carbotte, and G.L. Carr, “Unusual thickness dependence of the superconducting transition of α-MoGe thin ﬁlms,” Phys. Rev. B 78, 014509/1–7 (2008). [89] A. Sommerfeld and H. Bethe, “Elektronentheorie der Metalle” (“Electron Theory of Metals”), Handbuch der Physik 24, 333–622 (1933). [90] N.F. Mott and H. Jones, The Theory of the Properties of Metals and Alloys (Oxford University Press, London and New York, 1936). [91] A.H. Wilson, The Theory of Metals (Cambridge University Press, Cambridge, 1953). [92] T. Holstein, Phys. Rev., 96, 535 (1954); Ann. Phys. (N.Y.) 29, 410 (1964). [93] Handbook of Electronic Tables and Formulas; www.powerstream.com/Wire Size .htm. [94] P. Debye, “Zur Theorie der speziﬁschen W¨arme,” (“The theory of speciﬁc heat”), Ann. der Physik (Leipzig) 39, 789 (1912). [95] D.B. Tanner and D.C. Larson, “Electrical resistivity of silver ﬁlms,” Phys. Rev., 166, 652–655 (1968). [96] J. Cochran and M. Yaqub, “The mean free path of electrons in very pure gallium,” Phys. Lett. 5, 307–309 (1963). [97] K. Huang, Statistical Mechanics, 2nd ed. (John Wiley & Sons, New York, 1987). [98] M.L. Cohen and S.G. Louie, Fundamentals of Condensed Matter Physics (Cambridge University Press, Cambridge, 2016). [99] M.P. Marder, Condensed Matter Physics (John Wiley & Sons, New York, 2010). [100] J.M. Ziman, Principles of the Theory of Solids, 2nd ed. (Cambridge University Press, Cambridge, 1972). [101] J.M. Ziman, Electrons and Phonons: The Theory of Transport Phenomena in Solids (Clarendon Press, Oxford, 1960).

378

References

[102] R. de L. Kronig, “On the theory of the dispersion of X-rays,” J. Opt. Soc. Am. 12, 547–557 (1926). [103] H.A. Kramers, “La diffusion de la lumiere par les atomes” (“The diffusion of light by atoms”), J. Atti Cong. Intern. Fisici, (Transactions of Volta Centenary Congress) Como 2, 545–557 (1927); “Die dispersion und absorption von R¨ontgenstrahlen” (“The dispersion and absorption of X-rays”), Phys. Z. 30, 522–523 (1929). [104] C. Kittel Elementary Statistical Physics (Wiley, New York, 1958). [105] M. Dressel and G. Gr¨uner, Electrodynamics of Solids: Optical Properties of Electrons in Matter (Cambridge University Press, Cambridge, 2002). [106] J.S. Toll, “Causality and the dispersion relation: Logical foundations,” Phys. Rev. 104, 1760–1770 (1956). [107] R. Kubo and M. Ichimura, “Kramers-Kronig relations and sum rules,” J. Math. Phys. 13, 1454 (1972). [108] B.Y.-K. Hu, “Kramers-Kronig in two lines,” Am. J. Phys. 57, 821–821 (1989). [109] K.-E. Peiponen and E.M. Vartiainen, “Kramers-Kronig relations in optical data inversion,” Phys. Rev. B 44, 8301 (1991). [110] G.W. Milton, D.J. Eyre, and J.V. Mantese, “Finite frequency range Kramers-Kronig relations: Bounds on the dispersion,” Phys. Rev. Lett. 79, 3062–3065 (1997). [111] F.W. King, “Efﬁcient numerical approach to the evaluation of Kramers-Kronig transforms,” J. Opt. Soc. Am. B 19, 2427–2436 (2002). [112] F.W. King, “Alternative approach to the derivation of dispersion relations for optical constants,” J. Phys. A: Math. Gen. 39, 10427 (2006). [113] K.-E. Peiponen and J.J. Saarinen, “Generalized Kramers-Kronig relations in nonlinear optical- and THz-spectroscopy,” Rep. Prog. Phys. 72, 056401 (2009). [114] C.F. Bohren, “What did Kramers and Kronig do and how did they do it?” Eur. J. Phys. 31, 573–577 (2010). [115] A.L. Cauchy, “Oeuvres compl`etes,” Ser. 1, 4, Paris (1890). [116] F.C. Jahod, “Fundamental absorption of barium oxide from its reﬂectivity spectrum,” Phys. Rev. 107, 1261–1265 (1957). [117] H.R. Phillip and E.A. Taft, “Kramers-Kronig analysis of reﬂectance data for diamond,” Phys. Rev. 136, A1445–A1448 (1964). [118] E.A. Taft and H.R. Philipp, “Optical properties of graphite,” Phys. Rev. 138, A197– A202 (1965). [119] S. Tongay, J. Hwang, H.K. Pal, D.B. Tanner, D. Maslov, and A.F. Hebard, “Supermetallic conductivity in bromine-intercalated graphite,” Phys. Rev. B 81, 115428/1–6 (2010). [120] C.S. Jacobsen, D.B. Tanner, A.F. Garito, and A.J. Heeger, “Single-crystal reﬂectance studies of tetrathiofulvalene tetracyanoquinodimethane,” Phys. Rev. Lett. 33, 1559–1562 (1974). [121] C.S. Jacobsen, D.B. Tanner, and K. Bechgaard, “Dimensionality crossover in the organic superconductor tetramethyltetraselenafulvalene hexaﬂuorophosphate [(TMTSF)2 PF6 ],” Phys. Rev. Lett. 46, 1142–1145 (1981).

379

References

[122] M. Dressel, A. Schwartz, G. Gr¨uner, and L. Degiorgi, “Deviations from Drude response in low-dimensional metals: electrodynamics of the metallic state of (TMTSF)2 PF6 ,” Phys. Rev. Lett. 77, 398–402 (1996). [123] A.R. Beal and H.P. Hughes, “Kramers-Kronig analysis of the reﬂectivity spectra of 2H-MoS2 , 2H-MoSe2 and 2H-MoTe2 ,” J. Phys. C: Solid State Phys. 12, 881 (1979). [124] L.H. Greene, D.B. Tanner, A.J. Epstein, and Joel S. Miller, “Optical properties of the cation-deﬁcient platinum chain salt K1.75 Pt(CN)4 · 1.5H2 O,” Phys. Rev. B 25, 1331–1338 (1982). [125] W.A. Challener and P.L. Richards, “Far infrared optical properties of NbSe3 ,” Solid State Comm. 52, 117–121 (1984). [126] C.R. Fincher Jr, M. Ozaki, M. Tanaka, D. Peebles, L. Lauchlan, A.J. Heeger, and A.G. MacDiarmid. “Electronic structure of polyacetylene: Optical and infrared studies of undoped semiconducting (CH)x and heavily doped metallic (CH)x ,” Phys. Rev. B 20, 1589–1598 (1979). [127] S. Stafstr¨om, J.L. Br´edas, A.J. Epstein, H.S. Woo, D.B. Tanner, W.S. Huang, and A.G. MacDiarmid, “Polaron lattice in highly conducting polyaniline: Theoretical and optical studies,” Phys. Rev. Lett. 59, 1464–1467 (1987). [128] K. Lee, S. Cho, S.H. Park, A.J. Heeger, C.-W. Lee, and S.-H. Lee, “Metallic transport in polyaniline,” Nature 441, 65–68 (2006). [129] D.A. Bonn, J.E. Greedan, C.V. Stager, T. Timusk, M.G. Doss, S.L. Herr, K. Kamar´as, and D.B. Tanner, “Far-infrared conductivity of the high-Tc superconductor YBa2 Cu3 O7 ,” Phys. Rev. Lett. 58, 2249–2250 (1987). [130] M. Reedyk, D.A. Bonn, J.D. Garrett, J.E. Greedan, C.V. Stager, T. Timusk, K. Kamar´as, and D.B. Tanner, “Far-infrared optical properties of Bi2 Sr2 CaCu2 O8 ,” Phys. Rev. B 38, 11,981–11,984 (1988). [131] K. Kamar´as, S.L. Herr, C.D. Porter, N. Tache, D.B. Tanner, S. Etemad, T. Venkatesan, E. Chase, A. Inam, X.D. Wu, M.S. Hegde, and B. Dutta, “In a clean high-Tc superconductor you do not see the gap,” Phys. Rev. Lett. 64, 84–87 (1990). [132] S.L. Cooper, G.A. Thomas, J. Orenstein, D.H. Rapkine A.J. Millis, S.-W. Cheong, A.S. Cooper, and Z. Fisk, “Growth of the optical conductivity in the Cu-O planes,” Phys. Rev. B 41, 11,605–11,608 (1990). [133] F. Gao, D.B. Romero, D.B. Tanner, J. Talvacchio, and M.G. Forrester, “Infrared properties of epitaxial La2−x Srx CuO4 thin ﬁlms in the normal and superconducting states,” Phys. Rev. B 47, 1036–1052 (1993). [134] S.L. Cooper, D. Reznik, A. Kotz, M.A. Karlow, R. Liu, M.V. Klein, W.C. Lee, J. Giapintzakis, D.M. Ginsberg, B. Veal, and A.P. Paulikas, “Optical studies of the a-, b-, and c-axis charge dynamics in YBa2 Cu3 O6+x ,” Phys. Rev. B 47, 8233–8248 (1993). [135] C.C. Homes, T. Timusk, R. Liang, D.A. Bonn, and W.N. Hardy, “Optical conductivity of c axis oriented YBa2 Cu3 O6.70 : Evidence for a pseudogap,” Phys. Rev. Lett. 71, 1645 (1993).

380

References

[136] D.N. Basov, A.V. Puchkov, R.A. Hughes, T. Strach, J. Preston, T. Timusk, D.A. Bonn, R. Liang, and W.N. Hardy, “Disorder and superconducting-state conductivity of single crystals of YBa2 Cu3 O6.95 ,” Phys. Rev. B 49, 12,165–12,169 (1994). [137] D.N. Basov, R. Liang, D.A. Bonn, W.N. Hardy, B. Dabrowski, M. Quijada, D.B. Tanner, J.P. Rice, D.M. Ginsberg, and T. Timusk, “In-plane anisotropy of the penetration depth in YBa2 Cu3 O7−x and YBa2 Cu4 O8 superconductors,” Phys. Rev. Lett. 74, 598–601 (1995). [138] M.A. Quijada, D.B. Tanner, R.J. Kelley, M. Onellion, and H. Berger, “Anisotropy in the ab-plane optical properties of Bi2 Sr2 CaCu2 O8 single-domain crystals,” Phys. Rev. B 60, 14,917–14,934 (1999). [139] A.V. Puchkov, P. Fournier, T. Timusk, and N.N. Kolesnikov, “Optical conductivity of high Tc superconductors: From underdoped to overdoped,” Phys. Rev. Lett. 77, 1853 (1996). [140] S.G. Kaplan, M.A. Quijada, H.D. Drew, D.B. Tanner, G.C. Xiong, R. Ramesh, C. Kwon, and T. Venkatesan, “Optical evidence for the dynamic Jahn-Teller effect in Nd0.7 Sr0.3 MnO3 ,” Phys. Rev. Lett. 77, 2081–2084 (1996). [141] Y. Murakami, H. Kawada, H. Kawata, M. Tanaka, T. Arima, Y. Moritomo, and Y. Tokura “Direct observation of charge and orbital ordering in La0.5 Sr1.5 MnO4 ,” Phys. Rev. Lett. 80, 1932–1935 (1998). [142] K.H. Kim, J.H. Jung, and T.W. Noh, “Polaron absorption in a perovskite manganite La0.7 Ca0.3 MnO3 ,” Phys. Rev. Lett. 81, 1517–1520 (1998). [143] G. Li, W.Z. Hu, J. Dong, Z. Li, P. Zheng, G.F. Chen, J.L. Luo, and N.L. Wang, “Probing the superconducting energy gap from infrared spectroscopy on a Ba0.6 K0.4 Fe2 As2 single crystal with Tc = 37 K,” Phys. Rev. Lett. 101, 107004 (2008). [144] A. Lucarelli, A. Dusza, F. Pfuner, P. Lerch, J.G. Analytis, J.-H. Chu, I.R. Fisher, and L. Degiorgi, “Charge dynamics of Co-doped BaFe2 As2 ,” New J. Phys. 12, 073036 (2010). [145] N. Bariˇsi´c, D. Wu, M. Dressel, L. J. Li, G. H. Cao, and Z. A. Xu, “Electrodynamics of electron-doped iron pnictide superconductors: Normal-state properties,” Phys. Rev. B 82, 054518 (2010). [146] B. Cheng, B.F. Hu, R.Y. Chen, G. Xu, P. Zheng, J.L. Luo, and N.L. Wang, “Electronic properties of 3d transitional metal pnictides: A comparative study by optical spectroscopy,” Phys. Rev. B 86, 134503 (2012). [147] Y.M. Dai, B. Xu, B. Shen, H.H. Wen, J.P. Hu, X.G. Qiu, and R.P.S.M. Lobo, “Pseudogap in underdoped Ba1−x Kx Fe2 As2 as seen via optical conductivity,” Phys. Rev. B 86, 100501(R) (2012). [148] S.J. Moon, A.A. Schafgans, M.A. Tanatar, R. Prozorov, A. Thaler, P.C. Canﬁeld, A.S. Sefat, D. Mandrus, and D.N. Basov, “Interlayer coherence and superconducting condensate in the c-axis response of optimally doped Ba(Fe1−x Cox )2 As2 highTc superconductor using infrared spectroscopy,” Phys. Rev. Lett. 110, 097003/1–4 (2013).

381

References

[149] Y.M. Dai, B. Xu, B. Shen, H.H. Wen, X.G. Qiu, and R.P.S.M. Lobo, “Optical conductivity of Ba0.6 K0.4 Fe2 As2 : The effect of in-plane and out-of-plane doping in the superconducting gap,” Europhys. Lett. 104, 47006 (2013). [150] D.A. Bonn, J.D. Garrett, and T. Timusk “Far-infrared properties of URu2 Si2 , Phys. Rev. Lett. 61, 1305–1308 (1988). [151] A. Pimenov, T. Rudolf, F. Mayr, A. Loidl, A.A. Mukhin, and A.M. Balbashov, “Coupling of phonons and electromagnons in GdMnO3 ,” Phys. Rev. B 74, 100403(R) (2006). [152] X.S. Xu, M. Angst, T.V. Brinzari, R.P. Hermann, J.L. Musfeldt, A.D. Christianson, D. Mandrus, B.C. Sales, S. McGill, J.-W. Kim, and Z. Islam, “Charge order, dynamics, and magnetostructural transition in multiferroic LuFe2 O4 ,” Phys. Rev. Lett. 101, 227602 (2008). [153] K.H. Miller, P.W. Stephens, C. Martin, E. Constable, R.A. Lewis, H. Berger, G.L. Carr, and D.B. Tanner, “Infrared phonon anomaly and magnetic excitations in singlecrystal Cu3 Bi(SeO3 )2 O2 Cl,” Phys. Rev. B 86, 174104/1–11 (2012). [154] K.H. Miller, X.S. Xu, H. Berger, V. Craciun, Xiaoxiang Xi, C. Martin, G.L. Carr, and D.B. Tanner, “Infrared phonon modes in multiferroic single-crystal FeTe2 O5 Br,” Phys. Rev. B 87, 224108/1–8 (2013). [155] A.D. LaForge, A. Frenzel, B.C. Pursley, T. Lin, X. Liu, J. Shi, and D.N. Basov, “Optical characterization of Bi2 Se3 in a magnetic ﬁeld: Infrared evidence for magnetoelectric coupling in a topological insulator material,” Phys. Rev. B 81, 125120 (2010). [156] Ana Akrap, Micha¨el Tran, Alberto Ubaldini, J´er´emie Teyssier, Enrico Giannini, Dirk van der Marel, Philippe Lerch, and Christopher C. Homes “Optical properties of Bi2 Te2 Se at ambient and high pressures,” Phys. Rev. B 86, 235207 (2012). [157] C. Martin, E.D. Mun, H. Berger, V.S. Zapf, and D.B. Tanner, “Quantum oscillations and optical conductivity in Rashba spin-splitting BiTeI,” Phys. Rev. B 87, 041104(R)/1–5 (2013). [158] D.M. Roessler, “Kramers-Kronig analysis of non-normal incidence reﬂection,” Br. J. Appl. Phys. 16, 1359 (1965). [159] R.K. Ahrenkiel, “Modiﬁed Kramers-Kronig analysis of optical spectra,” J. Opt. Soc. Am. 61, 1651–1655 (1971). [160] J.A. Bardwell and M.J. Dignam, “Extensions of the Kramers-Kronig transformation that cover a wide range of practical spectroscopic applications,” J. Chem. Phys. 83, 5468–5478 (1985). [161] V. Lucarini, J.J. Saarinen, K.-E. Peiponen, and E.M. Vartiainen Kramers-Kronig Relations in Optical Materials Research (Springer-Verlag, Berlin Heidelberg, 2005). [162] A.B. Kuzmenko, “Kramers-Kronig constrained variational analysis of optical spectra,” Rev. Sci. Instrum. 76, 083108 (2005). [163] D. Crandles, F. Eftekhari, R. Faust, G. Rao, M. Reedyk, and F. Razavi, “KramersKronig-constrained variational dielectric ﬁtting and the reﬂectance of a thin ﬁlm on a substrate,” Appl. Opt. 47, 4205–4211 (2008).

382

References

[164] J.S. Plaskett and P.N. Schatz, “On the Robinson and Price (Kramers-Kronig) method of Interpreting reﬂection data taken through a transparent window,” J. Chem.Phys. 38, 612 (1963). [165] G. Andermann, A. Caron, and David A. Dows, “Kramers-Kronig dispersion analysis of infrared reﬂectance bands.” J. Opt. Soc. Am. 55, 1210–1212 (1965). [166] D.B. Tanner, “Use of x-ray scattering functions in Kramers-Kronig analysis of reﬂectance,” Phys. Rev. B 91, 035123 (2015). [167] “X-Ray Interactions With Matter,” http://henke.lbl.gov/optical constants/. [168] P.A. Doyle and P.S. Turner, “Relativistic Hartree-Fock X-ray and electron scattering factors,” Acta Cryst. A24, 390–397 (1968). [169] D.T. Cromer and J.B. Mann, “X-ray scattering factors computed from numerical Hartree-Fock wave functions,” Acta Cryst. A24, 321–324 (1968); Los Alamos Report LA–3816 [170] J.H. Hubbell, W.J. Veigele, E.A. Briggs, R.T. Brown, D.T. Cromer, and R.J. Howerton, “Atomic form factors, incoherent scattering functions, and photon scattering cross sections,” J. Phys. Chem. Ref. Data 4, 471–538 (1975). [171] B.L. Henke, “Low energy x-ray interactions: Photoionization, scattering, specular and Bragg reﬂection,” in Low Energy X-ray Diagnostics edited by D.T. Attwood and B.L. Henke (American Institute of Physics Conf. Proc. 75, New York, 1981), pp. 146–155. [172] P. Dreier, P. Rabe, W. Malzfeldt, and W. Niemann, “Anomalous X-ray scattering factors calculated from experimental absorption spectra,” J. Phys. C: Solid State Phys. 17, 3123–3136 (1984). [173] B.L. Henke, J.C. Davis, E.M. Gullikson, and R.C.C. Perera, “A preliminary report on x-ray photoabsorption coefﬁcients and atomic scattering factors for 92 elements in the 10–10,000 eV region,” Lawrence Berkeley National Laboratory Report LBL26259 (1988). [174] R.E. Burge, “The interaction of x-rays,” in X-ray Science and Technology edited by A.G. Michette and C.J. Buckley (Institute of Physics, Bristol, 1993), Chapter 5, pp. 160–206. [175] C.T. Chantler, “Detailed Tabulation of Atomic Form Factors, Photoelectric Absorption and Scattering Cross Section, and Mass Attenuation Coefﬁcients in the Vicinity of Absorption Edges in the Soft X-Ray ?Z = 30–36, Z = 60–89, E = 0.1 keV–10 keV?, Addressing Convergence Issues of Earlier Work,” J. Phys. Chem. Ref. Data 29, 597–1048 (2000). [176] K. Kozima, W. Suetaka, and P.N. Schatz, “Optical constants of thin ﬁlms by a Kramers-Kronig method,” J. Opt. Soc. Am. 56, 181–184 (1966). [177] D.B. Romero, C.D. Porter, D.B. Tanner, L. Forro, D. Mandrus, L. Mihaly, G.L. Carr, and G.P. Williams, “Quasiparticle damping in Bi2 Sr2 CaCu2 O8 and Bi2 Sr2 CaCuO6 ,” Phys. Rev. Lett. 68, 1590–1593 (1992). [178] Z. Wu, Z. Chen, X. Du, J.M. Logan, J. Sippel, M. Nikolou, K. Kamar´as, J.R. Reynolds, D.B. Tanner, A.F. Hebard, and A.G. Rinzler, “Transparent, conductive nanotube Films,” Science 305, 1273–1276 (2004).

383

References

[179] F. Borondics, K. Kamar´as, M. Nikolou, D.B. Tanner, Z.H. Chen, and A.G. Rinzler, “Study of charge dynamics in transparent single-walled carbon nanotube ﬁlms,” Phys. Rev. B 74, 045431/1–6 (2006). [180] P.C. Martin “Sum rules, Kramers-Kronig relations, and transport coefﬁcients in charged systems,” Phys. Rev. 161, 143–155 (1967). [181] W.M. Saslow, “Two classes of Kramers-Kronig sum rules,” Phys. Lett. 33, 157–158 (1970). [182] M. Altarelli, D.L. Dexter, H.M. Nussenzveig, and D.Y. Smith, “Superconvergence and sum rules for the optical constants,” Phys. Rev. B 6, 4502–4509 (1972). [183] M. Altarelli and D.Y. Smith “Superconvergence and sum rules for the optical constants: Physical meaning, comparison with experiment, and generalization,” Phys. Rev. B 9, 1290–1298 (1974). [184] D.Y. Smith and E. Shiles, “Finite-energy f-sum rules for valence electrons,” Phys. Rev. B 17, 4689 (1978). [185] F.W. King, “Some bounds for the absorption coefﬁcient of an isotropic nonconducting medium,” Phys. Rev. B 25, 1381 (1982). [186] G. L´evque, “Augmented partial sum rules for the analysis of optical data,” Phys. Rev. B 34, 5070 (1986). [187] H.K. Onnes, “Further experiments with liquid Helium G. On the electrical resistance of pure metals, etc. VI. On the sudden change in the rate at which the resistance of mercury disappears,” Comm. Phys. Lab. Univ. Leiden 122b, 818 (1911). [188] T.G. Berlincourt and R.R. Hake, “Superconductivity at high magnetic ﬁelds,” Phys. Rev. 131, 140 (1963). [189] B.T. Matthias, T.H. Geballe, S. Geller, E. Corenzwit Phys. Rev. 95, 1435 (1954). [190] G. Bednorz and K.A. Mueller, “Possible high TC superconductivity in the Ba-LaCu-O system,” Z. Physik B. 64, 189–193 (1986). [191] J. Nagamatsu, N. Nakagawa, T. Muranaka, Y. Zenitani, and J. Akimitsu, “Superconductivity at 39 K in magnesium diboride,” Nature 410, 63 (2001). [192] D. Jerome, A. Mazaud, M. Ribault and K. Bechgaard, J. Phys. Lett. 41, L95 (1980). [193] V.V. Walatka, Jr. M. M. Labes, and J.H. Perlstein, “Polysulfur Nitride—A onedimensional chain with a metallic ground state,” Phys. Rev. Lett. 31, 1139–1142 (1973). [194] Julian Eisenstein, “Superconducting elements,” Rev. Mod. Phys. 26, 277–291 (1954). [195] B.T. Matthias, “Superconductivity in the periodic system,” Prog. Low Temp. Phys. 2, 138–150 (1957). [196] B. Matthias, T. Geballe, and V. Compton, “Superconductivity,” Rev. Mod. Phys. 35, 1–22 (1963). [197] B.W. Roberts, “Survey of superconductive materials and critical evaluation of selected properties,” J. Phys. Chem. Ref. Data 5, 581 (1976). [198] D. Jerome and H.J. Schultz, Adv. Phys. 51, 293–479 (2002). [199] John Singleton and Charles Mielke, “Quasi-two-dimensional organic superconductors: A review,” Contemp. Phys. 43, 63–96 (2002).

384

References

[200] T.H. Geballe, “The never ending search for high temperature superconductivity,” J. Supercond. Nov. Magn. 19, 261–276 (2006). [201] A.G. Lebed (Ed.), “The Physics of Organic Superconductors and Conductors,” (Springer Series in Materials Science , Vol. 110, 2008). [202] A.A. Kordyuk, “Iron-based superconductors: Magnetism, superconductivity, and electronic structure,” Low Temp. Phys., 38, 888–899 (2012). [203] K. Kitazawa, “Superconductivity: 100th anniversary of its discovery and its future,” Jap. J. Appl. Phys. 51, 010001/1–14 (2012). [204] Y. Li, J. Hao, H. Liu, Y. Li, and Y. Ma, “The metallization and superconductivity of dense hydrogen sulﬁde,” J. Chem. Phys. 140, 174712 (2014). [205] D. Duan et al., “Pressure-induced metallization of dense (H2 S)2 sb2 with high-Tc superconductivity.” Sci. Rep. 4, 6968 (2014). [206] A. Drozdov, M. Eremets, I. Troyan, V. Ksenofontov, and S. Shylin, “Conventional superconductivity at 203 Kelvin at high pressures in the sulfur hydride system,” Nature 525, 73–76 (2015). [207] F. Capitani, B. Langerome, J.-B. Brubach, P. Roy, A. Drozdov, M. I. Eremets, E. J. Nicol, J. P. Carbotte, and T. Timusk, “Spectroscopic evidence of a new energy scale for superconductivity in H3 S,” Nat. Phys. 14, 000–000 (2017). [208] W. Meissner, “Messungen mit Hilfe von ﬂiissigem Helium. V. Supraleitf¨ahigkeit von Kupfersulﬁd” (“Measurements with the aid of liquid helium. V. Superconductivity of copper sulﬁde”), Z. fur Phys., 58, 570 (1929). [209] W. Meissner and R. Ochsenfeld, “Ein neuer Effekt bei Eintritt der Supraleitf¨ahigkeit” (“A new effect at the onset of superconductivity”), Naturwissenschaften 21, 787–788 (1933). [210] J. Bardeen, L.N. Cooper, and J.R. Schrieffer, “Theory of superconductivity,” Phys. Rev. 108, 1175 (1957). [211] J. Robert Schrieffer Theory of Superconductivity (W.A. Benjamin, New York, 1964; Perseus Books, 1999). [212] L.D. Landau and V.L. Ginzburg, “On the theory of superconductivity,” Pis’ma Zh. Eksp. Teor. Fiz. 20, 1064 (1950). [213] P.G. de Gennes, Superconductivity of Metals and Alloys (W.A. Benjamin, New York. 1966; Perseus Books 1999). [214] L.P. Gorkov, “Microscopic derivation of the Ginzburg-Landau equations in the theory of superconductivity,” Sov. Phys. JETP, 9, 1364–1367 (1959). [215] Michael Tinkham Introduction to Superconductivity (McGraw-Hill, New York, 1975; Robert E. Krieger, Malabar, 1980) [216] P. Townsend and J. Sutton, “Investigation by electron tunneling of the superconducting energy gaps in Nb, Ta, Sn and Pb,” Phys. Rev. 128, 591–595 (1962). [217] R.L. Frank, C. Hainzl, R. Seiringer, and J.P. Solovej, “Microscopic derivation of Ginzburg-Landau theory,” J. Amer. Math. Soc., 25, 667 (2012). [218] F. London and H. London, “The electromagnetic equations of the supraconductor,” Proc. Roy. Soc. A149, 71–88 (1935).

385

References

[219] A.B. Pippard, “The surface energies of superconductors,” Math. Proc. Camb. Phil. Soc., 47, 617–625 (1951); A.B. Pippard, Proc. Roy. Soc. A216, 547 (1953). [220] T.A. Fulton and G.J. Dolan, “Observation of single-electron charging effects in small tunnel junctions,” Phys. Rev. Lett. 59, 109–112 (1987). [221] X.X. Xi, J. Hwang, C. Martin, D.B. Tanner, and G.L. Carr, “Far-infrared conductivity measurements of pair breaking in superconducting Nb0.5 Ti0.5 N thin-ﬁlms induced by an external magnetic ﬁeld,” Phys. Rev. Lett. 105, 257006/1–4 (2010). [222] D.C. Mattis and J. Bardeen, “Theory of the anomalous skin effect in normal and superconducting metals,” Phys. Rev. 111, 412–417 (1958). [223] S.B. Nam, “Theory of electromagnetic properties of superconducting and normal systems. I,” Phys. Rev. 156, 470–486 (1967). [224] S.B. Nam, “Theory of electromagnetic properties of strong-coupling and impure superconductors. II,” Phys. Rev. 156, 487–93 (1967). [225] P.B. Miller, “Surface impedance of superconductors,” Phys. Rev. 118, 928–934 (1960). [226] S. Skalski, O. Betbeder-Matibet, and P.R. Weiss, “Properties of superconducting alloys containing paramagnetic impurities,” Phys. Rev. 136, A1500–A1518 (1964). [227] W. Zimmermann, E.H. Brandt, M. Bauec, E. Seider, and L. Genzel, “Optical conductivity of BCS superconductors with arbitrary purity,” Phys. C: Supercond. 183, 99–104 (1991). [228] D.R. Tilley and J. Tilley, Superﬂuidity and Superconductivity (Adam Hilger Ltd, Bristol, 1990). [229] X.X. Xi, Conventional and Time-Resolved Spectroscopy of Magnetic Properties of Superconducting Thin Films (Thesis, University of Florida, 2011). [230] D.J. Scalapino, “A common thread: The pairing interaction for unconventional superconductors,” Rev. Mod. Phys. 84, 1383–1417 (2012). [231] M.R. Norman, “The challenge of unconventional superconductivity,” Science 332, 196–200 (2011). [232] G.R. Stewart, “Unconventional superconductivity,” Adv. Phys. 66, 75–196 (2017). [233] M.K Wu, J.R. Ashburn, C.J. Torng, P.H. Hor, R.L. Meng, L. Gao, Z.J. Huang, Y.Q. Wang, and C.W. Chu, “Superconductivity at 93 K in a new mixed-phase Y-Ba-Cu-O compound system at ambient pressure,” Phys. Rev. Lett. 58, 908 (1987). [234] T. Timusk and D.B. Tanner, “Infrared properties of high-Tc superconductors,” in Physical Properties of High Temperature Superconductors I, edited by D.M. Ginsberg (World Scientiﬁc, Singapore, 1989) p. 339. [235] D.B. Tanner and T. Timusk, “Optical properties of high-temperature superconductors,” in Physical Properties of High Temperature Superconductors III, edited by D.M. Ginsberg (World Scientiﬁc, Singapore, 1992) p. 363. [236] T. Timusk, “Infrared properties of exotic superconductors,” Physica C 317–318, 18–29, 1999. [237] D.N. Basov and T. Timusk, “Electrodynamics of high-Tc superconductors,” Rev. Mod. Phys. 77, 721 (2005).

386

References

[238] D.B. Tanner, “Optical properties of one-dimensional systems,” in Extended Linear Chain Compounds, Vol. 2, edited by Joel S. Miller (Plenum Press, New York, 1982) pp. 205–258. [239] L. Degiorgi, “The electrodynamic response of heavy-electron compounds,” Rev. Mod. Phys. 71: 687–734, 1999 [240] T. Ishiguro, K. Yamaji, and G. Saito. Organic Superconductors (Springer-Verlag, Heidelberg, 2002). [241] M. Dressel and N. Drichko, “Optical properties of two-dimensional organic conductors: Signatures of charge ordering and correlation effects,” Chem. Rev. 104, 5689–5716 (2004). [242] D.C. Johnston, “The puzzle of high temperature superconductivity in layered iron pnictides and chalcogenides,” Adv. Phys. 59, 803–1061 (2010). [243] P.J. Hirschfeld, M.M. Korshunov, and I.I. Mazin, “Gap symmetry and structure of Fe-based superconductors,” Rep. Progress Phys. 74, 124508 (2011). [244] M. Reedyk, D.A. Bonn, J.D. Garrett, J.E. Greedan, C.V. Stager, T. Timusk, K. Kamar´as, and D.B. Tanner, “Far-infrared optical properties of Bi2 Sr2 CaCu2 O8 ,” Phys. Rev. B, 38, 11,981 (1988). [245] A. Puchkov, P. Fournier, D.N. Basov, T. Timusk, A. Kapitulnik, amd N.N. Kolesnikov, “Evolution of the pseudogap state of high-Tc superconductors with doping,” Phys. Rev. Lett. 77, 3212 (1996). [246] A.V. Puchkov, D.N. Basov, and T. Timusk, “The pseudogap state in high-Tc superconductors: An infrared study,” J. Phys.: Condens. Matter 8, 10049 (1996). [247] J. Hwang, J.P. Carbotte, and T. Timusk, “Evidence for a pseudogap in underdoped Bi2 Sr2 CaCu2 O8+δ and YBa2 Cu3 O6.50 from in-plane optical conductivity measurements,” Phys. Rev. Lett. 100, 177005 (2008). [248] P.B. Allen, W.E. Pickett, and H. Krakauer, “Band-theory analysis of anisotropic transport in La2 CuO4 -based superconductors,” Phys. Rev. B 36, 3926 (1987). [249] A. Umezawa, G.W. Crabtree, J.Z. Liu, T.J. Moran, S.K. Malik, L.H. Nunez, W.L. Kwok, and C.H. Sowers, “Anisotropy of the lower critical ﬁeld, magnetic penetration depth, and equilibrium shielding current in single-crystal YBa2 Cu3 O7−δ ,” Phys. Rev. B 38, 2843 (1988). [250] K. Kamar´as, S.L. Herr, C.D. Porter, N. Tache, D.B. Tanner, S. Etemad, T. Venkatesan, E. Chase, A. Inam, X.D. Wu, M.S. Hegde, and B. Dutta, “In a clean high-Tc superconductor you do not see the gap,” Phys. Rev. Lett. 64, 84–87 (1990). [251] J.I. Pankove, Optical Processes in Semiconductors (Dover, New York, 1971). [252] P.Y. Yu and M. Cardona, Fundamentals of Semiconductors: Physics and Materials Properties (Springer, New York, 1996). [253] R.E. Peierls, Quantum Theory of Solids (Clarendon Press, Oxford, England, 1955). [254] M. Grundmann The Physics of Semiconductors, An Introduction including Nanophysics and Applications (Springer, Heidelberg, 2016). [255] Wikipedia, the free encyclopedia, “List of semiconductor materials,” http://en.wikipedia.org/wiki/List of semiconductor materials.

387

References

[256] M. Ohring, Reliability and Failure of Electronic Materials and Devices (Academic Press, San Diego, 1998), p. 310. [257] Y. Tao, J.M. Boss, B.A. Moores, and C.L. Degen, “Single-crystal diamond nanomechanical resonators with quality factors exceeding one million,” Nat. Comm. 5, 3638 (2014). [258] A.K. Abass and N.H. Ahmad, “Indirect band gap investigation of orthorhombic single crystals of sulfur,”J. Phys. Chem. Solids 47, 143 (1986). [259] D.A. Evans, A.G. McGlynn, B.M. Towlson, M. Gunn, D. Jones, T.E. Jenkins, R. Winter, N.R.J. Poolton, “Determination of the optical band-gap energy of cubic and hexagonal boron nitride using luminescence excitation spectroscopy,” J. Phys.: Cond. Matt. 20, 75233 (2008). [260] C.F. Klingshirn Semiconductor Optics (Springer, Heidelberg, 1997), p. 127. [261] S. Banerjee et al. “Physics and chemistry of photocatalytic titanium dioxide: Visualization of bactericidal activity using atomic force microscopy,” Curr. Sci. 90, 1378 (2006). [262] O. Madelung, U. R¨ossler, M. Schulz (ed.), “Cuprous oxide (Cu2 O) band structure, band energies.” in Group III Condensed Matter. Numerical Data and Functional Relationships in Science and Technology. 41C: Non-Tetrahedrally Bonded Elements and Binary Compounds I. doi:10.1007/10681727 62. [263] B.G. Yacobi, Semiconductor Materials: An Introduction to Basic Principles (Springer, 2003) ISBN 0-306-47361-5; C. Hodes; Ebooks Corporation, Chemical Solution Deposition of Semiconductor Films (CRC Press, 2002), p. 319. [264] Y.N. Rajakarunanayake, Optical Properties of Si-Ge Superlattices and Wide Band Gap II-VI Superlattices, Dissertation (Ph.D.), California Institute of Technology, 1991 [265] H. Ehrenreich, “Band structure and electron transport of GaAs,” Phys. Rev. 120, 1951–1963 (1960). [266] M. Rohlﬁng, P. Kr¨uger, and J. Pollmann, “Quasiparticle band-structure calculations for C, Si, Ge, GaAs, and SiC using Gaussian-orbital basis sets,” Phys. Rev. B 48, 17791–17805 (1993). [267] S. Richard, F. Aniel, and G. Fishman, “Energy-band structure of Ge, Si, and GaAs: A thirty-band k · p method,” Phys. Rev. B 70, 235204 (2004). [268] W.G. Spitzer and J.M. Whelan, “Infrared absorption and electron effective mass in n-type gallium arsenide,” p. 114, 59–63 (1959). [269] M.D. Sturge, “Optical absorption of gallium arsenide between 0.6 and 2.75 eV,” Phys. Rev. 127, 768–773 (1962). [270] H.C. Casey, D.D. Sell, and K.W. Wecht, “Concentration dependence of the absorption coefﬁcient for n- and p- type GaAs between 1.3 and 1.6 eV,” J. Appl. Phys. 46, 250 (1975). [271] D.E. Aspnes, S.M. Kelso, R.A. Logan, and R. Bhat, “Optical properties of Alx Ga1−x As,” J. Appl. Phys. 60, 754–767 (1986). [272] D. Brust, J. C. Phillips, and F. Bassani, “Critical points and ultraviolet reﬂectivity of semiconductors,” Phys. Rev. Lett. 9, 94–97 (1962).

388

References

[273] E.O. Kane, “Energy band structure in p-type germanium and silicon,” J. Phys. Chem. Solids 1, 82–99 (1956). [274] M. Cardona and F.H. Pollak, “Energy-band structure of germanium and silicon: The k · p method”, Phys. Rev. 142, 530–543 (1966). [275] E.O. Kane, “Band structure of silicon from an adjusted Heine-Abarenkov calculation,” Phys. Rev. 146, 558–567 (1966). [276] W. Saslow, T.K. Bergstresser, and Marvin L. Cohen, “Band structure and optical properties of diamond,” Phys. Rev. Lett. 16, 354–357 (1966). [277] B.P. Zakharchenya and R.P. Selsyan “Diamagnetic excitons in semiconductors,” Sov. Phys. Uspekhi 12, 70 (1969). [278] R.P. Seisyan, “Spectroscopy of Diamagnetic Excitons,” Science, Moscow (1984). [279] P.W. Baumeister, “Optical absorption of cuprous oxide,” Phys. Rev. 121, 359 (1961). [280] R.A. Faulkner, “Higher donor excited states for prolate-spheroid conduction bands: A reevaluation of silicon and germanium,” Phys. Rev. 184, 713 (1969). [281] A. Baldereschi and N.O. Lipari, “Spherical model of shallow acceptor states in semiconductors,” Phys. Rev. B 8, 2697 (1973). [282] A. Baldereschi and N.O. Lipari “Cubic contributions to the spherical model of shallow acceptor states,” Phys. Rev. B 9, 1525 (1974). [283] J.W. Allen and J.C. Mikkelsen, “Optical properties of CrSb, MnSb, NiSb, and NiAs,” Phys. Rev. B 15, 2952 (1977). [284] W. G¨otze and P. W¨olﬂe, “Homogeneous dynamical conductivity of simple metals,” Phys. Rev. B 6, 1226 (1972). [285] P.B. Littlewood and C.M. Varma, “Phenomenology of the normal and superconducting states of a marginal Fermi liquid,” J. Appl. Phys. 69, 4979 (1991). [286] J.P. Carbotte, E. Schachinger, and J. Hwang, “Boson structures in the relation between optical conductivity and quasiparticle dynamics,” Phys. Rev. B 71, 054506 (2005). [287] J. Hwang, T. Timusk, and G.D. Gu, “Doping dependent optical properties of Bi2 Sr2 CaCu2 O8+δ ,” J. Phys.: Cond. Matt. 19, 125208 (2007). [288] P.B. Allen, “Electron self-energy and generalized Drude formula for infrared conductivity of metals,” Phys. Rev. B 92, 054305 (2015). [289] R.N. Gurzhi, “Mutual electron correlations in metal optics,” Sov. Phys. JETP 8, 673–675 (1959). [290] R.N. Gurzhi, “Hydrodynamic effects in solids at low temperature,” Sov. Phys. Uspekhi 11, 255–270 (1968). [291] J.B. Smith and H. Ehrenreich, “Frequency dependence of the optical relaxation time in metals,” Phys. Rev. B 25, 923–930 (1982). [292] A. Rosch, “Optical conductivity of clean metals,” Ann. Phys. 15, 526–534 (2006). [293] D.L. Maslov and A.V. Chubukov, “First-Matsubara-frequency rule in a Fermi liquid. II. Optical conductivity and comparison to experiment,” Phys. Rev. B 86, 155137 (2012).

389

References

[294] C. Berthod, J. Mravlje, X. Deng, D. van der Marel, and A. Georges, “Non-Drude universal scaling laws for the optical response of local Fermi liquids,” Phys. Rev. B 87, 115109 (2013). [295] D.L. Maslov and A.V. Chubukov, “Optical response of correlated electron systems,” Rep. Prog. Phys. 80, 026503 (2016). [296] C.M. Varma, P.B. Littlewood, S. Schmitt-Rink, E. Abrahams, and A.E. Ruckenstein, “Phenomenology of the normal state of Cu-O high-temperature superconductors,” Phys. Rev. Lett. 63, 1996 (1989). [297] F. Slakey, S.L. Cooper, M.V. Klein, J.P. Rice, E.D. Bukowski, and D.M. Ginsberg, “Gap anisotropy and phonon self-energy effects in single-crystal YBa2 Cu3 O7−δ ,” Phys. Rev. B 38, 11,934 1989. [298] C.G. Olson, R. Liu, D.W. Lynch, R.S. List, A.J. Arko, B.W. Veal, Y.C. Chang, P.Z. Jiang and A.P. Paulikas, “High-resolution angle-resolved photoemission study of the Fermi surface and the normal-state electronic structure of Bi2 Sr2 CaCu2 O8 ,” Phys. Rev. B 42, 381 (1990). [299] Y. Hwu, L. Lozzi, M. Marsi, S. La Rosa, M. Winokur, P. Davis, M. Onellion, H. Berger, F. Gozzo, F. L´evy, and G. Margaritondo, “Electronic spectrum of the hightemperature superconducting state,” Phys. Rev. Lett. 67, 2573 (1991). [300] M. Gurvitch and A.T. Fiory, “Resistivity of La1.825 Sr0.175 CuO4 and YBa2 Cu3 O7 to 1100 K: Absence of saturation and its implications,” Phys. Rev. Lett. 59, 1337–1340 (1987). [301] S. Martin, A.T. Fiory, R.M. Fleming, L.F. Schneemeyer, and J.V. Waszczak, “Temperature dependence of the resistivity tensor in superconducting Bi2 Sr2.2 Ca0.8 Cu2 O8 crystals,” Phys. Rev. B 41, 846 (1990). [302] J. Hubbard, “Electron correlation in narrow energy bands,” Proc. Roy. Soc. (London) A276, 238–257 (1963). [303] N.F. Mott, “Metal-insulator transition,” Rev. Mod. Phys. 40, 677–683 (1968). [304] E.H. Lieb and F.Y.Wu, “Absence of Mott transition in an exact solution of the shortrange one-band model in one dimension,” Phys. Rev. Lett. 20, 1445–1448 (1968). [305] J. Hubbard, “Generalized Wigner lattices in one dimension and some applications to tetracyanoquinodimethane (TCNQ) salts,” Phys. Rev. B 17, 494 (1978). [306] D.B. Tanner, C.S. Jacobsen, A.A. Bright, and A.J. Heeger, “Infrared studies of the energy gap and electron-phonon interaction in potassium-tetracyanoquinodimethane (K-TCNQ),” Phys. Rev. B 16, 3283–3290 (1977). [307] M.J. Rice. “Towards the experimental determination of the fundamental microscopic parameters of organic ion-radical compounds,” Solid State Commun. 31, 93–98 (1979). [308] A. Brooks Harris and Robert V. Lange. “Single-particle excitations in narrow energy bands,” Phys. Rev. 157, 295–314 (1967). [309] A. Painelli and A. Girlando, “Electron-molecular vibration (e-mv) coupling in charge-transfer compounds and its consequences on the optical spectra: A theoretical framework,” J. Chem. Phys. 84, 5655–5671 (1986).

390

References

[310] J.J. Hopﬁeld, “Infrared properties of transition metals (Electron phonon coupling and IR optical constants relationship to superconductivity in transition metals),” in Superconductivity in d- and f- band metals, edited by H. Suhl and M.B. Maple (Plenum, New York, 1972). [311] J.J. Hopﬁeld, “Infrared properties of transition metals,” AIP Conference Proceedings 4, 358–366 (1972). [312] P.B. Allen, “Electron-phonon effects in the infrared properties of metals,” Phys. Rev. B 3, 305–320 (1971). [313] R.R. Joyce and P.L. Richards, “Phonon contribution to the far-infrared absorptivity of superconducting and normal lead,” Phys. Rev. Lett. 24, 1007–1011 (1970). [314] G. Br¨andli and A.J. Sievers, “Absolute measurement of the far-infrared surface resistance of Pb,” Phys. Rev. B 5, 3550 (1972). [315] B. Farnworth and T. Timusk, “Far-infrared measurements of the phonon density of states of superconducting lead,” Phys. Rev. B 10, 2799–2802 (1974). [316] B. Farnworth and T. Timusk, “Phonon density of states of superconducting lead,” Phys. Rev. B 14, 5119 (1976). [317] W. Shaw and J.C. Swihart, “Theory of phonon contribution to infrared absorptivity of superconducting and normal metals,” Bull. Am. Phys. Soc. 16, 352 (1971). [318] H. Scher, “Far-infrared absorptivity of normal lead,” Phys. Rev. Lett. 25, 759–762 (1970). [319] M.J. Rice, “Organic linear conductors as systems for the study of electron-phonon interactions in the organic solid state,” Phys. Rev. Lett. 37, 36–39 (1976). [320] M.J. Rice, L. Pietronero, and P. Br¨uesch, “Phase phonons and intramolecular electron-phonon coupling in the organic linear chain semiconductor TEA(TCNQ)2 ,” Solid State Commun. 21, 757–760 (1977). [321] M.J. Rice, N.O. Lipari, and S. Str¨assler, “Dimerized organic linear-chain conductors and the unambiguous experimental determination of electron-molecular-vibration coupling constants,” Phys. Rev. Lett. 39, 1359–1362 (1977). [322] M.J. Rice, V.M. Yartsev, and C.S. Jacobsen, “Investigation of the nature of the unpaired electron states in the organic semiconductor N-methyl-Nethylmorpholinium-tetracyanoquinodimethane,” Phys. Rev. B 21, 3437–3446 (1980). [323] A. Brau, P. Br¨uesch, J.P. Farges, W. Hinz, and D. Kuse, “Polarized optical reﬂection spectra of the highly anisotropic organic semiconductor TEA(TCNQ)2 ,” Phys. Stat. Sol. (b) 62, 615–623 (1974). [324] D.B. Tanner, J.E. Deis, A.J. Epstein, and J.S. Miller, “Optical properties of the semiconducting ‘metal-like’ complex (NMe3 H)(I)(TCNQ),” Solid State Commun. 31, 671–675 (1979). [325] R.P. McCall, D.B. Tanner, J.S. Miller, and A.J. Epstein, “Optical properties of the 1:2 compound of dimethylferrocenium with tetracyanoquinodimethanide: [(Me2 Fc)(TCNQ)2 ],” Phys. Rev. B 35, 9209–9217 (1987).

391

References

[326] J.L. Musfeldt, C.C. Homes, M. Almeida, and D.B. Tanner, “Temperature dependence of the infrared and optical properties of N -dimethyl thiomorpholinium(tetracyanoquinodimethane)2 ,” Phys. Rev. B 46, 8777–8789 (1992). [327] Eugene J. Mele and Michael J. Rice. “Vibrational excitations of charged solitons in polyacetylene,” Phys. Rev. Lett. 45, 926–929 (1980). [328] S. Etemad, A. Pron, A. J. Heeger, A. G. MacDiarmid, E. J. Mele, and M. J. Rice, “Infrared-active vibrational modes of charged solitons in (CH)x and (CD)x ,” Phys. Rev. B 23, 5137–5141 (1981). [329] E. Ehrenfreund, Z. Vardeny, O. Brafman, and B. Horovitz, “Amplitude and phase modes in trans-polyacetylene: Resonant Raman scattering and induced infrared activity,” Phys. Rev. B 36, 1535–1553 (1987). [330] Y.H. Kim, and A.J. Heeger, “Infrared-active vibrational modes of heavily doped ‘metallic’ polyacetylene,” Phys. Rev. B 40, 8393–8398 (1989). [331] Ke-Jian Fu, William L. Karney, Orville L. Chapman, Shiou-Mei Huang, Richard B. Kaner, Franc¸ois Diederich, K´aroly Holczer, and Robert L. Whetten “Giant vibrational resonances in A6 C60 compounds,” Phys. Rev. B 46, 1937 (1992). [332] H.-Y. Choi and M.J. Rice, “Infrared absorption by charged phonons in doped C60,” in Electronic Properties of High-Tc Superconductors (Springer, Berlin Heidelberg, 1993) pp. 501–506. [333] T. Timusk and D.B. Tanner, “Evidence for strong bound-electron phonon interaction at 52 meV in YBa2 Cu3 O7 ,” Physica C 169, 425–428 (1990). [334] T. Timusk, C.D. Porter, and D.B. Tanner, “Strong electron-phonon interaction in the high-Tc superconductors: Evidence from the infrared,” Phys. Rev. Lett. 66, 663–666 (1991). [335] M.J. Rice, V.M. Yartsev and C.S. Jacobsen, “Investigation of the nature of the unpaired electron states in the organic semiconductor N-methyl-Nethylmorpholinium-tetracyanoquinodimethane,” Phys. Rev. B 21, 3437 (1980). [336] Y. Iida, “Electronic spectra and charge-transfer absorption of solid anion radical salts of 2,3-dicyano-p-benzoquinone and 2,3-dichloro-5,6-dicyano-p-benzoquinone,” Bull. Chem. Soc. Jap. 51, 631–632 (1978). [337] J. Tanaka, M. Tanaka, T. Kawai, T. Takabe and O. Maki, “Electronic spectra and electronic structure of TCNQ complexes,” Bull. Chem. Soc. Jap. 49, 2358 (1976). [338] A.B. Pippard, “The surface impedance of superconductors and normal metals at high frequencies. II. The anomalous skin effect in normal metals,” Proc. R. Soc. Lond. A 191, 385–399 (1947). [339] R.G. Chambers, “Anomalous skin effect in metals,” Nature 165, 239–240 (1950). [340] H.B.G. Casimir and J. Ubbink, “The skin effect: II. The skin effect at high frequencies,” Philips Tech. Rev. 28, 300–315 (1967). [341] E.H. Land, “Some aspects on the development of sheet polarizers,” J. Opt. Soc. Am. 41, 957–963 (1951). [342] B.P. Abbott et al. (LIGO Scientiﬁc Collaboration), “LIGO: The Laser Interferometer Gravitational-wave Observatory,” Rep. Prog. Phys. 72, 076901/1–25 (2009).

392

References

[343] W.S. Bickel and W.M. Bailey, “Stokes vectors, Mueller matrices, and polarized scattered light,” Am. J. Phys. 53, 468 (1985). [344] S.N. Savenkov, “Jones and Mueller matrices: Structure, symmetry relations and information content,” Light Scatter. Rev. 4, 71 (2009). [345] “The Physics Hypertextbook, ‘Refraction,’ ” http://physics.info/refraction/. [346] J.L. Duarte, J.A. Sanjurjo, and R.S. Katiyar, “Off-normal infrared reﬂectivity in uniaxial crystals: α-LiIO3 and α-quartz,” Phys. Rev. B 36, 3368–3372 (1987). [347] L. Landau, “Diamagnetismus der Metalle” (“Diamagnetism of metals”), Z. Phys. 64, 629 (1930). [348] Colin M. Hurd, The Hall Effect in Metals and Alloys (Plenum Press, New York, 1972). [349] E.H. Hall, “On a new action of the magnet on electric currents,” American Journal of Mathematics 2, 287–292 (1879). [350] D. Schoenberg, Magnetic Oscillations in Metals (Cambridge University Press, London, 1984). [351] B.W. Maxﬁeld, “Helicon waves in solids,” Am. J. Phys. 37, 241 (1969). [352] J.M. Goodman, “Helicon waves, surface-mode loss, and the accurate determination of the hall coefﬁcients of aluminum, indium, sodium, and potassium,” Phys. Rev. 171, 641 (1968). [353] R. Blewitt and A.J. Sievers, “Harmonic series of cyclotronlike resonances in Bismuth,” Phys. Rev. Lett. 30, 1041 (1973). [354] G. Dresselhaus, A.F. Kip and C. Kittel, “Cyclotron resonance of electrons and holes in silicon and germanium crystals,” Phys. Rev. 98, 368 (1955). [355] J. Kono, “Cyclotron resonance,” in Methods in Materials Research, edited by E.N. Kaufmann et al. (Wiley, 1999). [356] T.F. Rosenbaum, K. Andres, G.A. Thomas, and R.N. Bhatt, “Sharp metal-insulator transition in a random solid,” Phys. Rev. Lett. 45, 1723 (1980). [357] W.N. Shafarman, D.W. Koon, and T.G. Castner, “DC conductivity of arsenic-doped silicon near the metal-insulator transition,” Phys. Rev. B 40, 1216 (1989). [358] N. Mott, “On metal-insulator transitions,” J. Solid State Chem. 88 5–7 (1990). [359] I.I. Rabi, J.R. Zacharias, S. Millman, and P. Kusch, “A new method of measuring nuclear magnetic moment,” Phys. Rev., 53, 318 (1938). [360] G. Feher and A.F. Kip, “Electron spin resonance absorption in metals. I. Experimental,” Phys. Rev., 98, 337 (1955). [361] F.J. Dyson “Electron spin resonance absorption in metals. II. Theory of electron diffusion and the skin effect,” Phys. Rev. 98, 349 (1955). [362] J.H.E. Grifﬁths, “Anomalous high-frequency resistance of ferromagnetic metals,” Nature 158, 670 (1946). [363] C. Kittel, “On the theory of ferromagnetic resonance absorption,” Phys. Rev. 73, 155 (1948). [364] C. Kittel, “Theory of antiferromagnetic resonance,” Phys. Rev. 82, 565 (1951); F. Keffer and C. Kittel “Theory of antiferromagnetic resonance,” Phys. Rev. 85, 329 (1952).

393

References

[365] A. Pimenov, A. A. Mukhin, V. Yu. Ivanov, V. D. Travkin, A.M. Balbashov, and A. Loidl, “Possible evidence for electromagnons in multiferroic manganites,” Nature Physics 2, 97–100 (2006). [366] T. Yildirim, L.I. Vergara, Jorge ´I˜niguez, J.L. Musfeldt, A.B. Harris, N. Rogado, R.J. Cava, F. Yen, R.P. Chaudhury, and B. Lorenz, “Phonons and magnetoelectric interactions in Ni3 V2 O8 ,” J. Phys.: Cond. Mat. 20, 434214 (2008). [367] A. Shuvaev, V. Dziom, Anna Pimenov, M. Schiebl, A. A. Mukhin, A. C. Komarek, T. Finger, M. Braden, and A. Pimenov, “Electric ﬁeld control of terahertz polarization in a multiferroic manganite with electromagnons,” Phys. Rev. Lett. 111, 227201 (2013). [368] J.C.M. Garnett, “Colours in metal glasses and in metallic ﬁlms,” Phil. Trans. Roy. Soc. A203, 385 (1904). [369] J.C.M. Garnett, “Colours in metal glasses, in metallic ﬁlms, and in metallic solutions–II,” Phil. Trans. Roy. Soc. A205, 237 (1906). [370] D.A.G. Bruggeman, “Berechnung verschiedener physikalischer Konstanten von heterogenen Substanzen. I. Dielektrizit¨atskonstanten und Leitf¨ahigkeiten der Mischk¨orper aus isotropen Substanzen” (“Calculation of different physical constants of heterogeneous substances. I. Dielectric constants and conductivities of the mixed bodies of isotropic substances”), Ann. Physik (Leipz.) 24, 636 (1935). [371] R. Landauer, “The electrical resistance of binary metallic mixtures,” J. Appl. Phys. 23, 779 (1952). [372] B.E. Springett, “Effective-medium theory for the AC behavior of a random system,” Phys. Rev. Lett. 31, 1463 (1973). [373] D. Stroud, “Generalized effective-medium approach to the conductivity of an inhomogeneous material,” Phys. Rev. B 12, 3368 (1975). [374] G. Mie, “Beitr¨age zur Optik tr¨uber Medien, speziell kolloidaler Metall¨osungen (Contributions to optics via media, especially colloidal metal compounds),” Ann. Physik 25, 377 (1908). [375] P. Debye, “Der Lichtdruck auf Kugeln von beliebigem Material” (“The light pressure on spheres of any material”), Ann. Physik 30, 57 (1909). [376] H.C. Van de Hulst, Light Scattering by Small Particles (Dover, New York, 1981). [377] Z. Hashin and S. Shtrikman, J. Appl. Phys. 33, 3125 (1962). [378] W.T. Doyle, “Optical absorption by F centers in alkali halides,” Phys. Rev. 111, 1072 (1958). [379] F.L. Galeener, “Submicroscopic-void resonance: The effect of internal roughness on optical absorption,” Phys. Rev. Lett. 27, 421 (1971). [380] F.L. Galeener, “Optical evidence for a network of cracklike voids in amorphous germanium,” Phys. Rev. Lett. 27, 1716 (1971). [381] L. Genzel and T.P. Martin, “Infrared absorption by surface phonons and surface plasmons in small crystals,” Surf. Sci. 34, 33 (1973). [382] A.S. Barker, Jr. “Infrared absorption of localized longitudinal-optical phonons,” Phys. Rev. B 7, 2507 (1973).

394

References

[383] J.H. Weaver, R.W. Alexander, L. Teng, R.A. Mann, and R.J. Bell, “Infrared absorption of small silicon particles with oxide overlayers,” Phys. Stat. Sol. (a) 20, 321 (1973). [384] R.W. Cohen, G.D. Cody, M.D. Coutts, and B. Abeles, “Optical properties of granular silver and gold ﬁlms,” Phys. Rev. B 8, 3689 (1973). [385] B. Abeles, H.L. Pinch, and J.I. Gittleman, “Percolation conductivity in W-Al2 O3 granular metal ﬁlms,” Phys. Rev. Lett. 35, 247 (1975). [386] C.G. Granqvist and O. Hunderi, “Retardation effects on the optical properties of ultraﬁne particles,” Phys. Rev. B 16, 1353 (1977). [387] C.G. Granqvist and O. Hunderi, “Optical properties of ultraﬁne gold particles,” Phys. Rev. B 16, 3513 (1977). [388] I. Webman, J. Jortner and M.H. Cohen, “Theory of optical and microwave properties of microscopically inhomogeneous materials,” Phys. Rev. B 15, 5712 (1977). [389] W. Lamb, D.M. Wood, and N.W. Ashcroft, “Long-wavelength electromagnetic propagation in heterogeneous media,” Phys. Rev. B 21, 2248 (1980). [390] D. Stroud, “Percolation effects and sum rules in the optical properties of composities,” Phys. Rev. B 19, 1783 (1979). [391] H. Scher and R. Zallen, “Critical density in percolation processes,” J. Chem. Phys. 53, 3759 (1970). [392] Richard Zallen, “The percolation model,” in The Physics of Amorphous Solids (Wiley, 1983), pp. 135–204. [393] M.J. Powell, “Site percolation in randomly packed spheres,” Phys. Rev. B 20, 4194 (1979). [394] D.M. Grannan, J.C. Garland, and D.B. Tanner, “Critical behavior of the dielectric constant of a random composite near the percolation threshold,” Phys. Rev. Lett. 46, 375 (1981). [395] S. Kirkpatrick, “Classical transport in disordered media: Scaling and effectivemedium theories,” Phys. Rev. Lett. 27, 1722 (1971). [396] S. Kirkpatrick, “Percolation and conduction,” Rev. Mod. Phys. 45, 574–588 (1973). [397] S. Kirkpatrick, “Percolation phenomena in higher dimensions: Approach to the mean-ﬁeld limit,” Phys. Rev. Lett. 36, 69 (1976). [398] S. Kirkpatrick, “Percolation thresholds in Ising magnets and conducting mixtures,” Phys. Rev. B 15, 1533 (1977). [399] B.J. Last and D.J. Thouless, “Percolation theory and electrical conductivity,” Phys. Rev. Lett. 27, 1719 (1971). [400] V. Ambegaokar, S. Cochran, and J. Kurkijarvi, “Conduction in random systems,” Phys. Rev. B 8, 3682 (1973). [401] B.P. Watson, and P.L. Leath, “Conductivity in the two-dimensional-site percolation problem,” Phys. Rev. B 9, 4893 (1974). [402] I. Webman, and J. Jortner, “Numerical simulation of electrical conductivity in microscopically inhomogeneous materials,” Phys. Rev. B 15, 2885 (1975). [403] M.E. Levinshtein, B.I. Shklovskii, M.S. Shur, and A.L. Efros, “The relation between the critical exponents of percolation theory,” Sov. Phys JETP, 42, 197 (1975).

395

References

[404] G. Deutscher, R. Zallen, and J. Adler eds., Percolation Structures and Processes (Adam Hilger, Bristol, 1983). [405] D.S. Stauffer and A. Ahorony, Introduction to Percolation Theory (Taylor and Francis, 1994). [406] J.P. Straley, “Critical phenomena in resistor networks,” J. Phys. C: Solid State Phys. 9, 783 (1976). [407] J.P. Straley, “Critical exponents for the conductivity of random resistor lattices,” Phys. Rev. B 15, 5733 (1977). [408] J.P. Straley, “Random resistor tree in an applied ﬁeld,” J. Phys. C: Solid State Phys. 10, 3009 (1977). [409] R.B. Stinchcombe and B.P. Watson, “Renormalization group approach for percolation conductivity,” J. Phys. C: Solid State Phys. 9, 3221 (1976). [410] A.L. Efros, and B.I. Shklovskii, “Critical behaviour of conductivity and dielectric constant near the metal-non-metal transition threshold,” Phys. Stat. Sol. (B) 76, 475 (1976). [411] A.B. Harris and R. Fisch, “Critical behavior of random resistor networks,” Phys. Rev. Lett. 38, 796 (1977). [412] D.J. Bergman and Y. Imry, “Critical behavior of the complex dielectric constant near the percolation threshold of a heterogeneous material,” Phys. Rev. Lett. 39, 1222 (1977). [413] J.P. Straley, in Electrical Transport and Optical Properties of Inhomogeneous Media, edited by J.C. Garland and D.B. Tanner (The American Institute of Physics, New York, 1978), p. 118. [414] J. Wu and D.S. McLachlan, “Percolation exponents and thresholds obtained from the nearly ideal continuum percolation system graphite-boron nitride,” Phys. Rev. B 56, 1236 (1997). [415] D. Stroud and D.J. Bergman, “Frequency dependence of the polarization catastrophe at a metal-insulator transition and related problems,” Phys. Rev. B 25, 2061 (1982). [416] D.B. Tanner, A.J. Sievers, and R.A. Buhrman, “Far-infrared absorption in small metallic particles,” Phys. Rev. B 11, 1330–1341 (1975). [417] N.E. Russell, J.C. Garland, and D.B. Tanner, “Absorption of far-infrared radiation by random metal particle composites,” Phys. Rev. B 23, 632 (1981). [418] G.L. Carr, R.L. Henry, N.E. Russell, J.C. Garland, and D.B. Tanner, “Anomalous far-infrared absorption in random small-particle composites,” Phys. Rev. B., 24, 777 (1981). [419] S.-I. Lee, T.W. Noh, J.R. Gaines, Y.-H. Ko, and E.R. Kreidler, “Optical studies of porous glass media containing silver particles,” Phys. Rev. B 37, 2918 (1988). [420] G.L. Carr, S. Perkowitz, and D.B. Tanner, “Far-infrared properties of inhomogeneous materials,” in Infrared and Millimeter Waves, Vol. 13, edited by Kenneth J. Button (Academic Press, Orlando, 1985), pp. 171–263. [421] D. Stroud and F.P. Pan, “Self-consistent approach to electromagnetic wave propagation in composite media: Application to model granular metals,” Phys. Rev. B 17, 1602 (1978).

396

References

[422] H.B.G. Casimir, “On electromagnetic units,” Helvetica Phys. Acta, 41, 741–742 (1968) This article is reprinted in Robert L. Weber and Eric Mendoza, A Random Walk in Science (Institute of Physics Publishing, Bristol, 1973). [423] R. Nityananda and J. Samuel,“Fermat’s principle in general relativity,” Phys. Rev. D 45, 3862 (1992). [424] M.A. Dupertuis, M. Proctor, and B. Acklin, “Generalization of complex SnellDescartes and Fresnel laws,” J. Opt. Soc. Am. A 11, 1159–1166 (1994). [425] P.C.Y. Chang, J.G. Walker, and K.I. Hopcraft “Ray tracing in absorbing media,” J. Quant. Spect. Rad. Trans. 96, 327–341 (2005).

Index

absorptance, 112 absorption coefﬁcient, 24, 56, 319, 348 absorption edge, 221, 223 acceptor, 238 acoustic phonon, 69 Airy function, 105, 106 alkali halides, 93 aluminum, 86 amplitude reﬂection coefﬁcient, 26, 97, 100, 101, 111, 164, 273, 299 amplitude transmission coefﬁcient, 25, 100, 101, 111, 169 anisotropic materials, 14, 276, 285 anomalous dispersion, 58, 60 anomalous skin effect, 37, 196, 265–268, 270, 274 antibonding orbital, 208 band gap, 90, 91, 215, 216 band structure, 88, 115, 137, 207, 233 BCS coherence factors, 194, 195 BCS theory, 180, 189, 191, 197 Beer’s law, 24 biaxial crystal, 284, 285, 295 Bloch’s theorem, 212, 213, 220 Boltzmann equation, 130, 133, 134 bonding orbital, 208 Bose–Einstein statistics, 72, 231, 258 boundary conditions, 26 Bravais lattice, 280 Brewster’s angle, 354, 363 Brillouin zone, 67, 190, 213, 214 carrier density, 31 causality, 152, 156, 157, 242 cgs-Gaussian, 7, 347, 351 charge-density wave, 260 charge-transfer exciton, 233 charge-transfer transition, 257 charged phonons, 261 chemical potential, 121 circular polarization, 278, 279, 317, 322, 324, 326, 327, 329 classical skin depth, 60, 61, 268 Clausius–Mossotti model, 47, 49, 335 clean limit, 199 coherence, 99

397

coherence factors, 180, 200 coherence length, 189, 199 complete set of states, 148 complex conductivity, 18, 33, 35 complex dielectric function, 17, 18, 35, 49, 50, 96 complex refractive index, 19, 23, 38, 40, 96, 107, 164, 168, 286, 316 complex scattering rate, 244 conduction band, 137, 138, 217, 220, 222, 224–226, 228, 230, 232, 235, 236, 238 conductivity, 17, 18, 33, 34, 37, 51, 81, 88, 91, 150, 162, 163, 169, 224, 225, 232, 237, 321, 339, 340, 348, 349 conductivity tensor, 311, 314 constructive interference, 99 conventional superconductors, 180, 203 Cooper pairs, 180–182, 189, 192, 195, 203, 204 copper, 85 Coulomb energy, 247 critical angle, 363 critical points, 225 crystal optics, 276, 294 crystal symmetry, 279, 283 crystal systems, 281 cubic crystal, 281, 284 cyclotron frequency, 305–307, 310, 313, 317, 319, 320, 326, 327 cyclotron radius, 306 cyclotron resonance, 317–322 DC conductivity, 33 Debye frequency, 241 density of states, 122, 131 depolarizing ﬁeld, 32, 337 dielectric function, 17, 35, 37, 50, 83, 88, 90, 91, 146, 163, 327, 333, 347 dielectric tensor, 282, 283, 288, 298, 314, 315 dimerized ground state, 260 direct interband transition, 218, 224, 227, 232, 233 direct interband transitions, 218 dirty limit, 197 dispersion relation, 68–70, 79, 80 distribution function, 130, 131 donor, 238 donor level, 238

398

Index

dopant, 88 doping, 237 Drude model, 31–35, 55, 81, 83, 86, 103, 123, 125, 136, 150, 187, 205, 218, 237, 240, 241, 310, 318, 325, 334, 340, 343 effective dielectric function, 335, 337, 341 effective mass, 85, 216, 218, 221, 222, 238, 243, 244, 320 effective medium approximation, 335, 341–343, 345 effectiveness, 267 electric dipole matrix element, 230 electromagnetic waves in vacuum, 11 electromagnons, 325 electron–electron interactions, 31, 54, 115, 247, 249 electron–electron scattering, 247–249 electron-molecular vibration (EMV) interactions, 261 electron–phonon coupling constant, 257 electron–phonon interaction, 129, 257 electron–phonon matrix element, 227, 229, 230 energy bands, 207 energy gap, 88, 189, 198, 207, 221, 225, 226, 232, 233 excitation spectrum, 190, 191, 193, 196, 203, 235 exciton, 91, 224, 233, 234, 236 extinction coefﬁcient, 38, 39, 90, 93 extraordinary refractive index, 289 extraordinary wave, 289, 291, 292, 297, 299, 301 extrapolations, 166 Fano lineshape, 261, 262 Faraday geometry, 316, 326 Faraday isolator, 331 Faraday rotation, 324, 325 Faraday rotator, 330 Fermi–Dirac distribution, 115, 121, 131, 132 Fermi-liquid conductivity, 250 Fermi energy, 119, 120 Fermi momentum, 120 Fermi sphere, 248 Fermi surface, 124, 127, 190 Fermi temperature, 115, 120, 121 Fermi velocity, 120, 121 ferroelectric, 49, 62, 77, 171, 325 ﬂux quantum, 308 free-electron theory, 115 free carriers, 20, 31, 159 Frenkel exciton, 233 Fresnel reﬂectance, 97 GaAs, 223 generalized Drude model, 242 gerade, 73 Ginzburg-Landau theory, 180, 189 Glover-Tinkham formula, 110, 113, 201 gold, 85 golden rule, 143, 145

Hagen–Rubens relation, 41, 58, 60 half-wave plate, 302 Hall angle, 313 Hall effect, 312 helicons, 317, 319 hexagonal crystal, 282, 285 hole, 137, 212, 217, 218, 226, 228, 233–235, 237, 238 Holstein effect, 126, 242, 257–260 homogeneous media, 15 Hubbard model, 251, 252, 254 impedance of free space, 111, 273, 348 impurity, 236 incoherent light, 96 indirect band gap, 225 indirect transition, 227 infrared-active mode, 76 inhomogeneous medium, 333, 337, 339 inhomogeneous wave, 357 interband transition, 35, 81, 83–85, 91, 173, 207, 218, 224, 236, 243 interference, 99 intraband transition, 128, 137, 191, 218 inverting reﬂectance and transmittance, 109, 113 IRAV absorption, 261 isotropic materials, 14 joint density of states, 224, 225 kinetic energy, 149 Kramers-Kronig, 81, 96, 147, 152, 157, 158, 160, 162, 163, 169, 170, 172, 173, 183, 187, 204, 206, 242, 245, 247 Kramers-Kronig analysis of reﬂectance, 164 Kramers-Kronig analysis of transmittance, 169 Lambert’s law, 24 Landau Fermi liquid, 115 Landau level, 308 law of Malus, 301 law of reﬂection, 355 linear materials, 13 linear polarizer, 300 linearly polarized waves, 277 local electrodynamics, 13 local ﬁeld, 45, 47–49, 54, 63, 325 local response, 157 London gauge, 185 London model, 181, 182, 184, 185, 187 London optical conductivity, 184 London penetration depth, 184, 188, 204 longitudinal optical phonon, 73, 91, 93, 95 Lorentz–Lorenz model, 47, 335 Lorentz force, 7, 304, 312, 323, 325 Lorentz model, 44, 49, 51–56, 63, 73, 83, 89, 91, 146, 159, 325 Lyddane–Sachs–Teller relation, 76, 77, 95

399

Index

magnetic birefringence, 324 magnetic circular dichroism, 324 magnetic dipole absorption, 345 magnetic linear dichroism, 324 magnetic resonance, 324 magnetic susceptibility, 27 magneto-optic Kerr effect, 324 magnetoelectric effect, 325 marginal Fermi liquid, 250 mass enhancement, 243 matrix element, 141–143, 219–221, 229 matrix method, 107 Matthiessen’s rule, 37 Mattis Bardeen, 202 Maxwell’s equations, 6, 15, 17, 18, 22, 23, 138, 185, 272, 286, 291, 315, 350, 352, 353 Maxwell’s macroscopic equations, 7, 9 Maxwell-Garnett theory, 335, 338–342, 345 mean free path, 129, 265–270, 274, 306, 318 mean free time, 37 Meissner effect, 185, 186 Meissner state, 177 memory function, 244 metamaterials, 28 mobility, 321, 349 momentum space, 119 monoclinic crystal, 281, 285 Mott–Hubbard gap, 254 multiple internal reﬂections, 97, 99, 101, 105, 112 nearly free electrons, 209 negative index materials, 27 noble metals, 218 nonnormal incidence, 354 nonlocal electrodynamics, 13, 263 normal skin effect, 263, 265, 268, 271 number density, 32 Ohm’s law, 32, 33, 125, 135, 136, 169, 263, 270, 271, 310 optic axis, 284, 288, 289, 299, 301 optical phonon, 70, 102 optical resistivity, 245 optical self energy, 245 optically thick sample, 96 ordinary dispersion, 56, 58 ordinary wave, 288, 289, 291, 297, 299, 301 orthorhombic crystal, 281, 284 oscillator strength, 146, 147, 150, 223, 321 partial sum rule, 173 Pauli principle, 115, 118, 137 Peierls transition, 208, 260 penetration depth, 24, 348 percolation theory, 344 percolation threshold, 339 perfect conductor, 127, 187

periodic boundary conditions, 67, 117, 118, 213 perturbation expansion, 139, 227 phase phonons, 261 phonon, 64, 71, 73, 90, 92, 147, 226, 227, 231 phonons, 2 Pippard, 189 plane waves, 3, 10 plasma edge, 41, 53 plasma frequency, 35–37, 40, 42–44, 46, 49, 50, 81, 86, 243, 267, 314, 326, 348 polariton, 79, 80 polarizability, 30 polarizability of a sphere, 336 polarized light, 276, 283, 287, 289–291, 297, 298, 300 polaroid, 276, 301 poles and zeros, 73, 77 Poynting vector, 22–24, 286, 291, 351 principal axis, 282, 283, 285, 296–298 principal component, 298 quarter-wave plate, 301, 302 quasiparticles, 180, 191 range of wavelengths, 3 ray surfaces, 289, 290 reciprocal lattice, 67 reciprocal space, 119 reﬂectance, 3, 24, 26, 40, 53, 88, 98, 101, 103, 109, 111, 112, 164, 165, 354 refractive index, 19, 26, 38, 39, 53, 83, 93, 163, 172, 319, 327, 347 relaxation-time approximation, 133, 134 relaxation regime, 270 relaxation time, 32 renormalized scattering rate, 246 residual resistivity ratio, 37 resistivity tensor, 311 resonant frequency, 49 reststrahlen, 78 Rice effect, 254, 260–262 scattering rate, 32, 33, 37, 40, 81, 83, 86, 124, 136, 151, 237, 241, 244, 245, 251, 259, 309, 321 screened plasma frequency, 36, 60 selection rules, 73, 138, 218, 220, 226, 236, 282 sheet impedance, 113 Sievers, A.J., 1 silicon, 1, 3, 87, 88, 90 silver, 1, 2, 81, 83, 103, 241 simple harmonic oscillator, 62 single-bounce reﬂectance, 96, 98 skin depth, 24, 60, 113, 188, 264, 265, 349 Snell’s law, 29, 356, 361, 363 sodium chloride, 1, 3, 90 standing wave, 99

400

Index

sum rule, 84, 85, 148–150, 170, 172, 197, 201, 244 superconducting energy gap, 179–181, 184, 190–192, 197, 203, 259 superconducting plasma frequency, 183 superconductivity, 175 surface impedance, 270–275 surface resistance, 258 tetragonal crystal, 281, 284 Thomas-Reiche-Kuhn sum rule, 150 tight-binding, 149, 209, 252 total internal reﬂection, 354 transfer matrix, 108 transition rate, 143–145 transmittance, 3, 97, 101–103, 109, 111, 112 transverse optic phonon, 70 transverse optical phonon, 63, 73, 93, 95 triclinic crystal, 281, 285 trigonal crystal, 282, 285 two-ﬂuid model, 181, 182 type I superconductors, 177 type II superconductors, 177

U:Coulomb repulsion, 252, 255 umklapp scattering, 249 uncertainty principle, 129, 131, 189 unconventional superconductors, 203 ungerade, 73 uniaxial crystal, 284, 285, 288 units, 347 unpolarized light, 277 unrenormalized scattering rate, 246 valence band, 137, 138, 217, 220–222, 224–226, 228, 230, 232, 235, 236 van Hove singularities, 225 vector potential, 138 Verdet constant, 330 Voigt effect, 324 Voigt geometry, 322, 323 Wannier exciton, 233 wave equation, 353 wave propagation, 55, 56 wavenumber, 1, 347 Zeeman energy, 309